Springer Tracts in Modern Physics Volume 228 Managing Editor: G. H¨ohler, Karlsruhe Editors: A. Fujimori, Chiba J. K¨uhn...

Author:
R.E. Walstedt

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Springer Tracts in Modern Physics Volume 228 Managing Editor: G. H¨ohler, Karlsruhe Editors: A. Fujimori, Chiba J. K¨uhn, Karlsruhe Th. M¨uller, Karlsruhe F. Steiner, Ulm J. Tr¨umper, Garching C. Varma, California P. W¨olfle, Karlsruhe

Starting with Volume 165, Springer Tracts in Modern Physics is part of the [SpringerLink] service. For all customers with standing orders for Springer Tracts in Modern Physics we offer the full text in electronic form via [SpringerLink] free of charge. Please contact your librarian who can receive a password for free access to the full articles by registration at: springerlink.com If you do not have a standing order you can nevertheless browse online through the table of contents of the volumes and the abstracts of each article and perform a full text search. There you will also find more information about the series.

Springer Tracts in Modern Physics Springer Tracts in Modern Physics provides comprehensive and critical reviews of topics of current interest in physics. The following fields are emphasized: elementary particle physics, solid-state physics, complex systems, and fundamental astrophysics. Suitable reviews of other fields can also be accepted. The editors encourage prospective authors to correspond with them in advance of submitting an article. For reviews of topics belonging to the above mentioned fields, they should address the responsible editor, otherwise the managing editor. See also springer.com

Managing Editor Gerhard H¨ohler Institut f¨ur Theoretische Teilchenphysik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 33 75 Fax: +49 (7 21) 37 07 26 Email: [email protected] www-ttp.physik.uni-karlsruhe.de/

Elementary Particle Physics, Editors Johann H. K¨uhn Institut f¨ur Theoretische Teilchenphysik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 33 72 Fax: +49 (7 21) 37 07 26 Email: [email protected] www-ttp.physik.uni-karlsruhe.de/∼jk

Thomas M¨uller Institut f¨ur Experimentelle Kernphysik Fakult¨at f¨ur Physik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 35 24 Fax: +49 (7 21) 6 07 26 21 Email: [email protected] www-ekp.physik.uni-karlsruhe.de

Fundamental Astrophysics, Editor Joachim Tr¨umper Max-Planck-Institut f¨ur Extraterrestrische Physik Postfach 13 12 85741 Garching, Germany Phone: +49 (89) 30 00 35 59 Fax: +49 (89) 30 00 33 15 Email: [email protected] www.mpe-garching.mpg.de/index.html

Solid-State Physics, Editors Atsushi Fujimori Editor for The Pacific Rim Department of Physics University of Tokyo 7-3-1 Hongo, Bunkyo-ku Tokyo 113-0033, Japan Email: [email protected] http://wyvern.phys.s.u-tokyo.ac.jp/welcome en.html

C. Varma Editor for The Americas Department of Physics University of California Riverside, CA 92521 Phone: +1 (951) 827-5331 Fax: +1 (951) 827-4529 Email: [email protected] www.physics.ucr.edu

Peter W¨olfle Institut f¨ur Theorie der Kondensierten Materie Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 35 90 Fax: +49 (7 21) 6 08 77 79 Email: [email protected] www-tkm.physik.uni-karlsruhe.de

Complex Systems, Editor Frank Steiner Institut f¨ur Theoretische Physik Universit¨at Ulm Albert-Einstein-Allee 11 89069 Ulm, Germany Phone: +49 (7 31) 5 02 29 10 Fax: +49 (7 31) 5 02 29 24 Email: [email protected] www.physik.uni-ulm.de/theo/qc/group.html

R.E. Walstedt

The NMR Probe of High-Tc Materials

123

Russell E. Walstedt University of Michigan Department of Physics Ann Arbor, MI 48104, USA [email protected]

R.E. Walstedt, The NMR Probe of High-Tc Materials, STMP 228 (Springer, Berlin Heidelberg 2008), DOI 10.1007/ 978-3-540-75565-4

Library of Congress Control Number: 2007936864 Physics and Astronomy Classification Scheme (PACS): 76.60.- K NMR STUDIES IN GENERAL C UPRATE S UPERCONDUCTORS 74.72.- H ISSN print edition: 0081-3869 ISSN electronic edition: 1615-0430 ISBN 978-3-540-75564-7 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com c Springer-Verlag Berlin Heidelberg 2008 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: by the authors and Integra using a Springer LATEX macro package Cover design: eStudio Calamar S.L., F. Steinen-Broo, Pau/Girona, Spain Printed on acid-free paper

SPIN: 11935247

543210

To Erwin, Vince, and Hiroshi

Preface

To the old saying that if you want to learn something about a subject, teach a course on it, I would add the much more arduous option of writing a book about it. The upside, of course, is that you may gain a perspective on a longtime favorite subject which can be achieved in no other way. The fact is that the opportunity to write such a book as this is, indeed, a rare opportunity. This is especially so for someone who, by the calendar, is well into retirement years. While high Tc itself is the opportunity of a lifetime for those of us who experienced it, and revisiting the old milestones in writing this monograph was a genuine nostalgia trip, it is also important to reﬂect on the purpose of such a book as this. Now that the great majority of experimental high-Tc studies are ﬁnished, who could be interested in such a book? To give some kind of answer to this, let me pinpoint the 2006 M2 S Conference in Dresden.1 Not only was it at this conference that the idea for this book was hatched, but the conference itself evinced an astonishingly high level of interest in high-Tc issues, especially the theoretical aspects. Since it is now a number of years since a review of high-Tc studies with NMR has appeared, there may be a need on the part of theorists and other interested parties for an organized summary of results and of the ideas which have been advanced to bind them together. The foregoing oﬀers a partial answer to the “Why now?” question, but let me note that excellent answers to that question also emerge from the subject itself. Although many issues were settled as of 10 years ago, new ideas and even new phenomena have appeared since that time. Let me oﬀer two examples. The conﬁrmation by N. Curro and co-workers of a dynamical exponent crossover in the high-temperature phase diagram opens up a new arena of potential experimental activity. D. Pines and co-workers had predicted such an eﬀect and other theorists, including C. Varma, had predicted a phase 1

This was the 8th International Conference on Materials and Mechanisms of Superconductivity and High Temperature Superconductors, Dresden, July 9–14, 2006.

VIII

Preface

boundary in that region. Another interpretive breakthrough is to be credited to A. Uldry and P.F. Meier, who in 2005 created a new, general method for analyzing relaxation (T1 ) data in terms of temperature-dependent spin– spin correlation coeﬃcients for close-neighbor copper sites. Discussed at some length in this volume, this method rests on a very ﬁrm theoretical foundation. It has the great virtue that it separates spin-spin these correlation eﬀects from the temperature dependence of the quasiparticle dynamics, itself, which theoretical modelers have been trying to get at. If this extraordinarily simple method had been “available” 15 years ago, I suggest that our understanding of these issues would be greatly advanced from where it is. As for regrets, they come mainly under the heading of omissions. There are many excellent pieces of work which are not included, simply for want of time and space. The book was conceived of as a monograph and is in no sense an encyclopedia, not even within the narrow purview of high-Tc NMR. As an example, I greatly regret omitting the large and fascinating subject of impurity doping in cuprates, from which we have nonetheless learned a lot. Let me conclude by mentioning just a few of the people who have contributed, directly and indirectly, to the initiation and creation of this book. First let me thank Prof. Hiroshi Yasuoka, for bringing me to Tokai-mura in Japan for a 5-plus year extension of my career in solid-state NMR, and through which I also became involved in the European physics scene. Let me thank Prof. Dr. Frank Steglich for his support during my extensive visits to Dresden in 2006 and 2007. Invaluable support came from the Department of Physics at the University of Michigan in providing work space and the library facilities required for a project such as this. I want especially to thank Prof. Chandra Varma at the University of California at Riverside, for shepherding this book into existence through his role as editor for Springer Verlag and for his reading of much of the manuscript, giving penetrating, enlightening, and invaluable comments on the presentation. I also thank Jinan Yang for help with computer issues and with the preparation of the ﬁgures.

Ann Arbor, MI,

Russell E. Walstedt June 2007

Contents

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.1 The Basic Phenomenology of High-Tc Materials . . . . . . . . . . . . . 1 1.2 Carrier Doping and the Master Phase Diagram . . . . . . . . . . . . . . 2 1.3 The NMR Probe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 1.4 Outline of the Remaining Chapters . . . . . . . . . . . . . . . . . . . . . . . . 6 1.4.1 Summary of Chapter 2 – NMR Review . . . . . . . . . . . . . . . 6 1.4.2 Summary of Chapter 3 – Preliminary Cuprate NMR . . . 7 1.4.3 Summary of Chapter 4 – The Pseudogap . . . . . . . . . . . . . 7 1.4.4 Summary of Chapter 5 – T1 Models . . . . . . . . . . . . . . . . . 8 1.4.5 Summary of Chapter 6 – The Dynamical Susceptibility . 9 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10

2

Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Basic NMR Phenomenology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 The Basic Hamiltonian for NMR Spectra . . . . . . . . . . . . . 2.1.2 Observation of NMR/NQR Signals . . . . . . . . . . . . . . . . . . 2.1.3 Deﬁnition and Interpretation of NMR parameters: T2 . . 2.1.4 Deﬁnition and Interpretation of NMR parameters: The shift tensor Kαβ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.5 Deﬁnition and Interpretation of NMR parameters: T1 . . 2.2 NMR Probe of sp-Band Metals and Type I Superconductors . . 2.2.1 NMR Shifts and Relaxation in Simple Pauli Paramagnets 2.2.2 The Moriya Theory of Exchange Enhancement in Simple Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.3 NMR in the Superconducting State of Simple Metals . . 2.3 Static and Dynamic Magnetism in d-band Metals . . . . . . . . . . . . 2.3.1 The d-Electron HF Interactions . . . . . . . . . . . . . . . . . . . . . 2.3.2 Orbital Shift and Susceptibility . . . . . . . . . . . . . . . . . . . . . 2.3.3 Spin-Lattice Relaxation Eﬀects for d-Band Electrons . . . 2.3.4 NMR Studies of 3d Metals as Type-II Superconductors .

13 13 14 17 19 21 23 32 33 36 38 44 45 46 50 53

X

Contents

2.3.5 T1 Phenomenology for Type-II Superconductors . . . . . . . 58 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 63 3

The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO . . . . 68 3.1.1 LSCO: A superconductor with Tc (max) 40 K . . . . . . . 68 3.1.2 The 92 K Superconductor YBa2 Cu3 O7−x (YBCO) . . . . . 70 3.1.3 Physical Models of Itinerant Quasiparticles in Cuprates 71 3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 72 3.2.1 NMR Shift and Relaxation of the 89 Y in YBCO7 . . . . . . 73 3.2.2 Establishing the Site Assignment for the Cu(1) and Cu(2) NQR Spectra . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 75 3.2.3 Variation of the 89 Y shift K89 (x) with x for YBCO6+x . 76 3.2.4 Physical Models for the Relaxation of 63 Cu(2) in YBCO7 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79 3.2.5 Introduction of the Spin Hamiltonian Model for the Cu2+ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79 3.2.6 Experimental Breakthrough: Oriented Powder Samples . 80 3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81 3.3.1 General Deﬁnition of the HF Tensors . . . . . . . . . . . . . . . . 82 3.3.2 Extracting the Cu(1,2) HF tensors for YBCO7 from Shift and Susceptibility Data Using the Spin Hamiltonian Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 84 3.3.3 Quantum Chemistry of YBCO7 and the Hyperﬁne Tensor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 87 3.3.4 T1 Ratios and Electron Spin Correlation Eﬀects . . . . . . . 90 3.4 Incorporating 17 O and 89 Y data into the Mila-Rice-Shastry Picture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 92 3.4.1 Measurements of T1 for 17 O in YBCO7 . . . . . . . . . . . . . . 97 3.4.2 The One-Band, Two-Band Debate: 89 Y and 17 O(2,3) NMR in YBCO . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 98 3.5 Formulation of T1 in Terms of χ (q, ω) and q -Dependent HF Couplings . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 99 3.5.1 Derivation of Dynamical Susceptibility T1 Equation . . . 99 3.5.2 The Fluctuation-Dissipation Theorem . . . . . . . . . . . . . . . . 101 3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc . . . . . . . . 104 3.6.1 The NMR Shift Behavior for T < Tc . . . . . . . . . . . . . . . . . 105 3.6.2 The Monien-Pines Calculations of NMR Shifts below Tc 107 3.6.3 Calculating the Relaxation Decay Curve . . . . . . . . . . . . . . 108 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112

Contents

XI

4

Pseudogap Eﬀects in Cuprate NMR Studies . . . . . . . . . . . . . . . 115 4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x . . . . . . . . . . . . . . 117 4.1.1 HF Parameters for YBCO6.63 from Scaling of Shift Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 120 4.1.2 A Simple Model Theory of Spin Dynamics for YBCO6.63126 4.1.3 INS Data for the Pseudogap of Underdoped YBCO . . . . 128 4.1.4 A Comprehensive T1 Data Set for YBCO6.63 . . . . . . . . . 130 4.2 Pseudogap Phenomenology with Other Probes . . . . . . . . . . . . . . 134 4.2.1 Pseudogap Eﬀects in the Electronic Speciﬁc Heat . . . . . . 134 4.2.2 ARPES Studies of Pseudogapped Cuprates . . . . . . . . . . . 136 4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) . . . . . . . . . . . . . . . . . 138 4.3.1 NMR Shift and Relaxation Behavior in Y248 . . . . . . . . . 139 4.3.2 Measuring the Pseudogap Isotope Eﬀect in Y248 with NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 143 4.3.3 Theory of the Pseudogap by Varma. . . . . . . . . . . . . . . . . . 146 4.3.4 Eﬀect of Zn impurities on the Pseudogap in Y248 . . . . . 147 4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x) . . . . . . . . 148 4.4.1 Spin Susceptibility Scaling for La2−x Srx CuO4 . . . . . . . . . 149 4.4.2 Behavior of the 17 O and 63 Cu NMR Shifts in LSCO:x. . 152 4.4.3 63 Cu NQR spectra and Contrasting T1 Behaviors in LSCO:x. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 153 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 156

5

Relaxation Models for Cuprate NMR . . . . . . . . . . . . . . . . . . . . . . 159 5.1 The Uldry-Meier Parameterization Model . . . . . . . . . . . . . . . . . . . 160 5.1.1 Basic Formulation of the UM Analysis . . . . . . . . . . . . . . . 161 5.1.2 The Uldry-Meier Analysis of YBCO7 . . . . . . . . . . . . . . . . 163 5.1.3 The Uldry-Meier Analysis of YBCO6.63 . . . . . . . . . . . . . . 167 5.1.4 The Uldry-Meier Analysis of YBa2 Cu4 O8 (Y248) . . . . . . 169 5.2 The Millis, Monien, and Pines Model for T1 in Cuprates . . . . . 172 5.3 T1 Model for YBCO Using INS Data for χ (q, ω) . . . . . . . . . . . . 179 5.3.1 The Gaussian Model Susceptibility . . . . . . . . . . . . . . . . . . 180 5.3.2 Comparison with the UM Analysis Results for YBCO7 . 184 5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics . . . . . . . 187 5.4.1 Basic Formulation of the Dynamic Susceptibility . . . . . . 187 5.4.2 Remarks on the Hubbard Model Calculations . . . . . . . . . 189 5.5 The Large-U Hubbard Model of Si, Levin et al . . . . . . . . . . . . . . 192 5.6 Relaxation via Orbital Currents proposed by Varma . . . . . . . . . 195 5.7 Relaxation of Planar 63 Cu and 17 O at T < Tc . . . . . . . . . . . . . . . 199 5.7.1 χ (q , ω) for the Small-U Hubbard Model at T < Tc . . . 201 5.7.2 T1 and Spin-Spin Correlations below Tc : The UM Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 207 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210

XII

Contents

6

Dynamic Susceptibility Studies for the Cuprates . . . . . . . . . . . 213 6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 214 6.1.1 Some General Properties of the Indirect Spin-Spin Coupling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 216 6.1.2 The Gaussian model of Indirect Spin-Spin Coupling in YBCO . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 217 6.1.3 Measuring Indirect Spin-Spin Coupling via Spin-Echo Decay . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 218 6.1.4 Behavior and Interpretation of Indirect Couplings in YBCO and Y248 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 219 6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc . . . . . . . . 224 6.3 Coordinated Interpretation of NMR and INS Data for LSCO . . 227 6.3.1 Review of INS Data for Optimally-Doped LSCO . . . . . . 228 6.3.2 Interpretation of 63 Cu and 17 O T2 Data with INS Data for χ (q) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 236 6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) . . . . . . . . . 242 6.4.1 Phase Diagram and Basic Relationships for T1 , T2g . . . 242 6.4.2 The Dynamical Crossover Study by Curro et al: Y248 . . 245 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 250

A

Appendices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 A.1 Some Basic Properties of Spin Echoes . . . . . . . . . . . . . . . . . . . . . . 253 A.1.1 Basic Derivation of the Two-Pulse Spin Echo. . . . . . . . . . 253 A.1.2 Modelling Spin-Echo Decay . . . . . . . . . . . . . . . . . . . . . . . . . 257 A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling 257 A.2.1 Indirect Coupling with a Gaussian Susceptibility . . . . . . 258 A.3 Spin Echo Decay via Spin-Lattice Relaxation . . . . . . . . . . . . . . . 260 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 261

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 263

1 Introduction

The discovery of high-temperature superconductors among hole-doped CuO2 structures was one of those rare events in the scientiﬁc sphere which launches a whole new world of activity for hundreds of theorists and experimentalists alike. It is now more than twenty years since the New York City APS meeting dubbed the “Woodstock of Physics” witnessed the announcement of the original high-Tc results [1], but the level of activity on this topic remains extraordinarily high. For the nuclear magnetic resonance (NMR) probe, the high-Tc materials have oﬀered a panorama of new phenomenology to be analyzed and categorized in ways which had not previously come into use. It is the purpose of this volume to give a systematic account of many of the phenomena which have come to light in the process. The style of presentation is intended to be partly historical, partly tutorial for the non-specialist, and partly a review. There is by now a very large number of well-established ideas and eﬀects descriptive of the cuprates to be addressed. However, there is also the feeling, even twenty years on, that this monograph oﬀers only a snapshot of a vigorous and ongoing enterprise. We begin by presenting in this introductory chapter a broad perspective on the phenomenology and materials to be addressed, as well as on the NMR probe itself in the context of the cuprates. This is followed by an organizational synposis of the remaining chapters.

1.1 The Basic Phenomenology of High-Tc Materials The concept of a half-ﬁlled “conduction band” which cannot conduct on account of on-site Coulomb repulsion forces was inaugurated in 1949 by N.F. Mott – the “Mott insulator” [2]. Mott, who discussed the case of NiO, commented, “Experiments on the conductivity of cupric salts would be of great interest” [2]. Nearly forty years later a “cupric salt”, with a modest amount of hole-doping in the conduction plane, emerged as a superconductor,

R.E. Walstedt: Introduction, STMP 228, 1–11 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 1

2

1 Introduction

and “high-Tc ” was born. Just how such a system conducts – and superconducts – then became the investigative preoccupation of hundreds, possibly thousands of researchers around the world for many years to follow. The basic process whereby the entire system of localized, S = 12 , Cu2+ moments becomes a set of itinerant quasiparticles with the addition of a far smaller number of mobile hole “carriers” is one of great fascination, upon which even now there seems to be no clear theoretical consensus. As a basic mechanism, however, the Zhang-Rice singlet picture [3] provides at least a conceptual framework. Since the quasiparticles which result are known (through NMR studies) to pair oﬀ at low temperatures into a ground state of magnetically inert Cooper-pair singlets, the resulting scenario of fully itinerant character for the solitary holes on the Cu2+ sites seems at this point incontrovertible. Furthermore, these quasiparticles are known to possess a Fermi surface, with respect to which angle-resolved photoemission studies (ARPES) can be used to measure the superconducting energy gap. However, in many cases, gapping is found to occur in the normal state as well [4, 5, 6], in what is known as the “pseudogap” [7]. Many of the high-Tc systems also exhibit poor, but metallic-like conduction in the normal state, characterized by a non–Fermi– liquid temperature dependence ρ ∝ T instead of the usual T 2 . While the cuprates exhibit certain metallic attributes, they also clearly possess some features characteristic of the undoped insulating host, namely a powerful antiferromagnetic (AFM) exchange interaction between nearestneighbor Cu2+ moments. The eﬀects of these AFM couplings have emerged from virtually all inelastic neutron scattering (INS) studies of the cuprates, and are a major feature of theoretical modelling and experimental ﬁts to nuclear relaxation data as well (see Sect. 1.3).

1.2 Carrier Doping and the Master Phase Diagram There are by now hundreds of host structures known which contain CuO2 quadratic layers that superconduct under suitable doping conditions. A partial list is given in the review by Hazen [8]. In this volume, in order to limit the extent of material to be covered, we focus on the three principal systems La2−x Srx CuO4 (LSCO:x), YBa2 Cu3 O7−x (YBCO7-x), and the related stoichiometric compound YBa2 Cu4 O8 (Y248). These three were chosen, because they emerged early on as systems easy to synthesize and characterize. As a consequence, there is an extensive literature built up around them both in terms of experimental data and, naturally, of theoretical modelling as well. Even with our purview narrowed to these three systems, there are unfortunately many interesting studies which had to be omitted. One of the most important characteristics of the YBCO7-x and LSCO:x are their phase diagrams, plotted with coordinates T vs. δ, where δ represents the doping level of carriers in the CuO2 planes. An early version of the cuprate

1.2 Carrier Doping and the Master Phase Diagram

3

T TS AF

TR

Tc 0

δc

δ L

H

Fig. 1.1. The temperature vs. δ phase diagram of a typical cuprate structure, where δ is the number of hole carriers per formula unit. In the case of La2−x Srx CuO4 , one has δ ∼ x. For very small values of δ there is an antiferromagnetically ordered region. To the right of that is a roughly parabolic region of superconducting behavior which is centered on δ 0.15. See text for additional discussion. Reprinted ﬁgure from T. Tanamoto, H. Kohno, and H. Fukuyama, J. Phys. Soc. Japan 62, 717 (1993). Copyright 1993 Physical Society of Japan

phase diagram is shown in Fig. 1.1, where the superconducting phase lies under a dome extending from δ = 0.05 up to δ ∼ 0.35. At lower δ values there is an AFM phase which as δ → 0 occurs at TN 325 K. The lines extending above and to the left of the superconducting dome represent, in the present instance, maxima in the spin susceptibility and in the nuclear relaxation curves, respectively [9]. In versions of this phase diagram discussed in Chaps. 4 and 6, these lines have other interpretations as well, such as the pseudogap temperature or the crossover between the tetragonal and orthorhombic phases in LSCO, etc. – see Sect. 1.4). There is, in principle, a phase diagram similar to Fig. 1.1 for every cuprate structure. It happens for LSCO:Δ that the hole doping level can be varied across the entire superconducting range by varying δ. In YBCO7-x, on the other hand, the doping is controlled via the oxygen content. At x = 0 (YBCO7) the structure is stoichiometric and the hole-doping level is ∼ 0.33 per Cu ion, which is just slightly above optimal doping [10, 11]. As x is increased, the doping diminishes all the way into the AFM insulating phase. However, the overdoped phase which would correspond to negative values of x simply does not exist. The stoichiometric compound Y248 is structurally similar to YBCO7, but with an extra chain layer. It has a very stable oxygen content up to relatively high temperatures, but its doping level giving Tc 84 K cannot be altered without decomposition. It has been an attractive system for study and will be discussed in Chaps. 4, 5 and 6. Characterization of samples for experimental investigation is a matter of great importance, since a large body of reliable data for mainstream

4

1 Introduction

structures is on hand. Sample characterization includes morphology of the sample material, x-ray crystallography for phase purity, superconducting diamagnetism (Meissner eﬀect) including the value and sharpness of Tc , and magnetic susceptibility for excessive local moment content. The NMR and NQR studies themselves include sample characterization tests, to be mentioned in Sect. 1.3 to follow. For articles discussing structures and a variety of bulk and other measurements, see the reviews edited by D.M. Ginsburg [12].

1.3 The NMR Probe The NMR probe is a local, real–space probe, where the behavior of nuclear spins can be monitored on a site–by–site basis. The magnetic hyperﬁne (HF) interaction of a nucleus couples it to magnetic entities in its immediate environment. This interaction rarely goes beyond nearest-neighbors, though dipolar interactions may have some eﬀects beyond that range. One of the remarkable HF eﬀects in cuprates is the extraordinarily large coupling of 63,65 Cu with neighboring (Cu2+ ) electron spin moments, which is comparable with on–site interactions. There is, however, an intervening O2− ligand, so this is a second-neighbor interaction. Such an eﬀect was unprecedented. The eﬀect of HF couplings is also strongly aﬀected by site symmetry, where strong, but equal couplings to antiferromagnetically correlated neighbor spins may be rendered ineﬀective. Such eﬀects are well known for insulating antiferromagnets (e.g. 19 F in KMnF3 ). The measurements performed and type of data received are also very much conditioned by the properties of the naturally occurring nuclear species in the system investigated. Thus, the 100% abundant, I = 12 , 89 Y in YBCO7, with its nearly isotropic NMR shift, total absence of quadrupole eﬀects, and weak, but adequate relaxation times was the subject of the ﬁrst NMR study on cuprates to be published [13]. The 63,65 Cu isotopes with I = 32 , (nearly) axial site symmetry, and very substantial quadrupolar energies which allow both NMR and NQR to be performed, were quick to follow [14, 15, 16, 17]. Studies of 17 O, which only appeared after an interval of many months, were hampered by the fact that 17 O is present in only trace quantities in natural oxygen. Further, it is too expensive to incorporate into the sample synthesis and has to be diﬀusively exchanged into sample materials at an elevated temperature. Such a process is critically dependent on diﬀusion rates in any given material. In LSCO:x, for example, diﬀusion is fast and single crystals of moderate size are easily doped with 17 O. For YBCO7-x, however, this is only feasible with powders and crystals of the smallest size. With Y248 it is also very diﬃcult, requiring lengthy high-temperature anneals [18]. Nonetheless, 17 O doping eventually became a routine element of technique.

1.3 The NMR Probe

5

A Sampling of NMR Measurements and their Interpretation We give a brief survey of types of NMR observations made and their signiﬁcance for the behavior of cuprate materials. First, the NMR spectrum is fundamental and is a major element of sample characterization. The width and distribution of NMR/NQR resonance lines tells a great deal about the phase purity and microscopic quality of sample material. If there are crystallographically inequivalent sites, they usually have diﬀerent spectra. Quadrupolar frequency shifts and broadening and their ﬁeld/frequency dependence can usually be analyzed to yield values of coeﬃcients from the HF Hamiltonian. These matters are reviewed in some detail in Chap. 2. The NMR shift, which is measured as a frequency shift proportional to the applied ﬁeld, is fundamentally a measure of the various terms in the magnetic polarization of the sample, conveyed to the nuclear spins by HF coupling ﬁelds. The NMR shift is an important source of information on intrinsic susceptibilities. For example, the decay of the spin susceptibility in the superconducting state can usually only be measured via the NMR shift, where direct magnetic measurements would be swamped by the much larger diamagnetic response. There are various contributions to NMR shifts in metals. The s-contact shift, for which we reserve the term “Knight shift” [19], is a mainstay effect in sp-band and d-band metals. In cuprates this term is oddly absent. In its place are the core–polarization shift, orbital shift, dipolar shift, and even “spin-orbit shift”, a second-order eﬀect which arises in the spin Hamiltonian model. There are also very important transferred HF ﬁelds giving rise to NMR shifts, originating in the Mila-Rice [20] and Shastry [21] treatments of cuprate quantum chemistry. NMR shift measurements are a very important tool for determining the HF parameters, since any such determination is independent of model assumptions required for the dynamics. NMR dynamics, as represented by the spin-lattice relaxation time T1 , are a key diagnostic of quasiparticle dynamics in metals and in cuprates in particular. T1 is linked to χ (q, ω) via the ﬂuctuation dissipation theorem [22, 23]. In cuprates, T1 measurements have been interpreted (for the ﬁrst time!) through theoretical modeling of χ (q, ω). What makes this process particularly interesting is the interplay between the strong AFM ﬂuctuation eﬀects, which typically produce an AFM peak near q = (π, π), and the transferred HF couplings at 17 O(2,3) and 89 Y in, e.g. YBCO7-x, which allow their relaxation processes to avoid the AFM peak. Meanwhile, the 63 Cu(2) are quite sensitive to the AFM peak. In eﬀect one has, then, a “q–space spectrometer” for quasiparticle ﬂuctuations. These eﬀects occupy a substantial fraction of the discussion in this volume. T1 measurements are also very sensitive to the diﬀerence between s–wave and d–wave gap characteristics in the superconducting state. Calculations of d–wave T1 characteristics below Tc were among the ﬁrst strong evidences for d–wave singlet character of quasiparticle pairing in cuprates [24, 25].

6

1 Introduction

A second relaxation time, the spin-echo decay time T2g , has taken on a major signiﬁcance in the eﬀort to characterize the dynamic susceptibility of cuprate compounds. This decay time is actually used to measure a static interaction which occurs in cuprates, namely a c-axis indirect spin-spin coupling of the form Hzz = ij= αij Izi Izj , which was ﬁrst identiﬁed by Pennington et al. [26]. How this comes about is discussed in Appendix A.1 and in Chap. 6 of the book. Interpretation of Hzz in terms of χ (q, 0) for q in the vicinity of (π, π) was established by the Pennington–Slichter model calculation [27]. Through measurements of T2g the indirect coupling has become a major element in characterizing the strength of AFM ﬂuctuations in cuprates. In addition, the interpretation of T2g in the superconducting state by Bulut and Scalapino [24] again provided dramatic evidence in favor of d–wave pairing several years before it was widely accepted by the research community. The foregoing is just a sampling of interesting eﬀects which have come to light through NMR studies of cuprate superconductors. We refer the interested reader to sources on the fundamental principles of NMR [28, 29], on NMR studies of conventional metals and superconductors [30, 31, 32], as well as on NMR of high–Tc superconductors [33, 34, 35, 36, 37, 38]. We now give a brief summary of the remaining chapters.

1.4 Outline of the Remaining Chapters This section gives a brief summary of the content of Chaps. 2–6. 1.4.1 Summary of Chapter 2 – NMR Review In Chap. 2 we give a review of the elements of NMR technique and interpretation, where basic deﬁnitions of key NMR parameters are given and some of the pitfalls and complexities associated with powder samples are discussed. The use of spin echoes – the standard tool for conducting NMR measurements – is described, with a detailed derivation including spin echo decay mechanisms presented in Appendix A.1. This leads into a summary of basic relaxation mechanisms for simple metals, including the Moriya theory of electron–electron interaction eﬀects [22] and the BCS-based interpretation of the spin-paramagnetic shift and T1 behaviors in the superconducting state. The Anderson–Farrell resolution of spin-orbit coupling eﬀects for T < Tc is covered in some detail. These eﬀects were struggled over for many years, but almost all problems were ﬁnally resolved. Discussion of the foregoing is extended to d–band metals, including the discovery and establishment of orbital shifts and relaxation eﬀects. The interpretation of NMR spectra and relaxation eﬀects in the mixed state of type-II superconductors is discussed at some length, with data from the literature. Many of the associated problems have cropped up again with the cuprates. The discussion of, e.g. the V3 X’s is oﬀered as a foundation for understanding cuprate mixed-state NMR.

1.4 Outline of the Remaining Chapters

7

1.4.2 Summary of Chapter 3 – Preliminary Cuprate NMR Chapter 3 gives an account of the early stages of high-Tc NMR research. In the ﬁrst two years, almost all studies were done with either random powder samples or microcrystals with very low signal amplitude. There was an intense focus on YBCO7, because of its high Tc (∼ 90 K) and because of its relative ease of preparation. In random powders, 63 Cu(2) NMR spectra (just the − 12 ↔ 1 2 transition) were ∼ 5 kG wide in an 8T laboratory NMR magnet, taking several days of signal averaging to perform a single scan. T1 measurements on the 63,65 Cu were done mainly with NQR, once the frequencies had been extracted from NMR spectra. 63 Cu(2) NMR shifts persisting into the superconducting state were identiﬁed as Van Vleck orbital shifts. The anisotropy and magnitude of these shifts ﬁt well with a simple spin Hamiltonian model of the copper ionic state, which appears to resemble that of a Cu2+ ion in an insulating host for the purpose of analyzing HF eﬀects. This picture has held up even until now. Moreover, the dx2 −y2 ground state orbital dictates that the normally dominant orbital T1 mechanism eﬀectively vanishes in the cuprates. In Sect. 5.6 a proposal for its revival via the marginal Fermi liquid theory is presented [39]. The apparent vanishing of the c–axis spin HF ﬁeld led to the Mila-Rice A proposal: A massive transferred HF coupling from nn Cu2+ ions nearly 4˚ away. This unprecedented HF term made sense of the T1 and NMR shift data for the 63 Cu(2). Their watershed paper, including calculated quantum chemistry, provided a framework for interpretation of cuprate NMR data which has held up ever since [20]. The chapter closes with an account of the ﬁrst interpretation of T1 data in the superconducting state using d–wave pairing with BCS theory, by Monien and Pines [24]. This landmark result gave a clear indication of the correctness of d–wave and the inadmissibility of s–wave, even though it would be ﬁve more years before the correctness of this picture was widely accepted. 1.4.3 Summary of Chapter 4 – The Pseudogap Even before the Mila-Rice resolution of anomalous NMR shift behavior appeared, workers had begun to explore the highly unusual behavior in the underdoped region of the phase diagram in Fig. 1.1. There it was found that low-frequency ﬂuctuations which drive the T1 process, as well as the uniform susceptibility, were beginning to collapse at temperatures far above Tc . It was as though the superconducting energy gap was beginning to develop at some T ∗ well above Tc in anticipation of the actual transition to superconductivity. In the spirit of “spin–charge separation”, an idea that dominated early thinking on cuprate quasiparticle behavior [40], this eﬀect was at ﬁrst dubbed the “spin gap”. There was a tacit assumption that charge states were unaﬀected. Nonetheless, the spin pseudogap was soon recognized as a universal feature of the underdoped phases. Moreover, in a most astonishing bit of prescience,

8

1 Introduction

the appearance of such a precursive energy gap in the cuprates had actually been predicted by Friedel [7], who coined the term “pseudogap”. Pseudogap characteristics via NMR shift and T1 data are documented in detail for several compounds in Chap. 4. Several years after the spin ﬂuctuation properties of pseudogap systems were well established, it came to light through both electronic speciﬁc heat and ARPES measurements that charge properties were also profoundly altered in pseudogap systems. In this chapter we also review these eﬀects brieﬂy. With ARPES one ﬁnds that certain regions of the Fermi Surface, e.g. the quadratic axes, are gapped while while the diagonal regions are not. Since the dynamic susceptibility is a summation over the Fermi surface, this means that the gap reﬂected by χ (q, ω) may vary signiﬁcantly with q. It follows that pseudogap T1 behavior can be quite diﬀerent at the 63,65 Cu site from what it is at the 17 O sites. These diﬀerences are clearly observed in a number of cases discussed. The pseudogap behavior of LSCO:x is particularly interesting. In what was actually the ﬁrst pseudogap behavior to be reported [41], the remarkable scaling of susceptibilies for diﬀerent x values in this system was at ﬁrst interpreted with a model suited to 2D insulating antiferromagnets. This is possible, since the latter systems exhibit a susceptibility temperature maximum which resembles pseudogap behavior. The disparate behaviors of 1/T1 T for the 63,65 Cu and the 17 O also clearly tag this system as having a pseudogap. The low-T χ0 (T ) ∝ T 1/2 behavior of LSCO:x is in accord with the Varma theory of pseudogap behavior [39], as is that of Y248 [42]. 1.4.4 Summary of Chapter 5 – T1 Models From the earliest days of high-Tc NMR one of the main challenges has been to understand the disparate behaviors of T1 at various lattice sites. In addressing this question, there are several important branching points in the ﬂow diagram of deduction so to speak. Magnetic dipole processes are assumed to be predominant. First, then, one must decide whether spin ﬂuctuations alone will suﬃce to explain everything, or whether orbital relaxation, severely inhibited by the dx2 −y2 ground–state orbitals, will play a role as well. Many workers have opted for the spin ﬂuctuation picture, while the existence of a possible orbital mechanism has been pointed out by Varma [39]. A summary of the latter calculation is given in Sect. 5.6. In the purely spin-dynamical picture, one must next decide whether a single dynamical variable per Cu2+ site, namely the itinerant S = 12 hole, is suﬃcient, or do the doped–in hole carriers form a second dynamical entity? The general approach to this question has been to see whether a complete account of the data can be given with one variable per site. Several T1 modeling eﬀorts based on the latter assumption are described in Chap. 5, where it is presumed with Moriya [22] that any successful scenario can be expressed in terms of χ (q, ω). Three of these employ the random–phase approximation in order to incorporate the (mandatory) electron–electron interactions, and

1.4 Outline of the Remaining Chapters

9

one is simply based on the shape and width of the the AFM peak in χ (q, ω) determined by INS studies. Quite recently, however, a novel, but related approach was pioneered by Uldry and Meier [43], in which they attempt to systematize T1 data on several cuprates using electronic spin–spin correlations as parameters which vary with T and in which there is a universal spin ﬂuctuation frequency (correlation time), also a function of T, which applies to all T1 processes. The other central assumption is that the HF Hamiltonian has the Mila–Rice form ⎡ ⎤ (1.4.1) Siα ⎣Aα + B Ijα ⎦ HHF = α

i

j(nn)

for the planar 63,65 Cu nuclei, with similar forms for the ligands. With these ingredients all of the data are ﬁtted in a self-consistent way. The form (1.4.1) and the admissibility of the spin–spin correlations and correlation time as temperature–dependent parameters are the main assumptions here. A theoretical basis for this scheme is derived using χ (q, ω) in Chap. 3. It yields an internally consistent picture, in which the dynamically–derived HF constants basically agree with those derived from the shift. This scheme is useful for evaluating theoretical models as well as for analyzing experimental data. 1.4.5 Summary of Chapter 6 – The Dynamical Susceptibility In this chapter three topics related to modeling and characterization of χ(q, ω) are presented and discussed. First, large indirect spin-spin couplings in cuprates were noted early on and modeled quantitatively by Pennington and Slichter [25]. Further, the strength of indirect spin–spin couplings Hzz noted above can be measured by means of spin-echo decay if the entire nuclear spin transition observed can be inverted by the spin echo refocussing pulse (θ2 π). Measurements of this type have been carried out on a number of systems, yielding a quantitative measure of χ (q, 0) q = (π, π). This has become an important source of input data for the dynamical susceptibility. Another major data source for χ (q, ω) is INS. The compound LSCO:x with x 0.15 became an important test case for χ (q, ω). This system bears the distinction of having been measured with INS in absolute units over most of the ﬁrst Brillouin zone (all known structure), over energies ranging from 1–200 meV, and at temperatures ranging from below Tc to nearly 300 K [44]. The dynamical susceptibility determined in this way was found to be highly incommensurate. These data were used to calculate T1 for 63,65 Cu and for 17 O, with interestingly mixed results. The NMR data behave as though the discommensurations were either much smaller or simply not there at all. The ﬁnal section of Chap. 6 oﬀers a brief review of the behavior of T1 and T2g in the normal state region above and principally on the left side of the superconducting dome in Fig. 1.1. Sokol, Barzykin, and Pines have proposed

10

1 Introduction

a crossover in the value of the dynamical exponent from z = 1 (quantum critical phase) to z = 2 (non-scaling region) [45, 46]. The line dividing these two behaviors is suggested to take place where the correlation length ξ(T ) = 2a (a = lattice constant). This idea has been tested up to 700 K on the cuprate Y248 by Curro et al [47]. A clear transition from z = 1 to 2 was found at T = 500 K, giving support to this scaling theory.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12.

13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29.

J.G. Bednorz, K.A. Mueller, Z. Phys. B64, 189 (1986) 1 N.F. Mott, Proc. Phys. Soc. London Sect. A62, 416 (1949) 1 F.C. Zhang, T.M. Rice, Phys. Rev. B37, 3759 (1988) 2 J.M. Harris, Z.-X. Shen, et al., Phys. Rev. B54, R15665 (1996) 2 A.G. Loeser et al., Science 273, 325 (1996) 2 H. Ding et al., Nature (London) 382, 51 (1996) 2 J. Friedel, Physica C153–155, 1610 (1988) 2, 8 R.M. Hazen, in Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), p. 121 2 T. Tanamoto, H. Kohno, H. Fukuyama, J. Phys. Soc. Japan 62, 717 (1993) 3 T. Graf, G. Triscone, J. Muller, J. Less-Common Met. 159, 349 (1990) 3 M. Horvati´c, T. Auler, C. Berthier, Y. Berthier, et al., Phys. Rev. B47, 3461 (1993) 3 D.M. Ginsberg (ed.), Physical Properties of High Temperature Superconductors I (World Scientiﬁc, Singapore, 1989) and Physical Properties of High Temperature Superconductors II (World Scientiﬁc, Singapore, 1990) 4 J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts, Sol. St. Comm. 63, 847 (1987) 4 D. Brinkmann, L. Pauli, J. Roos, H. Zimmermann, Phys. Lett. A124, 112 (1987) 4 W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 59, 1860 (1987) 4 H. L¨ utgemeier, M.W. Pieper, Sol. St. Comm. 64, 267 (1987) 4 I. Furo, A. J´ anossy, L. Mih´ aly, et al., Phys. Rev. B36, 5690 (1987) 4 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 4 W.D. Knight, Phys. Rev. 76, 1259 (1949); C.H. Townes, C. Herring, W.D. Knight, Phys. Rev. 77, 852 (1950) 5 F. Mila, T.M. Rice, Physica C157, 561 (1989) 5, 7 B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 5 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 5, 6, 8 V. Jaccarino, in Physics of Solids, International School of Physics “Enrico Fermi”, Course XVIII (Acadamic Press, New York, 1966) 5 H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990) 5, 6, 7 N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 5, 9 C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 6 C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 6 A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 6 C.P. Slichter, Principles of Magnetic Resonance, 3rd edn. (Springer-Verlag, New York, 1992) 6

References

11

30. J. Winter, Magnetic Resonance in Metals (Clarendon Press, Oxford, 1971) 6 31. A. Narath, Hyperﬁne Interactions, ed. by A.J. Freeman and R.B. Frankel (Academic Press, New York, 1967), p. 287 6 32. D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, Vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 6 33. C.H. Pennington, C.P. Slichter, In Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsberg (World Scientiﬁc, Singapore, 1990), p. 269 6 34. R.E. Walstedt, W.W. Warren, Jr., Science 248, 1082 (1990) 6 35. C.P. Slichter, in Strongly Correlated Electron Systems, ed. by K.S. Bedell et al., (Addison – Wesley, Reading, MA, 1993), p. 427 6 36. D. Brinkmann, M. Mali, in NMR Basic Principles and Progress, Vol. 31 (Springer Verlag, Berlin, 1994), p. 171 6 37. C. Berthier, M.H. Julien, M. Horvati´c, Y. Berthier, J. Phys. I France 6, 2205 (1996) 6 38. C.P. Slichter, in Handbook of High Temperature Superconductivity, ed J.R Schriﬀer, J.S. Brooks (Springer Science+Business Media, New York, 2007), p. 215 6 39. C.M. Varma: Phys. Rev. Lett. 77, 3431 (1996) 7, 8 40. P.W. Anderson, Science 235, 1196 (1987) 7 41. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 8 42. G.V.M. Williams, et al., Phys. Rev. Lett. 80, 377 (1998) 8 43. A. Uldry, P.F. Meier, Phys. Rev. B72, 094508 (2005) 9 44. G. Aeppli, T.E. Mason, et al., Science 278, 1432 (1997) 9 45. A. Sokol, D. Pines, Phys. Rev. Lett. 71, 2813 (1993) 10 46. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 10 47. N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 10

This page intentionally blank

2 Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors

The ﬁeld of high-Tc NMR developed in a context of many years of NMR studies of conventional superconductors as well as of d-band transition metals, alloys, and intermetallic compounds. It is therefore appropriate to begin this volume with a brief review not only of the NMR probe, itself, but of the general physical phenomena probed by NMR in transition metal systems, in both the normal and superconducting states. The published literature on this subject matter is, of course, vast, and the references cited here will necessarily be rather limited. We begin by citing the standard works on nuclear magnetism by Abragam [1] and Slichter [2], where almost all basic NMR phenomena are derived and discussed. These sources also present an extensive guide to the early literature, which the interested reader will ﬁnd highly informative. For NMR of metallic systems, there are thorough reviews by Narath [3] and Winter [4] and for early NMR studies on superconductivity, there is a detailed and informative review by MacLaughlin [5]. We shall also have recourse to the treatments of superconductivity by Tinkham [6] and Schrieﬀer [7]. Relevant reviews of high-Tc NMR studies will be cited at the beginning of Chap. 3.

2.1 Basic NMR Phenomenology We begin with a brief review of current NMR technique and its capabilities. The basic data one usually hopes to acquire with resonance methods consist of the spectral shape and features, the frequency shift tensor Kαβ , and the relaxation times T1 and T2 . The acquisition and interpretation of these elements of data will be the preoccupation of most of this volume. Here we wish simply to introduce them, and in this Sect. 2.1 the basic measurement and interpretation of these parameters will be reviewed. Some additional discussion of NMR phenomenology is given in the Appendices.

R.E. Walstedt: Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors, STMP 228, 13–65 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 2

14

2 Introduction to NMR Studies of Metals and Superconductors

2.1.1 The Basic Hamiltonian for NMR Spectra The basic nuclear spin Hamiltonian for spectra is given by (2.1.1), including both the Zeeman term representing the eﬀect of an applied ﬁeld H and a quadrupolar term representing the interaction of the nuclear quadrupole mo∂2V at the nuclear ment with the electrical ﬁeld gradient (EFG) tensor Vuv = ∂u∂v site in question (see [1], Ch. VI). ˆ ·H + ˆ + K) Hspec = −γI · (1

e2 qQ η 2 2 [3I 2 –I(I + 1) + (I+ + I− )], (2.1.1) 4I(2I − 1) z 2

ˆ is the NMR shift tensor and 1 ˆ is the unit tensor. In this equation where K 2 we use conventional notation, where q = | ∂∂ZV2 | = VZZ is the principal component of the EFG tensor, and the EFG asymmetry parameter is deﬁned as η = (VXX -VY Y )/VZZ . The (X, Y, Z) are the principal axes of the tensor, where we deﬁne |VXX | ≤ |VY Y | ≤ |VZZ | and note that LaPlace s equation gives VXX + ˆ q, VY Y + VZZ = 0. It follows that 0 ≤ η ≤ 1. If we permit the parameters K, and η to be distributed, then Hspec will generate the vast majority of NMR spectra found in practice. Although (2.1.1) is frequently quoted, it has the disadvantage that it assumes that the quantization axis is along the principal axis of the EFG tensor. Since one often works with the ﬁeld along some principal axis of the EFG, it is useful to generalize (2.1.1) for an arbitrarily chosen principal axis. In principal axis coordinates, the quadrupolar Hamiltonian becomes [1] eQ Vαα Iα2 . (2.1.2) HQ = 2I(I + 1) α In terms of the Vαα , (2.1.1) becomes in traceless form [2] ˆ ·H + ˆ + ·K) Hspec = −γI · (1

eQ [Vαα (3Iα2 − I(I + 1)) 4I(2I − 1)

1 2 2 + (Vββ − Vγγ )(I+ + I− )] , (2.1.3) 2 where α is the quantization axis and (α, β, γ) are an arbitrary permutation of (X,Y,Z). In this form it is clear that ﬁrst-order splittings will be proportional to | Vαα |, and the second-order splittings will be proportional to (Vββ −Vγγ )2 . While (2.1.1) and (2.1.3) are useful for generating spectra, it should be noted that a number of other terms are necessary for a complete description of NMR phenomena. Some of the omissions are (a) terms to represent ﬁxed internal hyperﬁne (HF) ﬁelds which may occur in ordered magnetic systems, (b) spin and orbital ﬂuctuation terms which drive T1 processes, (c) dipolar and indirect spin-spin coupling terms which generate T2 processes, and (d) radiofrequency (rf ) excitation terms. Such terms will be invoked when the need arises. We make a number of general remarks about the use of (2.1.1) and (2.1.3) to generate and analyze spectra.

2.1 Basic NMR Phenomenology

•

• •

•

•

•

•

15

Experiments are usually carried out in one of two limiting cases, namely, H = 0, so that quadrupolar energies alone determine the spectrum (NQR), e2 qQ and secondly, the high ﬁeld limit γH 4I(2I –1) , wherein the quadrupolar terms may be treated with perturbation theory. For I = 12 the nuclear quadrupole moment Q vanishes identically, according to the Wigner–Eckart theorem (e.g. see [2], Ch.10). For nuclear spin sites with cubic symmetry, one has VXX = VY Y = VZZ = 0, greatly simplifying the spectrum as with I = 12 . For quadrupolar nuclei, the eﬀects of stray EFG’s in nominally cubic structures may still play a role in the spectrum, however. Crystalline disorder caused by impurities, dislocations, etc., often cause a distribution of stray EFG’s to occur at the nuclei of interest. Thus, one often ﬁnds cubic NMR lines with complete ﬁrst-order broadening, so that only the (- 12 ↔ 12 ) transition is easily resolved. Such cases will be discussed as they arise. In the almost universally encountered high-temperature limit deﬁned by γH kB T , Boltzmann factors are always small compared with unity. The sign of qQ in (2.1.1) is immaterial to the spectra and is, in fact, indeterminate. For convenience, we shall always take qQ to be positive. Note also that the term “-I(I+1)” in (2.1.1) has been inserted only to render the quadrupole tensor traceless. It plays no role in the spectral transition frequencies and may be omitted or replaced by some other quantity for calculational convenience. In the most frequently occurring cases of non-cubic site symmetry, i.e. tetragonal or trigonal, the EFG symmetry is termed “axial”, giving VXX = VY Y . Thus, η = 0 and the quadrupolar Hamiltonian is greatly simpliﬁed. We shall focus primarily on this case and comment on how the results are aﬀected if η > 0. In the high-ﬁeld limit with η = 0, we comment brieﬂy on how the EFG term aﬀects the spectrum. If we let the angle between H and the EFG principal axis Z be θ, then the simplest case is when θ = 0. The eigen-energies then have the exact form Em = −γH(1 + K)m + hνQ m2 /2, where νQ = 3e2 qQ 2hI(2I –1) , m is the Iz quantum number, and we have assumed a scalar shift K. In such a case, the energy levels are shifted as shown in Fig. 2.1. In the spectrum shown, the (- 12 ↔ 12 ) transition is not aﬀected by the νQ term, and the (±m ↔ ±(m + 1)) transitions are displaced by ±νQ , ±2νQ , . . ., for m = 12 , 32 , . . ., respectively, as shown in the ﬁgure. The lines displaced by ±nνQ are known as ﬁrst-order satellites. For θ = 0 the eigenfrequencies can often be estimated satisfactorily with second-order perturbation theory (see [1], Ch. VI). The ﬁrst-order resonance frequencies become (1)

νL + ν±n = νL ± nνQ (3cos2 θ − 1)/2,

(2.1.4)

n = 1, 2, . . .. Here, n = 1 corresponds to the (± 12 ↔ ± 23 ) transitions and n > 1 corresponds to transitions with progressively higher values of m.

16

2 Introduction to NMR Studies of Metals and Superconductors Zeeman m = –3/2 m = –1/2 m = 1/2

Zeeman + Quadrupolar

νL

νL + νQ

νL

νL

νL

νL – νQ

m = 3/2 Spectra:

νL

νL – νQ νL νL + νQ

Fig. 2.1. On the left, the nuclear Zeeman term gives uniformly spaced energy levels and a single NMR line. On the right, ﬁrst-order quadrupole splittings produce “ﬁrstorder satellites” from the (±1/2 ↔ ±3/2) transitions. The (−1/2 ↔ 1/2) transition is not aﬀected to ﬁrst order

In the case of powder samples with a uniform distribution of θ over the unit sphere, the ﬁrst-order quadrupole shift stated above gives rise to an intensity distribution over frequencies ranging from νL −nνQ /2 to νL +nνQ if the θ = 0 satellite displacement is nνQ . The normalized distribution function is 1 (2.1.5) ρq (ν) = [6nνQ (ν − νL + nνQ /2)]− 2 ,

•

•

so that the θ = 0 line at frequency nνQ becomes a powder pattern with a square-root singularity at ν = νL − nνQ /2. Here, the Larmor frequency νL = γH(1 + K). We note that m is no longer strictly a good quantum number, so there are second-order frequency shifts as well. Interestingly, the second-order frequency shifts of the satellites at ±nνQ (3cos2 θ − 1) are equal, so that the second-order correction to their pairwise separation 2nνQ (3cos2 θ−1) vanishes. If η > 0, however, the singularities all disappear and the peak at that position becomes progressively broader as η increases. For the often-used (- 12 ↔ 12 ) transition, the frequency to second order is given by 2 νQ 3 (2) ν± 1 = νL − (2.1.6) I(I + 1) − sin2 θ (9 cos2 θ − 1). 2 16νL 4 In the case of a random powder sample, (2.1.4) and (2.1.6) give rise to characteristic powder patterns which are easy to recognize. Such a pattern is shown in Fig. 2.2, where a small amount of Gaussian broadening has been added. In cases where η > 0, these powder patterns are altered signiﬁcantly. Also, if there is shift anisotropy K(θ) with a range comparable to the second-order quadrupole shift of the (- 12 ↔ 12 ) transition, its powder-pattern shape will also be altered signiﬁcantly, whereas the ﬁrstorder peaks will all reﬂect the shift value K(π/2). Further discussion of these eﬀects is given below. When H = 0 we have the case of nuclear quadrupole resonance (NQR). The nuclear spin energies are determined entirely by Q, I, and the local

2.1 Basic NMR Phenomenology

17

Quadrupolar Powder Pattern for (–½ ↔ ½) Transition

–1.5

–1

–0.5

0

0.5

1

1.5

2

2.5

Quadrupole Shift (units of 3νQ2/16νL)

Fig. 2.2. Quadrupolar powder pattern for the (−1/2 ↔ 1/2) transition based on the second-order quadrupolar energy given in 2.1.6 (axial case). Minimal Gaussian broadening has been applied. The coeﬃcient given is for I = 3/2. For arbitrary 2 /64νL half-integral I the coeﬃcient becomes (4I(I + 1) − 3)νQ

EFGs. If νQ (see item 6 above) is large enough, i.e. in the MHz range, then NQR spectroscopy is feasible. Considering the case of η = 0, (2.1.1) then shows that E|m|+1 - E|m| = (2|m| + 1)νQ . Thus, there is a series of I − 12 NQR lines at frequencies νQ , 2νQ , . . .. The m–levels are doubly degenerate, since Em is independent of the sign of m. The two parallel transitions produce identical signals under the usual excitation conditions1 . If η > 0, the levels are still doubly degenerate, but the transition frequencies are now a function of η. If there are two or more NQR frequencies, their ratio can be used to determine η.

2.1.2 Observation of NMR/NQR Signals In the early days of solid-state NMR, it was customary to employ continuous wave methods to observe NMR signals. Techniques such as the marginal oscillator and the popular crossed-coil rf bridge spectrometer manufactured by Varian Associates were used to obtain a wealth of useful NMR data. Compared with pulsed NMR this method has, however, a number of inherent drawbacks. It is not useful for severely broadened lines, it cannot distinguish between static and dynamic line broadening, so it cannot measure T2 , nor a

1

It is possible to separately excite, e.g. the (1/2,3/2) and the (-1/2,-3/2) transitions, using circularly polarized rf pulses (M.J. Weber and E.L. Hahn, Phys. Rev. 120, 365 (1960)). However, for most measurements, there is no advantage in doing so.

18

2 Introduction to NMR Studies of Metals and Superconductors

short value of T1 , to name just a few. Thus, it gradually gave way to pulse methods for solid-state NMR studies2 . The Spin Echo The spin echo[9] is used almost universally for measurement and observation of NMR/NQR signals in solids. Typically, short, medium-power rf pulses applied at the frequency of a |Δm| = 1 transition of the Hamiltonian Hspec are followed by a spin-echo signal as shown in Fig. 2.3. The rf ﬁelds are applied transverse to the axis of spin quantization. The ﬁrst pulse produces a precessing, transverse nuclear magnetization proportional to the instantaneous spin polarization at the time it is applied. The precessing moment following the ﬁrst pulse often decays in a time of the order of the pulse width, as shown in the ﬁgure, and is usually unobservable because of the “dead time” of the receiver. Such a decay time is known as T2∗ 3 . A second rf refocussing pulse at time τ causes the precessing moment to reappear brieﬂy at time 2τ as shown. Using digital electronic methods, such spin echo signals are recorded, noise averaged, and stored for manipulation and analysis. A basic calculation of the spin echo response is presented and discussed in Appendix A.1, including a simple treatment of spin echo decay processes.

Nuclear Spin Echo

–5

–4

–3

–2 –1 0 2ω1 (t – 2τ)/π

1

2

3

Fig. 2.3. A simulated spin echo signal is shown (solid curve), corresponding to the (0.8π/2, π/2) pulse pair (shown) applied to a broad, inhomogeneous distribution of NMR frequencies. The echo is the sum of two contributions which are symmetric and antisymmetric, respectively, (dashed lines) with respect to the center point of the echo. The latter point is at time 2τ + tw2 − tw1 from the leading edge of the ﬁrst pulse, where τ is the time interval between the leading edges of the pulses and tw1,w2 are the respective pulse widths [8] 2

3

There are certain advantages to cw technique, however. If T2 is shorter than a few μs, spin echoes may become unobservable, whereupon cw methods become the only way to observe an NMR signal. T2∗ is often a reﬂection of the inhomogeneous linewidth ΔH, in which case T2∗ ∼ 1/γΔH. If such broadening is severe, then T2∗ will be determined by the length and shape of the exciting rf pulse. In the latter case it is usually unobservable because of ampliﬁer dead time.

2.1 Basic NMR Phenomenology

19

We touch here brieﬂy on an important point regarding spin-echo spectroscopy. This is the frequency resolution of this technique, which is discussed in detail in Appendix A.1. Since the NMR signals are excited using pulse ﬁelds H1 of typically 100 Gauss amplitude, one might suppose that these large ﬁelds would limit the available frequency resolution to ∼ γH1 . However, this is not the case. It is straightforward to demonstrate that the total area under the spin echo waveform is proportional to the line intensity at the frequency of excitation to within a very narrow bandwidth. The resolution obtained in this way is formally independent of the magnitude of the excitation ﬁeld H1 . See Appendix A.1 for details. The question of observability of spin-echo signals is an important one for the NMR spectroscopist. We note here that solid-state NMR signals are typically of the order of microvolts, with expected raw signal-to-noise ratios which are typically of the order of unity or less. Thus, one cannot overemphasize the importance of digital signal averaging methods to the success of modern pulsed NMR technique. The great majority of solid-state NMR studies reported nowadays have used digital signal averaging to improve the signalto-noise ratio. It is also possible to estimate the available NMR signal strength given reasonable estimates of the experimental parameters. A detailed discussion of such matters is beyond the purview of the present volume. 2.1.3 Deﬁnition and Interpretation of NMR parameters: T2 The relaxation time T2 represents a fairly complex realm of phenomenology in NMR. Put most simply, T2 is the transverse decay time for nuclear magnetization. But there are several fundamentally diﬀerent mechanisms for T2 processes as well as two major categories of T2 eﬀects, namely (i) T2 for the free-induction signal excited by a single pulse and (ii) T2 for spin echoes. For both of these, homogeneous broadening refers to the eﬀect of local spin-spin interactions such as dipolar [1], pseudo-dipolar [10], and RKKY [11]. Often, however, NMR lines are statically broadened by disorder and other spurious eﬀects, such that free induction signals are not observable. In contrast, one can nearly always observe the spin echo, which typically does not “see” inhomogeneous broadening. The spin echo is a signal observed when two rf pulses are applied at a time interval τ . At time 2τ from the ﬁrst pulse a signal appears which has typically a much longer decay time than the free induction. For the spin echo, T2 is the decay time constant of the echo amplitude E(2τ ) as the pulse separation τ is increased. A simulated spin echo is shown in Fig. 2.3. A basic discussion of spin echo formation and decay mechanisms is given in Appendix A.1. In high-Tc materials, indirect spin-spin couplings are particularly important. A new and useful formulation of indirect spin-spin couplings in terms of dynamical susceptibilities has been given by Pennington and Slichter[12]. This calculation is discussed in detail in Chap. 6. The

20

2 Introduction to NMR Studies of Metals and Superconductors

measurement of the latter indirect spin-spin couplings via spin-echo decay is analyzed in some detail in Appendix A.1. It is interesting that one can write down a formally exact solution to the spin echo decay problem. The following expression represents the variation of the spin echo amplitude at time 2τ for rf pulses applied at 0 and τ :

∗ ∗ ∗ ∗ E(2τ ) = T r Ix eiHi τ eiθ2 Iy eiHi τ Ix e−iHi τ e−iθ2 Iy e−iHi τ /T r(Ix2 ) , (2.1.7) where the spin system I = i I i is being excited with pulses along the y axis which are assumed for simplicity to be uniform over the entire resonance line. Thus, the initial magnetization lies along the x axis and the refocussing pulse is given a pulse angle θ2 . The interaction Hamiltonian Hi represents all pairwise interaction terms between the spins I i as well as with and among any other nuclear species in the system considered. All such terms have been transformed into a reference frame rotating at the frequency of the applied rf pulses, Hi∗ = exp(iωIz τ )Hi exp(−iωIz τ ), and any non-secular time-dependent terms which result are dropped. Included in Hi is a truncated Zeeman term which might ∗ be written HZ = − i [γH(1 + Ki ) − ω]Iiz . If locally non-uniform, the latter term would have a very important eﬀect on E(2τ ) in that it inhibits ﬂip–ﬂop ﬂuctuation processes among the I i . It is slightly ironic that an inhomogeneous term such as this is frequently necessary for the observation of a spin echo. An expression such as (2.1.7) is not often useful for direct evaluation. However, it can be used to argue the basic features of many special cases of echo decay. We give here a few simple examples. It is the essence of spin echo ∗ mentioned above has no direct eﬀect on formation that a term such as HZ echo amplitude. Any other term in Hi∗ which is static and is unaﬀected by the θ2 pulse will also have no direct eﬀect on echo amplitude. Many spin-spin coupling terms cause ﬂuctuations among the spins I i or among spins which are coupled to the I i . These will cause the echo to decay, and will present many highly complicated sub-cases. A simple example of this behavior is analyzed in Appendix A.1. A case of interest which arises in cuprate NMR is the simple case where all spin ﬂip–ﬂop interactions are blocked by local inhomogeneities. There would be no echo decay process except for the fact that the spins I i are inverted (with a substantial probability) by the θ2 pulse. The typically Gaussian echo decay 2 ] found in this case can then be used to measure the E(2τ ) exp[−(2τ )2 /2T2g indirect spin-spin coupling, as mentioned above. The other important contributor to spin-echo decay is the spin-lattice interaction, which modiﬁes the expression (2.1.7) with a multiplicative factor exp(−2τ /T1E ). The decay constant T1E is a parameter of some complexity and is therefore discussed in detail in Appendix A.2. T1E is only equal to T1 in the case where T1 is isotropic and I = 12 for the nuclei observed, or for I > 12 in the highly unusual case that all |Δm| = 1 transitions are degenerate and are contributing to the echo signal. For a more typical case of half-integral I > 12 , where the (− 12 ↔ 12 ) transition is being observed, then 1/T1E = (I + 12 )2 /T1

2.1 Basic NMR Phenomenology

21

(isotropic T1 ) [13]. It is usually important to account for the eﬀect of T1 in spin echo decay in cuprate NMR studies. Expressions derived for this purpose are given in Appendix A.2. 2.1.4 Deﬁnition and Interpretation of NMR parameters: The shift tensor Kαβ NMR frequency shifts are useful for characterizing a resonance line as well as analyzing diﬀerent components in the magnetic susceptibility of a metallic compound. NMR shifts are useful probes, because they always reﬂect one or more components of magnetic polarization in the system, such as spin or Van Vleck paramagnetism. There can, of course, be magnetic polarization without a palpable NMR frequency shift, but there is no magnetic NMR shift without a source of polarization, i.e. susceptibility, to drive it. There are complications, of course, when there are ﬁxed sources of internal magnetic polarization, such as in the mixed state of a type-II superconductor. Such cases are considered in Sect. 2.3. In general, we have omitted consideration of cases which involve magnetic ordering. Shifts, then, are deﬁned to be linear in the applied magnetic ﬁeld H. Analysis of shifts can be quite complex with random powder samples when the shift is anisotropic, and even more so if they are combined with inherently anisotropic quadrupolar splittings. Such cases occur frequently, and it is important to know how to analyze and characterize them. Deﬁning the NMR Shift In general terms, the NMR shift is a measure of how the magnetic induction B diﬀers at a nuclear site in a metallic specimen from its value in free space when the sample is removed. In practice, shifts are referred to bare values of the nuclear gyromagnetic ratio γ, where γ is the ratio γ=

μ I

(2.1.8)

of the nuclear magnetic moment μ to its angular momentum I. “Bare” values of γ are measured in compounds or other environments which are as magnetically neutral as possible. For nuclei of elements which are highly active magnetically, deﬁning γ can be diﬃcult and somewhat arbitrary. On the other hand, even compounds lacking a form of paramagnetism almost always have so-called chemical shifts, which are typically of the order of tens or hundreds of ppm. Such shifts are orbital in origin and have been discussed in detail in [2], Chap. 4. NMR shifts in metals are typically two orders of magnitude larger than chemical shifts, so that the latter are often ignored. In high-Tc compounds, however, we shall see that, e.g. for 17 O and 89 Y , chemical shifts will play a role in the discussion. In d-band metals, however, the NMR shift is dominated by

22

2 Introduction to NMR Studies of Metals and Superconductors

the spin-paramagnetic and Van Vleck terms mentioned earlier. In Sect. 1.2 we discuss a detailed formulation of these eﬀects as well as methods for analyzing NMR shift data. Here we focus on deﬁning and measuring the shift tensor. Given a suitable reference γ, then, the NMR shift K is deﬁned with respect to a change in the resonant frequency νres = γH(1 + K), or K =

νres − 1. γH

(2.1.9)

Since a lot of NMR spectroscopy is done by scanning the magnetic ﬁeld, it is important to note that the fractional shift in the resonant ﬁeld, which is −K/(1 + K), not only has the opposite sign, but a palpably diﬀerent magnitude than K if the shift is large. The unmistakable hallmark of an NMR frequency shift or of a spectrum of shifts for a powder is that they scale precisely with the applied ﬁeld. If this is not the case, then one is dealing with quadrupole eﬀects or other complications. The NMR Shift: Tensor or Scalar? In practice, most shifts are characterized as scalar parameters. However, formally the NMR frequency shift tensor Kαβ is deﬁned to be the α component of the internal ﬁeld at the nuclear spin divided by the β component of the applied ﬁeld ([1], Ch. VI). In general, then, the induced, internal shift ﬁeld is not parallel to the external ﬁeld. This can be a complication in the interpretation of large shift eﬀects. However, in cases where the shift anisotropy is 1% or less, it is a good approximation to replace the shift tensor with a scalar shift given by K(θ, φ) = KX sin2 θ cos2 φ + KY sin2 θsin2 φ + KZ cos2 θ, where the KX,Y,Z are the principal values of the shift tensor and (θ, φ) give the orientation of the ﬁeld H in the principal axis coordinates. Another approach, which involves no approximation, is to conﬁne shift measurements on oriented powder or single crystal samples to ﬁeld orientations along the principal axes. The (X,Y,Z) axes will generally coincide with crystalline axes of symmetry. In metals with cubic crystal structure or with single crystals, then, shift measurements are usually straightforward. If microscopic disorder is reasonably low, then line-broadening eﬀects will be 0.01% or less and a 1% shift can be reliably measured to good accuracy. If the nuclear site is non-cubic, however, there is the possibility of an anisotropic shift as well as the virtual certainty of quadrupolar shifts and broadening for I > 12 . For such cases it is very helpful to have either single crystals or oriented powders for non-cubic systems4 . Otherwise, data will have to be obtained by analyzing powder patterns, i.e. broadened spectra which result from a sample made up of randomly 4

Oriented powder samples are samples with anisotropic susceptibilities which have been induced to form partially-to-fully ordered dominant magnetic axes in a magnetic ﬁeld. This technique was of great importance for NMR and susceptibility studies of high-Tc materials. See Sect. 3.1 for a more extensive discussion.

2.1 Basic NMR Phenomenology

23

oriented particles. The functional form of the axial shift powder pattern is the same as for the ﬁrst-order quadrupolar satellite pattern (2.1.5), namely, 1

ρK (K) = [6Kax (K − Kiso + Kax /2)]− 2 ,

(2.1.10)

where K is the shift variable, which is distributed over the range Kiso - Kax /2 ≤ K ≤ Kiso + Kax . For a crystal with applied ﬁeld at an angle θ with respect to the axis of symmetry, the shift may be written Kiso + Kax (3cos2 θ − 1)/2, where Kiso and Kax are the isotropic and axial components of shift, respectively. If the three principal shift values are all diﬀerent, then the symmetry is lower than axial and the singularity disappears. The distribution will have edges at the maximum and minimum shift values, with a peak at the intermediate principal shift value. It is possible, although it may be somewhat laborious, to extract anisotropic shift as well as quadrupole frequency parameters from powder patterns. For the (- 12 ↔ 12 ) transition the change of these two eﬀects with ﬁeld are opposite, so that ﬁeld dependence can be employed to determine their separate values. An example of this is shown in Fig. 2.4 axial shift powder patterns. 2.1.5 Deﬁnition and Interpretation of NMR parameters: T1 T1 is the time constant which describes the exchange of nuclear spin energy with the surrounding lattice, hence it is known as the spin-lattice relaxation time. Referring to the energy levels in Fig. 2.1, T1 determines the rates at which nuclei make transitions between these levels. Magnetic T1 processes are generated by ﬂuctuating HF ﬁelds. Each magnetic HF interaction5 has a ﬂuctuation spectrum with an amplitude and an autocorrelation time. The corresponding T1 process is driven by the fourier component of the latter spectrum at NMR/NQR resonance frequency. The magnetic dipole T1 processes are divided broadly into those driven by spin and orbital HF ﬁelds. The formulation of the various relaxation processes for metallic systems including superconductors has been a major work in progress since NMR was ﬁrst discovered. Below we review the interpretation of T1 eﬀects for simple metals and Type I superconductors (Sect. 2.2) and for d-band metals and Type-II superconductors (Sect. 2.3). The interpretation of T1 processes for the cuprate superconductors will be discussed extensively in Chaps. 3–6. Particularly important is the role played by electron-electron interactions in T1 phenomena. Accordingly, we review Moriya’s theory of correlated electron eﬀects in the T1 processes of simple metals in Sect. 2.2. Rather more rare in occurrence are quadrupolar T1 processes generated by ﬂuctuating components of EFG. A general theory of such eﬀects caused by the phonon Raman scattering process was put forward by Van Kranendonk in the early days of NMR [14]. Such processes are extraordinarily weak, however, 5

See Sect. 2.2 for a comprehensive deﬁnition of the magnetic HF interactions.

24

2 Introduction to NMR Studies of Metals and Superconductors 2nd Order Quadrupole + Anisotropic Shift A = 1/2, B = 2

A = 2/3, B = 3/2

A=B=1

A = 2, B = 1/2 –4

–2

0

2

4

Fig. 2.4. Powder patterns are shown for several cases the combined eﬀects of an anisotropic shift and second-order quadrupolar broadening. The total broadening perturbation is A sin2 θ (9 cos2 θ − 1) + B (3cos2 θ − 1). In applied ﬁeld H, A ∝ 1/H and B ∝ H. In reduced units we let B = H, and the frequency displacement is in 2 /16νL (for I = 3/2). The spectra then show a progression of powder units of 3νQ patterns as H is varied from 1/2 up to 2. The dashed vertical lines show the positions of the three edges in the absence of broadening. The prominent upper singularity (see Fig. 2.2) converges with the θ = 0 edge with increasing ﬁeld and disappears above B/A = 8/3. However, there is still a visible maximum for the top example, where B/A = 4. Note that these spectra are actually oriented the way they would appear in a ﬁeld sweep increasing to the right, and, therefore, the anisotropic shift coeﬃcient is negative. With B/A < 0, the patterns would be quite diﬀerent. Studies such as are shown here allow the practitioner to extract values of A and B from experimental data

and have rarely been identiﬁed in metals. Nonetheless quadrupolar relaxation processes for the 63,65 Cu isotopes have occasionally been claimed to exist in solids, using the isotopic ratio of T1 values as a diagnostic.6 When quadrupolar T1 eﬀects occur in metals, it is our conjecture that they are much more likely to be caused by ionic motion (e.g. diﬀusion) than by phonons. The Magnetic Dipole Relaxation Process Nuclear spin transitions generated by the HF interactions in (2.2.1) are known as magnetic dipole transitions (as opposed to electric quadrupolar transitions). Here, we analyze the magnetic dipole T1 process in some detail. We review methods to measure it as well as certain pitfalls to be avoided in conducting 6

The ratio 63 T1 /65 T1 is a good diagnostic for this purpose, since it is (γ65 /γ63 )2 = 1.148 for magnetic relaxation and is (Q65 /Q63 )2 = 0.854 for electric quadrupolar relaxation.

2.1 Basic NMR Phenomenology

25

such measurements. Whether measuring T1 with high-ﬁeld NMR or in zero ﬁeld with NQR, the nuclear spin energy levels Em will be labeled with the Iz quantum number m. To the extent that m is a good quantum number, the transition rate between states m and m may be written | m |I+ |m|2 W = | m|I− |m |2 W = (I − m)(I + m + 1)W δm ,m+1 (2.1.11) If I = 12 , then there is only a single rate W involved. For I > 12 there are I + 12 rate constants and 2I relaxation eigenmodes. The formula (2.1.11) will be correct for the cases (a) when I = 12 , (b) for arbitrary values of I when η = 0 and the ﬁeld is applied along the principal axis of the EFG tensor, and (c) for NQR when η = 0. It is approximately correct for arbitrary η values when νQ γH/2π and for NQR when η is small. In other cases m-state mixing eﬀects become important and it may be necessary to solve the spin Hamiltonian (2.1.1) numerically to obtain accurate matrix elements of I± . In this discussion of T1 analysis, we shall assume (2.1.11) to be valid, and we shall also neglect nuclear quadrupole relaxation eﬀects. They are, as noted above, quite rare in metallic systems. Detailed Balance in T1 Processes T1 in metals is simpliﬁed by the fact that ﬂuctuation spectra for itinerant fermions are constant over the range of typical NMR frequencies. T1 values are therefore found to be independent of the Zeeman splitting and are the same for NMR and NQR measurements alike.7 We shall assume, further, that the lattice constitutes an inﬁnite heat reservoir at equilibrium at temperature T . To illustrate the incorporation of detailed balance into the rate equations, we analyze a two-level system with energies E2 > E1 , deﬁning ΔE = E2 E1 . The populations of these levels are designated p1,2 and will be treated as continuous variables. The rates at which up and down transitions occur are deﬁned to be W21 (up) and W12 (down), respectively. At thermal equilibrium the principle of detailed balance gives W21 = e−βΔE W12 ([2], Ch.5). The rate equations for populations are then dp1,2 = ±[p2 W12 − p1 W21 ] , dt

(2.1.12)

where p1 + p2 = N is the total number of nuclei in the ensemble. When the p1,2 are at equilibrium we have dp1,2 /dt = 0, giving p2 /p1 = W21 /W12 = e−βΔE . Thus, the Boltzmann distribution of spin populations follows from detailed balance. Writing p1,2 = ± 21 (p2 − p1 ) + N/2, the (2.1.12) may be combined to give 7

Note, however, that NMR and NQR reﬂect diﬀerent relaxation modes, as will be seen below. For example, if I = 32 , for NMR 1/T1 = 2W , whereas the single rate measured with NQR is 6W , or one-third the length of the conventionally deﬁned T1 .

26

2 Introduction to NMR Studies of Metals and Superconductors

d(p2 − p1 )/dt = (p2 − p1 )(W12 + W21 ) − N (W12 − W21 ). From this relation we see that the relaxation rate of (p2 − p1 ) is (W12 + W21 ). Since this quantity must be independent of ΔE, we set (W12 + W21 ) = 2W , where W is a rate constant which depends only on T . Detailed balance then leads immediately to W12 =

2W 2W e−βΔE ; W . = 21 (1 + e−βΔE ) (1 + e−βΔE )

Using (2.1.13), (2.1.12) then becomes dp1,2 N e−βE1,2 = −2W p1,2 − −βEi . dt ie

(2.1.13)

(2.1.14)

Even though p1 and p2 appear to act independently, they are not, of course, independent. The general solution to (2.1.14) is seen to be p1,2 (t) = (p1,2 (0) − p01,02 )e−2W t + p01,02 , (2.1.15) where p01,02 = N exp (−βE1,2 )/ i exp (−βEi ) are the equilibrium population values. This result also satisﬁes p1 (t) + p2 (t) = N if p1 (0) + p2 (0) = N , which must be the case. Relaxation Equations for I >

1 2

Generalization of the foregoing result to multi-level nuclear relaxation equations is straightforward. They can always be written in terms of the diﬀerence variables dm = pm – p0m , with p0m = N exp(−βEm )/

exp(−βEm ),

(2.1.16)

m

where m is the quantum number for the energy eigenvalues. We note that the value of p0m does not depend on the choice of the zero-point of energy. In general, then, one can measure T1 by creating a non-equilibrium population distribution, then observing the decay toward equilibrium of the population diﬀerence of some suitable pair of levels using spin-echo excitation. The latter pair must be chosen to have |Δm| = 1 for magnetic excitation, and they must be chosen to reﬂect a non-equilibrium population diﬀerence during the equilibration process. If the initial non-equilibrium condition is created by applying an rf pulse to some pair of levels, note that the recovery can often be observed using spin-echo signals from a diﬀerent pair of levels.8 This degree of experimental freedom is not often used in NMR. It could be used, for example, to avoid multiple echo eﬀects in a T1 measurement when T1 is very short. 8

This requires the ability to be able to apply rf pulses to the sample at two separate frequencies, which can be a very useful adjunct to the usual spectrometer setup.

2.1 Basic NMR Phenomenology

Relaxation Eigenmodes for I >

27

1 2

For multi-level nuclear spin Hamiltonians (I > 12 )9 there is an eigenmode structure to the relaxation equations with multiple relaxation eigenrates. We illustrate this situation with the simple example of I = 32 , for which there are four energy levels as shown in Fig. 2.1. The dynamical equations for the diﬀerences dm are then dd3/2 dt dd1/2 dt dd−1/2 dt dd−3/2 dt

= −3W d3/2 + 3W d1/2

(2.1.17a)

= 3W d3/2 – 7W d1/2

(2.1.17b)

= 4W d1/2 – 7W d−1/2 + 3W d−3/2

(2.1.17c)

= 3W d−1/2 – 3W d−3/2

(2.1.17d)

We seek solutions of the form dm = cm exp(−λW t). Substitution into (2.1.17) then yields the matrix equation ⎧ ⎫ ⎫ ⎡ ⎤ ⎧ 0⎪ λ−3 3 0 0 c3/2 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎨ ⎪ ⎬ ⎬ ⎨ ⎢ 3 λ−7 4 0 c1/2 0 ⎥ ⎢ ⎥ ⎣ 0 0⎪ c 4 λ−7 3 ⎦ ⎪ ⎪ = ⎪ ⎪ ⎪ ⎩ ⎪ ⎭ ⎭ ⎩ −1/2 ⎪ 0 c−3/2 0 0 3 λ−3 This matrix is solved straightforwardly. The characteristic equation is λ4 –20λ3 + 108λ2 –144λ = 0 ,

(2.1.18)

for which the solutions are λ = (0, 2, 6, 12). The corresponding decay rates are 0, 2W = T1−1 , 6W = 3T1−1 , and 12W = 6T1−1. Ignoring the null mode, the corresponding eigenvectors for T1 , T1 /3, and T1 /6 may be written {3, 1, -1, -3}, {-1, 1, 1 ,-1}, and {-1/3, 1, -1, 1/3}, respectively. The solutions to (2.1.17) may be applied to diﬀerent techniques for measuring T1 . We illustrate their use in the simple case of a cubic environment where Em = −γn (1 + K)Hm. Since |Em | kB T , we may write (2.1.16) N p0m ≈ 2I+1 (1 − δm), where δ = γn H(1 + K)β. Then if we apply an rf pulse with pulse angle θ to the spins, the resulting initial condition is pm (0) ≈

N (1 − δ cos θ m). 2I + 1

N As a result, the initial values are dm (0) ≈ 2I+1 (1 − cosθ) m. The dm (0) have the form {3, 1, -1, -3} of the “T1 ” mode, so that the solution can be written 9

This discussion only applies to nuclei with odd half-integer spin quantum numbers. Many nuclei of interest answer to this description, and, in fact, there will be no nuclear spins of interest in this volume which have integer values of I.

28

2 Introduction to NMR Studies of Metals and Superconductors

dm (t) ≈

N mδ (1 − cos θ) e−t/T1 . 2I + 1

If θ = π, then one has a perfect inversion, which gives the largest excursion in signal amplitude. The time variation of the spin echo signal for arbitrary θ is then proportional to pm (t) − pm+1 (t) =

Nδ [1 − (1 − cos θ) e−t/T1 ]. 2I + 1

(2.1.19)

If pm (0) = pm+1 (0) for all applicable m, then we have a condition known as saturation, which also yields a single-exponential recovery ∝ (1−exp(−t/T1 )), regardless of the distribution of the energies Em . Recovery Mode when only the (− 12 ↔ 12 ) Transition is Excited If there are quadrupolar splittings, then a single pulse applied to the (-1/2 ↔ 1/2) transition results in a {dm (0)} vector with the form a0 {0, 1, −1, 0}. Writing the decay mode as a superposition of the foregoing eigenmodes, we have {dm (t)} =

1 a0 [{3, 1, −1, −3} exp−t/T1 +9{−1/3, 1, −1, 1/3} exp−6t/T1 ]. 10

The spin echo signal for the (-1/2 ↔ 1/2) transition will therefore exhibit the well-known decay function E(t) = E0 (0.9 exp−6t/T1 + 0.1 exp−t/T1 ) .

(2.1.20)

Such a precise mathematical form occurs only for excitation of a single pair of levels over a time interval which is short compared with T1 /6. If relaxation begins to take place during the initial excitation phase, then the simple form of the initial condition is lost and the decay will be rather more complicated. In the foregoing example, d3/2 (t) would be proportional to (exp −t/T1 - exp −6t/T1), so that it would deviate very quickly from its initial value of zero. As we noted earlier, the relaxation measurement could be conducted in this fashion, i.e. by monitoring a diﬀerent transition frequency from the one used for the initial excitation. The NQR Case Continuing our discussion of an I = 32 nucleus, we consider ﬁnally the NQR case, where the ± 12 levels and the ± 32 levels are degenerate pairs separated by an energy diﬀerence of hνN QR = hνQ (1 + η 2 /3)1/2 . A single excitation pulse at the NQR frequency then creates an initial condition given by {dm } = a0 {-1, 1, 1, -1}. This eﬀectively 2-level system relaxes entirely via the symmetric mode with a single decay rate 3/T1 . One must be careful to take account of the relaxation mode eﬀects when comparing T1 data obtained with diﬀerent methods.

2.1 Basic NMR Phenomenology

29

We make a few additional remarks about the decay mode eﬀects described above for the I = 32 system. First, there are many nominally cubic systems where the observed signal is dominated by the (-1/2 ↔ 1/2) transition, because transitions to higher m-values are broadened by stray ﬁrstorder quadrupolar splittings. Such splittings are the consequence of impurities and other forms of crystalline disorder. If such broadening is severe, magnetization recovery may take place via (2.1.5) rather than with the expected single-exponential T1 decay. Since there is a dramatic diﬀerence between these two cases, it is very important to be aware of such broadening eﬀects. A second point we wish to emphasize is that the analysis of T1 relaxation curves given here for I = 32 is entirely independent of the nature of the NMR spectrum. The functional behavior depends only on which pair of levels is used to excite a non-equilibrium initial condition, and on the fact that the quantum numbers m = Iz are relatively pure in characterizing the energy eigenstates. If the latter condition is not fulﬁlled, then numerically evaluated eigenfunctions may be needed to generate suﬃciently accurate relaxation curves. Measuring T1 in the Presence of Spectral Diﬀusion We consider brieﬂy some well-known problems encountered in T1 measurements. Two of the most troublesome are the related problems of inhomogeneous broadening and spectral diﬀusion. These problems occur frequently in d-band metals and intermetallic compounds. The key to accurate T1 measurements is the experimenter s ability to create a strongly non-equilibrium population diﬀerence between a pair of nuclear energy levels as an initial condition. The T1 recovery will then be accompanied by a spin-echo signal which undergoes a substantial change in amplitude. In cases of severe inhomogeneous broadening such as that shown in Fig. 2.5, a diﬃculty arises from the fact that a single pulse of rf ﬁeld will only aﬀect a region of width γH1 , where H1 is the amplitude of the rf pulse ﬁeld. The narrow region saturated by a single pulse is shown as a dotted line in Fig. 2.5(a). If the broadening is entirely static, it may be possible to focus the measurement on the polarization behavior at precisely the irradiation frequency, i.e. the center frequency of the population disturbance shown in the ﬁgure. As noted in Sect. 1.2.2, this can be done by carefully integrating the entire area under the spin echo, so that the measured recovery curve will accurately reﬂect what is taking place at ω = ωrf . However, such broadening may actually have a partially dynamical character owing to the presence of spin-spin couplings of the form Hﬀ = BIi± Ij∓

(2.1.21)

between neighboring nuclei. Under circumstances which occur frequently, the Hﬀ interactions lead to ﬂip–ﬂop dynamical processes between neighboring spins, which then leads to a rapid smearing of the band of excited spins

30

2 Introduction to NMR Studies of Metals and Superconductors

Polarization (Arbitrary Units)

1.2

(a)

1 0.8 0.6 0.4 0.2 0

0

200

400

600

Frequency (Arbitrary Units)

Polarization (Arbitrary Units)

1.2

(b)

1 0.8 0.6 0.4 0.2 0

0

200

400

600

Frequency (Arbitrary Units)

Fig. 2.5. (a) The saturation eﬀect of a π/2 pulse applied at frequency ω0 is shown for an eﬀective pulse ﬁeld amplitude of 20 in units of the frequency scale. The polarization curve is also shown at several later times as T1 recovery takes place without spectral diﬀusion. (b) Development with time of the polarization curve is shown at several stages following the same initial saturation pulse as in (a). The curves are a Gaussian model in which there is no T1 recovery eﬀect, thus the total polarization, plus its ﬁrst moment (ω − ω0 )P (ω)dω, are conserved over the time interval shown. Note the spurious “recovery” of the polarization at frequency ω0 as a function of time

over a much wider range of frequencies than those excited directly by the rf pulse(s). This process, known as spectral diﬀusion, is illustrated with dashed lines in Fig. 2.5b. There results what appears to be a rapid recovery of the polarization at the excitation frequency. However, such a recovery has nothing to do with the T1 process, but is easily mistaken for it. Often it is much faster than T1 , and results in the experimenter’s inability to achieve inversion of the

2.1 Basic NMR Phenomenology

31

polarization10 . This highly undesirable eﬀect has been known in adverse cases to render T1 measurements unfeasible. We consider here the circumstances which give rise to spectral diﬀusion eﬀects and oﬀer a few suggestions on how to deal with this problem. The ﬂip– ﬂop process (m, m ) → (m ± 1, m ∓ 1) between (primarily) nearest-neighbor (nn) spins has been recognized since the early days of NMR as essential for spin diﬀusion, as well as for maintaining thermal equilibrium within the nuclear spin system. Spectral diﬀusion is, in fact, a process whereby a disturbance in a narrow frequency range is able to diﬀuse over the entire NMR line so as to create a uniform spin temperature. However, since an energy-conserving ﬂip–ﬂop transition can only take place between neighbors with nominally the same Larmor frequency, i.e. the same shift value, it is interesting to consider how polarization can migrate over large frequency intervals such as depicted in Fig. 2.5b. With coupling energy of the form of (2.1.21), it is plausible that a ﬂip–ﬂop transition could take place between neighboring spins with a Zeeman frequency mismatch of the order of Δω ∼ B and still conserve energy. The diﬀerence in Zeeman energies is taken up by the transverse terms and eventually dissipated by other ﬂip-ﬂop processes. Over a large number of such ﬂuctuations, the narrow polarization disturbance created by an rf pulse could broaden symmetrically over frequencies well beyond the conﬁnes of the initial excitation proﬁle. To have this happen, of course, the inhomogeneous broadening must be local in character and be otherwise conﬁgured to facilitate the process. One method for measuring T1 under these circumstances is to endeavor to saturate the entire line with a string of pulses known as a comb instead of a single pulse. Were this possible, then all polarization variables would relax back to equilibrium with the single time constant T1 . If pulses at a single frequency do not produce the desired saturation eﬀect, then applying frequency modulation to cover the entire resonance line is known to be eﬀective11 . At low temperatures, however, long strings of pulses may produce undesirable heating eﬀects. If T1 is long enough, another more exotic (but widely used) method is to use ﬁeld switching to create a non-equilibrium initial condition for the T1 measurement. The ﬁeld at the sample can be switched mechanically or electronically. The most obdurate cases occur when T1 is too short, even at low temperatures, for ﬁeld switching, and pulse combs are also not feasible. Ones only option may to be hope that spectral diﬀusion will run its course in a time less than T1 , and that the ﬁnal stage of the polarization recovery process can be analyzed to extract the T1 rate. Needless to say, such an approach also has limited applicability. 10

11

Inability to invert polarization can result from fast spectral diﬀusion, but it is also caused by an inhomogeneous rf ﬁeld H1 so that the pulse condition varies over the sample volume. The author is indebted to W.G. Clark for this observation.

32

2 Introduction to NMR Studies of Metals and Superconductors

2.2 NMR Probe of sp-Band Metals and Type I Superconductors In order to put high-Tc materials into context, this section gives as background material a brief summary of the basic static and dynamic magnetism of “simple” metals as sensed by the NMR probe. These systems give a historical perspective of the subject and provide foundation for the treatment of the more complex d-electron metals. In typical good metals we think about electrons as itinerant fermions which occupy Bloch wavefunctions uk (r)eik·r . Such orbitals are often far removed in character from the atomic states they are actually composed of. Calculations of NMR shift, relaxation, and indirect spin-spin couplings in metals were originally formulated in this bandtheoretical language. The s-character of band electrons is always present and often plays a major role. In contrast, high-Tc systems are bad metals, often with just enough mobile carriers to render the d-holes on the Cu2+ sites itinerant. Some properties remain atomic-like in character and can be thought of usefully in terms of localized wavefunctions. Perhaps by accident, there is very little s-character in the wavefunctions of most high-Tc ions, allowing the less familiar p and d orbitals to dominate. In this section we review the energy-band, k-space picture used to describe the static and dynamic magnetism sensed by the NMR probe in both the normal (nonsuperconducting) and superconducting (SC) states. We begin the discussion with the idealized Korringa treatment of NMR shifts and relaxation, then discuss important modiﬁcations of this picture for actual sp-band metals. Historically, the ﬁrst NMR studies of superconductivity were done on this class of materials. We review problems encountered in reconciling both the shift and relaxation behavior with the BCS theory [15] for these systems. It was with the elemental metals Hg, Sn, Pb, and Al that questions such as the role played by spin-orbit coupling in the behavior of the spin susceptibility and corresponding NMR (Knight) shift ﬁrst came to light. They also gave us our ﬁrst clear understanding of the BCS coherence peak in the T1 rate [16]. Since even before the BCS theory of superconductivity[15] was announced, NMR shifts have been employed to investigate the nature of the superconducting state. In the early days the only known metallic NMR shift was the s-contact Knight shift. Moreover, the original BCS ground state was an eigenfunction of Sz , leading to the naive expectation that K(T ) ∝ χspin (T ). The actual reality was rather more complex. This interesting piece of NMR history will be touched upon in Sect. 2.2. Measurement of such eﬀects has become a standard application for NMR studies. Observation of shift behavior is also very important in the study of high-Tc systems and for any of the latter-day unconventional superconductors.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

33

2.2.1 NMR Shifts and Relaxation in Simple Pauli Paramagnets Following on the discovery of the s-contact NMR shift by Knight [17], one of the ﬁrst theoretical milestones for the NMR study of metals was the Korringa relation between the latter shift and the product T1 T , which was also shown to be independent of temperature [18]. These results were expected to apply to cubic sp-band metals, where it is noteworthy that the p-electrons with their far smaller HF couplings have a nearly negligible eﬀect on both the NMR shift and T1 . The surprise of substantial deviations from the Korringa relation for simple systems such as the alkali metals were therefore a stimulus for Moriya’s treatment of electron-electron interactions in these systems. The result was important modiﬁcations to the Korringa relation, which were then veriﬁed experimentally. This was an important step in the treatment and understanding of electron interactions in metals. We review these developments in the following subsections. The Comprehensive HF Coupling Hamiltonian in Solids As a preliminary step we introduce here the comprehensive HF Hamiltonian l s 3r(s · r) 8 πsδ(r) , (2.2.1) + HHF = 2γμB I · 3 − 3 + r r r5 3 where γI is the nuclear moment located at r = 0 and l and s are the orbital and spin angular momentum operators, respectively, of an itinerant fermion located at r (see [1], Ch. VI). (2.2.1) can be written −γI · He , where He is an eﬀective HF-ﬁeld operator which is the ultimate source of all magnetic shift and relaxation eﬀects in the metallic environment. There are three distinct types of interactions, namely the orbital ﬁeld, the dipolar ﬁeld, and the s-contact interaction. Although it took a number of years for them to emerge, calculations for the metallic shifts listed above were all ultimately based on (2.2.1). Evaluating the thermally averaged eﬀects of He in metallic systems is a matter of great subtlety and complexity. In a very real sense, this is the essence of the high-Tc problem for the NMR probe. The Knight Shift: S-contact HF Coupling in an sp-band Metal The so-called s-contact HF ﬁeld and its corresponding NMR shift in copper metal were discovered by W. D. Knight [17]. This shift is simply given by the expectation value of the ﬁnal term of (2.2.1) when spin polarization from an external ﬁeld H is present. There results a temperature-independent NMR shift given by (2.2.2) Ks = αs χsp , 2 where αs = 8π 3 |uk (0)| , indicating an average over the Fermi surface. χsp = 12 (gμB )2 n(EF ) is the spin susceptibility of the sp band, where n(EF ) is the

34

2 Introduction to NMR Studies of Metals and Superconductors

Fermi surface density of states per atom for one direction of spin12 . We also note that the dipolar HF coupling, i.e. the second and third terms of (2.2.1), also yields a palpable NMR shift in many cases. It vanishes at sites having cubic symmetry, and is, in any case, an order of magnitude or so smaller than the contact shift. In high-Tc materials, where contact shifts are often absent, the dipolar terms take on a much greater signiﬁcance than for cubic metals. Interestingly for the case of copper metal, it later developed that some 40% of the orbital character of the Fermi surface is d-like [19]. As a result, a signiﬁcant fraction of the observed Knight shift for copper is attributable to the orbital Van Vleck term discussed in the next subsection [20]. The Korringa Calculation of T1 The idealized viewpoint regarding a simple metal is epitomized by the seminal calculation of NMR shift and relaxation time by Korringa [18]. In this case, noninteracting electrons were assumed, with a density of states at the Fermi surface describable by band theory. HF interactions with the relevant nuclear spins were limited, not unreasonably, to the s-contact interaction (2.2.1), the p-electron dipolar coupling being negligibly weak in comparison. Cubic symmetry allowed quadrupolar eﬀects and p-electron contributions to the NMR shift to be ignored, and any gradient to the density of states deemed too small to alter low–temperature behavior. The shift expression is given above in (2.2.2). Next, we need to develop an expression for T1 at the same level of approximation. We use the basic golden rule expression from time-dependent perturbation theory, where the perturbing interaction is the s-contact term 2 from (2.2.1), Hsc = − 8π 3 γn γe δ(r)I · s. If we consider the elemental transition from state |k ↑ m to state |k ↓ m + 1, where m is the initial nuclear spin quantum number, the rate for such a transition may be written [2] Wk ↓m+1,k↑m =

2π | k ↑ m + 1|Hsc |k ↓ m|2 δ(Ek − Ek ).

(2.2.3)

To complete the calculation this transition rate must be summed over initial electron states |k ↑ which are occupied and ﬁnal states |k ↓ which are unoccupied. The operative term in Hsc is the one ∝ I+ S− , whereupon the squared matrix element becomes 2 4π 2 γn γe |uk (0)uk (0)| (I − m)(I + m + 1). | k ↑ m|Hsc |k ↓ m + 1| = 3 (2.2.4) The principal approximation is to assume that all states in the vicinity of the Fermi surface have approximately the same probability density at the

12

2

In discussions of experimental susceptibilities, it will be more convenient to use molar units, whereupon the shift coeﬃcient αs will be written 8π|uk (0)|2 /3NA , where NA is Avogadro’s number.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

35

nucleus. Thus, we may replace the quantity |uk (0)uk (0)|2 with the squared Fermi surface average |uk (0)|2 2 . Introducing the restricted sums on k and k and noting further that 1/T1 is twice the coeﬃcient of (I − m)(I + m + 1) (see (1.10) 13 ), this gives 1/T1 =

2 (r) 4π 4π γn γe 2 |uk (0)|2 δ(Ek − Ek ). 3

(2.2.5)

k,k

(r) The restricted sums k,k can be replaced with energy integrals where, for example, the sum on k of states with energy E becomes n(E)dE, where n(E) is the density of states, and the occupation restriction is enforced with the Fermi occupation function f (E) = [exp β(E − EF ) + 1]−1 . The summation in (2.2.5) then becomes dE dE n(E)n(E )f (E)(1−f (E ))δ(E−E ) = n(E)2 f (E)(1−f (E)) dE. (2.2.6) The ﬁnal step is to note that the function f (E)(1 − f (E)) is very sharply peaked at EF at the usual experimental temperatures, so that n(E)2 can be replaced with n(EF )2 . Then we note that the area under the peak in f (E)(1 − f (E)) is easily shown to be kB T . The relaxation rate becomes 1/T1 =

4πkB T

2 4π γn γe 2 |uk (0)|2 n(EF )2 . 3

(2.2.7)

This expression may be combined with the result in (2.2.2) to give the Korringa product, which we write as 1 4πkB γn2 = . T1 T Ks2 γe2

(2.2.8)

Equation (2.2.8) suggests that 1/T1 T divided by Ks2 for these kinds of metals should equal an expression made up of physical constants which is independent of the other properties of the metal. As we shall see below, the result of Moriya’s theory is to multiply the right-hand side of (2.2.8) by a constant factor < 1. Setting that aside for the moment, however, let us see how well the Korringa relation is obeyed in simple metals. In Table 2.1 shift and relaxation data from the literature are listed for the alkali metals and the noble metals Cu, Ag, and Au [3]. These elemental metals all have cubic crystal structures, so that dipolar shift eﬀects do not come into play. Using the measured shift values, values of T1 T extracted from (2.2.8) are compared with experimental values. It is seen that the latter values are generally smaller than those obtained from 13

For simplicity, detailed balance considerations are omitted here.

36

2 Introduction to NMR Studies of Metals and Superconductors

Table 2.1. NMR shift and relaxation data are tabulated for alkali metals and for the noble metals, along with values of T1 T derived from (2.2.8). To test the validity of the Korringa relation, a relative Korringa product deﬁned as (T1 T Ks2 )−1 divided by 4πkB γn2 /γe2 is listed in column ﬁve Metal and Isotope 7

Li Na 85 Rb 133 Cs 63 Cu 109 Ag 197 Au 23

Ks (%)

T1 T(expt.) (secK)

0.0263 0.112 0.650 1.47 0.232 0.522 1.4

45.0 4.8 0.81 0.13 0.9 9.0 4.0

± ± ± ± ± ± ±

2 0.1 0.08 0.01 0.2 1.0 0.5

T1 T(Korringa) (secK)

Relative Korr.Prod.

26.0 3.1 0.63 0.069 0.7 4.5 4.5

0.58 0.65 0.78 0.53 0.78 0.50 1.13

(2.2.8). Including p-electron dipolar hyperﬁne ﬁelds in the relaxation calculation would only make this discrepancy larger. Thus, the most serious defect in the Korringa treatment appears to be the neglect of electron-electron exchange enhancement eﬀects, which we shall discuss next. 2.2.2 The Moriya Theory of Exchange Enhancement in Simple Metals There are various corrections one could make to the Korringa treatment of relaxation. The electron-electron interaction potential has the eﬀect of enhancing the spin susceptibility, and thus the NMR shift [21], in close analogy with the enhancement eﬀect of ferromagnetic exchange among localized moments. However, it was pointed out by Moriya [22] that exchange ﬂuctuations would also enhance the T1 process. Moriya’s calculation of this eﬀect in the random phase approximation showed this enhancement eﬀect to be substantial, but not as great as that of the shift and susceptibility. This is consistent with the values shown in Table 2.1, where the experimental Korringa product (Relative Korr. Prod.) is consistently smaller than the result in (2.2.8). Thus, the measured Korringa products can be used with the Moriya theory (see below) to estimate the magnitude of these enhancement eﬀects. We give an outline of the random-phase approximation calculation here, and refer the interested reader to [22] and [3] for a more detailed account. As noted above, the shift has a simple exchange-enhancement factor, Ks = Ks0 /(1 − α) = αs χs0 /(1 − α), where α = ρ0 χs0 , and ρ0 = 2πζ/2 γe2 . Finally, ζ is the q-independent (by assumption) electron-electron interaction potential. The single parameter ζ drives the enhancement of both static and dynamic spin susceptibilities in the random phase approximation picture. For T1 the ﬂuctuation enhancement is q-dependent. In Sect. 3.5 these magnetic properties will be discussed in terms of q and ω–dependent susceptibilities. Here, we simply state the result for a spherical Fermi surface:

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

1 4πkB γn2 = K(α), 2 T1 T Ks γe2

37

(2.2.9)

1 where K(α) = 2(1 − α)2 0 dx x/[1 − αG(x)]2 , and G(x) is the Lindhard function for free electrons given by 12 {1 + [(1 − x2 )/2x]ln|(1 + x)/(1 − x)|}, with x = q/2kF . G(x) is integrated over the range of q values which span the Fermi surface. We see in (2.2.9) that the Korringa product of (2.2.8) is simply multiplied by the quantity K(α). The enhancement factor for Ks is that for q = 0 (G(0) = 1), while that for 1/T1 is for G(q > 0) < 1. Therefore, K(α) declines from 1 to 0 as α varies from 0 to 114 . If other eﬀects which modify the Korringa product are largely absent15 , the experimental value of K(α) can be used to estimate the electron-electron exchange (i.e. the value of α) in sp-band metals. A few examples are given in Table 2.2, where α values in the range of 0.2 ≤ α ≤ 0.4 are seen to be typical. Rather surprisingly, susceptibility enhancement eﬀects are present to the degree of 25% to more than 50% in these nearly free-electron metals. The Korringa product is often used as a diagnostic tool to examine the nature of the T1 process. Table 2.2. A tabulation of enhancement parameters α derived for a selection of s-band metals from experimental data using (2.2.9). For comparison, calculated values given by Pines [21] are listed Elemental Metal 7

Li Na 85 Rb 109 Ag 23

14 15

α from K(α)

α calc. (Pines)

0.36 0.30 0.19 0.43

0.37 0.24 0.15 0.32

A plot showing K(α) vs. α is given in [3]. Experimental values of the Korringa product can deviate sharply from that in (2.2.8) for a number of reasons. We give three examples, First, if the s-character of Fermi surface orbitals is unusually weak, then p-electron contributions which have been neglected here may play a large role. Second, if the degree of s-character is strongly non-uniform over the Fermi surface, then one of the principal assumptions of the calculation breaks down. Third, if there are multiple bands or multiple neighbors (in the case of ligand nuclei), the experimental Korringa product will change drastically. For example, if a ligand nucleus has N independent but equivalent sources of HF ﬁeld and ﬂuctuations, then the shift and relaxation rate will both be N times that from a single source. It follows that the Korringa product will be the value from a single source divided by N. The latter case is encountered frequently for ligand nuclei in intermetallic compounds.

38

2 Introduction to NMR Studies of Metals and Superconductors

2.2.3 NMR in the Superconducting State of Simple Metals We present here a brief account of the superconducting properties of sp– band metals. Historically, several fundamental issues were resolved with these systems following initial uncertainties regarding both theory and experiment. A clear and comprehensive review of early work was given by MacLaughlin [5]. Some elemental metals addressed in the early days were Hg(4.15K), βSn(3.74K), Pb(7.22K), and Al(1.18K), where their respective values of Tc are given in parentheses. They are all Type I superconductors, which means that their coherence lengths ξ(0) are long compared with their London penetration depths λ(0)16 . With the announcement of BCS theory [15], there were a number of interesting issues to investigate. The principal ones for the NMR probe were (a) the expected collapse of the spin susceptibility at T < Tc owing to the SC energy gap for quasiparticle excitations and (b) the existence of a singularity, which becomes the coherence peak, just below Tc in a plot of 1/T1 vs. T . Because of the large superconducting diamagnetism which occurs below Tc , virtually the only means of measuring the relatively tiny Pauli susceptibility term is through the associated Knight shift Ks (2.2.2). We shall discuss the superconducting shift measurements ﬁrst. The Knight shift for T < Tc : Verifying the Yosida function Performing NMR measurements in the SC state of Type I superconductors was a particular experimental challenge, because of the limited magnetic ﬁeld penetration depth λ ∼ 500˚ A for these systems. In order to get a reasonably uniform internal ﬁeld for NMR studies, experiments were performed on ﬁne particles or thin ﬁlms with at least one dimension which was small compared with λ. The resulting samples generally exhibited superconductivity with Tc near the bulk value and NMR lines with relatively little diamagnetic shift or inhomogeneous broadening. Particles with dimension d λ have greatly reduced diamagnetism in the SC state. Other than that, it was generally believed that these samples exhibited bulk NMR properties. However, the peculiar results obtained at ﬁrst for K(T ) vs. T for T < Tc demonstrated that the foregoing statements were not entirely correct. To see this clearly, we must ﬁrst describe the results that were expected from the shift measurements, then what was actually found, and ﬁnally, how to account for the observed data. The BCS theory prescribed an energy gap Δ(T ) above the superconducting ground state for quasi-particle excitations when T < Tc . As Δ(T ) increases below Tc the spin susceptibility χsp (T ) and Ks (T ) = αs χsp (T ) were expected to decline and asymptotically approach 0 as T → 0. The theoretical functional form of χsp (T ) for T < Tc is known as the Yosida function [23]. 16

A brief discussion deﬁning the coherence length and penetration depth parameters is given in Sect. 2.2.4.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

39

Experimentally, however, large residual T → 0 shift values were reported. For the 199 Hg NMR in SC Hg, for example, Ks (T → 0)/K(T > Tc ) 2/3 was found [24], with similar results for 119 Sn in βSn [25], 207 P b in P b [26], and 27 Al in Al [27]. These results caused great consternation and confusion, and it was a number of years before a satisfactory understanding was reached [28]. Spin–Orbit Scattering: The Ferrell–Anderson Picture In the end, it was realized that the theoretical preparation was incomplete, and further developments with the Al metal samples showed that the earliest results were incorrect. We shall return to the Al story below. The problem with the Yosida/BCS calculation was that it had neglected spin-orbit coupling and its role in generating spin-ﬂip scattering processes. The situation was eventually addressed and for the most part resolved in short papers by Ferrell [29] and Anderson [30], as well as in a longer paper by Abrikosov and Gorkov [31]. We consider brieﬂy the physical picture presented in Anderson s treatment [30]. In the presence of spin-orbit coupling one must bear in mind that Sz for the electrons is no longer a good quantum number, and that the spin-up and spin-down states are mixed into eigenstates which are no longer have any particular average value of spin. However, a very subtle point is this: In clean, bulk regions of the pure metal there is no spin-ﬂip scattering even in the presence of strong spin-orbit coupling. Thus, the spin susceptibility will still vanish as T → 0 in the SC state. However, what modiﬁes this ideal result is a spin-ﬂip scattering lifetime τso which is short enough that the quantity /Δ(0)τso is no longer small. In other words the smearing of the eigenstate energies from τso becomes comparable with the SC energy gap. Spin-ﬂip scattering occurs only where ordinary potential scattering is strong, e.g. near surfaces and near impurities in the bulk. Ironically, then, this eﬀect will be important near surfaces where rf ﬁelds penetrate and NMR signals are excited, but not necessarily in bulk regions which cannot be probed. Anderson treated the spin-orbit scattering problem using his theory of dirty superconductors[32]. His result for the T → 0 susceptibility ratio is an expression which can be integrated numerically, from which the following limiting cases are given [30]: χso (T χso (T χso (T χso (T

1 Tc ) ≈ , Δ(0) /τso > Tc ) 6 Δ(0)τso Δ(0)τso Tc ) ≈1−2 , Δ(0) /τso . > Tc )

(2.2.10a) (2.2.10b)

Equations(2.2.10) show that when τso is long there is only a small residual value of χsp (T Tc ), but when it is short, i.e. strong spin-orbit scattering near surfaces, χsp (T Tc ) is only slightly perturbed from its normal state value. The latter case is often found for heavy metals such as Hg [24] and Pb [26], and was also found for βSn [25, 33]. These authors performed various

40

2 Introduction to NMR Studies of Metals and Superconductors

doping experiments, which were also consistent with (2.2.10). Ferrell obtained a result similar to (2.2.10b) by means of a physical argument [29]. In a metal as light as elemental Al one might expect spin-orbit eﬀects to be very small. Since colloids of Al are diﬃcult to prepare, shift studies were performed on thin ﬁlm samples. The ﬁrst results gave, surprisingly, residual shift values of ∼75% [27]. It appears that orientation of their multi-ﬁlm samples was quite critical, as subsequent work [34] yielded a very small residual shift. Later measurements by Fine, et al., on a single thin-ﬁlm sample [35] gave results in good agreement with the Yosida function [23]. These data are displayed in Fig. 2.6, ﬁnally giving veriﬁcation to the BCS theory-based prediction. T1 Behavior Below Tc : The BCS Coherence Factor The behavior of T1 for an sp-band (Type I) superconductor according to the BCS theory was ﬁrst investigated, theoretically and experimentally, by Hebel and Slichter [16]. We sketch the calculation of T1 in the SC phase following the derivation in [5]. First, recall from Sect. 1.2.1 that the T1 process consists of scattering fermions from an initial state |kσ to a ﬁnal state |k − σ, while the nuclear spin goes from m to m ± 1 so that angular momentum is conserved. This outline is maintained in the SC state, but other circumstances change drastically. For T < Tc there is some fraction of fermions which are paired (|kσ with | − k − σ) into singlet states and do not scatter. The quasiparticles not condensed into the ground state are thermally excited above the energy gap Δ(T ) and are available to scatter as sketched above. The main diﬀerences are that, ﬁrst, there appears in the summation in 2.2.5 a factor C± (k, k) = 1 2 2 [1 ± (Δ /Ek Ek )] known as the coherence factor, and second, the normal state density of states factors in the integrals leading to 2.2.7 are replaced by the BCS density of states nBCS (E) = n(EF )E/(E 2 − Δ2 )1/2 , where Δ ≤ 1.2 27Al

Ks /Ks(T = Tc)

1

in Al

0.8 0.6 0.4 0.2 0

0

0.5

1

1.5

T/ TC

Fig. 2.6. Data for the 27 Al Knight shift in Al metal from [35] are shown, plotted in units of the normal state shift as a function of T /Tc . The solid curve is the Yosida function, i.e. behavior expected on the BCS theory

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

41

E ≤ ∞. The coherence factor arises because of the pairing of electrons in the condensed phase, and is characteristic of many dynamical properties treated with BCS theory [7]. The choice of sign for C± (k, k ) depends on whether the scattering perturbation is invariant under time reversal applied to the fermion bath. If it is, as in the case of phonons (e.g. ultrasonic attenuation) then C− (k, k ) applies. If it is not invariant, such as for electromagnetic absorption and magnetic dipolar nuclear relaxation, then C+ (k, k ) applies. For the superconducting nuclear relaxation rate 1/T1s one ﬁnds, in units of the normal state rate 1/T1n, ∞ 2 dE (EE + Δ2 ) f (E) (1 − f (E )) T1n = , (2.2.11) T1s kB T Δ [(E 2 − Δ2 )(E 2 − Δ2 )]1/2 where E = E ± γn H. Below Tc the excitation probability is the Fermi function f (Eg ) = [exp(βEg )+ 1]−1 of the gapped energy Eg = (E 2 + Δ2 )1/2 . Since the nuclear Zeeman energy γn H is minuscule on the scale of the quasiparticle energy, there is in fact a logarithmic singularity in 2.2.11 for the case of the coherence factor C+ (E, E ). The most satisfactory explanation for how this singularity is “tamed” is by means of anisotropy of the gap energy Δ(T ) [5, 36]17 . The nuclear Zeeman energy will be neglected henceforward. The behavior of T1n /T1s in 2.2.11 may be divided into two regions, kB T Δ(T ) and kB T > Δ(T ). For kB T Δ(T ) the integral is dominated by the peak in nBCS (E) near the gap, which becomes very nearly constant Δ(T ) ≈ Δ(0). In this limit the factor f (E)(1 − f (E)) ≈ exp(−βΔ(0)), so that 1/T1s decays exponentially at low T. In the other limit kB T > Δ(T ) (T near Tc ), the factor f (E)(1 − f (E)) will have nearly its normal-state value, and the singularity in 2.2.11 has the potential to elevate T1n /T1s to values considerably in excess of 1. This is the source of the well-known BCS coherence peak in 1/T1 (T ) at T < Tc . This peak was ﬁrst measured on 27 Al in Al metal and identiﬁed by Hebel and Slichter [16], establishing a major milestone in experimental conﬁrmation of the BCS theory. It is important to note that for measurements such as ultrasonic attenuation the appropriate coherence factor to use is C− (k, k) , whereupon the factor (EE + Δ2 ) in the numerator of (2.2.11) is replaced by (EE − Δ2 ). This eﬀectively cancels the singularity at E Δ. As a result, the ultrasonic attentuation coeﬃcient was expected to fall abruptly below Tc , as had been conﬁrmed experimentally [37]. This striking contrast between results obtained with probes having diﬀerent symmetry properties was an important conﬁrmation of the correctness of the BCS picture. Following the Hebel-Slichter results, Masuda and Redﬁeld [36] reported further T1 measurements on 27 Al in Al metal taken at temperatures ranging 17

This broadening mechanism was suggested in [36], where it was noted that it gave a good account of the variation of T1 below Tc . The uniform energy gap parameter Δ(T ) in BCS theory is, in fact, an approximation, where the actual gap parameter is properly a function of k. See the book by Tinkham [6], Sect. 2–6, for more discussion of this point.

42

2 Introduction to NMR Studies of Metals and Superconductors

from above to well below Tc . Their results (Fig. 2.7) oﬀered a full panorama of the BCS-theoretical behavior, with a coherence peak (in 1/T1 ) rising above the normal state Korringa curve by a factor ∼ 2, then descending into the superconducting state in a clearly exponential fashion. These data were obtained with a ﬁeld-switching technique similar to that used in [16], the main diﬀerence being that pumped 3 He cooling allowed them to extend the measurements to 0.35K, i.e. far below Tc = 1.18K for Al metal. Analyzing T1 Data in the Superconducting State Since the formulation of (2.2.11) has been widely employed to analyze SC-state data on high-Tc materials as well as all manner of unconventional superconductors, we recount here the analytic procedure used to ﬁt the Al data in some detail [5, 36]. These results are referred to in other sections of the book as well. In order to control the singularity in (2.2.11), Hebel and Slichter [16] postulated a broadening of the electronic energy levels. While such a device enabled them to obtain a reasonable result for the coherence peak, it lacked a clear physical basis. Masuda and Redﬁeld, on the other hand, suggested that the

10.0

T1 (SEC)

5.0

THEORY (r = IOεo(O)/εo(T); GAP = 3.2 kTc)

1.0 0.5

PURE 325 MESH POWDER

0.1

1.0

1.5

2.0 Tc / T

2.5

3.0

Fig. 2.7. A semilog plot of T1 data for the superconducting state of Al metal vs. Tc /T (dots) [36]. Also shown is their ﬁt of the data to the BCS theory (solid line), where the coherence peak (i.e. T1 miminum) amplitude was adjusted using a distribution of energy gap values attributed to anisotropy. The low–temperature energy gap value is adjusted to the slope of the data, yielding Δ0 = 3.2 kB Tc in reasonable accord the the BCS weak-coupling value of 3.52 kB Tc . Reprinted ﬁgure from Y. Masuda, A. C. Redﬁeld, Phys. Rev. 125, 159 (1962). Copyright 1962 American Physical Society

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

43

observed peak was conditioned by a mild anisotropy of the gap parameter Δ(T ). This has a clear physical origin in the BCS equations and gives quite a good ﬁt to the data a well. There, the gap parameter is formally a function of k, and the k-independent gap parameter is just a convenient approximation used to solve the equations. Ample theoretical evidence has been reported for gap anisotropy eﬀects from van Hove singularities and other causes [38]. To illustrate the T1 analysis with (2.2.11) we summarize brieﬂy the development in [5] and [36], and refer the reader to these sources for a more detailed discussion. The procedure is to incorportate the gap anisotropy into the BCS density of states factors in (2.2.11) at the point where sums on k and k are converted to energy integrals. We therefore back up a step from (2.2.11) and rewrite it as ∞ T1n 2 = [Ns (E)2 + Ms (E)2 ] f (E) (1 − f (E))dE, (2.2.12) T1s kB T 0 where

a2

E P (a)da , 2 − Δ(T )(1 + a)2 ]1/2 [E a1 a2 Δ(T )(1 + a) P (a)da and Ms (E) = Re . 2 − Δ2 (1 + a)2 ]1/2 [E a1 Ns (E) = Re

(2.2.13a) (2.2.13b)

In (2.2.13) the variation of Δk over the Fermi surface is represented as a distribution P (a) extending over a1 ≤ a ≤ a2 , where Δk ⇒ Δ(T )(1 + a) and a P (a)da = 0 by deﬁnition. As noted in [5], because the averaging over a is followed by integration over E, the precise shape of P (a) is functionally immaterial to the ﬁnal results. In ﬁtting the T1 data of Fig. 2.7, a2 determines the depth of the T1 minimum and Δ(0) ﬁxes the slope of the exponential tail. The ﬁt shown corresponds to 2Δ(0) = (3.2 ± 0.2)kB Tc and a2 1/2 0.05, in reasonable agreement with the BCS weak-coupling theoretical value 2Δ(0) = 3.52kB Tc . Comparable gap values are given by other probes [5]. There has also been extensive experimentation with doping eﬀects on the SC T1 behavior, yielding some interesting eﬀects. For example, it was found that shortening the mean free path l of the quasi-particles led to even larger coherence peaks in the T1 data for Al [39] and In-based [40] dilute alloys. This eﬀect can be rationalized in terms of the theory of “dirty superconductors” [32], where potential scattering caused by impurities can become strong enough to cause eﬀective mixing between Bloch functions on diﬀerent parts of the Fermi surface. The result is a smoothing out of intrinsic gap anisotropy. Data for the Al-based systems was in good agreement with a theory of this eﬀect [41], but for In-based alloys, there was only agreement for l > ξ0 , where ξ0 is the coherence length. It was suggested that gap inhomogeneity might be suppressing the coherence peak in such a case. However, no further resolution of this point has apparently been reported. As we shall see in the next subsection, there are a number of d-electron superconductors where T1 has no coherence peak for reasons which are also not

44

2 Introduction to NMR Studies of Metals and Superconductors

clear. Moreover, among high-Tc systems, suppression of the coherence peak in T1 is universal, as is also the case for many unconventional superconductors. We defer further discussion of this point to subsections below, where fuller descriptions of the systems concerned are presented.

2.3 Static and Dynamic Magnetism in d-band Metals In this subsection we review the additional complexities which arise when a conductive solid has an open d-shell in addition to its sp-band eﬀects. D-electrons in solids are typically more tightly bound to their host ion, interacting more weakly with neighbors. As a result they have narrower, more highly structured energy bands with substantially higher densities of states at their Fermi surfaces. Moreover, they are subject to a crystalline electric ﬁeld (CEF) which results from bonding and proximity to neighboring ions, which breaks the full rotational potential symmetry enjoyed by a free ion. As a result, the d-electron angular momentum “always” has a zero expectation value in the ground state. On the other hand, the greater densities of states of d-bands, when combined with the electron-electron exchange eﬀects [21] which came to light in the Moriya treatment of enhanced NMR shifts and relaxation [22], lead to strongly enhanced susceptibilities and even to permanently magnetized ground states in a number of pure metals (e.g. Fe, Co, and Ni in the 3d series). Moreover, ions with d-electrons as dilute impurities or dopants frequently possess a localized magnetic moment. However, discussion of d-ion systems possessing full atomic magnetism is beyond the scope of this volume. Special Features of NMR in d–Band Metals and Superconductors Keeping superconductivity in mind, we shall restrict our attention to d-electron systems which do not order magnetically. We consider, as an example, the behavior of the V3 X series of compounds, which are superconductors as well. There is a wealth of interesting NMR phenomena which arise in such systems, including: •

•

Prominence of the core-polarization (CP) d-spin HF ﬁeld in studies of d-band magnetism. Since d-electrons have no contact interaction, this isotropic, negative HF coupling, which was identiﬁed by Heine [42] and by Wood and Pratt [43], takes it place. The core polarization plays a major role, since dipolar interactions are often smaller and are cancelled by cubic symmetry. The greatly enhanced importance of orbital eﬀects, both the static (Van Vleck) shift and susceptibility and the robust orbital T1 mechanism. The d-band orbital susceptibility was ﬁrst formulated by Kubo and Obata [44]. Its contribution to the NMR shift was identiﬁed by Clogston et al., [45] in connection with the V3 X compounds, where it had important consequences for the interpretation of superconducting shift data.

2.3 Static and Dynamic Magnetism in d-band Metals

•

•

45

The latter authors [46] also pioneered the use of the K−χ plot as a means of analyzing NMR shifts and their corresponding susceptibility components in d-band metals. This technique continues to be used very widely and has led to great insight into the magnetic infrastructure of metals and intermetallic compounds. We present their method below. When d-electron metals are superconductive, they are nearly always TypeII superconductors. Thus, NMR studies are very often conducted in the mixed state, i.e. in the presence of a large magnetic ﬁeld and a vortex lattice. The ﬁeld penetrates throughout the sample, dividing itself into as many ﬂux bundles as possible, which occurs when each vortex contains just one ﬂuxon. We shall review results on NMR shifts, lineshapes, and on T1 studies as well. These eﬀects are directly relevant to superconductive highTc NMR studies, since they are often conducted under the same conditions.

2.3.1 The d-Electron HF Interactions In general there are two types of d-electron HF interactions, namely spin and orbital, the latter arising from the ﬁrst term in (2.2.1), and the former from the second two terms. In d-band metals there are also multiple bands with their own Fermi surface density of states and corresponding HF interaction terms. These terms will make additional contributions to the NMR shift and relaxation rates, rendering the task of analyzing experimental data for these parameters a bit more complex. By and large, however, d-electron bands are somewhat more “lively” than their rather prosaic s and p counterparts, and tend to dominate the nuclear spin properties. In high-Tc materials, depending on your point of view, there is scant evidence for actual sp-bands per se, so the d-electron HF eﬀects are, by any measure, the dominant ones. Anisotropic d-Spin Susceptibility and HF Tensor If we allow the d-spin HF coupling to be anisotropic, we then take Hds =

Adξ Iξ Sξ with χdξ =

ξ=x,y,z

NA gξ μB Sξ . H

(2.3.1)

The d-spin shift coeﬃcient is then deﬁned as αdξ =

Kdξ Adξ = . χdξ NA γgξ μB

(2.3.2)

For ordinary 3d metals we shall take gξ ∼ 2, whereupon αd becomes isotropic. However, these deﬁnitions will carry over into the cuprate discussion in Chap. 3, where for the cuprates there is evidence for substantial g-shifts. We also note here that the HF coeﬃcient can be quoted as simply Adξ in ergs, as Adξ / in units of s−1 , as 10−3 Adξ /γ in kG/spin, as 10−3 Adξ /γgξ in units of kG/μB , or as Adξ /1.60218 × 10−12 in eV. Although it may be somewhat

46

2 Introduction to NMR Studies of Metals and Superconductors

confusing, one ﬁnds all of these units in use in the high–Tc literature. The d-spin HF ﬁeld is also known as the core-polarization HF ﬁeld (hence Ad → Acp ), which we now discuss. Core-Polarization Hyperﬁne Coupling: The Mechanism Since d-electron wavefunctions vanish at the site of the nucleus, they possess no direct contact HF ﬁeld from the ﬁnal term in (2.2.1). However, they do activate the contact HF term indirectly in such a way as to generate an eﬀectively isotropic HF coupling with the nuclear spins. This mechanism came to light with the work of Heine [42] and of Wood and Pratt [43]. Detailed calculations have been given by Freeman and Watson [47]. The mechanism of the core polarization HF ﬁeld is a simple consequence of the Pauli exclusion principle, and works as follows. In d-electron atoms there are two or more ﬁlled s-shells which are magnetically inert. Nonetheless, these ﬁlled s-shells undergo repulsive coulombic interactions with the Fermi-surface d-electrons which, generally speaking, lie outside of them, i.e. at larger distances from the nucleus. Thus, coulomb repulsion drives the s-shell electron orbitals closer to the nucleus. This repulsive eﬀect is, however, dependent on spin. Consider the majority d-spin moment to point up. The up-moment s-shell electrons are then known to avoid close proximity with the up-moment d-electrons in a Pauli-exclusion eﬀect known as the Fermi hole. The down-moment s-electrons have no such eﬀect. With the same wavefunction, then, the down-moment s-electrons will have a higher coulomb repulsion energy. For that reason, the down-moment s-shell orbitals will tend to “shrink” toward smaller radii relative to the upmoment s-shell orbitals, creating a net down moment of s-electron density at the nucleus, i.e. a net negative contact HF interaction. The diﬀerential orbital distortion eﬀect is small, but the core s-shell HF couplings are enormous, so that there is a substantial net HF coupling. For 3d-electrons the resulting Hf ﬁeld is ∼ −125kG/μB , increasing gradually across the 3d series. For the 4d and 5d shells the eﬀect is generally larger [47]. As an example, we note that the 5μB S-state moment of Mn2+ in MnF2 generates a HF ﬁeld −127kOe/μB at the 55 Mn nucleus. This compound has purely 3d-spin magnetism. 2.3.2 Orbital Shift and Susceptibility The orbital term in (2.2.1) comes into play for both the NMR shift and T1 . The orbital shift is driven by the Van Vleck orbital susceptibility, which was ﬁrst formulated for band electrons by Kubo and Obata [44]. The susceptibility was formulated in a tight-binding approximation, yielding the following expression for the α-axis susceptibility, dk f (Enk ) − f (En k )

nk|lα |n k n k|lα |nk , χorb = NA Ωμ2B (2π)3 En k − Enk nn (2.3.3)

2.3 Static and Dynamic Magnetism in d-band Metals

47

where NA is Avogadro’s number, Ω is the atomic volume, and the summing indices n and n represent the ﬁve d-orbital subbands as well as the spin quantum number. The quantity f (Enk = [exp(β(Enk − EF )) + 1]−1 is the Fermi occupation function. χorb is written here as a molar susceptibility. Clogston et al., [48] have derived a companion expression to (2.3.3), which gives the induced orbital hyperﬁne ﬁeld at the nucleus when the eﬀects of the spin-orbit coupling and certain other terms in the general expression, deemed to be small, are neglected. The simpliﬁed expression is dk f (Enk ) − f (En k ) 2

nk|2lα /r3 |n k n k|H lα |nk, Horb = ΩμB (2π)3 En k − Enk nn (2.3.4) where the ﬁeld H is taken to be directed along the α axis. If we make the assumption that the radial functions of all the d-orbitals in the band are approximately the same, then we may extract 1/r3 from the latter expression, ﬁnding (2.3.5) Korb = [2 1/r3 /NA ] χorb , where the quantity in brackets is identiﬁed as the orbital shift coeﬃcient αorb . When using calculated ionic values for 1/r3 [47], the foregoing authors suggest that a correction factor ξ = 1/r3 metal / 1/r3 ion 0.75 be invoked for realistic estimates of the metallic shift coeﬃcient αorb . Analysis of NMR Shift and Susceptibility for d-Band Metals: The (K, χ) plot With the foregoing additions to our list, we are now in a position to formulate a complete model of the shift and susceptibility of a d-band metal. The following model would apply to a pure metal from the 3d, 4d, or 5d transition series, but is also intended to represent a binary or ternary intermetallic compound a long as its Fermi surface can be modeled with two bands, an sp-band which belongs mostly to the transition metal atoms and a d-band which belongs exclusively to the transition metal atoms. The p–orbitals on the ligands are assumed to be strongly mixed into the d–band, while the s–orbitals are not, i.e. are presumably nearly ﬁlled [46]. We then write for the susceptibility, χtot = χdia + χs + χd (T ) + χorb ,

(2.3.6)

where χs and χd (T ) are the spin-paramagnetic terms, χorb is the d-electron orbital term given by (2.3.3), and χdia is the core diamagnetic term. Among these, χs is quite small, though its associated Knight shift may not be, so that any Landau diamagnetism is very small, indeed. Neither the latter nor χdia has any appreciable NMR shift eﬀect[48]. Molar susceptibilities are used throughout this volume18 18

From the standpoint of the microscopic physics of solids, we regard the susceptibilities per atom χat (or per formula unit χf u ) as fundamental, representing the

48

2 Introduction to NMR Studies of Metals and Superconductors

The NMR shift for the nucleus of a transition-metal ion, then, has three signiﬁcant terms [48], K(T ) = Ks + Kd (T ) + Korb = αs χs + αd χd (T ) + αorb χorb ,

(2.3.7)

in conventional notation for the shift coeﬃcients. Typically, the only temperature dependence originates in χd (T ). Therefore an experimental plot of K(T ) vs. χtot (T ) with T as the implicit variable should yield a straight line of slope αd . An experimental K vs. χ plot is just the beginning of a full (K, χ) analysis of the various terms in (2.3.6) and (2.3.7). Such an analysis for the case of Pt metal was presented in [48], with the plotted result shown here in Fig. 2.8. We give a brief account of the analytic procedure. First, any K − χ analysis must begin at the origin, and several parameters need to be estimated in order to proceed. We refer the reader to the original paper for full details. The ﬁrst step is to plot χdia −28 × 10−6 emu/mole

(3) (2)

1

(1) –40

0

40

120 160 200 χ (10–6 emu/mole)

–1

K(%) –2 –3

Range of experimental data:

Fig. 2.8. A K-χ plot is shown for 195 P t in Pt metal. Plotting of successive contributions to (K,χ) carries one from the origin to point 1 (χdia ), then from point 1 to point 2 (Ks , χs ), and ﬁnally from point 2 with an estimated slope αorb . The intersection at point 3 with the line through the experimental data completes the partition of the susceptibility. A detailed discussion of the analysis is given in the text. Reprinted ﬁgure from A. M. Clogston, V. Jaccarino, Y. Yafet: Phys. Rev. 134, A650 (1964). Copyright 1964 American Physical Society magnetic polarization which occupies one Wigner-Seitz (or unit) cell. Their companion molar susceptibilities are χM = NA χat and χM f u = NA χf u . If Ω is the atomic (or Ωc the unit cell) volume, then the dimensionless volume susceptibility fundamental to electromagnetic theory is χV = χat /Ω (χf u /Ωc ), and the gram susceptibility is χgm = χat /Ωρ, where ρ is the volume density. It is clear that the actual dimensions of χM are cm3 and of the α shift coeﬃcients are cm−3 , although these are usually cited as emu/mole and (emu/mole)−1 .

2.3 Static and Dynamic Magnetism in d-band Metals

49

at K = 0 (point 1), since there is no appreciable diamagnetic shift [48]. This value of χdia may be taken from the literature [49]. From point 1 we construct a line of slope αs to extend over the interval Δχ = χs . For this step, αs was obtained from HF structure parameters derived from optical data, yielding αs 2.12 × 103 (emu/mole)−1 . χs is estimated using a free-electron model, where the number ns,d of (s, d) electrons satisﬁes ns + nd = 10. With a parabolic model for the 5d-band a value of ns = 10 − nd = 0.2 was obtained, giving χs 4.8 × 10−6 (emu/mole). The s-band line in Fig. 2.8 then extends from point 1 to point 2. Next, we construct a line from point 2 with a slope equal to the estimated value of αorb = 2 1/r3 /NA . The ionic value of 1/r3 has been estimated to be 9.5a.u. from HF spectroscopic data, leading to the value αorb 264(emu/mole)−1, including a relativistic correction [48]. Drawing a line with slope αorb from point 2, the intersection of that line with the line through the data (point 3) then partitions the remaining susceptibility into orbital and d-spin contributions as shown. In the case of Pt metal, χtot is dominated by χd (T ), and χorb is a relatively small fraction ( 15%) of χtot . In cases where χorb is a signﬁcant fraction of the total, its temperature dependence may be a big enough eﬀect so that a simple (K, χ) plot is no longer reliable [48]. Nonetheless, the (K, χ) method has been widely used to analyze NMR shift data with experimental susceptibilities. For example, it was used to determine that substantial χorb terms were present in the V3 X’s and in V metal [45]. We reproduce in Table 2.3 the table of results from [45]. In this table, values of χorb from (K, χ) analyses are subtracted from experimental susceptibilities to estimate χd , which is given as χexpt - χorb . The latter values are then to be compared with d-spin susceptibilities estimated 2 from the speciﬁc heat coeﬃcient γ, where χsp.ht. = 3μ2B γ/π 2 kB . A simple theory gives electron-phonon enhancement of γ by a factor [1 + N (0)V]. V is the BCS electron-phonon interaction parameter. Since χd is not so enhanced Table 2.3. Table of susceptibility components and BCS parameters for V3 X compounds and V metal. The estimates for χorb were determined using (K, χ) plot analyses. The values of χd = χexpt - χorb so deduced are checked using density-of-states estimates from speciﬁc heat data as corrected for electron-phonon enhancement by means of BCS theory. See text for detailed explanation. All susceptibilities are in units of 10−4 emu/mole R ≡ χd (0) /χd (Tc )

χexpt

χorb

χsp.ht.

χexpt − N (0)V χorb (Sp.Ht.)

N (0)V (BCS)

V3 Ga

0 ≤ R ≤ 0.25

17.9

5.2–7.5

14.0

0.35

V3 Si

0 ≤ R ≤ 0.25

15.7

5.2–7.5

10.7

12.7– 10.4 10.5– 8.2 0.971

V

3.08

2.11

1.22

0.13– 0.39 0.09– 0.35

0.35 0.244

50

2 Introduction to NMR Studies of Metals and Superconductors

[50], one may estimate VN (0) χsp.ht. /χd − 1. In the last two columns of Table 2.3, values of N (0)V deduced in that way are compared with those derived from Tc using the BCS formula N (0)V = [ln(0.855 θD /Tc)]−1 . Considering the diﬃculty of estimating the relevant parameters, this analysis gives a nicely consistent picture in which it is established that (a) χd at T Tc is a small fraction of its normal-state value, and (b), values of χd consistent with electron-phonon enhancement of γ are obtained. Note that χs 0.3 (units of Table 2.3) has been ignored and is essentially negligible. 2.3.3 Spin-Lattice Relaxation Eﬀects for d-Band Electrons An open d-band brings added richness - and complications - to the T1 process as well, contributing a total of three additional terms to the T1 rate. These are the d-spin core polarization (CP), the d-spin dipolar, and the d-orbital terms. The d-orbital relaxation process was ﬁrst discussed by Obata [51]; we shall spell out the results of that calculation below. The general treatment of the CP relaxation process, on the other hand, is an enterprise of great complexity. Under a set of straightforward restrictions, Yafet and Jaccarino have presented a very clear discussion of this problem [52], which has been useful under a variety of circumstances. Here we discuss brieﬂy the approximations employed and give the results. The stated approximations are as follows: • • • • • • •

Spin-orbit coupling is disregarded. The unperturbed states (i.e. without HF terms) are taken to be HartreeFock solutions of the simpliﬁed Hamiltonian. Exchange intergrals responsible for the CP eﬀect are treated in ﬁrst order. Exchange eﬀects between conduction band orbitals are neglected. Conduction band states are self-consistent Bloch states, which are admixtures of s, p, and d orbitals. The conduction band d-states are treated in a tight-binding approximation. Finally, consideration is limited to the case of a cubic metal. As a result, the cross terms between sp and d-orbital matrix elements can be shown to vanish. The resulting expressions for the shift and relaxation rate are: K=

4π (γe )2 [ φ2s (0)(1 − Fd ) − |φcp (0)|2 Fd ]n(EF ) 3

(2.3.8)

and 1 = T1 T

4πkB

4π 3

γn γe 2

2

[ φ2s (0)(1 − Fd )2

+|φcp (0)|4 Fd2 ( 13 f 2 + 12 (1 − f )2 )]n(EF )2 ,

(2.3.9)

2.3 Static and Dynamic Magnetism in d-band Metals

51

where Fd is the fraction of d-character of all the states at the Fermi surface, and n(EF ) is the total density of states (of all “bands”) at the Fermi surface. Thus, even if there is appreciable s-d mixing in the Bloch functions the contributions to shift and relaxation will occur separately as shown. CP terms are only kept for the d-orbitals, even though they may occur in the calculation for the s and p orbitals. The reason for this is that the contact terms dominate the sp regions of the Fermi surface, and any CP terms are neglected for those states as small corrections. The parameter f gives the relative weight of Γ5 character for d-orbitals at the Fermi surface, while 1 − f gives the proportion of Γ3 character19 . It is seen that the sp-contact and d-CP portions of the formulas for K and 1/T1 T obey separate Korringa-like relations (see 2.2.8), where the Korringa relation for the CP terms has a reduction factor q(f ) = 13 f 2 + 12 (1 − f )2 , i.e.

2

4πkB γn2 2 Kcp q(f ), γe2 (2.3.10) where the second equality shows the modiﬁed Korringa relation. q(f ) is essentially a degeneracy factor, having a value 1/2 for the two Γ5 orbitals (f = 1), 1/3 for the three Γ3 orbitals (f = 0), and 1/5 when all ﬁve d-orbitals are equally weighted (f = 0.6). Thus the ﬁve d-orbitals contribute independently to 1/T1CP , very much like the ﬂuctuations of separate magnetically-active neighbors contribute to the T1 process of a ligand nucleus. The diﬃculty in utilizing (2.3.10 is that the parameter f for d-band metals is generally unknown. The orbital T1 process was ﬁrst discussed in detail by Obata [51], treating both orbital and dipolar relaxation rates in the same calculation. As with the CP calculation above, spin-orbit coupling is neglected, the d-orbitals are treated in a tight-binding approximation, and the system considered is a cubic metal. There are no cross terms between orbital and spin-scattering relaxation processes. It was noted in [52] that the dipolar process has interference with the contact and CP processes, but if the states at the Fermi surface can be separated into a d-band and an sp-band, then the interference terms vanish. For a cubic metal, both the orbital and dipolar relaxation rates are isotropic, but both depend on the symmetry parameter f , according to 1 4πkB 1 , [γn Horb ]2 nd (EF )2 p(f ), [d(f )], (2.3.11) = T1orb T T1dip T 4πkB = T1cp T 1

4π γn γe 2 |φcp (0)|2 3

nd (EF )2 q(f ) =

5 1 2 [ 3 f + 25 (1 − f )]. where Horb = 2μB 1/r3 , p(f ) = 23 f [2 − 53 f ], and d(f ) = 49 Comparison of the dependences of q(f ), p(f ) and d(f ) on f is shown in Fig. 2.9. The orbital relaxation rate (p(f )) is seen to vary from zero, when the Γ5 orbitals alone are occupied at the Fermi surface, to a maximum when all 19

In the present notation of d-functions in the cubic space group, Γ3 refers to the d functions dxy , dyz , and dzx , while Γ5 refers to dx2 −y 2 and d3z 2 −r2 .

52

2 Introduction to NMR Studies of Metals and Superconductors 0.5 0.45 q

0.4 q, p, and d

0.35 0.3 0.25 0.2

p

0.15 0.1

d

0.05 0 0

0.2

0.4

0.6

0.8

1

f

Fig. 2.9. The symmetry factors q(f ), p(f ), and d(f ) pertaining to CP, orbital, and dipolar relaxation rates discussed in the text [52], respectively, are plotted as a function of the fraction f of Γ5 character in the relevant d-band orbitals at the Fermi surface. The point f = 0.6 represents equal weight of all ﬁve d-orbitals and is the maximum and minimum point of p(f ) and q(f ), respectively. In many cases the dipolar rate is negligible, as it is only ∼ 9% of the average value of the closely related orbital rate. Reprinted ﬁgure from Y. Yafet, V. Jaccarino: Phys. Rev. 133, A1630 (1964). Copyright 1964 American Physical Society

ﬁve orbitals are equally occupied, since the orbital matrix elements between the two symmetries are the largest ones. The dipolar relaxation rate (d(f )) varies only slightly across the full range of f , but it is only about 10% of the average value of p(f ). Thus, the dipolar relaxation is only signiﬁcant when p(f ) is near zero. The complete list of magnetic relaxation processes for d-band metals is then (2.3.12) 1/T1 = 1/T1s + 1/T1cp + 1/T1orb + 1/T1dip . We illustrate the analysis of experimental T1 rates into these diﬀerent contributions with calculations given in [52] for d-band metals V and Nb. In stating these results we deﬁne Hs = (8/3)πμB φ2s (0) and Hcp = (8/3)πμB |φcp (0)|2 , whereupon (2.3.9) becomes 1 4πkB = [γn Hs,cp ]2 n2s,d [1, q(f )] T1s,cp T

(2.3.13)

for the s-band and CP contributions. The parameters Hs,cp are the HF ﬁelds per unit of spin from these sources. The T1 contributions from the three main sources have been estimated [52] for V and N b metals as listed in Table 2.4. For this purpose, Hs has been estimated using data from the literature [52], and Hcp and Horb have been derived from Hartree-Fock calculations given by Freeman and Watson [53]. The total densities of states for these elements are taken from speciﬁc heat measurements, where the s-band components are

2.3 Static and Dynamic Magnetism in d-band Metals

53

Table 2.4. Table of HF parameters and speciﬁc heat densities of states leading to estimates of (T1 T )−1 for elemental V and N b using the formulas given in the text. The total relaxation rates are stated for f = 0.6, but would not change signiﬁcantly for other values of f . The theoretical estimate undoubtedly exceeds the experimental numbers because of the electron-phonon enhancement of the speciﬁc heat density of states, which does not aﬀect nuclear relaxation rates. See text for data sources and additional discussion. HF ﬁelds are given in units of 106 Oe, densities of states in states/eV-atom, and relaxation rates in (sK)−1 Hs

Hcp

Horb ns (EF ) nd (EF ) Rs

V 1.12 -0.117 0.19 0.12 Nb 2.48 -0.21 0.285 0.14

1.84 1.66

Rcp R1orb (T1calc kT )−1 (T1exp T )−1

0.642 1.65 4.35 3.76 3.74 6.9

2.86 7.55

1.27 2.8

estimated assuming for simplicity one s-electron per atom. The quantities Rs , Rcp , Rorb are deﬁned to be the expressions given above for 1/T1 T from these sources without the symmetry factors [1, q(f ), p(f )]. The experimental values of (T1exp T )−1 are data reported by Butterworth [54]. This table illustrates the importance of the CP and orbital relaxation mechanisms in d-band metals. For the lighter metals, where the s-band contribution is smaller, these d-electron terms may even be the dominant ones. On the other hand, we see that the speciﬁc heat density of states clearly overestimates the relaxation rates, pointing to a substantial electron-phonon enhancement eﬀect for V and Nb metals (which are also superconductors). In [5] a quantitative discussion of the latter eﬀect is given, ﬁnding reasonable agreement between the nuclear relaxation data and estimates from other measurements, somewhat like the comparisons in Table 2.3. As the details go beyond the intended scope of this discussion, the reader is referred to [5] and references therein for details. This completes our discussion of normal-state NMR shift and relaxation eﬀects in transition metals. The mechanisms in (2.3.2) and (2.3.12) are the foundation of eﬀects to be found in high-Tc materials, though the details remain to be worked out. We next consider the eﬀects of Type II superconductivity in the d-band metals. 2.3.4 NMR Studies of 3d Metals as Type-II Superconductors The type-II superconductivity of d-band metals and intermetallic compounds presents a rather diﬀerent set of problems from those of the type-I systems discussed in Sect. 1.2.2. First, type-II systems exhibit great complexity of behavior in a magnetic ﬁeld, showing three phases as a function of the magnitude of the applied ﬁeld for T < Tc and exhibiting two critical ﬁelds, Hc1 and Hc2 . Below Hc1 there is the typical Meissner exclusion of all magnetic ﬂux except for the usual penetration depth λ. Between Hc1 and Hc2 there is a state of essentially complete, but inhomogeneous ﬁeld penetration in the form of superconducting current vortices

54

2 Introduction to NMR Studies of Metals and Superconductors

which allow a single ﬂuxon of ﬁeld to exist in a region of normal (i.e. nonsuperconducting) metal with a diameter ∼ ξ0 , the Pippard coherence length. Of course, the magnetic ﬁeld of a ﬂuxon penetrates the surrounding material to a depth of ∼ λ. Each ﬂuxon comprises one ﬂux quantum Φ0 = hc/2e = 2.07 × 10−7 G cm2 . Because of the accommodation of type-II superconductivity to applied ﬁelds through the penetration of vortices, the superconducting state can persist up to ﬁelds much higher than the thermodynamic critical ﬁeld Hc . One can make a rough estimate of Hc2 using a picture of vortices with normal cores of approximate radius ξ0 . In the mixed state with ﬁeld H (T Tc ) the density of vortices is H/Φ0 . The fraction of normal sample material is then ∼ πξ02 H/Φ0 . Setting this expression equal to 1 gives an estimate Hc2 ∼ Φ0 /πξ02 . This is only slightly larger than the expression deduced from Ginzburg-Landau (GL) theory, Φ0 . (2.3.14) Hc2 = 2πξ02 As was ﬁrst demonstrated by Abrikosov√[55], the normal-superconducting boundary wall has positive energy for λ < 2ξ. On the other hand, if the GL √ parameter κ = λ/ξ > 2, then the boundary wall has negative energy, so that the system will lower its free energy by making the boundary area as large a possible. Thus, the ﬁeld arranges iself into individual ﬂuxons, each surrounded by a normal-superconducting wall. Abrikosov predicted the existence of such a mixed state, in which the vortices arrange themselves (in reasonably clean material) into an ordered lattice [55]. The lowest energy state of such a lattice was shown to be minimized by a triangular arrangement of vortices by Kleiner et al., [56]. Below, we describe NMR spectra which are consistent with this theoretical conclusion. It is interesting to look at simple expressions for ξ and λ to see why there is a general tendency for d-electron superconductors to exhibit type-II superconductivity. The expressions m c2 vF , (2.3.15) and ξ0 = a λ0 = 2 4πns e kB Tc where a is a constant of order unity, come from the London equations and from Pippard’s uncertainty principle argument, respectively. Since d-bands tend to have large eﬀective masses and high-Tc materials in particular have low carrier densities ns , we expect λ0 values to be larger than for sp-band superconductors. Furthermore, small values of EF (and thus of vF ) as well as higher √ values of Tc will make for short ξ0 ’s. Thus, it is generally expected that λ > 2ξ0 . As an example, we mention V3 Si, a superconductor at ∼ 17K which we shall discuss further below. Here, we only note that Greytak and A and a related estimate of Wernick [57] reported a measurement of λ0 = 1500˚ ξ0 = 25˚ A. Thus, κ 60 and from (2.3.14) we estimate Hc2 530 kG. A second estimate can be made from the thermodynamic critical ﬁeld Hc = 6370 G [58]

2.3 Static and Dynamic Magnetism in d-band Metals

55

and the measured value of λ0 using (4–62) from [6], Hc2 = 4πλ20 /Φ0 . This yields Hc2 = 550kG, which is in surprisingly good accord with the previous number. In any case, V3 Si is a very “hard” superconductor, indeed. Internal Field Distributions in the Mixed State from NMR Studies NMR studies of type-II superconductors are typically done in the mixed state, i.e. for Hc1 < H < Hc2 . There is substantial NMR line broadening from spatially-dependent shielding supercurrents in the mixed state. We shall ﬁrst review studies conducted to map the distribution of such currents, after which we will look at shift and relaxation studies. A number of internal ﬁeld studies have been reported for V and Nb metals [59, 60, 61]. We review brieﬂy the results given by Redﬁeld [60], who conducted the following ﬁeld-switching NMR experiment on 51 V in V metal. The sample was polarized in 10 kG, after which the ﬁeld was switched to a value below Hc2 ∼ 3, 000 G for a time of 0.1s, during which an rf ﬁeld was applied transverse to the steady ﬁeld. The ﬁeld was then switched back to 10 kG where the nuclear polarization was recorded. By scanning the frequency of the rf, the spectrum of internal ﬁelds could be mapped out. Results from this study are shown in Fig. 2.10a for two ﬁeld values. These data have been ﬁtted to calculated internal ﬁeld distributions based on the GL equations in the Abrikosov limit, assuming both square and triangular lattices [60]. The raw calculated distributions are shown in Fig. 2.10b. Fits are carried out by convoluting the latter distributions with a Gaussian of adjustable width, then adjusting the width and total area for best ﬁt. The triangular lattice unit cell is shown as an inset to Fig. 2.10b, where the points V, C, and S are seen to correspond to the maximum ﬁeld, minimum ﬁeld, and the singularity in the distribution, respectively. The singularity appears much closer to C for triangular lattice than for the square lattice. Results for the lower ﬁeld value ( 0.73Hc2 ) are seen to be in good accord with the triangular lattice. The higher ﬁeld value is rather closer to Hc2 , where a kind of gapless superconducting state sets in and there are many corrections to the simple ﬁeld-distribution calculation. Thus, it is not surprising that the simple triangular lattice calculation is no longer accurate [60]. Studies of eﬀects near Hc2 are reviewed in [5]. We shall, however, restrict our attention here to the region Hc1 H Hc2 . It is interesting to compare the ﬁeld distribution results from [60] with theoretical predictions. For example, the results from Kleiner, et al., [56] predict that HV − HS = 1.35 (H − B). From [60] we ﬁnd for the conditions of Fig. 2.10 the experimental value HV − HS = 285 G, while 1.35 (H − B) under the same conditions 165 G, a considerable underestimate. On the other hand, 1.35 (H − B) according to the Abrikosov solution [5, 55] equals 1.35 (Hc2 − H)/βa (2κ2 − 1), which we ﬁnd to be 520 G, which is a considerable overestimate. For this purpose we take βa = 1.16 for the triangular

56

2 Introduction to NMR Studies of Metals and Superconductors

(a)

RELATIVE ABSORPTION

(a) B = 0.73 HC2

LOCAL FIELD

(b) B = 0.88 HC2

LOCAL FIELD

RELATIVE ABSORPTION

TRIANGULAR LATTICE UNIT CELL

(b)

SQUARE LATTICE

V S V

C S

S V

S B

B

C

V FREQUENCY OR LOCAL FIELD H

Fig. 2.10. (a) Distributions of diamagnetic shielding ﬁelds measured using rf saturation of the 51 V NMR in superconducting V metal, and (b) simulations of internal ﬁeld distributions under similar circumstances for both square and triangular vortex lattices. In (a) results are given for T 1.4 K and for ﬁelds of 0.73 Hc2 and 0.88 Hc2 as shown, where Hc2 = 2720 G. For (b) the ﬁeld simulations were done on the basis of solutions of the Ginzburg-Landau equations in the Abrikosov limit. The inset shows the triangular lattice unit cell, with points there and on the distribution labelled V, S, and C corresponding to a vortex (V), a saddle point (S) showing a divergence, and the minimum ﬁeld (C). Reprinted ﬁgure from A. G. Redﬁeld: Phys. Rev. 162, 367 (1967). Copyright 1967 American Physical Society

lattice from [56] and employ (2.3.14) to obtain ξ0 = [Φ0 /2πHc2 ]1/2 = 348˚ A. The estimate λ = 400˚ A [62] then leads to κ = 1.15. Substantial corrections to these simple theoretical results have been given by Eilenberger [63].

2.3 Static and Dynamic Magnetism in d-band Metals

57

The NMR Shift in Type-II Superconductors In the foregoing study of elemental vanadium, the precision with which the vortex lattice could be characterized was not great enough to resolve changes in the d-spin shift Kd (T ) below Tc [60]. However, in a truly hard type-II system where κ 1, it is possible to resolve small shift changes at ﬁeld values such that Hc1 H Hc2 . The reason for this is that the NMR lineshape is then strongly dominated by the singularity from the saddle regions S (Fig. 2.10b), which is therefore shifted only slightly away from the applied ﬁeld. Moreover, the NMR linewidth from diamagnetic shielding is typically only modestly greater than one might ﬁnd in the normal state. We illustrate these points with data and discussion of the closely related cases of V3 Si and V3 Ga, where V3 Si was touted earlier as a truly hard superconductor. Interestingly, somewhat before the nature of the the type-II diamagnetic shielding was investigated in detail in the 1960’s, The NMR shifts in these compounds of both 51 V and 71 Ga were reported by Clogston et al., [45]. We reproduce their (K, χ) plot in Fig. 2.11. The interesting point here is that all NMR shift values here are consistent with the interpretation that, at T = 1.8 K, the corresponding d-band susceptibility is diminished to ∼ 25% of its value at 20 K. Further, its low temperature value is smaller than that at room temperature. Since these NMR shifts were measured in the mixed state at a ﬁeld of 14 kOe, where they found “negligible diamagnetic rf susceptibility” [45], one can only conclude that spurious frequency shift eﬀects from the diamagnetic shielding are negligibly small in comparison. Note that the total range of 51 V shift values in Fig. 2.10 is only ∼ 0.1%. It is interesting to consider the nature of the internal ﬁeld distribution in A and 1500˚ A, respecV3 Si given the values of its parameters ξ0 and λ0 (25˚ tively) stated above. First, the second moment of this distribution has been calculated by Pincus et al., [58], yielding the expression

ΔH 2 1/2 av

Φ0 4π 3/2 λ2

(2.3.16)

under conditions where not only Hc1 H Hc2 holds, but also λ/d 1, where d is the separation of vortices in the√mixed state. At H = 14 kOe (i.e. A for the triangular for the data of Fig. 2.11), we ﬁnd d = [2Φ0 / 3H]1/2 = 413˚ 1/2 lattice, giving λ/d = 3.6. For these conditions (2.3.16) gives ΔH 2 av = 41 Oe for a square lattice. This may be a slight overestimate, but is of the right order, since the measured peak-to-peak derivative linewidth is 39 ± 5 Oe [58]. It is interesting to note in this case, where κ 1, the Abrikosov relation [5, 55] yields HV − HS = 86 G, barely twice the second moment estimate. We therefore ﬁnd for the hard type-II superconductors that it is quite feasible to measure shift values with weak temperature dependences in the mixed state of superconductivity. This is a very important result for high-Tc NMR studies.

58

2 Introduction to NMR Studies of Metals and Superconductors

2.3.5 T1 Phenomenology for Type-II Superconductors In this ﬁnal subsection of Chap. 2 we review T1 behavior at T < Tc for typeII d-band superconductors. Because of the complications which attend the measurement and interpretation of T1 in the mixed state of these systems, our discussion of this topic will be limited to a few simple cases. A clear and thorough discussion of these eﬀects, in terms of both theory and experiment, is given in [5]. The hallmarks of type-I system T1 behavior are the coherence peak (in T1−1 ) just below Tc and the exponential decay T1−1 ∝ exp(−Δ0 /kB T )

1.0 V51

0.8

1.8° B

295°

0.6

KNIGHT SHIFT IN PERCENT

1.8°

295° V3Si

0.4

V3Ga x x

20° 20°

0.2 0 1.8°

–0.2

295° –0.4

V3Ga

Ga71 –0.6

–0.8 1.0

20°

0

2

4

6

8

10

12

SUSCEPTIBILITY (EMU/MOLE)

14

16 18 ×10–4

Fig. 2.11. Measured Knight shifts are plotted vs. molar susceptibilities for 51 V in both V3 Si and V3 Ga and for 71 Ga in V3 Ga [45]. For the 51 V shifts a (K, χ) construction is shown, including the s-band contribution (point A) and the orbital contribution (points A-B), which intersects with lines through the data points. For the 71 Ga the results clearly show a transferred shift which is driven by the temperaturedependent d-band susceptibility. In both cases the location of the shift values measured at 1.8 K are shown, indicating that the negative CP shift is diminished to ∼ 75% of its value at 20 K, and that the values of |Kd (T )| in both cases are smaller than the values found at room temperature. Reprinted ﬁgure from A. M. Clogston, A. C. Gossard, V. Jaccarino, Y. Yafet: Phys. Rev. Lett. 9, 262 (1962). Copyright 1962 American Physical Society

2.3 Static and Dynamic Magnetism in d-band Metals

59

for T Tc . For type-II systems these behaviors carry over in a modiﬁed way or not at all. The diﬀerences found between type-I and type-II behavior appear to be caused by the ﬁeld penetration in the mixed state and the consequent spatial inhomogeneities. The Coherence Peak Region, T ≤ Tc (H) Caroli et al., have shown that in the vicinity of a vortex core the excited state energies are diminished to ΔE ∼ Δ20 /EF Δ0 [64]. Thus, for points near the (H, T ) phase boundary, i.e. for H near Hc2 (T ), there is a gapless region which has received a detailed theoretical examination [65, 66, 67]. The ﬂuctuation (i.e. T1 ) properties in this region are diﬀerent from a type-I system and appear to depend on whether the carriers have a long mean-free path l ξ0 (“clean”) or whether it is short l < ξ0 (“dirty”). In the simpler dirty limit case the electronic properties are local in character, and Cyrot [68] has derived the relation ec T1n =1+ (Hc2 − H) g(t), T1s σkB Tc

(2.3.17)

where t = T /Tc , σ is the normal state conductivity and Hc2 = Hc2 (T ). This relation is only valid for (Hc2 − H) Hc2 , so that it only gives the slope −1 T1n d(T1s )/dH near Hc2 . The function g(t) > 0 for t > 0.6, while g(t) < 0 below that point. One must be very careful in using (2.3.17) to interpret actual data, since T1 is usually measured by scanning temperature rather than ﬁeld. Masuda and Okubo have obtained T1 data on 51 V in V3 Sn, a superconductor with Tc 3.6 K (their sample) and Hc2 (0) = 16 kG [69, 70]. Their data are shown for three values of applied ﬁeld in Fig. 2.12. These authors used (2.3.17) to show that d(T1n /T1s )/dT ∝ g(t) (T ≤ Tc (H)),

(2.3.18)

as well, and have evaluated the constant of proportionality. We note that for H = (4470, 8940, 13410) G, Tc (H) = (3.2, 2.6, 1.8) K and thus t(Hc2 ) = (0.89, 0.72, 0.50) for the three data curves in Fig. 2.12. Thus, the slopes of the data plots at T ≤ Tc are nicely consistent with these parameters, since d(T1n /T1s )/dT is positive for the ﬁrst two, then turns negative for the third, where t(Hc2 ) falls below 0.6. It seems, then, that measurements at low (or zero) ﬁeld on V3 Sn yield a conventional BCS coherence peak, but that it is gradually quenched out by ﬂuxoids at higher ﬁeld values. We mention three other cases of type-II T1 studies at T ≤ Tc . Each is somewhat anomalous in its own way. The ﬁrst is the case of elemental V metal [71], where no convincing coherence peak was observed. The authors considered a number of possible explanations, ﬁnally suggesting that the T1 peak may be suppressed by trapped ﬂux. However, sometime after these results were published, a theory of T1 in the clean limit emerged [65], and this interpretation was applied to the case of vanadium by Pesch [67]. The result

60

2 Introduction to NMR Studies of Metals and Superconductors

was a good ﬁt to the data for both samples [71], with no sign of a coherence peak. It seems, then, that coherence peaks will appear at low ﬁelds in the dirty limit, but not in clean samples. No coherence peaks were observed in any of the V3 X compounds, where X = Ga, Si, Ge, and Pt, in the study conducted by Silbernagel et al., [72, 73]. The ostensible reason for this is disorder caused by the “Martensitic” structural transformation which was reported at temperatures just above Tc in these compounds [74, 75]. The authors oﬀer no further discussion of the point [73]. The third and most anomalous case to be reported was that of niobium [76]. The relaxation of 93 N b nuclear spins was studied in the SC state at ﬁeld values varying from 2.40 kG up to 6.80 kG corresponding to Tc values which vary from 6.8 K down to 3.0 K. Using (2.3.14), Hc2 corresponds to A, so that the given mean-free path l 140˚ A is on the borderline ξ0 ∼ 200˚ between the clean and dirty cases. In any case, the T1 data were found to ﬁt the gapless theory [66, 67] for the higher ﬁeld values. For the lower two ﬁeld values, however, the T1 data were found to execute a deep minimum just below Tc (H), contrary to the gapless theoretical ﬁts. Such behavior is clearly reminiscent of the V3 Sn data in Fig. 2.12, and one might inquire as to whether the calculation of d(T1n /T1s )/dT given in [70] based on (2.3.17) could be applied in this case. The authors did such a calculation and found that the coeﬃcient of g(t) for Nb is smaller by a factor 150–200, so that 2000 GAP = 3.5 kTc(O)

1000

T1

2.6 °K 3.2 °K 3.6 °K

T1T = 0.42 sec °K

msec

15 MHz 1.8 °K

100

50 0.5

1

2 Tc(O)/T

(13410G)

10 MHz

(8940G)

5 MHz

(4470G)

3

Fig. 2.12. A semilog plot of data for T1 of 51 V in V3 Sn vs. Tc (0)/T in the superconducting state for three values of applied ﬁeld [69]. The data shown exhibit coherence peaks for 1341 G and 8940 G, but not for 13410 G. All three plots show deviations from the exponential BCS behavior at the lowest temperatures, an eﬀect attributable to spin diﬀusion to the normal cores. See text for discussion. Reprinted ﬁgure from N. Okuda, Y. Masuda: Phys. Rev. Lett. 20, 1475 (1968). Copyright 1968 American Physical Society

2.3 Static and Dynamic Magnetism in d-band Metals

61

similar behavior cannot be expected on that basis. There seems to be no straightforward explanation for this anomalous result. Type-II T1 Behavior for T Tc −1 For values of T well below Tc , an exponential decay T1s ∝ exp(−Δ0 /kB T ) has generally been found to appear. However, as this intrinsic BCS rate weakens, another contribution attributable to the ﬂuxoids is often seen. Since the energy gap near the ﬂuxoids is very small [64], T1s for a region of area ∼ ξ02 is essentially that of the normal state. When the BCS T1 process in the bulk of the SC material becomes very slow, then a process whereby the nuclear polarization diﬀuses to the normal cores becomes predominant. This process was found to be present in three of the four examples given above [69, 71, 72] but was studied most systematically in the case of V3 Si [72]. 51 V T1s data for V3 Si [72] are plotted semilogarithmically in Fig. 2.13 as a function of Tc /T , where Tc = 15.35 K. Results are given for four

1000

BCS

T1 (BCS Theory) Experimental Data H0 = 4.45 kG

100 T1 seconds 10

H0 = 8.95 kG H0 = 13.4 kG H0 = 17.8 kG

Values of T1 Extrapolated to H0 = 0

1.0

N

T1 (Korringa Theory) 51

V3 Si T1 vs T1 / T T = 4.2 °K – 1.4 °K Tc = 15.35 °K

0.1

0.01

2

4

6

8

10

12

14

Tc / T

Fig. 2.13. A semilog plot of data for T1 of 51 V in V3 Si vs. Tc /T in the superconducting state for four values of applied ﬁeld as shown [72]. The data shown exhibit no coherence peaks, but follow exponential BCS-theory behavior up to Tc /T ∼ 4. Beyond that point the mechanism of spin diﬀusion to the normal ﬂuxoid cores takes over, giving a relaxation rate which is proportional to the applied ﬁeld (i.e., to the ﬂuxoid density), as expected. See text for further discussion. Reprinted ﬁgure from B. G. Silbernagel, M. Weger, J. H. Wernick: Phys. Rev. Lett. 17, 384, (1966). Copyright 1966 American Physical Society

62

2 Introduction to NMR Studies of Metals and Superconductors

diﬀerent ﬁeld values at temperatures in the SC state which extend down below Tc /10. At higher temperatures the data points asymptotically approach the dashed line which represents BCS behavior, i.e. T1s ∝ exp Δ0 /kB T , where Δ0 = 1.76 kB Tc . T1s veers away from the BCS curve at Tc /T ≥ 4, then ranges up to values more than three orders of magnitude longer than its value at Tc . The ﬂattening of these curves is suggested to be caused by spin diﬀusion to the normal cores, which then becomes the only eﬀective T1 mechanism at the lowest temperatures. If the spin diﬀusion time, estimated below, is not an impediment, then at the lowest temperature we should have pξ 2 H T1n = 0 . T1s Φ0

(2.3.19)

where p is a numerical factor of order unity. Equation (2.3.19) simply states that the normal T1 should be diluted by the ratio of pξ02 to the area per ﬂuxoid Φ0 /H. First, we note that 1/T1s should be linear in H, as is clearly the case in A for V3 Si given above, we ﬁnd p = 1.9, Fig. 2.13. With the estimate ξ0 25˚ so that the eﬀective area of normal-state relaxation is a circle of radius slightly smaller than ξ0 for each ﬂuxoid. The corresponding spin diﬀusion times for the results in Fig. 2.13 can be estimated with tdiﬀ ∼

d2 , 4Dsp

(2.3.20)

where d is the distance between ﬂuxoids and Dsp is the spin diﬀusion constant. √ Taking d = [2Φ0 / 3H]1/2 and Dsp ∼ 10−12 cm2 s [77], we ﬁnd tdiﬀ ∼ 13s at H = 4450 G. This is an order of magnitude less than T1 itself, lending credence to the use of (2.3.19). While the foregoing scenario gives an appealingly straightforward interpretation of the V3 Si data for T1s , there did arise in the literature a rather knotty problem in connection with this interpretation. Genack and Redﬁeld suggested some time later [78] that the spin diﬀusion relaxation mechanism in type-II superconductors would not work, because it did not conserve energy. We give the essence of their argument here, then cite further work which provided something of an antidote to this objection. If spin diﬀusion takes place along a ﬁeld gradient, then the simple ﬂip–ﬂop events between neighboring nuclei no longer conserve energy. The diﬀerence in Zeeman (ﬁeld) energies has to be taken up by the spin-spin (usually dipolar) interactions. Viewing this process thermodynamically, the dipolar reservoir then quickly becomes overheated and must, itself, relax to the lattice. The total relaxation process by spin diﬀusion is thus formulated as a dual process, with Zeeman (magnetization) and dipolar energies both diﬀusing to the normal cores in the mixed superconducting state. These processes were analyzed in [78] and found to be too slow to provide the observed T1 processes in V metal [71]. It was concluded that these clearly observed diﬀusion-like T1 processes must originate in some other way [78].

References

63

The problem is, of course, that no other ideas to explain type-II relaxation have been forthcoming. However, more recently, this problem has been revisited in terms of basically the same ideas, but using more sophisticated mathematical methods (see [79] and references cited therein). These authors have analyzed in detail the relaxation curves of 51 V in V metal at T Tc taken from [71] in terms of spatially varying Zeeman and dipolar spin temperatures. They ﬁnd a good ﬁt to the vanadium data, where the dipolar relaxation time constants are relatively short, thus not obstructing the longer diﬀusion-mediated Zeeman T1 ’s. It seems, then, that the phenomenology of (2.3.19) is basically correct, so that low-temperature type-II T1 behavior is clearly understood. This is very important for the interpretation of T1 data for high-Tc systems as well. However, as we shall see, the fundamental behavior of T1 in high-Tc compounds involves SC gap symmetries which usually have line nodes, giving power-law behavior at low temperatures [80]. Thus, the issues regarding T1 data analysis diﬀer somewhat from those of d-band SC metals discussed here. Nonetheless, the spin-diﬀusion-to-normal-cores T1 mechanism in the mixed state has been found to play a signiﬁcant role in the phenomenology of cuprate superconducting T1 eﬀects. The understanding of this eﬀect gained with ordinary 3d metals will be an important resource in the chapters to follow.

References 1. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 13, 14, 15, 19, 22, 33 2. C.P. Slichter, Principles of Magnetic Resonance, 3rd edn. (Springer-Verlag, New York, 1992) 13, 14, 15, 21, 25, 34 3. A. Narath, Hyperﬁne Interactions, ed. by A.J. Freeman and R.B. Frankel (Academic Press, New York, 1967), p.287 13, 35, 36, 37 4. J. Winter, Magnetic Resonance in Metals, (Clarendon Press, Oxford, 1971) 13 5. D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 13, 38, 40, 41, 42, 43, 53, 55, 57, 58 6. M. Tinkham, Introduction to Superconductivity, (McGraw-Hill, New York, 1975) 13, 41, 55 7. J.R. Schrieﬀer, Theory of Superconductivity, (Westview Press, Boulder, 1999) 13, 41 8. R.E. Walstedt, “The two-pulse spin echo revisited”, in Pulsed Magnetic Resonance: NMR, ESR and Optics, ed. by D. M.S. Bagguley (Clarendon Press, Oxford, 1992), p. 242 18 9. E.L. Hahn, Phys. Rev. 80, 580 (1950) 18 10. N. Bloembergen, T.J. Rowland, Phys. Rev. 97, 1679 (1955) 19 11. M.A. Ruderman, C. Kittel, Phys. Rev. 96, 99 (1954); T. Kasuya, Prog. Theoret. Phys. 16; K. Yosida, Phys. Rev. 106, 893 (1957) 19 12. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 19 13. R.E. Walstedt, Phys. Rev. Lett. 19, 146 (1967); 19, 816 (1967) 21

64 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54.

2 Introduction to NMR Studies of Metals and Superconductors J. Van Kranendonk, Physica 20, 781 (1954) 23 J. Bardeen, L.N. Cooper, J.R. Schrieﬀer, Phys. Rev. 108, 1175 (1957) 32, 38 L.C. Hebel, C.P. Slichter, Phys. Rev. 113, 1504 (1957) 32, 40, 41, 42 W.D. Knight, Phys. Rev. 76, 1259 (1949); C.H. Townes, C. Herring, W.D. Knight, Phys. Rev. 77, 852 (1950) 33 J. Korringa, Physica 16, 601 (1950) 33, 34 D.L. Randles, Proc. Roy. Soc. London, Ser. A331, 85 (1972) 34 R.E. Walstedt, Y. Yafet, A.I.P. Conference Proceedings 24, 522 (1974) 34 D. Pines, in Solid State Physics, vol. I, ed. by F. Seitz, D. Turnbull (Academic Press, New York, 1954), p. 1 36, 37, 44 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 36, 44 K. Yosida, Phys. Rev. 110, 769 (1958) 38, 40 F. Reif, Phys. Rev. 102, 1417 (1956); 106, 208 (1957) 39 G.M. Androes, W.D. Knight, Phys. Rev. 121, 779 (1961) 39 W.A. Hines, W.D. Knight, Phys. Rev. Lett. 18, 341 (1967); Phys. Rev. B4, 893 (1971) 39 R.H. Hammond, G.M. Kelly, Rev. Mod. Phys. 36, 185 (1964) 39, 40 See Ref.5 for a more detailed account of these developments 39 R.A. Ferrell, Phys. Rev. Lett. 3, 262 (1959) 39, 40 P.W. Anderson, Phys. Ref. Lett. 3, 325 (1959) 39 A.A. Abrikosov, L.P. Gorkov, Zh. Eksp. Teor. Fiz. 42, 1088 (1962); [Sov. Phys.–JETP 15, 752 (1962)] 39 P.W. Anderson, J. Phys. Chem. Solids 11, 26 (1959) 39, 43 F. Wright, W.A. Hines, W.D. Knight, Phys. Rev. Lett. 18, 115 (1967) 39 R.H. Hammond, G.M. Kelly, Phys. Rev. Lett. 18, 156 (1967) 40 H.L. Fine, M. Lipsicas, M. Strongin, Phys. Lett. 29A, 366 (1969) 40 Y. Masuda, A.C. Redﬁeld, Phys. Rev. 125, 159 (1962) 41, 42, 43 H. B ommel, Phys. Rev. 96, 220 (1954) 41 C.R. Leavens, J.P. Carbotte, Solid State Commun. 9, 75 (1971); Ann. Phys. (N.Y.) 70, 338 (1972) 43 Y. Masuda, Phys. Rev. 126, 1271 (1962) 43 J.D. Williamson, D.A. MacLaughlin, Phys. Rev. B8, 125 (1973) 43 J.R. Clem, Phys. Rev. 148, 392 (1966) 43 V. Heine, Phys. Rev. 107, 1002 (1957) 44, 46 J.H. Wood, G.W. Pratt Jr., Phys. Rev. 107, 995 (1957) 44, 46 R. Kubo, Y. Obata, J. Phys. Soc. Japan 11, 547 (1956) 44, 46 A.M. Clogston, A.C. Gossard, V. Jaccarino, Y. Yafet, Phys. Rev. Lett. 9, 262 (1962) 44, 49, 57, 58 A.M. Clogston, V. Jaccarino, Phys. Rev. 121, 1357 (1961) 45, 47 R.E. Watson, A.J. Freeman, Hyperﬁne Interactions, ed. by A. J. Freeman, R.B. Frankel (Academic Press, New York, 1967), p. 53 46, 47 A.M. Clogston, V. Jaccarino, Y. Yafet, Phys. Rev. 134, A650 (1964) 47, 48, 49 F.E. Hoare, J.C. Matthews, Proc. Roy. Soc. (London) A212,137 (1952); D.W. Budworth et al., ibid. A257, 250 (1960) 49 L.P. Kadanoﬀ, Phys. Rev. 132, 2073 (1963) 50 Y. Obata, J. Phys. Soc. Japan 18,1020 (1963) 50, 51 Y. Yafet, V. Jaccarino, Phys. Rev. 133, A1630 (1964) 50, 51, 52 R.E. Watson, A.J. Freeman: Phys. Rev. 123, 2027 (1961) 52 J. Butterworth, Phys. Rev. Lett. 5, 305 (1960); J. Butterworth, Proc. Phy. Soc. London 85, 735 (1965) 53

References

65

55. A.A. Abrikosov, Zh. Eksperim. i Teor. Fiz. 32,1442 (1957) [English transl.: Soviet Phys.- JETP 5, 1174 (1957) 54, 55, 57 56. W.H. Kleiner, L.M. Roth, S.H. Autler, Phys. Rev. 133, A1226 (1964) 54, 55, 56 57. T.J. Greytak, J.H. Wernick, J. Phys. Chem. Solids 25, 535 (1964) 54 58. P. Pincus, A.C. Gossard, V. Jaccarino, J.H. Wernick, Phys. Lett. 13, 21 (1964) 54, 57 59. J.-M. Delrieu, J.-M. Winter, Solid State Commun. 4, 545 (1966) 55 60. A.G. Redﬁeld, Phys. Rev. 162, 367 (1967) 55, 57 61. D. Rossier, D.E. MacLaughlin, Phys. Kondens. Mater. 11, 66 (1970) 55 62. P.R. Radebaugh, P. Keesom, Phys. Rev. 149, 209 (1966); 149, 217 (1966) 56 63. G. Eilenberger, Phys. Rev. 153 584 (1967) 56 64. C. Caroli, P.G. deGennes, J. Matricon, Phys. Lett. 9, 307 (1964) 59, 61 65. U. Brandt, W. Pesch, L. Tewordt, Z. Physik 201, 209 (1967) 59 66. U. Brandt, Phys. Letters 27A, 645 (1968) 59, 60 67. W. Pesch, Phys. Letters 28A, 71 (1968) 59, 60 68. M. Cyrot, J. Phys. (Paris) 27, 283 (1966) 59 69. N. Okuda, Y. Masuda, Phys. Rev. Lett. 20, 1475 (1968) 59, 60, 61 70. Y. Masuda, N. Okuda, J. Phys. Soc. Japan 26, 309 (1969) 59, 60 71. W. Fite, A.G. Redﬁeld, Phys. Rev. 162, 358 (1967) 59, 60, 61, 62, 63 72. B.G. Silbernagel, M. Weger, J.H. Wernick, Phys. Rev. Lett. 17, 384, (1966) 60, 61 73. B.G. Silbernagel, M. Weger, W.G. Clark, J.H. Wernick, Phys. Rev. 153, 535 (1967) 60 74. B.W. Batterman, C.S. Barrett, Phys. Rev. Lett. 13, 390 (1964) 60 75. A.C. Gossard, Phys. Rev. 149, 246 (1966) 60 76. D. Rossier, D.E. MacLaughlin, Phys. Rev. Lett. 22, 1300 (1969) 60 77. A.G. Redﬁeld, W.N. Yu Phys. Rev. 169, 443 (1968); 177, 1018 (1969) 62 78. A.Z. Genack, A.G. Redﬁeld, Phys. Rev. Lett. 31, 1204 (1973) 62 79. G.B. Furman, S.D. Goren, Phys. Rev. B68, 064402 (2003) 63 80. H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990); N. Bulut, D. Scalapino, Phys. Rev. B45, 2371 (1992) 63

This page intentionally blank

3 The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR

The purpose of this chapter is twofold. First, it is partly historical, to recount the somewhat uncertain beginnings and explain how ideas developed the way they did, and secondly, to review the early milestones which laid the foundations for the many years of study which were to follow. These agendas will unfold simultaneously in an essentially chronological recounting of the important ﬁrst steps in constructing the ediﬁce of high-Tc NMR phenomenology which exists today. Although the cuprates form a large family of compounds1 , in recounting the major accomplishments in the ﬁeld of NMR studies, one’s attention is drawn to three compounds, namely La2−x Srx CuO4 (LSCO:x), YBa2 Cu3 O7−x (YBCO7-x), and YBa2 Cu4 O8 (Y248). These three have played a major role, both in terms of experimental results and theoretical interpretation. There are other interesting compounds with higher Tc ’s (e.g. Tl2 Ba2 CaCu2 O8 ) and with quantum chemistry just as clean (Hg2 Ba2 Cu2 O4 ). It seems that it was just an historical accident that the three listed above became prominent. Accordingly, they will become our main focus. In Sect. 3.1 we review the structures, phase diagram, and some of the early theoretical models regarding transport and quasiparticle dynamics. Of course with a research topic as completely new and unfamilair as the cuprates, one spends a great deal of time and eﬀort at the outset simply establishing the basic experimental features of the system under investigation. Some of this activity is reviewed in Sect. 3.2, where we shall see that the anomalous nature of the spin dynamics (i.e. T1 ) emerged from the earliest papers to appear. A major milestone in understanding all HF eﬀects in the cuprates came with the Mila-Rice-Shastry picture of predominant transferred HF couplings with their quantum-chemical foundations [2, 3]. This work, presented and discussed in Sect. 3.3 for 63,65 Cu, established a model HF Hamiltonian for the principal nuclei which has been an important touchstone ever since. The 1

See, for example, the wide variety of cuprate structures reviewed by Hazen [1].

R.E. Walstedt: The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR, STMP 228, 67–114 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 3

68

3 Preliminary Steps in Cuprate NMR

application of this picture to the NMR studies of planar 17 O and the 89 Y in the YBCO structure is the subject of Sect. 3.4. The relationship between nuclear spin-lattice relaxation (T1 ) and the dynamical susceptibility χ(q, ω) via the ﬂuctuation-dissipation theorem has been well known for many years [4]. With the cuprates, however, this quantity quickly became the basis for the expression of static and dynamic NMR, for inelastic neutron scattering (INS) results, as well as for theoretical modeling. In Sect. 3.5 we review the derivation of the basic results and give standard expressions for T1 at various nuclear sites in cuprates for reference throughout the book. Finally, in Sect. 3.6 the early and highly signiﬁcant d-wave interpretation of T1 in the superconducting state by Monien and Pines [5] is reviewed in some detail. This was based on an RPA model of the dynamical susceptibility which formed a basis for future modeling of normal-state dynamics as well [6, 7]. As we shall see throughout the volume, fundamentally d-wave behaviors for T1 and for the transverse decay constant T2g were ﬁrmly established several years in advance of the Josephson junction phase-boundary results which ﬁnally turned the tide on the d-wave vs. s-wave question.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO The ﬁrst high-Tc materials to be announced [8] left some degree of uncertainty about the actual crystal structures of the superconducting phases. In the weeks that followed, among the ﬁrst structural reﬁnements to be announced were those of La2−x Srx CuO4 (LSCO) [9] and Y Ba2 Cu3 O7−δ (YBCO) [10]. For that reason as well as the fact of their ease of synthesis into high-quality specimens and of subsequent characterization, these two compounds and closely related materials have been a strong focus of NMR/NQR studies from the inception down to the present era. In this section we present a brief discussion of the structures, doping, and quasiparticle dynamics in these typical cuprates. Discussions of NMR studies on the LSCO family of compounds will be given in Chaps. 4 and 6. 3.1.1 LSCO: A superconductor with Tc (max) 40 K LSCO has the K2 N iF4 crystal structure shown in Fig. 3.1(a) [11]. The key structural element in all of the cuprate superconductors is the CuO2 quadratic array (Cu-O1 in Fig. 3.1(a)), which has been identiﬁed as the region where the hole current is carried in these systems. Note that the O1 ions also form a ◦ quadratic √ array rotated 45 from that of the Cu, and having a lattice constant of a/ 2. Cu ions in adjacent planes are staggered, so that AFM couplings between layers are exremely weak. The physics of these structures is strongly two dimensional.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO

69

(a)

(b)

Cu (2) Y

O (2)

O (3)

c

Ba O (4) O (1) Cu (1)

b

La, Sr O2 O1 Cu

a

Fig. 3.1. (a) The (K2 NiF4 ) structure of La2−x Srx CuO4 , showing the locus of the CuO2 conducting plane. The Sr2+ dopant ions go substitutionally into the La3+ sites, leading to a set of mobile holes which run on the square lattice of planar O2− ions [11]. The structure shown has tetragonal symmetry. However, below a few hundred K an orthorhombic distortion sets in, where the CuO6 octahedra tilt through small angles in the [110] planes. Reprinted ﬁgure from J.D. Jorgensen, H.-B. Sch¨ uttler, et al., Phys. Rev. Lett. 58, 1024, (1987). Copyright 1987 American Physical Society. (b) The YBa2 Cu3 O7−x structure is shown with the chain layers (Cu(1)) on the top and bottom and a pair of Cu(2)O(2,3)2 layers in the middle [12]. Note that there is no bonding between adjacent Cu(2) layers except via rather inert Y3+ ion cores. The O1 sites are shown ﬁlled, forming chains along the b axis. The structural symmetry is orthorhombic. Reprinted ﬁgure from J.D. Jorgensen, B.W. Veal, W.K. Kwok, et al., Phys. Rev. B36, 5731 (1987). Copyright 1987 American Physical Society

The physics of transport is dramatically diﬀerent in the cuprates from what it is in an ordinary d-band metal. For LSCO we consider ﬁrst the case of x = 0, i.e. La2 CuO4 . With the expected valence (La3+ , Cu2+ , and O2− ), the conduction plane consists of Cu2+ ions, i.e. with a single hole in the d shell (dx2 −y2 ) plus O2− closed-shell ion cores. The 3d holes are strongly hybridized with the O2− 2p orbitals, such that over 30% of the localized d-hole density resides on the planar oxygens [13, 14]. In the conventional picture of weaklyinteracting fermions, this would simply be a half-ﬁlled band like an alkali metal. On the contrary, however, the hopping process which might lead to hole conduction is strongly inhibited by coulomb repulsion (U ∼ 10 eV ) on the Cu+2 ion complexes in what is known as a “Mott insulator” [15]. Instead, immobile S = 1/2 local moments on the Cu+2 ions condense to an insulating, antiferromagnetic ground state with TN 325 K. In order to generate conductivity in the CuO2 planes, it is necessary to dope additional holes into the system. This may be done by replacing some of the La+3 ions with Sr+2 ions

70

3 Preliminary Steps in Cuprate NMR

as in LSCO. For each such subsititution a hole must appear in or near the CuO2 plane. Above a small threshold concentration these holes become mobile. In the Zhang-Rice singlet picture, they combine with Cu2+ holes to form a singlet quasiparticle. After considerable investigation and debate, such singlets have ﬁnally been concluded to have negligible HF interactions on their own. It has been suggested that they serve the function of rendering the Cu2+ holes itinerant [16]. The LSCO Phase Diagram The phase diagram of Fig. 1.1 illustrates the resulting behavior as a function of the hole-doping parameter δ ∼ x. First, the antiferromagnetism collapses very quickly with hole doping. At x ∼ 0.02 there is an insulator-to-metal transition, though conductivity is still rather poor. In this region, spin-glassbehavior is thought to occur. At x 0.05 the superconducting phase appears, although the normal-state conductivity is still that of a very bad metal. With an optimum concentration of x = 0.15, Tc then peaks at ∼ 40 K. Beyond that point is the overdoped region, where the system becomes more and more like a normal metal. Tc then declines to zero at x ∼ 0.35. The pattern seen with LSCO is repeated with essentially every cuprate superconductor, except that in many cases it is not possible to vary the carrier content all the way from the antiferromagnetic phase through superconductivity and into the overdoped phase. The line in Fig. 1.1 running from the top of the superconducting dome upward to the left (“S”) is the locus of maxima in the spin susceptibility, and also an approximate boundary between the tetragonal (above) and orthorhombic (below) phases in LSCO. However, there is a “crossover” line in approximately that position in various theories of magnetic behavior [17, 18], for which there is growing experimental evidence in other cuprate compounds. In the Barzykin-Pines model this is a boundary between mean-ﬁeld behavior for the dynamical exponent (z = 2) on the high-temperature side and quantum-critical (z = 1) behavior on the low-temperature side. NMR evidence supporting this picture will be presented and discussed in Chap. 6. 3.1.2 The 92 K Superconductor YBa2 Cu3 O7−x (YBCO) Many cuprates have multiple CuO2 planes neighboring each other with a single layer of cations between them. Y Ba2 Cu3 O7−x (YBCO7-x) has two such neighboring planes separated by a single layer of Y 3+ ions, as shown in Fig. 3.1(b) [12]. This structure also features a “chain” layer, known as the Cu(1) sites, which is a quadratic array of copper ions, but where half of the ligand O2− ions seen in the Cu(2) layers are absent, leaving 1D Cu-O chains running along the b axis of the crystal. The chain sites are a complication in understanding the behavior of YBCO, because as we shall see below, the Cu(1) and Cu(2) sites behave rather diﬀerently.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO

71

On the other hand, regarding the level of mobile carriers, the YBCO7-x system is self-doping. The minimum doping level is eﬀectively zero when x = 1, giving six oxygens per formula unit. With the expected valencies (Y3+ , Ba2+ , Cu(1)+ , Cu(2)2+ , and O2− ), YBa2 Cu3 O6 is in a vacuum state for conductivity similar to La2 CuO4 . In this structure there are no oxygens at all in the Cu(1) planes, and their corresponding valence state is Cu1+ . The maximum doping occurs when x = 0, whereupon the Cu(1) chains are fully oxygenated, and one has an average valence of 2.33 per Cu ion. This is considered to be slightly overdoped, where the maximum Tc 92 K occurs for x 0.1. It is noteworthy, however, that YBCO7 is stoichiometric and therefore has minimal disorder, i.e. far less disorder than optimally doped LSCO. 3.1.3 Physical Models of Itinerant Quasiparticles in Cuprates At optimum doping levels, then, the cuprate conduction planes then appear to contain a small concentration of mobile holes moving in a sea of S = 1/2, exchange-coupled local moments. Because of the coulomb repulsion, these holes are thought to be restricted to the oxygen sites. The description of this mixture as a superconducting quantum ﬂuid is therefore dramatically diﬀerent from a simple 3d-band of partially-occupied Bloch functions. It has posed a stiﬀ theoretical challenge from the beginning, and even now there is not a clear consensus about it. One thing we understand is that it is not a set of exchange-coupled local moments simply coexisting with a hole band of itinerant fermions. For example, at T Tc all spin magnetism decays to a small fraction of its normal-state level, as we know from NMR shift and relaxation measurements (Sect. 3.2.5). Upon a (low, but) suﬃcient level of doping, then, all Cu2+ holes become eﬀectively itinerant and part of a superconducting quantum ﬂuid at T < Tc . The t-J Model How this takes place has been the topic of many theoretical papers. We mention here the “t-J” model [19, 20], which is an approximation to the one-band Hubbard model. A number of theory papers have shown that the t-J model Hamiltonian (here simplﬁed) Ht−J = J Si · Sj + t [c∗i cj + ci c∗j ] (3.1.1) i,j(nn)

i,j(nn)

results in a band of itinerant quasiparticles of width ∼ J ∼ 0.15 eV [21]. Zhang-Rice Singlets A detailed model for the structure of the quasiparticles themselves, known as the “Zhang-Rice singlet model”, appeared very early on and is still considered an interesting conceptual picture [16]. In this model the mobile holes form

72

3 Preliminary Steps in Cuprate NMR

a singlet complex with neighboring Cu2+ “localized” holes, rendering them itinerant. In spite of their small numbers, the mobile holes are said to render all of the Cu2+ moments eﬀectively itinerant and part of a quantum liquid which condenses into a superconducting spin-paired ground state. That this actually occurs is concluded from decay of the Cu(2) Knight shift and relaxation rate, and thus the spin paramagnetism of YBCO7, to a value small compared with its normal-state value for T Tc (see Sect.3.2). The “Oxygen Hole Band” Issue Contrary to the Zhang-Rice singlet picture, many early papers considered that the doped holes in cuprates would result in a separate hole band residing on the oxygen lattice with its own independent HF eﬀects. This idea was often advanced when it seemed that the ﬂuctuating S = 12 moments which occupy the Cu2+ sites would not give an adequate explanation of NMR shift and relaxation eﬀects at all sites studied. Often the papers concerned made important contributions in spite of maintaining this point of view. Eventually, as will become clear in Chap. 4 and 5, it was realized that there was simply no need for oxygen hole bands with independent HF eﬀects and no evidence for them either. This issue will be mentioned as appropriate in reviewing the relevant literature.

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO It was, of course, realized immediately that NMR studies of the 63,65 Cu, 17 O, and in the case of YBCO, 89 Y nuclear spins could yield a great deal of detailed information about static and dynamic fermion behavior in these systems. Perhaps because of its very high Tc value, there was an intense focus on YBCO at the outset, which was facilitated by the ease with which samples could be synthesized. Accordingly, there were a great many NMR papers on YBCO, mainly fully doped (YbCO7) during the ﬁrst year or two. Our focus in this section will be these early studies of YBCO and the issues they raised. LSCO eventually received its share of attention, and will be addressed both in the next chapter and in Chap. 6. In this section we examine the developments which took place during 1987-88 following the discovery of high-Tc superconductors. It was a time of intensive activity, but at the same time, sample preparation was still in a rather primitive state. There was a deﬁnite focus on YBCO7, the 90 − 92 K superconductor, because of its spectacularly high Tc value and because it is a stoichiometric compound. Even so, almost all of the samples studied during this period were either random powders or milligram-scale crystals which gave narrow resonance lines, but very small signals. The random powders gave (− 12 ↔ 12 ) transition spectra ∼ 5T wide in a typical laboratory (7–8 T) ﬁeld,

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO

73

and it took a great deal of noise averaging to obtain a single spectrum. Only with NQR was it possible to do a T1 measurement. Even so, many basic issues concerning the NMR/NQR study of the cuprates were addressed during this time period, and impressive progress was made toward their resolution. At the end of the two-year period we are focusing on, there were two events which marked the beginning of a more settled period, namely the appearance of the Mila-Rice-Shastry papers to clarify the quantum chemistry and transferred HF interaction picture [2, 3], and secondly, the advent of the oriented powder sample preparation method, which dramatically improved the prospects for precise determination of nearly all experimental NMR parameters. The Mila-Rice-Shastry picture for HF couplings in YBCO is presented in Sect. 3.3. 3.2.1 NMR Shift and Relaxation of the

89

Y in YBCO7

Not surprisingly, the ﬁrst papers on cuprate nuclear spin dynamics to appear featured studies of 89 Y T1 behavior in both the normal and superconducting states [22, 23]. The 89 Y nuclei have very small, I = 1/2 nuclear spin moments, but are 100% abundant. They are very weakly hybridized with the Cu(2) 3d moments, giving them a long T1 , but a relatively isotropic NMR shift, so that they are easy to study in a random powder sample. The quick appearance of these 89 Y studies was a harbinger of a great many fruitful 89 Y NMR studies to follow. The T1 data from [22], shown in Fig. 3.2, immediately revealed two striking behaviors. First, T1 follows a Korringa-like, inverse–T law in the normal state, giving actually a misleading impression of the behavior at its neighboring Cu(2) site to be unveiled soon after. The normal-state data of [23] were in agreement with this ﬁnding, and both papers found a normal-state shift K 0.02% as well. As for T1 , there is no hint of any coherence peak below Tc ; moreover, the decline of 1/T1 below Tc is remarkably abrupt. It behaves in a roughly exponential fashion when plotted vs. T /Tc , and has a slope much larger that the expected asymptotic BCS slope (plotted). If the BCS curve reﬂects a gap 2ΔBCS 3.5 kB Tc , the 89 Y T1 curve shows a gap value 2ΔY 11.2 kB Tc . While such a characterization is somewhat superﬁcial at this stage, it shows at least that the superconducting T1 behavior is dramatically diﬀerent from that of any ordinary d-band metal. (See Sect. 3.6 for further elucidation of T1 behavior below Tc .) NMR/NQR Studies of and T1 (T)

63,65

Cu(1, 2): The Quadrupolar Tensor

Next, many papers appeared in which the four-line NQR spectrum (or part thereof) was reported (63,65 Cu(1) and 63,65 Cu(2)) in YBCO7 [23, 24, 25, 26]. Of course, for the I = 3/2, 63,65 Cu nuclei the value of η cannot be derived from NQR frequencies alone. The full quadrupolar frequency tensor has been

74

3 Preliminary Steps in Cuprate NMR

Spin–lattice Relaxation Rate (s–1)

10–1 YBa2Cu3O9 – δ

Korringa 10–2 89Y

fo = 12.2 MHz BCS

0

1 Tc / T

2

Fig. 3.2. 1/T1 of 89 Y in Y Ba2 Cu3 O9−δ is plotted vs. Tc /T in a semilog plot, where δ 2.1 [22]. In the normal state the data are within error limits of a Korringa curve (solid line, 1/T1 ∝ T ). Below Tc the measured relaxation rate drops much faster than the BCS energy gap would allow (dashed curve - BCS). See text for discussion. Figure reprinted from J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts: Sol. St. Comm. 63, 847 (1987). Copyright 1987 Elsevier Ltd.

deduced from NMR studies of small single crystals of YBCO7-x, with x 0 [27, 28], yielding essentially equivalent results. After some reﬁnement, these tensors may be given (in MHz) as ναα = (-19.03(7), 19.17(7), -0.16(3)) for Cu(1) and (15.94(5), 15.56(5), -31.50(5)) for Cu(2) at 100 K [29], where the numbers in parentheses are the uncertainties in the last digit quoted. This quadrupolar tensor has been analyzed by Frank Adrian [30]. NQR Studies of Cu(1,2) T1 in YBCO7 NQR was used to measure T1 for both the 63 Cu(1) and 63 Cu(2) lines at 22 M Hz and 31.5 M Hz, respectively, giving the ﬁrst glimpse of T1 behavior for the copper sites in the cuprates [24, 23]. The T1 data from [24] are displayed in Fig. 3.3, where markedly diﬀerent behavior is seen to occur for the two copper sites, both above and below Tc . In the normal state, the Cu(1) site T1 behavior is rather Korringa-like, similar to the 89 Y , whereas the Cu(2) site 1/T1 behaves initially like a+bT , but then ﬂattens oﬀ near room temperature. The normal state data from [23] behave in a similar fashion to that in Fig. 3.3, except that T1 values appear to be about 15% longer than from [24]. The value quoted in [31] is also slightly longer, but well within error limits of the data in Fig. 3.3. The reader may note that diﬀerent references cited here give T1 values which are deﬁned variously, none of which agree with the discussion

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 30

(T1T)–1 (sK)–1

12.0

RELAXATION RATE (103 s–1)

75

10.0 8.0

20 10 0 60

6.0

80

100

120

140 160

TEMPERATURE (K)

4.0 2.0 0

0

100 200 TEMPERATURE (K)

300

Fig. 3.3. The 63 Cu relaxation rate 1/T1 is shown plotted vs. T for Cu(1) and Cu(2) in a YBCO7 sample (Tc 92 K) [24]. The NQR rate is shown, which is 3 times the formally deﬁned rate 1/T1 . Reprinted ﬁgure from W.W. Warren, Jr., R.E. Walstedt et al: Phys. Rev. Lett. 59, 1860 (1987). Copyright 1987 American Physical Society

of T1 in Sect. 1.1.5. Recall that the NQR value of relaxation time measured for I = 3/2 is 1/3 of the formally deﬁned T1 (see Sect. 1.1.5). Finally, regarding the data shown in Fig. 3.3, we shall not consider the temperature dependence of T1 in depth until Chap. 5. We comment brieﬂy on the general features of these data. Below Tc the Cu(2) relaxation rate declines very steeply, rather like the 89 Y data in Fig. 3.2. The data from [23] for T < Tc are also similar, the main diﬀerence being that the Cu(2) curve is extended to somewhat lower temperatures, where it is found to level oﬀ markedly. Such behavior is very likely sample dependent. Fitting the Cu(2) rate below Tc (Fig. 3.3) to a BCSstyle exponential decay, a reasonable ﬁt gives 2ΔY 8.3 kB Tc with Tc = 92 K [24]. This is a qualitatively similar result to the slope found above for the 89 Y , but since the latter studies were done in a ﬁeld of 50 kG and the present data were taken in zero ﬁeld, a quantitative comparison may not be warranted. As we shall see in Sect. 3.6, this low-temperature behavior is characteristic of d-wave pairing. 3.2.2 Establishing the Site Assignment for the Cu(1) and Cu(2) NQR Spectra Following the publication of [24] (and [32]) there was a brief period of controversy, caused by the fact that the identiﬁcation of the NQR frequencies with the Cu(1) and Cu(2) sites in these papers was reversed from the correct assignment stated above. The T1 results are valid when attributed to the correct sites, but a large portion of the discussion, based on the incorrect identiﬁcation, would need to be revised [24, 32]. Since a number of discussion points have also been rendered moot by later insights and improved understanding,

76

3 Preliminary Steps in Cuprate NMR

we shall attempt no such revision here. The incorrect assignment was made on the basis of (i) similarity of normal-state T1 curves between the 63 Cu(1) (Fig. 3.3) and the 89 Y (Fig. 3.2) and (ii) on the relative intensities of the 21 M Hz and 31.5 M Hz NQR lines in [24] as well as in other papers [25, 26]. These intensities were essentially reversed from the 2:1 ratio expected from the Cu(2):Cu(1) site count, showing the general unreliability of NQR intensities recorded at diﬀerent frequencies. Following these papers, other papers appeared whose main purpose was to document the correct site assignment. References [27, 28] argued the correct assignment on the basis of data for the EFG tensor. After all, the Cu(2) site has very nearly axial symmetry, while Cu(1) does not, features which are expressed very strikingly in the EFG tensor. Meanwhile, [33] argued the case on the basis of 63 Cu relaxation studies conducted on a sample of GdBa2 Cu3 O7 . The Gd3+ ions each possess a localized moment of nearly 7μB , which ﬂuctuates as a consequence of exchange couplings with the other Gd3+ moments. The nearby Cu(2) nuclei are strongly relaxed by ﬂuctuating dipolar ﬁelds from these moments, whereas, the Cu(1) are largely unaﬀected. These observations conﬁrm the correct assignment. The (− 12 , 12 ) Quadrupolar Powder Pattern for Cu(2) in YBCO7 The authors of [24, 32] also conducted NMR intensity studies for the purpose of site veriﬁcation, partitioning the (-1/2,1/2) NMR line intensity for YBCO7 into Cu(2) and Cu(1) contributions [34] (see also [27]). The intensity of the NMR spectrum was calibrated by comparison with spectra from a known quantity of Cu2 O, yielding an absolute intensity of 2.7 ± 0.3 Copper ions per unit cell of the YBCO7. The Cu(2):Cu(1) intensity ratio was found to be 2 within experimental error. A by-product of the latter exercise was a very precise ﬁt to the η = 0, second-order quadrupolar powder pattern for the (-1/2,1/2) (central) transition at T = 105 K [34], using the same procedures which gave sample powder patterns in Figs. 2.2 and 2.4. This ﬁt is shown in Fig. 3.4, both as spin echo intensity data recorded at pulse separation τ = 20 μs and as the extrapolated, τ = 0 curve with its ﬁt to a quadrupolar powder pattern form (see Fig. 2.2) with Gaussian broadening shown as a dashed line. The residual area above the dashed line ﬁt curve is identiﬁed as the Cu(1) site intensity. See [34] for a detailed discussion. Shift values for the Cu(2) are also deduced from this ﬁt (see below). 3.2.3 Variation of the

89

Y shift K89 (x) with x for YBCO6+x

A study of the doping dependence of the 89 Y NMR shift K89 (x) in YBCO6+x by Alloul and coworkers [35] uncovered some very interesting behavior regarding the Pauli paramagnetism of this system. For x ≥ 0.4 they found an essentially linear increase K89 (x) ∝ (x − 0.4), below which K89 levelled oﬀ to a value which remained constant throughout the insulating phase. It was

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 5

SPIN ECHO AMPLITUDE (ARBITRARY UNITS)

4

77

63Cu:YBa Cu O 2 3 7

(a)

3 2 τ = 20μsec 1

0 (b)

4

2 τ=0 0 70

72

74

76

78

Ho(kG)

Fig. 3.4. NMR ﬁeld-sweep spectrum of 63 Cu in YBCO7 at T = 105 K and an NMR frequency of 84.07 M Hz. Part (a) is uncorrected data taken with a spin-echo pulse separation of 20 (μs). In part (b) the signal has been extrapolated back to τ = 0 using measured values of T2 at various points in the spectrum. The outer singularity peaks are characteristic of an η = 0 (-1/2,1/2) quadrupolar powder pattern. Such a powder pattern has been ﬁtted to these peaks (dashed line), and serves to distinguish the Cu(2)-site intensity from that of the Cu(1) sites, which lies above the dashed line. There is a spurious peak to the left of center thought to be caused by accidental powder orientation in this otherwise random sample. The calculated Cu(1) intensity with this scheme is 54% of that assigned to the Cu(2) sites. Reprinted ﬁgure from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B38, 9299 (1988). Copyright 1988 American Physical Society

concluded that the latter value of shift K89 2.25 × 10−5 relative to the shift of YCl3 is actually the zero of K89 in this system. The discrepancy with the YCl3 was attributed to a diﬀerence in the chemical shifts of the two systems. However, similar results by Balakrishnan et al. [36] included a study of chemical shifts suggesting that the actual chemical shift in YBCO6+x at low values of x is somewhere above 200 ppm relative to YCl3 , contrary to the foregoing

78

3 Preliminary Steps in Cuprate NMR

conclusion. Eventually, the latter value gained acceptance as the correct zero for the 89 Y spin paramagnetic shift in YBCO. The behavior of K89 (x) with doping is shown in Fig. 3.5. The change in K89 above x = 0.4 is seen to be negative and is attributed to the core polarization of the Y3+ 4d orbitals hybridized into the conduction band in the CuO2 planes of YBCO6+x. The Pauli paramagnetism varies in a similar fashion to K89 , so that in a plot of K89 (x) vs. χm (x) the behavior for x > 0.4 is linear with a slope dK89 /dχm = -4.6 (emu/mole)−1. This is much smaller than would correspond to the full core polarization HF ﬁeld, showing that the 4d admixture is very slight. The authors comment that this behavior seems contrary to the proposed separation of spin and charge behavior of the RVB model [19, 20].

89Y

8

NMR

YBa2Cu2O6 + x

Bo = 7.5 Tesla T = 293 K 6

–105 ΔK

4

2 AF 89YCl

0

–2

3

K=0

0

0.2

0.4

0.6

0.8

1

X 89

Fig. 3.5. The room temperature Y NMR shift in YBa2 Cu3 O6+x is plotted for a series of x value ranging from nearly zero to one. The is interpreted (see text) to mean that the Pauli paramagnetism vanishes below X = 0.4 and the shift value below that point is simply the diﬀerence in chemical shifts between YBCO6 and YCl3 . Figure reprinted from H. Alloul, P. Mendels, et al., Phys. Rev. Lett. 61, 746 (1988). Copyright 1988 American Physical Society

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO

3.2.4 Physical Models for the Relaxation of

63

79

Cu(2) in YBCO7

One of the major challenges to the NMR community and to the theorists as well has been the interpretation of the copper-site T1 data, which is to say the magnitude of T1 , its anisotropy, and its temperature dependence. We discuss the temperature dependence of T1 (for all sites) in Chap. 5, and as of this writing, it is still an unsettled issue. The magnitude and anisotropy of T1 , however, came to light early and were the main inﬂuences which brought about the Mila-Rice discussion and formulation of the problem. We review here two background developments which highlighted the situation, namely the model treatments of T1 in experimental papers by Walstedt et al. [37] and by Pennington et al. [29]. Reference [37] reported the ﬁrst data on the anisotropy of the 63 Cu(2) T1 , ﬁnding T1c /T1ab 3.5.This was done with a random powder sample, using NQR (θ = 0), and the up-ﬁeld and down-ﬁeld singularities of the (-1/2,1/2) powder pattern (θ 43◦ and θ = 90◦ , respectively). The data were not ﬁrstrate, but the result for T1c /T1ab held up in later studies with oriented powders [38]. The paper goes on to discuss the feasibility of explaining the foregoing T1 data using the typical formulation of spin-lattice relaxation in 3d metals given by Yafet and Jaccarino [39] and discussed in detail in Sect. 2.3. The hyperﬁne constants are well-known for the Cu2+ , and the density of states is derived from the susceptibility, where the orbital component is estimated and subtracted oﬀ. The result is, if anything, an overestimate for n(EF ). The normally dominant orbital relaxation mechanism is vitiated in YBCO by the nearly pure dx2 −y2 ground state, which has negligible matrix elements for the orbital HF process. As a result, the estimated relaxation rate with this scheme falls far short of the magnitude of the observed rates, and the peak anisotropy available falls well short of the measured ratio. The standard dband relaxation model was concluded to be incapable of accounting for the cuprate T1 data. 3.2.5 Introduction of the Spin Hamiltonian Model for the Cu2+ A diﬀerent tack was taken by Pennington, Durand, et al. [29]. The Cu(2) relaxation tensor was measured using NMR on single crystal samples, ﬁnding similar numbers, but an anisotropy of 4.2, rather larger than the 3.5 reported in [37]. This discrepancy is most likely a diﬀerence in samples. In any case it has never been resolved. For the analysis of T1 these authors adopt a model of ﬂuctuating Cu2+ local moments, adopting a spin Hamiltonian form for the spin HF tensor [40] and simply deducing the anisotropy of the spin HF ﬁeld from the corresponding anisotropy of T1 for Cu(2) given above. Simultaneously, however, Takigawa, Hammel et al. announced their result that the c axis NMR shift changed very little below Tc , while other components underwent substantial changes [33, 41]. They concluded that the spin paramagnetism declined eﬀectively to zero for T Tc . It followed that the net c axis

80

3 Preliminary Steps in Cuprate NMR

spin HF component for Cu(2) is nearly zero! From this observation sprang the Mila-Rice model for Cu(1,2) HF couplings, presented in Sect. 3.3. Both papers introduced a local moment-based calculation of the orbital susceptibilities on the Cu2+ sites, which, along with the spin and orbital HF tensors, constitutes the spin Hamiltonian picture for the detailed physics of the Cu2+ ions [42]. We shall discuss this point of view in detail in Sect. 3.3. In the meantime, it is interesting to consider the vanishing of the cuprate spin susceptibility χs (T ) at temperatures T Tc , postulated above, in the context of all of the diﬃculties over this point which occurred vis-a-vis the simpler superconductors discussed in Sect. 2.2.2. We recall that vanishing of χs (T ) required that the inverse lifetime from spin-orbit scattering must be small compared with the energy gap [43] (see (2.2.8)). That this must be so for YBCO7 results from that combined facts that (i) Cu is a very light element with relatively small spin-orbit coupling and (ii) energy gaps in the cuprates are roughly an order of magnitude larger than those found for sp-band superconductors. It is reasonable to suppose, then, that /Δ(0)τso 1 (1.2.8a), even in the mixed state, from which it follows that χs (T Tc )/χs (T > Tc ) 1. 3.2.6 Experimental Breakthrough: Oriented Powder Samples Late in 1987 a paper appeared which reported the technique of creating powdered samples of YBCO in which each crystallite is oriented with its c axis parallel to an applied magnetic ﬁeld [44]. This scheme relies upon the anisotropy of the (orbital) susceptiblity to provide the torque necessary to align each particle with the ﬁeld. The other necessary condition has to do with the morphology of the polycrystalline material to be oriented. It is assumed that upon reducing sample material synthesized in polycrystalline form to ﬁne powder, each particle of such a powder will be a single crystal, and thus, free to orient with its c axis along the applied ﬁeld. Any particle consisting of two or more crystallites will not align properly. The success of this technique is therefore dependent on the particular cuprate under study. YBCO is generally a good candidate for this eﬀect, where one can generally expect the Cu(2) (- 12 , 12 ) NMR line to assume a width of 100 Oe or less [38]. Following the original announcement, many NMR studies have appeared using oriented samples [28, 38]. Powder orientation results in an emormous improvement in the NMR signal strength, where signals requiring accumulation of ∼ 105 echo traces for adequate noise resolution [32] become visible on a single oscilloscope trace. The Cu(1) NMR signal is also greatly improved, where the quadrupole splitting along the c axis corresponds to an extraordinarily small component of the quadrupolar tensor, resulting in a weakly split line [38]. The real signiﬁcance of this method is that one can now measure the anisotropy of T1 with a conveniently large signal [38], although remarkably good results were obtained with milligram-scale single crystals [29]. To measure oriented samples in a transverse ﬁeld, one customarily sets the oriented particles in epoxy. Field oriented samples yield a 2D powder

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

pattern in a transverse ﬁeld, which is also important for studies of the and 89 Y NMR parameters.

81 17

O

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates The Mila-Rice-Shastry model [2, 3] for HF coupling with itinerant Cu2+ holes in a superconducting cuprate clariﬁed a number of murky points regarding NMR shift and T1 behavior. Important features were (i) transferred HF couplings, (ii) the ability to account for observed behavior with a single “band” of excitations, and (iii) the quantum chemistry framework for the HF Hamiltonian which emerged. Looking back, this was an important turning point in our understanding of HF interactions and of their dynamics. Previous workers had tried to formulate the NMR shift and relaxation in terms of Cu2+ local moment dynamics driving purely on-site HF couplings, but found peculiar results when trying to ﬁt the extraordinarily large T1 anisotropy at the Cu(2) site [29]. The demise of the local HF coupling picture was sealed by the observation that the Cu(2) c–axis shift term attributable to 3d-spin moments was vanishingly small [33, 41], while, in contrast, c–axis HF ﬂuctuations dominated the T1 process [29, 37, 38]. It was clear that there were two or more independent contributions to the c–axis HF coupling which vanished when superimposed to form the net shift, but produced ﬂuctuations which did not cancel and were in fact very large. The Cu(2)-Cu(2) Transferred HF Coupling The resolution of the vanishing c-axis spin shift question was concluded to be a highly unusual transferred HF coupling between a Cu-site nuclear spin and the four nn Cu spin moments, which is a great deal larger that previously identiﬁed interactions of this sort [45]. The putative isotropic transferred nn coupling may be written HTr = B I · Si , (3.3.1) i(nn)

where the sum is over the four nearest-neighbor Cu(2) sites to the site in question. Nonetheless, it was argued that the only alternative to this was HF coupling with mobile holes on the planar oxygen lattice. Any such hole state would need to hybridize with the Cu(2) 4s state, in order to explain the large, isotropic HF coupling. Suitable oxygen hole states for this purpose were argued to be energetically unfavorable [2]. It was also argued by Mila and Rice that doped holes would be in singlet states which have negligible HF coupling with nuclear moments [46]. Whether this is correct or not is unresolved. To

82

3 Preliminary Steps in Cuprate NMR

our knowledge, however, no unidentiﬁed HF eﬀect, static or dynamic, has ever been reported to contradict this conclusion. The result is a quantum ﬂuid of Cu2+ holes which is expected to be the sole source of HF eﬀects in the normal state and to form spin pairs in the superconducting ground state. Hybridization with the O2− neighbors has been proposed as the source of spin HF eﬀects for the 17 O(2,3) sites by Shastry [3], and hybridization with the Y3+ 4d orbitals has been demonstrated by Alloul et al. [35]. That this is a correct picture is evidenced by the vanishing of 1/T1 at T Tc for the 63,65 Cu, 17 O, and 89 Y NMR lines for which data have been reported, as well as of the spin-paramagnetic NMR shifts. 3.3.1 General Deﬁnition of the HF Tensors Before entering into the details of extracting the HF tensors from shift and susceptibility data, we set down a general framework for the structure of all HF couplings to be discussed from this point forward. The YBCO HF tensor components are deﬁned by ⎧ ⎫ ⎪ (1) ⎪ ⎪ ⎪ (1) (1) ⎪ ⎪ Aα Siα + B Iiα ⎪ Sjα ⎪ HHF = ⎪ ⎪ ⎩ ⎭ i,α j(nn) ⎧ ⎫ ⎪ (2) ⎪ ⎪ ⎪ ⎪A(2) ⎪ + Iiα ⎪ Siα + B (2) Sjα ⎪ ⎪ ⎪ α ⎩ ⎭ i,α

+

i,α

17

Iiα

j(nn)

j(nn)

Cα Sjα +

i,α

89

Iiα

Dα Sjα .

(3.3.2)

j(nn)

The four terms in (3.3.2) refer, respectively, to nuclei on the Cu(1), Cu(2), O(2,3), and Y sites. In the ﬁrst two terms the nn couplings B (1,2) are in(1,2) troduced as deﬁned in the foregoing paragraph. The coeﬃcients Aα are composites of the on-site Cu(1,2) HF couplings which are derived from the spin Hamiltonian model below. For the O(2,3) and Y, the sums on j cover two and eight nn Cu(2) sites, respectively. Omitted are oxygen sites O(1) and O(4) for the sake of simplicity. Their shift and relaxation behavior have been recorded, but are not essential to our understanding of the CuO2 planes where (1) the superconductivity resides. The 63,65 Cu(1,2) nuclear spins are labelled I i (2) 17 17 and I i in an obvious notation. The O(2,3) spins are labelled I i and the 89 Y spins are labelled 89 I i . Note that all HF eﬀects are assumed to be driven by the Cu2+ spin operators S j , which are rendered itinerant by the hole doping as in the Zhang-Rice model [16]. Our viewpoint regarding hole doping is that there are no HF effects which stem directly from the doped holes [46]. Such eﬀects have been discussed extensively in the literature, and we shall review these discussions where appropriate. It is not felt, however, that convincing evidence for oxygen hole-band HF eﬀects has ever been developed for the cuprates.

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

83

Evaluation of the HF Coeﬃcients (1)

(2)

The clearest and simplest way to evaluate HF coeﬃcients (e.g. Aα , Aα , Cα , and Dα in (3.3.2)) is by means of analysis of the NMR shifts and the measured susceptibility. In the case of YBCO7-x which we are concerned with here, there is the complication of partitioning the measured susceptibility between the Cu(1,2) sites and neighbors, principally because modeling the behavior of the Cu(1) sites involves a certian amount of guesswork. The spinHamiltonian model is used to estimate the orbital terms. In the end, MR simply partitioned χs (T ) equally between the three copper sites. Eﬀorts in the literature to improve on this have only been partially successful [47]. To proceed, then, we ﬁrst estimate the orbital (Van Vleck) susceptibilities and NMR shifts by means of the spin Hamiltonian model [42]. The core diamagnetic term can be estimated from tables. Subtracting these terms from the measured total then yields the spin susceptibility χs (T ). Provisions to be described below will be made for its anisotropy, which for the Cu(2) sites will be ∝ gα2 , α = ab, c, according to the spin Hamiltonian. HF tensor components will then be derived We take the 17 O(2,3) as17follows. sites as a typical example, where HHF17 = i Iiα Cα j Sjα is the O(2,3) nuclear spin Hamiltonian term from (3.3.2). Taking the expectation value of this term in the presence of a ﬁeld H along the ξ axis and equating this result to a nuclear shift Zeeman term −γ17 H i Iiξ Kξ , we ﬁnd Kξ (T ) =

2Cξ χsξ (T ) = α17ξ χsξ (T ), γ17 gξ μB NA

(3.3.3)

where α17ξ is the shift coeﬃcient and χsξ (T ) = −gξ μB NA Sjξ /H is the molar susceptibility ( Sjξ < 0 is independent of j) of a Cu(2) site. In practice the shift coeﬃcient is determined experimentally by dividing a measured spin-paramagnetic shift by a “best estimate” of the corresponding molar susceptibility. The tensor Cβ has the units of energy, so what we will tabulate is the quantity Cξ = NA μB α17ξ /2 = Cξ /γ17 gξ ,

(3.3.4)

in units of “kOe/μB ”, since this is the HF ﬁeld which would be found if there were a magnetization of one μB on each Cu(2) site. It is divided by 2, because each O(2,3) has two Cu(2) neighbors. Appropriate deﬁnitions of the HF constant for each case discussed will be given as they come up. We ﬁnally want to emphasize one point, which is that the scale of the HF constants will depend on the value of the χs (T ) tensor adopted. It is given in Table 3.4, and corresponds to T = 100K. No other standard will be used for HF coeﬃcients for YBCO7-x, including for the deoxygenated phases. As we shall see, the shift values for YBCO7 are fairly well established, and if more accurate values for the χsξ (100K) are determined, it is a simple matter to scale all of the HF coeﬃcients uniformly. We proceed, then, with the determination of the HF coeﬃcients.

84

3 Preliminary Steps in Cuprate NMR

3.3.2 Extracting the Cu(1,2) HF tensors for YBCO7 from Shift and Susceptibility Data Using the Spin Hamiltonian Model As a preamble to their quantum chemical calculation of hybridized wavefunctions for the Cu(1,2) sites, Mila and Rice [2] analyzed the measured shifts and susceptibility for YBCO7 with the aid of a spin Hamiltonian model, yielding both spin and orbital HF tensors for the Cu(1,2) sites, as well as crystal-ﬁeld splittings for the Cu(2) site. Although the spin Hamiltonian model is most appropriate for insulators, it appears to provide an accurate description of HF eﬀects in the narrow-bandwidth doped cuprate superconductors. Since late 1988 when this was ﬁrst proposed, a good deal of additional data for all the experimental quantities has been reported. Although the original data used served a very important purpose, newer data were published with smaller error bars, and we believe that they lead to a picture with better internal consistency. Accordingly, we discuss here the original K and χ analysis, but re-work the numbers at the same time. The changes are small, but appear to be signiﬁcant. The Spin and Orbital NMR Shift Tensors for Cu(1) in YBCO7 (1,2)

(1,2)

(1,2)

We shall use the notation Kt (a, b, c) = Korb (a, b, c) + Ks (a, b, c) to represent the total, orbital, and spin shifts along the a, b, c axes for Cu(1,2). In Table 3.1 we list the original Cu(1)-site shifts [33, 41] and other data which were published a bit later. The total shift values listed were measured at T = 100 K, and the orbital shifts, which are assumed to be temperature (1,2) independent, were measured at 4.2 K, where it is assumed that Ks (a, b, c) = 0. The spin components listed then correspond to 100 K. Note that the diﬀerences between these two sets of data are not large, but are outside of the stated error bars in a number of cases. Spin and Orbital NMR Shift Tensors for Cu(2) in YBCO7 For the Cu(2) NMR shift data in Table 3.2 there are additional data sources listed, and we also include susceptibility data. Since it is not feasible to resolve Table 3.1. Table comparing Cu(1)-site shift values from the original Mila-Rice data [33, 41] and other data which appeared later. The data from [48] are used in the analysis discussed in the text. The spin components are obtained by subtraction: Ks = Kt - Korb . Shift values are in (%). The numbers in parentheses are uncertainties in the last digit quoted (1)

(1)

(1)

(1)

(1)

(1)

(1)

(1)

(1)

Source Kt (a) Kt (b) Kt (c) Korb (a) Korb (b) Korb (c) Ks (a) Ks (b) Ks (c) [33, 41] 1.34(2) 0.61(2) 0.60(8) 1.18(2) 0.43(2) 0.31(8) 0.16(2) 0.18(2) 0.29 (8) [29] 1.38(7) 0.55(7) 0.60(4) [48] 1.32(2) 0.56(2) 0.59(1) 1.08(4) 0.27(4) 0.25(1) 0.25(4) 0.29(4) 0.33(1)

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

85

Table 3.2. Table comparing Cu(2)-site shift values for YBCO7 from the original Mila-Rice data [33, 41] with other sets of data which have subsequently been reported. Data from the bottom line are employed for the analysis discussed here [48]. No distinction is made between the a and b planar axes. The susceptibility components given for [34] are derived by the procedure stated in the text. We note that the spin components are obtained by subtraction: Ks = Kt - Korb . Shift values are in (%) and susceptibilities in units of (10−6 emu/mole f.u.). The numbers in parentheses are uncertainties in the last digit quoted (2)

(2)

(2)

(2)

(2)

(2)

Source Kt (ab) Kt (c) Korb (ab) Korb (c) Ks (ab) Ks (c) χt (ab) χt (c) [33, 41] 0.61(2) [29] 0.59(4) [34] 0.55(5) [50] [48] 0.58(2)

1.27(8) 0.24(2) 1.267(1) 1.30(3) 0.25(2) 1.27(1) 0.28(1)

1.35(8) 0.37(2)

−0.08(8) 250

339

224(10) 361(10) 1.28(2) 1.28(2) 0.30(1)

−0.01(1)

a and b axis data for the Cu(2) shift, nor for the susceptibility, the in-plane data are labelled “ab”. Again, the original Mila-Rice data are given on the top line, and other sources of data are listed below. There is reasonably good consistency between the last two sources listed. We shall use the bottom line numbers for analysis here. The susceptibility components attributed to [34] were obtained in the following way. The actual data in [34] are measurements on a random powder sample. The 100K susceptibility from these data (2.70×10−4(emu/molef.u.)) has been partitioned between χt (c) and χt (ab) assuming the ratio χt (c)/χt (ab) = 1.61, as reported in [49]. This is, to our knowledge, the largest anisotropy ratio which has been reported for an oriented powder sample, and therefore corresponds to an unusually high degree of crystalline alignment. The resulting values for χt (ab) and χt (c) are given in the table and are used in the analysis discussed in the text. Determination of the Orbital Susceptibility Tensors Our next step is to use the Cu(1,2) shift tensors from the bottom lines of Tables 3.1 and 3.2 to determine the orbital susceptibilities, using the relation χorb (a, b, c) = Korb (a, b, c)/αorb ,

(3.3.5)

where αorb = 2 r−3 /NA . Equation (3.3.5) may be employed for either Cu site. We take r−3 = 6.3 a.u. from [2], yielding αorb = 141 (emu/mole)−1. The resulting orbital susceptibility values for the Cu(1,2) sites are listed in Table 3.3. Note that the a and b axis values are identical for Cu(2). Also tabulated are susceptibility values labelled “s+orb”, which are obtained with the following equation: tot tot χtot s+orb = χs + χorb = χt − χdia

(3.3.6)

86

3 Preliminary Steps in Cuprate NMR

Table 3.3. Table listing orbital susceptibility components derived from the orbital shifts from the bottom lines of Tables 3.1 and 3.2 using (3.3.5). Also, total susceptibilities from second line of Table 3.2 are listed here after correction for atomic core diamagnetism (see text). Susceptibilities are given in units of (10−6 emu/mole) for individual sites and (10−6 emu/molef.u.) for χtot s+orb (1)

(1)

(1)

(2)

(2)

76.5

19.1

17.7

19.8

90.7

tot χorb (a) χorb (b) χorb (c) χorb (ab) χorb (c) χtot s+orb (ab) χs+orb (c)

399

536

where χt is the experimental value, and where we use the (isotropic) χdia = −1.75 × 10−6 (emu/mole) from [2]. The measured susceptibilities cannot distinguish between the a and b axes. Determination of the Spin Hamiltonian Parameters Using the spin Hamiltonian expressions [42] χorb (c) = 0.70 (8μ2B /Δ0 ) and χorb (ab) = 0.70 (2μ2B /Δ1 ), we may now use the numbers in Table 3.3 to estimate the crystal ﬁeld energies Δ0,1 . The numerical factors 0.70 in these formulas are reduction factors based on measurements [13] and calculations [14] of covalency in the CuO2 planes. (2) Inserting the values of χorb (ab, c) from Table 3.3 then leads to Δ0 = 2.00 eV and Δ1 = 2.29 eV, in accord with calculations by McMahan et al. [51] which suggest that the Δ0,1 lie in the vicinity of 2.0 eV and diﬀer by ∼ 10%. We can now evaluate the g-factor expressions g⊥ = 2 − 2λ/Δ1 and g = 2 − 8λ/Δ0 , where λ is the spin-orbit coupling parameter. The free ion value of λ −830 cm−1 ([42], Table 7.6). Mila and Rice adopted the value λ = −710 cm−1 = −0.088 eV . We suggest that a slightly greater reduction factor is appropriate here, such as the value 0.75 given by Owen and Thornley for N i2+ in MgO [52]. This yields λ = −0.077 eV , which we employ henceforward. With this value we ﬁnd g⊥ = 2.067 ; g = 2.308.

(3.3.7)

The expected value for the anisotropy As of the spin susceptibility, is As = 2 = 1.247. We note that g-factor anisotropies in metals are χs /χs⊥ = g 2 /g⊥ not unusual, as may be seen in data reported for Cu and other noble metals [53]. Our next task is to partition the measured susceptibility between the Cu(1) and Cu(2) sites. Where Mila and Rice assumed the same isotropic spin susceptibilities for Cu(1) and Cu(2), we shall use the same axial susceptibility tensors for both sites. As discussed in [2] this is an oversimpliﬁed viewpoint for the Cu(1) site, for which the error incurred is hopefully not too large. We equate the “s+orb” values in Table 3.3 to expressions using the same axial spin susceptibility tensor components for the Cu(1) site (a axis) and the

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

87

Cu(2) sites (c axis). For this purpose we introduce the variable χs⊥ for a singlesite transverse component and χs = A χs⊥ for the longitudinal component, where A and χs⊥ are to be determined. This leads to the following equations for A and χs⊥ : (2)

(1)

χtot s+orb (c) = 2 χorb (c) + χorb (c) + (2A + 1) χs⊥ (3.3.8a) (2)

(1)

(1)

2 χtot s+orb (ab) = 4 χorb (ab) + χorb (a) + χorb (b) + (A + 5) χs⊥ . (3.3.8b) Inserting the numbers from Table 3.3 we solve (3.3.8), ﬁnding A = 1.166 and χs⊥ = 1.01 × 10−4 (emu/mole). This ”experimental” value for A is somewhat smaller than the spin Hamiltonian g-factor-based estimate of 1.247 calculated in the previous paragraph. The spin susceptibility tensor components deduced here are then 1.01 and 1.18×10−4(emu/mole) for χs⊥ and χs , respectively, as compared with the isotropic Mila-Rice value of 1.08×10−4(emu/mole). It is interesting to inquire what the possible source might be for the foregoing discrepancy in values for A. First, it seems likely that the correct value would agree with the spin Hamiltonian model, since other aspects of the model are quite successful. Next, it seems unlikely that approximate treatment of the Cu(1) site behavior is the source of the discrepancy. For example, assuming the Cu(1) site susceptibility to be isotropic would only increase the deduced anistropy for the Cu(2) site by ∼ 1%. On the other hand, the deduced anistropy A is quite sensitive to the experimental anisotropy value, which was taken to be χt (c)/χt (ab) = 1.61 [49] in the foregoing analysis. If this were increased by less than 4% to 1.67, (3.3.8) would yield the the spin Hamiltonian value χs /χs⊥ = 1.247. This result suggests that the correct value for the susceptibility anisotropy may be a few percent larger than the largest value which has been reported. 3.3.3 Quantum Chemistry of YBCO7 and the Hyperﬁne Tensor While it is to be expected that there is strong covalency between the Cu2+ moments and the oxygen ligands in the cuprate conducting planes, it seems quite surprising that there is a substantial admixture of the 4s wavefunctions of the nearest-neighbor Cu2+ ions, as posited in (3.3.1). Yet this is precisely what the quantum-chemical calculations show [2, 54]. We outline the calculation here and refer the reader to the original papers for the details. The tight-binding quantum-chemical calculations for Cu(2) are based on the diagram shown in Fig. 3.6, where the relevant orbitals are shown at each ionic site. The dx2 −y2 orbital is shown at the central (planar) Cu2+ ion, the pσ orbitals on the oxygen ligands, and the 4s orbitals on the four nn Cu2+ ions. With the sign conventions given in the ﬁgure, the p and s-orbital admixtures which couple to the central dx2 −y2 orbital are p = (p1x − p2y − p3x + p4y )/2 and s = (s1 − s2 + s3 − s4 )/2. The energies are as follows: The 3d-orbital energy is taken as the origin, d = 0. The ligand on-site energies are taken to be p = 4 eV and s ∼ −6 eV . The hopping energies shown in Fig. 3.6 are t1

88

3 Preliminary Steps in Cuprate NMR + s 2

×

+ p2y t8 s3

+ ×

t1

–

dx2 – y2 +

–

p3x

–

+

+

+ –

p1x –

–

+

+ ×

s1

t3 p4y

+ × s4

Fig. 3.6. A schematic representation of the dx2 −y 2 orbital at a Cu(2) site and the pσ orbitals of the O2− ligands, as well as the 4s orbitals on the four nn Cu(2) sites, which are admixed to form the total wavefunction of the Cu(2) 3d-holes for the Mila-Rice quantum chemistry calculation (see text). The tα ’s show hopping matrix elements, and the signs give phase conventions for admixed orbitals. Figure reprinted from F. Mila, T.M. Rice, Physica C157, 561 (1989). Copyright 1989 Physica C

= 0.33 eV, t3 = 1.38 eV, and t8 = 3.9 eV. The Hamiltonian is then solved in conjunction with the somewhat more complex Cu(1)-site Hamiltonian. The Wannier Wavefunction for Cu(2) The Cu(2) tight-binding (Wannier) wavefunction is written |ψ(2) = αd |dx2 −y2 + αp |p + αs |s ,

(3.3.9)

where the solution presented gives αd = 0.9, αp = -0.34, and αs = -0.26. In addition there is a coupling via the oxygen ligand to the nearest Cu(1) site and to the 4s state on that site. This coupling has some eﬀect on the Cu(2) shift, but an essentially negligible eﬀect on the Cu(2) T1 . For simplicity we shall omit these terms. The transferred isotropic HF coupling (3.3.1) from the nn Cu(2) sites may be estimated as follows. The 4s contact HF coupling from EPR data for atomic Cu [55] is 16π |ψ4s (0)|2 = 0.45 × 1027 cm−3 . 3

(3.3.10)

Referring to (1.2.2) and (1.2.7), the corresponding 4s contact HF coupling is 2,080 kOe/μB . The total transferred coupling is then estimated to be α2s ×2080 = 141 kOe/μB , as compared with ∼ 160 kOe/μB required to give the nearly vanishing c axis spin-paramagnetic shift. Mila and Rice note that the value stated is for atomic Cu, whereas Cu2+ will have an enhanced value of |ψ4s (0)|2 because of the ionic plus charge. There seems little doubt that the nn 4s admixture eﬀect is the correct answer to the c axis HF anomaly.

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

89

The Composite Cu(2) Spin Hyperﬁne Tensor Let us now state the remainder of the HF coupling terms for Cu(2) and then formulate the Mila–Rice T1 relaxation tensor. The full HF tensor may be written [42], (2) HHF = A(2) I · Si , (3.3.11) α Iα S0α + B(2) α

with

i(nn)

(2)

(2) (2) A(2) α = Acp + Adip,α + Aso,α ,

(3.3.12)

where the three terms shown are the isotropic core polarization term, the dipolar term, and the spin-orbit term, and where α = (ab, c) for the axially symmetric Cu(2) site. The spin-orbit terms, being a second-order perturbation eﬀect to higher crystal ﬁeld states driven by the spin-orbit coupling, are a special feature of the spin Hamiltonian picture. They are actually an orbital ﬁeld admixed into the spin HF terms. The core-polarization term is sometimes given as proportional to r−3 , which is a holdover from EPR studies where the origin of this term had not been identiﬁed2 . Here we shall simply appeal to systematic studies, which give Acp /2γn −127 kOe/μB . The dipolar and spin-orbit terms may be written (in energy units) 2 Adip,ab = 2γn μB r−3 , 7 4 Adip,c = −2γn μB r−3 , 7 11λ −3 , Aso,ab = 2γn μB r − 7Δ1 6λ 8λ . − Aso,c = 2γn μB r−3 − 7Δ1 Δ0

(3.3.13a) (3.3.13b) (3.3.13c) (3.3.13d)

We use the same parameters used earlier to evaluate the Van Vleck orbital susceptibilities and in (3.3.7) for the anisotropic g-factor to calculate the spin HF tensor. These are λ = −0.077 eV , Δ0 = 2.00 eV , Δ1 = 2.29 eV , and r−3 = 6.3 a.u. The resulting values for the Cu(2) spin HF tensor (3.3.11) are listed in Table 3.4 in units of kOe/μB (see Sect. 2.3.1). We also employ a reduction factor of 0.70 derived from determinations of covalency [13, 14] for these parameters, as well as the core polarization HF ﬁeld, in the second line of Table 3.4. The value of B (2) shown is adjusted to give minimum error for (2) (2) the Cu(2) spin-paramagnetic shift values Ks (ab) and Ks (c) (bottom line (2) (2) of Table 3.2). The estimated values KsE (ab) and KsE (c), given by 2

The work of Heine [56] later revealed that it had no connection with r −3 .

90

3 Preliminary Steps in Cuprate NMR

Table 3.4. Listing of values of spin HF tensor components for the Cu(2) sites, as derived in the foregoing paragraph. On the second line the free-ion component values have been corrected with a reduction factor 0.70 to account for covalency as mentioned above. A value of B (2) is stated (see (3.3.11)) which minimizes the errors in the spin-paramagnetic shift components given in the bottom line of Table 3.2. This value of B (2) is in reasonable accord with the estimate derived from quantum chemistry [2]. The spin susceptibility tensor associated with each Cu(1,2) site deduced earlier is shown, along with the Cu(2) site spin-paramagnetic shift tensor corresponding to the HF parameters given. Finally, the composite on-site HF tensor components given by (3.3.12) are listed. All HF tensor components are in units of kOe/μB , with susceptibilities in 10−6 (emu/mole) (2)

Acp

(2)

(2)

(2)

(2)

(2)

(3.3.13) −127 113 Corr. −89 79

−225 21 −158 15

131 92

55 38

(2) KsE (ab, c) (2)

(2)

(2)

(2)

Adip,ab Adip,c Aso,ab Aso,c B (2) χs⊥ χs KsE (ab) KsE (c) Aab Ac

(2)

(2)

=

101 118 0.28%

(2)

Aab,c NA μB

−0.01% 5

−155

χs⊥, ,

(3.3.14)

(2)

where Aξ = Acp + Adip,ξ + Aso,ξ + 4B (2) , are also listed in the table. A good ﬁt is seen to be achieved. To the far right are listed the components (2) of the composite on-site HF tensor Aα deﬁned by (3.3.12). 3.3.4 T1 Ratios and Electron Spin Correlation Eﬀects Mila and Rice introduced the concept of electronic spin-spin correlation factors in their T1 calculation, but did not use them in their discussion of T1 anisotropy. Subsequent discussions of the T1 problem in cuprates have made extensive use of this idea. Here, we ﬁnd it necessary to consider the eﬀect of spin-spin correlations to obtain agreement with experimental data. All HF constants are given in (kG/μB ). The primed notation for this option introduced with (3.3.4) is suppressed in this subsection for simplicity. Using expressions similar to MR, we now present results for the Cu(2) 2 (ab, c)χs (ω0 ), where the relaxation tensor. The 1/T1ab,c have the form HHF squared HF ﬁeld parameters are (2) 2

(2)

2 (c) = 2 [Aab +4 B (2) 2 +8 Aab B (2) K01 +4 B (2) 2 (2 K12 +K13 )] (3.3.15) HHF

and (2) 2

2 HHF (ab) = [Aab

(2)

2 (2) + A(2) + 8 B (2) 2 + 8 (Aab + A(2) K01 c c )B

+8 B (2) 2 (2 K12 + K13 )],

(3.3.16)

where Kij = · S j is the normalized spin-spin correlation between sites labeled i and j (see Fig. 3.6). The quantity χs (ω0 ) has the dimensions of a correlation time, but also has in it the density of states and temperature factors 4 3 S i

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

91

that arise out of some speciﬁc model of quasiparticle dynamics appropriate to the cuprates. If the system were a Fermi liquid one would have χs (ω0 ) ∝ T . Without such modeling this theory cannot give absolute values for T1 , but it can predict the anisotropy of T1 at the Cu(2) site using the HF tensor data from Table 3.4. Having minimized the error in the spin paramagnetic shift tensor to estimate the value of B (2) given in the table, we insert the parameter values into the ratio of (3.3.16) to (3.3.15) to determine the expression, T1c [1 − 1.69 K01 + 0.38 (2 K12 + K13 ] = 2.64 . T1ab [1 + 0.29 K01 + 0.99 (2 K12 + K13 )]

(3.3.17)

Equation (3.3.17) is to be compared with experimental data giving values of T1c /T1ab of ∼ 4.5 [29], ∼ 3.6 [38], or the later value ∼ 3.4 [57]. 3 In any case, it is clear that the spin-spin correlation factors in (3.3.17) are going to have to play a role in order to achieve quantitative consistency with experiment. Regarding (3.3.17), since K01 is a nearest-neighbor correlation it must be negative, while K12 and K13 are correlations between neighbors on the same “sublattice”, so to speak, so they will be positive and undoubtedly smaller in magnitude that K01 . Thus, K01 will have a clear eﬀect of increasing the ratio if its value is negative and appreciable. For example, if we neglect the K12,13 terms for the moment, then a value of K01 = -0.07 would yield a T1 ratio of 4. With only a modest amount of correlation we can obtain a realistic value for T1c /T1ab . Temperature-Dependent Spin-Spin Correlations It is not clear from the Mila-Rice presentation, either, whether they intended the correlations to be used as temperature-dependent parameters or not, but a number of subsequent developments have employed them in just that role. For example, temperature-varying correlations give a straightforward explanation for the variation found for the T1 anisotropy in YBCO7 between 100 K and 300 K [38]. These data are shown in Fig. 3.7, where it is seen that T1c /T1ab diminishes by barely 10% over that temperature interval, and is only barely outside of the error bars. Nonetheless, the trend persists over a series of data points and is clearly established.4 As we shall see in Chap. 5, extensive use has been made of the Kij ’s as temperature-dependent parameters to describe the behavior of T1 . In the Uldry-Meier T1 analysis, for example, the temperature dependence of all T1 ’s is described in terms of the spin-spin correlations and an eﬀective correlation time [58]. The theoretical basis for this approach is derived in Sect. 3.5. 3

4

The diﬀerence between these two measurements is outside of error estimates, and can only be attributed to a diﬀerence in samples. The lower numbers agree with earlier measurements made on a random powder [37]. It would have been desirable to have this eﬀect conﬁrmed by another experimental group. To our knowledge, no such conﬁrmation has been reported.

92

3 Preliminary Steps in Cuprate NMR 5

1.4

1.2 (θ = π/2)

4

3 0.8 (θ = 0) 0.6

2 63Cu

T1–1 (msec–1)

T1–1 (msec–1)

1.0

(2) 0.4

ν = 85 MHz 1

0.2

0

0

100

200 T (K)

300

Fig. 3.7. 1/T1ab (θ = π/2) and 1/T1c (θ = 0) are plotted vs. temperature over the range 90 K ≤ T ≤ 300 K for Cu(2) sites in an oriented powder sample of fully oxygenated YBCO7 [38]. The data are scaled so that T1 values for the two orientations coincide at T = 100 K, so as to highlight the decrease of the T1c /T1ab ratio over range of T measured. Reprinted ﬁgure from R.E. Walstedt, W.W. Warren, Jr., et al: Phys. Rev. B40, 2572 (1989). Copyright 1989 American Physical Society

Meanwhile, we also recall that the ﬁrst Mila-Rice paper [2] made no attempt to apply their model to the interpretation of the peculiar temperature dependence of the T1 data. Indeed, theories addressing the behavior of T1 (T ) were fairly quick to follow, but are still under discussion, as will be seen in Chap. 5.

3.4 Incorporating 17 O and 89 Y data into the Mila-Rice-Shastry Picture Following the Mila-Rice (MR) paper there were many new developments, some going beyond the scope of the present chapter. There were new data on 17 O NMR in YBCO, as well as a great deal of discussion regarding the question of a two-ﬂuid picture of quasiparticle dynamics, i.e. whether there is evidence for a separate hole band on the oxygen sites. There were also eﬀorts to treat

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

93

the temperature dependence of the copper T1 , along with discussion of just how the Cu(1) chain sites in YBCO diﬀer from the Cu(2). In the midst of these many challenging questions and almost immediately following Mila and Rice, reports on the peculiar behavior of the oxygen-deﬁcient phases made a sudden appearance. These eﬀects, known collectively as the pseudogap and their interesting history in the high-Tc ﬁeld are the subject of Chap. 4. We consider here the ﬁrst reports on the behavior of the planar 17 O NMR, as well as the closely related 89 Y. Detailed theories which address the contrasting behavior of 63,65 Cu, 17 O, and 89 Y in YBCO are presented in Chap. 5. Following the discussion of the 17 O data for YBCO7, we consider again the possible occurrence of oxygen hole bands along with the Cu2+ -related (ZhangRice) quasiparticles in the total picture of fermion dynamics. 17

O(2,3) NMR Data and Interpretation for YBCO7

By the middle of 1989, 17 O NMR studies on YBCO7 had been reported by several groups [59, 60, 61, 62]. Here we shall review and discuss the results reported by Takigawa, Hammel et al. [59, 60] in some detail. A comparable set of results was reported by Horvati´c et al. [61], covering a wider range of temperatures. The high temperature results for the quadrupolar and shift tensors for the O(2,3) sites from the latter study were found to agree within error bars with those from [59], and the quadrupolar data from [62] are also in accord. The HF tensor is analyzed below and compared with the MR model calculation. There is some disagreement in detail, but this, we suggest, may arise from inaccuracies in the MR quantum chemistry results. 17 O spectra were taken on oriented powder samples of YBCO7 [59], for which 17 O-enriched oxygen gas was used to exchange 17 O into the sample material at a temperature of 900◦ C. The resulting (nearly) complete NMR spectrum for all of the oxygen sites is shown in Fig. 3.8 for the case of ﬁeld oriented along the c axis. The identiﬁcation of all the peaks in this spectrum is a real tour-de-force of NMR shift and quadrupole splitting analysis. Although the c axis is expected to be one of the principal axes of the EFG tensors for each oxygen site, the EFG tensors are decidedly non–axial in character. The peaks have been ﬁtted using the I = 52 second-order perturbation formulas [59] 1 1 2 − ↔ (3.4.1a) : Δν = ν0 Kz + (νx − νy )2 /ν0 , 2 2 9 5 1 3 (3.4.1b) ± ↔± : Δν = ν0 Kz ± νz + (νx − νy )2 /ν0 , 2 2 36 5 1 3 (3.4.1c) ± ↔± : Δν = ν0 Kz ± 2νz − (νx − νy )2 /ν0 , 2 2 9 where ν0 = γn Hres and Δν = νres - ν0 . The NMR frequency is νres , and Hres is the value of the ﬁeld at the peak in question. The quantities νx,y,z are quadrupole frequency parameters deﬁned as να = 3eQ 20 Vαα . Equation (3.4.1a)

94

3 Preliminary Steps in Cuprate NMR

SPIN ECHO INTENSITY

A0, A1, A2 : O (1) B0 – B4 B1´ – B´4 : O (2), O (3)

νres / γ

N

C0, C1, C2 : O (4) B0 B´3

B3

B2

B1

B4

B´1

C1

B´2

B´4

C2 A2

C0

A1 A0 × 7.2 84

× 7.2 85

× 4.5

×1

× 2.6

86

× 5.1 87

× 7.2 88

MAGNETIC FIELD (kOe)

Fig. 3.8. 17 O NMR spectrum taken at 49.8 MHz on an oriented powder sample of YBCO7 with enriched 17 O content [59]. The ﬁeld was oriented along the c axis. Sample temperature was 160 K. For 17 O γn /2π was taken to be 0.577186 kHz/Oe. The sites were identiﬁed as labelled, with the (Bn , Bn ) pairs of lines very close together for the O(2,3) sites. See text for discussion of the quadrupolar and shift tensors for the O(2,3) sites. Reprinted ﬁgure from M. Takigawa, P.C. Hammel, et al: Phys. Rev. Lett. 63, 1865 (1989). Copyright 1989 American Physical Society

will be recognized as (2.1.3) written out with Vαα parameters. Note that no relative size or sign relationship is implied here among the νx,y,z , except, of course, that α να = 0. The parameters are adjusted for each site so as to give a best ﬁt to the spectrum shown, as well as spectra taken with H ⊥ the c axis, an exercise of considerable complexity. For the case of the O(2,3) sites, it was not clear from the data alone whether the principal axis of the EFG was along the c axis or along the bond axis. To decide this, trial calculations of the EFG tensor were made assuming a point-charge contribution multiplied by a Sternheimer factor (1 − γ∞ ) [63], where γ∞ was taken to be 9, plus an on-site p-electron contribution of 3 ( 20 )( 45 e2 |Q| r−3 , where r−3 was taken to be 3.63 a.u. [59]. On this basis, the only reasonable outcome was obtained assuming the principal axis is the bond axis, giving an estimated result (0.97, −0.42, −0.55) MHz as compared with (0.976, −0.598, −0.378) MHz shown in Table 3.5. Note that the transverse axis values are reversed between modeling and experiment, so that the ﬁt is close, but not exact. The principal EFG values for all sites lie along the bond axes. Our interest in the shift data shown in the table is in comparing them with the results calculated by MR, and ultimately to see whether the 17 O data are compatible with a single-ﬂuid description of the distribution of electronic

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

95

(i.e. hole) spin density. Shift values are given for all sites at two temperatures, 160 K and 30 K. In the latter case, we suppose that the spin susceptibility is essentially zero (see e.g. shift measurements for T < Tc in [41, 48]), so that these residual values may be regarded as orbital shifts. This surmise is veriﬁed by a detailed plot of Kc (T ) vs. T by Horvati´c et al., (see Fig. 4 in [61]). Subtracting the 30 K shift values from the 160 K ones, we ﬁnd estimates of the spin paramagnetic shift components, listed under “Ks (160 K)”. The latter values form a tensor for each site, which has been divided into an isotropic component Kiso = (K + 2K⊥ )/3 and an anisotropic (axial) component with Kax = (K − K⊥ )/3. The latter parameters are tabulated in the ﬁnal two columns. It is seen for the O(2,3) that there is a fairly large isotropic component as expected, with quite a sizeable axial shift Kax = 0.03% as well. It seems that the main hybridization is into the 2pσ orbitals as expected. On the other hand, the MR quantum chemistry calculation predicted a rather smaller value for Kax than what was found. We analyze this point by noting that the axial shift coeﬃcient for a pσ orbital occupied with a fraction f of the S = 12 moment is given by αax = 25 f r−3 /NA . According to the MR quantum chemistry (Sect. 3.3), f = α2p /2 = 0.058. Using the value

r−3 = 3.63 a.u. [59], we ﬁnd ασ = 0.94(emu/mole)−1. With a transverse susceptibility component of 1.01 × 10−4 (emu/mole Cu(2)) (Table 3.4), we ﬁnd Kax (MR) 0.0095%. This is approximately 1/3 the experimental value in Table 3.5. So although the experimental value has a large error bar, it is certainly much larger than the MR calculated value. Is this evidence for an oxygen hole band? We think not, but unfortunately, there is no trend with doping or even temperature dependence to check such a hypothesis. However, there is another experimental number which comes to mind here, namely the determination of the covalency of La2 CuO4 at high Table 3.5. Experimental quadrupolar tensors and shift data from spectra such as Fig. 3.8 are shown at two temperatures in the left-hand columns, followed by deduced spin components, which are then broken down into isotropic and axial parts [59]. The 30 K values are taken to be of purely orbital origin. Site and orientation labels are shown at the far left. Frequencies are given in MHz and shifts in % Site

Axis να

Kα (160 K) Kα (30 K) Ks (160 K) Ks (iso) Ks (ax)

O(1)

⊥ c -0.484 ⊥ c 1.629 c -1.145

0.23 0.22 0.24

... 0.13(1) 0.13(3)

... 0.09(1) 0.11(3)

0.10(1) 0.01(1)

O(2,3) ⊥ c (0.986,0.966) 0.31 ⊥ c -0.598 0.17 c (-0.389,-0.369) 0.18

0.05(1) 0.01(1) 0.02(3)

0.26(1) 0.16(1) 0.16(1)

0.19(1) 0.03(1)

-0.01(1) 0.04(1) 0.03(1)

-0.01(1) -0.01(1) 0.05(1)

0.01(1) 0.02(1)

O(4)

⊥ c -0.375 ⊥ c -0.721 c 1.096

-0.02 0.03 0.08

96

3 Preliminary Steps in Cuprate NMR

temperatures using 17 O NMR shift measurements [13]. The total fraction of spin density residing on the O(2,3) with the MR result (foregoing paragraph) is 2f = 11.6%. The comparable experimental result for La2 CuO4 is 31% [13]. Scaling the foregoing estimate by the ratio of these numbers, one ﬁnds a result nearly a factor of 3 larger and in much better agreement with the O(2,3) axial shift in Table 3.5. The La2 CuO4 measurement is also in good agreement with, but actually slightly less than theoretical values given by H¨ usser, et al. [14]. We suggest that the value for La2 CuO4 should not be very diﬀerent from that for YBCO7. Thus, it is possible that the expected number for the 2pσ spin density is quite a bit larger than the MR value, and that the reported 17 O(2, 3) shift values in [59] are consistent with a one-band picture. HF Tensors for

17

O(2,3) and

89

Y in YBCO7

In Table 3.6 we collect data for the 17 O(2,3) and 89 Y NMR shift tensors and list the corresponding HF tensors deﬁned in (3.3.2) and (3.3.4). For the 17 O(2,3) case we take NMR shift data from Table 3.5. For the 89 Y case the data are taken from Alloul et al. [64], which reports the highest numbers available for an oriented powder sample5 . The HF tensors are then obtained with (3.3.4) using the spin susceptibilities in Table 3.4. The HF constants for the various sites in and near the CuO2 in Tables 3.4 and 3.6 are expected to hold for reduced oxygen phases of YBCO7-x as well. A very important test of this idea occurs in Chap. 4, where these values are compared with precisely determined relative values for the YBCO6.63 phase. Table 3.6. Spin components of NMR shift are tabulated for the 17 O(2,3) and 89 Y, 17 Ksα and 89 Ksα , respectively, for YBCO7 at T = 100 K. See text for the source of these data. The corresponding HF tensors obtained with (3.3.4) are also listed, along with the susceptibility tensor from Table 3.4. Note that for the 89 Y case the denominator in (3.3.4) is “8” rather than “2”. Cα and Dα are given in kOe/μB and χsα in 10−4 (emu/mole) Axis a b c

5

17

Kα (%)

0.26(1) 0.16(1) 0.16(1)

89

Kα (ppm) Cα

247 247 315

Dα

χsα (100 K)

72(3) 1.71(9) 1.01 44(2) 1.71(9) 1.01 38(2) 1.86(9) 1.18

We take larger numbers for the 89 Y NMR shift at 100 K to be a sign of full oxygenation. Moreover, the plot reported for 89 Kα (T ) vs. T [64] shows a gradual increase from 300 K down to a maximum at T ∼ 120 K. This is a characteristic of a fully oxygenated sample as well [47], rather than declining curves which then give smaller values of 89 Kα at T = 100 K [65].

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

3.4.1 Measurements of T1 for

17

97

O in YBCO7

The foregoing authors also reported T1 measurements for various oxygen sites in YBCO7 [60]. As found earlier for the 89 Y [22, 23], the 17 O(2,3) relaxation in the normal state is very Korringa-like, with T1 T 2.7 sK. The authors chose to give a qualitative discussion of this result, along with their 63 Cu(2) data, in terms of the Korringa relation (1.2.8). Following that, however, they discuss the T1 results in terms of the dynamic susceptibility χ (q, ω), which became the method of choice for analyzing relaxation data. In the following sect. (3.5) we present for reference purposes a derivation of the relaxation rates for 89 Y, 17 O(2,3), and 63 Cu(2) in YBCO in terms of χ (q, ω). We shall use formulas given there for our present discussion of data from [60]. First, let us consider the simple Korringa relation (2.2.8) in relation to the current problem. One could hardly expect it to apply in any strict fashion to YBCO, owing to unknown particle dynamics, q-dependent HF coupling tensors, etc. Nonetheless, it does serve a sort of qualitative purpose in comparing the behavior of diﬀerent nuclear sites. The 89 Y and 17 O(2,3) T1 processes are at least Korringa-like in their temperature dependence, though this may be somewhat illusory because of spin-spin correlation effects. Nonetheless, if you take the isotropic shift value from Table 3.5, you ﬁnd for 17 O(2,3) 4πkB γn2 1 1.4 × . (3.4.2) Ks (iso)2 T1 T γe2 To compare the latter result with the Cu(2) site they used T1ab , because it relates to the largest on-site HF term Ac = -221 kOe/μB . Since Aab is very small, however, they divided the expression (3.4.2) by two,6 ﬁnding a multiplier of 11 for the Cu(2) Korringa product. So there is a very clear enhancement of the Cu(2) relaxation, with almost none for the O(2,3). If we look at the q-dependent expressions for 1/T1 in Sect. 3.5, the Cu(2) expression for the ﬁeld ⊥ c axis, it is essentially independent of q, whereas for both the 89 Y and 17 O(2,3) cases, the integrand vanishes at QAF = (π/a, π/a). If χ (q, ω) has an AFM enhancement peak, the Cu(2) rate will receive full enhancement, but the 89 Y and 17 O(2,3) will have little or none. This is the explanation oﬀered in [60] for the discrepancy in Korringa ratios which they ﬁnd, but has been put forward by many other observers as well [66]. It was also generally thought to be related to the peculiar temperature dependence of the Cu(2) relaxation rate while the 89 Y and 17 O(2,3) rates were Korringalike. Reference [60] also presented data on relaxation rates for T < Tc for YBCO7, but discussion of those results will be combined with consideration of the Cu(2) data in Sect. 3.6. 6

Thus, only one axis is eﬀectively contributing to the T1 rate.

98

3 Preliminary Steps in Cuprate NMR

3.4.2 The One-Band, Two-Band Debate: in YBCO

89

Y and

17

O(2,3) NMR

The MR model theory purported to explain the Cu(1,2) NMR (in YBCO7) behavior at 100 K with a single spin ﬂuid, where all HF couplings were assumed to originate with the S = 1/2 coupled moments on the Cu2+ sites. At the same time or slightly later, other interpretive papers appeared as well as experimental papers with more data on the 89 Y and 17 O NMR shift and relaxation properties. In this subsection we consider arguments presented on the question of one quantum ﬂuid vs. two separate ﬂuids needed to account for the T1 data. Monien, Pines, and Slichter [67] presented an analysis similar to MR, including the transferred HF term for the Cu(2) sites, but also considering a possible “oxygen hole band” characterized by susceptibility χh as well as a Cu(2) HF coupling Ah . In similar fashion to Sect. 3.3, they concluded that the one-ﬂuid model could not explain the data unless there were spin-spin correlations. However, they also pointed out the possibility that the (χh , Ah ) oxygen band, if present, could be the explanation. The question was how to decide whether the hole band was necessary. A substantive discussion of this point was given by Mila and Rice themselves in a follow-up paper [46]. We shall brieﬂy recap their main points here. First, they note that while one could consider the possibility of a hole band on the O(2,3) sites, the Zhang-Rice singlet picture essentially rules this out, since the singlets are magnetically inert 7 . Thus, one would expect that HF parameters should not depend on the doping level. In this connection they noted that in the large 89 Y study by Alloul et al. [65], the slope of K vs. χ plots is invariant from full doping all the way down into the insulating regime. Thus, the 89 Y HF coupling is independent of doping, consistent with the Zhang-Rice singlet picture. Next, they consider what one would expect if there actually were a hole band. On the basis of quantum chemistry, MR argue that such a hole band would have a much stronger HF coupling with the 89 Y nuclei than the Cu2+ moments have. The reasoning is as follows. First, the Cu2+ are too far from the 89 Y for direct coupling, and for the (strongly) hybridized 2pσ orbitals on the O(2,3), the MR Wannier wavefunction (3.3.9) has the wrong symmetry to couple to the Y s or d orbitals. The answer, they suggest, is a possible double hybridization path through 2pπ orbitals to the Y 4d. This is, of course, very weak, and they argue that any hole band which occupies either the 2pσ or 2pπ orbitals will have hybridization at least 5 times larger. Because of this, the 89 Y HF parameter in such a case would vary sharply with hole concentration. Since it does not, they conclude that an oxygen hole band is essentially ruled out. 7

There were, however, two-band models proposed at the time, such as that given by Emery and Reiter [68].

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

99

There was further discussion of oxygen bands in a few additional papers [48, 5], but no really cogent evidence conﬁrming their existence. In Chap. 5 a discussion is presented of several models for calculation and interpretation of T1 data for various nuclear species in the YBCO family of compounds. With the development of various theoretical models and schemes for interpretation of relaxation eﬀects, there seemed less and less motivation to include oxygen hole bands. There was no evidence to support their suggested existence once it was realized that q–dependence susceptibilities and HF couplings could account for the observed behavior. There, however, we shall also reconsider the possibility of an orbital relaxation term (see Sect. 5.6).

3.5 Formulation of T1 in Terms of χ(q, ω) and q-Dependent HF Couplings Even though transferred HF couplings quite obviously underlie the shift and relaxation eﬀects of the 89 Y nuclei in YBCO [22, 23, 35, 36], their presence – and the concomitant eﬀects of antiferromagnetic (AFM) spin-spin correlations – were brought to our attention by the MR [2] analysis. However, the spin-spin correlation picture was not destined to become the language of choice for this problem, but rather that of the well-known dynamical susceptibility χ(q, ω) [69, 70]. While these pictures are, as will be seen below, completely equivalent, the q–space methodology is perhaps a bit more convenient, as well as tying in directly with INS measurements. While the potential of this approach to distinguish the behavior of 63,65 Cu, 17 O, and 89 Y in YBCO was noted early on [34], its dramatic consequence of cancelling AFM ﬂuctuations at the planar oxygen was ﬁrst articulated by the analysis of Shastry [3]. Subsequently, it has been widely invoked for discussion of T1 eﬀects [6, 7, 46, 60, 66, 71]. 3.5.1 Derivation of Dynamical Susceptibility T1 Equation The formula for T1 in terms of χ (q, ω) and q-dependent HF couplings is widely quoted. For reference, we give here a simple derivation of this result, starting from the master equation for the interaction representation density matrix for nuclear spins ρ∗ (t) [72], ∞ dρ∗ =− dτ [H1∗ (t), [H1∗ (t − τ ), ρ∗ (t)]], (3.5.1) dt 0 where H1 is the spin-lattice interaction being treated here as a perturbation, and the overline represents an average over t which is long compared with the correlation time scale of τ , but short compared with the time for the nuclear spin polarization to change. The star indicates operators which have been transformed into the interaction representation as in O∗ (t) = exp(i(F + H0 )t)O exp(−i(F + H0 )t), where H0 is the unperturbed nuclear

100

3 Preliminary Steps in Cuprate NMR

spin Hamiltonian, and F is the Hamiltonian for the rest of the dynamical variables in the system. Here, for simplicity we take H0 to be a Zeeman term with a ﬁeld H applied along the cartesian axis labelled α, H0 = −ω0 Iαi , (3.5.2) i

where ω0 = γn H. The densitymatrix for spin-lattice relaxation in such a case is simply ρ∗ (t) = ρ(t) = a(t) i Iαi , where a(t) is a variable which represents the changing nuclear magnetization during a T1 experiment. We illustate the q-dependent HF coupling eﬀects with H1 for the Cu(2) sites, Ijβ Aα Sjβ + B Skβ , (3.5.3) H1 = j,β

k=nn

where the B term is an isotropic coupling between I j and the four nn spins Sk to the j site. It will simplify the procedure if we neglect the imaginary part of the time factors exp(±iω0 t) which occur for each of the operators Ijβ in the interaction representation, and simply represent them as a factor cosω0 τ times the correlation functions. The correlation functions are assumed to be even in the variable τ , and the sinω0 τ terms will always vanish in the applications considered here. A second simpliﬁcation occurs if we operate on both sides of (3.5.1) with T r(Iiα ...). Since the spin correlation functions are even functions of τ so that Sjβ (t)Skβ (t + τ ) = Sjβ (t + τ )Skβ (t), we may write (3.5.1), in part, as (N)

a−1

da =− dt i

∞ 0

dτ cosω0 τ [Ax Six (t) + B

Skx (t)][Ax Six (t + τ ) + B

k=nn

Skx (t + τ )], (3.5.4)

k=nn

where we are displaying only the x axis ﬂuctuation term as an example. The next step is to Fourier transform the spin operators with Siβ (t) =

(N )

eiq·ri Sq (t) , β = x, y, z,

(3.5.5)

q

(N ) where the summations are normalized so that q exp[iq · (r − r i )] = δr,ri , etc. In (3.5.5) Sq (t) is deﬁned to be an isotropic, q-dependent spin ﬂuctuation operator. Using (3.5.5) in both factors in (3.5.4) and noting that (N ) exp[i(q + q ) · ri ] = δq,−q , (3.5.4) becomes i a

−1 da

dt

= −

(N ) q

2

Ax (q)

∞

dτ Sq (t)S−q (t + τ )cosω0 τ, 0

(3.5.6)

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

101

where Ax (q) = [Ax + 2B(cos(qx a) + cos(qy a)]. In (3.5.6) the Ax (q) are in circular frequency units per unit of spin. We now proceed to replace the time average with an ensemble average ∞ ∞ dτ Sq (t)S−q (t + τ ) cos ω0 τ = dτ Sq (0)Sq (τ )Ens cos ω0 τ = S(q, ω0 ), 0

0

(3.5.7) where we have also assumed that Sq (t) has inversion symmetry. The quantity on the far right of (3.5.7) is known as the dynamical structure factor. 3.5.2 The Fluctuation-Dissipation Theorem The dynamical structure factor may be related to χ(q, ω0 ) using the ﬂuctuationdissipation theorem [4], which says (eω0 β − 1) S(q, ω0 ), (3.5.8) eω0 β where β = 1/kB T and we note that ω0 β 1. The subscript “s” is a reminder that the spin-only susceptibility deﬁned by (3.5.8) has a dimension of inverse energy. Inserting this into (3.5.6) and combining terms for x and y-axis ﬂuctuations yields for −a−1 da/dt, Im [χs (q, ω0 )] = χs (q, ω0 ) =

(N ) γ 2 kB T 1 = Aξ (q)2 χξ (q, ω0 )/(gξ2 ω0 ). T1α μ2B q

(3.5.9)

ξ

The latter expression for 1/T1α uses Aξ (q) in Gauss per unit of spin (see Sect. 2.3.1) and a conventional susceptibility per formula unit of CuO2 . The sum on ξ is over the two directions normal to α. Next, we introduce a convenient simpliﬁcation. One could use (3.5.9) by absorbing the g-factor denominator into the HF coeﬃcients and work with the primed coeﬃcients via (3.3.4). Following Auler et al., [73], we ﬁnd it more convenient to deﬁne an isotropic susceptibility via χiso (q, ω) = 4 χξ (q, ω)/gξ2 , whereupon (3.5.9) becomes (N ) γ 2 kB T 1 = Aξ (q)2 χiso (q, ω0 )/ω0 . T1α 4 μ2B q

(3.5.10)

ξ

In this way only the natural anisotropy of the HF couplings from (3.3.2) comes into the T1 formula. We now present expressions for 1/T1 for the various nuclear species in YBCO, using the HF tensors developed in the text. For the c axis relaxation of Cu(2), Aξ = Aab , for both terms, so (3.5.9) becomes (N ) 1 γ 2 kB T = [Aab + 2B (cos qx a + cos qy a)]2 χiso (q, ω0 )/ω0 , T1c Cu(2) 2 μ2B q (3.5.11)

102

3 Preliminary Steps in Cuprate NMR

where the susceptibility is per CuO2 . For the ﬁeld in the ab plane, we have 1 T1ab

= Cu(2)

(N ) 1 γ 2 kB T + [Ac + 2B (cos qx a + cos qy a)]2 2T1c Cu(2) 4 μ2B q χiso (q, ω0 )/ω0 .

(3.5.12)

However, for the Cu(2) HF couplings given in Table 3.4, Ac is the dominant term, so that for 1/T1ab the contribution of 1/2T1c is essentially negligible. Unless the correlations are known to be large, a good estimate can be obtained by dropping the “B” term as well, so that the HF coupling becomes essentially independent of q. For the planar oxygen sites and the yttrium sites in YBCO the HF couplings are dominated by hybridization eﬀects with the 2s [3] and 4d [35] holes, giving HF coupling terms AO,ξ (q) = 2Cξ cos qx a/2 and AY,ξ (q) = 8Dξ cos qx a/2 cos qy a/2, (3.5.13) respectively, where it is noted that the HF coupling for the Y3+ is thought to be dominated by the 4d core-polarization HF ﬁeld [35]. The corresponding expression for the 17 O relaxation rate is, e.g., (N ) 1 γ 2 kB T 2 = [C (1 + cos qy a) + Cy2 (1 + cos qx a)]χiso (q, ω0 )/ω0 , T1c O 2 μ2B q x (3.5.14) where T1 along other axes is analogous to the case for Cu(2). For the case of 89 Y, we give here an expression in which interplanar correlations are neglected. Thus, (N ) 1 4γ 2 kB T 2 = [Dx + Dy2 ](1 + cosqx a)(1 + cosqy a)χiso (q, ω0 )/ω0 . T1c Y μ2B q (3.5.15) Kij and Xat Expressed in Terms of χ (q, ω) Dynamical AFM spin-spin correlation eﬀects in these relaxation processes are embodied in the factors such as (1 + cos qx,y a), the mean value of which will approach zero in the event of strong correlations. Such correlation factors were introduced by Mila and Rice [2], where in Sect. 3.3 they took the form Kij = 4 Siα Sjα . It is useful to introduce an equivalent deﬁnition of the Kij in terms of χ (q, ω). For example, the sum on q in (3.5.14) can be put into the form (N ) [ ] = [Cx2 + Cy2 ][1 + K01 ]Xat , (3.5.16) q

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

103

where Xat =

(N ) χ (q, ω0 ) is

ω0

q

and K01 =

(N ) 1 χ (q, ω0 ) cos kx,y a is . Xat q ω0

(3.5.17)

The quantity Xat (T ) is a fundamental dynamical index for χis (q, ω) at low frequencies. It contains the basic correlation time for the spin ﬂuctuations. Furthermore, the quantity (kB T )/μ2B )Xat ∼ kB T N (0)2 gives the correlation time along with the statistical weight of the T1 process, where N (0) is the density of states/atom at the Fermi surface for one direction of spin in an energy band environment. The other factor (1 + K01 (T )) gives the temperature variation of T1 arising from dynamical correlations for the case of transferred HF interactions. Equation (3.5.16) therefore eﬀects a separation of these two fundamental – and physically very diﬀerent – factors in the temperature dependence of T1 . To complete the picture of spin–spin correlations used for the YBCO family of compounds, we have, in analogy with (3.5.17), K12

(N ) 1 χ (q, ω0 ) = cos kx a cos ky a iso and Xat q ω0

K13 =

(N ) 1 χ (q, ω0 ) cos 2kx,y a iso . Xat q ω0

(3.5.18)

We may now introduce these forms into the T1 expressions (3.5.11)– (3.5.15). As an example we consider the expression (3.5.11), where the HF coeﬃcient factor [ ]2 may be expanded as A2α + 4B 2 + 2B 2 (cos 2qx a + cos 2qy a) + 8B 2 cos qx a cos qy a (3.5.19) + 4Aα B (cos qx a + cosqy a). Using the deﬁnitions (3.5.17) and (3.5.18), the expression for 1/T1 becomes 2 γ63 kB T 1 = Xat {A2ab + 4B 2 [1 + 2 K12 + K13 ] + 8Aab BK01 }, (3.5.20) T1c Cu(2) 2 μ2B where we recognize the same expression for the HF constants and correlation functions as in (3.3.14) and (3.3.15). Expressions such as (3.5.20) give a more direct idea of the dependence of T1 on the spin-spin correlations than expressions given earlier in terms of χ (q, ω). The corresponding equations for 17 O(2,3) and 89 Y are γ 2 kB T 1 = 17 2 Xat [Cx2 + Cy2 ][1 + K01 ], (3.5.21) T1z O 2 μB

104

and

3 Preliminary Steps in Cuprate NMR

2 1 kB T 4 γ89 = Xat [Dx2 + Dy2 ][1 + 2K01 + K12 ], T1z Y μ2B

(3.5.22)

for any permutation of axes (x,y,z). Equations (3.5.20), (3.5.21), and (3.5.22) are quite general and are useful for discussing cases where Xat (T ) and the Kij (T )’s are both changing substantially with temperature. The formulation of T1 in terms of Xat and the Kij ’s described here is the theoretical basis for the comprehensive T1 data interpretation scheme pioneered by Uldry and Meier [58], which is discussed in Chap. 5.

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc Following Mila and Rice, a number of relaxation model calculations were developed which made use of the random phase approximation (RPA) to include the eﬀects of electron–electron interactions. Several of these model calculations are reviewed in Chap. 5, as well as a proposed orbital relaxation term for the 63 Cu(2) based on the marginal Fermi liquid hypothesis [74]. Among the RPA schemes which appeared early on was an interacting Fermi liquid theory with strong AFM exchange couplings put forward by Monien and Pines (MP) [5], where they used the RPA to construct a model for χ (q, ω) with an adjustable enhancement level in the vicinity of QAF . An important innovation in this work was the introduction of an energy gap with d-wave symmetry for T1 and NMR shift calculations for T < Tc . Even though there were theoretical developments from very early on suggesting the suitability of d-wave superconductivity for the cuprates [75, 76, 77], up to this point no one had tried to interpret NMR data with the d-wave picture. In spite of the apparent success of this interpretation as seen in [5], widespread acceptance of d-wave symmetry did not occur until the dramatic conﬁrmation of d-wave superconductivity in the cuprates by means of phase jumps at Josephson junction boundaries, which was still several years away [78, 79]. The NMR modeling described here followed closely upon a successful application of d-wave theory to Raman scattering experiments [80]. The RPA theory of [5] was applied to giving a realistic account of the shift and of T1 vs. T at the Cu sites in YBCO7 for T < Tc . This ﬁrst NMR test of dwave calculations was an important step along the path of eventual adoption of the singlet d-wave interpretation of cuprate superconductivity. By this point in time, there was ample T1 data below Tc on which to apply calculations such as this. As we shall see, however, both the theoretical details and some of the data were destined to undergo revision in later years. Nonetheless, these preliminary exercises in understanding the cuprate NMR data were both very encouraging and highly suggestive.

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

105

3.6.1 The NMR Shift Behavior for T < Tc To discuss the Cu(1,2) NMR shift below Tc , we must ﬁrst address the experimental situation. We therefore digress brieﬂy here to discuss the NMR shift measurements conducted by Takigawa et al., [81] and by Barrett et al., [48]. Both papers appear to be very careful pieces of work. The biggest problem involved in such measurements is accounting for the diamagnetic shift of the internal ﬁeld in the superconducting vortex state. This was dealt with in sharply contrasting ways in the two papers cited, leading, unfortunately, to slightly diﬀerent results. Here we suggest a compromise interpretation. Correcting for Diamagnetism via Magnetization In [81] the internal ﬁeld was corrected for using an eﬀective demagnetizing factor, which is applied to the measured magnetization of the oriented powder sample. The demagnetizing factor was determined with a careful calibration procedure, which is too lengthy to discuss here. However, the risk with such a procedure lies perhaps not in the demagnetizing factors, but in using magnetization measurements on a powder sample set in epoxy. There is a risk of non-intrinsic Curie-Weiss-like anomalies aﬀecting such a procedure. Indeed, the c-axis shift for Cu(2) has an upturn below ∼ 50K which we suggest may be spurious. This is shown in Fig. 3.9(a) where the Cu(2)site shift results are plotted with corrections. Interestingly, no such feature is found for the ab-plane result. This same kind of anisotropic Curie-Weiss background eﬀect was also reported later in an attempt to determine the intrinsic normal-state susceptibility of YBCO [50]. In the present case we note that the shift corrections become nearly 0.25% as T → 0. The size and temperature dependence of this eﬀect does not seem compatible with superconducting diamagnetism. Calibration of Internal Field with the

89

Y Shift

On the other hand, in [48] the 89 Y NMR line was used as a reference for the internal ﬁeld at low temperatures, which is a very sound method in principle, as long as the 89 Y NMR shift is reliably known. If, for example, the resonance frequencies ν63 and ν89 were measured in the same ﬁeld, then we have ⎧ ⎫ ν γ ⎩ 63 89 ⎪ ⎭ + KY − 1. (3.6.1) KCu = ⎪ ν89 γ63 In practice, KY −0.03% at T = 100 K, and it was assumed [48] that KY ∝ Ys (T ), Ys (T ) being the Yosida function [82] for s-wave gap symmetry. Since one may be looking here for a d-wave Yosida function eﬀect, the foregoing assumption may cause a problem, but in fact the diﬀerence is small enough to be within the error bars. The Cu(2) shift results are shown in Fig. 3.9(b) and (c). It is noteworthy that the maximum c-axis internal ﬁeld correction (for Ks (c)) is ∼ 0.05% or only ∼ 20% of that found at low T in Fig. 3.9(a).

106

3 Preliminary Steps in Cuprate NMR

Although the latter correction cannot be arbitrarily curtailed, it seems likely that it is primarily responsible for the discrepancy between the c-axis results. The ab-plane results are also slightly outside error bars [0.37(2)% for [81] and 0.30(2)% for [48]]. However, this diﬀerence is as much a result of disparate normal-state shifts as it is of low-T corrections, which are similar. We suggest the following composite picture based on the combined results of [81] and [48]. The c-axis result of [48] is to be accepted as is, which says that Ks (c) is negligibly small on the scale of Ks (ab). The axial and isotropic shifts thus behave in a very similar fashion, since they both reﬂect the behavior of Ks (ab). Thus, we suggest that the contrasting behaviors of Kax (T ) and Kiso (T ) highlighted in [81] may have been generated, in part, by subtracting and adding the strongly corrected c-axis shift, respectively. It is suggested that the sharp contrast which results is unreliable. On the other hand, the corrected Kab (T ) curve in Fig. 3.9(a) shows a very interesting linear-T behavior below 50 K which is clearly not a result of the correction process. This may therefore be a sign of d-wave symmetry behavior, as reﬂected in the MP interpretation below. The behavior of Kax (T ) in Fig. 3.9(b) and (c) is also compatible with d-wave, as we shall see below. Both of these papers considered the isotropic 1.5 χs(T)/χs(100)

1.0 →

1.0 Cu(2)

(a)

0.8

(b)

0.6 0.4 0.2 0.0

→

H⊥ cˆ

0.5

1.0

Ks Korb

0

0

100 T(K)

(c)

0.8

200

χs(T)/χs(100)

KNIGHT SHIFT (%)

H cˆ

0.6 0.4 0.2 0.0

–0.2

0.2 0.4 0.6 0.8 1.0 1.2 1.4 T/ Tc

Fig. 3.9. (a) Corrected and uncorrected NMR shift data for Cu(2) in YBCO7 from [81] are shown plotted as a function of temperature for ﬁeld parallel (top) and perpendicular (bottom) to the c axis. The correction scheme is described in the text. Figure reprinted from M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989). Copyright 1989 American Physical Society. In (b) and (c), Cu(2) NMR shift data for YBCO7, i.e. Ks (c) - Ks (ab) normalized to 1 at 100 K, are plotted vs. T /Tc [48]. Yosida function ﬁts to the data are shown using s-wave symmetry (b) and d-wave (d’-wave) symmetries (c) from Fig. 3.10(a) as a solid (dashed) line. Fit parameters are shown in Table 3.7 and discussed in the text. Figure reprinted from S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990). copyright 1990 American Physical Society

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

107

component of shift as heavily contaminated with “oxygen hole band” eﬀects. Following MR and MR2 [2, 46], we maintain their occurrence to be unlikely. 3.6.2 The Monien-Pines Calculations of NMR Shifts below Tc MP began by applying diﬀerent pairing symmetries to the interpretation of NMR shift variation below Tc . For comparison purposes they applied the pairing symmetries shown in Fig. 3.10(a). The pure s-wave and d-wave are ﬂat and ∝ cos φ, respectively, where φ is the azimuthal angle for the cylindrical 2D Fermi surface for the CuO2 planes. They argue in detail that triplet pairing states are inappropriate for this case [5]. Then, still concerned about the possibility of an oxygen hole band, following [81] they consider only the axial component of the shift, which they suggest would reﬂect only the spin paramagnetism of the Cu(2)2+ sites 8 The data which were ﬁtted are shown in Fig. 3.10(b) [81] and in Fig. 3.9(b) and (c). 1.2

(a)

s

1.0

Data of Takigawa et al.[4] d state d´ state

1.0 s´

0.8

0.8 0.6

s

Kax(2)

Δ /Δ max

d´

0.6 d

0.4

0.4 0.2 0.2 0

(a) 0

0

π/4 φ

(b)

π/2

–0.2

0

0.2

0.4

0.6 T / Tc

0.8

1.0

1.2

Fig. 3.10. (a) Gap energy variation for several choices of gap symmetry from [5] shown as a function of azimuthal angle φ over one quadrant. (b) Plot of Ks (ax) from [81] as a function of T /Tc (dots) for temperatures in the superconducting state. The solid and dashed lines are calculated ﬁts for gap functions labelled “d” and “d ” in the (a) portion [5], as described in the text. Noteworthy is the d-wave-like linear T behavior at the lowest temperatures. Figure reprinted from H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990). Copyright 1990 American Physical Society 8

The essential assumption here is that any oxygen hole-band NMR shift would be isotropic.

108

3 Preliminary Steps in Cuprate NMR

Calculating the Yosida Function To compare with NMR shift data, the Yosida function Y(T) is calculated using the weak-coupling BCS formula for an anisotropic, singlet superconductor, ∞ ⎧ ⎫ ∂f ⎪ ⎩− ⎭ N (E), (3.6.2) Y (T ) = dE ⎪ ∂E −∞ where N (E) is the density of states, and f is the Fermi distribution function. The behavior of Y (T ) for an s-state gap is Ys (T ) ∝ exp(−Δmin /kB T ) for T Tc , Δmin being the minimum gap energy as T → 0. In contrast, for the case of a d-state gap N (E) ∝ E for E Δ(0), leading to a linear variation of Yd (T ) with T for T Tc . MP used the maximum gap value Δ(0)/kB Tc and the speciﬁc heat jump at Tc ⎫ ⎧ ⎪ ∂Δ2 ⎪ ⎪ ΔC/C ∝ ⎪ (3.6.3) ⎭ ⎩ ∂T Tc as parameters for calculating Yd (T ), which is plotted in Fig. 3.10(b). The dwave result is seen to be in good agreement with the Cu(2)-site Kax data from [81]. Values of the parameters for the cases of (i) weak-coupling BCS theory and (ii), (3.6.2) ﬁtted to the NMR shift data in Fig. 3.10(b) and in Fig. 3.9(b) and (c), are given in Table 3.7. Strong coupling eﬀects are seen to be appreciable, but also, the d-wave calculation is quite successful in reproducing the linear temperature behavior of the shift data. 3.6.3 Calculating the Relaxation Decay Curve By ﬁtting the relaxation, the viability of using d-wave gap symmetry to interpret NMR data was tested BCS theory of T1 for the d-wave case. We begin Table 3.7. Table of ﬁtting parameters Δ0 /kB Tc and ΔC/C from [5] for the NMR shift data in Fig. 3.10(b) [81] (top part) and for the data in Fig. 3.9(b) and (c) (bottom). The values of these parameters for weak-coupling BCS theory are shown on the left-hand side for comparison. The pairing states shown in Fig. 3.10(a) were used for these calculations Data Plot

Weak Coupling Weak Coupling Optimal Fit Optimal Fit ΔC/C Δ0 /kB Tc ΔC/C Pairing State Δ0 /kB Tc

Fig. 3.10(b) d Fig. 3.10(b) d

2.13 1.93

0.95 1.17

2.44 1.74

1.97 2.36

Fig. Fig. Fig. Fig.

1.76 2.10 2.13 1.93

1.43 1.27 0.95 1.17

1.90 2.16 14.7 3.13

2.77 2.49 1.76 2.14

3.9(b) 3.9(b) 3.9(c) 3.9(c)

s s d d

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

109

with a brief synopsis of the calculation of T1 [5]. In the presence of an AFM interaction Jef f (q, T ) the RPA expression for the dynamic susceptibility becomes χ0 (q, ω) , (3.6.4) χ(q, ω, T ) = 1 − N (0)Jef f (q, T )χ0 (q, ω) where χ0 (q, ω) is the ”bare spin-spin correlation function” [5]. For a T1 calculation such as (3.5.9) from the previous subsection, one only needs the imaginary or dissipative part χ (q, ω). Monien and Pines make the following approximations to treat T1 behavior below Tc . Assuming AFM enhancement eﬀects are large (such as for Cu(2) in YBCO), the enhancement denominator in (3.6.4) is ﬁrst replaced by its average, temperature-dependent value at QAF , so that (3.6.4) becomes

where

1 1 1 = , T1 (T1 )f ree [1 − λ(T )]2

(3.6.5)

λ(T ) = N (0)Jef f (QAF , T )χ0 (QAF , T ).

(3.6.6)

It was then further assumed that the real part of the dynamic susceptibility at QAF , χ0 (QAF , T ), scales with temperature like the noninteracting uniform susceptibility χ0 (q = 0, T ). T1 (3.6.5) can then be expressed in terms of the Yosida function (see Sect. 1.2.2)

as

Y (T ) = χ0 (q = 0, T )/χ0 (q = 0, Tc)

(3.6.7)

1 1 1 = , T1 (T1 )BCS [1 − λ(Tc )Y (T )]2

(3.6.8)

where 1/(T1 )BCS may be calculated for any pairing symmetry desired in the absence of quasiparticle interactions. In this simple approximation the falloﬀ of 1/T1 below Tc will be enhanced by the decline of the enhancement factor, which in turn falls oﬀ according to how the Yosida function diminishes below Tc . For other than s-wave gap symmetries, we may write the BCS relaxation expression (cf. Sect. 1.2.2) ∞ ⎧ ⎫ 1 ∂f ⎪ 2 ⎩− ⎭ [N (E) + M 2 (E)], ∝ dE ⎪ (3.6.9) (T1 T )BCS ∂E −∞ where N (E) and M (E), which account for the BCS coherence factor, are deﬁned by [83] N (E) =

⎧ ⎪ ⎪ Re ⎪ ⎩

⎫ ⎪ E ⎪ ⎪ ⎭ (E 2 − Δ2k )1/2

and M (E) = FS

⎧ ⎪ ⎪ Re ⎪ ⎩

⎫ ⎪ Δk ⎪ ⎪ . ⎭ (E 2 − Δ2k )1/2 FS (3.6.10)

110

3 Preliminary Steps in Cuprate NMR

The latter deﬁnitions allow for the possibility of a complex gap function. Combining (3.6.8) with (3.6.10) yields an expression for the relaxation rate which will decline below Tc , both because of the growth of the superconducting energy gap and because of the decline of the enhancement factor owing to the decrease in Y (T ). Because of the d-wave gap function described above, the linear-E density of states will lead to asymptotic 1/T1 ∝ T 3 behavior for T Tc . Application of MP T1 Calculations to Cu(2) Data for YBCO7 MP illustrated the above formalism by using it to ﬁt the NQR T1 data on Cu(2) in YBCO7 by Imai et al., [84]. The ﬁtting function is shown as a solid line in Fig. 3.11(a), and is seen to give an excellent representation of the data over two full orders of magnitude of the decline of 1/T1 below Tc . We make a number of remarks regarding this T1 ﬁt. First, for the d-wave gap function (see Fig. 3.10(a)), there is no vestige of the coherence peak, unlike what is found for the s-wave cases [5]. Moreover, the very steep decline found just below Tc can be achieved in two diﬀerent ways. This is illustrated by the ﬁt parameters shown in Table 3.8. The actual curve plotted in Fig. 3.11 does not allow the enhancement factor to change below Tc , for reasons to be discussed presently. As a consequence, a very large gap parameter of 5.12kB Tc is needed to cause the steep fall-oﬀ near Tc . However, MP have calculated another ﬁt curve for the data shown, corresponding to the second row of parameters in the table, which is almost indistinguishable from the ﬁrst ([5], Fig. 3(d)). In the latter case the enhancement parameter λ 0.5 (see ([5])) contributes to the decline of 1/T1 , but the gap parameter Δ0 /kB Tc = 2.44 is only half as great as for the calculation shown. This may be a more physically reasonable scenario. The corresponding (second row) parameters from Table 3.8 is in fact the same set used to ﬁt the shift data in Fig. 3.9(c). Referring to Fig. 3.11(b), the solid dots plot the same data as in the (a) panel. There we compare the decline of 1/T1 with a line of slope ∝ T 3 in the middle region and a linear T curve at the lowest temperatures. The ∝ T 3 behavior is expected at low T as mentioned earlier, because of the 63

Table 3.8. Table of ﬁtting parameters for the T1 data of Fig. 3.11(a) using a d-wave gap function [5]. The top line shows parameter values for a ﬁt assuming a constant enhancement below Tc . In this case the eﬀective value of λ is zero. The second line shows an essentially equivalent ﬁt in which λ is allowed to decay below Tc according to the d-wave Yosida function. The remaining parameters are those used to ﬁt the NMR shift data, as shown in Fig. 3.9(c) Weak Coupling Weak Coupling Optimal Fit Optimal Fit ΔC/C Δ0 /kB Tc ΔC/C λ(Tc ) Δ0 /kB Tc 2.13 2.13

0.95 0.95

5.12 2.44

1.89 1.97

0.0 0.5

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc 10

10

(a) YBCO7

(b) YBCO7 1

1/ T1 (ms–1)

1

1/ T1 (ms–1)

111

0.1

0.01

0.1

∝T3

NMR 0.01 0.001

0.001 0.0001 0.1

MP Fit

NQR 0.0001

1 T/ Tc

10

0.00001

∝T 1

10

100

1000

T(K)

Fig. 3.11. (a) NQR T1 data for Cu(2) in YBCO [84] is plotted vs. T /Tc for temperatures above and below Tc . The MP theoretical ﬁt described in the text is shown as a solid line. Figure reprinted from H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990). copyright 1990 American Physical Society (b) The same data as in part (a) are plotted as dots on a scale of absolute temperature. Also plotted for comparison are a set of NMR data (open squares) for the same nominal compound taken in a ﬁeld of 7.4 T [60]. For the NQR data the regions of data which vary as T 3 and as T are indicated with straight lines (see text for discussion). Figure reprinted from P.C. Hammel, M. Takigawa et al., Phys. Rev. Lett. 63. 1992 (1989). Copyright 1989 American Physical Society

linear-E character of N (E) which results from the d-wave gap having a line of nodes. Further, the suggested crossover to linear T behavior often results from disorder in the sample causing quasiparticle states to occur in the gap region. The progression of T 3 → T behavior has been found to occur below Tc in many non-cuprate unconventional superconductors. A few cases we could mention are 115 In in CeIrIn5 [85], 69 Ga in PuCoGa5 [86], 69 Ga in PuRhGa5 [87], and 23 Na in Na0.35 CoO2 ·yH2 O [88]. Does AFM Enhancement Decay Below Tc ? Next, we discuss the diﬀerence between the NMR and NQR data shown in Fig. 3.11(b). Along with the NMR data shown, Hammel et al., also reported a T1 curve for the (planar) O(2,3) sites over the same temperature range. Their NMR data for the Cu(2) and the O(2,3) created something of a sensation when the variation below Tc turned out to be precisely the same for these two nuclei over two decades. In terms of the MP theory outlined above the implication is that even though the Cu(2) undergoes substantial enhancement in the normal state, any such enhancement becomes temperature independent below Tc . This was taken to be a constraint on the theory, and is the reason

112

3 Preliminary Steps in Cuprate NMR

why MP calculated the solid curve ﬁt in Fig. 3.11(a) without allowing the enhancement to vary with temperature. However, the contrast between the NQR and NMR measurements suggests very strongly that there is an additional T1 mechanism operating in a high magnetic ﬁeld. Detailed studies which came later showed this to be the case, namely relaxation to the normal cores in the vortex state just as occurred in V3 Si (see Fig. 2.13). For that reason, the Cu(2) and O(2,3) relaxation curves in [60] are not really intrinsic superconducting behavior. Later studies, as we shall see in Chap. 5, show that the AFM enhancement in the SC state really does decay away to zero at low temperatures. Therefore, for the data of Fig. 3.11(a), the ﬁt calculated including enhancement decay is probably the more realistic one. In sum, we ﬁnd that the d-wave description of the YBCO7 NMR eﬀects for T < Tc according to the MP model theory was successful in an essentially quantitative way. Fitted parameter values suggest that strong-coupling eﬀects are quite important. It remained to be seen whether this kind of RPA model for the dynamic susceptibility could be applied to interpret the disparate temperature dependences which occur in the normal state. This is the theme of a series of theory papers which came soon after MP and which are expounded in some detail in Chap. 5. We shall see that the latter papers uphold the continued success of the single quantum ﬂuid picture of these systems which was initiated by the calculations of Mila and Rice. Meanwhile, the pseudo-gap eﬀect for low-doping materials came to light, and as we shall see in the next chapter, this eﬀect became a major sub-theme of cuprate physics.

References 1. R.M. Hazen, in Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), p. 121 67 2. F. Mila, T.M. Rice, Physica C157, 561 (1989) 67, 73, 81, 84, 85, 86, 87, 90, 92, 99, 102, 107 3. B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 67, 73, 81, 82, 99, 102 4. T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 68, 101 5. H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990) 68, 99, 104, 107, 108, 109, 110 6. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 68, 99 7. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 68, 99 8. J.G. Bednorz, K.A. Mueller, Z. Phys. B64, 189 (1986) 68 9. R.J. Cava, R.B. Van Dover, B. Batlogg, E.A. Rietman, Phys. Rev. Lett. 58, 408 (1987) 68 10. M.K. Wu, J.R. Ashburn, et al., Phys. Rev. Lett. 58, 908 (1987) 68 11. J.D. Jorgensen et al., Phys. Rev. Lett. 58, 1024 (1987) 68, 69 12. J.D. Jorgensen et al., Phys. Rev. B36, 5731 (1987) 69, 70 13. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B64, 014404 (2001) 69, 86, 89, 96 14. P. H¨ usser, H.U. Suter, E.P. Stoll, P.F. Meier, Phys. Rev. B61, 1567 (2000) 69, 86, 89, 96 15. N.F. Mott, Proc. Phys. Soc. London Sect. A 62, 416 (1949) 69 16. F.C. Zhang and T.M. Rice, Phys. Rev. B37, 3759 (1988) 70, 71, 82 17. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 70

References

113

18. C.M. Varma, Phys. Rev. Lett. 77, 3431 (1996) 70 19. P.W. Anderson, Science 235, 1196 (1987) 71, 78 20. P.W. Anderson, in Frontiers and Borderlines in Many-Particle Physics, ed. by R.A. Broglia, J.R. Schrieﬀer, International School of Physics “Enrico Fermi,” Course CIV (North-Holland, Amsterdam, 1988) 71, 78 21. S. Trugman, Phys. Rev. B37, 1597 (1988); B.J. Shraiman, E.D. Siggia, Phys. Rev. Lett. 60, 740 (1988); S. Sachdev, Phys. Rev. B39, 12232 (1989); C.K. Lane, P.A. Lee, N. Read, Phys. Rev. B39, 6880, (1989) 71 22. J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts, Sol. St. Comm. 63, 847 (1987) 73, 74, 97, 99 23. D. Brinkmann, L. Pauli, J. Roos, H. Zimmermann, Phys. Lett. A 124, 112 (1987) 73, 74, 75, 97, 99 24. W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 59, 1860 (1987) 73, 74, 75, 76 25. H. L¨ utgemeier, M.W. Pieper, Sol. St. Comm. 64, 267 (1987) 73, 76 26. I. Furo, A. J´ anossy, L. Mih´ aly et al., Phys. Rev. B36, 5690 (1987) 73, 76 27. C.H. Pennington, D.J. Durand et al., Phys. Rev. B37, 7944 (1988) 74, 76 28. T. Shimizu, H. Yasuoka, T. Imai et al., J. Phys. Soc. Japan 57, 2494 (1988) 74, 76, 80 29. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 74, 79, 80, 81, 84 30. F. Adrian, Phys. Rev. B38, 2426 (1988) 74 31. C.H. Pennington, D.J. Durand, C.P. Slichter et al., Phys. Rev. B39, 2902 (1989) 74 32. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B36, 5727 (1987) 75, 76, 80 33. M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B38, 2832 (1988) 76, 79, 81, 84, 85 34. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B38, 9299 (1988) 76, 85, 99 35. H. Alloul, P. Mendels, et al., Phys. Rev. Lett. 61, 746 (1988) 76, 82, 99, 102 36. G. Balakrishnan, R. Dupree et al., J. Phys. C: Solid State Phys. 21 L847 (1988) 77, 99 37. R.E. Walstedt, W.W. Warren, Jr., R. Tycko et al., Phys. Rev. B38, 9303 (1988) 79, 81, 91 38. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 79, 80, 81, 91, 92 39. Y. Yafet, V. Jaccarino, Phys. Rev. 133, A1630 (1964) 79 40. B. Bleaney, K.D. Bowers, M.H.L. Pryce, Proc. R. Soc. London A228, 166 (1955) 79 41. M. Takigawa, P.C. Hammel et al., Phys. Rev. B39, 300 (1989) 79, 81, 84, 85, 95 42. A. Abragam and B. Bleaney, Electron Paramagnetic Resonance of Transition Ions, (Clarendon Press, Oxford, 1970), p. 455 80, 83, 86, 89 43. P.W. Anderson, Phys. Ref. Lett. 3, 325 (1959) 80 44. D.E. Farrell et al., Phys. Rev. B36, 4025 (1987) 80 45. R.E. Watson, A.J. Freeman, Hyperﬁne Interactions, ed A.J. Freeman, R.B. Frankel (Academic Press, New York, 1967), p. 53 81 46. F. Mila and T.M. Rice, Phys. Rev. B40, 11382 (1989) 81, 82, 98, 99, 107 47. R.E. Walstedt et al., Phys. Rev. B45, 8074 (1992) 83, 96 48. S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 84, 85, 95, 99, 105, 106 49. W.C. Lee, D.C. Johnston, Phys. Rev. B41, 1904 (1990) 85, 87 50. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990) 85, 105 51. A.K. McMahan, R.M. Martin, and S. Satpathy, Phys. Rev. B38, 6650 (1988) 86 52. J. Owen, J.H.M. Thornley, Rep. Prog. Phys. 29, 675 (1966) 86

114 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63. 64. 65. 66. 67. 68. 69. 70. 71. 72. 73. 74. 75. 76. 77. 78. 79. 80. 81. 82. 83.

84. 85. 86. 87. 88.

3 Preliminary Steps in Cuprate NMR D.L. Randles, Proc. Roy. Soc. London, Ser. A331, 85 (1972) 86 F. Mila, Phys. Rev. B38, 11358 (1988) 87 T. Moriya, J. Phys. Soc. Japan 19, 681 (1964) 88 V. Heine, Phys. Rev. 107, 1002 (1957) 89 J.A. Martindale, S.E. Barrett et al., Phys. Rev. Lett. 68, 702 (1992) 91 A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 91, 104 M. Takigawa, P.C. Hammel, et al., Phys. Rev. Lett. 63, 1865 (1989) 93, 94, 95, 96 P.C. Hammel, M. Takigawa et al., Phys. Rev. Lett. 63. 1992 (1989) 93, 97, 99, 111, 112 M. Horvati´c, Y. Berthier, et al., Physica C159, 689 (1989) 93, 95 C. Coretsopoulos et al., Phys. Rev. B39, 781 (1989) 93 R. Sternheimer, Phys. Rev. 84, 244 (1951); 86, 316 (1952); 95, 736 (1954) 94 H. Alloul, A. Mahajan, H. Casalta, O. Klein, Phys. Rev. Lett. 70, 1171 (1993) 96 H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989) 96, 98 N. Bulut, D.W. Hone et al., Phys. Rev. B41, 1797 (1990); Phys. Rev. Lett. 64, 2723 (1990) 97, 99 H. Monien, D. Pines, C.P. Slichter, Phys. Rev. B41, 11120 (1990) 98 V.J. Emery, G. Reiter, Phys. Rev. B38, 4547 (1988) 98 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 99 V. Jaccarino, in Physics of Solids, International School of Physics ”Enrico Fermi”, Course XVIII (Academic, New York, 1967) 99 H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990); N. Bulut, D. Scalapino, Phys. Rev. B45, 2371 (1992) 99 A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 99 T. Auler, M. Horvatic et al., Physica C313, 255 (1999) 101 C.M. Varma, P. Littlewood et al., Phys. Rev. Lett. 63, 1996 (1989) 104 C. Gros, R. Joynt, T.M. Rice, Z. Phys. B68, 425 (1987) 104 F.C. Zhang, C. Gros, T.M. Rice, H. Shiba, Supercond. Sci. Technol. 1, 36 (1988) 104 G. Kotliar, J. Liu, Phys. Rev. B38, 5142 (1988) 104 J. Kirtley, C.C. Tsuei, et al., Nature (London) 373, 225 (1995) 104 D.H. Wollman, D.J. van Harlingen, et al., Phys. Rev. Lett. 74, 797 (1995) 104 H. Monien, A. Zawadowski, Phys. Rev. Lett. 63, 911 (1989) 104 M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 105, 106, 107, 108 K. Yosida, Phys. Rev. 110, 769 (1958) 105 D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, Vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 109 T. Imai, T. Shimizu, H. Yasuoka, J. Phys. Soc. Jpn. 57, 2280 (1988) 110, 111 G.-q. Zheng, et al., Phys. Rev. Lett. 86, 4664 (2001) 111 N.J. Curro, et al., Nature 434, 622 (2005) 111 H. Sakai, Y. Tokunaga, et al., J. Phys. Soc. Japan 74, 1710 (2005) 111 T. Fujimoto, G.-q. Zheng, et al., Phys. Ref. Lett. 92, 047004 (2004) 111

4 Pseudogap Eﬀects in Cuprate NMR Studies

Up to this point the discussion has focused on fully oxygenated YBCO7 and nearby compositions, for which Tc is very near its peak value 92 K for this compound. In 1989, detailed studies began to appear for underdoped YBCO7x, x ∼ 0.4, as well as for La2−x Srx CuO4 over its entire range of superconducting behavior 0.05 ≤ x ≤ 0.35. These phases brought new and surprising eﬀects to light, detailed theories for which are only recently beginning to appear. The principal new eﬀect was a gapped appearance to the NMR shifts, susceptibility, and low-energy excitations via 1/T1 T . These eﬀects were at ﬁrst attributed to pairing correlations forming at temperatures well above Tc , since there appeared to be no clear distinction between the pseudogaps and superconducting gaps. In the prevailing notion of “spin-charge separation” these eﬀects were initially called “spin gaps” in the mistaken belief that they only aﬀected spin–magnetic properties. Eventually, energy gaps were observed with a wide variety of probes (e.g. ARPES), uncovering a major element in the phenomenology of cuprate superconductivity. In this chapter we recount the beginnings as well as the current status of the pseudogap eﬀect. In the pre-pseudogap days, the behavior of YBCO7 did not appear to be aﬀected by pseudogap eﬀects. With its relatively ﬂat susceptibility and Korringa-like relaxation for the 89 Y and 17 O, the NMR properties seemed to resemble a normal Fermi liquid. However, in retrospect, such a simple picture was illusory. A cuprate with no trace of a pseudogap is clearly a very special case, and the vast majority of other phases which came to light were dominated by pseudogap behavior. Typically, as the doping level decreases from the optimum Tc value, (i) the susceptibility develops a gapped appearance, beginning at progressively higher temperatures, (ii) the temperature variation of 1/T1 T for 89 Y and 17 O develops a similar shape, while that for 63,65 Cu(2) remains non-monotonic with a peak at a lower temperature, and (iii) instead of a sharp break downward in the NMR shift and 1/T1T below Tc , these quantities execute smooth, declining curves through Tc without any noticeable discontinuity in slope. Among conventional superconductors, behavior such as this is unknown.

R.E. Walstedt: Pseudogap Eﬀects in Cuprate NMR Studies, STMP 228, 115–157 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 4

116

4 Pseudogap Eﬀects in Cuprate NMR Studies

Δν (MHz)

We illustrate these eﬀects with data from two early NMR papers on the pseudogap [1, 2]. Similar results for the Cu(2) were given by Horvati´c et al. [3] and Yasuoka et al. [4]. Warren et al. presented NQR curves for 1/T1 T vs. T for 63 Cu(2) and similar NMR measurements for 89 Y in the Tc 64 K phase of YBCO7-x, 0.3 ≤ x ≤ 0.51 . These are shown in Fig. 4.1

(a)

30

0.4 0

1 / T1 T (s K)–1

60

80

100

TEMP (K)

20

10

63Cu

0 0

100

200

300

T(K) 0

1 / T1 T (10+4 s K)–1

(b) 2

1 89Y

0

0

100 200 TEMPERATURE (K)

300

Fig. 4.1. (a) 1/T1 T is plotted vs. T over the interval 40K ≤ T ≤ 300K for two NQR peaks associated with 63 Cu(2) sites in YBCO6.64 (Tc 64K) [1]. For comparison, the dashed line shows the behavior recorded earlier for the YBCO7 phase (Tc 90K). The inset shows the shift in the resonance frequency of the NQR coil which occurs as the sample goes superconducting at T 64K. (b) 1/T1 T is plotted vs. T for 89 Y NMR in the same sample used as in (a). These data show a sharp deviation from YBCO7-phase Korringa behavior, which is characteristic of the pseudogap. Figure reprinted from W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 62, 1193 (1989). Copyright 1989 American Physical Society 1

Although a continuum of Tc values has been reported for YBCO7-x, the 60 K phase is the most homogeneous underdoped phase, since dTc /dx is quite small in that region.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

117

where the low-frequency excitation spectrum ( q A2q χ (q, ω)/ω) is seen to decline at low temperatures as though an energy gap had set in below T ∼ 300 K. At Tc 64 K there is no break or other feature in the Cu(2) T1 data (Fig. 4.1(a)), in complete contrast with the sharp drop which takes place for the YBCO7 phase (see Fig. 3.11). Nonetheless, monitoring the rf coil susceptibility (Fig. 4.1(a), inset) gives good evidence that the sample material undergoes a transition to bulk superconductivity at that temperature. This behavior will be conﬁrmed below for this as well as other cuprates. A second body of both NMR shift and relaxation data for 89 Y in YBCO6+x is shown in Fig. 4.2, where curves with very similar shapes for both parameters are presented [2]. There, a progressive gapping eﬀect is seen to advance steadily from x ∼ 1.0 to the non-superconducting phase at x ∼ 0.4. Although these results were ﬁrst interpreted on a Fermi-liquid model, that interpretation was later revised [5]. In retrospect, the results concerned appear to establish another important pseudogap result contrary to the usual Korringa behavior. The relaxation rate product 1/T1 T is very nearly proportional to Ks (T ) and therefore to the spin susceptibility χs (T ). In Sect. 4.1 we will discuss the physical meaning of this along with a theoretical model which yields this result. Reference was made [2] to the theoretical prediction by Friedel [6] that precursive pairing eﬀects in 2D superconductors might give rise to a “pseudogap” well above Tc in the excitation spectrum. As we shall see in Sect. 4.2, the pseudogap also turned up fairly quickly in charge-related eﬀects such as speciﬁc heat and ARPES data. We mention one ﬁnal result which appeared around the same time as the foregoing eﬀects were reported, namely the susceptibility scaling eﬀect for underdoped LSCO which was reported by D.C. Johnston [7]. It was found that χs (T ) for a series of underdoped samples of La2−x Srx CuO4 not only exhibited a gap-like feature, but were found to scale rather precisely with a reduced temperature variable T /T ∗ . Although this eﬀect was interpreted at the time in terms of a theoretical model for insulating antiferromagnets and was not linked for some time with the pseudogap eﬀect, it seems clear in retrospect that it was, in fact, closely related to the eﬀects presented above for YBCO7-x. Later in this chapter we shall also discuss pseudogap eﬀects in the high-Tc systems LSCO and Y248.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x Since spin pseudogap eﬀects in the NMR data ﬁrst came to light in studies of YBCO7-x with some depletion of the oxygen content (and thus of hole doping), it was for this system that the most precise and comprehensive bodies of data were ﬁrst developed. In this section we present and discuss a set of results on both the NMR shifts and relaxation rates for 89 Y, 17 O(2,3), and

118

4 Pseudogap Eﬀects in Cuprate NMR Studies

63

Cu(2) for a representative composition YBCO6.63 [8, 9, 10]. This compound is a well-characterized example of a high-Tc pseudogap system. –ΔK (ppm) 50

x = 1.0

1–ε

0.85 0.75 0.63 0.53

0

0.48 0.35 0.41

–50

(a) 89Y

–100

104 (T1T)–1 (sec °K)–1

2

ν0 = 15.64 MHz

Y Ba2 Cu3 O6 + x 200 T (°K)

100 3

89Y

NMR

300

NMR

(b)

ν = 15.64 MHz x=1 1–ε 0.85

0.75 0.63 0.53 0.48

1

0.41

Y Ba2 Cu3 O6 + x 0

100

200 T (°K)

300

Fig. 4.2. (a) The negative of the 89 Y NMR shift ΔK is plotted as a function of temperature for a series of compositions YBCO6+x, for 0.4 ≤ x ≤ 1.0 [2]. ΔK is measured relative to the 89 Y gyromagnetic ratio found with a solution of YCl3 . In Sect. 4.1 the chemical shift is determined to be 89 Korb,α 160 ppm, where α = ab,c. (b) Plots of 1/T1 T vs. T for the same series of compositions used in (a) [2]. In both cases the data show the progressive development of a pseudogap eﬀect in which they exhibit a maximum at progressively higher T for increasing dilution of hole carriers. These data can also be plotted to show the relation 1/T1 T ∝ (89 Korb,α − ΔKα (T )) characteristic of the pseudogap region. Figure reprinted from H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989). Copyright 1989 American Physical Society

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

(a)

(b)

Fig. 4.3. Continued

119

120

4 Pseudogap Eﬀects in Cuprate NMR Studies

4.1.1 HF Parameters for YBCO6.63 from Scaling of Shift Data We ﬁrst discuss NMR shift and susceptibility data for YBCO6.63. In Fig. 4.3(a) NMR shift data for 63 Cu(2) in an oriented powder specimen are plotted for ﬁeld orientation both parallel to and perpendicular to the c axis [1]. The c axis data show only a slight increase below Tc , so that 63 Korb,c = 1.28(1)% and 63 Ks,c = –0.01(1)% (near 300K). This result for 63 Korb,c is indistinguishable from that for YBCO7.0 [11]. The zero–temperature intercept for 63 Kab (T ) is 63 Korb,ab = 0.25(2)%, which is also unchanged from YBCO7 [11]. The downward–curving spin paramagnetism is the essence of spin pseudogap behavior. In Fig. 4.3(b) are plotted 17 O NMR shift values (17 K , 17 K⊥ , 17 Kc ) as functions of temperature for the three principal axes of the O(2,3) sites [9]. The quadrupole tensor has also been evaluated and is virtually indistinguishable from what was determined for YBCO7 (see Fig. 3.8 and discussion). The shift 17 K (T ) corresponding to the Cu(2)-Cu(2) bond axis is seen to be more than half again as large as the transverse components. The latter (17 K⊥ (T ) and 17 Kc (T )) have slightly diﬀerent chemical (i.e. orbital) shifts, but their temperature variation is essentially indistinguishable. The 17 O(2,3) shift can therefore be characterized by axial and isotropic components deﬁned by 17 Kax = (17 K - 17 K⊥ )/3 and 17 Kiso = (17 K + 17 K⊥ + 17 Kc )/3. As with YBCO7 (Sect. 3.4) there is a dominant isotropic HF eﬀect from 3d-2s hybridization [12] and a lesser axial shift term corresponding to dipolar coupling from the 3d-2pσ hybridization, although the latter admixture is much greater than the former. The 17 O NMR shifts for 17 K and 17 K⊥ , plus that for 63 Cu(2) [9] have been scaled to coincide with 17 Kc (T ), the most accurate data set, between Tc and 300K, and are plotted with separate vertical axes in Fig. 4.4. All shifts are seen to follow a common temperature variation very closely, i.e. that of the spin susceptibility. From the scaling ﬁts the following relations are obtained: Fig. 4.3. (a) The NMR shift for 63 Cu(2) in an oriented-powder sample of YBCO6.64 [8] is plotted vs. temperature for ﬁeld orientation parallel and perpendicular to the c axis. The upper solid line is a representation of data for YBCO7, while the lower one is a guide to the eye. As with YBCO7 it is assumed that the orbital shifts are independent of temperature and that the spin susceptibility goes to zero at T Tc . The breakdown of both shifts into spin and orbital components is given in the text. Figure reprinted from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990). copyright 1990 American Physical Society (b) Data for the 17 O(2,3) NMR shift is plotted as a function of temperature up to 300K for an oriented powder sample with ﬁeld oriented along three mutually perpendicular axes, where the axis for 17 K is the Cu(2)-Cu(2) bond axis [9]. The solid line is the variation of 17 Kc (T ) for YBCO7 [11]. Analysis of these results is given in the text. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). copyright 1991 American Physical Society

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x 17

121

Kax (T ) = 0.1886 ×17 Kc (T ) + 0.0151%,

(4.1.1a)

Kiso (T ) = 1.057 × Kc (T ) + 0.039%, 63 Kab (T ) = 1.522 ×17 Kc (T ) + 0.32%.

(4.1.1b) (4.1.1c)

17

17

This result gives additional strong evidence for a one-component quasiparticle state, since multiple bands would have to have susceptibilities with precisely matching spin-gapped temperature variation to produce this result. Such an eﬀect seems quite implausible. 0.2

0.25

10

0.05

0.6

0.2

χ

0.4

(%)

(%) 17K C

0.15

1 0

17K ax

(%) 17K iso

0.5

63K ab

(%)

0.04

6 5

10 15 20 25

1000/T(K) 0.1 17

0.03

17

Tc

0.1

17K iso 63 Kab

y = 0.37

0.05

Kc Kax

4

2

χspin [10–5 emu/mol Cu (2)]

0.15

8

ΔGap = 104K

0.02 0.05 0

100

200

0 300

T (K)

Fig. 4.4. (a) Data for 63 Kab (T ) for the Cu(2) sites [9] (similar to Fig. 4.3(a)) as well as for 17 K (T ) and 17 K⊥ (T ) have been scaled to 17 Kc (T ) and are plotted with the latter data as a function of temperature. The T → 0 (orbital shift) limits of these shifts plots have been determined as discussed in the text, leading to an estimate for the zero of the spin components of the shifts and of the spin susceptibility. Scales for the various shift components are shown on the left. The scale for χs (T ) has been estimated from the knowledge of HF constants (see text) and is shown on the right side of the plot. The solid line represents the estimate of χs (T ) so determined. The inset shows an Arrhenius plot of ln(χs (T )) vs. 1000/T(K). The linear behavior suggests an energy-gap nature for χs (T ), where ΔGap 104K. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). copyright 1991 American Physical Society

The scaled curves in Fig. 4.4 come apart a bit below Tc , an eﬀect which is attributed to varying levels of diamagnetic shielding for the diﬀerent cases. However, because 17 K and 17 K⊥ are both measured with ﬁeld ⊥ c axis, there is no diamagnetic correction to 17 Kax . Directly from extrapolating the

122

4 Pseudogap Eﬀects in Cuprate NMR Studies

curves in Fig. 4.3(b) to T = 0, then, one ﬁnds 17 Kax (0) = 0.013(2)%. One can then use the (4.1.1) to obtain the other orbital (i.e. zero temperature) shift values. One ﬁnds 17 Kc (0) = -0.014(7)%, 17 Kiso (0) = 0.024(11)%, and 63 Kab (0) = 0.30(2)%. These values are virtually unchanged from 17 O orbital shifts determined earlier for YBCO7 (See Table 3.2). Using the relation χs (T ) = 63 Kab (T )/fCu (Aab + 4B), where Aab + 4B 198 kOe/μB [13], and the estimate fCu 0.7 for the fraction of χs which resides on the Cu(2) site, the scale shown for χspin (T ) in Fig. 4.4 has been determined. The parameters derived from a Mila-Rice ﬁt to the data in Sect. 3.2 (see Table 3.4) would give a slightly larger value for (Aab + 4B). Other ﬁts to the shift and relaxation data in Chap. 5 will also give slightly diﬀerent values for the scale of χs (T ). We only note that this scaling factor is not critical at this point. It will be discussed further in Chap. 5. Regardless of the scale of χs (T ), we may examine the question of its gapped nature by plotting the data of Fig. 4.4 in an Arrhenius plot, i.e. as χs (T ) = χ0 exp(−ΔGap /T ). Such a plot is shown in the inset to Fig. 4.4,2 where it is found to yield a very accurate representation of the data, with ΔGap 104K. Such a result was implied by the ﬁtting procedure of Uldry and Meier [14], to be discussed in Chap. 5. To our knowledge, this representation has not been predicted by any model calculation up to now and has not been emphasized in the literature. This result will be compared with INS data on a similar sample below. The 89 Y NMR shift and relaxation data which came two years later [10] completed the NMR data picture for YBCO6.63. The corresponding shift data for both YBCO6.63 and YBCO7 cases were plotted vs. T as in Fig. 4.5(a), where the “6.63” data are seen to exhibit a very similar temperature dependence as the scale plot Fig. 4.4. This idea is tested in Fig. 4.5(b) where the latter data for both ﬁeld orientations are plotted vs. 17 Kc (T ) data from Fig. 4.3. The resulting curves are straight lines within narrow error limits, and the extrapolation to 17 Kc (0) = -0.014(7)% then gives the chemical shifts 89 Korb,c = 160(15) and 89 Korb,ab = 152(10) ppm. Thus, the 89 Y shift data also follow the curve in Fig. 4.4 to high precision. Scaling of HF Coeﬃcients to Match YBCO7. We therefore have a complete characterization of NMR shifts for all signiﬁcant sites and ﬁeld orientations in YBCO6.63 in terms of a single universal curve [9]. The resulting shift values at T = 300K are listed in Table 4.1 (“300K Values”). Also listed there is the estimated Cu(2) susceptibility tensor at 300K from [9]. We suggest, however, that the latter values are very approximate and that better values for both the susceptibility tensor and the HF coeﬃcients can be assigned by scaling the HF tensor components so that they match the 2

Please note that this inset was not part of the original ﬁgure in [9], but was added later.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

123

200

–89

K (ppm)

(a) 100

O7

Kc Kab

0 O6.63 Kc Kab

–100 0

100

200 T (K)

300

100 (b)

0

89

Kc

89

Kab

–89

K (ppm)

50

–50

–100

0

0.05

0.1 17

0.15

Kc (%)

Fig. 4.5. (a) The negative of the 89 Y NMR shift in YBCO6.63 is plotted as a function of temperature for applied ﬁeld both parallel and perpendicular to the c axis of an oriented powder sample [10], which is actually the same sample used in the foregoing Cu(2) and O(2,3) NMR studies [9]. For comparison, previous data on YBCO7 [10] are also shown. (b) The YBCO6.63 shift data from part (a) are plotted vs. the oxygen shift data 17 Kc (T ) from [9]. Extrapolation of these curves to 17 Kc (0) yields the chemical shift values for 89 Y given in the text. These linear ﬁts also demonstrate that all NMR shifts in YBCO6.63 follow the same temperature dependence, namely that of χs (T ). Figure reprinted from M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993). Copyright 1993 American Physical Society

YBCO7 values from Tables 3.4 and 3.6 as closely as possible. For convenience, the latter set of values (“YBCO7 (Ai )”) is listed in Table 4.1. A “trial” set of HF coeﬃcients can be deﬁned from the data in Table 4.1 using the relation from (3.3.4) Ai = NA μB Ki /zi χsi ,

(4.1.2)

where Ki are the “300K” values from the table, zi are the numbers of Cu(2) neighbors, and χsi is the appropriate susceptibility estimate from the same

124

4 Pseudogap Eﬀects in Cuprate NMR Studies

Table 4.1. The NMR shift tensors for 17 O(2,3) and 89 Y in YBCO6.63 at 300 K [9, 10] are listed in the top line, then the corresponding HF coeﬃcients are stated for YBCO7 from Tables 3.4 and 3.6, below which the scaled coeﬃcient values for YBCO6.63 derived from the stated shift values are listed for comparison. The scaling procedure is described in the text, wherein the weighted sum of fractional errors deﬁned by (4.1.3) is minimized. Weighting factors wi are designed to give each species the statistical weight it has in the unit cell. NMR shift values are given in %, the spin HF coeﬃcients in kOe/μB , and susceptibilities in 10−6 emu/Cu(2) Shift Comp.

63

Ks,ab

17

300K Values 0.218 (2) Aab

Spin HF Coef. YBCO7 (Ai ) 155 YBCO6.63 152 Ri 1.370 4 wi

Ks,a

17

Ks,b

17

Ks,c

89

Ks,ab

89

Ks,c χs⊥ (300 K) χs (300 K)

0.205 0.124 0.143 0.0173 0.0255 Ca

Cb

Cc

72 44 38 71.4 43.2 40.0 1.386 1.372 1.470 8/3 8/3 8/3

Dab

Dc

1.71 1.51 1.231 1

1.86 1.87 1.338 1

58

72

80

100

line of the table. The Ai are multiplied by a scaler S, which is then adjusted to minimize a weighted total fractional squared error deﬁned by ERR =

wi [SAi − Ai ]2 = wi [1 − SRi ]2 , 2 A i i i

(4.1.3)

where the YBCO7 coeﬃcients are labelled Ai , and Ri = Ai /Ai . This procedure will also yield a new estimate of the susceptibility tensor, from (4.1.2), of χsi /S. The ratios Ri are listed in Table 4.1, and are seen to be grouped closely around a value 1.36. It is easy to show that the errors are minimized when wi Ri (4.1.4) S = i 2 = 0.723. i wi Ri The optimally scaled coeﬃcients obtained are stated in Table 4.1 (“YBCO6.63”). Correspondence with the YBCO7 values is seen to be quite satisfactory. The resulting (scaled) susceptibility components are also given. They are somewhat larger than the values from Fig. 4.4, but are ∼ 80% of the corresponding values in Table 3.4, in reasonable agreement with the relative values shown by experimental data given by Takigawa et al. in [9]. One important consequence of this ﬁtting procedure is that the reduction factor 0.70 used to estimate the HF coeﬃcients in Table 3.4 is corroborated by the YBCO6.63 shift scaling (Fig. 4.4) results. These results strongly suggest (2) that the composite Cu(2) shift coeﬃcient, for which we ﬁnd the value Aab 155kOe/μB (Table 4.1), must, in fact, be rather smaller than the value 198kOe/μB given by Monien et al. [13].

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

125

Next, we consider the anisotropy of the 17 O(2,3) and 89 Y HF coeﬃcients and Dα , respectively. Not surprisingly, the Cα have a strong axial component along the Cu(2)-Cu(2) bond axis owing to the 2pσ hybridization. The observed c/a axis anisotropy is, however, mainly a g-factor eﬀect. The constants Cα to be used in the main Hamiltonian (3.3.4) are proportional to gα Cα , which diﬀers by only a few percent between the b and c axes. This is within the expected errors. The Dα values, however, display a clear anisotropy if we consider the quantities g Dc vs. g⊥ Dab , where the former is ∼ 30% larger. The origin of this eﬀect is not clear, but the Y 3+ HF response is clearly more than simply the isotropic core polarization HF ﬁeld, as noted in [9]. Cα

Dipolar Contribution to

89

Y HF Coupling.

One candidate eﬀect for the Dα anistropy is direct dipolar coupling from the Cu2+ moments, which has been considered by Takigawa et al. [10]. Since the 89 Y HF couplings are rather small for YBCO, one must considerthe possibility that the dipolar interaction between any Cu2+ moment − α gα μB Sα u ˆα , where u ˆα is a cartesian unit vector, and a 89 Y nuclear spin moment 89 I, 89 ( I · r) g S r γ89 μB α α α (89) α Hdip = − (4.1.5) gα Sα 89 Iα − 3 2 r3 r α is a signiﬁcant HF energy. The importance of this is that (4.1.5) does not have the simple diagonal form of (3.3.2), thereby changing the nature of the dynamical calculations if it is an important eﬀect. To consider the direct dipolar HF coupling with the 89 Y, we note that owing to hybridization, the Cu2+ moment at the origin (Fig. 2.1(b)) actually consists of a fraction 1 − 4δ on the Cu(2) site and fractions δ located on the four nn O(2,3) sites. At the hybridization level δ 0.08, the two O(2,3) sites nearest the 89 Y are quite signiﬁcant, since they are rather closer to the Y 3+ than the Cu(2). We ignore the two more distant O(2,3) sites in this estimate. The positions of various ions in the crystal (Fig. 3.1) are such that the Cu(2)O(2,3) horizontal distance is d = 1.95 ˚ A, and the vertical distances between 89 Y and Cu(2) and O(2,3) are Δc1 = 1.65 ˚ A and Δc2 = 1.42 ˚ A, respectively. Using (4.1.5) we then ﬁnd for the total contribution to the HF coeﬃcients ⎧ ⎫ ⎧ ⎫ 1 − 4δ ⎪ d2 ⎪ δ ⎪ d2 ⎪ ⎪ ⎪ ⎪ ⎪ − 3 + − 3 = −8μB ΔDdip,ab ⎩1 ⎭ ⎩2 3 2 3 2 ⎭ (4.1.6a) rCu rCu rO rO ⎧ ⎫ ⎧ ⎫ 1 − 4δ ⎪ Δc12 ⎪ 2δ ⎪ Δc22 ⎪ ⎪ ⎪ ⎪ ⎪ 1 − 3 + 1 − 3 = −8μB ΔDdip,c ⎩ ⎭ 3 2 3 ⎩ 2 ⎭ ,(4.1.6b) rCu rCu rO rO ˆ + kΔc1 ˆ ˆ where rCu = ˆid + jd and rO = ˆid + kΔc2. Inserting the foregoing numbers into these equations, we ﬁnd ΔDdip,ab = 0.14 kOe/μB and ΔDdip,c = -0.28 kOe/μB . These are of the order of 20-30% of Dα and so they are quite appreciable as suggested in [9]. However, since they have the opposite sign of

126

4 Pseudogap Eﬀects in Cuprate NMR Studies

the observed anisotropy, it is clear that there is another source of anisotropy which is twice as large.3 The other noteworthy point is that there are a number of dipolar terms which are eﬀective for the T1 process but which have an angular dependence which does not vanish at the “magic angle” and therefore may be considerably larger than the shift coeﬃcients estimated above. Thus, one may not ﬁnd that T1 for 89 Y exhibits the expected anisotropy from the measured Dα coeﬃcients. The dipolar eﬀects for the 89 Y were also discussed in detail by Auler et al. [15]. We shall address this matter further in the next subsection. 4.1.2 A Simple Model Theory of Spin Dynamics for YBCO6.63 The Spin-Hamiltonian formulation of HF coupling at the Cu2+ sites combined with the Mila-Rice-Shastry [12, 16] picture of transferred HF couplings from the Cu2+ moments to the Y and O(2,3) sites provides a deﬁnite basis for discussing electron spin-based static and dynamic NMR properties. In the last subsection we saw that one ﬁnds a consistent picture of HF couplings from NMR shift data, which apply to both YBCO7 and YBCO6.63. The coupling constants we refer to here are found in Tables 3.4, 3.6, 4.1. They were used in the Mila-Rice discussion of T1 in Chap. 3. Meanwhile, here we consider the relaxation properties of YBCO6.63, where spin-spin correlations will be used to discuss comparative temperature variations of T1 in terms of dynamical spin ﬂuctuations. As was noted in Sect. 3.3.3, dynamical spin correlations are the apparent cause of the T-varying 63 Cu(2) T1 anisotropy for YBCO7 [17]. Although a comparable data set is not available for YBCO6.63, we shall ﬁnd application in this case for similar formulations of the 89 Y and 17 O(2,3) relaxation properties as well as the 63 Cu(2). Let us anticipate some of the themes as well as stumbling blocks which arise in the course of trying to account for the relaxation behavior of the YBCO6.63 (60 K) phase. First, we note the pervasive characteristic temperature variation 1/T1 T ∝ Ks (T ), which arose in an empirical way, but then found a measure of theoretical justiﬁcation [18]. Secondly, the case of 89 Y has two special problems, which have been discussed by Takigawa et al. [10]: (i) The direct dipolar interaction is large enough to make an important contribution to the overall HF coupling, as we saw in the previous subsection. Thus, the HF coupling Hamiltonian does not have the simple form of (3.3.2). This complicates the relaxation calculations. (ii) The 89 Y relaxation is driven by Cu2+ spin moments in neighboring CuO2 planes (see Fig. 3.1), so the question of interplanar spin correlations is an important one for T1 . As there is neutron-scattering evidence for such correlations [19], the 89 Y T1 phenomena are more complex on that account. 3

A simple sign check is the following: For the c–axis case, ΔDdip,c has the same sign as for the limit Δc1, 2 → 0. In the latter case, ”up” moments on the Cu(2) or O(2,3) sites would clearly give ”down” (i.e. negative) HF ﬁelds at the 89 Y sites, in accord with the calculated result.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

127

T1 Enhancement and a Model Susceptibility for Underdoped Cuprates. It was ﬁrst noted empirically that the quantity (T1 T Ks (T ))−1 is approximately constant for 89 Y and 17 O(2,3) in both the YBCO7 and YBCO6.63 phases [8]. Moreover, the same quantity for the 63 Cu(2) no longer exhibits a peak around 150 K, but executes a roughly power-law rise as T approaches Tc in the normal state. These behaviors are shown in Fig. 4.6 using data from various sources (see ﬁgure caption). Interestingly, the 63 Cu(2) data for YBCO7 show a similar temperature characteristic. The 89 Y and 17 O(2,3) shown indicate very little change with T , i.e. 1/T1T ∝ χs (T ). Later, more complete data, however, deviated from this simple picture. The data plotted in Fig. 4.6 are scaled as [T1 (Korr.)/T1 (T )][Ks (300K)/ Ks (T )], where T1 (Korr.) = Ns γe2 /(4πkB T γn2 Ks2 ), (4.1.7) which is the usual Korringa expression with a factor Ns to account for multiple sources of HF ﬂuctuations. Here, Ns = 4, 2, and 8 for Cu(2), O(2,3) and Y, respectively. Note that Ns = 4 for the c-axis Cu(2) T1 process, which is dominated by the four nn couplings. The shift has also been normalized arbitrarily to its room-temperature value, so that the absolute values plotted are only a relative indication of ﬂuctuation enhancement levels. Clearly, for Cu(2) the YBCO6.63 case is smartly enhanced over the YBCO7, and both of these by a considerable margin over the ligands. These eﬀects are attributed to AFM ﬂuctuations, which barely touch the ligands, but strongly enhance the Cu(2) relaxation and increase quickly with carrier dilution. The proportionality between 1/T1 T and Ks (T ) is suggested by the model form [8, 22] πχ0 ω χ (q, ω) = G(q) (4.1.8) Γ for the low-frequency dynamics (ω Γ ) of the quasiparticles, where χ0 is interpreted as an estimate of the static susceptibility, and the factor G(q) embodies any q-dependent enhancement eﬀects which occur. Since 1/T1 T ∝ G(q), this form suggests that 1/T1 T ∝ χ0 . To use this form even when χ0 q has the gapped temperature characteristic of an underdoped cuprate is to go beyond the usual mean-ﬁeld theory interpretation of (4.1.8). Nonetheless, this procedure has been adopted in order to treat T1 phenomena in spin-gapped superconductors [23]. However, not long after the latter work appeared, a theoretical model was developed which actually exhibited such behavior. This was the “attractive” (i.e. negative-U) Hubbard model of Randini and Trivedi, which was studied using QMC techniques [18]. The authors only studied local, q-independent HF couplings, and emphasized that this was not a suitable model for cuprate physics in other ways. Nonetheless, their results for the gapped behavior of both susceptibility and 1/T1 T , shown in Fig. 4.7, give a remarkably realistic version of the eﬀects seen in Fig. 4.6 for, e.g. the 89 Y and 17 O(2,3) sites.

4 Pseudogap Eﬀects in Cuprate NMR Studies (T1T)–1 (sK)–1

128

100

8

6

4

KORRINGA RATIOS

0

50

T (K)

300

10 5

1 50

70

90

200

300

T (K)

Fig. 4.6. The quantity [T1 (Korr.)/T1 ][Ks (300 K)/Ks (T )] is plotted vs. T in a log-log plot over the range 50 K ≤ T ≤ 300 K for a series of cases as follows: Open and closed circles are for 63 Cu(2) in YBCO6.63 [8] and YBCO7 [17], respectively. Closed squares are 89 Y data from Alloul et al. [2] using, however, an independently determined value for the 89 Y chemical shift [8]. (A similar value was reported later by Alloul et al. [5].) The open squares are data for YBCO7 from [20] using the same chemical shift. Finally, the open triangles represent 17 O(2,3) data on YBCO7 from [21]. See text for a deﬁnition of T1 (Korr.) Figure reprinted from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990). Copyright 1990 American Physical Society

To account for the Cu(2) data would require inclusion of q-dependent enhancement eﬀects in the negative-U Hubbard model, which has not, to our knowledge, been done. In any case, the results of Fig. 4.7 oﬀer some support for the phenomenological treatment based on (4.1.8) with χ0 = χs (T ). 4.1.3 INS Data for the Pseudogap of Underdoped YBCO Before we attempt to interpret T1 data for YBCO6.63 it is also important to discuss some neutron-scattering studies which are related to the low-frequency dynamical behavior. Several groups have reported spin correlations as well as AFM ﬂuctuation peaks in χ (q, ω) for this compound [19, 24, 25]. INS data for a YBCO6.6 sample with Tc = 53 K are shown in Fig. 4.8 [19]. At ω = 15 meV, q-scans through the AFM point [h(1 + δ), h(1 - δ), -1.8], for two values of δ and h = 0.5, record the ﬂat-topped AF peaks in χ (q, ω) at T = 10 K shown in Fig. 4.8(a) and (b) [19]. This appears to be a superposition

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

129

0.1

[ T1T ] –1

0.075

0.05

(n) = 0.5

0.025

U=4 U=8

0

0

0.05

0.1

0.15

χs Fig. 4.7. The variation of 1/T1 T vs. χs , with T as an implicit parameter, for the attractive-U Hubbard model calculations of [18]. Over the lower 40% of the variation of 1/T1 T , this quantity shows a very clear linearity with the spin susceptibility, with a constant of proportonality which is essentially independent of the value of U . Figure reprinted from M. Randeria, N. Trivedi, A. Moreo, R.T. Scalettar, Phys. Rev. Lett. 69, 2001 (1992). Copyright 1992 American Physical Society

of incommensurate peaks, but in any case it is a sign of strong in-plane AFM correlations. The authors suggest that this is strong enough to account for any observed enhancement of the Cu(2) relaxation. The temperature dependence of the integrated area under the AFM peak in χ (q, ω) (q ∼ QAF ) shows an energy-gap behavior with a gap value given as 9 meV 104 K [19]. This is the same gap energy as was derived from the static susceptibility data with an Arrhenius plot (Fig. 4.4, inset) for YBCO6.63. It seems that χs (T ) (i.e. q = 0) and χ (q, ω), q ∼ QAF (for YBCO6.60) exhibit the same gap energy. Such a result is implied by the dynamic susceptibility model (4.1.8) and is therefore supportive of such a model. Finally, a very substantial neutron intensity modulation has been observed in scanning q along the c axis. The scan of (0.5,0.5,l) for −3.5 ≤ l ≤ 3.5 is shown in Fig. 4.8(c), where a modulation amplitude approaching 50% is seen to occur at T = 100 K. Since the in-plane correlation length is only a few lattice spaces at most, the c-axis modulation reﬂects a larger exchange coupling between layers than one can easily account for. As was emphasized in [10], such an intensity modulation implies relatively strong interplanar spin correlations which cannot be ignored when we estimate the 89 Y relaxation rate. However, it is possible that the c-axis correlation eﬀect could diminish rapidly with increased doping level, and thus be smaller for YBCO6.63. Such a measurement needs to be compared with NMR data on the same sample material.

130

4 Pseudogap Eﬀects in Cuprate NMR Studies 150

(a)

δ=0

50 Intensity (counts / 16 min)

Intensity (counts / 7 min)

100

0 (b)

δ = 0.066 100 50 0 0.2

0.3

0.4

0.5

0.6

0.7

0.8

150

100

50 (c) 0 –4

–2

0

2

4

Fig. 4.8. (a) Neutron scattering intensity is shown for two scans in the vicinity of the AFM point along the diagonal (see text for details). These steep-sided peaks show signs of an incommensurability. They have been ﬁtted with a pair of Gaussians as shown. (b) A scan along (0.5,0.5,l) is recorded for an energy transfer of 9 meV at T = 100 K on a crystal of YBCO7-x, with x = 0.55 and Tc 45 K. The solid line is a resolution-corrected calculation of the inelastic structure factor from [19]. The variation of modulation amplitude with x is not known. Figure reprinted from J.M. Tranquada, et al., Phys. Rev. B46, 5561 (1992). Copyright 1992 American Physical Society

4.1.4 A Comprehensive T1 Data Set for YBCO6.63 We now consider the relaxation data for 63 Cu(2), 17 O(2,3), and 89 Y corresponding to the NMR shift and spin susceptibility results of Figs. 4.4 and 4.5. In Fig. 4.9 are displayed the high-quality T1 data for 63 Cu(2) and 17 O(2,3) in YBCO7 (“y = 0”) and YBCO6.63 (“y = 0.37”) from Takigawa et al. [9]. The Tc points indicated refer to YBCO6.63, where Tc 64 K. For the case of YBCO7 (open circles) the data for both 17 O(2,3) and 63 Cu(2) show very similar sharp declines at Tc 92 K. For YBCO6.63 (closed circles), however, the overall curves are very diﬀerent, and neither data plot shows any visible feature at Tc (indicated by arrows), where both curves are smooth and continuous. As shown in the inset to Fig. 4.1(a), however, the resistive superconducting transition remains as sharp as ever. As with χs (T ) (Fig. 4.4), then, the low-frequency spin dynamics show only a smooth decline in the vicinity of Tc . This behavior shows that the pseudogap merges smoothly into the superconducting gap which presumably forms below Tc . Considering the 63 Cu(2) T1 data in Fig. 4.9(b), a plot of these data similar to Fig. 4.6 yields essentially the same result4 . However, in spite of the 4

As an example we consider the value of [T1 (Korr.)/T1 ][Ks (T )/Ks (300)] at T = 100 K. Using (4.1.7) with Ns = 4, we take 1/T1 630 s−1 from Fig. 4.9(b),

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x 0.4

131

y = 0.37 6

y=0

TC

(63T1T)–1 (s–1K–1)

(17T1T)–1 (s–1K–1)

0.3

y = 0.37

0.2

0.1

0

2

(a)

TC 0

y=0 4

100

200 T (K)

(b) 300

0

0

100

200

300

T (K)

Fig. 4.9. (a) Data for 1/T1 T for 17 O(2,3) in both YBCO7 (“y = 0”, open circles) and YBCO6.63 (“y = 0.37”, closed circles) are plotted from 300 K down to well below Tc [9]. (b) With the same notation and symbols as in (a) the corresponding data for 63 Cu(2) are shown. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). Copyright 1991 American Physical Society

large numbers one sees in Fig. 4.6, the actual enhancement of 1/T1 T for Cu(2) is a relatively small number. From (3.3.14) one sees that 1/T1c ∝ χs (T )[1+0.29K01 +0.99(2K12 +K13 )]. The Kij ’s presumably have small values above 300 K, and as T → Tc could approach −1 for K01 and +1 for K12 and K13 . Thus, the AFM exchange enhancement factor [ ] varies from unity to a maximum [ ] 3.68. Examination of the data plot in Fig. 4.9(b) shows that it changes substantially between 100 K and 300 K, but stays well within those limits. Considering T1 data for 17 O(2,3) in Fig. 4.9(a), we see that it very closely resembles the susceptibility curve in Fig. 4.4. A plot of (T1 T Kc (T )) vs. T using data from the latter ﬁgures yields a curve varying by only a few percent between 100 K and 300 K [9]. The simple model form (4.1.8) for χ (q, ω) now 17 O(2,3) is leads us, however, into some diﬃculty. The correlation factor for simply [1 + K01 ], where the remainder of the expression ∝ q χ (q, ω)/ω, has been shown by neutron studies to vary with temperature in the same energygapped fashion as χs (T ). Thus, (T1 T Ks (T ))−1 constant for the 17 O(2,3) means [1 + K01 ] constant, which is not consistent with the “substantial” change in the correlations required by the 63 Cu(2) above. We shall now see that the 89 Y data lead to further diﬃculties with the model susceptibility (4.1.8). Ks (100 K) 0.11%, and [Ks (T )/Ks (300)] 0.5. Inserting these parameter values, one ﬁnds [T1 (Korr.)/T1 ][Ks (100)/Ks (300)] 39, which lies among the closed circle points in Fig. 4.6.

132

4 Pseudogap Eﬀects in Cuprate NMR Studies

The Problem of

89

Y T1 Behavior in YBCO6.63.

In Fig. 4.6 89 Y T1 data are plotted so as to test the pseudogap scaling with χs (T ). The result is a very ﬂat curve, based on data from [2]. However, there are two more recent sets of T1 measurements, by Takigawa et al. [10] and by Alloul et al. [5], neither of which agree with the previous conclusion. Data plots from [10] are shown in Fig. 4.10. In Fig. 4.10(a) are plotted 1/T1T for 89 Y in YBCO6.63 with both ﬁeld orientations as a companion to the NMR shift measurements in Fig. 4.5 on the same sample, as well as the 17 O(2,3) relaxation data from Fig. 4.9 for comparison. It is clear that 1/T1 T for the oxygen declines rather less at low temperatures than either 89 Y measurement. This point is illustrated further in Fig. 4.10(b), where 17 T1c /89 T1c is plotted for 100 K ≤ T ≤ 300 K. At 100 K this ratio is seen to have increased by more than 20% over its value at 300 K. Similar data are given in [5] for both Ks (T ) and 1/T1T for 89 Y in YBCO6.64. Although the latter data have somewhat larger error bars, they are consistent with the data shown in Fig. 4.10. Since these more recent data are much more complete than those shown in Fig. 4.6, we conclude that (T1 T Ks (T ))−1 for 89 Y is not constant in this composition, in contrast with the 17 O(2,3) data in Fig. 4.9. We discuss the data in Fig. 4.10 further by means of the general T1 formulas (3.5.22) and (3.5.21). Taking the ratio of these equations, we ﬁnd 89

T1ab 17 T 1c

=

2 [1 + K01 ] [Ca2 + Cb2 ] γ17 2 2 + D 2 ] [1 + 2K IC ] γ89 [Dab 01 + K12 + K c

(4.1.9)

where we have added an interplanar correlation coeﬃcient KIC to take account roughly of that possibility for the 89 Y. In the high temperature limit where 2 2 2 [Ca2 + Cb2 ]/γ89 [Dab + Dc2 ]. Kij 1, one would expect 89 T1ab /17 T1c → γ17 Inserting parameter values from Table 4.1, we ﬁnd a limiting ratio of 2360, as compared with the experimental ratio of 1305 at T = 300 K (Fig. 4.10) [10]. It seems, then, that the estimated rate 1/89 T1 is too small by as much as a factor ∼ 2 when analyzed on the same basis as the 17 O(2,3). On the other hand, this analysis has some positive points. First, the anisotropy of 89 T1 according to the model (3.5.22) is given by 89 T1c /89 T1ab = 2 2 [Dab + Dc2 ]/[2Dab ] 1.17 by the data in Table 4.1. With modest error bars on that value, the data in Fig. 4.10 are in reasonable agreement with the latter estimate for both YBCO7 and YBCO6.63 and at all temperatures shown. Furthermore, when correlations become important at low temperatures, one would certainly expect that [1 + 2K01 + K12 + KIC ] < [1 + K01 ].

(4.1.10)

One would therefore expect 89 T1α /17 T1α to increase at low T, as it does in Fig. 4.10(b). If we examine the eﬀects of dipolar terms, in the case of negligible correlations they add less than 10% to the estimated rates. The case of dipolar

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

89W (sec–1K–1)

x10–4 O7

2

89W ab 89W c 17W c

0.4

0.2

1 89

O6.63

(a) 0

100

0

200

Wab

–1 –1 c (sec K )

0.6

17W

3

133

89

Wc 17W c 300

0

T(K)

R = 17Wc / 89Wc

2000

1800

1600

O6.63 O7

1400 (b) 1200

0

100

200

300

T(K)

Fig. 4.10. (a) Data for 1/T1 T for 89 Y (89 Wab,c ) in both YBCO7 (O7 ) and YBCO6.63 (O6.63 ) and for both “ab” and “c” axis ﬁeld orientations are plotted from 100 K to above 300 K [10]. For comparison, 1/T1 T for 17 O(2,3) (17 Wc ), measured on the same samples, is also plotted. (b) With the same notation as in (a) the ratios R = 17 Wc /89 Wc are plotted for both compositions and the same temperature range. Figures reprinted from M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993). Copyright 1993 American Physical Society

terms in the presence of intraplanar and interplanar correlations has been discussed in detail by Takigawa et al. [10]. While they could become signiﬁcant in such a case, they have the opposite anistropy to the Dα ’s, which is a serious drawback. One cannot see how a calculation based entirely on the model Hamiltonian (3.3.2) can heal the disparity in the estimated T1 for 89 Y. Additional calculations with the full dipolar Hamiltonian have been performed by Auler et al. [15], where a substantial dipolar contribution to the 89 Y relaxation was estimated. These results are discussed in Sect. 5.3. Another possible answer for the 89 Y T1 problem is that there may be enough Y(3d)-hole character hybridized into the Cu2+ spin states to generate

134

4 Pseudogap Eﬀects in Cuprate NMR Studies

a signiﬁcant orbital T1 eﬀect. After all, the measured Dα coeﬃcients in Table 4.1 are undoubtedly the result of such an hybridization, which has its main eﬀect through the core-polarization term. The orbital HF eﬀects are typically of the same order, but are probably more nearly isotropic. Since there is no Fermi-surface orbital shift eﬀect related to the orbital T1 term, the latter would just appear as a “background” relaxation eﬀect unrelated to the spin HF eﬀects. There could also be a small Van Vleck orbital NMR shift as part of the positive, temperature-independent chemical shifts recorded for the 89 Y. We turn now to pseudogap phenomenology as seen with other probes.

4.2 Pseudogap Phenomenology with Other Probes In this section we address brieﬂy several topics relating to pseudogap eﬀects in the cuprates, but not directly related to NMR. Thus, we are discussing “background material”, the point of which is to give a deeper context in which to present and discuss the NMR results. It is essential to point out that pseudogap eﬀects have been observed and studied in great detail with several other techniques. In particular, it is interesting to note that the presence of the pseudogap is felt in both spin and charge-based properties. One example is the in-plane conductivity σab (T ) of underdoped YBCO at 250 cm−1 , which according to Rotter et al. [26] exhibits a gap-like feature at low temperatures very similar to 1/T1 T for 89 Y and 17 O(2,3) for that case (see Figs. 4.1(b) and 4.9(a)). A clearly presented review of pseudogap eﬀects has been given by Randeria [27]. 4.2.1 Pseudogap Eﬀects in the Electronic Speciﬁc Heat We oﬀer brief descriptions of experimental results which detect and elucidate the pseudogap eﬀect in cuprates, the ﬁrst of which is the electronic speciﬁc heat. By using a very precise diﬀerential technique, J.W. Loram and co-workers have produced an extraordinarily clear and detailed picture of the behavior of low-energy electronic states in the cuprates [28, 29, 30]. We review here a selection of their results on YBCO7-δ. A sampling of speciﬁc heat results is shown in Fig. 4.11(a) and (b). In (a) one sees that, ﬁrst, the peak in γ el (T) (≡ Cp (T )/T ) at Tc gradually vanishes as δ is increased from 0, and simultaneously a pseudogap maximum appears at temperatures T Tc , causing γ el to decline as it approaches Tc from above. The peak at Tc makes a rather weak reappearance at Tc ∼ 60 K, then declines further as superconductivity fades away at larger δ values. T In Fig. 4.11(c) the entropy S el = 0 γ el (T )dT is plotted as S el /T vs. T. Such a plot closely resembles γ el (T ). The superconducting gap feature is very pronounced for δ 1, persisting up to δ ∼ 0.20. Then entropy loss at T > Tc becomes a major feature, namely the pseudogap, as δ increases, while

4.2 Pseudogap Phenomenology with Other Probes

135

7

δ

6

0.08

0.03

(a)

5 0.13

4 3

0.20

γel (mJ / g-at K2)

2

0.24 0.27

1 0

(b)

0.20 2

0.24 0.43 0.52 0.57

0.27 1

0.62 0

0

50

100

150

0.71

0.84

200

250

T(K) 2

δ 0.03 0.08 0.13 0.20 0.24 0.27 0.33 0.43 0.52 0.57

Sel / T (mJ / g-at K2)

1.5

1

0.62 0.71 0.84

(c) 0.03 0.13 0.20 0.43 0.52 0.57

0.5

0.62 0.71 0.84

0

0

50

100

150 T(K)

200

250

300

Fig. 4.11. (a) and (b) Data for the electronic speciﬁc heat coeﬃcient γ el of YBCO7δ, obtained via diﬀerential measurements with YBCO6.0, are plotted for diﬀerent doping levels δ as a function of temperature up to 250 K [30]. In (b) there is clear

136

4 Pseudogap Eﬀects in Cuprate NMR Studies

the decline in S el /T begins at ever higher temperatures. Note, however, that a vestige of the superconducting gap feature beginning at T ∼ Tc remains in place until superconductivity disappears altogether. These eﬀects on γ el and S el (T) seem to be entirely consistent with what one would expect based on the spin susceptibility and low-energy spin excitations reﬂected in the 1/T1 T results given in Sect. 4.1. Loram et al. present a companion set of spin susceptibility curves [30] to conﬁrm this point. There is a clear conclusion here of non-separation of spin and charge behavior, contrary to some of the early models of high-Tc properties [31, 32]. 4.2.2 ARPES Studies of Pseudogapped Cuprates Angle-resolved photoemission studies (ARPES) on cuprates exhibiting pseudogap eﬀects have also given a great deal of insight into the microscopic physics of cuprate superconductors as well as the pseudogap phenomena per se. Since this method oﬀers good resolution of energies as well as of k values, one is able to study both gap energies and their anisotropy over the Fermi surface. Extensive investigations of the cuprate properties have been conducted. We shall brieﬂy review studies of pseudogap eﬀects in the Bi2212 family of superconductors by Harris, Shen et al. [33, 34, 35]. What ARPES reveals is not only that gaps appear anisotropically around the Fermi surface, but also that quasiparticle peaks in the normal state are greatly diminished. They appear mainly at temperatures below Tc . Gap energies are measured, then, as the distance between EF and the “leading edge midpoint” of the photoemission intensity. The pseudogap is found to behave in similar fashion to a d-wave superconducting gap, namely to be at its maximum along the cut from (π, 0) to (π, π) and to vanish along the diagonal cut (0, 0) to (π, π). With that in mind, we examine the temperature dependence of experimental gap data, which oﬀers some insight into the relation between the pseudogap behavior and that of the superconducting gap which sets in below Tc . Harris et al. reported a study of Bi2 Sr2 Ca1−x Dyx Cu2 O8+δ untwinned thinﬁlm crystals with variable doping controlled by the parameters x and δ [33]. Fig. 4.11. (Continued) evidence for a pseudogap creating broad maxima in γ el at progressively higher temperatures with increasing carrier dilution. (c) The quantity S el /T, where S el is the electronic entropy calculated from the data in (a) and (b), is plotted as a function of temperature up to 300 K. The superconducting gaps occurring at Tc as well as the pseudogap eﬀects in these data are discussed in the text. Figure reprinted from W.Y. Liang, J.W. Loram, Physica C 263, 277 (1996). Copyright 1996 Physica C

4.2 Pseudogap Phenomenology with Other Probes

137

Their gap energy data scans extend over 1/8 of the (2D) Fermi surface.5 Two separate doping levels yielded a sample with a “strong” pseudogap eﬀect (Tc = 42 K) and a second one with a much “weaker” pseudogap (Tc = 78 K), where “strong” and “weak” are to be deﬁned presently. In Fig. 4.12(a) and (b) experimental gap energies are shown along an arc of the Fermi surface which extends from the diagonal (0.4, 0.4)π) where the abscissa is zero to (1, 0.2)π, where it is nearly one. The abscissa is deﬁned as 0.5|cos kx a-cos ky a|, which would yield a linear variation of gap energy with a d-wave (dx2 −y2 ) superconducting gap. For the data in Fig. 4.12(a), the superconducting state data (closed circles) show a nearly linear variation of gap energy along this path. In a conventional superconductor there would be no gap energy above Tc ; thus, the curve would remain ﬂat. However, this Tc = 78 K sample has a “weak” pseudogap, such that substantial gap energies occur

30

25 leading edge midpoint (meV)

10%Dy-BSCCO Tc = 46 K

10%Dy-BSCCO Tc = 78 K

20

13K

13K

100K

75K

150K

150K

15

(a)

(b) 10

5 0 0

0.2 0.4 0.6 0.8

1 0

0.2 0.4 0.6 0.8

1

0.5Icoskxa – coskyal

Fig. 4.12. ARPES measurements of gap energies, taken as decribed in the text on untwinned thin ﬁlm crystals of Bi2 Sr2 Ca1−x Dyx Cu2 O8+δ . In (a), gap variation results are shown along the Fermi surface at three temperatures for a “strong” pseudogap composition, and in (b) gap energies are shown at three temperatures for a “weak” pseudogap system, as described and discussed in the text. Figure reprinted from J.M. Harris, Z.-X. Shen, et al, Phys. Rev. B54, R15665 (1996). Copyright 1996 American Physical Society

5

The region of k-space considered is triangular, extending from (0,0) to (π,0), then to (π, π) and back to (0,0). The Fermi surface is an arc extending from ∼(0.4,0.4)π on the diagonal around to the point ∼(1,0.2)π on the (0,π) - (π, π) axis.

138

4 Pseudogap Eﬀects in Cuprate NMR Studies

at 100 K and 150 K, but which behave only qualitatively like the superconducting gap. On the other hand, the Tc = 46 K sample exhibits a “strong” pseudogap, which means that the gap energy proﬁle shown is the same both above and below Tc , exhibiting a ﬂat region near the null (abscissa = 0) and rising to a maximum which is the same near the point (1,0.2)π both above and below Tc . At 150 K the gap energy shows a small decline. Thus, with a “strong” pseudogap, the gap energy proﬁle in k–space is very nearly the same above and below Tc . For either a weak or strong pseudogap, the gap energy behaves in k–space in a very similar fashion to a superconducting gap, giving the impression that these eﬀects are related. At what temperature, then, does the energy gap ﬁnally collapse in an underdoped sample? An experimental answer to this question was given in [33], where measured gap energies at the maximum point were plotted vs. temperature up to T = 250 K on a sample with Tc = 85 K. Over this range of T the pseudogap declines completely to zero, beginning somewhere below Tc . The anisotropic gap behavior found in this system and presumably occurring widely in the cuprates would have interesting consequences for the behavior of χ (q, ω) and therefore for T1 measurements of pseudogap systems. Although to our knowledge no such calculation has been reported, it seems very likely that the observed anisotropy of gap eﬀects over k space would result in some distribution of gapping eﬀects in q space as well. Speculating about the consequences of this, it seems likely that nuclei such as 89 Y and 17 O(2,3) in YBCO, which depend for relaxation on q values over the entire zone except near the (0,π) axes would therefore always be subject to pseudogap eﬀects. On the other hand, the pseudogap anisotropy may allow situations where the ﬂuctuations peak strongly at (π, π) and are driven by k vectors on or near the diagonals. Such behavior could tend to dominate the planar 63 Cu T1 process, which would not then be strongly aﬀected by the pseudogap behavior. Such a case is found for La2−x Srx CuO4 , as will be discussed in Sect. 4.4.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) Another pseudogap system which has been studied intensively is Y248, a superconductor which is unique among the cuprates in having a ﬁxed, stoichiometric carrier doping level, which pegs it as slightly underdoped. It appears to have a pseudogap not unlike that of YBCO6.63 presented in Sect. 4.1. The structure of Y248 is closely related to YBCO7, except that there are two oxygenated chain layers between the pairs of CuO2 planes instead of one. Cu(1) sites in the chain layers are staggered along the b (chain) axis, so that the b-axis oxygen sites O(4) for one chain are apical oxygens for Cu(1) sites in the neighboring chain. Thus, planar arrays separated by a double chain layer

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

139

˚ high [36]. This structure of are also staggered, making the unit cell ∼ 27A chains is unusually stable, as the chain oxygens remain bound in the crystal up to temperatures beyond 700 K. Thus, Y248 is a nearly ideal cuprate on which to conduct high-temperature studies. The equilibrium stoichiometric structure of Y248 also yields unusually narrow NMR lines, oﬀering the possibility of high-precision NMR studies. We shall see some examples of this in Sect. 4.3.2. It is very diﬃcult to measure the ratio of mobile holes which occupy the Cu(1) and Cu(2) regions of the Y248 structure. It is, however, useful to estimate the doping level with the simple valence method. Assigning the usual valences, there is a single mobile hole per formula unit of YBa2 Cu4 O8 , which gives 0.25 carrier holes per Cu ion. With YBCO6.63, by comparison, the situation is more complicated in that 63% of the chain sites are oxygenated Cu2+ and 37% are two-fold coordinated Cu+ ions. On that basis one calculates 0.24 mobile holes per Cu2+ ion, giving very nearly equal doping for these two systems. There are marked diﬀerences in Tc , however, which is ∼ 81 K for the “best” samples of Y248, but only 60-65 K for YBCO6.63. As we shall see, there are other important diﬀerences as well. 4.3.1 NMR Shift and Relaxation Behavior in Y248 It is both interesting and informative to compare the pseudogap character of Y248 with that of YBCO6.63 and other systems. Owing to the simple and seemingly immutable character of this compound, a large responsibility seems to have been placed upon it and a great deal expected of it. Here we examine the general behavior of the pseudogap eﬀect as reﬂected in NMR shift (i.e. susceptibility) and relaxation data. Our point of reference will be the simple behavior found for YBCO6.63 as reﬂected by the data in Figs. 4.4 and 4.9. As concerns the immutability issue, we shall consider the reproducibility of experimental measurements in data from several research groups. Let us ﬁrst look at the overall relaxation behavior in Fig. 4.13. The log scales give a broad overview of the Cu(1,2) sites both above and below Tc [37]. The Cu(1) relaxation rate crosses through Tc looking Korringa-like, much as it did in YBCO7. For the Cu(2) there is a near discontinuity of slope at Tc which is much more pronounced than in the YBCO6.63 data of Fig. 4.9. Below Tc there is a steep drop into a very brief T 3 region, which then ﬂattens into a presumably disorder-related (i.e. states in the gap) Korringa runout below ∼ 20 K. Above Tc there is a near-Korringa stretch which ﬂattens into a very gradual increase above ∼ 200 K. Similar data have been given by Zimmerman et al. [38]. Apart from the pseudogap onset point around ∼ 200 K, the normal state behavior is quite featureless. Nonetheless, it is useful to have data extending as high as 700 K. For another view of 63 Cu(2) data for Y248 see the presentation by Yasuoka [39]. In Fig. 4.14 similar data for 63 Cu(2) are plotted as 1/T1 T vs. T [40]. These data were also taken with NQR, but on a diﬀerent sample, and are

140

4 Pseudogap Eﬀects in Cuprate NMR Studies

Spin-lattice relaxation rate 1 / T1(sec–1)

10000 YBa2Cu4O8 Cu(1) site Cu(2) site

1000

Tc

100

10

1

.1

1

10 100 Temperature (K)

1000

Fig. 4.13. NQR results for 1/T1 vs. T are shown for the 63 Cu(1) and 63 Cu(2) sites in Y248 and for temperatures ranging from 4.2 K up to 700 K [37]. The log-log plot emphasizes major features in the data. See text for detailed discussion. Figure reprinted from T. Machi, I. Tomeno, et al, Physica C173, 32 (1991). Copyright 1991 Physica C

in good agreement with Fig. 4.13. In Fig. 4.14, data for the 17 O(2,3) are compared with those for 63 Cu(2) up to 250 K. The 17 O(2,3) data also show a very deﬁnite kink at Tc , below which they fall well below the corresponding curve for YBCO6.63. Recall that the latter 17 O(2,3) T1 data in Fig. 4.9(a) show no feature whatever at Tc . The pseudogap eﬀect in Y248 is therefore somewhat like the Tc = 78 K BSCCO sample in Fig. 4.12(b) for which the superconducting gap has its own distinct character, while YBCO6.63 is like the Tc = 46 K (a) sample in that same ﬁgure, where the SC gap is completely merged into the pseudogap. In contrast with T1 data, neither the Cu(2) NMR shift [37] nor that of the 17 O(2,3) shown any abrupt change at Tc . The latter shift data 17 Ki,c (T ), i = 2 and 3, are shown in Fig. 4.15 where, unlike the case of YBCO6.63, they are resolved and separately measurable. The latter data presumably oﬀer a reasonable measure of the pseudogap, but unfortunately these data have a very large, negative intercept at T = 0, and no value of the zero shift has been given for either site. We shall make some guesses about the T = 0 shifts and diamagnetic corrections in our analysis below. Another peculiar feature of the latter 17 O(2,3) NMR shift data is the fact that these two sites have distinct and well-resolved T = 0 shift values, but as

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) Cu(2)

0.25

141

7

0.20

5

0.15

4 O(2,3) 3

0.10

2 0.05

1

Tc = 81K 0.00

0

50

100

(83T1T)–1 (sec–1 K–1)

(17T1T)–1 (sec–1 K–1)

6

150

200

250

0 300

Temperature (K)

Fig. 4.14. Relaxation data for both 63 Cu(2) and 17 O(2,3) in Y248 are plotted as 1/T1 T vs. T , showing detailed behavior near Tc . Like the 63 Cu(2) plot in Fig. 4.13, the planar 17 O show a visible break in slope at Tc . Figure reprinted from I. Tomeno, T. Machi, et al., Phys. Rev. B49, 15327 (1994). Copyright 1994 American Physical Society

the temperature rises above Tc the two lines gradually merge together. This could be entirely coincidental, resulting from slightly diﬀerent HF coeﬃcients. Alternatively, there could be chemical migration of O2− ions in the CuO2 −1 planes at a rate τcm which increases with temperature and eventually becomes fast enough (4.3.1) γ17 HΔK2,3 τcm 1 , so that the two NMR lines merge into one. The latter possibility seems a bit remarkable, but would avoid an even more remarkable coincidence with the HF coeﬃcients. It would be easy to test the chemical migration hypothesis with selective saturation techniques. As far as we know this has not been done. We now inquire as to whether the Y248 NMR shift data can provide a simple measure of the pseudogap energy, as they did for YBCO6.63 (see the inset to Fig. 4.4). Accordingly, several NMR shift data sets are plotted as ln(K(T)) vs. 1000/T in Fig. 4.16 for temperatures down to Tc . The linear slope of such a plot gives one measure of the pseudogap energy. The data shown here have been scaled up and down for display purposes. At the top we see data set (i), 17 Kc,ab (T ) and 65 Kab (T ) (triangles, diamonds and circles) from Bankay et al. [41]. The straight line drawn through these points deﬁnes a gap energy TG 84 K, which is ∼ 20% smaller than that of YBCO6.63. The open and ﬁlled squares are both plots of the data for 17 O(3) from Fig. 4.15, with two diﬀerent assumptions regarding 17 K3,c (0). In (ii) 17 K3,c (0) is assumed to be -0.04%, with a diamagnetic correction of -0.005%, while in (iii) it is assumed to be -0.02% with a diamagnetic correction of -0.025%. Both assumptions

142

4 Pseudogap Eﬀects in Cuprate NMR Studies 0.15 YBa2Cu4O8

17K

i,c (%)

0.10

0.05

17K

0.00 Tc = 81K –0.05

0

50

100 150 200 Temperature (K)

2,c

17K

3,c

250

300

Fig. 4.15. 17 O(2,3) NMR shift data for Y248 are plotted vs. T for temperatures up to 300 K [37]. Note that the O(2) and O(3) NMR lines are resolved below T ∼ 150 K, but merge above that point. See text for discussion and possible interpretation. Figure reprinted from T. Machi, I. Tomeno, et al, Physica C173, 32 (1991). Copyright 1991 Physica C

lead to a reasonable straight line, with TG 96 K and 106 K for (ii) and (iii), respectively. Option (ii) probably makes better physical sense and gives a gap energy closer to that of data set (i). Our main conclusion from plots (i)-(iii) is that Y248 NMR shifts show Arrhenius-type behavior with pseudogap energies 10-20% smaller than YBCO6.63. Data plot (iv) in Fig. 4.16 shows the 89 Y NMR shift data by Williams et al. [42], which the authors presented in a proposed test of the pseudogap isotope eﬀect. The undiﬀerentiated data points shown are for both 16 O and 18 O-doped samples, which gave indistinguishable behavior over the range of temperatures (131 K - 370 K) shown. The data are very precisely measured as one can see from the small scatter of the points, but the most striking thing is, ﬁrst, how diﬀerently these 89 Y data points behave compared with the other two data sets, and secondly, that they do not appear to correspond to a welldeﬁned gap energy in this kind of plot. Noting that in a stoichiometric sample of Y248 with low disorder one would expect NMR shifts of the 89 Y, 17 O(2,3), and 63,65 Cu(2) to follow a common temperature dependence as they did in YBCO6.63 (Fig. 4.4), the results shown suggest that the sample material used for data set (iv) is somewhat diﬀerent from that used for data sets (i)-(iii). In the following subsection we review eﬀorts which have been reported to measure the pseudogap isotope eﬀect in Y248.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

143

1

YBa2Cu4O8 (Scaled)

(i)

(ii)

17K, 63K, 89K

(iii) (iv)

0.1 0

2

4 1000/T

6 (10–3

8

10

12

K–1)

Fig. 4.16. An Arrhenius plot of several sets of NMR shift data for Y248 is presented to make estimates of the pseudogap energy for the density of states. The data are scaled to arbitrary positions along the vertical axis for display purposes. The data shown are, set (i): 17 Kab (T ) (triangles), 17 Kc (T ) (diamonds), 65 Kab (T ) (circles) from [41]; set (ii) and (iii) (same data, see text) 17 Kc (T ) (open and closed squares) from [40]; and set (iv) 89 Kc (T ) (dots) from [42]. The lines drawn are approximate ﬁts to the data for the purpose of extracting pseudogap energies from the slopes

4.3.2 Measuring the Pseudogap Isotope Eﬀect in Y248 with NMR The 89 Y data set (iv) in Fig. 4.16 were reported as part of an eﬀort to evaluate the isotope eﬀect, if any, on the pseudogap and on Tc in Y248 [42]. The samples employed for that purpose were annealed with 16 O and and with 18 O, respectively, and were found to have Tc (16 O) - Tc (18 O) 0.65 K, in reasonable agreement with previous work [43]. The shift data, as noted in the previous subsection, show no isotope eﬀect to the unaided eye for T > 130 K, while undergoing a pseudogap-related decrease of ∼ 40% from their peak values at 370 K. It is interesting at this point to inquire as to how large a change in the NMR shift curve is expected if the isotope eﬀect on the pseudogap temperature Tg is the same as that on Tc . First, let us deﬁne αc,g = dln(Tg,c )/dln(M ), where M is the oxygen atomic weight. Note that if αc = αg , then ΔTg /Tg = ΔTc /Tc . We shall now use this in a very simple way to estimate the change which might be expected in the 89 Y NMR shift curve. If we consider the gap function K(T) = K0 exp(−Tg /T ) (or any function purely of Tg /T ), then the temperature interval ΔT between equal values of shift for the two curves is |ΔT /T | = |ΔTg /Tg |. The ﬁts to shift data in Fig. 4.16 gave Tg ∼ 90 K; at T = 130 K, then, we expect curves

144

4 Pseudogap Eﬀects in Cuprate NMR Studies

shifted by ΔT ∼ 1.1 K.6 At the lower end of the data curve the slope is ∼ 1 ppm/K, leading one to expect deviations with the foregoing temperature shift of ∼ 1 ppm. As the inset shows, there are deviations of that order, but the ﬂuctuations are large. To resolve such an eﬀect would require a very precise ﬁtting curve and a large number of data points. In the light of the analysis given below for a diﬀerent experimental eﬀort to achieve the same end, we suggest that the 89 Y NMR shift data given were excellent, but the foregoing analysis in the present case does not quite rule out the possibility of a pseudogap isotope eﬀect. A second eﬀort to measure the pseudogap isotope eﬀect was made via NQR studies of the 63 Cu(2) relaxation curve for Y124, with the basic data plot of 1/T1T vs. T shown in Fig. 4.18(b) [44]. The data shown are for two samples, one with 16 O and one with ∼ 90%18 O, as in the previous case. The peaks in the two curves are seen to occur at T ∼ 150 K, where there is a razorthin margin between the curves ﬁtted to the two sets of data. The measured diﬀerence in Tc values ∼ 0.47 K for the 16 O and 18 O samples is slightly smaller than in the previous case. The key to analyzing the isotope eﬀect here is to ﬁnd a precise functional ﬁt to the data curves. For this purpose the authors have used Δ C 1 2 = 1 − tanh , (4.3.2) 63 T T Ta 2kB T 1 where the factor T −a , a ∼ 1, ﬁts the Curie-like decline of 1/T1 T at high temperatures, and Δ = kB T ∗ acts as the spin pseudogap energy - see discussion below. The data are a good ﬁt to (4.3.2), but the deviations were not quite random. The authors have therefore tinkered with the temperature scale a bit [44] and thus achieved the high-quality ﬁt to the data shown in Fig. 4.18. This ﬁt gives a shift in T ∗ for the two samples tested of 0.96 K. It is interesting that this temperature shift is less than was predicted for the 89 Y NMR shift curves in Fig. 4.17, but was resolved using a precisely ﬁtting function and a large number of data points. The pseudogap energy value turned out to be T ∗ = 246.9 K for the 1/T1 T curves [44]. This is more than twice the values found with the Arrhenius plots in Fig. 4.16. Further, although (4.3.2) is just a ﬁtting function, T ∗ really serves as an energy gap, since the asymptotic form of (4.3.2) is 1/T1 T ∝ T −a exp(−T ∗ /T ) for T ∗ /T 1. Note, however, that the NMR shifts represent the residual density of states, whereas T ∗ may represent the DOS squared. The appropriate comparison would then be between T ∗ /2 and Tg ∼ 90 K from the NMR shift results. This point of view does not appear, however, to be supported by pseudogap theory [45] (see the following subsection). It seems, then, at least for the dynamics that there is a pseudogap isotope eﬀect which is similar to that of Tc . As far as we are aware, there is no 6

This estimate is somewhat smaller than that of the authors [42], which is not stated explicitly.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

145

( Y(18O)–89Y(16O)) (ppm)

40 20 0 –20

– 89

–89Y

NMR Shift (ppm)

60

–40 150

1.0 0.5 0.0 –0.5

200 300 Temperature (K)

200 250 300 Temperature (K)

350

Fig. 4.17. 89 Y NMR shift data measured on two samples of Y124, one with nearly 100% 16 O (+ symbols) and the other with 94% 18 O (circles) [42]. The diﬀerence between these data plots is clearly smaller than the plotting symbols. Inset: Plot of the diﬀerences along with calculated diﬀerence curves. See text for discussion. Figure reprinted from G.V.M. Williams, et al., Phys. Rev. Lett. 80, 377 (1998). Copyright 1998 American Physical Society

(T1T)–1 (s–1T–1)

20

18 21

16 20

14

12

19 100

100

140

180

300

200 T(K)

Fig. 4.18. T1 data are plotted as 1/T1 T vs. T for two samples of Y124, one with 16 O and the other with ∼ 88% 18 O [44]. Using the functional ﬁt shown (see text) the diﬀerence in these two relaxation curves near their peak at T ∼ 150 K is analyzed to ﬁnd a diﬀerence in the pseudogaps roughly equal to that found for Tc . See text for detailed discussion. Inset: Detailed view of the peak vicinity. Figure reprinted from F. Raﬀa, T. Ohno, et al., Phys. Rev. Lett. 81, 5192 (1998). Copyright 1998 American Physical Society

146

4 Pseudogap Eﬀects in Cuprate NMR Studies

theoretical prediction available for the variation of the pseudogap with the atomic weight of the oxygen. 4.3.3 Theory of the Pseudogap by Varma. The only successful theory of the pseudogap which we are aware of is that by Varma [45]. Varma has constructed a theory of cuprate superconductivity and ancillary properties, based on the existence of a quantum critical point (QCP) at the center of the superconducting dome of the phase diagram shown in Fig. 4.19, where the abscissa is the doping level or carrier concentration in the CuO2 planes. Region I is the marginal Fermi liquid regime proposed and expounded in [46]. The pseudogap eﬀects occur in Region II below the line Tp (x) [45]. In Region II there is a broken symmetry based on time-reversal violating (TRV) states in which ﬂuctuating currents ﬂow in the CuO2 plane. The existence of such currents has been veriﬁed experimentally via neutronscattering experiments [47]. The aforesaid theory also predicts anisotropic gapping in k-space near the chemical potential in Region II of the phase diagram, as was depicted by the gapping curves in Sect. 4.2.2. Corresponding calculations of the density of states in the pseudogap regime have been presented for comparison with experimental data on Y248. In Fig. 4.20 the 89 Y NMR shift data from [42] (see

T Pseudogapped metal

Tp

II

Crossover

Marginal Fermi liquid

I

III Fermi liquid

AFM

x (doping) QCP Superconductivity

Fig. 4.19. Phase diagram of doped cuprates showing the putative quantum critical point at the center of the superconducting dome [45]. From normal metal behavior at high doping levels (III), there is a crossover to the marginal Fermi liquid behavior in (I) followed by pseudogap behavior below the line Tp (x) emanating from the QCP. The calculations presented in [45] are for Region II. Figure reprinted from C.M. Varma, Phys. Rev. B73, 155113 (2006). Copyright 2006 American Physical Society

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

147

T/TG 60

0.4

0.6

0.8

1.0

89Y

NMR Shift (ppm)

40 20 0

89Y in YBa2Cu4O8

–20 –40 100

200

300

400

T(k)

Fig. 4.20. The 89 Y NMR shift data from Y248 (see Fig. 4.17) is shown here ﬁtted by the pseudogap theory given by Varma [45] (solid line), yielding an excellent ﬁt

Fig. 4.17) are compared with a calculated pseudogapped density of states from [45], where an excellent correspondence is seen to occur. It would, of course, be most interesting if more detailed calculations of, e.g. χ (q, ω) would be forthcoming, for comparison with the q-dependent relaxation eﬀects in these systems. 4.3.4 Eﬀect of Zn impurities on the Pseudogap in Y248 From early on it has been known that Zn impurities – thought to substitute for the Cu(2) – cause a dramatic reduction of Tc in high-Tc cuprates [48]. Even though Zn2+ is a nonmagnetic ion core, its presence in the CuO2 plane (as well as Li+ ) is thought to cause potential scattering which destroys d-wave pairs, and it also causes the occurrence of a small localized magnetic moment in the same vicinity [49]. The latter is a very interesting eﬀect in its own right, even exhibiting a Kondo eﬀect [50, 51]. The strategy of Zn-doping to eliminate the eﬀect of the SC transition on the pseudogap was adopted by Zheng et al. [52]. However, instead of the collapse of AFM spin ﬂuctuations as found with YBCO7-x, the Zn-doped Y248 undergoes an enhancement of 1/T1 for 63,65 Cu similar to the ”CurieWeiss” behavior of T1 T in LSCO:x [53], as shown in Fig. 4.21. With 2% Zn substitution, the peak value of 1/T1 T is almost three times the peak value of that quantity in the undoped case. Meanwhile, the NMR shift proﬁle remains spin-gapped with eﬀectively no change [52], in spite of a reduction of Tc by a factor ∼ 3. The latter result suggests that the SC transition was already having very little eﬀect on the shift proﬁle in the undoped case.

148

4 Pseudogap Eﬀects in Cuprate NMR Studies

1/ T1T (sec–1K–1)

20 YBa2(Cu1–xZnx)4O8 : X=0 : X = 0.01 : X = 0.02 10

0

200 100 Temperature (K)

300

Fig. 4.21. A plot of data for 1/T1 T for 63 Cu(2) in Y248 made with samples which are undoped (open circles) and doped with 1% Zn (closed circles) and 2% Zn (closed diamonds), showing suppression of Tc from 74 K to 53 K and ∼ 27 K, respectively, combined with large progressive increases in the value of 1/T1 T at T = Tc [52]. The corresponding change in the NMR shift curve is slight and barely resolvable. Figure reprinted from G.–Q. Zheng, T. Odaguchi, T. Mito, Y. Kitaoka et al: J. Phys. Soc. Japan 62, 2591 (1993). Copyright 1993 Physical Society of Japan

The Zn impurities, while suppressing Tc , have the very speciﬁc eﬀect of un-gapping the Fermi surface regions which contribute to χ (q, ω) near q = (π, π), or so it would appear. In connection with these remarkable data, the results of two additional relaxation measurements would be of great interest. First, a comparative plot of T2g for the 63 Cu(2) over the same temperature range would give a direct measure of the doping eﬀect on χ (Q) (see Sect. 6.1). Second, the T1 behavior of either 89 Y or of 17 O(2,3) would test the eﬀect of Zn doping on low–frequency ﬂuctuations away from Q as a corroboration of the unchanged NMR shift results. In other words, these measurements would further test the scenario where the Zn doping eﬀect appears to be conﬁned to the region of the AFM peak.

4.4 “Pseudogap-like” Eﬀects in La2−xSrxCuO4 (LSCO:x) Apart from introducing the LSCO structure in Sect. 3.1, there has been up to this point no discussion of LSCO. In spite of its rather low Tc relative to other cuprates, LSCO played a major role in high-Tc physics research. This was because, (i) it was one of the ﬁrst cuprate structures identiﬁed [54], (ii) it has a very interesting and accessible phase diagram similar to Fig. 1.1, and (iii) it is relatively easy to make large, homogeneous single crystals of LSCO:x. For the latter reason a great many neutron scattering measurements have been conducted on this system, making its dynamic susceptibility perhaps the best

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

149

characterized of all of the cuprates. This will be discussed extensively, along with NMR measurements, in Chap. 6. From the standpoint of NMR technique, LSCO is a far simpler system to work with than YBCO. First, there are only one Cu2+ site and two O2− sites, making spectra and relaxation studies generally easier to interpret. For the purposes of conducting 17 O NMR studies in crystals, LSCO is also a favorable case, because it has very high oxygen mobility at relatively modest temperatures. Thus, it is easy to exchange 17 O into a crystal and homogenize it with simple annealing procedures. The foregoing circumstances notwithstanding, we shall see that the pseudogap eﬀect in LSCO is not quite the same as in the other cuprates. One rarely even ﬁnds the word pseudogap applied to LSCO, so we refer here instead to “pseudogap-like” eﬀects. While the NMR shift and susceptibility behavior is pseudogap-like (with important diﬀerences), the relaxation behavior of the 63 Cu is quite diﬀerent from that of YBCO6.63. On the other hand, the planar 17 O shift and relaxation appear to follow the spin susceptibility rather like the 17 O(2,3) data for YBCO6.63 in Fig. 4.9(a), making the overall picture pseudogap-like except for the 63 Cu T1 results. We now present a detailed account of these points. 4.4.1 Spin Susceptibility Scaling for La2−x Srx CuO4 . Around the time that the ﬁrst studies of underdoped YBCO7-x appeared, it was revealed by D.C. Johnston that the susceptibility of LSCO:x obeys a simple scaling law over essentially the entire range of superconducting compositions [7], χ(x, T ) = χ0 (x) + χs,max (x) Fs (T /Tmax (x)) + C(x)/T ,

(4.4.1)

where χ0 (x) is a temperature-independent background susceptibility, χs,max is the maximum spin susceptibility for composition x, which occurs at Tmax (x), and Fs (T /Tmax(x)) is a scaling function valid for 0.05 ≤ x ≤ 0.30 [7]. C(x) is a spurious Curie term which occurs at higher doping levels [55]. By deﬁnition, Fs (1) = 1. The term χ0 (x) represents Van Vleck orbital and diamagnetic contributions (see Sect. 2.3.2). The function Fs (T /Tmax (x)) is such that χ(x, T ) is qualitatively similar to the YBCO6.63 result in Fig. 4.4. To illustrate the behavior of χ(x, T ) for LSCO:x we display the somewhat more complete data set reported later by Nakano et al. [55] in Fig. 4.22 for 0.08 ≤ x ≤ 0.26, all superconducting samples. While the latter data extend up to ∼ 550 K, data from another study extending up to ∼ 1000 K show that χ(x, T ) for x ≤ 0.09 had no (accessible) maximum value, but all data plots for x > 0.09 exhibited a maximum at some temperature [56]. This CurieWeiss-like rise in susceptibilities at low temperatures for the higher doping levels is one factor which sets LSCO:x apart from the pseudogap behavior of other cuprates.

150

4 Pseudogap Eﬀects in Cuprate NMR Studies X = .26 La2–xSrxCuO4 χ (10–7 emu/g)

4

.22 .20 .18

2

.14 .10 .08

0

200

400

600

T(K)

Fig. 4.22. Susceptibility data for La2−x Srx CuO4 are plotted as a function of temperature for a series of random powder samples with 0.08 ≤ x ≤ 0.26 [55]. These data are found to scale as described in the text and in Fig. 4.23. Figure reprinted from T. Nakano et al., Phys. Rev. B49, 16000 (1994). Copyright 1994 American Physical Society

Nonetheless, there is a clear gap feature in χ(x, T ), which may be seen in Fig. 4.23, where χs (T )/χs,max = (χ(x, T ) − χ0 )/χs,max vs. T /Tmax is plotted [55]. The data for the eleven compounds shown follow this scaling curve to a remarkable degree. It seems highly plausible that this behavior is related to the pseudogap eﬀect identiﬁed in both YBCO6.63 and Y1248. This scaling of data may not reﬂect a simple energy gap parameter as in Fig. 4.4. The limiting, lowT behavior χs (T ) ∝ T β , β ∼ 0.5, is actually one of the predictions of Varma’s theory of the pseudogap [45], which was ﬁtted to the data in Fig. 4.20. It is interesting to examine the behavior of the other parameters in the ﬁt to (4.4.1). The values obtained for Tmax (x), χ0 (x), and C(x) are displayed as a function of x in Fig. 4.24(a). It is seen that there is a peculiar sort of transition point between data ﬁts for 0.10 ≤ x < 0.20 (Region I) and 0.20 ≤ x ≤ 0.28 (Region II). In Region I, Tmax declines in a roughly linear fashion7 from Tmax ∼ 700 K for x = 0.10 down to Tmax ∼ 100 K at x = 0.20. In region II, Tmax ∼ 100 K. In Region I, χ0 rises from a slightly negative value at x = 0.10 to χ0 ∼ 1.8×10−7 emu/g at x = 0.20 and remains constant above that point. Finally, C(x) = 0 in Region I, rising rapidly in Region II to where it becomes a major feature of the susceptibility data. Although there is no result given which identiﬁes χ0 (x) as the residual susceptibility at T Tc , we regard χs (T ) as the spin susceptibility. The magnetic behavior then distinguishes Regions I and II very clearly as “underdoped” and “overdoped”, respectively. In a more speculative vein, one could term these subcritical and supercritical relative to a putative quantum critical point at x 0.20. 7

There were no ﬁts to data below x = 0.10.

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

151

2 1

χs(T)/χs max

s s χ (T)/χ max

La2–xSrxCuO4

0

1

1

T/Tmax

X = 0.10 0.11 0.16 0.18 0.115 0.22 0.125 0.24 0.14 0.26 0.15 Universal Curve F

0

2 T/Tmax

5

4

Fig. 4.23. The data from Fig. 4.22 are plotted as χs (T )/χs,max vs. T /Tmax as deﬁned in (4.4.1). The resulting scaling curve deﬁnes the function Fs (T /Tmax (x)) from the latter equation as well, identiﬁed as “Universal Curve F” [55]. The inset shows that compared with previous scaling curves (e.g. [7]) represented by the dashed line, the present data decline more sharply as T → 0. As noted in the text, the theory by Varma [45] predicts χs (T ) ∝ T 1/2 near T = 0, very near to what is observed 800

(a) 400

1

χo (10–7emu/g)

Tmax(K)

2

0

C(10–7emu K/g)

0 60 La2–xSrxCuO4 40

(b)

20

0

0.1

0.2

0.3

X

Fig. 4.24. (a) The ﬁtting parameters Tmax (x) and χ0 (x), and (b) C(x) from (4.4.1) are plotted as a function of x for the series of ﬁts shown in Fig. 4.23 [55]. The behavior of these parameters clearly divides this doping range into regions I and II, where x 0.20 is the boundary line. See text for more discussion

152

4 Pseudogap Eﬀects in Cuprate NMR Studies

4.4.2 Behavior of the

17

O and

63

Cu NMR Shifts in LSCO:x.

Scaled 17 O NMR shift values are plotted as a function of temperature in Fig. 4.25 for x = 0.15 and 0.24 [55]. The shift data used for these plots are from Ishida et al. for x = 0.15 [57] and from Zheng et al. for x = 0.24 [58]. The lines drawn represent susceptibility data from [55], but the shift scales have been omitted from the ﬁgure. We note that the original data reﬂects c-axis shift coeﬃcients 50 − 60 kOe/μB , which is somewhat larger than the values of Cα for YBCO6.63 in Table 4.1. In both cases, the scaled 17 O shift values are a good quantitative match to the susceptibility data. Data for the 63 Cu c-axis NMR shifts in LSCO:x (not shown) have been found to have the following features [59]. With ﬁeld along the c axis, compositions in the superconducting range show a very nearly constant shift Kc 1.22% independent of temperature. For ﬁelds in the ab plane, shift data appear to follow the same trends as the susceptibility data in Fig. 4.22. Although to our knowledge they have not been scaled with susceptibility data as in Fig. 4.25, a simple estimate of ΔKab /Δχ gives a value Aab 149 kOe/μB , within 2-3% or so of the values given (Table4.1) for the composite 63 Cu(2) shift coeﬃcients in YBCO. For the Cu2+ at least, the Mila-Rice HF Hamiltonian from Sect. 3.3.3 appears to have near universal validity in the cuprates. The static spin-paramagnetic eﬀects for LSCO:x therefore behave in an internally consistent fashion, exhibiting a gap-like decline at low temperatures which becomes more pronounced at lower doping levels. The gapping feature is, however, superimposed on a Curie-Weiss-like increase at low temperatures which is often found in itinerant antiferromagnets. There is also a weak maximum in the susceptibility of the Cu(2) sites in YBCO7. Since the overdoped region is inaccessible for YBCO, one cannot say whether or not Curie-Weiss

La2–xSrxCuO4

χ (10–7 emu/g)

2

Tc 1

Tc x = 0.15 (K. Ishida et al.) x = 0.24 (G. –Q. Zheng et al.)

0

200 T(K)

400

Fig. 4.25. The 17 O NMR shifts measured for La2−x Srx CuO4 with x = 0.15 [57] and 0.24 [58] are ﬁtted to susceptibility curves such as those shown in Fig. 4.22 and plotted vs. temperature [55]. The scale of shift values is such that Cc = 50-60 kOe/μB

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

153

behavior is found there. Be that as it may, we shall now see that the Cu-site T1 behavior is distinctly diﬀerent for these two systems. 4.4.3

63

Cu NQR spectra and Contrasting T1 Behaviors in LSCO:x.

Whereas oxygen-deﬁcient YBCO7-x shows line-broadening caused by crystalline disorder, LSCO:x has nearly resolved 63 Cu NQR and NMR “impurity” lines attributable to sites neighboring the Sr2+ dopant ions. NQR spectra are shown in Fig. 4.26 for three Sr2+ doping levels [60]. The spectra have been analyzed into pairs of 63,65 Cu NQR lines representing sites neighboring the impurities and “bulk” Cu2+ sites away from the Sr2+ sites. Since the charge environment near a dopant site is quite diﬀerent from that of a bulk site, it is not surprising to ﬁnd a diﬀerent EFG at such sites. For a sample with x = 0.30 there is a very high probability that a Cu2+ site will have a Sr2+ neighbor, and the corresponding impurity line is now larger than the bulk line (see Fig. 4.26). Perhaps it is because of this high level of impurity-induced disorder in LSCO:x that Tc peaks at ∼1/2 the peak value for YBCO7-x. T1 Results for

63

Cu.

As noted earlier, the peak Tc value in LSCO:x also occurs in samples (x 0.15) with quite a pronounced pseudogap feature in the susceptibility. However, the T1 curve for 63 Cu in such a sample is shown in Fig. 4.27 is not unlike what is found for YBCO7, although the relaxation rate is nearly three times as great. There is a ﬂatter-than-linear characteristic in the normal state and a pronounced T 3 region in the superconducting state just below a region which is somewhat steeper than that. These measurements have been taken both on the bulk and impurity-neighbor NQR lines, with very similar results for both sites [60]. There is little indication of the spin-gapped nature of the susceptibility data in the behavior of T1 for this composition. Apart from the fact that the LSCO relaxation is ∼ 3 times faster, the results in Fig. 4.27 bear a strong resemblence to the YBCO7 results in Fig. 3.11. T1 and NMR Shift Results for

17

O.

The dynamic susceptibility χ (q, ω) for underdoped LSCO:x near q ∼ QAF = (π/a, π/a) is therefore not aﬀected by the static, uniform pseudogap eﬀect noted earlier. For the behavior of low-frequency excitations over the rest of the zone we look at T1 behavior of the planar 17 O nuclear spins. A plot of 1/T1 T for the planar 17 O in LSCO:0.15 is shown in Fig. 4.28, along with NMR shift data on the same system [61]. The 17 O data stand in sharp contrast with the 63 Cu results, where they are seen to follow the shift data, 1/T1 T ∝ Ks (T ). This is similar behavior to the 17 O(2,3) data for YBCO6.63 in Fig. 4.9(a), and therefore a “classic” pseudogap result. The 17 O data suggest that gapped excitations similar to those at q ∼ 0 occupy the bulk of the Brillouin zone, and only those near QAF are immune to the gapping eﬀect. The latter excitations

154

4 Pseudogap Eﬀects in Cuprate NMR Studies A

La2–xSrxCuO4

SPIN-ECHO INTENSITY (arbitrary units)

B x = 0.15

x = 0.20

x = 0.30

30

35 40 FREQUENCY (MHZ)

45

Fig. 4.26. NQR spectra for 63,65 Cu in LSCO:x are shown for three typical values of x. the spectra have been analyzed into a pair of “A” lines , which represent bulk material away from the doping centers, and a pair of “B” lines representing sites which have at least one Sr2+ neighbor. For each case there are two lines representing the two isotopes with their roughly 7:3 (63:65) abundance ratio. For x = 0.30 the B lines have well over half of the intensity. The dashed lines shown are Gaussian components in the spectrum which sum up to the solid lines drawn, giving a reasonable facsimile of the experimental spectra. Figure reprinted from K. Yoshimura, T. Imai, et al., J. Phys. Soc. Japan 58, 3057 (1989). Copyright 1989 Physical Society of Japan

must be very strong, however, as they dominate the ultra-fast relaxation of the 63 Cu. The LSCO:x system therefore exhibits a mixture of pseudogap and nonpseudogap-like features. However, it seems quite clear that the pseudogap eﬀect is present and well-deﬁned for LSCO:x, for both static, q = 0 behavior, as well as for low-frequency quasiparticle excitations over the bulk of the Brillouin zone. However, the Fermi surface, which is known to be diﬀerent from that of YBCO7, could very well be situated so that the dynamic susceptibility near (π, π) samples only the non-gapped regions (see discussion of this point in Sect. 4.2). Moreover, the AFM peak for LSCO:x=0.15 must be so large that it completely dominates the 63,65 Cu relaxation rate. The planar oxygen then evidently have a dramatically diﬀerent relaxation character.

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

155

104 Tc = 38 k

1/T1 (sec–1)

103

102

10

~T3

La1.85Sr0.15CuO4 1

1

102

10

103

T (K)

Fig. 4.27. Data are plotted for 1/T1 as a function of temperature for both the A (open circles) and B (closed circles) sites identiﬁed in Fig. 4.26 in a sample with x = 0.15. The two data sets, where comparable, are quite similar in character. The A-site measurements show a typical ﬂat region in the normal state, with a steep drop below Tc , then a T 3 region [60]. Very little evidence is seen of the pseudogap feature found in the susceptibility for this composition

0.20 2.5 0.15

2.0 1.5 La1.85Sr0.15CuO4

1.0

0.05

0.5 0.0

0.10

Ks17p(%)

(17T1pT)–1 (10–1sec–1K–1)

3.0

(17T1pT)–1

Ks

17p

0.00 0

50

100

150

200

250 300

Temperature(K)

Fig. 4.28. 1/T1 T data for the planar 17 O in the LSCO 0.15 system are plotted (solid circles, left axis) in comparison with scaled data on the same sample for Ks (T ) (open triangles, right axis), showing that these two quantities are proportional over the range 100 K ≤ T ≤ 200 K [61]. Note the sharp contrast in behavior between the 63 Cu relaxation, represented by the dotted line, and the planar 17 O in this system. Figure reprinted from R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994). Copyright 1994 American Physical Society

156

4 Pseudogap Eﬀects in Cuprate NMR Studies

There will be further discussion of relaxation eﬀects in LSCO:x in Chap. 6, where there is extensive discussion of INS results on this compound as well as of T2g data in connection with the quantum critical scaling model of Pines and co-workers.

References

1. W.W. Warren, Jr., R.E. Walstedt et al., Phys. Rev. Lett. 62, 1193 (1989) 116, 120 2. H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989) 116, 117, 118, 128, 132 3. M. Horvati´c, P. S´egransan, C. Berthier, Y. Berthier et al., Phys. Rev. B39, 7332 (1989) 116 4. H. Yasuoka, T. Imai, T. Shimizu, In Strong Correlations and Superconductivity, ed H. Fukuyama, S. Maekawa, A.P. Malozemoﬀ (Springer-Verlag, Berlin, 1989) See also H. Yasuoka, S. Kambe, et al., Physica B199&200, 278 (1994) 116 5. H. Alloul, A. Mahajan, H. Casalta, O. Klein, Phys. Rev. Lett. 70, 1171 (1993) 117, 128, 132 6. J. Friedel, Physica C153-155, 1610 (1988) 117 7. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 117, 149, 151 8. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990) 118, 120, 127, 128 9. M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991) 118, 120, 121, 122, 12 10. M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993) 118, 122, 123, 124, 11. S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 120 12. B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 120, 126 13. H. Monien, D. Pines, M. Takigawa, Phys. Rev. B43, 258 (1991) 122, 124 14. A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 122 15. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 126, 133 16. F. Mila, T.M. Rice, Physica C157, 561 (1989) 126 17. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 126, 128 18. M. Randeria, N. Trivedi, A. Moreo, R.T. Scalettar, Phys. Rev. Lett. 69, 2001 (1992) 126, 127, 129 19. J.M. Tranquada et al., Phys. Rev. B46, 5561 (1992) 126, 128, 129, 130 20. G. Balakrishnan, R. Dupree et al., J. Phys. C: Solid State Phys. 21 L847 (1988) 128 21. M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 128 22. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 127 23. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 127 24. P.M. Gehring, J.M. Tranquada, et al., Phys. Rev. B44, 2811 (1991) 128 25. J. Rossat-Mignod, et al., Physica B169, 58 (1991) 128 26. L.D. Rotter et al., Phys. Rev. Lett. 67, 2741 (1991) 134 27. M. Randeria, Precursor Pairing Correlations and Pseudogaps, [Varenna Lectures 1997]; cond-mat/9710223 134 28. J.W. Loram et al., Phys. Rev. Lett. 71, 1740 (1993) 134 29. J.W. Loram et al., Physica C 135-140 134 (1994) 134 30. W.Y. Liang, J.W. Loram, Physica C 263, 277 (1996) 134, 135, 136 31. P.W. Anderson, Science 235, 1196 (1987) 136 32. N. Nagaosa, P.A. Lee, Phys. Rev. B45, 966 (1992) 136

References 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61.

157

J.M. Harris, Z.-X. Shen et al., Phys. Rev. B54, R15665 (1996) 136 A.G. Loeser et al., Science 273, 325 (1996) 136 H. Ding et al., Nature (London) 382, 51 (1996) 136 R.M. Hazen, in Physical Properties of High Temperature Superconductors, ed D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), Vol. II, p.121 139 T. Machi, I. Tomeno, et al., Physica C173, 32 (1991) 139, 140, 142 H. Zimmerman, et al., Physica C159, 681 (1989) 139 H. Yasuoka, Hyperf. Int. 105, 27 (1997) 139 I. Tomeno, T. Machi et al., Phys. Rev. B49, 15327 (1994) 139, 143 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 141, 143 G.V. M. Williams et al., Phys. Rev. Lett. 80, 377 (1998) 142, 143, 144, 145, 146 J.P. Franck, in Physical Properties of High Temperature Superconductors, ed D.M. Ginsburg (World Scientiﬁc, Singapore, 1994), Vol. IV, p.189 143 F. Raﬀa, T. Ohno et al., Phys. Rev. Lett. 81, 5192 (1998) 144, 145 C.M. Varma, Phys. Rev. B73, 155113 (2006) 144, 146, 147, 150, 151 C.M. Varma, P. Littlewood et al., Phys. Rev. Lett. 63, 1996 (1989) 146 B. Fauqu´e et al., Phys. Rev. Lett. 97, 197001 (2006) 146 G. Xiao, M.Z. Cieplak et al., J. Phys. Soc. Japan 62, 2591 (1993) 147 A.V. Mahajan, H. Alloul, G. Collin, J.F. Marucco, Phys. Rev. Lett. 72, 3100 (1994) 147 J. Bobroﬀ, W.H. MacFarlane, H. Alloul, P. Mendels et al., Phys. Rev. Lett. 83, 4381 (1999) 147 W.H. MacFarlane, J. Bobroﬀ, H. Alloul, P. Mendels, N. Blanchard, Phys. Rev. Lett. 85, 1108 (2000) 147 G.–Q. Zheng, T. Odaguchi, T. Mito, Y. Kitaoka et al., J. Phys. Soc. Japan 62, 2591 (1993) 147, 148 S. Ohsugi, Y. Kitaoka, K. Ishida, G.-q. Zheng, K. Asayama, J. Phys. Soc. Japan 63,700 (1994) 147 R.J. Cava, R.B. Van Dover, B. Batlogg, E.A. Rietman, Phys. Rev. Lett. 58, 408 (1987) 148 T. Nakano et al., Phys. Rev. B49, 16000 (1994) 149, 150, 151, 152 R. Yoshizaki et al., Physica C 166, 417 (1990) 149 K. Ishida et al., J. Phys. Soc. Japan 60, 3516 (1991) 152 G.-q. Zheng, et al., Phys. Rev. Lett. 86, 4664 (2001) 152 S. Ohsugi, Y. Kitaoka, K. Ishida, G.-Q. Zheng, K. Asayama, J. Phys. Soc. Japan 63, 700 (1994) 152 K. Yoshimura, T. Imai et al., J. Phys. Soc. Japan 58, 3057 (1989) 153, 155 R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 153, 155

This page intentionally blank

5 Relaxation Models for Cuprate NMR

From the very beginning of cuprate NMR studies, it was clear that understanding the relaxation properties for all sites with nuclear spin species would be a major challenge for theorists and experimentalists alike. In Chap. 3 the Mila-Rice-Shastry model [1, 2] was presented, including the quantum-chemical basis for transferred HF couplings and the spin Hamiltonian treatment of local spin and orbital HF eﬀects at the Cu2+ sites. With the latter formulation a complete characterization of the NMR shift tensors for YBCO7 and YBCO6.63 has been carried out in Chaps. 3 and 4. Then, using general expressions for 1/T1 , Mila and Rice discussed T1 anisotropy for 63 Cu(2) in YBCO7 (Sect. 3.3.4). A simpliﬁed model given in Sect. 4.1.2 oﬀered an interpretation of T1 anisotropies and spin correlation eﬀects for the 89 Y and 17 O(2,3) sites. These developments set the stage for the most serious challenge, which is the locally-varying, overall temperature dependences of the T1 processes in these compounds. Such a panorama of complex relaxation behavior had never been encountered before the cuprates were discovered. A variety of models treating the relaxation processes have been put forward in the literature. Here, we will review the results of several of these models in an eﬀort to gauge the present status of our understanding of these matters. There have been phenomenological models put forward by Monien and Pines [3] and Millis, Monien, and Pines [4, 5], where the AFM ﬂuctuations are taken into account by means of an RPA treatment of the AFM exchange interactions. Moreover, it is assumed and is consistent with experiment that the Cu2+ spin variables are itinerant and undergo pairing in the superconducting state. Similar modeling along these lines has also been put forward by Horvati´c et al. [6]. These models were presented early on and gave a reasonable account of the data which were available at the time. In particular, they met the challenge of explaining the behavior of all measured relaxation processes with a single dynamical variable per Cu site, and did so using only HF couplings generated by the Cu2+ spin moments, in a picture consistent with the Mila-Rice model [1] of on-site spin–Hamiltonian and transferred HF couplings of the general

R.E. Walstedt: Relaxation Models for Cuprate NMR, STMP 228, 159–211 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 5

160

5 Relaxation Models for Cuprate NMR

form α Aα Sα Iα . A possible deviation from this form may occur in the case of 89 Y in YBCO compounds, where the transferred coupling is very weak and the dipolar interactions, which do not have the latter form, come into play. A slightly diﬀerent approach to modeling the dynamical susceptibility has been pursued by Auler et al., [7], where the basic form of the dynamic susceptibility was taken directly from INS data. This scenario had the unusual feature that the range of spin-spin correlations was ﬁxed, although their strength certainly increased as temperature was lowered. These authors also made the unusual step of using spin-echo decay time (T2g ) measurements to determine the strength of the AFM susceptibility peak. In reviewing the results of their an analysis, we shall ﬁnd that a satisfactory account of the data can be achieved in this fashion. Beyond phenomenology, there have also been ﬁrst-principles model calculations by Bulut and Scalapino [8] and by Si, Levin, and co-workers [9]. The latter are, of course, more diﬃcult to formulate and execute, but these have yielded impressive insights. Finally, there has been a proposal by Varma which departs from the usual spin HF-only picture wherein an intersite orbital matrix element is suggested to make an important contribution to the Cu(2)-site relaxation process [10]. The essence of these various results will be summarized below. This chapter will begin, however, with a discussion of the characterization of the cuprate relaxation properties developed quite recently by Uldry and Meier [11] (UM). This is a scheme of a fairly general nature for characterizing the spin dynamics and spin-spin correlations which determine the relaxation behavior in the CuO2 planes. It serves as a useful framework for evaluating almost any experimental data or theoretical model.

5.1 The Uldry-Meier Parameterization Model The Uldry-Meier (UM) approach to the analysis of cuprate relaxation data relies only on a general formulation of spin-ﬂuctuation T1 processes, which is characterized by just three elements, (i) the HF constants, (ii) real-space, dynamical spin-spin correlation coeﬃcients, and (iii) an eﬀective correlation time parameter in which the temperature variation of the spin dynamics is also implicit in a very general way. The HF parameters used are those derived from the Mila-Rice-Shastry model (3.3.2) for each site in and near the CuO2 planes.1 The spin-spin correlations and correlation time which characterize the relaxation processes are assumed to apply to all nuclear species considered, e.g. the 63 Cu(2), 17 O(2,3), and the 89 Y in YBCO7 and YBCO6.63, etc. The spin-spin correlations are allowed to be anisotropic, but the correlation time variable is assumed to be isotropic and common to all spin ﬂuctuation processes. After describing the UM analysis, the broader signiﬁcance of this methodology will be discussed at the end of this section. 1

The Cu(1) sites and environs in YBCO are set aside as a separate problem.

5.1 The Uldry-Meier Parameterization Model

161

5.1.1 Basic Formulation of the UM Analysis In the ﬁrst step, UM deﬁne single-axis T1 components 1 = Uβ + Uγ , T1α

(5.1.1)

where the subscripts are a permutation of the axes (a,b,c). Thus, Uα is an axis-speciﬁc ﬂuctuation term given by Uα =

1 α [Aiα Ajα Kij ]τeﬀ , 4 i,j

(5.1.2)

where Aiα is the HF coeﬃcient for the ith neighbor spin S iα (see (3.3.2)), and α the Kij are now deﬁned as α = 4 Siα Sjα , Kij

(5.1.3)

where the index α allows the spin-spin correlations to be anisotropic. The α α α α α ’s which will occur in the analysis are Kii = 1 and K01 , K12 , and K13 , only Kij where the subscripts refer to the sites in Fig. 3.6. These correlation factors, originally introduced by Mila and Rice [1] were deﬁned and discussed in Sect. 3.3 and 3.5. In particular, they are easily expressed in terms of χ (q, ω) (see (3.5.17) and (3.5.18)). The parameter τeﬀ plays the role of a correlation time in (5.1.2), but also contains the eﬀects of quasiparticle dynamics in the calculation. At low temperatures, for example, τeﬀ ∝ T . In (3.5.17) a similar quantity Xat was introduced, where we can make the identiﬁcation τeﬀ = (kB T /)Xat . In ﬁtting (5.1.2) to the experimental data, the principal assumption is the form of the HF coupling Hamiltonian (3.3.2), where it should be noted that deviations from this form (e.g. dipolar coupling) are not unusual. In Sect. 3.5 the Kij ’s were also formulated in terms of χ (q, ω), giving a ﬁrm theoretical foundation for (5.1.2) in terms of spin-ﬂuctuation relaxation processes. The determination of T1 for any nuclear spin site given χ (q, ω) and a set of HF tensors is clear enough in terms of the foregoing deﬁnitions. However, the innovative task performed by Uldry and Meier was to devise a scheme to extract the HF constants, τeﬀ , and the Kij ’s, including temperature dependences, from a comprehensive body of relaxation data for a cuprate compound. We review their method here, using the example of YBCO7. In order to fully characterize the relaxation process of a given nuclear site, it is necessary to have T1 data from all three axes, since from (5.1.1) we have Uα = 12 [1/T1β + 1/T1γ - 1/T1α ]. It simpliﬁes, of course, if there is ab plane symmetry. Thus, it is necessary to have a full data set for all nuclear sites of interest in order to apply this scheme of analysis to any given cuprate. In Fig. 5.1(a)–(c), a 100 K - 300 K data set is shown for 63 Cu(2) [12, 13], 17 O(2,3) [14], and 89 Y[15] in YBCO7, plotted as 1/T1 T vs. T . Using (5.1.1), the corresponding (interpolated) plots for 63 Uα , 17 Uα , and 89 Uα are shown

162

5 Relaxation Models for Cuprate NMR 50

4000

(a) 63Cu(2) Uα [S–1]

3000

30 20

(d) 63Cu(2) 2000

63

(63T1αT)–1[S–1K–1]

40

1000 10 0

0

200

400

0 100

600

150

250

300

250

300

Uα [S–1]

60

0.3 0.2

40

17

17 –1 –1 –1 ( T1αT) [S K ]

300

(e) 17O(2,3)

0.4

(b) 17O(2,3)

0.1

0

200

400

600

20

0 100

800

150

Temperature[K]

200 Temperature[K]

0.05

2.5

0.04 Uα [S–1]

3

2

89

(89T1αT)–1[10–4 S–1K–1]

250

80

0.5

0

200 Temperature[K]

Temperature[K]

1.5

(f) 89Y

0.03 0.02

(c) 89Y 0.01

1 0 0

200

400 Temperature[K]

600

800

0 100

150

200 Temperature[K]

Fig. 5.1. (a)–(c) Relaxation data for YBCO7 plotted as circles, upward triangles, and diamonds from [12] (63 T1c ), [13] (63 T1ab ), [14] (17 T1α ), and [15] (89 T1γ ) are plotted as 1/T1 T vs. T . Solid lines drawn are ﬁtted curves derived from the UM model calculations (see text). The downward triangles are supplemental data included to illustrate high-T behavior for the 17 O(2,3) [16] and the 89 Y [17], as discussed in the text. (d)–(f) Interpolated values of k Uα (T) derived from the data shown and described in (a)–(c), with which the actual ﬁtting process was conducted. The solid lines drawn are guides for the eye. The straight line drawn in panel (d) shows 1/63 T1 vs. T for Cu metal for comparison. Reprinted ﬁgures from A. Uldry and P. F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

5.1 The Uldry-Meier Parameterization Model

163

in Fig. 5.1(d)–(f). It is remarkable how similar the latter curves look when plotted as 1/T1 rather than as 1/T1T . The next step was to make a simplifying approximation regarding the Kij ’s. Since the three √ described above correspond to spin sites separated α by distances a/2, a/ 2, and a, respectively, UM have assumed that K12 = √ α α α 2 2 (K01 ) , and K13 = (K01 ) , which is equivalent to the assumption of the form α Kij = exp(−2rij /aλα ). At each temperature, then, the ﬁt procedure only has α to determine the two values λab,c , rather than six Kij ’s. If this approach should prove unsatisfactory it could easily be modiﬁed. It is also convenient to deﬁne, along with the k Uα ’s, a parallel set of coeﬃcients k Vα , given by k Uα = k Vα τeﬀ . Then from (3.5.20), (3.5.21), and (3.5.22) we have 1 2 α α [A + 4B 2 + 8 Aα BK01 (T ) + 8B 2 K12 (T ) 4 α α (T )] +4B 2 K13 1 17 α Vα (T ) = Cα2 [1 + K01 (T )] 2 89 2 α α Vα (T ) = 2 Dα [1 + 2 K01 (T ) + K12 (T )], 63

Vα (T ) =

(5.1.4a) (5.1.4b) (5.1.4c)

where superscripts are used to label the isotope concerned. Since the HF coeﬃcients used here relate directly to (3.3.2), their anisotropies as well as those of the λα ’s should stem directly from the data in a natural way. 5.1.2 The Uldry-Meier Analysis of YBCO7 The following procedure was used to apply the foregoing analytical scheme to the data in Fig. 5.1(d)–(f). Deﬁning the six ratios, 63

r1 =

Uc

17 U

c

63

; r2 =

Uab ; 17 U a

63

r3 =

Uab ; 17 U b

17

r4 =

Ub

17 U

c

89

; r5 =

Uc

89 U

ab

17

; r6 =

Ua , 89 U c

(5.1.5) the HF constants in (5.1.4) and the λα ’s are then determined by minimizing the quantity np nr 1 [riexp (Tj ) − rimod (Tj )]2 χ2 = , (5.1.6) nr i j riexp (Tj )2 where nr and np are the numbers of ratios (= 6) and the numbers of points (= 10), respectively, and where the rimod for the “model” are actually calculated from (5.1.4) in terms of the HF constants and the λα ’s. Note that the ri ’s do not involve the quantity τeﬀ . The HF parameters so obtained are listed in Table 5.1, where for comparison a “standard” set of parameter values from UM are given, as well as the YBCO parameters derived from NMR shift data in Chaps. 3 and 4. We consider these comparisons in detail below. A plot of τeﬀ vs. T is then determined for each parameter Uα via (5.1.2). The λα ’s and the results for τeﬀ so determined are displayed in Fig. 5.2(a) and

164

5 Relaxation Models for Cuprate NMR

Table 5.1. HF coeﬃcients deﬁned in (3.3.4) and derived from the UM ﬁt procedure with the T = 100 K relaxation data shown in Fig. 5.1, as described in the text, are listed and compared with data presented by Nandor et al., [17] as well as with data derived from NMR shift measurements as described and presented in Tables 3.4 and 3.6. HF coeﬃcient values are given in units of 10−6 eV . See text for discussion of these results HF Constant UM Fit Nandor Shift Coef.

63

Ac

−1.68 −1.6 −1.67

63

Aab

0.168 0.29 0.05

B 0.438 0.4 0.409

17

Ca

0.259 0.25 0.355

17

Cb

0.173 0.13 0.217

17

Cc

−89 Dab

−89 Dc

0.196 0.156 0.209

0.00280 0.0048 0.00286

0.00349 0.0048 0.00369

(b), respectively. The correlation lengths, which are of the order of the lattice constant, are seen to execute a smooth progression toward longer values as T decreases, a process which accelerates below 150 K. They also ﬁnd consistent anisotropy of ∼ 20%, the stronger c-axis correlations suggesting the possibility of a corresponding exchange anisotropy between neighboring Cu2+ spins. Although the ﬁtting scheme with the ratios ri promotes consistency among τeﬀ values it is nonetheless remarkable how nicely they each describe a very similar arc with temperature. As we shall see below, some of the most subtle physics of the cuprate spin ﬂuctuations is embodied in the behavior of τeﬀ , where even at this point a great deal remains to be understood. The HF coeﬃcients from the ﬁt are compared with values from other sources in Table 5.1. The HF constants labelled “Nandor” [17] are actually mostly derived from Barzykin and Pines [18], and are seen to be in rough accord with the ﬁt. The “Shift Coef.” values shown have been converted from the primed coeﬃcients in Tables 3.4 and 3.6 using (3.3.4) so that g-factor anisotropy (3.3.7) comes into play. The value of B given, for example, comes from c-axis shift measurements. The value of 63 Aab = 0.05×10−6eV is obtained by subtraction of large values and is correspondingly unreliable. The agreement of the 63 Ac and of the 89 Dα tensors is very good, indeed. The ﬁtted values of the 17 Cα are 10–20% below those derived from the NMR shifts. This is an interesting point, because the “T1 problem” for the 89 Y discussed in Sect. 4.1.2 has been managed in the UM ﬁt process not by enhancing the 89 Dα tensor coeﬃcients, but by reducing the 17 Cα ones. Either way, there will be a discrepancy between shift coeﬃcients and those derived from relaxation. We continue to believe that there is an additional 89 Y relaxation process (orbital or dipolar), which is beyond the eﬀects of the MR Hamiltonian (2.3.2). In spite of this eﬀect, there is quite a good correspondence between HF constants derived from the UM ﬁt and those from NMR shifts. It is also noteworthy that the ﬁtting procedure based on 5.1.5 is independent of scale. That is, all HF constants (e.g. the k Vα ’s in (5.1.4)) can be multiplied by a uniform scale factor and the results will not be aﬀected. Thus,

5.1 The Uldry-Meier Parameterization Model

165

any set of results for the HF constants needs to be keyed to some particularly reliable value. In Table 5.1 the results are, in eﬀect, keyed to 63 Vc . The UM ﬁtting procedure leads to temperature dependences for the correlation lengths λα shown in Fig. 5.2(a) and to seven estimates (from the k Vα ’s in (5.1.4)) for the correlation time curve τeﬀ (T ), which are summarized in a plot in Fig. 5.2(b). In the latter case the extrema of the bundle of seven curves are shown as dashed lines, where the circles are the average values. The dotted line is a functional ﬁt described below. Considering the 89 Y relaxation rate

λ[a]

(a)

λ[a]

1.2

1

100

1

300 T[K]

0.8

0.6 100

150

200

250

300

Temperature[K]

(b)

τeff[10–15 s]

1.5

1

0.5

0

0

100

200

300

400

500

600

Temperature[K]

Fig. 5.2. (a) Correlation lengths λab (circles) and λc (triangles) derived from the UM ﬁt to YBCO7 are plotted vs. T over the range of the ﬁt. Inset: Low and high-T asymptotic behavior used to extrapolate the λα ’s is shown with dotted lines. (b) The average (circles) and extremal (dashed lines) values for the seven sets of τeﬀ parameters obtained from the T1 data ﬁt for YBCO7 are plotted vs. T . The dotted line is a ﬁt to these data which is extrapolated down to T = 0 and upward to T = 600 K. This ﬁt and its interpretation are described in the text. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

166

5 Relaxation Models for Cuprate NMR

anomaly noted above and in Sect. 4.1.2, the degree of consistency among τeﬀ values is surprisingly good. Extrapolation of the Fits to Higher Temperatures In Fig. 5.1(a)–(c) we see that the ﬁts are generally very good over the ﬁtting temperature range. However, UM went on to extrapolate their ﬁts to higher temperatures with a ﬁtting function ansatz as follows. The general behavior of τeﬀ (T ) in Fig. 5.2(b) is one of downward curvature, but linear in T at the lowT end. The latter feature is expected in metallic hosts, but the curving over is much greater than could be attributed to loss of Fermi-statistical degeneracy. They propose a ﬁtting function wherein a Fermi-statistical term τ1 = aT is combined in an inverse fashion with a constant term τ2 which dominates at high temperatures. Thus [11], 1 1 1 1 1 + , = + = τeﬀ τ1 τ2 aT τ2

(5.1.7)

where a = 7 × 10−18 s/K and τ2 = 3 × 10−15 s. The line representing this function is plotted in Fig. 5.2(b) as a dotted line up to 600 K. In Sect. 5.4 and 5.5 we shall look for the possible origin of this ﬂattening eﬀect in the Hubbard models. However, it does not appear to have been successfully identiﬁed yet. The physics of the ansatz (5.1.7) is a bit unfamiliar, because normally when two rates combine inversely, it is the “faster” of the two which dominates. Here, however, at high temperatures when the Korringa T1 is very short, it is undercut by a weaker relaxation process. As for the form of τ1 , Pines and Slichter [19] suggest a picture where τ1 = τc T /TF is made up of a correlation time factor τc ∼ /EF representing the dwell time of a carrier in the unit cell, and T /TF represents a Fermi-statistical scattering probability factor. Thus, a = /kB TF2 , from which UM estimated TF ∼ 1000 K. Meanwhile, τ2 appears to represent the behavior of the gas of quasiparticles when the degeneracy is completely lifted. This extrapolation of the curve for τeﬀ (T) is also used to extrapolate the ﬁt curves in Fig. 5.1(a)–(c). It is interesting to compare these extrapolations with high-temperature data by Nandor et al., [17] for 17 O(2,3) and for 89 Y, shown in panels (b) and (c) as downward triangles. The data for 17 O(2,3) fall somewhat below the ﬁtted data, but show a temperature dependence which is in general accord with the extrapolated model prediction. For the 89 Y, however, contrary to the model the data are ﬂat if not slightly rising with temperature. This behavior is consistent with the ﬁnding in Sect. 4.1.2 that there is an additional relaxation term for the 89 Y beyond what is derived from (2.3.2). A possible orbital term was mentioned in Sect. 4.1.2. There are also dipolar terms which do not follow the spin-spin correlations [15]. The dipolar terms have also been calculated by Auler et al., [7] and are discussed further in Sect. 5.3.

5.1 The Uldry-Meier Parameterization Model

167

The Spin Correlations and the “Basic” Relaxation Mechanism The ﬁt to YBCO7 data illustrates rather dramatically the role played by antiferromagnetic (AFM) spin-spin correlations in the relaxation processes of all nuclei. It is interesting in this connection to examine the behavior of the k Vα (T ). According to the deﬁnitions (5.1.4), the k Vα (T ) can vary from a hightemperature limit where Kij → 0, to a fully correlated limit at low T where (in principle) K01 → −1 and K12 , K13 → 1. The T → ∞ limits for the k Vα (T ) are deﬁned to be k Vα0 , and are given by 63

Vα0 =

1 2 (A + 4B 2 ) 4 α 1 17 0 Vα = Cα2 2 89 0 Vα = 2 Dα2 .

(5.1.8a) (5.1.8b) (5.1.8c)

The “basic” relaxation mechanism is what it would be in the absence of AFM correlations and is given by 1/k T1α = k Vα0 τeﬀ . Thus, apart from a scale factor, it is the same for all nuclei in the system. The AFM correlation factors are the only thing which distinguishes the behavior of diﬀerent nuclei. Fig. 5.3(a)–(c) illustrate this point by plotting the k Vα (T ) vs. T for the YBCO7 ﬁt. (Fig. 5.3(d)–(f) plot the same quantities for YBCO6.63 - see discussion below.) The high-temperature (Kij = 0) limits are shown as solid bars on the right, and the low-temperature limits by solid bars on the left side of the ﬁgures. The T → 0 behaviors are estimated by extrapolating the correlation lengths in Fig. 5.2(a) by means of the dotted lines shown in the inset. The behavior seen in these plots shows (i) that the correlation causes the relaxation rates of the 63 Cu(2) to increase and those of the 17 O(2,3) and the 89 Y to decrease, and (ii) that the behavior of all three nuclear species is changed by similar amounts as a result of the correlations. In this picture it is something of an accident that the 17 O(2,3) and the 89 Y relaxation processes appear to be Korringa-like in the normal state. According to Fig. 5.3(a)-(c) the AFM correlations make sharp increases in the superconducting state. It must be emphasized that this is an extrapolation of normal-state behavior and is entirely hypothetical. As we shall see in Sect. 5.7, the actual behavior below Tc is quite diﬀerent from what is shown here. 5.1.3 The Uldry-Meier Analysis of YBCO6.63 A very similar analysis to that described above was carried out by UM for YBCO6.63. The quality of the input data was perhaps not quite as good, and there were no data at all for 63 T1ab . The analysis was simpliﬁed a bit by adopting the HF tensor values shown in Table 5.1 for the YBCO6.63 analysis (recall that the values derived from NMR shifts in Chap. 4 were found to be nearly the same). The ﬁtted curves (not shown) were only slightly less good, where, not surprisingly, the 89 Y ﬁts were noticeably worse than the others.

168

5 Relaxation Models for Cuprate NMR 5000

7000

Cu(2)

4000

YBCO7

4000 3000

(d) 63Cu(2) 3000

YBCO6.63 2000

63

Vα [1015s–2] 63

5000

Vα [1015s–2]

(a)

6000

63

2000

1000 1000 0 0

100

200

300

400

500

0

600

100

Temperature [K]

200

300

Temperature [K] 60

80

(e) 17O(2,3) Vα [1015s–2]

(b) 17O(2,3)

17

40

17

Vα [1015s–2]

60

20

YBCO6.63

40

20

YBCO7 0 0

100

200

300

400

500

100

600

Temperature [K]

(f) 89Y

(c) 89Y Vα [1015s–2]

0.05 0.04 0.03

89

Vα [1015s–2]

300

0.03

0.06

89

200 Temperature [K]

0.02

0.02

0.01

YBCO7

YBCO6.63

0.01 0

0 0

100

200

300

400

Temperature [K]

500

600

100

200

300

Temperature [K]

Fig. 5.3. (a)–(c) Curves are plotted representing 63 Vα (T ), 17 Vα (T ), and 89 Vα (T ) for the ﬁt to YBCO7 in (a), (b), and (c), respectively. The solid bars on the right represent the values of k Vα0 corresponding to zero spin correlations, and the bars on the left represent maximum correlations as explained in the text. The data plotted are seen to run between these two limits. The zero-temperature points for these curves were obtained by extrapolating the variation of the λα ’s near 100 K to zero temperature. Such an extrapolation is entirely hypothetical. (d)–(f) Curves are plotted representing 63 Vα (T ), 17 Vα (T ), and 89 Vα (T ) for the ﬁt to YBCO6.63 in (d), (e), and (f), respectively. These results are similar to those on the left, but AFM correlations show a wider range and reversed curvature as compared with YBCO7. Reprinted ﬁgures from A. Uldry and P. F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

5.1 The Uldry-Meier Parameterization Model

169

The results for k Vα (T ) curves are shown in Fig. 5.3(d)–(f), where they are seen to be quite diﬀerent from those for YBCO7. The correlation lengths for YBCO6.63 were longer than for YBCO7, reaching ∼ 2.5 a or so. As a result the range and magnitude of the correlation factors driving the k Vα (T ) curves are considerably greater than for YBCO7. Another interesting feature is that the curvature of the k Vα (T ) curves is in all cases the opposite in these two systems. There was also slightly more scatter in the τeﬀ (T ) curves for YBCO6.63, shown in Fig. 5.4(a), where they execute a considerably greater range than for YBCO7 (Fig. 5.2(b)). This, of course, results from the gapped nature of the static and dynamical properties of YBCO6.63. The average curve for τeﬀ (circles) was again ﬁtted with the ansatz (5.1.7), except that a gap feature is introduced into the density of states with τ1 (T ) = a T exp(−Tg /T ).

(5.1.9)

With that modiﬁcation, (5.1.7) was ﬁtted to the data in Fig. 5.4(a) and is shown as a dotted line extending from 0 K to 600 K. The ﬁtting parameters are listed below in Table 5.2, where a and τ2 are seen to be quite similar to those for YBCO7. The gap energy Tg = 94 K is very close to that (104 K) derived from the susceptibility in Fig. 4.4, rather than being twice that value as we found for Y248 in Sect. 4.3. The slightly lower value for a suggests a somewhat lower degeneracy temperature for YBCO6.63 as shown in the table. 5.1.4 The Uldry-Meier Analysis of YBa2 Cu4 O8 (Y248) The foregoing analytical scheme was also applied, in a somewhat restricted fashion, to the case of Y248, analyzing the same body of NQR data for 63 Cu(2) as were discussed in Sect. 4.3. The method was restricted owing to a total lack of T1 data for other sites and orientations. As a consequence, the 63 Vab (T ) curve for YBCO7 (see Fig. 5.3(a)) was adopted for the Y248 calculation, where 1 = 2 63 Vab τeﬀ . (5.1.10) 63 T 1c This is a fairly “neutral” assumption, since the temperature proﬁle of 63 Vab (T ) is seen to be very ﬂat for both YBCO7 and YBCO6.63 in Fig. 5.3, but particularly in the former case. In any case, the ﬁt to the data for 1/63 T1c T , shown in Fig. 5.5(a) and (b), is seen to be excellent, and furthermore, extends up beyond 700 K. Note that the 100 K – 350 K data set from Raﬀa et al., [20] (crosses) has been augmented with high-temperature data from Curro et al., [21] (triangles pointing right) and from Tomeno et al., [22] (triangles pointing down). Although the proﬁle of τeﬀ (T ) may be slightly diﬀerent from what one would ﬁnd with a full-blown analysis such as that for YBCO7, it behaves in a very interesting fashion as shown in Fig. 5.4(b). Here there is only one

170

5 Relaxation Models for Cuprate NMR 2

τeff[10–15 s]

1.5

1 (a) YBCO6.63 0.5

0

0

100

200

300

400

500

600

500

600

Temperature[K] 2

τeff[10–15 s]

1.5 (b) Y248 1

63Cu(2)

0.5

0

0

100

200

300

400

Temperature[K]

Fig. 5.4. (a) The data for τeﬀ (T ) derived from the ﬁt to several relaxation curves from YBCO6.63, as described in Sect. 5.1.3. The circles plot the average values of τeﬀ , and the dashed lines show the most extreme values. The dotted line is a ﬁt of (5.1.7) and (5.1.9) to the average values, extrapolated to 0 K and 600 K. (b)Values for τeﬀ (T ) derived from the ﬁt to the relaxation curve for 63 Cu(2) in Y248, shown in Fig. 5.5, as described in Sect. 5.1.4. The dotted line is a ﬁt of (5.1.7) and (5.1.9) to the data (circles), extrapolated to 0 K and 600 K. Parameters from the ﬁts shown are presented in Table 5.2 and discussed in the text. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

data set from the ﬁt (circles), which has very little scatter. The dotted line is a ﬁtting of the ansatz (5.1.7) with the gap modiﬁcation (5.1.9) used for YBCO6.63. The parameters from this ﬁt are given in Table 5.2, where they may be compared with those for YCBO7 and YBCO6.63. The parameters in Table 5.2 show an interesting progression for the three YBCO-related systems. Although the forms of τeﬀ (T ) in (5.1.7) and (5.1.9) are really just educated guesses, they match the temperature dependence from

5.1 The Uldry-Meier Parameterization Model

171

Table 5.2. Parameters from ﬁts to the ansatz (5.1.7) for YBCO7 and with the gap modiﬁcation (5.1.9) for YBCO6.63 and Y248 are listed, showing a, τ2 , and the gap, crossover, and Fermi temperatures derived from their respective (average) data curves for τeﬀ (T ). The crossover temperature is where τ1 = τ2 , and the estimated Fermi temperature is obtained from TF ∼ (/kB a)1/2 . These results are discussed in the text System

a (s/K)

YBCO7 YBCO6.63 Y248

7 × 10−18 10 × 10−18 44 × 10−18

τ2 (s) 3.0 × 10−15 2.9 × 10−15 1.9 × 10−15

Tg (K) 0 97 195

Tcr (K) 420 375 154

TF (K) 1,050 880 420

the ﬁts better than one might have expected, giving very convincing extrapolations to higher and lower temperatures. After modest changes between YBCO7 and YBCO6.63, with the appearance of a ∼ 100 K gap in the √ latter case, the jump to Y248 shows a doubling of the density of states (∝ a) and a corresponding reduction by half of the estimated degeneracy temperature, as well as a doubling of the gap energy, which now exceeds the cross-over temperature. A somewhat diﬀerent view of the dynamic magnetism of Y248 via dynamical scaling theory is presented in Sect. 6.4. The Wider Role of the Uldry-Meier Model Analysis The UM analysis has oﬀered a highly revealing and greatly unifying look into the microscopic phenomena associated with the cuprate T1 processes. From this perspective, the diﬀerence between diﬀerent sites and nuclear species essentially ceases to be an issue. This analysis is in no sense a theory, though it incorporates a widely accepted and time-tested formulation of the T1 process, and it puts the Mila-Rice HF Hamiltonian to a severe test, which it mostly passes in good order. Note that this Hamiltonian is essentially unique to cuprates among metallic environments. It is worth emphasizing that the UM picture is also implicit in the general χ (q, ω) formulation of the T1 process, as demonstrated in Sect. 3.5. Perhaps the most signiﬁcant advantage of the UM analysis is that it partitions the T1 problem into three independent phenomenological pieces. These are (i) HF constants, which are essentially inert, (ii) AFM correlation factors, which are much larger and universally more important than hitherto realized, and (iii) a comprehensive ﬂuctuation rate, which embodies all of the lowfrequency spin ﬂuctuation physics of the cuprates, including, but not limited to, Fermi liquid, spin pseudogap, and exchange-coupled local moments. The ability to separate elements (ii) and (iii) in either an experimental or theoretical evaluation is a considerable simpliﬁcation and an enormous advantage over previous practice. We emphasize that this analysis oﬀers a useful way to evaluate model theories of χ (q, ω). One can simply evaluate (ii) and (iii)

172

5 Relaxation Models for Cuprate NMR

7

(63T1cT)–1

(a) 6

5

4 50

100

150

200

250

300

350

400

Temperature[K] 7 6 (b)

(63T1cT)–1

5 4 3 2 1 0 200

400

600

800

Temperature[K]

Fig. 5.5. (a) 63 Cu(2) NQR data from [20] for Y248 (crosses) are plotted as 1/T1 T vs. T . The solid line shows the Uldry-Meier ﬁt to these data described in Sect. 5.1.4. (b) The ﬁt curve shown in part (a) is extended to above 700 K. Also shown there are high-temperature data by Curro et al., [21] (triangles pointing right) and by Tomeno et al., [22] (triangles pointing down). The data and the ﬁt are seen to be extremely precise. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

as deﬁned above and judge these components separately on their own merits. This procedure oﬀers a new perspective on theory building for the cuprates and quite possibly for other materials as well.

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates This straightforward phenomenological model [4, 5] served the important role of discussing and testing certain key ideas in the early days when both NMR

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates

173

shift and relaxation data were still unfolding. This model emerged at a time when there was still a great deal of uncertainty about what the ultimate theoretical basis for cuprate T1 processes was going to be. Of the several lines of theoretical approach to cuprate spin dynamics which we discuss in this chapter, the conceptually simple MMP model is a good place to begin. One of the main objectives of MMP was to show that the relaxation of 63 Cu(2), 17 O(2,3), and 89 Y can all be accounted for with a single dynamical variable associated with each Cu2+ site. In ths matter they largely succeeded, although as noted in Sects. 4.3 and 5.1 there are other apparent contributions to the 89 Y relaxation process. However, there is no evidence for another set of dynamical variables besides the Cu2+ spin moments. In addition to the foregoing, these two papers [4, 5] give an in-depth discussion of the physics issues surrounding the NMR T1 problem in cuprates. Although the actual model they expound is a phenomenological treatment of the Mila-Rice Hamiltonian [1], they present a derivation [5] showing that such treatment is equivalent to a tight-binding, band-theory model of an interacting Fermi liquid. The MMP model is based on a mean-ﬁeld treatment of AFM exchange interaction eﬀects in a system of itinerant quasiparticles, i.e. a metal, which would be a simple Fermi liquid without the exchange interactions. We begin by reviewing their derivation of the mean-ﬁeld dynamic susceptibility, in the course of which the relevant parameters are introduced and discussed. The following is just a brief summary. We refer the interested reader to the original papers for greater detail [4, 5] dynamical susceptibility, RPA model. The mean-ﬁeld complex susceptibility χ(q, ω) = χ (q, ω) + i χ (q, ω) of an interaction spin system is given by χ(q, ω) =

χ(q, ω) , 1 − Jq χ(q, ω)

(5.2.1)

where χ(q) is the noninteracting susceptibility, and Jq is the interaction potential. Since NMR frequencies are generally much smaller than the electronic frequencies in such a system, we are concerned here with the region near ω → 0. In this limit it is assumed that ω ω χ (q, ω)|ω→0 → π χ (q, ω = 0) ≡ π χq , (5.2.2) Γq Γq where Γq is a characteristic energy for spin ﬂuctuations at wave vector q. Correspondingly, in the same limit (5.2.1) gives χ (q, ω) −→ π

ω 1 χ , Γq (1 − Gq )2 + (πω/Γq )2 G2q

(5.2.3)

where Jq χq ≡ Gq . As we are treating AFM ﬂuctuations which appear to be diverging as the system is approaching a Ne´el point, Gq is assumed to be peaked at the AFM point Q = (π/a, π/a), at which point it has a value of

174

5 Relaxation Models for Cuprate NMR

slightly less than 1. For (5.2.3) we expand Gq about the AFM point: Gq ≈ GQ - q 2 β02 , where q is measured from Q. The correlation length is deﬁned by GQ = 1 - ξ02 /ξ 2 . Setting Gq = 1 in the second term of the denominator of (5.2.3), we obtain πχ0 πχ (ξ/ξ0 )4 (ξ/ξ0 )4 χ (q, ω) = . 2 2 2 2 4 ω Γ (1 + q ξ ) + (πω/Γ ) (ξ/ξ0 ) Γ (1 + q 2 ξ 2 )2

(5.2.4)

Because of the peaked nature of this function, the q-dependence of the parameters χq and Γ q has been dropped. They argue further that when q is far away from Q, χ (q, ω) should be comparable with the uncorrelated value, so a q-independent term of that magnitude is added in, giving χ (q, ω) πχ (ξ/a)4 = , (5.2.5) 1 + β ω (1 + q 2 ξ 2 )2 Γ ω→0 where β = (a/ξ0 )4 (χ/χ0 )(Γ/Γ ), χ0 is the uniform susceptibility, and Γ is the spin ﬂuctuation frequency of the noninteracting system. Equation (5.2.5) may then be used to model quasiparticle dynamics for cuprate systems not too far from an AFM instability, i.e. when ξ/a 1. From (5.2.4) we also see that the eﬀective spin ﬂuctuation frequency is ωSF ∼

Γ ξ02 , ξ2

(5.2.6)

which can be greatly diminished if ξ ξ0 . The q-dependent HF coupling Hamiltonian terms are denoted k Fα (q) here (3.5.6) for nuclear spin species k and axis α. Thus, the relaxation rate k Wα ≡ 1/k T1α is given by [5] kB T k k 2 k 2 χ (q, ω) Wα = Fβ (q) + Fγ (q) , (5.2.7) 4μ2B q ω ω→0 where (α, β, γ) is any permutation of the (a,b,c) axes. In (5.2.7) the k Fα (q) have the dimension of s (cf. (3.5.10)), where g-factor anisotropy is not included. For YBCO the k Fα (q) are Fα (q) =63 Aα − 2B(cos qx a + cos qy a), 17 Fα (q) = 2 Cα cos2 ( qx,y a/2) ,

(5.2.8a) (5.2.8b)

Fα (q) = 8Dα cos(qx a/2) cos(qy a/2) cos(qz a/2)

(5.2.8c)

63

89

(see (3.5.10) - (3.5.14)). The ﬁtting procedure, which is described brieﬂy below, thus consists of estimating the HF constants (A, B, C, D’s) from NMR shift and susceptibility data, and then adjusting the parameters Γ , β0 , and ξ from (5.2.5) to match the calculated rates k Wα (T ) as well as possible with experimental data.

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates

175

The MMP Fitting Process for YBCO7 Here we summarize the issues regarding this ﬁtting procedure as well as a brief description of the procedure itself. We ﬁrst note that the squared Lorentzian form for χ (q, ω) in (5.2.5) is valid when ξ/a 1, whereas the deduced YBCO7 values of ξ/a are of order unity. For this reason, MM also discussed the case of a Gaussian form for the peak at Q [5]. The latter is more nearly consistent with peaks in χ (q, ω) which have been reported from neutron scattering studies [23]. The latter results also showed some sign of incommensurability, which is also a major eﬀect in LSCO. The question is whether the incommensurability observed by neutron scattering at energies of more than 1 meV is still present at NMR frequencies, which are roughly four orders of magnitude smaller. In Chap. 6 it will be shown that incommensurability in χ (q, ω) is incompatible with NMR data on LSCO. We assume this is also true here and adopt with MM [5] a picture with commensurate AFM ﬂuctuations. The HF parameters used by MM are compared with those from the UM ﬁt as well as those from NMR shift values in Chap. 3 (see Table 5.1) in Table 5.3. In MM the HF values are given in units of μ2B /χ0 . Here we convert them to units of 10−6 eV . Since the susceptibility is assumed to be isotropic, we have used the powder average susceptibility per Cu(2) ion from Table 3.4 for this purpose. It was also assumed that Ac + 4B = 0, essentially consistent with earlier practice. The other MM values show some small diﬀerences with the other values listed. The ratio Ca to Cc is ∼ 1.5, in rough agreement with the others. However, the ratio Ca /D 69 is rather smaller than the “Shift Coef.” value 113, so that the “problem” with the T1 of 89 Y (see Sect. 4.1.2) will not arise here. We ﬁrmly believe this problem to exist. In the MM ﬁt there was no value available for Aab , so this was left as a parameter to be “ﬁtted”. From the Cu(2) T1 anisotropy 63 Wab /63 Wc it was decided that 0.1 ≤ Aab /4B ≤ 0.2, which is not unreasonable. This estimation is compared with other values in Table 5.3. The susceptibility parameters β and ξ from (5.2.5) – and their temperature dependences – were to be extracted Table 5.3. The HF parameters for YBCO7 and YBCO6.63 used by MM [5] are compared with values from the UM ﬁt and those derived from NMR shift coeﬃcients in Chap. 3 (both given in Table 5.1). The coeﬃcients in MM were given in units of μ2B /χ0 , which have been converted to eV using the powder average susceptibility based on values given in Table 2.4, where χ0 is interpreted to be the value for a single Cu(2) site. The values for Ca and Cc have been reversed, since the larger value corresponds to the Cu-O-Cu (a) axis and the smaller one to the c axis. Parameters are given in units of 10−6 eV Source

Aab + 4B

Aab /4B

Ca

Cc

D

MM [5] UM Fit Shift Coef.

1.45 1.92 1.69

0.1-0.2 0.096 0.03

0.33 0.259 0.355

0.22 0.196 0.209

0.0048 0.00303 0.00314

176

5 Relaxation Models for Cuprate NMR

from the data ﬁts. This was not a simple matter, since these parameters have qualitatively similar eﬀects on the results. There were two main questions to be decided: (i) Can the relaxation of all three nuclei be quantitatively accounted for with (5.2.5) and (5.2.8); and (ii) does a picture of AFM correlations emerge here, where ξ(T ) increases when T descends toward Tc ? The ﬁrst answer is deﬁnitely “yes”, but the second one is a bit more murky. It depended on the relative behavior of 17 Wα (T ) and 89 Wα (T ), for which the available data for the input parameters were not particularly accurate. Calculated ratios of these relaxation rates from MM are shown in Fig. 5.6 for the cases of Gaussian and Lorentzian models for χ (q, ω) and several sets of parameters. The calculations are based on the assumption that 63 Wc /17 Wc = 19 at 100 K and 63 Wc /17 Wc = 10 at 300 K, these values being taken from experiment. Shown is the variation of 17 Wc (T )/89 Wc (T ) between 100 K and 300 K for several sets of parameters, which are shown in Table 5.4. There are two assumed cases here: (i) β is constant and ξ varies with temperature, and (ii) ξ is constant and β varies with temperature. The experimental ratio is around 1,300 and is very nearly ﬂat. These circumstances favor the Gaussian form for χ and the assumption of a constant β with temperature-varying ξ, and thus the solid line in Fig. 5.6(b), case (B). Thus, it was concluded that the constant β picture was more the satisfactory, because if β varies, while ξ is constant, then Γ must have a compensating temperature dependence to keep the pre-factor in (5.2.5) approximately constant. This may be diﬃcult to account for. MM also concluded that ξ/a 1.0–1.5 for the Gaussian case and 1.5–2.0 for the Lorentzian case, while β ∼ 15 or greater. It is interesting to view the results of the MMP analysis in the context of the results of the UM analysis of Sect. 5.1. The parameter values obtained in these cases are similar with some important diﬀerences. The MMP scheme assumed HF parameters derived from NMR shift measurements which are at Table 5.4. Parameter values for the calculated curves in Fig. 5.6 are listed for the three cases plotted for a Lorentzian susceptibility peak (a) and for a Gaussian peak (b). Two curves are plotted for each case, both with the same parameters at T = 100 K and at 300 K with a constant value of β with ξ varied (ﬁrst values listed) and with both ξ and β varied (values in parentheses). The constant β curves are solid lines and those for varying β are dashed lines Case

T(K)

ξ (Lor.)

β (Lor.)

ξ (Gauss.)

β (Gauss.)

A A B B C C

100 300 100 300 100 300

1.9 1.3(1.9) 2.4 1.7(2.4) 3.7 2.5(3.7)

30 30(16) 10 10(3.4) 3.0 3.0(1.1)

1.4 1.1(1.4) 2.0 1.4(2.0) 3.3 2.2(3.3)

30 30(11) 10 10(4) 3.0 3.0(1.2)

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates (a) YBa2Cu3O7 α = 0.2 Lorentzian χ”

(A) 1500

c/

89W c

177

17W

(B) (C)

1000

100

200

300

T(K)

17W / 89W c c

(b) YBa2Cu3O7 α = 0.2 Gaussian χ” 1500

(A)

(B) (C) 1000

100

200 T(K)

300

Fig. 5.6. Plots of the ratio 17 Wc (T )/89 Wc (T ) vs. T for 100 K ≤ T ≤ 300 K calculated with the model susceptibility shown in (5.2.5) (Lorentzian case) in panel (a) and a Gaussian version in panel (b). The Gaussian is written as β exp(−q 2 ξ 2 ) and is centered at Q. The calculations are based on the ratios 63 Wc /17 Wc = 19 at 100 K and 10 at 300 K. Since the variation of 17 Wc (T )/89 Wc (T ) is roughly linear, straight lines are drawn between values calculated for the two extremal temperatures. Calculations are carried out for constant β and T-varying ξ (solid lines) and for constant ξ with β varying (dashed lines). The parameter sets used are listed in Table 5.4. The same parameters are used at 100 K, but then diﬀerent ones for 300 K. These calculated results are simply connected with a straight line. Reprinted ﬁgures from A. J. Millis and H. Monien, Phys. Rev. B45, 3059 (2005). Copyright 1992 American Physical Society

least a rough facsimile of those obtained in Chap. 3 and of those obtained from the UM ﬁt (Table 5.3). The coherence lengths appear to be similar, though it is not clear whether ξ from MMP can be directly compared with the λα ’s in Fig. 5.2(a). The trend with temperature is, of course, the same. trouble spot in this comparison is the variation of the integrated area One q χ (q, ω)/ω with temperature. For the UM picture, this simply goes as τeﬀ /T , while in the MMP case (i.e. from (5.2.5)) this area is very nearly equal to

178

5 Relaxation Models for Cuprate NMR

q

χ (q, ω)/ω

πχ [1 + βξ 2 ]. Γ

(5.2.9)

If the prefactor is independent of T as one might suppose for YBCO7, then the known behavior of τeﬀ (T ) from the UM ﬁts tells us that βξ 2 from the MMP model should be roughly constant. Thus, if ξ varies appreciably with T , β should vary inversely and twice as fast. This does not square well with the MM result. On the positive side of things, one could say that the results of the UM analysis would be an excellent starting point for someone setting out to model the mean-ﬁeld dynamic susceptibility as MMP did. As regards the possibility of accounting for cuprate T1 behavior with an RPA type of model where the q-dependence of χ (q, ω) (and thus ξ) has no temperature dependence, the UM analysis also gives a deﬁnite negation of any such possibility. Millis and Monien: Discussion of YBCO6.63 and of Neutron Scattering Characterization of χ (q, ω) MM analyze YBCO6.63 in a fashion similar to YBCO7. They note that rather larger values of 63 Wc /17 Wc indicate stronger AFM correlations in YBCO6.63, in accord with the UM result. As a result, they note that the constant-ξ option implies a somewhat larger increase in the ratio 17 Wc /89 Wc at lower temperatures, inconsistent with preliminary data available at the time. However, the subsequent T1 results of Takigawa et al., [15] showed an increase in the latter ratio of ∼ 20% below 300 K, which therefore cannot quite rule out the constant-ξ hypothesis. Again, the UM analysis of YBCO6.63, showing longer and more temperature-dependent correlation lengths in YBCO6.63, would preclude a ﬁxed-ξ scenario. One slightly troubling point about the MM discussion of YBCO6.63 is the assumption without justiﬁcation that χ0 in (5.2.5) be simply replaced by the gapped χ(T ) shown in Fig. 4.4 (or its equivalent). Some kind of assumption along these lines is evidently necessary for this model, but then leads to diﬃculties in accounting for 89 Wα (T ) and 17 Wα (T ), as was noted in Sect. 4.1.2. This played, unfortunately, into the weakness of employing the MMP model to deduce the temperature dependences of both ξ and β from NMR data alone. MM oﬀer a deep and useful discussion [5] of the behavior of χ (q, ω) at higher frequencies, with an eye to gleaning further insight about its characteristics from inelastic neutron scattering (INS) data. Again, speciﬁcally, would it be possible to determine the behavior of ξ(T ) from the width of the peak at Q? They note, with a detailed model example, that there is a tendency at typical INS frequencies for the measured peak width to appear independent of temperature while ξ is undergoing a signiﬁcant variation with T1 and that measurements must be conducted at very low energies to avoid this. There appears to be relatively little useful data from INS on the T-dependence of AFM peak widths in cuprates or on pseudogap eﬀects on χ (q, ω), the main exception to this being LSCO. If we take the INS results

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

179

of Tranquada et al. [23] as an example, the desired eﬀects are often masked by incommensurability. However, unknown at the time of MMP and MM, penetrating insights about pseudogap behavior in cuprates would come not from INS, but from ARPES (see a brief review of this in Sect. 4.2). This point will be considered further in Chap. 6, where extensive INS studies of LSCO will be discussed.

5.3 T1 Model for YBCO Using INS Data for χ(q, ω) In the ﬁrst two subsections of this chapter we saw how both UM and MMP interpreted cuprate relaxation data in terms of AFM ﬂuctuations with a temperature-dependent correlation length. In the present subsection we review a ﬁt procedure performed by the Berthier group, wherein T1 data from a YBCO6.9 sample are interpreted in terms of an AFM ﬂuctuation peak characterized by INS measurements [7]. INS data are quoted which show the AFM peak to have a constant width, i.e. the ﬂuctuations are interpreted to have a temperature-independent correlation length.2 Here we review the data and analysis for this interesting case, which also includes extracting dynamic susceptibility parameters from data for T2g , the Gaussian spin-echo decay from indirect spin-spin couplings (see Chap. 6). We compare this case with the UM ﬁts in Sect. 5.1 in some detail. In the end, it is found that they are strikingly similar, and that the contrast between them reﬂects a diﬀerence in samples rather than one of methods. When large single crystals of YBCO7 became available, extensive neutron scattering measurements were reported, e.g. by Regnault et al., [24], RossatMignod et al., [25], and by Tranquada, Sternleib et al., [23, 26]. NMR measurements on 63 Cu(2) and 89 Y in single crystals so characterized have been reported by Auler et al., [7], where they noted that the AFM peaks from INS data on their sample and related samples are well-ﬁtted by a Gaussian, with a peak width which is essentially independent of temperature. The sample of YBCO6.9 in question gave some indication of disorder in spite of being nearly fully oxygenated. This was attributed to the presence of Sr2+ as a dilute substitutional impurity for Ba2+ , leading to fairly broad NMR lines with ﬁeld ⊥ c axis [27]. However, the NMR measurements were conducted normally. The other apparent consequence of this was that the sample exhibited a somewhat pseudogapped character compared with other YBCO samples with Tc = 90 ± 1 K. The pseudogap eﬀect is noticeable in relaxation curves for 63 Cu(2) shown in Fig. 5.7, where the data are seen to roll oﬀ below T ∼ 125 K for both ﬁeld orientations. Furthermore, there is no visible break in the relaxation curve at Tc , which is a characteristic of pseudogapped material. On the other hand, the 2

The MMP picture did not rule this possibility out, but in the absence of reliable INS data favored the scenario with temperature-variable correlation lengths [5].

180

5 Relaxation Models for Cuprate NMR

20 H0 // ab 15 10

H0 // c

63(T

1

T)–1 (s–1 K–1)

25

NQR 5 0

100

200

300

T (K)

Fig. 5.7. Relaxation rate 1/T1 T for 63 Cu(2) in YBCO6.9 [7], showing typical anisotropy for YBCO7, but pseudogap-like rolling oﬀ of the data below 120-130 K. Note that there is no break or other feature in the data at Tc ∼ 90 K. Reprinted ﬁgure from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

ratio T1c /T1ab 3.7 at T ∼ 100 K and declines slightly at higher temperatures, which is typical behavior for YBCO7. This YBCO sample is therefore rather unique in having pseudogap features with Tc ∼ 90 K. Both NMR shift and relaxation data for the 89 Y nuclei are shown in Fig. 5.8. The NMR shift is seen to roll oﬀ at lower temperatures, much like one of the slightly deoxygenated samples in Fig. 4.2. Correspondingly, 1/T1 T in Fig. 5.8(b) is also seen to decline at lower temperatures, though not quite so much as for YBCO6.6 (see, e.g. Fig. 4.1(b)). Again, like the 63 Cu(2), the general character is that of a pseudogapped system. 5.3.1 The Gaussian Model Susceptibility The authors introduce their Gaussian susceptibility model as follows [7]. Beginning with the standard form (cf. (4.2.2)) χ (q, ω) χ (q, 0) = , (5.3.1) ω Γq ω→0 it is supposed that on account of AFM exchange forces χ (q, 0) is peaked at q ∼ Q, and the spin ﬂuctuation frequency Γq has a minimum at the same point. Further, it is assumed that χ (q) = χAF (Q) f (q − Q) and Γq−1 = −1 f (q − Q) have the same functional form in the vicinity of Q, which is ΓAF taken to be a Gaussian f (Δq) = exp(− | Δq |2 ξ 2 /4).

(5.3.2)

The value ξ = 1.3a is taken from INS measurements on the same sample material [7]. Then, if we put the origin in q-space at Q, we may write f (Δq)

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

181

–150 (a) (ppm)

–100

89K

–50 H0 // ab

0

H0 // c (b)

2

1

89(T

1T)

–1

(104 S–1 K–1)

50

0 50

100

150

200

250

300

T (K)

Fig. 5.8. (a) NMR shift data for 89 Y in YBCO6.9 from [7] for ﬁeld oriented both and ⊥ c axis. 89 Kα (T ) shows pseudogap-like decline below T ∼ 200 K. (b) Data for the 89 Y relaxation rate 1/T1 T for the same sample and conditions as in part (a) Reprinted ﬁgure from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

= exp[−0.4225 (qa)2]. As in the MMP model, a noninteracting, q-independent term χ0 /Γ0 is added to give the relations χ (q, ω) χ0 χ (Q) exp[−0.845 (qa)2] = + AF (5.3.3a) ω Γ0 ΓAF (Q) ω→0 χ (q) = χ0 + χAF (Q) exp[−0.4225 (qa)2] .

(5.3.3b)

The parameters in this model ((5.3.2) and (5.3.3)) were then extracted from experimental data. We give here just a brief summary of the procedure. χ0 (T ) was deﬁned to be the uniform susceptibility, the temperaturedependence of which is derived from NMR shift data in Fig. 5.8(a), where the orbital shift value 89 Kc,orb = 160 ppm is taken from [15]. The scale factor for χ0 (T ) was obtained by comparing shift coeﬃcients for 89 Y and 17 O with values from the literature [7]. The resulting curve of χ0 (T ) vs. T is shown in Fig. 5.9(a). In that same ﬁgure is shown the curve for χAF (T ). This was extracted from data for 63 T2g (T ), which is shown in Fig. 5.9(b), using the relations ⎡ 2 ⎤ 1 c63 ⎣ z (5.3.4) = (aind (q))2 − azind (q) ⎦ 63 T 2 8 2g q q

182

5 Relaxation Models for Cuprate NMR

with azind (q) =

γ63 χ (q) [Ac + 4B cos qx a]2 . gc2 μ2B

(5.3.5)

These formulas are derived and discussed in Chap. 6. Here, we simply note that the T2g data of Fig. 5.9(b) were analyzed with the foregoing equations to obtain the plot of χAF (T ) shown in Fig. 5.9(a).

χ′ (10–4 emu / mol Cu(2))

1,5 10

χ′AF (QAF)

1,0

(a) 5

0

χ0

100

150

0,5

250

200

0,0

T (K)

8 (T2g)–1 (ms–1)

4

10 Δ ν1/2

63

63(T

12

(b)

–1 2g)

(ms–1)

12

8

0 50

100

0

100

150

T = 120 K 200 300 1/τ (kHz)

200 T (K)

400

250

300

Fig. 5.9. (a) The susceptibilities χ0 and χAF are plotted as a function of temperature. χ0 is the uniform susceptibility, with temperature dependence and amplitude scale derived principally from 89 Y NMR shift measurements as discussed in the text. χAF is the amplitude of the AFM ﬂuctuation peak at Q. Its value as a function of temperature was derived from measurements of T2g for the 63 Cu(2) NMR line. Equations (5.3.4) and (5.3.5) were used to interpret T2g data shown in part (b) of this ﬁgure. See text and Chap. 6 for more details [7]. (b) Data for T2g on 63 Cu(2) taken in the present study [7]. These data were interpreted to yield the values of χAF shown in part (a) of this ﬁgure. See text and Chap. 6 for more details of interpretation. The inset shows how data vary with the bandwidth of the refocussing π-pulse of the echo sequence, where a large bandwidth is essential to obtain accurate data Reprinted ﬁgures from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

183

The ﬁnal step, which is to evaluate the spin ﬂuctuation parameters Γ0 and ΓAF as functions of temperature, requires a bit more explanation. Auler et al., [7] note that the dipolar interaction makes an appreciable contribution to 1/89 T1 , which is not taken account of by the “D” terms of the HF tensor (3.3.2). This point has been noted by Takigawa et al., [15] and was discussed brieﬂy in Sect. 4.1.2. Auler et al., provide a separate calculation to estimate the extra dipolar relaxation terms, which behave a bit like the 63 Cu(2) terms in that they do not cancel at q = Q. In evaluating Γ0 and ΓAF as functions of temperature, these authors present several “options” regarding the dipolar terms. We ﬁrst describe their procedure for obtaining the Γ ’s and then describe the options. The values of Γ0 and ΓAF are obtained by ﬁtting the 63 Cu(2) and 89 Y T1 data with the model susceptibility (5.3.3) with (5.3.2), using (3.5.11)-(3.5.14), i.e. the standard Mila-Rice HF Hamiltonian. As an example, these authors note that if the AFM susceptibility peak were narrow enough it would not make a signiﬁcant contribution to 1/89 T1 T , which would then be given by [7] 1 89 T

1T

=

2 2γ89 kB Dab gab μB Γ0 (T )

89

Kab (T ) ,

(5.3.6)

so that Γ0 (T ) could be extracted directly from the data for 89 Kab (T ) and T1 (T ). In practice, (5.3.6) is not a good approximation, but serves to illustrate the method. In general, one has to use the data mentioned plus 63 T1 (T ) to evaluate both Γ0 and ΓAF simultaneously. For this purpose they have used values of the 63 Cu(2) and 89 Y HF tensors, in units of 10−6 eV , as follows: Ac = -1.56 (-1.64), Aab = 0.35 (0.16); B = 0.39 (0.41); Dab = -0.0035 (-0.0028); and Dc = -0.0043 (-0.0035), where the values in parentheses are the ﬁtted values from the UM analysis in Table 4.1 for comparison. Apart from Aab , which is small and diﬃcult to evaluate, these are all quite reasonable. The values derived for Γ0 and ΓAF are plotted in Fig. 5.10(a) and (b), respectively. The down triangles are obtained ignoring the dipolar terms altogether, while the open circles correspond to taking the dipolar terms fully into account. For the up triangles the value of Aab was also increased by 25%. Our main concern here will be the open circles, which correspond to apportioning a sizeable fraction of the 89 Y relaxation to dipolar terms. Since the susceptibility model has an AFM peak with a temperatureindependent width, the temperature dependence of the T1 data has to be accounted for by assigning the temperature variation (of 1/T1 T ) to the susceptibilities χ0 and χAF and to the spin-ﬂuctuation parameters Γ0 and ΓAF . The value of Γ0 is seen to approximately double from 250 K down to 100 K and ΓAF to change by less than that. It is, of course, very diﬃcult to know whether this is a reasonable scenario from the standpoint of microscopic physics, but it describes the data well enough. What is interesting is to compare this outcome with the results of the UM analysis, for which a temperature-dependent correlation length ξ(T ) was employed (Sect. 5.1). 89

184

5 Relaxation Models for Cuprate NMR 400

Γ0 (meV)

(a) 200

0 (b)

ΓAF (meV)

40

20 T* 0

100

150

200

250

T (K)

Fig. 5.10. (a) Values of the spin-ﬂuctuation frequency Γ0 deduced from ﬁtting the relaxation data for both 63 Cu(2) and 89 Y to the form for χ (q, ω) (5.3.3) discussed in the text. Results from the oversimpliﬁed approximation in (5.3.6) are shown as solid squares. Open circles show values obtained when the dipolar terms for the 89 Y relaxation are taken into account, and down triangles show values obtained when they are not. The up triangles result when the dipolar terms are kept, and the value of Aab is increased by 25 % over that given in the text. See text for discussion. (b) Values of ΓAF (see (5.3.3)) obtained in same way as in (a), with symbols indicating the same cases listed there. Reprinted ﬁgures from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

5.3.2 Comparison with the UM Analysis Results for YBCO7 To eﬀect a comparison with the UM analysis, we use (3.5.17) and (3.5.18) to calculate τeﬀ and the Kij ’s, since χ (q, ω) is fully speciﬁed by (5.3.3) and (5.3.2) with the parameter values in Fig. 5.9(a) and Fig. 5.10(a) and (b) (circles). For these evaluations we use the other parameter values from [7], which were stated above. We ﬁrst note the contrast in parameterization of the Kij ’s between UM and the present work. We adopt a general form (5.3.7) Kij = K0 g(rij /λ) , where K0 and λ are both possible functions of temperature. In the UM analysis, K0 was taken to be unity and g(rij ) = exp(−2 rij /aλ), with all temperature dependence in the correlation length λ. For the Gaussian χ (q, ω) model of Auler et al., [7], however, the width parameter ξ is ﬁxed. The temperature variation has to reside in K0 (T ). Thus, it is possible to have temperature

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

185

varying correlations even when there is a ﬁxed correlation length. Calculations of the Kij ’s (see below) reveal that K01 (T ) reaches a value of –0.47 at 100 K and is about half that value at 250 K. These are typical numbers from the UM analysis. For comparison purposes the quantities τeﬀ (T) and the 63 Vα ’s have been evaluated using the model susceptibility parameters given by the analysis of Auler et al., described above. First, we evaluate τeﬀ (T) using (3.5.17) and (5.3.3), ﬁnding kB T χ0 χ τeﬀ (T ) = 2 + 0.0936 AF , (5.3.8) 4μB NA Γ0 ΓAF where the prefactor has been adjusted for susceptibilities in (emu/mole). Using the parameters from Fig. 5.9(a) and 5.10(a) and (b) (circles), we ﬁnd the values plotted in Fig. 5.11(a) vs. T (open squares). For comparison, The curves of τeﬀ (T) for YBCO7 (open circles) and YBCO6.63 (closed circles) from the UM analyses (Fig. 5.2(b) and 5.4(a), respectively) are plotted. Recalling that the YBCO6.63 curve was “gapped”, we see that there is a remarkably close correspondence in absolute magnitudes for τeﬀ and that the values from the present study are deﬁnitely “gapped” as well. As we noted earlier, the NMR shift and relaxation curves showed deﬁnite signs of a spin pseudogap. Corresponding to the foregoing expression for τeﬀ , we ﬁnd for the Kij ’s, Kij =

0.0936 χAF Γ0 [−0.745; 0.555; 0.309] , χ0 ΓAF + 0.0936χAF Γ0

(5.3.9)

where the numbers in the brackets represent K01 , K12 , and K13 , respectively. To plot 63 Vc and 63 Vab , this expression was used with interpolated data from Fig. 5.9(a) and 5.10(a) and (b) to calculate the 63 Vα ’s shown in Fig. 5.11(b) (ﬁlled squares for 63 Vc and ﬁlled diamonds for 63 Vab ). For comparison the same quantities for YBCO7 from the UM analysis (Fig. 5.3(a)) are plotted as solid lines. Again, considering that these materials are quite diﬀerent in detail, the correspondence is remarkably close. Notice that the three Kij ’s are in a constant ratio of -0.745:0.555:0.309 at all temperatures, but their coeﬃcient changes by about a factor two over 100 K≤ T ≤ 250 K. It seems, then, that there may be a variety of parameterizations which will give the same form for τeﬀ (T) and k Vα (T ), which is all that is needed to ﬁt the relaxation data. If follows that it will be very diﬃcult to work backward from such data to try to determine the details of some particular parameterization, as was the case with MMP. In ﬁrst-principles model theories such as those in the next two subsections, however, we suggest that it would be very useful and informative to calculate both τeﬀ and the Kij ’s as diagnostics.

186

5 Relaxation Models for Cuprate NMR 1.4 (a)

1.2

τeff (10–15 S)

1 0.8 0.6 0.4 0.2 0

0

50

100

150

200

250

300

200

250

300

T(K) 4.5 4

(b)

63Vα(1015s–2)

3.5 3 2.5 2 1.5 1 0.5 0

0

50

100

150 T(K)

Fig. 5.11. (a) Data for τeﬀ (T) have been calculated using (5.3.8) with interpolated data from Fig. 5.9(a) and 5.10(a) and (b) (open squares). These are compared with plots of τeﬀ (T) for YBCO7 (open circles) and for YBCO6.63 (dots), which have been calculated using (4.1.17) and (4.1.19) with parameter values form Table 4.2. Comparison shows a marked similarity with a clearly gapped character for the present YBCO6.9 sample. The main diﬀerence between the present case and the UM YBCO7 ﬁt is the marked pseudogap character of the results. (b) Plots of 63 Vc (ﬁlled squares) and 63 Vab (ﬁlled diamonds) for the same series of temperatures shown for τeﬀ in part (a). These quantities have been calculated with the HF parameter values from [7] given in the text using (5.3.9). Shown for comparison are the same quantities from the YBCO7 ﬁt by UM (Fig. 5.3(a)) (solid lines), where the discrepancy in both cases is a scale factor of order unity

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

187

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics Extensive model calculations of NMR shift and relaxation behavior have been performed by Bulut et al. [8], using the 2D Hubbard model to represent a cuprate-like system with enhanced magnetic ﬂuctuations near the AFM wavevector Q. These calculations with the Hubbard model bear some similarity to the mean-ﬁeld phenomenological model of MMP, the diﬀerence being that one is actually doing a ﬁrst-principles calculation of quasiparticle dynamics using a simpliﬁed Hamiltonian and approximate methods. The up side of this is that the results of such calculations have been adapted to realistic cuprate (i.e. Mila-Rice-Shastry) HF couplings and form factors to obtain shift and relaxation behavior which is not unlike typical experimental data. If there is a down side, it is that the 2D Hubbard model, as solved in this way, presents some rather quirky behavior with certain parameters which have no clear relation to microscopic physics. There is also some “implausible ﬁne tuning” of parameters to obtain desired behavior. The authors argue that this is simply a necessary aspect of using such a Hubbard model. In this section we present a brief summary of Hubbard model behavior and some calculated results for the NMR shift and relaxation of 63 Cu(2) and 17 O(2,3) sites of YBCO7. Behavior at T < Tc has also been treated in detail with these methods. The latter results will be presented in Sects. 5.7 and 6.2, along with other model results for the superconducting state. 5.4.1 Basic Formulation of the Dynamic Susceptibility The following is a summary and discussion of results for the square-lattice Hubbard model of a doped system with metallic behavior. For derivations the reader is referred to the original papers [8] and references therein. The basic Hamiltonian is + H = −t [c+ ni↑ ni↓ , (5.4.1) iσ cjσ + cjσ ciσ ] + U ijα

i

consisting of nearest-neighbor hopping terms and on-site coulomb repulsion, where U is actually a renormalized interaction parameter. The basic (U = 0) band proﬁle has width W = 8t with a logarithmic singularity at the center. The band ﬁlling is 0 ≤ n ≤ 2 particles per site. Near half ﬁlling there are commensurate and incommensurate spin-density wave phases, which must be avoided. For the assumed ratio U/W = 0.25, the critical value is nc = 0.865, above which there is an “unphysical phase transition” for the Hubbard model where U χ(q ∗ , 0) = 1. The amount by which n falls below nc determines the temperature T ∗ at which the amplitude of AFM ﬂuctuations saturates on lowering the temperature. Thus, n is only qualitatively related to the doping level parameter of the cuprate being modeled.

188

5 Relaxation Models for Cuprate NMR

The basic solutions to the Hubbard model (5.4.1) are as follows: The band energy is E(k) = −2t (cos kx a + cos ky a) and the single-particle density of states is 1 N (E) = K[(1 − (E/4)2 )1/2 ], (5.4.2) 2π 2 where K[ ] is the complete elliptic integral. The U = 0 (noninteracting) susceptibility is then given by χ0 (q, ω) =

f (Ep+q ) − f (Ep ) 1 , N p ω − (Ep+q − Ep ) + i0+

(5.4.3)

where f (Ep ) = 1/[exp(β(Ep − μ)) + 1] is the Fermi occupation function and μ is the chemical potential. For the interacting system the authors use the RPA to approximate χ(q, ω), giving χ0 (q, ω) , (5.4.4) χ(q, ω) = 1 − U χ0 (q, ω) closely analogous to (4.2.1). However, while (4.2.1) gave a peak near Q which dominated the behavior of interest or could be modeled with something else, here it was pointed out that the RPA approximation (5.4.4) does not accurately render the detailed dependences of K(T ) and 1/T1 on U and on the band ﬁlling n [8]. The best one can hope for is to choose U and n appropriately to extract the essential features of large-q spin ﬂuctuations. If we choose a band ﬁlling n near to but less than nc , then AFM ﬂuctuations will grow with declining temperature down to some point T ∗ where their amplitude saturates. T ∗ is controlled by the value of n. By choosing U/W = 0.25 and n = nc , the authors presented results for a case with large AFM enhancement eﬀects and a peak in χ (q, ω) near (but not precisely at) Q. The calculated NMR properties then give for the shift at low temperatures K=

N (μ) 2γe , A(0) γn 1 − U N (μ)

(5.4.5)

for a HF interaction parameter A(q), and for the relaxation rate 1 χ (q, ω0 ) kB T = A(q)2 , T1 N q ω0

(5.4.6)

where A(q) has the dimensions of frequency and χ (q, ω) of inverse energy (see (3.5.8)), and where the actual form of A(q) varies from site to site as usual. With the RPA susceptibility (5.4.4), (5.4.6) can be rewritten ! 1 |A(p − p )|2 kB T = , (5.4.7) T1 N [1 − U χ0 (p − p )]2 where the brackets indicate that p and p are to be summed over the Fermi surface.

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

189

The foregoing formalism has been used to calculate approximations to the NMR shift and relaxation behavior for 63 Cu(2), 17 O(2,3), and 89 Y in YBCO7. For this purpose calculations on the simple square-lattice Hubbard model have been generalized to include the eﬀects of Cu-O hybridization in a Hubbard model of CuO2 [8]. With a 3-center unit cell, the CuO2 lattice is modeled using “partial susceptibilities”, with coulomb repulsion only on the Cu site [8]. T1 calculations were presented with and without this modiﬁcation and, remarkably, the diﬀerences in T1 behavior were found to be fairly subtle. Here we present some of the results for each model. The NMR shifts at all sites undergo some Stoner enhancement according to (5.4.5), with very little temperature dependence. In Figs. 5.12 and 5.13, some of the T1 results are displayed, to be compared with experimental data for YBCO7. The bandwidth W is set at 1.2 eV, with U/W = 0.70, and n = 0.865, very near to the critical value. The ﬁeld is placed along the c axis. An on-site HF coupling form has been used for both the Cu(2) and O(2,3) for the ﬁrst two results shown. In Fig. 5.12(a), the relaxation curves for Cu(2) and O(2,3) are compared, where each is plotted as a fraction of its value at T /W = 0.025, which is approximately room temperature. The Cu(2) relaxation rate is seen to level oﬀ completely by room temperature, with rather more downward curvature than exhibited by the data (see Fig. 3.7), while the O(2,3) data also exhibit a slight downward curvature which is not unlike the experimental data (Fig. 4.9(a)). It seems that this extreme rollover of the Cu(2) relaxation is necessary in order to achieve the desired level of enhancement. The enhancement is shown for both Cu(2) and O(2,3) in Fig. 5.12(b), where the Korringa products (T1 T K 2 )−1 are plotted vs. T as fractions of the noninteracting values (T1 T K 2 )−1 = [(4π/kB )(γn /γe )2 ]. This gives an 0 enhancement of 4 for the Cu(2) and slightly greater than 1 for the O(2,3). The authors quote experimental values of 5.5 for Cu(2) and 1.4 for O(2,3) [12], in reasonable accord with their calculations. The Cu(2) enhancement, however, has declined to near the noninteracting value by just above room temperature, which is rather unlike the experimental results. Finally, we show in Fig. 5.13 a comparison of Hubbard model calculations with experimental data for 63 Cu(2) and 17 O(2,3) in YBCO7. For these calculations, the simple Hubbard model results were used [8] with realistic MilaRice-Shastry HF coupling form factors (i.e. | Aab /Ac | = 0.21 and | B/Ac | = 0.22), where we note that Aab is a bit larger here than usual estimates. In this case the Hubbard model parameters were also slightly diﬀerent from the foregoing, with U/W = 0.25 and n = 0.86 slightly below the critical value. Taken with the others, these calculations show that a fair range of T1 behaviors can be obtained with this model. 5.4.2 Remarks on the Hubbard Model Calculations One must, of course, evaluate the merits of this model in terms of the time frame of its development, in which case it was obviously highly successful. This

190

5 Relaxation Models for Cuprate NMR 1.2

1.0

ε / W = 0.7

(a)

U/W = 0.7 nh = 1.165

0.8 T1–1 T1–1(0.025)

0.6

0.4 Cu U = 0 Cu RPA O RPA

0.2

0.0 0.000

0.005

0.010

0.015

0.020

0.025

T/ W 10

ε / W = 0.7 U/W = 0.7 nh = 1.165

(b)

8 Cu O

6 (T1TK2)–1 (T1TK2)0–1 4

2

0 0.000

0.005

0.010

0.015

0.020

0.025

T/ W

Fig. 5.12. (a) Relaxation rates 1/T1 calculated for the Cu(2) and O(2,3) sites in YBCO7 and scaled to their values at T /W = 0.025 (approx. 300 K) are plotted vs. T /W . Calculations are made with the CuO2 model described in the text and references, using on-site HF couplings. The U = 0 (dashed) curves are also shown for reference. Conditions shown are E = 0, U/W = 0.7, and nh = 2 − n = 1.165, where E is the energy of the O(2pσ) orbitals where Ed = 0, and nh is somewhat above the critical value nh = 1.135. (b) The Korringa ratios for both Cu(2) and O(2,3) are plotted as a function of T /W in units of their noninteracting fermion values (4π/kB )(γn /γe )2 . The low-T enhancement ∼ 4 for the Cu(2) has decayed most of the way to its noninteracting, high-T limit by 300 K. Reprinted ﬁgure from N. Bulut, D. W. Hone, D. J. Scalapino, and N. E. Bickers, Phys. Rev. B41, 1797 (1990). Copyright 1990 American Physical Society

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

O Cu O Exp. Cu Exp.

1.5

60 1.0 40

(T1 –1)c (msec–1)

(T1 –1)0 (sec–1)

80

191

0.5 20

0

0

100

200

0.0 300

T (K) Fig. 5.13. Small-U Hubbard model calculations, similar to those for Fig. 5.12, have been applied to ﬁtting T1 data, where the Mila-Rice HF tensor given in the text has been used. Calculated T1 curves have been ﬁtted to 63 Cu(2) (+) and 17 O(2,3) (•) data curves from [12] and [28], respectively. The conditions are slightly diﬀerent from Fig. 5.12, with U/W = 0.25 and n = 0.86. Reprinted ﬁgure from N. Bulut, D. W. Hone, D. J. Scalapino, and N. E. Bickers, Phys. Rev. Lett. 64, 2723 (1990). Copyright 1990 American Physical Society

is a ﬁrst-principles model for the spin dynamics of superconducting cuprates which gives a remarkable facsimile of experimental behavior with a single dynamical variable. The model was also an important test for the use of suitable form factors to shield the O(2,3) sites from enhanced AFM ﬂuctuations while the Cu(2) sites are very directly aﬀected by them. That said, the authors note that this model probably cannot be made to give a truly quantitative account of the NMR data in the normal state. The physics of the high-temperature region is quite diﬀerent from an actual cuprate, which typically approaches the degeneracy temperature not far above room temperature. The Hubbard model spin dynamics will clearly be Korringa-like up to any experimentally attainable temperature, while it seems that the cuprates are making a transition to insulator-like dynamics at high temperatures. The latter result is illustrated by the behavior of τeﬀ (T) for several systems in Sect. 5.1. In spite of the apparent drawbacks, however, the authors went on to treat relaxation in the superconducting state with the Hubbard model, yielding very interesting results. The latter results are discussed in Sects. 5.7 and 6.2.

192

5 Relaxation Models for Cuprate NMR

5.5 The Large-U Hubbard Model of Si, Levin et al An RPA model of cuprate quasiparticle dynamics, which is of the same class of models as the MMP mean-ﬁeld model [4, 5] and the small-U Hubbard model of Bulut et al., [8], has been developed and discussed extensively by Si, Levin, and co-workers [9, 29, 30, 31]. This is a 3-band Hubbard model with U essentially inﬁnite, wherein the nearest-neighbor AFM exchange from combined O2− –mediated superexchange plus RKKY sources is incorporated using the RPA approximation. Thus, it is similar to the foregoing models, except that the authors report that they have microscopically derived the Lindhard (noninteracting) susceptibility. As we shall see, this is not only a ﬁrst-principles calculation, but one with entirely realistic physical parameters. Here we will comment very brieﬂy on their results, and discuss a comparison with INS data and with T1 curves for 63 Cu and 17 O nuclei in the CuO2 planes. We suggest below that further calculations with this theory would be very interesting. The interesting diﬀerence between this model and those mentioned in previous subsections is that on a decrease in doping level, the system nears a localization transition rather than a magnetic (AFM) one. Moreover, owing to strong coulomb correlation eﬀects, the renormalized antibonding band narrows as the insulating limit is approached. Thus, the principal bandwidth parameter tpd → tpd (1 − nd )1/2 , where Mott localization occurs as the electron concentration nd → 1. The latter eﬀect, then, lowers the coherence temperature at which Fermi liquid behavior gives way to temperature-independent relaxation. In cases under consideration, this has been estimated to occur at a few hundred Kelvin [9, 29, 30]. Evidence for such eﬀects is clearly present in the Uldry-Meier analysis of cuprate T1 data in Sect. 5.1. For example, in Table 4.2 the eﬀective degeneracy temperature for YBa2 Cu4 O8 (Y248) is seen to be as low as 420 K. It would be very interesting if the large-U, tight-binding, Hubbard model calculation could account for this eﬀect. Extensive calculations of dynamical susceptibilities have been made with the method described [31]. These results may then be compared with INS data and with T1 data for both the 63 Cu and 17 O nuclei in the CuO2 plane. Plots of the structure factor S(q, ω) (i.e. χ (q, ω)) for two diﬀerent scans in q − space (see ﬁgure caption) are shown in Fig. 5.14(a) for YBCO7 and (b) for YBCO6.7.3 These results were calculated with the expression χrr (q, ω) = χ0rr (q, ω) +

χ0rd (q, ω)[−JH (q]χ0dr (q, ω) , 1 + JH (q)χ0dd (q, ω)

(5.5.1)

where the χrr ’s are “partial susceptibilities” [32], with r = p or d, χ0rr (q, ω) is the microscopically-derived Lindhard function [32], and JH (q) is the composite Cu-Cu exchange coupling, which is modeled here with 3

Similar results were also presented for LSCO. These are invoked in a discussion of that system in Chap. 6.

5.5 The Large-U Hubbard Model of Si, Levin et al

193

Q = (q,q)

0.2 0

T = II mev

q (r..u.) 0.3

0.5

0.7

S(Q,w) [arb. units]

T = 1 mev

0

0.2 S(Q*,w)

YBo2Cu3O7

Q = (q,q)

0.2

Q* = (1,qy) 2

T = 1 mev

Q* = (1,qy) 2

0.2 (a) 0 0.1

0.3

q Q = (q,q)

1

0.5 0.7 qy (r..u.)

0.9

T = II mev

q (r..u.) 0.3

0.5

Q* = (1,qy) 2

0.7 T = 1 mev

qy 0

Q* = (1,qy) 2

1

T = II mev

T = 1 mev

0

1

qy

0

Q = (q,q)

1

0 S(Q,w)

S(Q,w) [arb. units]

0.4

0 0.1

T = II mev

(b) 0.3 0.5 0.7 qy (r..u.)

0.9

Fig. 5.14. (a) Cross sections of S(q, ω) for YBCO7 are shown for ω = 15 meV, ﬁrst along the diagonal at T = 1 meV and 11 meV, and then along the qy axis for q = ( 12 , qy ) for the same two temperatures. (b) Cross sections of S(q, ω) for YBCO6.7 are shown for the identical set of conditions as in part (a). See the original papers for details of these calculations. Reprinted ﬁgures from Q. Si, Y. Zha, K. Levin, and J. P. Lu, Phys. Rev. B47, 9055 (1993). Copyright 1993 American Physical Society

JH (q) = J0 [cos qx a + cos qy a].

(5.5.2)

There is a critical value J0 = Jc , above which χrr (q, ω) is unstable. For YBCO7, J0 was taken to be 0.5Jc and for YBCO6.7 J0 = 0.7Jc , while the doping for these two was x = 0.18 and 0.36, respectively. For other details we refer the reader to [31] and [32]. Referring to the theoretical scan results in Fig. 5.14, plots of χ (q, ω) are shown for T ∼ 12 K and T ∼ 120 K. The AFM peak is commensurate and noticeably narrower for YBCO6.7, as expected. Although the authors emphasize the constancy of these results with temperature [31], the peaks in all cases seem somewhat lower and wider at 120 K, this eﬀect being incrementally greater for YBCO6.7. One can only imagine that at 300 K the peaks would be even wider, giving a palpable temperature dependence to the correlation lengths. Comparing these results with the INS data for reduced oxygen YBCO given by Tranquada et al., in Fig. 4.8 [23], there is some diﬀerence in peak shape, with the INS scan distinctly narrower. On the other hand, the INS crystal had a nominally lower doping level at x = 0.6 with Tc 50 K. The frequency of the measurement was ω ∼ 15 meV, while that of the calculation is 10 meV. All in all, one would say that the correspondence is satisfactory. The authors also use their results for χ (q, ω) to simulate relaxation rate curves for 63 Cu and 17 O as a function of temperature, using the same HF

194

5 Relaxation Models for Cuprate NMR

tensors as those employed by Bulut et al., in [8]. The results are shown for both compositions in Fig. 5.15 as temperature plots up to 360 K [31]. We make the following remarks about the nature and signiﬁcance of these results. •

•

•

•

Comparing these plots with experimental data (see Fig. 4.9), certain trends are seen to be qualitatively correct. The deviation from Korringa behavior is greater for the 63 Cu than for the 17 O, and greater for the YBCO6.7 than for the YBCO7. The amplitude trends are dramatically diﬀerent from the experimental data, where for 63 Cu, the experimental curves are intertwined so that YBCO6.7 rises above YBCO7 at T ∼ 150 K, but falls below YBCO7 at room temperature. For 17 O the curves are reversed, where experimentally (Fig. 4.9(a)), 1/T1 T for YBCO7 is relatively ﬂat and lying above the curve for YBCO6.7, which descends to a small fraction of its room temperature value at T = Tc ∼ 60–65 K. The latter circumstances arise, in part, because YBCO6.7 exhibits a spin pseudogap eﬀect in which the susceptibility, as well as 1/T1 T for the 17 O, decline at low temperatures ∝ exp(−Δ/kB T ), where Δ/kB = 104 K (see Sect. 4.1.2). The Hubbard model discussed here [31, 32] does not have this feature, so that comparison with YBCO6.7 data, especially at low temperatures, is not meaningful. A model of low-frequency spin ﬂuctuations for the case of a pseudogap has been given by Varma [33]. The authors have some concern that the 17 O results are not as Korringalike as the experimental data for YBCO7 and/or are not compatible with their calculation for 63 Cu. The straightforward answer to this is found in the Uldry-Meier analysis of T1 data, presented in Sect. 5.1. This type 3.5

3.5

(a)

2.5 2.0 1.5 YBa2Cu3O7

1.0 0.5 0

(b)

3.0 YBa2Cu3O6.7

(1/ T)0 [arb. units]

(1/T1)Cu [arb. units]

3.0

YBa2Cu3O6.7

2.5 2.0 1.5 1.0

YBa2Cu3O7

0.5 0

60

120 180 240 300 360 T(K)

0

0

60

120 180 240 300 360 T(K)

Fig. 5.15. (a) Relaxation rates 1/T1 for 63 Cu, calculated for both YBCO7 and YBCO6.7 using the results for χ (q, ω) shown in Fig. 5.14 and the HF tensor given by Bulut et al., [8], are plotted as a function of temperature [31]. (b) Similar calculated results are plotted vs. T for the case of planar 17 O, using the same methods. Reprinted ﬁgures from Q. Si, Y. Zha, K. Levin, and J. P. Lu, Phys. Rev. B47, 9055 (1993). Copyright 1993 American Physical Society

5.6 Relaxation via Orbital Currents proposed by Varma

•

•

•

195

of analysis was not, of course, available in the early 1990’s when the Hubbard-model calculations were being developed. The main signiﬁcance of the UM analysis is that it separates the dynamical from the quasiparticle spin-spin correlations (Kij from (2.5.17)–(2.5.18)) dynamical function (2.5.17) Xat (T ) = q [χ (q, ω)/ω]ω→0 . (The UM analysis uses the related parameter τeﬀ (T ) = (kB T /)Xat (T ).) Given a theory for χ (q, ω), then Kij and τeﬀ are straightforward quantities to evaluate. In the latter formulation, the 63 Cu and 17 O curves contain the same dynamical information, but very diﬀerent correlation eﬀects. The latter may be seen in Fig. 5.3(a) and (b). The experimental dynamical function for YBCO7 is shown in Fig. 5.2(b). Si et al., attributed the strong curvature of the 63 Cu 1/T1 curve to a coherence temperature [29]. This may be something of a misapprehension, since the curve is strongly aﬀected by T-dependent spin-spin correlations. The true picture of dynamical behavior with temperature would be given by τeﬀ vs. T . It would be most interesting to see whether this theory would provide an explanation for the ﬂattening oﬀ of dynamical ﬂuctuations at high temperatures, since at the present time there is no theory for this available. The large-U RPA model seems especially suited to this, because the band-narrowing eﬀect with hole dilution [9] is similar to what is observed in practice (see Table 4.2). We further suggest that the reason for the strong deviation from Korringalike behavior for the 17 O in Fig. 5.15(b) is that the corresponding peak in Fig. 5.14 has much wider wings than the INS-measured peak in Fig. 4.8. This situation is a bit like the Lorentzian vs. Gaussian models by MM [5], where the Gaussian model with steeper sides gives far less contribution to the 17 O(2,3) relaxation rate. The downward curvature of the plot of 1/T1 for the 17 O is probably mainly due to the dynamical correlation factor, leaving the impression that τeﬀ (T) may be nearly linear in T . Nonetheless, an actual evaluation of τeﬀ for diﬀerent carrier levels would answer a very interesting question about the large-U Hubbard model, namely whether it can account for the high-temperature transition in the dynamics seen in the experimental data, such as Fig. 5.2(b) and Fig. 5.4(b).

5.6 Relaxation via Orbital Currents proposed by Varma Up to this point only spin-paramagnetic T1 processes have been considered for the doped cuprate superconductors. However, in 1989 a somewhat radical idea was proposed for these systems, namely that for a certain class of charge excitations the polarizability has a term which obeys [34] " −N (0)(ω/T ) f or | ω |< T ImP˜ (q, ω) ∼ , (5.6.1) −N (0) sgn(ω) f or | ω |> T

196

5 Relaxation Models for Cuprate NMR

where N(0) is the one-particle density of states. Applying this marginal Fermi liquid (MFL) ansatz to magnetic processes at NMR frequencies ω0 kB T /, we have 2 N (0)ω0 χmf l (q, ω) = , (5.6.2) kB T where we have added the factor 2 /kB to make clear that this is dimensionally a correlation time. To apply this ansatz to an HF perturbation process, we suppose that there is a quasiparticle interaction term γn Hmf l I ·f (q) with a (dimensionless) q-dependence factor f (q). Then, by the usual argument ((3.5.8)–(3.5.9) this generates a temperature-independent T1 process 2 χmf l (q, ω0 ) 4γn2 Hmf 1 l kB T 2 = f⊥ (q)2 = 4γn2 Hmf f⊥ (q)2 , l N (0) T1 ω 0 q q

(5.6.3) where the second step used (5.6.2), and N (0) ∼ /EF is a correlation time. Such processes in metals would be very strong. It has already been noted that such a dynamic would not apply to spin ﬂuctuation processes in cuprates. However, it was subsequently proposed by Varma [10] that the MFL scenario could be applied to magnetic ﬂuctuations which result from circulating orbital currents, yielding a T1 process for the Cu(2) sites. Here we review the arguments leading to an estimate given for 63 T1orb [10]. The proposed T1 mechanism would operate via the orbital HF interaction (see (2.2.1)) Horb = I · M orb = iI · L/r3 = iI·r × ∇/r3 ,

(5.6.4)

where the local angular momentum operator L is associated with the Cu(2) site. Horb could then act to scatter quasiparticles from k + q/2 to k − q/2, where the squared matrix element for the relaxation process would be summed over k and q. However, since the occupied 3d wavefunction in the cuprates is thought to be purely dx2 −y2 , the orbital HF matrix element ∗ (r)

k + q/2 | M orb | k − q/2 = e−iq·r Uk+q/2

L Uk−q/2 (r), r3

(5.6.5)

(exp[i(k + q/2) · r]Uk+q/2 (r) is a typical Bloch function) will have no intrasite contribution ∼ forb γn μB r−3 , where forb is the orbital symmetry factor (see Fig. 2.9) and r−3 ∼ 6 a.u. for 3d electrons. Thus, for a dx2 −y2 ground state forb = 0. It is for this reason that the conventional orbital T1 mechanism, which is often predominant in d-band metals, is absent in the cuprates. The leading contribution to (5.6.5) will come from cross terms between the Cu(2) site and its oxygen neighbors. To show how this develops, the behavior of k + q/2 | Morb | k − q/2 was examined [10] for k ∼ 0 and small values of q. In this limit, Uk+q/2 (r) ∼ U0 (r) can be written 1 Ai,α (0) φ(r − Ri,α ) , U0 (r) = √ N i,α

(5.6.6)

5.6 Relaxation via Orbital Currents proposed by Varma

197

where α is summed over the three sites in the CuO2 unit cell, and i is summed over cells. The local wavefunctions are φ(r − Ri,α ) ∼ dx2 −y2 in a Cu(2) site and ∼ pσ = px,y on the oxygen neighbors. The phase factors Ai,α (0) = ±1 must be adjusted appropriately (see [10], Fig. 1). The principal HF ﬂuctuations from orbital currents will be along the c axis, which we label z. Since Lz φd (r) ∼ dxy for φdx2 −y2 at the origin, one must ﬁnd dxy -like symmetry on the oxygen neighbors. For small q the relevant term (5.6.5) becomes Lz q · rφp (r − Rn ) 3 φd (r), (5.6.7)

k + q/2 | Morb | k − q/2 i r n where n is summed over the neighbors. One can then choose the term from rφp (r − Rn ) which has xy symmetry to obtain a non-zero matrix element. There will evidently be a non-zero contribution from larger values of q as well. On the other hand it is argued that there is no corresponding non-zero Cu-O term if the origin is placed on the oxygen site. This is fairly obvious, because at r ∼ ˆix, Lz px ∼ py , and xpy is orthogonal to dx2 −y2 . So the orbital currents can produce a z-axis T1 ﬂuctuation, and possibly through the apical oxygens some smaller in-plane ﬂuctuations at the Cu(2) site, but not at the O(2,3) sites. To estimate the strength of the corresponding T1 process, we can write the orbital dynamical structure factor, in analogy with (3.5.4)–(3.5.7), as 1 T1orb

=

2 2 μB 2kB T γ63

Morb (q)Morb (−q)ω0 ω0 2 q

=

kB T ω0

63

A2orb

(qa)2 χmf l (q, ω0 ) ,

(5.6.8)

q

where 63 Aorb is γ63 μB / times the intersite matrix element from the righthand side of (5.6.7). To obtain the ﬁnal expression for T1orb the MFL ansatz correlation time (5.6.2) is modiﬁed by replacing the eﬀective quasiparticle scattering rate kB T / in the denominator by kB T / + 1/τ0 , where 1/τ0 is a disorder-generated scattering rate of the order of tens of degrees [10]. With this change, (5.6.8) then gives 1 kB T = 63 A2orb N (0) . T1orb kB T + /τ0

(5.6.9)

In applying this to cuprate relaxation data, we note that for T > 100 K (5.6.9) assumes a nearly constant value 1/T1orb 63 Aorb N (0). The HF parameter 63 Aorb is very diﬃcult to estimate from (5.6.7). The main contribution will come from the overlap region between the Cu(2) and O(2,3) sites, and is probably 1–2 orders of magnitude smaller than the 3d on-site orbital HF ﬁeld (see Sect. 3.2.3 and Table 3.4) Horb = 2μB r−3 3d ∼ 125 kOe/μB . From the UM analysis of Sect. 5.1 (Table 5.2) we estimate N (0) ∼ /kB TF

198

5 Relaxation Models for Cuprate NMR

8 × 10−15 s for YBCO7. In this case, taking an optimal symmetry factor forb = 0.6, we ﬁnd for the maximal, on-site orbital relaxation rate 1 2 2 = forb γ63 Horb N (0) = 3.8 × 103 s−1 . (5.6.10) T1orb opt This is ∼ 3 times the measured relaxation rate for YBCO7 at T = 100 K. The rate in (5.6.9) is estimated to be a few percent of (5.6.10) at most. Interestingly, the combination of (5.6.9) and spin-paramagnetic processes which vary as 1/T1 ∝ T have been shown to give a good account of 63 Cu(2) relaxation data for both YBCO7 and optimally-doped LSCO. These results are shown in Fig. 5.16, where they are compared with data from [13] and [35]. For the calculated curves in this ﬁgure 1/τ0 is taken to be 25 K and 100 K for YBCO7 and LSCO, respectively. The quantity 63 A2orb N (0) is taken to be ∼ 3 × 103 s−1 , which is very near the estimated upper limit for an orbital contribution. A ﬁnal point has to do with how the orbital relaxation would ﬁt into the scheme of T1 analysis described in earlier subsections of this chapter. Since the UM analysis in Sect. 5.1, for example, is internally consistent and is consistent with the Mila-Rice, spin Hamiltonian parameters derived from shift measurements in Chaps. 3 and 4, a contribution from 1/T1orb at the 10% 5

–1) –1 (msec CuT1,⊥

4

3

2 –1 (YBa Cu O CuT1,⊥ 2 3 6,9)

1

0

–1 CuT1,NQR (La1.85Sr0.15CuO4)

0

100

200 300 Temperature (K)

400

Fig. 5.16. Orbital relaxation rates estimated with (5.6.9) are compared with experimental data for YBCO7 [13] and optimally-doped LSCO [35] as shown. For the plotted curves 63 A2orb N (0) is taken to be 3200 s−1 and 2800 s−1 , and 1/τ0 is taken to be 25 K and 100 K for YBCO7 and LSCO, respectively. See text for discussion of these calculations. Reprinted ﬁgure from C. Varma, Phys. Rev. Lett. 77, 3431 (1996). Copyright 1996 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

199

level would pose no problem. To accommodate a larger contribution than that would pose something of a challenge to the internal consistency of our current thinking on T1 in the cuprates. The presence of orbital current ﬂuctuations in cuprates has now been veriﬁed by neutron scattering studies [36], so there is no doubt about their existence. Further, they appear to be closely associated with the pseudogap eﬀect. Whether these ﬂuctuations are observable via NMR (other than the well-known NMR pseudogap eﬀects reviewed in Chap. 4) remains to be established. An important theoretical step toward further elucidation would be a serious eﬀort to evaluate the intersite orbital matrix element in (5.6.7).

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

In Sect. 3.6 we saw how a straightforward adaptation of the RPA susceptibility model to the BCS formulation of nuclear relaxation by Monien and Pines [3] gave a good account of the NQR T1 (T ) for 63 Cu(2) at T < Tc (YBCO7). Following that pioneering work there were important developments on the experimental side. As shown in Fig. 3.11(b), there had been a serious discrepancy between high-ﬁeld NMR T1 data below Tc and that obtained with NQR. One suspected that, as was found for the V3 X compounds in Sect. 2.3.5 (see Fig. 2.13), relaxation by spin diﬀusion to the normal cores becomes appreciable in high ﬁelds. Thus, the precise scaling between T1 curves for 63 Cu(2) and 17 O(2,3) observed by Hammel et al., is strongly dependent on the applied ﬁeld [12]. In an eﬀort to determine the intrinsic relaxation times for 63 Cu(2), a careful study of the ﬁeld dependence of T1 below Tc in YBCO7 using oriented powder samples was conducted by Martindale et al., [37]. The results are as follows: For ﬁeld (i.e. quantization axis) along the c axis, T1 was measured in 8.31 T, 4.14 T, and 0 T (NQR). For ﬁeld ⊥ c axis, T1 was measured in 8.31 and 0.45 T. Measurements were conducted at a series of temperatures 20 K≤ T ≤ 100 K, with the results plotted semilogarithmically in Fig. 5.17(a). For H0 c axis, the variation of T1 with ﬁeld is substantial, where at 20 K and 8 T ﬁeld increases the relaxation rate by a factor ∼ 5. The ﬁeld dependence with the ﬁeld in the ab plane is measureable, but much smaller.4 In the remainder of the discussion, then, NQR data or data taken in very low applied ﬁeld will be preferred. In Fig. 5.17(b) 1/63 T1ab T , scaled to its value at Tc , is plotted semilogarithmically vs. T . It is seen to behave very nearly as 1 e−b(1−T /Tc ) , (5.7.1) 63 T 1ab T 4

The authors refer to the conclusion by Redﬁeld and Genack [38] that relaxation by diﬀusion to the normal cores in the vortex state is not physically viable. Further analysis of this problem by Furman and Goren seems to have restored the validity of such a T1 process [39]. Expermental evidence for it is, of course, very strong.

200

5 Relaxation Models for Cuprate NMR 101

(a)

63W 1

(ms–1)

100

H0 = 0.45T

10–1

H0 = 8.31T H0 = 0T

10–2

H0 = 8.31T H0 = 4.14T

10–3

0

20

40

60 80 100 Temperature (K)

120

140

100

63W

10–1 T / Tc

1a /

63W

1a(Tc)

(b)

H0 = 0.45T

10–2

H0 = 8.31T 10–3 0.0

0.2

0.4

0.6

0.8

1.0

T / Tc

Fig. 5.17. 63 Cu(2) relaxation data from the work of Martindale et al., [37]. (a) Semilog plot of 1/T1 for 63 Cu(2) (63 W1 ) vs. T in the range 0≤ T ≤ 100 K for YBCO7. Data are presented for diﬀerent values of applied ﬁeld, including NQR data for zero ﬁeld. The open symbols show data with ﬁeld (i.e., quantization axis) along the c axis, while ﬁlled symbols are for ﬁeld ⊥ the c axis. (b) Semilog plot of 1/T1ab T for 63 Cu(2) (63 W1a /T ), normalized to its value at Tc , as a function of T ≤ Tc . This plot illustrates the exponential behavior, as well as the weak ﬁeld dependence of 1/T1ab T below Tc . Reprinted ﬁgures from J.A. Martindale, S.E. Barrett, C.A. Klug, K.E. O’Hara, S.M. DeSoto, C.P. Slichter, T.A. Friedmann, and D.M. Ginsburg, Phys. Rev. Lett. 68, 702 (1992). Copyright 1993 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

201

with b ∼ 6. The c axis data exhibits similar behavior, except that it begins a bit more slowly and the coeﬃcient b is slightly larger. Over a decline in −1 63 −1 relaxation rates of a factor ∼ 300, the ratio 63 T1ab / T1c behaves as shown in Fig. 5.19(a). To discuss the curves and data presented there, however, we must ﬁrst review the calculations reported by Bulut and Scalapino [40, 41]. 5.7.1 χ (q , ω) for the Small-U Hubbard Model at T < Tc The calculations by Bulut et al., [8] of T1 behavior in the normal state based on χ(q, ω) =

χ0 (q, ω) , [1 − U χ0 (q, ω)]

(5.7.2)

where U is the coulomb repulsion renormalized due to particle-particle correlations, is discussed at some length in Sect. 5.4. This theory was ﬁtted to relaxation data by choosing U = 2t and band occupation number n = 0.86. Their treatment of the superconducting state with these same parameter values [40, 41] is discussed in this subsection. To model the dynamic susceptibility for T < Tc , these authors used the RPA form (5.7.2) with the “irreducible BCS susceptibility” given by [41] χ0 (q, ω) = f (Ep+q ) − f (Ep ) 1 1 Ep+q Ep + Δp+q Δp 1+ N p 2 Ep+q Ep ω − (Ep+q − Ep ) + iΓ 1 Ep Ep+q Ep + Δp+q Δp 1 − f (Ep+q ) − f (Ep ) Ep+q + 1− + − 4 Ep+q Ep Ep+q Ep ω + (Ep+q + Ep ) + iΓ Ep Ep+q Ep + Δp+q Δp 1 − f (Ep+q ) − f (Ep ) 1 Ep+q − − − 1+ 4 Ep+q Ep Ep+q Ep ω − (Ep+q + Ep ) + iΓ (5.7.3) In (5.7.3) the dispersion relation is Ep = (Ep2 +Δ2p )1/2 and Ep = −2t (cos pxa + cos py a) −μ, where μ is the chemical potential and Δp is the gap function. For Δp we will consider here the case of a d-wave form Δp (T ) = [Δ0 (T )/2](cos pxa − cos py a),

(5.7.4)

where a BCS temperature dependence is adopted for Δ0 (T ). There is a ﬁnite broadening parameter Γ (T ) to be speciﬁed below. Finally, the superconducting transition temperature was taken to be Tc = 0.1 t, where at T = Tc the 63 Cu(2) relaxation rate has approximately the correct value and degree of AF enhancement to correspond to YBCO7 at 100 K. In [41] this formalism was used to treat and discuss both s-wave and d-wave gap symmetries with diﬀerent choices of parameter values. Since this work was completed several years before d-wave symmetry was conﬁrmed for the

202

5 Relaxation Models for Cuprate NMR

cuprates through the observation of phase jumps at the boundaries of Josephson junctions [42, 43], at that time there were still many proponents of s-wave pairing. We shall not dwell on the s-wave case here, but will point out how convincingly the relaxation behavior argues in favor of d-wave pairing in this theory. The early work of Monien and Pines [3] discussed in Sect. 3.6 also weighed heavily on the side of d-wave. We ﬁrst look at the behavior of T1 as treated with this formalism [41]. The usual expression (4.2.7) kB T 1 2 χ (q, ω0 ) = | A(q) | (5.7.5) T1 4 q ω ω→0

is employed with with the Mila-Rice-Shastry HF tensors (4.2.8). To see how this model distinguishes s-wave and d-wave behavior, it is useful to consider how the quantity [χ (q, ω)/ω]ω→0 χ (q, ω) = 0 (5.7.6) ω [1 − U χ0 (q)]2 ω→0 behaves with temperature in diﬀerent regions of q-space. For the s-wave case, χ0 (q, 0) declines for all q values below Tc , so that the enhancement factor [1 − χ(q, 0)]−2 will decline for all HF tensors [41]. In contrast, for the d-wave case, χ0 (q, 0) is only suppressed for | q |≤ 1/ξsc , where ξsc is the superconducting correlation length. The region around Q = (π, π) is not suppressed because of the nodes in the gap. Thus, AFM ﬂuctuations persist into the SC state for the d-wave case. The other factor present in (5.7.6) is χ (q, ω) D0 (q) = 0 . (5.7.7) ω ω→0 Fig. 5.18(a) is a plot of how D0 (q) varies with temperature for a very small value of q, and in part (b) it is shown how it varies for q near to Q. In the s-wave case the two are very nearly the same, but for d-wave they are quite diﬀerent. This sets up a diagnostic where if we look at the ratio of T1 values for sites which depend very diﬀerently on q, there will be a large expected diﬀerence between predicted behavior for s-wave and d-wave. Comparison of RPA Calculations with T1 Data The authors have calculated and discussed T1 behavior for a number of cases of parameter values with both s-wave and d-wave gap symmetry. The contrast between these two symmetries is best displayed by taking the ratio of T1 values for cases which have diﬀerent degrees of dependence on ﬂuctuations near Q, as shown in Fig. 5.18. As was clearly illustrated by Takigawa et al., [44], T1ab for 63 Cu(2) is most strongly dependent on AFM ﬂuctuations, with a lesser

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

203

dependence for T1c , and very nearly zero dependence for the oxygen 17 O(2,3) relaxation T1O (for any axis). To illustrate the foregoing eﬀect, calculations and experimental data were presented for T1c /T1ab (63 Cu(2) in YBCO7) [40], which we reproduce in Fig. 5.19(a). Over a range of ∼ 3 orders of magnitude in relaxation rates, the variation of T1c /T1ab is relatively slight, but has a deﬁnite signature. The data shown are the low-ﬁeld measurements of Martindale et al., [37] (squares) reviewed above, and similar low-ﬁeld measurements of T1ab combined with low-ﬁeld NMR measurements (ﬁlled circles) and NQR (H = 0) measurements (open circles) of T1c [44], which give equivalent results. The theory curves plotted for s-wave (2Δ0 /kB Tc = 4 (dotted line) and 8 (dashed line)) are seen to drop slightly, then remain ﬂat, since there is no real distinction between the D0 (q) curves (Fig. 5.18). For the d-wave case (solid curve), however, the drop and then rise reﬂect clearly the diﬀerence in behavior of the respective D0 (q) curves in Fig. 5.18(a) and (b). The observed ratio in Fig. 5.19(a) is a very clear sign in favor of d-wave gap behavior, which appeared several years before d-wave symmetry was widely accepted for the cuprates. The ratio T1O for 17 O(2,3) to T1c in Fig. 5.19(b) is also clearly supportive of d-wave symmetry. The message here is somewhat muted, owing to the fact that no low-ﬁeld 17 O(2,3) T1 data were available at the time, so the entire data base for the latter plot is 7–8 T NMR data [12]. The latter circumstance would only aﬀect behavior at the low-temperature end, however, so the comparison with theory is for the most part justiﬁed. 1

1.5 s – wave d – wave

0.8

(b) D0(q)

(a)

1 D0 (q)

s – wave d – wave

q = (0.05π, 0) 0.5

0.6 q = (π, 0.9π) 0.4 0.2

0

0

0.2

0.4 0.6 T/ TC

0.8

1

0

0

0.2

0.3

0.6

0.8

1

T/ TC

Fig. 5.18. (a) The quantity D0 (q), deﬁned in (5.7.7), characterizes the variation in intensity of low-energy ﬂuctuations over the Brillouin zone. In part (a) this quantity is plotted vs. T /Tc at q = (0.05π, 0) for s-wave and d-wave gaps as shown. Here and in part (b), 2Δ0 = 3.52 kB Tc , and broadening Γ = 0.3Tc has been used to control the coherence factor singularity. (b) The quantity D0 (q) is plotted for the same parameters as in part (a), except that q = (π, 0.9π). A sharp contrast between s-wave and d-wave behavior is seen to occur. Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. B45, 2371 (1992). Copyright 1992 American Physical Society

204

5 Relaxation Models for Cuprate NMR 6 5

T1c / T1ab

4 3 2

(a)

1 0

0

0.2

0.4

0.6

0.8

1

0.6

0.8

1

T/ TC 0.4 0.2

T10 / T1c

1 0.8 0.6 0.4

(b) 0.2 0

0

0.2

0.4 T/ TC

Fig. 5.19. (a) For 63 Cu(2) in YBCO7, a plot of the ratio T1c /T1ab vs. T /Tc for temperatures in the superconducting state. The square symbols represent low-ﬁeld data from Fig. 5.17 [37]. The circles are data from Takigawa et al., [44], where the open circles represent T1c data taken using NQR (H = 0) and the closed circles represent data taken in a c-axis ﬁeld of 0.44 T. The data for T1ab were taken in a transverse ﬁeld of 0.44 T. See the text for an explanatory note on these measurements. The solid line is the calculated curve for a d-wave gap as described in the text, using 2Δ0 /kB Tc = 8. The other lines represent calculations with an s-wave gap assuming 2Δ0 /kB Tc = 4 (dotted) and 8 (dashed), respectively. (b) The ratio of the 17 O(2,3) relaxation time T1O and T1c (for 63 Cu(2)) is plotted vs. T /Tc as in (a), but with plotted data scaled to their value at Tc . The data are from Hammel et al., [12] and were measured in ﬁelds of 7–8 T. The calculated curves correspond to the same set of cases as in (a). Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. Lett. 68, 706 (1992). Copyright 1992 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

205

It is interesting to note that a simple modiﬁcation of the analysis would make the displayed eﬀect in Fig. 5.19(a) somewhat more dramatic. This is suggested by the method of T1 measurement employed by Takigawa et al., [44], in which they write 1 1 = Jab + Jc ; = 2 Jab , T1ab T1c

(5.7.8)

where the Jα ’s are terms corresponding to HF ﬂuctuations along the α axis.5 With ﬁeld applied ⊥ to the NQR principal axis to measure T1ab , a complex set of terms occurs in the relaxation process. Thus, Jc (T ) and Jab (T ) are actually measured separately. Compared with T1c /T1ab , a plot of Jab /Jc [44] would show a more striking contrast between s-wave and d-wave. Finally, it is interesting to simply compare an RPA calculation of T1c (T ) for T < Tc [41] with NQR data attributed to Takigawa, Smith, and Hults [44]. These results are shown in Fig. 5.20(a), where the experimental points are open circles and the calculation is shown as a solid line. The data points are seen to drop very steeply below Tc , then approach a T 3 behavior (dashed line), as expected for a d-wave gap. The RPA calculation gives a very good account of this behavior [41].

RPA Theory for the NMR Shift below Tc Bulut and Scalapino also calculated the NMR shift behavior with their model [40, 41], which is simply given by Ks (T ) ∝ χ(q → 0, 0) =

χ0 (q → 0, 0) . 1 − U χ0 (q → 0, 0)

(5.7.9)

There is also a temperature-independent Van Vleck shift term, which renders the zero of Ks (T ) a bit uncertain. This has been subtracted oﬀ in the data plot of Fig. 5.20(b). The data shown are for 63 Cu(2) by Barrett et al., [16] (crosses) and 17 O(2,3) by Takigawa et al., [45, 46] (circles). All data are scaled to their total estimated excursion between Tc and 0 K. Theoretical curves are shown for U = 2t and several values of the d-wave gap parameter 2Δ0 /kB Tc . As the authors note [41], the lowest-temperature value is very important here. If the curves had been least-squares ﬁtted to the two sets of data, it appears that the dashed curve (2Δ0 /kB Tc = 6) would have been an excellent ﬁt. The distinction between Ks (T ) for s-wave and that for d-wave is that for d-wave the curve approaches T = 0 with a ﬁnite slope, but with zero slope for s-wave [41]. The data are certainly consistent with a ﬁnite slope, although 5

This is the same procedure as that used in the UM analysis of Sect. 5.1., where the Uα ’s deﬁned there are the same as the present Jα ’s.

206

5 Relaxation Models for Cuprate NMR

log10[T1–1(T)/ T1–1(Tc)]

0

(a) –1

–2

–3 –0.8

–0.6

–0.4 –0.2 log10(T/ Tc)

0

0.2

1.2 2Δ0 = 3.52KTc

1

2Δ0 = 5.0KTc 2Δ0 = 6.0KTc 2Δ0 = 3.52KTc

Ks(T)/Ks(Tc)

0.8 0.6

(b) 0.4 0.2 O(2,3) 0 –0.2

Cu(2) 0

0.2

0.4

0.6 T/ Tc

0.8

1

1.2

Fig. 5.20. (a) The c-axis relaxation rate T1c for 63 Cu(2), scaled to its value at Tc , is plotted logarithmically vs. T /Tc . The data are attributed to Takigawa, Smith, and Hults [44]. The relaxation rate drops sharply below Tc , then falls very nearly as T 3 (dashed line). The solid curve shows the RPA theory calculation for the d-wave case with U = 2t and 2Δ0 /kB Tc = 8. (b) The behavior of the NMR shift Ks (T ), scaled to its value at Tc , is plotted for 0≤ T /Tc ≤ 1. The crosses with error bars are 63 Cu(2) data from Barrett et al., [16], and the open circles are 17 O(2,3) data from Takigawa et al., [45, 46]. The lines plotted are calculations for a d-wave gap with U = 2t and various values of Δ0 as shown. Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. B45, 2371 (1992). Copyright 1992 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

207

the scatter is large enough so that s-wave is not ruled out. All in all, the shift results are a nice complement to the T1 data. The two together make a very strong case for d-wave symmetry. 5.7.2 T1 and Spin-Spin Correlations below Tc : The UM Analysis In this ﬁnal subsection we consider the behavior of T1 below Tc from another standpoint, one which does not employ any particular microscopic model of the spin dynamics, but relies only on the general formulation of the T1 process involving χ (q, ω) and the Mila-Rice HF Hamiltonian (3.3.2) (see Sect. 3.5.3). This, of course, is the basic premise of the Uldry-Meier analysis of cuprate T1 data presented in Sect. 5.1. These authors and co-workers have also employed this approach to discuss the behavior of spin-spin correlations above and below Tc and have come to two remarkable conclusions [47]. First, they ﬁnd that inplane spin-spin correlations vanish as T → 0 in a fashion roughly symmetrical to how they vanish at high temperatures. Secondly, they give evidence that it is only the in-plane correlations which vanish, while the c-axis correlations remain basically unchanged below Tc . To review the UM formulation, relaxation of the k th nuclear spin species quantized along the α axis is written (see Sect. 5.1) 1 kT

1α (T )

= [k Vβ (T ) + k Vγ (T )] τeﬀ (T ) ,

(5.7.10)

where (α, β, γ) are a permutation of the axes (a,b,c) and k Vα (T ) is expressed in α terms of the HF constants and the correlation functions Kij (T ). For example, 17 for O(2,3) one has 17

Vα (T ) =

1 2 α C [1 + K01 (T )] , 22 α

(5.7.11)

α where we emphasize that the Kij were allowed to be anisotropic. For YBCO7 c ab it was found, for example, that the Kij were ∼ 20% larger than the Kij (see Fig. 5.2(a)).

Behavior of ab Plane Correlations In this same notation we also have (5.1.4) 63

Vα (T ) =

1 α α α [A2 + 4 B 2 + 8 Aα BK01 (T ) + 8 B 2 K12 (T ) + 4 B 2 K13 (T )] . 42 α (5.7.12)

Thus, 17

T1c = 63 T 1c

2 2 2 63 Vab (T ) =⇒ Aab + 4 B K →0 ij 2 17 V (T ) + 17 V (T ) Ca2 + Cb a b

(5.7.13)

is purely a function of in-plane correlations, approaching the value on the right as they vanish.

208

5 Relaxation Models for Cuprate NMR

Several sets of low-ﬁeld data for 17 T1c /63 T1c are plotted in Fig. 5.21(a) as a function of T /Tc for 0 ≤ T /Tc ≤ 4.5 for YBCO7 [17, 48, 49, 50] (see ﬁgure caption for details) and for Y248 [51]. Since the only temperature dependence for this ratio comes from the Kij (T )’s, what the ﬁgure shows is that correlations are small at the highest temperature, grow as T is reduced until they ab (Tc ) ∼ -0.4, and then decline again toward zero at low reach a peak value K01 temperatures. The dashed line in this plot shows the value of 17 T1c /63 T1c for ab Kij = 0 (5.7.13), evaluated with numbers from the UM ﬁt to YBCO7 data (Table 5.1). This line is seen to be in very good agreement with the high and low-temperature limiting values of the experimental T1 ratio. The shaded triangles in Fig. 5.21(a) show the same plot for Y248, taken from the results of Bankay et al., [51]. There we see that the correlation eﬀects are more than twice as great as in YBCO7 and do not seem to be very much aﬀected by the spin pseudogap, which has quite a powerful eﬀect on τeﬀ for ab this compound. It follows that the Kij (T )’s are not much aﬀected. Behavior of c-axis Correlations ab The foregoing results show that the ab-plane correlations Kij (T ) are strongly peaked at Tc in these systems and vanish at low temperatures T Tc . However, if one looks at the ratio T1c /T1ab for 63 Cu(2), the value of T1ab is strongly dominated by c-axis ﬂuctuations, for which 63 Vα (T ) is markedly dependent c on Kij (T ). What Uldry et al., found is that 63 Vα (T ) behaves as though the c Kij (T ) do not change appreciably below Tc [47]. Data for T1c /T1ab vs. T /Tc are plotted in Fig. 5.21(b), showing the variation of this ratio for both YBCO7 and Y248 [51]. Both sets of data were measured in low magnetic ﬁelds. In the normal state T1c /T1ab is fairly ﬂat for both of these compounds, with a value ∼ 3.7 for YBCO7 and ∼ 3.3 for Y248. Below Tc the data decline slightly, then rise to new maximum values, Y248 slightly higher than YBCO7. To discuss these data we use 63 Vc (T ) 1 T1c = 1 + 63 . (5.7.14) T1ab 2 Vab (T )

Data for T2G , to be deﬁned and discussed in Chap. 6, suggest that c-axis correlations do not change much below Tc [47]. If that were true, then the T1 ratio in (5.7.14) will have the value 12 [1 + 63 Vc (Tc )/63 Vab (Tc )] at Tc and the value 12 [1 + 63 Vc (0)/63 Vab (Tc )] at T = 0. For YBCO7, these values are obtained from the ﬁts and parameter plots from the original UM paper [11] (see Table 5.1 and Fig. 5.3). The resulting ratio values are plotted in Fig. 5.21(b) (open circles), where they are seen to be in good agreement with the YBCO7 data. To evaluate T1c /T1ab for Y248 one needs a special procedure, because the magnitude of the correlations at Tc is not known from experimental data. The asymptotic, high-temperature value of T1c /T1ab 3.3 for 63 Cu(2) was obtained from the measurements of Bankay et al., [52]. However, it seems

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

209

70

R63c /17c = 63T1c–1/ 17T1c–1

60

(a)

50 40 30 20 10 0

0

2 T/ Tc

1

4

3

R63ab/63ac = 63T1ab–1/ 63T1c–1

7

(b)

6 5 4 3 2 1 0

0

0.2

0.4

0.6

0.8

1

1.2

T/ Tc

Fig. 5.21. (a) The ratio of 17 O(2,3) to 63 Cu(2) T1c values is plotted vs. T /Tc for YBCO (squares and circles) and for Y248 (shaded triangles). For YBCO7 the open circles are high-ﬁeld data from Yoshinari et al., [48], and ﬁlled circles are lowﬁeld data from Martindale et al., [49]. The ﬁlled squares denote data points where 63 Cu(2) data from Barrett et al., [50] are combined with 17 O(2,3) data from Nandor et al., [17]. The Y248 data are high-ﬁeld 17 O(2,3) data combined with NQR data for 63 Cu(2), both from Bankay et al., [52]. The dashed line is the model prediction ab = 0). (b) The ratio T1c /T1ab for for vanishing transverse AFM correlations (K01 63 Cu(2) is plotted vs. T /Tc for YBCO7 (ﬁlled circles) and for Y248 (ﬁlled triangles). The YBCO7 data are low-ﬁeld data from Takigawa et al., [44] and the Y248 data are low-ﬁeld data from Bankay et al., [52]. The dotted and dashed lines are normal state ratios from the same sources for YBCO7 and Y248, respectively. The open symbols are corresponding predictions from UM model calculations at Tc and at 0 K, which are obtained as described in the text. Reprinted ﬁgures from A. Uldry, M. Mali, J. Roos, and P. F. Meier, J. Phys. Condens. Matter 17, L499 (2005). Copyright 2005 I.O.P

210

5 Relaxation Models for Cuprate NMR

α unlikely that this corresponds to Kij ∼ 0. From ﬁt results for YBCO7 [11], if α α Kij = 0, one has T1c /T1ab 2.75. For Y248, then, the values of K01 were estimated from the ﬁt values for YBCO6.63, arguing that these two compounds ab (Tc ) -0.53 and have similar carrier densities and pseudogaps. Taking K01 c K01 (Tc ) -0.61 from data ﬁts for YBCO6.63 [11], they obtained T1c T1c 3.00; 5.78 . (5.7.15) T1ab T =Tc T1ab T =0

These approximate values are plotted in Fig. 5.21(b) as open triangles, and are seen to correspond well with the data [47]. The point here is, of course, that these results give good evidence that the c-axis correlations do not decay at low temperatures. If the c-axis correlations decay to zero as T → 0, then according to (5.7.14) T1c /T1ab → 2.75 in Fig. 5.21(b) for both compounds. This value is below the dashed and dotted lines and is not in good accord with the data. Comparing this discussion with the analysis given by Bulut and Scalapino in Sect. 5.7.1, their Hubbard model gives a functional form for χ (q, ω) at low frequencies at T < Tc which they have used in eﬀect to evaluate the α (T ) (see (3.5.17) and (3.5.18)), and thus the behavior of T1c /T1ab vs. T , Kij etc. The major diﬀerence with the present analysis by Uldry et al., [47] is that χ (q, ω) for the Hubbard model is isotropic and would not predict the anisotropic correlation eﬀects seen here. Further, the Hubbard model with d-wave symmetry does not inhibit AFM correlations in the superconducting state. As we have seen from the analysis of this subsection, only the c-axis correlations survive below Tc , with in-plane correlations declining to zero as T → 0. Thus, with the simple analytic method pioneered by Uldry and Meier, important eﬀects have been uncovered which might never have seen the light of day through the usual process of theoretical modeling.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12.

F. Mila, T.M. Rice, Physica C157, 561 (1989) 159, 161, 173 B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 159 H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990) 159, 199, 202 A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 159, 172, 173, 192 A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 159, 172, 173, 174, 175, 178, 179, 192, 1 M. Horvati´c, C. Berthier, Y. Berthier, et al., Phys. Rev. B48, 13848 (1993) 159 T. Auler, M. Horvatic, et al., Physica C 313, 255 (1999) 160, 166, 179, 180, 181, 182, 183, 18 N. Bulut, D.W. Hone, et al., Phys. Rev. B41, 1797 (1990); Phys. Rev. Lett. 64, 2723 (1990) 160, 187, 188, 189, 192, 194, 201 J.P. Lu, Q. Si, J.H. Kim, K. Levin, Phys. Rev. Lett. 65, 2466 (1990) 160, 192, 195 C.M. Varma, Phys. Rev. Lett. 77, 3431 (1996) 160, 196, 197 A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 160, 166, 208, 210 P.C. Hammel, M. Takigawa, et al., Phys. Rev. Lett. 63. 1992 (1989) 161, 162, 189, 191, 199

References 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52.

211

R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 161, 162, 198 J.A. Martindale, P.C. Hammel, et al., Phys. Rev. B57, 11769 (1998) 161, 162 M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993) 161, 162, 166, 178, S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 162, 205, 206 V. Nandor, et al., Phys. Rev. B60, 6907 (1999) 162, 164, 166, 208, 209 V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 164 D. Pines, C.P. Slichter, Phys. Rev. 100, 1014 (1955) 166 F. Raﬀa, T. Ohno, et al., Phys. Rev. Lett. 81, 5192 (1998) 169, 172 N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 169, 172 I. Tomeno, T. Machi, et al., Phys. Rev. B49, 15327 (1994) 169, 172 J.M. Tranquada, et al., Phys. Rev. B46, 5561 (1992) 175, 179, 193 L.P. Regnault, et al., Physica C 235-240, 59 (1994); Physica B 213-214, 48 (1995) 179 J. Rossat-Mignod, et al., Physica B 192, 109 (1993) 179 B.J. Sternleib, et al., Phys. Rev. B47, 5320 (1993); Phys. Rev. B50, 12915 (1994) 179 M. Horvati´c, C. Berthier, Y. Berthier, et al., Phys. Rev. B48, 13848 (1993) 179 M. Takigawa, P.C. Hammel, et al., Physica (Amsterdam) 162-164C, 853 (1989) 191 Q. Si, J.H. Kim, J.P. Lu, K. Levin, Phys. Rev. B42, 1033 (1990) 192, 195 Q. Si, K. Levin, Phys. Rev. B44, 4727 (1991) 192 Q. Si, Y. Zha, K. Levin, J.P. Lu, Phys. Rev. B47, 9055 (1993) 192, 193, 194 Q. Si, J.P. Lu, K. Levin, Phys. Rev. B45, 4930 (1992) 192, 193, 194 C.M. Varma, Phys. Rev. B73, 155113 (2006) 194 C.M. Varma, P. Littlewood, et al., Phys. Rev. Lett. 63, 1996 (1989) 195 R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 198 B. Fauqu´e, et al., Phys. Rev. Lett. 97, 197001 (2006) 199 J.A. Martindale, et al., Phys. Rev. Lett. 68, 702 (1992) 199, 200, 203, 204 A.Z. Genack, A.G. Redﬁeld, Phys. Rev. Lett. 31, 1204 (1973) 199 G.B. Furman, S.D. Goren, Phys. Rev. B68, 064402 (2003) 199 N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 68, 706 (1992) 201, 203, 205 N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 201, 202, 205 J. Kirtley, C.C. Tsuei, et al., Nature (London) 373, 225 (1995) 202 D.H. Wollman, D.J. van Harlingen, et al., Phys. Rev. Lett. 74, 797 (1995) 202 M. Takigawa, J.L. Smith, W.L. Hults, Phys. Rev. B44, 7764 (1991) 202, 203, 204, 205, 206, M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 205, 206 M. Takigawa, P.C. Hammel, et al., Physica (Amsterdam) 162-164C, 853 (1989) 205, 206 A. Uldry, M. Mali, J. Roos, P.F. Meier, J. Phys. Condens. Matter 17, L499 (2005) 207, 208, 210 K. Yoshimura, T. Imai, et al., J. Phys. Soc. Japan 58, 3057 (1989) 208, 209 J.A. Martindale, S.E. Barrett, et al., Phys. Rev. B47, R9155 (1993) 208, 209 S.E. Barrett, J.A. Martindale, et al., Phys. Rev. Lett. 66, 108 (1991) 208, 209 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 208 M. Bankay, M. Mali, et al., Phys. Rev. B46, R11228 (1992) 208, 209

This page intentionally blank

6 Dynamic Susceptibility Studies for the Cuprates

In Chap. 3 and 5 we saw how the dynamic susceptibility has come to play a pivotal role in interpreting cuprate spin-lattice relaxation data and rationalizing the sharp contrasts in T1 behavior among sites in and near the CuO2 planes. The principal driving force in all of the magnetic phenomenology of the cuprates is clearly the AFM ﬂuctuation peak at or near Q = (π, π), which occurs in varying degrees of dominance depending in an inverse fashion on the degree of carrier doping. This scenario appears to be a unique property of doped Mott insulators. A second consequence of strong AFM ﬂuctuation eﬀects is the indirect spin-spin coupling between neighboring nuclear spins which is thereby induced. This eﬀect was recognized early on by Pennington et al., [1], shortly after which the Pennington-Slichter (PS) theory of indirect spin-spin coupling appeared, formulating this eﬀect in terms of the static, q-dependent susceptibility χ (q, 0). Equally important was the recognition that these couplings were responsible for a Gaussian spin-echo decay (T2g ) process which, with due care, could be measured experimentally [2]. In the ﬁrst section of this chapter we review the PS formulation and survey a range of experimental cuprate results and interpretations. The importance of indirect spin-spin couplings for cuprate magnetism research is that T2g (T ) oﬀers a second method of characterizing χ(q, ω). T2g has been shown (and we document in Sect. 6.1) to be a fairly direct measure of the key parameter χ (Q). It soon became de rigueur to measure T2g as well as the NMR shift and T1 in a cuprate NMR study. In this chapter we illustrate why this is the case. The connection between χ (q, ω) and χ (q, 0) is the rather tenuous one through the Kramers-Kronig (KK) relation. It is, of course, not tenuous in principle, but diﬃcult to implement experimentally, because it requires the entire frequency spectrum of χ (q, ω). In theoretical modeling, T2g through the KK relation becomes a constraint on model parameters. For example, Bulut and Scalapino have extended their calculations of dynamical properties using a small-U Hubbard model to the case of indirect spin-spin coupling (T2g )

R.E. Walstedt: Dynamic Susceptibility Studies for the Cuprates, STMP 228, 213–251 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 6

214

6 Dynamic Susceptibility Studies for the Cuprates

in the superconducting state. When compared with the data of Ohsugi et al., [3], the result was a dramatic conﬁrmation of d-wave gap structure below Tc for Y248. We review these developments at the end of Sect. 6.1. For a purely experimental implementation of the KK relation we turn to the case of optimally doped LSCO:x, x ∼ 0.15. For this system there has been an INS characterization of χ (q, ω) for eﬀectively all q values (in the ﬁrst BZ) and for all frequencies for which there is a substantial contribution. Moreover, the latter characterization is in absolute units, leading to a direct comparison between INS and T1 data with no adjustable parameters. The story of this ﬁrst-ever quantitative juxtaposition of quantitative INS and NMR data is recounted in detail in Sect. 6.2. A closely-related T2 study for both 63,65 Cu and 17 O is included as well, where a successful implementation of the KK integral has been reported. The points where INS and NMR data are clearly incompatible is also an interesting part of the story. An interesting interconnection between T1 , T2g , and the dynamic susceptibility components has been created by the dynamic scaling theories of Pines and co-workers. This topic is addressed in Sect. 6.4, where in the limit of long AFM correlation lengths ξ the two parameters ξ(T ) and the spin ﬂuctuation frequency ωsf (T ) appear to control the dynamical properties accessible to the NMR probe. In this context a high-temperature investigation of 63 Cu(2) static and dynamic NMR/NQR properties of YBa2 Cu4 O8 (Y248) by Curro et al., [4] has given evidence for a sharply-deﬁned crossover temperature (∼ 500 K) for the dynamical exponent (z = 1→2) in this system. These interesting developments are reviewed in detail, as well as suggestions for extension to other systems.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter Indirect couplings between nuclear spins are very strong in the cuprates [1]. As was ﬁrst demonstrated by Pennington and Slichter [2], these can be formulated in terms of the real part of the dynamic susceptibility χ (q, 0). χ (q, 0) can, in turn, be expressed in terms of χ (q, ω), so the estimation of χ (q, ω) (ω = 0) through measurements of the spin-echo T2 make the indirect couplings a powerful element in the NMR methodology for solids. In this section we give the derivation of the Pennington-Slichter result, which is straightforward, after which various applications of this result will be presented throughout the chapter. There are indirect couplings between any pair of neighboring nuclei in (or near) the CuO2 plane. We shall begin with the pertinent example of interactions among the 63,65 Cu nuclear spins. Although T1 can be formulated in terms of χ (q, ω) having the dimension of inverse energy (see discussion in Sect. 3.5), here we will use susceptibilities per mole, since χ (q, ω) becomes the measurable uniform, static susceptibility at ω = 0. We calculate the indirect coupling

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

215

of a 63 Cu with surrounding 63,65 Cu spins, an eﬀect which is mediated via the bath of ﬂuctuating electronic spins S i . It is driven by the HF coupling tensor HHF =

⎡ ⎣Aα Iiα Siα + B

α,i

⎤ Iiα Sjα ⎦ ,

(6.1.1)

j(nn)

where j(nn) is taken over the four nearest-neighbor spins to the site i. Through this HF Hamiltonian a spin polarization is created in the local environment by a nuclear spin I i located at Ri . The HF energy (6.1.1) can be written as an eﬀective ﬁeld Hiα (R) which this nucleus exerts on spin moments −gα μB Sα (R) in the vicinity. The ﬁeld is given by Hiα (R) =

Iiα Fαα (R, Ri ), with Fαα (R, Ri ) = [Aα δR,Ri + B δR,Rj ] . gα μB j(nn)

(6.1.2) The eﬀect of Hiα (R) on the surrounding medium can be calculated in terms of χ (q, 0), which we denote χα (q). The ω = 0 component is used, because in a metallic environment nuclear spin motion is very slow on the time scale of electronic spin ﬂuctuations. However, the ﬁeld driving χα (q) is the q–component of Hiα (R). One may write the Fourier transform Hiα (q) = k exp(−iq · Rk )Hiα (Rk ) in the form Iiα −iq·Ri e Fαα (q), with Fαα (q) = [Aα + 2B (cos qx + cos qy )]. gα μB (6.1.3) Hiα (q) then induces a q-component of spin moment Hiα (q) =

Sα (q) = −

1 Hiα (q)χα (q) , NA gα μB

(6.1.4)

where we divide χ (q) by Avogadro’s number for an atomic susceptibility. The inverse Fourier transform of Sα (q) gives the resulting spin polarization in the vicinity of Ri , i.e. Sα (R) =

q

eiq·R Sα (q) = −

Iiα iq·(R−Ri ) e χα (q)Fαα (q) , (6.1.5) NA gα2 μ2B q

where q is a normalized sum over the Brillouin zone. The interaction energy with a second nucleus I j may now be obtained by inserting (6.1.5) into (6.1.1), where we use the notation of (6.1.2) to ﬁnd aα (i, j)Iiα Ijα = Ijα Sα (Rk )Fαα (Rk , Rj ) . (6.1.6) α

α

Rk

216

6 Dynamic Susceptibility Studies for the Cuprates

Substituting from (6.1.5) then gives the general result [5] 1 eiq·(Rj −Ri ) χα (q)Fαα (q)2 . NA gα2 μ2B q

aα (i, j) =

(6.1.7)

Under suitable conditions the spin-spin interactions in (6.1.6) and (6.1.7) can be measured via the spin-echo decay time (T2 ) process, to be discussed in Sect. 6.1.3. The parameter controlling this process is the second moment contribution of the interaction (6.1.7). A useful relation for calculating the second moment of the line as well as the Gaussian decay time T2g of the spin echo may be derived using (6.1.7). This result, given independently by Takigawa [6] and by Thelen and Pines [7], is ⎡ 2 ⎤ 1 ⎣ [χα (q)Fαα (q)2 ]2 − aα (i, j)2 = χα (q)Fαα (q)2 ⎦ . 2 μ2 )2 (N g A α B q q j (6.1.8) 6.1.1 Some General Properties of the Indirect Spin-Spin Coupling We adopt a notation where q is dimensionless and Ri = (nxi , nyi ) in units of a, where nxi,yi are integers. We shift the origin of the q sum to Q, i.e. q = p + π π (π, π). Then χα (p) is a symmetric function, where p → (1/2π)2 dpx dpy , π

π

and Fαα (p) = [Aα − 2B(cos px + cos py )]. The exponential factor in (6.1.7) reduces to cos (nx px ) cos (ny py ), since the sine terms cancel by symmetry, where nx = nxj - nxi , etc. Thus, (6.1.7) becomes aα (i, j) =

(−1)(nx +ny ) NA gα2 μ2B

where Gα (nx , ny ) =

1 π2

n x +2

Cα (nx , ny )Gα (nx , ny ) ,

(6.1.9)

nx =nx −2 ny =ny −2

π

dpx 0

ny +2

π

dpy χα (p) cos(nx px ) cos(ny py ),

(6.1.10)

0

and where the Cα (nx , ny ) are functions of Aα and B. Some general properties of aα (i, j) are as follows: • • •

Terms in χ (q, 0) which are independent of q give no contribution to aα (i, j). The essential range function of a(i,j) is the Fourier transform of the peak function χα (q). A sign reversal on moving between nn sites results from the the AFM nature of the ﬂuctuations.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

• •

217

The range function depends only on the magnitudes of the nx,y and is invariant on exchange of nx and ny . Therefore aα (i, j) is symmetric about the x and y axes, and also about the x = ±y axes.

6.1.2 The Gaussian model of Indirect Spin-Spin Coupling in YBCO In the MM follow-up to MMP [8], a Gaussian model was suggested for χ (q, ω). Citing this example, Imai et al., [9] made use of this model in their interpretation of data for T1 and T2g (see below for deﬁnition of T2g ). More recently, Auler et al., [10] employed this model for similar purposes, citing INS studies which showed a Gaussian-like shape with a width essentially independent of temperature. Their interpretation of T1 data on this basis was presented and discussed in Sect. 5.3. INS data provide an important characterization of χ (q, ω), which is then used to interpret NMR data. An important question regarding INS data is to what extent they are dependent on the frequency scale. Does a peak in χ (q, ω) at or near Q with a certain measured width at ω = 10 meV have the same shape and width at an NMR frequency four orders of magnitude lower? With the limitations of current spectroscopic techniques one cannot answer this question experimentally. Many discussions of NMR T1 interpretation tacitly assume that the INS results will still be valid at NMR frequencies. We address this question in various contexts throughout this chapter. For the purposes of the present discussion we adopt the Gaussian shape and width for the AFM peak given by Auler et al.,: χα (q) =

gα2 −(qx2 +qy2 )ξ2 /4 χ e , 4 AF

(6.1.11)

with ξ 1.3, where we place the origin at Q = (π, π) and we denote χ (Q) = χAF . Inserting this into (6.1.10), a simpliﬁcation occurs, where we can write Gα (nx , ny ) = (gα2 /4)χAF g(nx )g(ny ), with g(n) =

1 π

0

π

2 2

dpe−p

ξ /4

2 2 1 cos(np) ≈ √ e−n /ξ . πξ

(6.1.12)

In (6.1.12) the result on the far right is obtained by extending the upper integration limit to ∞. Since exp(−π 2 ξ 2 /4) 0.015, we suggest that this is a reasonable approximation. Inserting this expression for Gα (nx , ny ) into (6.1.9), we ﬁnd, with nx = nxj - nxi , etc.,

218

6 Dynamic Susceptibility Studies for the Cuprates

aα (i, j) = (−1)(nx +ny )

2 2 2 χAF e−(nx +ny )/ξ {A2α + 4B 2 πNA ξ 2 gα2 μ2B 2

− 4Aα B e−1/ξ [cosh(2nx /ξ 2 ) + cosh(2ny /ξ 2 )] 2

+ 8B 2 e−2/ξ cosh(2nx /ξ 2 ) cosh(2ny /ξ 2 ) 2

+ 2B 2 e−4/ξ [cosh(4nx /ξ 2 ) + cosh(4ny /ξ 2 )]} .

(6.1.13)

Equation (6.1.13) is used below to calculate indirect coupling energies for YBCO6.9 and to discuss results which have appeared in the literature. Before that, however, we make a brief digression to introduce spin echo decay measurements. 6.1.3 Measuring Indirect Spin-Spin Coupling via Spin-Echo Decay Under suitably restrictive assumptions, it is possible to get good estimates of the indirect spin-spin coupling (6.1.7) by measuring spin-echo decay times. We give here a brief review of some of the essential points of spin-echo decay, followed by a discussion of results from the literature in the next subsection. We consider spin-echo decay for the speciﬁc problem of 63,65 Cu(2) NMR in the CuO2 planes of a cuprate superconductor. If the 63,65 Cu isotopes are labelled A and B, where the A spins are under observation, then the nuclear spin-spin coupling has the general form AA AB BB + HII + HII . HII = HII

(6.1.14)

For cases of orthorhombic symmetry or higher, the latter terms can be written AA A A A A A A AB A A αij Izi HII = Izj + βij Ixi Ixj + γij Iyi Iyj , and HII = αij Izi Izj , i>j

i>j

(6.1.15) AB the x and y terms where we have taken z to be the quantization axis. For HII have been omitted, because they are non-secular and have no measurable AA are secular, i.e. physically eﬀects. Whether or not the x and y terms for HII viable, is a matter of some discussion. In cases where there is no detuning of neighboring A spins, i.e., where locally, the Zeeman splitting γA (1 + K)H as well as quadrupolar splittings are homogeneous, then the x and y terms are technically viable. However, if the zz coeﬃcient αij is much larger than βij and γij (a realistic case as we shall see below), then “ﬂip-ﬂop” processes such as | mA , mB → | mA + 1, mB − 1 may become severely inhibited and the transverse terms become de facto nonsecular. Below, a simple test is suggested to determine the eﬀectiveness of the dynamical terms. For the moment we shall assume the ﬂip-ﬂop terms to be inoperative. This is a simple limiting case for which the spin-echo decay process has been calculated in Appendix A.1. Approximating the decay function with a Gaussian 2 ), then the echo decay time constant is found to be exp(−(2τ )2 /2T2g

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

⎤1/2 ⎡ c 1 63 = sin(θ2 /2) ⎣ α2 ⎦ , T2g 8 j ij

219

(6.1.16)

where c63 0.69, and the sum is over all neighbors. The dependence on refocussing pulse angle θ2 suggests an interesting test for the spin dynamics of the sample. If the spins are completely static on the time scale of the echo sequence, then T2g should become correspondingly long when θ2 is small. If T2g does not change a great deal over a range of values for θ2 , it probably means that there is an appreciable degree of ﬂip-ﬂop motion taking place among the spins. 2 In applying (6.1.16) to actual measurements of j αij , it is clearly necessary to be able to ﬂip over nearly all of the spins with the θ2 pulse. This is an important constraint on experimental technique. For cuprates this means that one will probably have to employ only the (−1/2 ↔ 1/2) transition, and possibly work at low ﬁelds in addition in order to narrow the line. 6.1.4 Behavior and Interpretation of Indirect Couplings in YBCO and Y248 There have been a number of measurements of T2g for both YBCO and Y248 in the literature, with much discussion of its behavior as compared with T1 . Since they are both driven, at least in part, by AFM ﬂuctuations, these relaxation times are reﬂections of the same underlying quasiparticle physics. Thus, the advent of T2 g as an additional characterization of cuprate hole dynamics was a most welcome development. Results Given by Pennington and Slichter In their original paper formulating the indirect couplings, expounded in the previous subsection, PS [2] presented calculations of coupling coeﬃcients aα (i, j) as well as of T2g for fully oxygenated YBCO7. They calculated their range function using the MMP Lorentzian form (ξ/ξ0 )2 ) χ (q) = χ0 1 + (6.1.17) 1 + (q − Q)2 ξ 2 centered on Q. The ξ 2 factor gives only a rough normalization for χ (q), since q χ (q) depends on ln(ξ). The resulting relaxation time is found to vary 1/T2g ∝ ξ [2]. The parameters and assumptions for various calculations of T2g discussed here are shown in Table 6.1. Adopting the MMP estimate [11] ξ = 2.5 a, the half-width of the AFM peak in the PS calculations with (6.1.17) is 0.4. Also from (6.1.17), χ (Q) = 1.66 × 10−3 emu/mol Cu(2). With values of Ac and B as shown in Table 5.1, PS ﬁnd a value of 1/T2g which is just slightly smaller than their experimental number, which clearly validates their formulation of the indirect spin-spin coupling.

220

6 Dynamic Susceptibility Studies for the Cuprates

Table 6.1. Models, data, and results for c-axis indirect coupling values of 1/T2g are presented from various sources for diﬀerent doping levels in YBCO. The ﬁrst line gives the original results of Pennington and Slichter with a Lorentzian model. HF parameters vary only slightly between calculated results given. Experimental data in the ﬁnal column corresponds generally to 100 K. Under “Source”, Imai and Auler are ﬁrst authors, as are Bulut and Itoh. The Takigawa reference is [6]. For Imai et al., and Auler et al.,, the estimated values of 1/T2g have been made using (6.1.13) and direct summation to give j ac (i, j)2 . For the Takigawa estimate, which was made with a Lorentzian model, the PS result is simply scaled to the larger value of χ (Q) shown. The units of parameters given are as follows: Ac and B (10−6 eV ); χ (Q) (10−3 emu/mol); 1/T2g (ms−1 ). These results are discussed extensively in the text System

Source

χ (q) Form

H.W.(a−1 ) Ac

B

χ (Q) (1/T2g )est (1/T2g )exp

YBCO7 YBCO7 YBCO7 YBCO6.9 YBCO6.9 YBCO6.63

PS[2] Bulut/Itoh Itoh(c63 = 1) Imai[9] Auler[10] Takigawa

Lorentzian Hubbard RPA Hubbard RPA Gaussian Gaussian Lorentzian

0.40 0.5 0.5 0.37 1.28 0.40

0.38 0.38 0.38 0.45 0.39 0.38

1.66 1.23 1.23 3.28 1.41 6.14

-1.53 -1.53 -1.53 -1.77 -1.56 -1.53

5.26 9.0 10.8 9.2 7.5 19.5

7.7 11.1 12.9 9.6 11.5 18.4

Eﬀects of Transverse Coupling and of Dipolar Fields Before proceeding with discussion of experimental data, we note in passing that transverse and dipolar coupling contributions to Hzz are much smaller and can be ignored for most purposes. The dipolar coupling coeﬃcient for 2 3 quantization axis ⊥ CuO2 plane is simply αdip c (i, j) = γ /Rij , which has −1 63 the value 908 s for nn Cu(2). The corresponding second moment value is less than 6% of the estimated indirect coupling value calculated above. Moreover, it has a constant positive sign for all in-plane neighbors, so that its eﬀects tend to cancel when combined with the staggered indirect coupling. We shall ignore the dipolar terms from this point forward. The transverse indirect coupling terms are also much smaller than the c-axis contribution, giving a second moment only 15% of the latter eﬀect using Aab ∼ 0.31 in the units of Table 6.1, with B having the same value as for the c-axis terms. As far as we are aware, no eﬀort has been made to measure the transverse terms, and we shall not discuss them further. Comparison of the PS Results with Other Models and Data Throughout the derivation of indirect spin-spin coupling given above [2], it is assumed that the resulting spin-echo decay process will be Gaussian in form or nearly so. Itoh et al. have tested this hypothesis for the case of NQR studies of 63 Cu(2) in Y248 [12]. Their results are plotted in Fig. 6.1(a) and (b) for several temperatures. After corrections for T1 eﬀects (see Appendix A.3), it is seen that these decay curves exhibit nearly perfect Gaussian character over two orders of magnitude. Some discussion of the origin of such Gaussian behavior, which is very widespread in T2g studies, is presented in Sect. 6.3.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter 1.0

221

(b)

(a)

E(2τ)/E(0)

280K 0.1 4.2K 0.01 100K 0.001 0

242 (2τ)2/102μsec2

484 0

98

196

(2τ)2/102μsec2

Fig. 6.1. (a) and (b) Spin echo decay curves, corrected for T1 eﬀects, are plotted semilogarithmically vs. (2τ )2 , showing nearly perfect Gaussian behavior over two orders of magnitude of decay at several temperatures. These are data for 63 Cu(2) in YBa2 Cu4 08 . Reprinted ﬁgures from Y. Itoh, H. Yasuoka, et al.,, J. Phys. Soc. Japan 61, 1287 (1992). Copyright 1992 Physical Society of Japan

In the second line of Table 6.1 we list the calculated result of Bulut and Scalapino (BS) based on their small-U Hubbard model calculations [13] along with experimental numbers from Itoh, Yasuoka et al., [12]. BS calculated the indirect coupling using the same model and parameters they had applied to the T1 problem [14, 15], ﬁnding good agreement with experimental data with an AFM peak width ∼ 25% greater than that used by PS. Itoh et al., also tested the proportionality of 63 Cu(2) second moment to the concentration of 63 Cu by measuring a sample which contained 100% 63 Cu. The result, shown on the third line of Table 6.1, is within experimental error of the expected increase 1/T2g ∝ (c63 )1/2 . The BS calculated result scaled in this fashion is shown for comparison. Itoh et al. [12] also measured the behavior of T2g in the superconducting state of Y248. The latter results and the BS model calculations for this case are discussed in the next subsection. We make further comparisons with the results in Table 6.1 with calculations using (6.1.13) based on the parameters provided by Auler et al., [10]. Results obtained with a Gaussian peak for χ (q) and other parameters from Auler et al., [10] are listed in line ﬁve of the table. The INS-derived peak width is more than three times that used by PS. The value of (1/T2g )est is substantially larger than the PS value with a slightly smaller value for χ (Q). Although this is a satisfactory result, it is puzzling that it does not give the rather larger relaxation rate which they quote, and from which the value given for χ (Q) was supposedly derived [10]. The origin of this discrepancy is not understood. In line four of Table 6.1 are listed the results of a similar calculation based on (6.1.13) as well as the HF coupling, χ (Q), and peak width parameters given by Imai et al., [9], on which the calculation is based. The estimated value of 1/T2g is in good agreement with the experimental value given. A result

222

6 Dynamic Susceptibility Studies for the Cuprates

reported by Takigawa [6] is given in the bottom line of the table. Parameter values were stated in [6] for the Lorentzian model with a range of peak widths. Choosing the peak width used by PS for the same model with the same HF parameter values, we simply scale the PS result to the larger value of χ (Q) given in [6] to yield the value of (1/T2g )est stated in the table, which is in good agreement with the experimental value given for YBCO6.63. The greatly enhanced AFM ﬂuctuations in YBCO6.63 are clearly reﬂected in a shorter decay time T2g . Before continuing to discuss the signiﬁcance of these results, we address the question of how the results for 1/T2g scale with the correlation length. Scaling of T2g with χ (q) Parameters There appears to be an interesting diﬀerence between Lorentzian and Gaussian models of χ (q) which has to do with their dependence on the correlation length parameter ξ. For the Gaussian model as prescribed by Auler et al., [10], we ﬁnd that the second moment ∝ j α(i, j)2 varies roughly as ξ −1 . From (6.1.16) it follows that T2g ∼ ξ 1/2 . In contrast, PS note that T2g ∝ ξ −1 for their Lorentzian model. However, the latter model (see (6.1.17)) included a prefactor ∝ ξ 2 multiplying a peak function of unit amplitude, whereas the Gaussian has none. The ξ 2 prefactor by itself accounts for the stated variation of T2g with ξ. Without the prefactor eﬀect, then, the PS result is that T2g is essentially independent of ξ. We next consider whether it is possible to account for the foregoing behaviors using the expression (6.1.8) for the second moment. While under some circumstances it may be possible to deduce how j α2ij scales with ξ using (6.1.8), there is no simple answer to this question in general for two reasons. First, if Fαα (q) contains transferred HF couplings, the cosine factors do not scale in any way. Second, in the case of a Lorentzian form for χ (q), simple the sum q χ (q) does not converge at the boundaries, so that the integration limits become ξ–dependent. This problem is particularly severe for small values of ξ. Nonetheless we shall consider what sort of results (6.1.8) gives for q-independent HF couplings. Such a calculation is presented in Appendix A.2 for the case of a Gaussian susceptibility, with the result 1 2 2 αij = 1− 2 . (6.1.18) 2πξ 2 πξ j Thus, as ξ declines, the leading term gives T2g ∝ ξ. However, at small values of ξ the correction term in the brackets becomes increasingly important. For ξ ∼ 1.3, the correction term increases T2g by ∼ 25%. We suggest that the q-dependent HF couplings also contribute to the behavior mentioned above for YBCO, where T2g ∝ ξ 1/2 . For the Lorentzian case, with χ (q) = χ (Q)/(1+q 2 ξ 2 ), the leading term in (6.1.8) gives T2g ∝ ξ as with the Gaussian case. However, the second term gives

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

223

a somewhat larger correction than in (6.1.18), so that j α2ij levels oﬀ and may even diminish at low values of ξ. It is plausible that over a modest range of ξ values j α2ij may be rather ﬂat, leading to the ξ-independent behavior noted, in eﬀect, by PS. Therefore, it appears that the contrast between Gaussian and Lorentzian susceptibilities may be accounted for in this simple fashion. A second and equally important conclusion which we draw from this discussion is that the results for T2g do not depend strongly on ξ or on the choice of Gaussian or Lorentzian for the shape of the AFM peak in χ (q). For this reason it will also be diﬃcult to extract information from T2g data on either of these points. At the same time, the results in Table 6.1 show that T2g can be analyzed to yield semi-quantitative results for χ (Q), even if the width and detailed character of the associated AFM peak are not well established. Comparing the Temperature Variation of T2g with that of T1 The relatively weak dependence of T2g on the width of the AFM peak in χ (q) leads to an interesting contrast between echo decay times and T1 processes. While 1/T1T is given by sums of χ (q, ω) over all of q-space, 1/T2g is very nearly proportional to χ (Q), i.e. to the staggered susceptibility. T1 is, of course, also sensitive to the staggered susceptibility, since it measures the area under the AFM peak in χ (q, ω) at Q. But T1 for 63 Cu(2) has major contributions from the rest of the Brillouin zone as well, much of which collapses in the presence of a pseudogap. We see the result of this in Fig. 6.2 from Takigawa [6]. The curve for 1/T2g indicates that the staggered susceptibility is rising fairly rapidly in a Curie-Weiss-like fashion. T1 for the 63 Cu(2) rises below 300 K at a similar rate. When the spin pseudogap sets in around 200 K, however, 1/T1T goes over a maximum and then begins a steep descent which indicates collapsing behavior for χ (q, ω) over much of the BZ. The fact that 1/T2g is immune to the pseudogap decline suggests that χ (Q) is made up from parts of the Fermi surface which are not gapped. A related result is presented in the next subsection, where 1/T2 for Y248 does not decay in the superconducting state, presumably because contributions to χ (Q) are not aﬀected by the superconducting gap either. Curie-Weiss behavior for 1/T2g is also found in YBCO7 [9, 10], though with rather smaller increases between 300 K and Tc . It would be, of course, most enlightening to be able to compare such results with INS data on the same systems, including temperature dependences. While the INS characterizations are not easy to perform, the cuprates provide an ideal test bed for comparison of results for the dynamic susceptibilities. We shall see this in more detail in Sect. 6.3 with the system LSCO. Takigawa also made an eﬀort to apply the scaling theory of Sokol and Pines [16] to the susceptibility behavior of YBCO6.63 [6]. The scaling eﬀect may be seen in Fig. 6.2, where just at the upper end of the temperature range the ratio T1 T /T2g approaches a constant value. Eﬀects such as this have become a major branch of the study of cuprate magnetism and will be reviewed at some length in Sect. 6.4.

224

6 Dynamic Susceptibility Studies for the Cuprates

6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc Bulut and Scalapino (BS) used their small-U Hubbard model of spin dynamics to treat both T1 (Sect. 5.7) and T2g in the superconducting state [13]. In the latter case they found a major distinction between the cases of s-wave and d-wave pairing. We ﬁrst describe their calculation, and then review the experimental T2g data of Itoh, Yasuoka et al., [12] on YBa2 Cu4 O8 (Y248) which has been compared with the BS theory. Model Calculations of Bulut and Scalapino: T2g in the Normal State The BS calculations of T2g used much the same parameter values as employed in related work on T1 (see Sect. 5.4) [14, 15], where they used the RPA formula χ (q) =

χ0 (q) 1 − U χ0 (q)

(6.2.1)

for the real part of the dynamic susceptibility χ (q) at ω = 0. They give for the noninteracting susceptibility χ0 (q → 0) = 0.214 t−1, where t is the hopping integral giving band energies Eq = −2t[cos qx + cos qy ] − μ. The chemical potential was set so that the band occupation n = 0.86, very near the critical value for instability (see [15] and Sect. 5.4). The enhanced curve of χ (q) from the BS model is shown in Fig. 6.3(a) for the path in q-space shown in the inset. We determine the molar value of χ (Q) 20 8

6

10

4 –1/T2G

5

1/T1 T(s–1K–1)

1/T2G (ms–1)

15

2

–1/T1T

0

0 0

100

200

300

T(K)

Fig. 6.2. Measured values of 1/T2g and 1/T1 T for 63 Cu(2) in YBCO6.63 are plotted vs. temperature. The data have been scaled to coincide near room temperature, where they show similar behavior. Reprinted ﬁgure from M. Takigawa, , Phys. Rev. B49, 4158 (1994). Copyright 1994 American Physical Society

6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc

225

as follows. From discussion of NMR shift calculations in [15] the q = 0 Stoner enhancement is given as 1.75. Equating their c-axis susceptibility result to χc = 1.18 × 10−4 emu/mol Cu(2) from Table 2.4, we ﬁnd χ0 (0) = 6.74 × 10−5 emu/mol Cu(2). Relative to that value, the peak value in Fig. 6.3(a) is enhanced by a factor ∼ (3.8/0.214), giving the estimate χ (Q) 1.23 × 10−3 emu/mole Cu(2). The latter value is within ∼ 15% of the result obtained by taking t = 0.1 eV [15]. The AFM peak half-width of ∼ 0.5 (Table 6.1) is also taken from Fig. 6.3. The latter results apply in the vicinity of 100 K. BS also calculated the temperature variation of 1/T2g , both in the normal state up to 300 K and below Tc down to essentially zero temperature. Their results as given are shown as the dashed line in Fig. 6.3(b), where they are seen to fall just below the YBCO7 data from Itoh et al., [12] (ﬁlled circles). The open circles in the same ﬁgure are a plot of measured values of 1/T2g for 63 Cu(2) in Y248 also taken from [12]. The latter data have been compared with the BS calculations (solid lines) from [13], which have been scaled to coincide with the experimental data in the region around 100 K1 . The result is a dramatic comparison of T2g data with the s and d-wave BS model calculation [13]. The Superconducting State: A Dramatic Success for d-Wave The normal-state calculation gives a reasonable account of the Y248 data for 1/T2g in Fig. 6.3. In the superconducting state, these data, combined with the BS calculations, give a very dramatic conﬁrmation of d-wave pairing symmetry. The eﬀect of superconducting pairing on the susceptibility curve is shown in Fig. 6.3(a) where calculated susceptibility curves at T = 0.8Tc are shown for both s-wave (dashed line) and d-wave (dotted line). The contrast between these two is attributed by BS to nodes in the d-wave energy gap which simply allow contributions to χ (Q) to persist into the superconducting state. This is very likely related to the continued c-axis spin correlations below Tc which were demonstrated by Uldry et al., [17], as was discussed in Sect. 5.7. It may also be related to the fact that χ (Q) is immune to the pseudogap in the normal state, exhibiting Curie-Weiss behavior down to Tc . Thus, the pseudogap and the superconducting gap have similar character in this respect. 1

Since the Y248 data were obtained using NQR, the original (dotted) curve was √ ﬁrst rescaled by 2 to reﬂect the enhanced NQR relaxation rate (see Appendix A.2.1 for a discussion of this eﬀect). Following that, rescaling with the Stoner factor has been done using (6.2.1) as follows. It is presumed that the temperature dependence of χ (Q) is driven by that of χ0 (Q). From [13] it was determined that the enhancement at the peak of the curve in Fig. 6.3(a) is 5.4 at T = 100 K. Using that fact and (6.2.1) to recover χ0 (Q) as a function of T, the dotted curve with an adjusted value of U was plotted as the solid curve in Fig. 6.3(b). For the region below Tc , the original curves from [13] were simply rescaled to meet the normal-state curve at T = 82 K.

226

6 Dynamic Susceptibility Studies for the Cuprates 6

(a)

5

(π,π)

4

χ(q)

q 3 (π,0)

(0,0) 2 1 0 (0,0)

(π,0)

(π,π)

(0,0)

q

25

D

(b) Y248

1/T2G ms–1

20

15

10

S YBCO7

5

0

0

100

200

300

T(K)

Fig. 6.3. (a) The enhanced susceptibility χ (q) obtained with (6.2.1) [13] is plotted for the path in q-space shown in the inset. The solid curve shows behavior at T ∼ 100 K, while the dashed and dotted curves show behavior for s-wave and d-wave pairing, respectively, at T = 0.8 Tc . See text and part (b) of this ﬁgure for discussion of this eﬀect. (b) NMR measurements of 1/T2g for YBCO7 (dots) and NQR measurements for Y248 (open circles) by Itoh et al., [12] are plotted vs. temperature. The dotted line shows the normal-state calculations of Bulut and Scalapino [13] for 63 Cu(2) NMR in YBCO7. The solid curves are determined as follows. For the nor√ mal state the dotted line is scaled by 2 for the NQR case, then the enhancement is re-calculated using (6.2.1) to match the experimental curve near 100 K. For T < Tc the curves from [13] are simply scaled to meet the normal-state curve at Tc = 82 K. See text for additional discussion

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

227

The present results along with the dramatic T1 eﬀects discussed in Sect. 5.7 consitituted a very strong case for d-wave pairing several years before it was widely accepted by the high-Tc community. To summarize, we have seen in this section and the last that the formulation of indirect spin-spin coupling in terms of χ (q) by Pennington and Slichter opened up a very important new avenue of approach for the characterization of the AFM enhancement peaks as well as of χ (Q).

6.3 Coordinated Interpretation of NMR and INS Data for LSCO In Sect. 4.4 we discussed data for the NMR shift, uniform susceptibility, and spin-lattice relaxation time T1 for 63 Cu in LSCO:x, for x ranging over the superconducting region, 0.06 ≤ x ≤ 0.25. This system was seen to exhibit a peculiar sort of pseudogap eﬀect, which strongly aﬀects the susceptibility even at the peak of the Tc curve, but allows the 63 Cu T1 curves to follow a Curie-Weiss-like behavior down to temperatures very close to Tc . Here, we look at another aspect of the LSCO system which came about, because this system emerged as being unique among the cuprates in havineg received a very thorough characterization of χ (q, ω) by means of INS. The detailed geometry of the four mildly incommensurate peaks near (π, π) has been scanned in great detail over a wide range of frequencies. As a consequence, LSCO became a classic “test bed” for the theoretical relationship between NMR and χ (q, ω). We ﬁrst review the theoretical basis for such an investigation. The ﬂuctuation-dissipation theorem relation between spin-ﬂuctuationgenerated T1 processes in a metallic environment and the dissipative term χ (q, ω) of the dynamical susceptibility, as recounted in Sect. 3.5, had been known for many decades [18] before it was tested using experimental INS data for χ (q, ω). The latter test was conducted via T1 measurements for 63 Cu and 17 O (both planar and apical) in LSCO:0.15 [19] and was based on the INS data of Cheong et al., [20] and Mason et al., [21]. Such an enterprise – to correlate two pieces of experimental data using an “exact” theoretical relationship2 – may not seem well motivated at the outset. However, this relationship had not been tested experimentally before. Furthermore, it led to the uncovering of some interesting limitations, among which is the clash between INS and NMR data for the case of planar 17 O [19], which we review below. In this section we review the circumstances of the latter test, which call into question the usual assumption that INS results may safely be extrapolated to NMR frequencies, which are lower by a factor ∼ 104 . Additional INS data which have appeared since that time may throw some new light on the 2

This relationship is very nearly exact under the assumption that spin hyperﬁne processes are predominant. However, it has not yet been determined how important the orbital relaxation rates are for the cuprates (see Sect. 5.6).

228

6 Dynamic Susceptibility Studies for the Cuprates

situation, as well. We shall also review indirect spin-spin coupling measurements for LSCO:0.15, interpreted with values of χ (q) which were calculated from the measurements of χ (q, ω) using the Kramers-Kronig relation [22] 2 ∞ χ (q) = dωχ (q, ω)/ω . (6.3.1) π 0 From (6.3.1) one sees that such a procedure requires data for χ (q, ω) over a wide range of frequencies. Since that time, such high-frequency data have actually appeared in the literature [23]. The latter data will be taken into account in reviewing this calculation. For the T2 processes we come to a similar conclusion as with T1 , namely there is a successful account of the 63 Cu data with (or without) discommensurations, but not for the planar 17 O (see Sect. 6.3.2). 6.3.1 Review of INS Data for Optimally-Doped LSCO We ﬁrst set the stage with a brief review of relevant INS data for LSCO:x, with x ∼ 0.15. It seems that of all the cuprate compounds, LSCO alone was available in large, uniform crystals with homogeneous oxygen content. Conveniently enough, χ (q, ω) is a quantity which can be measured directly by means of INS. The principal diﬃculty is that INS measurements can only be made at frequencies several orders of magnitude higher than those at which NMR data are recorded. We examine the available INS data with that problem in mind. INS data for χ (q, ω) at energies of a few mV are shown in Fig. 6.4. In part (a) we see data for scans through two of the four incommensurate peaks located at (π, π) ± δ(0, π) and (π, π) ± δ(π, 0), where δ = 0.245 for La1.86 Sr0.14 CuO4 [21]. The peaks are seen to be well resolved, with relatively little diﬀerence between behavior near Tc = 35 K and that at 4.6 K. There is, however, an increase in intensity at the point between the peaks at higher energy. That trend is also visible in the lower-energy scans from Thurston et al., [24] in part (b) of Fig 6.4, where at ω = 1.5 meV the peaks are completely resolved, while) at 4.0 meV there is already some ﬁlling in of the space between peaks. The incommensurability varies with composition, δ 2x [20], but it shows no measureable variation with energy at the lowest energies scanned [24]. From available INS results for LSCO, then, it does not appear that discommensurations will vanish at lower (i.e. at NMR) frequencies, although the point remains at issue. At higher frequencies, however, early work showed the discommensurations fading into a single broad peak by ω = 15 meV [20]. That this trend would continue to higher energies was veriﬁed by studies to above 200 meV carried out at ISIS [23]. In that study, results for LSCO:x, x = 0.14, were compared with the undoped antiferromagnet La2 CuO4 , both qscans and energy spectra. For LSCO:0.14, discommensurations are not visible

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

229

ζ 1.1 1.2

–10

150

(a)

counts (11 min)

90 70 90 70 Background

50 T = 35 K T = 4.6 K

120 80 60 60

40

20

40

Q = ζ(π,π) + δ/√2(–π,π)

0.6

0.8

1.0 ζ

1.2

75

1.4

ω = 3.0mev T = 35K

0 150 ω = 3.0mev T = 10K 75

50

50

25

25

150

ω = 1.5mev T = 35K

0 200 ω = 1.5mev T = 10K 150

100

100

50

50

0

counts (11 min)

100

40

80

0 200

6.1 mev

counts (11 min)

140

35K

150 ω = 2.0mev T = 35K 120

40

0 100

110

ω = 4.0mev

counts (11 min)

Intensity (Counts/6 minutes)

130

60

(b)

counts (11 min)

0

T = 35 K T = 4.6 K

ΔI (Counts)

9 mev

counts (11 min)

80 10

0 0.6 0.8 1.0 1.2 1.4 0.6 0.8 1.0 1.2 1.4 q1/π q1/π

Fig. 6.4. (a) INS q-scans along the path shown at the bottom of the ﬁgure are plotted for T ∼ Tc and for T Tc for the two scattering energies shown [21]. These data show the well-resolved incommensurate peaks and a relatively small diﬀerence in scattering intensity for the two temperatures. The inset shows the diﬀerence in intensity measured for the two temperatures at 9 meV. Note the small, but deﬁnite increase in intensity between the peaks between 6 meV and 9 meV. Reprinted ﬁgure from T. E. Mason, G. Aeppli, H. Mook, Phys. Rev. Lett. 68, 1414 (1992). Copyright 1992 American Physical Society. (b) INS data at energies ω ≤ 4.0 meV, showing very well-resolved incommensurate peaks with no measurable variation of the discommensuration δ with ω. These authors ﬁnd δ = 0.22 for La1.85 Sr0.15 CuO4 . They also ﬁnd relatively small variation of intensity with temperature below Tc . Reprinted ﬁgure from T. R. Thurston, P. M. Gehring, G. Shirane, et al.,, Phys. Rev. B46, 9128 (1992). Copyright 1992 American Physical Society

in the lowest energy scans (25-50 meV) reported [23], nor any above that. The resolution in q-space may be somewhat marginal for this purpose, although the AFM (Bragg?) peak at 295 K for La2 CuO4 showed a width Δq ∼ 0.25 r.l.u. We display three composite data plots from Hayden et al., [23], namely ∞ the equal-time spin correlation function S(q) = −∞ dω χ (q, ω), the zero∞ frequency susceptibility χ (q) = (2/π) 0 dωχ (q, ω) /ω, and the local sus ceptibility χ (ω) = q χ (q, ω). These quantities have been computed from the results of the spallation–source study [23]. The local susceptibilities are shown in Fig. 6.5(a) and (b), where it is noteworthy that the results are plot-

230

6 Dynamic Susceptibility Studies for the Cuprates

ted in absolute units, and where in (b), reactor-based results are included below ∼ 25 meV . Below we shall compare these data with the absolute susceptibility results which were used to calculate T1 in [19]. The results in Fig. 6.5(a) and (b) show that the eﬀect of doping is to concentrate χ (q, ω) at energies below 50 meV (as compared with La2 CuO4 ), and that the peak seen at 22 meV is a “new energy scale” for this superconductor [23]. This energy is also a rough upper limit for the appearance of discommensurations. The solid line plotted in panel (b) is Γω , (6.3.2) χ = (Γ 2 + ω 2 ) with Γ = 22 ± 5 meV . The equal-time correlation function S(q) and the zero-frequency susceptibility χ (q) obtained with (6.3.1) in [23] are shown in Fig. 6.5 for the undoped ((c) and (d)) and the doped ((e) and (f)) cases, respectively. Owing to the near-constant width of χ (q, ω) in q-space for LSCO:0.14 [23], there is very little diﬀerence between S(q) and χ (q). The associated energy integrals have been carried out for ω ranging from 15 to 150 meV. The central peak in Fig. 6.5(e) and (f) has an HWHM of κ = 0.26(5) ˚ A−1 , which is just slightly larger than the incommensurate splitting. (See below for deﬁnition of κ.) Since the Kramers-Kronig integral favors low energies, one wonders whether there would be visible incommensurate peaks in χ (q) if the reactor-based intensity (e.g. that which gives the open circles in Fig. 6.5(b)) were included in the calculation of χ (q). As noted below, such a contribution might be appreciable for indirect spin-spin coupling with the planar 17 O. The Calibrated Susceptibility for T1 Calculations in LSCO In order to discuss T1 behavior in LSCO we need two main ingredients. The ﬁrst is a calibrated susceptiblity function χ (q, ω) for vanishing ω, with detailed q-dependence, and the second is a measured HF tensor or a near approximation thereto. We begin with the calibrated susceptibility, which was used earlier in [19], but originated with the measurements of Mason et al., [21]. The absolute calibration to these was presented in [25], but had also been used, it seems, in the paper by Hayden et al., [23]. We shall recount here the calibration used in [19]. Some careful checking ﬁnds that the latter result leads to a value for the initial slope of χ (ω) in Fig. 6.5(b) within 10% or less of the plotted value. The low-energy INS data for χ (q, ω), part of which is displayed in Fig. 6.4(a), may be represented in the normal state by the function χ (q, ω) K0 A2 θ[Γc − Γn (q)] = , (6.3.3) ω Γn (q)2 ω→0 where Γn (q) = A2 [κ2 + R(q)], with R(q) =

1 8π 2 a2L δ 2

{[(qx − qy )2 − π 2 δ 2 ]2 − [(qx + qy )2 − π 2 δ 2 ]2 } .

(6.3.4)

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

231

(a) La2CuO4(T = 295K)

4 3

χ′(ω)(μ2B eV–1 tu–1)

2 1 0 4

(b) La186Sr0.14CuO4(T = 17K)

3

Risa ISIS

2 1

S(Q)(μ2Btu–1)

0

0

50

100 hω

150

200

250

(meV)

3

(e)

15–150 meV

2

(c) 1

2

χ′(Q)(μBeV–1tu–1)

0 40 30

(d)

(f)

20 10 0 0

0.5

1 1.5 h (r.l.u)

0

0.5

1 1.5 h (r.l.u)

2

Fig. 6.5. (a) and (b) The local susceptibilities χ (ω) for La2 CuO4 (295 K) and LSCO:0.14 (17 K), derived from the data presented in [23], are plotted as a function of energy ω. As compared with La2 CuO4 , the eﬀect of doping is seen to concentrate the amplitude at low energies, giving a peak at ∼ 22 meV . Below that point are plotted data from earlier reactor-based studies [21], which serve to determine the initial slope used for T1 calculations. (c) and (e) are the equal-time spin correlation functions S(q) deﬁned in the text, for La2 CuO4 and LSCO:0.14, respectively. (d) and (f) are zero-frequency susceptibilities χ (q) obtained with (6.3.1) in a similar fashion. For LSCO:0.14 ((e) and (f)) these quantities are nearly indistinguishable, since the width of χ (q, ω) shows very little dependence on energy [23]. In (c)–(f) the rise in intensity to the right is caused by phonons, where the suggested behavior of the quasiparticle properties is indicated by dashed lines. Although the spallation source resolution width is not as good as in reactor-based studies, it is clearly well below the peak widths found for LSCO:0.14 in (e) and (f). Reprinted ﬁgures from S. M. Hayden, G. Aeppli, H. Mook, et al.,, Phys. Rev. Lett. 76, 1344 (1996). Copyright 1993 American Physical Society

232

6 Dynamic Susceptibility Studies for the Cuprates

Here aL = 3.8˚ A is the CuO2 lattice constant and δ = 0.245 is the discommensuration [21]. The other quantities in (6.3.3) are • •

• •

The constant A2 = 3.858 eV ˚ A2 comes from a form used to ﬁt INS data at ﬁnite values of ω [21]. The peak width parameter κ = [(0.034)2 + 31.35(kB T )2 ]1/2 ˚ A−1 is also from an expression used to ﬁt data over a range of ω values, but is stated here for ω = 0. In this expression kB T is to be entered in units of eV. We note that this representation of κ has been updated [25] from what was used in [19]. The two expressions give very similar values for temperatures of 100 K or less. The calibration obtained using acoustic phonons [25] gives K0 A2 2.5μ2B . The function θ[p] = 1 if p > 0 and 0 otherwise. In (6.3.3) Γc is taken to be an estimated maximum magnon energy ∼ 0.3 eV .

The foregoing function describes χ (q, ω) in q-space as having four incommensurate peaks located at (π, π)± (0, π)δ and (π, π)± (π, 0)δ. These peaks have calibrated widths given by κ. As stated, the function has units of μ2B /eV 2 per formula unit. This is the initial slope of χ (q, ω), determined by INS data at energies of just a few meV. From the standpoint of INS methodology, it is supposed that this function would apply in the energy range in which it was determined and to all energies below that as well. As we shall see below, however, there is a problem with this interpretation in connection with the T1 data for the planar 17 O, which will be discussed in Sect. 6.3. We note here that there is also a second problem with using INS measurements as a calibration of χ (q, ω) for NMR frequencies. This has to do with the behavior in the superconducting state. We know from T1 measurements for 63 Cu in LSCO (as well as those for other superconductors at T < Tc ) that the eﬀective value of χ (q, ω) declines typically by a large factor. For LSCO 1/T1 drops by a factor ∼ 100 at a temperature of 4.2 K relative to its value in the normal state [3]. The INS data for χ (q, ω) as given by Thurston et al.,, for example, shows no decline whatever below Tc , particularly at the lowest energies tested ω ∼ 1.5 meV. As the latter authors have commented [24], this is a situation for which ”further theory is required”. It seems, then, that we do not always understand when the INS results will apply at NMR frequencies and when they do not. NMR Shift and Susceptibility Analysis for LSCO Below, we apply the calibrated expression (6.3.3) for χ (q, ω) to T1 data for Cu and planar 17 O in LSCO. For this purpose, The numbers are similar to those for YBCO given in Chap. 3, but need, of course, to be established independently. Working from the 63 Cu shift results of Ohsugi et al. [3], it is ﬁrst noted that Kc (T ) is constant at ∼ 1.20% well into the superconducting state. Similar to YBCO, then, we have Ac + 4B 0. Next, Kcvv is slightly smaller than that ( 1.28%) for YBCO. Thus, the crystal-ﬁeld energies for 63

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

233

Table 6.2. Compilation of parameters related to the analysis of 63 Cu and planar 17 O NMR shifts and susceptibilities for LSCO:0.15 at T = 300 K. These quantities are deﬁned and discussed in the text. The units are as follows: NMR shifts: %; susceptibilities: 10−6 emu/mol; HF constants: kOe/spin. The HF constants are deﬁned by (3.3.2). They will have their proper energy units when multiplied by 103 γ17,63 gab gc

vv s vv Kab Kcvv Kab χvv χsab χsc B Aab Ac ab χc

Ka17 Kb17 Kc17 Ca Cb Cc

2.06 2.27 0.27 1.20 0.41 19.1 85.1 145 177 76 19 -304 0.274 0.162 0.214 108 64 77

LSCO are a bit higher and the g-factors slightly smaller as well. Estimated values are given in Table 6.2. From the Kαvv tensor we use the eﬀective orbital HF shift coeﬃcient αorb = 141 (emu/mol)−1 given with (2.3.5) for YBCO. This leads to the Van Vleck susceptibility components given in Table 6.2. The Van Vleck susceptibility tensor is combined with the estimate χdia −99 × 10−6 emu/mol [26, 27] to extract the spin susceptibility tensor from χexpt = χsα + χvv α α + χdia .

(6.3.5)

The powder average susceptiblity was found to be 98 × 10−6 emu/mol (300 K) [19], a value within 5% of those given by Ishida et al., [28] and Johnston [29]. Since χsα ∝ gα2 [18], we deﬁne a quantity χs0 with the relation χsα = (gα2 /4)χs0 . This leads to the expression for the powder average spin susceptibility 13 (χsc + 2 χsab ) = 1.137 χs0 using g-values from the table. With (6.3.5) and the numbers given, we ﬁnd χs0 = 137.1 × 10−6 emu/mol. The values for χsα in Table 6.2 follow immediately. These are essentially the susceptibility results given in [19]. Note that the spin susceptibilities are substantially larger than those found for YBCO7 (Table 3.4). We now can extract the 63 Cu spin HF constants for LSCO:0.15. The shift s s coeﬃcient for Kab 0.41% (300 K) [3] is Kab /χsab = 28.3 (emu/mol)−1 . Using (2.3.4) this gives Aab + 4B = γ63 325 kOe/spin. From studies of undoped La2 CuO4 [30] we take the result Aab − 4B = −286 kG/spin. Combining the latter two relations leads to Aab and B as given in Table 6.2, as well as the estimate Ac = −4B = −304 kG/spin. All results are summarized in Table 6.2. We believe that these slightly smaller numbers than used in [31] give a more realistic outcome. The corresponding values Cα for the planar 17 O were derived from roomtemperature NMR shift measurements and reported in [19]. The shift meaorb surements, which have been corrected for orbital background shifts Ka,b,c = (0.046,0.008,-0.027) (in %, from Takigawa et al., [32]), and their corresponding HF constant values are listed in Table 6.2. Evaluation of T1 for

63

Cu and

17

O from INS Data

With HF couplings from Table 6.2, we can now evaluate T1 for 63 Cu and 17 O in LSCO:0.15 using the INS susceptibility data embodied in (6.3.3). Relaxation rates were calculated for 63 Cu with (3.5.11) and for 17 O with (3.5.14) [19].

234

6 Dynamic Susceptibility Studies for the Cuprates 40

8

(63T1NQRT)–1

6

30

4

20

2

10

(63T1NQRT)–1 sec–1 K–1)

(17T1pT)–1 (10–3 sec–1 K–1)

(a)

(17T1pT)–1 0

0

50

100 200 150 Temperature(K)

250

300

0

3.0 0.20

0.15

2.0 1.5

0.10

1.0

Ks17p(%)

(17T1pT)–1 (10–1 sec–1 K–1)

(b) 2.5

0.05 0.5

(17T

–1 1pT)

Δ

K317p 0.00

0.0 0

50

100 150 200 Temperature(K)

250

300

Fig. 6.6. (a) Data for 1/T1 T are plotted vs. T for 63 Cu (ﬁlled squares, +’s: righthand scale) and for apical 17 O (dots: left-hand scale) in LSCO:0.15 [19]. The data plotted as +’s are from Imai et al. [33]. The dotted curve is a plot of the calculated rate based on INS data given with (6.3.3) and HF constants from [19]. See text for discussion of expected behavior with HF constants from Table 6.2. (b) 1/T1 T data (dots) are plotted vs. T for planar 17 O in LSCO:0.15 [19]. Also plotted are s (open triangles), which have been scaled data points for the c-axis NMR shift K17p to coincide with the relaxation data (right- hand scale). The calculated behavior for 1/T1 T based on INS data given with (6.3.3) and HF constants from Table 6.2 is shown as a dotted line. See text for discussion of these results. Reprinted ﬁgures from R. E. Walstedt, B. S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994). Copyright 1994 American Physical Society

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

235

Experimental data plotted as 1/T1 T for both 63 Cu and the apical 17 O in LSCO:0.15 are shown in Fig. 6.6(a). 63 Cu NQR data are plotted as ﬁlled squares, while some earlier data from Imai et al., [33] are plotted as “+” symbols. These data sets are in very good accord where they overlap. In addition, data for the apical 17 O scaled to coincide with the 63 Cu data between 100 K and 200 K are shown as dots with error bars. Since the apical 17 O is relaxed purely by local HF contact with one Cu-site spin, it is expected to behave roughly like the 63,65 Cu. Owing to a very weak HF coupling, the latter data (i.e. 17 T1 ) are in the seconds range at 50 K, while the corresponding numbers for 63 Cu are in the sub-millisecond region. The apical oxygen appears to be diverging at the lowest temperatures a bit faster than the 63 Cu, but they otherwise show a very similar temperature dependence. The calculated values of 1/T1 T for the 63 Cu based on INS data for χ (q, ω) are shown as a dotted line cutting through the data plot at a rather steep angle [19]. With very limited parameter adjustability, the agreement between INS data and the 63 Cu relaxation rate is quite satisfactory. However, our current estimate of the HF parameters, i.e. B in particular in Table 6.2, is somewhat smaller than that used in [19]. The latter values would therefore lead to estimates of 1/T1 T ∼ 30% smaller than those plotted in the ﬁgure. We suggest that this would give a somewhat more realistic result, although it would clearly show that some other mechanism – presumably from a “background” contribution to χ (q, ω), which cannot be see with INS – becomes important at higher temperatures. In Fig. 6.6(b) are plotted 1/T1 T data for the planar 17 O (dots: lefthand scale) scaled with three NMR shift data points (open triangles: righthand scale). Thus, 1/T1 T follows the susceptibility curve as was found for YBCO6.63 (Figs. 4.4 and 4.9), in behavior which is typical of a spin pseudogap. On the other hand, the calculated 1/T1 T curve based on INS data and (3.5.14), shown as a dotted line, has the correct magnitude, but varies with temperature in a fashion which is totally incompatible with the NMR data. The magnitude of the INS-based estimates of 1/T1 T is generally correct for both nuclear spin species, verifying in part the extrapolated use of INS data at such low frequencies. What appears to be the case for the planar 17 O , however, is that the discommensurations do not appear to hold up at the very low NMR frequencies3 . With the same parameters for χ (q, ω), except that δ ∼ 0, the planar 17 O curve would drop by more than an order of magnitude. It follows, then, that the 17 O relaxation process is completely dominated by 3

The decay of the discommensurations at low frequencies implies, of course, that there is another energy scale in the problem where this happens. We must point out that there is no other evidence for such an eﬀect. Moreover, such a crossover to commensurate ﬂuctuations has been suggested to imply an instability in the system as well (C. Varma, private communication). We only wish to emphasize that the discommensurations observed in INS studies lead to predicted NMR eﬀects which are not found.

236

6 Dynamic Susceptibility Studies for the Cuprates

a broad background term in χ (q, ω) which covers most of the BZ and which has the pseudogap (NMR shift–like) temperature dependence. In [19] it was suggested that a two-band model of quasiparticle dynamics may be the answer to the 17 O T1 problem. However, in view of all of the negative discussion of that option in earlier chapters, such a possibility seems to be quite out of the question at this point. On the other hand, just how the discommensurations disappear and below what energy scale this happens are just as much a mystery now as they were in 1994. To this we must add the discrepancy which occurs in the superconducting state, where INS shows only a modest decline in the vicinity of Q = (π, π) [21, 24]. Before concluding from this discrepancy with NMR data that there is some problem in principle here, however, one must verify that this is not a sample-dependent eﬀect.4 6.3.2 Interpretation of for χ (q)

63

Cu and

17

O T2 Data with INS Data

In Sect. 6.1 the interpretation of spin-echo decay (T2g ) measurements with the purely static indirect coupling term Hzz (see Appendix A.1) was discussed in some detail. This technique has been applied widely to cuprate NMR/NQR measurements. Here we consider the case of LSCO:0.15, for which we shall use the INS-derived calibration of χ (q, ω), along with the Kramers-Kronig relation (6.3.1), to obtain quantitative estimates of χ (q). The latter data, combined with HF constants from Table 6.2, are used for the indirect coupling calculation. Spin echo decay in LSCO:0.15 presents a number of complications which did not occur in the “static” cases discussed in Sect. 6.1. The eﬀects of T1 ﬂuctuations, both direct and indirect (i.e., of neighbors), are quite important. Moreover, there is strong evidence that like-spin 63,65 Cu neighbors in the m = ± 21 states are ﬂuctuating among themselves on the time scale of T2 , changing the nature of the problem in a fundamental way. The planar 17 O also present a diﬀerent and unique situation, in that T2 is dominated by the 63,65 Cu-17 O indirect spin-spin coupling term, which is time-modulated by the 63,65 Cu T1 processes. The 17 O-17 O coupling term is reckoned to be negligibly small. The somewhat diﬀerent methodology needed to treat these cases was reported in [31]. The techniques used there will be reviewed brieﬂy here in the course of discussing the T2 data for LSCO:0.15 and its interpretation. 63,65

Cu T2 Data and Simulations of Nuclear Spin Fluctuations

Spin-echo decay measurements for 63,65 Cu were carried out on a partially oriented powder sample of LSCO:0.15 containing ∼ 30% 17 O [31] at T 100 K. The measurements were made on the (− 12 ↔ 12 ) transition in a ﬁeld of 7 T. Decay curves were measured for 63 Cu with several levels of refocussing 4

The author thanks T. E. Mason for an informative discussion of this point.

6.3 Coordinated Interpretation of NMR and INS Data for LSCO 100

237

100 63

Cu: Cu:

Cu: Δ + O

65

63 65

(a)

10–1

Echo Decay (Arb. units)

Echo Decay (Arb. units)

Cu: ×

(b) 10–1 100 63

Cu: Cu:

65

(c)

10–2 0.0

10–1 0.5 1.0 (2τ)2(μ sec2)

1.5 ×104

0.0

0.5

1.0

(2τ)2(μ sec2)

1.5

×104

Fig. 6.7. (a) Spin echo decay curves for 63,65 Cu taken on the (− 21 ↔ 12 ) transition in a ﬁeld of 7 T at a temperature of 100 K. Data for diﬀerent refocussing pulses have been displaced vertically for clarity. Conditions are as follows: Full power, θ2 π (63 Cu: Δ). Power down 10 db, θ2 3π/4 (63 Cu: +). Power down 10 db, θ2 π/4 (63 Cu: ◦). Full power, θ2 π (65 Cu: ×). The curvature is thought to be caused by a distribution of indirect coupling strengths. The bottom curve is a composite of all the data. The solid line is the estimated Gaussian decay with T2g = 75.6 μs. These data have all been corrected for direct T1 eﬀects as described in the text. (b) and (c) Simulated decay curves obtained with random-number selection techniques as described in [31]. Small dots and triangles show static decay curves for 63 Cu and 65 Cu, respectively, where the decay is caused by a single π pulse. The solid lines show pure Gaussian decay. For (b) the large triangles and dots show how the decay curves are modiﬁed if random transitions simulating T1 relaxation eﬀects are included. For (c) the large triangles and dots show results for when both T1 ﬂuctuations and ﬂipﬂop transitions between the ± 21 levels for 63,65 Cu are included as described in the text. Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

pulse as well as for 65 Cu with θ2 π. The echo decay data obtained are shown in Fig. 6.7(a) [31]. The decay data shown have been corrected for direct T1 relaxation eﬀects using results from Appendix A.3. The essence of the procedure is as follows. Direct T1 relaxation eﬀects result in a factor exp(−2τ /T1E ) multiplying the spin echo decay function. The value of T1E depends on the T1 process of the nuclei observed, i.e. on its anistropy and on the transition being excited. Deﬁning Wα to be the contribution to 1/T1 from ﬂuctuations along the α axis,

238

6 Dynamic Susceptibility Studies for the Cuprates

then the relaxation rate with ﬁeld along the z axis becomes 1/T1z = Wx + Wy . For arbitrary half-integral spin the (− 12 ↔ 12 ) transition echo decay rate for isotropic spin-lattice relaxation is 1/T1E = (I + 12 )2 /T1 . For the anisotropic case this becomes 1 T1Ez

=

[I(I + 1) − 3/4] 1 1 + + , T1z 2T1x 2T1y

(6.3.6)

in terms of T1 values measured along the three axes. For axial symmetry with I = 32 this becomes 1/T1Ez = 3/T1z + 1/T1xy in an obvious notation. With known values of T1α for LSCO:0.15, this formula gives T1Ec = 90μs for 63 Cu and 80 μs for 65 Cu. The corresponding correction factors have been applied to the echo decay data in Fig. 6.7(a). The decay curves in Fig. 6.7(a) have been shifted vertically for clarity. At the bottom of the ﬁgure is a composite plot of all four curves, which shows that they are very nearly indistinguishable. This is a remarkable result in the sense that the decay is independent of θ2 and is also the same for both isotopes, whose γ values diﬀer by ∼ 7%. The ﬁrst eﬀect shows that there is considerable amount of “ﬂip-ﬂop” motion taking place, and the second can be rationalized by means of the latter eﬀect combined with the eﬀect of T1 ﬂuctuations [31]. We give here a brief account of these mechanisms, which were presented in detail in [31]. In order to take account of the foregoing eﬀects in a calculation of spin echo decay, the decay process has been simulated with a model where the spin in question is coupled to neighbor spins with a set of randomly chosen coeﬃcients. The coeﬃcients are scaled to give a second moment adjusted at ﬁrst to produce the observed value of 1/T2g (line drawn in Fig. 6.7(a)) in a static decay process for 63 Cu. In a statistical simulation of such a static echo decay this yields the small dots in Fig. 6.7(b) for 63 Cu and small triangles for 65 Cu. Straight lines representing precise Gaussian decay functions are drawn for comparison. Note that the 65 Cu spin echo decays much more slowly than the 63 Cu. This is because the 31% abundant 65 Cu has only half as many “like-spin” neighbors with which to relax the echo [31]. The next step is to introduce the “indirect T1 eﬀects” by allowing the neighbor spins to execute random transitions between m levels at the correct rate dictated by magnetic dipole coupling T1 processes. The result of this is shown as large dots (63 Cu) and large triangles (65 Cu) in Fig. 6.7(b). The decay constant 1/T2g for 63 Cu is increased by ∼ 15% by the T1 ﬂuctuations, but for 65 Cu the increase is nearly three times as much. This is because the number of neighbor spins relaxing the 65 Cu is increased by about a factor of six, whereas the increase for 63 Cu is much smaller. Now the 63 Cu are relaxing ∼ 10% faster than the 65 Cu. The ﬁnal step is to initiate ﬂip-ﬂop transitions between the ± 12 levels of both isotopes. That these are actually taking place is evidenced by the absence of change in the decay curve with θ2 in Fig. 6.7(a). Since the (± 12 ↔ ± 32 ) transitions undergo severe ﬁrst-order quadrupolar broadening, ﬂip-ﬂop transitions

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

239

are only allowed for the ± 12 levels. Estimates from the indirect interaction calculations suggest that ﬂip-ﬂops are present on a time scale of about 50 μs. Introducing these into the simulation then gives the decay curves shown in Fig. 6.7(c) (large dots and triangles). The 65 Cu decay time increases slightly, but the 63 Cu increases by more than 10%, so that the two now very nearly coincide. Evidently, the ﬂip-ﬂops give a slightly greater “narrowing” eﬀect for like spins than for unlike spins. In any case, now the decay times are nearly the same for both isotopes, as was observed. Quite coincidentally, they are both now equal to the initially estimated static decay time for 63 Cu within just a small error. We do not believe that there is any simple way to obtain this result except by simulation [31]. Indirect Coupling Calculations for

63

Cu

Having determined a reasonable experimental estimate of 1/T2g for the 63 Cu in LSCO:0.15, we could now compare that number with calculations based on an evaluation of aα (i, j) with (6.1.7), the HF parameters from Table 6.2, and χ (q) calculated with INS data for χ (q, ω) using the Kramers-Kronig relation (6.3.1). This kind of calculation was reported in [31], using the form (6.3.3) for χ (q, ω) at all energies. Below, we display the latter results and then make a critical commentary on how this evaluation should be modiﬁed in the light of more recent INS data, particularly the high-energy spallation source results [23].

χ0′ (ω,T)/hω (103μB2 /eV2)

2.0 × 104

|αij|(sec–1)

1.5

1.0

ωpeak 5

0

ωco

0

20 40 hω (meV)

0.5

0.0

0

2

4

6

8

10

rij /aL

Fig. 6.8. The calculated range function αij for the “zz” indirect coupling terms among the 63,65 Cu is shown as ﬁlled circles vs. rij . Only coeﬃcients greater than 2% of the nn value are included in the plot. The inset shows the coeﬃcient from (6.3.7) which occurs in the KK integral, adjusted to yield the measured value of T2 . Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

240

6 Dynamic Susceptibility Studies for the Cuprates

In [31] the same basic expression (6.1.9) was used for the coeﬃcients, where the Kramers-Kronig integral of the expression χ (q, ω) =

χ0 (ω, T )κ4 (ω, T ) , [κ2 (ω, T ) + R(q)]2

(6.3.7)

in the same notation as (6.3.3), is used for χα (q). In this expression, one has A−1 and ET = κ2 (ω, T ) = κ20 + a2L [(kB T /ET )2 + (ω/Eω )2 ], with κ0 = 0.034 ˚ Eω = 47 meV [25]. For the low-frequency region (ω < 20 meV ), the function χ (ω, T ) can be represented as linear in ω and declining with temperature as 1/T 2 [25]. It was found that the KK integral up to 20 meV was insuﬃcient to account for 1/T2g , so the integral was extended, with χ (ω, T ) = constant, up to a cutoﬀ for an evaluation at T = 100 K. Adjusting the cutoﬀ to obtain the experimental value of 1/T2g , it was found to be ωco 50 meV. The range function αij for the 63 Cu coupling (Hzz ) calculated as described is displayed in Fig. 6.8(a), where the KK integrand χ (ω, T )/ω is shown in the inset. Since there are usually four neighbors at each value of rij , this ﬁgure shows that the indirect coupling second moment is dominated by 15–20 neighbor nuclei. It is interesting to consider what modiﬁcation would be made to this analysis in the light of high-frequency χ (q, ω) data [23] (Fig. 6.5), which were not available at the time [31] was submitted. There are two main diﬀerences if one envisions using the data of Fig. 6.5. First, to the extent that discommensurations survived in χ (q), they would no doubt be greatly diminished in importance with data from Fig. 6.5, which would be represented by a single peak with amplitude varying as Γ ω/(Γ 2 + ω 2 ) with Γ = 22 ± 5 meV . This is probably of little signiﬁcance for the 63,65 Cu, but it will ﬁgure in our discussion of 17 O below. Second, the Lorentzian gives a broader “spectrum” of contributions, extending out to 150 meV and beyond. Interestingly, if one performs the KK integral for these two cases, the results agree within a few percent. Thus, the new data [23] corroborate the earlier result for 63,65 Cu[31]. T2 Decay of the Planar

17

O at 100 K

The planar 17 O spin-echo decay data at 100 K are displayed in Fig. 6.9. This decay curve cannot be characterized in a simple way, a circumstance resulting, we believe, from the nature of the sample. Whereas only a modest percentage of ﬁeld-oriented sample material contributed to the Cu NMR signals, the 17 O second-order quadrupolar shifts are negligibly small. As a result, essentially all of the poorly-aligned sample material contributes to the planar 17 O line. We therefore treat the system as a random powder. Furthermore, quite unexpectedly, the dipolar spin-spin coupling alone accounts for the decay curve in Fig. 6.9. Its peculiar character, with a long tail of low amplitude, is caused by the “magic angle” region of phase space where 3 cos2 θ − 1 ∼ 0. The corresponding subset of nuclei relax very slowly.

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

241

100

SPIN ECHO AMPLITUDE (Arb. Units)

17 17O: 0:

10–1

10–2 0

1

2

3

4

5

6

(2τ)2(msec2)

Fig. 6.9. Experimental data for the 17 O spin echo decay at 100 K (ﬁlled circles) are plotted vs. (2τ )2 . The ﬁeld is oriented along the c axis. A simulated decay curve calculated with the combined eﬀects of dipolar and indirect coupling calculated as for the 63,65 Cu is shown as “×” symbols. A simulated decay curve with purely dipolar couplings modulated by T1 processes alone is plotted with ﬁlled triangles connected by a solid line. The same calculation with both T1 modulation and dynamic ﬂip-ﬂop transitions between the ± 12 levels of the 63,65 Cu neighbors, shown as ﬁlled squares connected by a solid line, is seen to be in good accord with the data [31]. Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

There is, however, more to the story than just those simple points. On evaluating the indirect coupling terms for the planar 17 O, it was found that the 17 O–17 O terms were small, but that there was a sizeable 63,65 Cu –17 O term, which gives an unlike spin indirect second moment Δω 2 IAB = 1.5 × 107 s−2 6 −2 [31], larger than the corresponding dipolar term Δω 2 dip AB = 6.25 × 10 s 63,65 (98% of which is contributed by the two nn Cu spins). This unlike-spin second moment is expected to dominate the 17 O spin-echo decay, because of its time-modulation by the 63,65 Cu T1 processes. Thus, for a crystal of unique orientation one has 1/T2O = Δω 2 AB T1Cu . The calculation of the powder-average decay curve, including indirect couplings evaluated as for the 63,65 Cu case above, leads to the decay curve plotted with “×” symbols in Fig. 6.8(b). This is widely at variance with the

242

6 Dynamic Susceptibility Studies for the Cuprates

experimental data. The diﬃculty, we surmise, is again related to the assumed discommensurations at NMR frequencies. If δ → 0 in R(q) (6.3.4), the indirect coupling drops by a large factor and its contribution to Δω 2 AB becomes negligibly small. This inconsistency with discommensurations is on the same scale as the estimate of T1 in Fig. 6.6(b). It again suggests that the discommensurations in the INS data ((6.3.3) and (6.3.4)) are not “seen” at NMR frequencies. There is yet another small surprise in the interpretation of Fig. 6.9. If one takes the dipolar second moment in the foregoing formula, i.e. 1/T2O =

Δω 2 dip AB T1Cu , averaged over all orientations, one ﬁnds the curve plotted with small triangles in Fig. 6.8(b), not quite in quantitative agreeement with the data. The ﬁnal curve, plotted with ﬁlled squares, is only obtained when one includes the 50 μs–rate ﬂip-ﬂops between the ± 12 levels. These, we recall, were important in interpreting the 63,65 Cu T2 decay curves as well. In the end, however, the most astonishing result is the total abnegation of indirect spin-spin coupling for the planar oxygen nuclei.

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) A large body of work has grown up around the discussion of scaling theories in the normal state of YBCO, Y248, and LSCO by Pines and co-workers [16, 34] and Moriya et al., [35]. We oﬀer here a brief summary of NMR/NQR results and interpretation in terms of the theories mentioned. Although a great deal has been done, there seem to be important questions which remain unresolved as well. The details of these theoretical models go beyond the scope of this book, so we shall focus here on predicted behavior and experimental tests thereof. In the interest of presenting a compact account of this subject, many interesting experimental details have been omitted. The interested reader is referred to the literature cited for a more detailed account of these matters. 6.4.1 Phase Diagram and Basic Relationships for T1 , T2g To facilitate discussion we display the basic phase diagram presented by Barzykin and Pines (BP) [34] in Fig. 6.10, which refers speciﬁcally to YBCOy (see also the paper by Sokol and Pines (SP) [16]). For the superconducting phases (6.45≤ y ≤7.0) the important regions are labelled “quantum critical” (QC), “quantum disordered” (QD), and “no scaling”, which was formerly termed the “overdamped” (OD) region [16]. These terms refer, of course, to the behavior of the AFM ﬂuctuations in the system, which are generally assumed to control the static and dynamic magnetic properties. One of the key parameters is a temperature-varying correlation length ξ, which is dimensionless in units of the lattice constant a. In the QC region, ξ 1 but grows shorter with increasing temperature, until at ξ ∼ 2 there is a crossover labelled Tcr to the OD region, in which ξ is of the order of 1 or less. At higher

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

243

temperatures and doping levels the AFM ﬂuctuations cease to be a controlling factor and the system reverts to a normal Fermi liquid. The temperature T∗ which marks the boundary between QC and QD will be deﬁned below. It is useful to note that the phase boundary in Fig. 6.10 is similar to the phase boundary between regions I and II of the phase diagram proposed by Varma (see Fig. 4.19). The implied physical signiﬁcance of these phase boundaries may also be quite diﬀerent in detail [36]. In Fig. 6.10, Tcr has also been identiﬁed with a maximum in the uniform susceptibility by BP, and data points shown in Fig. 6.10 for Tcr have derived from NMR shift data. Large error bars reﬂect the ﬂatness of such maxima. Below, we review an eﬀort to locate Tcr more precisely with NQR studies of T1 and T2 of 63 Cu(2) in Y248. From the behavior of 89 Y NMR shift data, Han et al., [37] have determined that the equivalent oxygen level of Y248 in the YBCOy family is at YBCO6.8. On that basis, BP suggest that Tcr for Y248 should occur at ∼ 500 K. Although drawn for YBCO, the phase diagram structure shown in Fig. 6.10 is presumed to apply to all cuprates. The superconducting region lies within the QD region. A system doped to the right of the Tcr line has no pseudogap and lies in the OD region at all temperatures. If there are AFM ﬂuctuations in the OD region, they are assumed to obey mean-ﬁeld behavior [35] as opposed to QC behavior. We now deﬁne the behavior of χ(q, ω) according to the BP model [16, 34]. 1400 1200

Temperature (K)

1000

No scaling

800 RC(z = 1)

600

QC(z = 1)

400 Neel

200

Tcr

T QD

0 6

6.2

6.4 6.6 6.8 oxygen content, y

7

Fig. 6.10. Phase diagram from Barzykin and Pines [34] for magnetic scaling behavior in the YBCO family of cuprates. In the superconducting phases there are three regions identiﬁed, the quantum critical (QC: z=1), the quantum disordered (QD: z=1), and the “no scaling” (or overdamped OD: z=2). Deﬁnition and measurement of the phase boundaries is discussed in the text. Reprinted ﬁgure from V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995). Copyright 1995 American Physical Society

244

6 Dynamic Susceptibility Studies for the Cuprates

To consider the SP-BP model, AFM correlations are characterized by the correlation length ξ and the low-frequency ﬂuctuation energy scale ωsf , both of which may vary with temperature. These energy and length scales are related by the dynamical exponent z, thus ωsf ∼ ξ z . In this connection it is also useful to employ the MMP model susceptibility [4, 11, 16] χ(q, ω)MMP =

ξ 2 χ0 1 + q 2 ξ 2 − iω/ωsf

(6.4.1)

as was employed by PS in their indirect coupling calculation [2]. Then, taking the simpliﬁed forms χ (q, ω) 1 1 ∼ d2 q , ∼ d2 q χ (q, 0)2 , (6.4.2) T1 T ω T2g ω→0 one ﬁnds the relations

T 1 1 ∼ , ∼ ξ. T1 ωsf T2g

(6.4.3)

Without paying much attention to the approximations involved, we apply (6.4.3) to diﬀerent parts of the phase diagram. In the overdamped, z = 2 −1 2 region, we have ωsf ∼ ξ 2 , leading to T1 T /T2g ∼ constant, which was the scaling prediction of Moriya et al., [38]. On this basis it was suggested that 2 is approximately constant for YBCO7 [6, 16] (however, see further T1 T /T2g discussion of this point below). At high temperatures BP suggest ωsf ∼ T , so that T1 ∼ constant and T2g ∼ T 1/2 , which is at least a semiquantitative description of the data of Imai et al., [9]. The point here is that across the Tcr line in Fig. 6.10 the behavior is expected to be qualitatively diﬀerent. Moreover, the approximations for (6.4.2) −1 ∼ ξ and one and (6.4.3) are better in that ξ 1. Thus, with z = 1, ωsf expects that T2g /T1 T ∼ constant. Again, at high T , ωsf ∼ T , so with (6.4.3) on again expects T1 ∼ constant[34]. An interesting example of the latter behavior is seen in the LSCO data of Ohsugi et al., [3] shown in Fig. 6.11. The behavior of T1 T vs. T is such that the curve is linear at high temperatures for all compositions of LSCO:x up to x = 0.24. Lest one suppose that x = 0.24 is “overdoped” (or OD), however, it is noteworthy that at low temperatures 1/T1 T for LSCO:0.24 is more than twice as great as for YBCO7 [3]. What is quite remarkable, however, is that for x = 0.075 the linear behavior of T1 T in Fig. 6.11 extrapolates nearly to the origin; T1 is almost perfectly constant from ∼ 75 K up to 300 K. The latter ﬁgure also illustrates the QC-QD boundary T∗ , which is the point at which the data for T1 T break away from the linear high-T behavior. T∗ is seen to range from ∼ 50 K to ∼ 100 K over the range of compositions tested. We note in passing that the behavior of T1 T in Fig. 6.11 suggests that the 63,65 Cu relaxation process over this range of temperature and concentrations is dominated by a single mechanism, namely the contribution of the AFM

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) La2–xSrxCuO4

63Cu

NQR x= 0.24 0.20 0.15 0.13 0.10 0.075

100

T1T (10–3 secK)

245

50

Tc –100

0

100 T (K)

200

300

400

Fig. 6.11. Plot of T1 T data vs. T for compositions of LSCO:x, with x ranging over the supeconducting phase [3]. These data exhibit the high-temperature limiting behavior of the SP model [16], where T1 T goes asymptotically as ωsf ∼ T . Reprinted ﬁgure from S. Ohsugi, Y. Kitaoka, K. Ishida, G-q. Zheng, and K. Asayama, J. Phys. Soc. Japan 63, 700 (1994). Copyright 1994 Physical Society of Japan

peak(s) in the vicinity of (π, π). That viewpoint, however, is not quite consistent with the behavior seen in Fig. 6.6(a), where it appears from the INS data employed there that by room temperature the relaxation will be dominated by a “background” term not resolvable with INS. This discrepancy remains to be analyzed and understood. n , n = 1 or As for the behavior of T2g in LSCO, the variation of T1 T /T2g 2, was examined in some detail in a study where the indirect T1 corrections to spin echo decay discussed in Sect. 6.3 were carefully evaluated [39]. It was found for LSCO:0.15 that T1 T /T2g is constant well within the errors and 2 T1 T /T2g was not, clearly placing this system in the QC category. Interestingly, a similar evaluation for YBCO7 found that QC behavior for this system was favored as well [39], contrary to the conclusion mentioned earlier [16]. In much of the literature, the indirect T1 corrections to T2g have not been taken account of. Note, however, the work of Keren et al., [40]. 6.4.2 The Dynamical Crossover Study by Curro et al: Y248 A very interesting piece of experimental work regarding the z = 1 to z = 2 crossover is that of Curro et al., [4], who performed a temperature scan of the dynamics on the system Y248. To our knowledge, no other such test of the

246

6 Dynamic Susceptibility Studies for the Cuprates

Tcr boundary has been reported. Y248 is an excellent system for such a test, because it is stable (i.e. does not lose oxygen) for temperatures well beyond 700 K. This study reported T1 and T2g data up to the latter temperature. In order to perform such a study it was necessary to use a random powder sample, since no known epoxy resin would be stable at such high temperatures. Thus, T1 and T2g were measured using NQR and the NMR shift was measured using the powder-pattern NMR spectrum. Stray magnetic ﬁelds had to be shielded out of the sample space to a fraction of a Gauss, because they disturb the NQR spin echo decay function. Finally, the authors examined and corrected for the indirect T1 modiﬁcations of T2g described in Sect. 6.3 for LSCO [31]. One stimulus for the Y248 study discussed here was the conjecture by Barzykin and Pines [34] that the Y248 system would exhibit a crossover transition at T ∼ 500 K. The 63 Cu(2) T1 data from Y248 exhibited a curve of T1 T vs. T very similar to one of the lightly-doped compounds in Fig. 6.11 with T∗ ∼ 200 K, but showed no feature at 500 K [4]. The T2g data, on the other hand, showed a deﬁnite kink near 500 K, as may be seen in Fig. 6.12. Also shown in that ﬁgure are data (open circles) from a previous study by Corey et al., [41] which are in excellent accord, but extend only to ∼ 450 K. In Fig. 6.13 T1 and T2g data for 63 Cu(2) are combined to make plots of both 2 (lower panel), using the data described. T1 T /T2g (upper panel) and T1 T /T2g

160 140

NQR T2G (μS)

120 100 80

500K

60 40 20 0 0

200

400

600

800

Temperature (K) Fig. 6.12. Plot of measured T2g for 63 Cu(2), taken on the NQR line of Y248. Data from the study of the dynamical crossover in Y248 by Curro et al. [4] are shown as solid circles. The open circles are from a previous study by Corey et al., [41]. Note the abrupt change of slope at 500 K. Reprinted ﬁgure from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

247

5000 (a) T1T/ T2G (K)

4000 3000 2000 500K

1000

(a)

0 0

200

400 600 Temperature (K)

800

80

T1T/ T2G2 (Kμs–1)

(b) 60

500K

40

20 (b) 0 0

200

400 600 Temperature (K)

800

Fig. 6.13. Data for T1 and T2g for 63 Cu(2) in Y248, plotted as T1 T /T2g vs. T (a) 2 vs. T (b) (closed circles). The (a) panel shows the scaling (QC: z=1) and as T1 T /T2g regime extending from T∗ ∼ 200 K to Tcr 500 K. The (b) panel shows the onset of the non-scaling (OD: z=2) regime at 500 K. The earlier data of Corey et al., [41] are shown as open circles. Reprinted ﬁgures from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

The upper panel data show that once past T∗ ∼ 200 K, T1 T /T2g remains very nearly constant up to the crossover Tcr 500 K, as expected for QC behavior. Above that point it veers upward very slightly. In the lower panel, the ratio 2 T1 T /T2g is plotted with the same data. Up to 500 K the latter ratio is seen to execute a downward path, levelling oﬀ at 500 K just where the putative entry into the OD phase should occur. This seems about as clear-cut a crossover as one could expect. Moreover, these data show that the transition from QC to OD behavior is relatively sharp. The foregoing identiﬁcation of the crossover was also corroborated by NMR shift data, which indicate (Fig. 6.14) a ﬂat maximum in the uniform susceptibility in the vicinity of 500 K. These data do not locate the crossover as

248

6 Dynamic Susceptibility Studies for the Cuprates

precisely as the dynamical plots, but they are consistent with the results in Fig. 6.13. The authors have also developed a procedure to observe the crossover directly in terms of ξ(T ). Using, ﬁrst, (6.4.3) with the coeﬃcient adjusted to give the BP predicted value 2.0˚ A at the crossover, they ﬁnd the bottom curve in Fig. 6.15 (triangles). Secondly, they have adopted the exact solution for the susceptibility of a Heisenberg AFM given by Sokol, Singh, and Elstner (SSE) [42] to give a second estimate of the ξ(T ) curve, where the latter workers also suggested that this would be a reasonable approximation to the behavior of lightly-doped cuprates at high temperatures [4]. The latter susceptibility is given by χ0 (T )[1 + θ(T )] , (6.4.4) χ(q, ω, T )SSE = 1 + θ(T )γ(q) + iΓq ω where γ(q) = 12 [cos qx + cos qy ], θ(T ) = 4ξ 2 (T )/[1 + 4ξ 2(T )], and Γq is a ﬂuctuation rate which is not required for χ (q, 0) (and thus T2g ). In using (6.4.4) to interpret the T2g data, the value of χ0 (T ) was taken from the NMR shift measurements, the known HF constants were used, and the second moment was calculated using the full expression (6.1.8). The only unknown parameter ξ(T ) is then extracted from the T2g data in Fig. 6.12. These values are plotted in Fig. 6.15 as open circles. According to this determination, ξ = 1.4 at the crossover temperature, somewhat less than the BP estimate. If the de-

0.25

63KS

⊥ (%)

0.20

0.15

0.10

0.05

0.00 0

100

200

300

400

500

600

700

800

Temperature (K) Fig. 6.14. The 63 Cu(2) NMR shift is plotted vs. temperature, showing the maximum of the uniform susceptibility at Tcr ∼ 500 K, in agreement with the plot of T2g (Fig. 6.12. Reprinted ﬁgure from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

249

termination using (6.4.3) is adjusted to give ξ = 1.4 at 500 K, then the curve with ﬁlled squares results, which is remarkably similar to the exact solution by SSE. In all three of the plotted curves for ξ(T ) vs. T there is a deﬁnite point very near to 500 K which one would naturally associate with a transition from one type of behavior to another, even if there had been no theoretical prediction of such a point. With the SSE susceptibility (6.4.4), however, there is a remarkably large change in the slope of the curve at Tcr , giving very dramatic evidence of the dynamical crossover. In conclusion, it seems that the QC, z = 1 behavior for AFM ﬂuctuations is clearly established for Y248 as well as for LSCO [39]. For Y248, the present work ﬁnds a clear-cut crossover transition at T 500 K. In the case of LSCO there is evidence for a crossover curve from susceptibility [43, 44] as well as Hall eﬀect data [34, 45]. It appears quite possible that a crossover curve for n plots as was done with Y248. LSCO could also be established using T1 T /T2g Measurements would probably have to be done with single-crystal samples and conducted in an oxygen atmosphere in order to maintain sample integrity at

0.9 0.8 0.7

(ξ /a)–1

0.6 0.5 0.4 0.3 0.2 0.1 0

200

400

600

800

Temperature (K) Fig. 6.15. Values of correlation length ξ(T ) derived from the data for T2g in Fig. 6.12 as follows: Triangles are from (6.4.3) with coeﬃcient adjusted to give ξ = 2.0 at T = 500 K. Open circles are from the SSE exact solution ([42]), where χ0 (T ) is derived from the shift data in Fig. 6.14. Closed squares are from (6.4.3) with the coeﬃcient adjusted to give ξ = 1.4 at T = 500 K. See text for interpretation of this result. Reprinted ﬁgure from N. Curro, T. Imai, C. P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

250

6 Dynamic Susceptibility Studies for the Cuprates

elevated temperatures (e.g. see [46]). It would be interesting and important to investigate the sharpness of the crossover transition in this fashion, since the present work has shown that this could be a very interesting issue [4].

References

1. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 213, 214 2. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 213, 214, 219, 220, 244 3. S. Ohsugi, Y. Kitaoka, K. Ishida, G-q. Zheng, K. Asayama, J. Phys. Soc. Japan 63,700 (1994) 214, 232, 233, 244, 245 4. N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 214, 244, 245, 2 5. D. Pines, C.P. Slichter, Phys. Rev. 100, 1014 (1955) 216 6. M. Takigawa, Phys. Rev. B49, 4158 (1994) 216, 220, 222, 223, 244 7. D. Thelen, D. Pines, Phys. Rev. B49, 3528 (1994) 216 8. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 217 9. T. Imai, C.P. Slichter, et al., Phys. Rev. B47, 9158 (1993) 217, 220, 221, 223, 244 10. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 217, 220, 221, 222, 223 11. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 219, 244 12. Y. Itoh, H. Yasuoka, et al., J. Phys. Soc. Japan 61, 1287 (1992) 220, 221, 224, 225, 226 13. N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 67, 2898 (1991) 221, 224, 225, 226 14. N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 68, 706 (1992) 221, 224 15. N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 221, 224, 225 16. A. Sokol, D. Pines, Phys. Rev. Lett. 71, 2813 (1993) 223, 242, 243, 244, 245 17. A. Uldry, M. Mali, J. Roos, P.F. Meier, J. Phys. Condens. Matter 17, L499 (2005) 225 18. T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 227, 233 19. R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 227, 230, 232, 20. S-W. Cheong, G. Aeppli, T.E. Mason et al., Phys. Rev. Lett. 67, 1791 (1991) 227, 228 21. T.E. Mason, G. Aeppli, H. Mook, Phys. Rev. Lett. 68, 1414 (1992) 227, 228, 229, 230, 231, 22. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 228 23. S.M. Hayden, G. Aeppli, H. Mook et al., Phys. Rev. Lett. 76, 1344 (1996) 228, 229, 230, 23 24. T.R. Thurston, P.M. Gehring, G. Shirane et al., Phys. Rev. B46, 9128 (1992) 228, 232, 236 25. G. Aeppli, T.E. Mason et al., Science 278, 1432 (1997) 230, 232, 240 26. K. Ishida et al., J. Phys. Soc. Japan 60, 2351 (1991) 233 27. B. Batlogg, in Physics of High-Temperature Superconductors, ed S. Maekawa and M. Sato, Springer Series in Solid-State Sciences, Vol. 106 (Springer-Verlag, Berlin, 1992), p. 219 233 28. K. Ishida et al., J. Phys. Soc. Japan 60, 3516 (1991) 233 29. D.C. Johnston, J. Magn. Magn. Mater. 100, 219 (1991) 233 30. T. Imai, C.P. Slichter, et al., Phys. Rev. Lett. 70, 1002 (1993) 233 31. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995) 233, 236, 237, 238, 239, 240, 241 32. M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991) 233 33. T. Imai et al., J. Phys. Soc. Japan 59, 3846 (1990) 234, 235 34. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 242, 243, 244, 246, 249 35. T. Moriya, Prog. Theor. Phys. 28, 371 (1962) 242, 243 36. C.M. Varma, Phys. Rev. B73, 155113 (2006) 243 37. Z.P. Han, R. Dupree et al., Phys. Rev. Lett. 69, 1256 (1992) 243

References

251

38. T. Moriya, Y. Takahashi, K. Ueda, Phys. Rev. Lett. 59, 2905 (1990) 244 39. R.E. Walstedt, S-W. Cheong, Phys. Rev. B53, R6030 (1996) 245, 249 40. A. Keren, H. Alloul, P. Mendels, Y. Yoshinara, Phys. Rev. Lett. 78, 3547 (1997) 245 41. R.L. Corey, N. Curro, et al., Phys. Rev. B53, 5907 (1996) 246, 247 42. A. Sokol, R.P. Singh, N. Elstner, Phys. Rev. Lett. 46, 4416 (1990) 248, 249 43. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 249 44. T. Nakano et al., Phys. Rev. B49, 16000 (1994) 249 45. H.Y. Hwang, B. Batlogg, H. Takagi et al., Phys. Rev. Lett. 72, 2636 (1994) 249 46. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B64, 014404 (2001) 250

A Appendices

A.1 Some Basic Properties of Spin Echoes We give in this appendix a brief discussion of the behavior of two-pulse spin echoes. For the original derivations of spin echo phenomena see the paper by Hahn [1]. A shorter exposition by this author discussed some special topics having to do with echo studies in solids [2]. A brief list is (i) echo behavior with phase variation between the pulses, (ii) the “area theorem” (see also below), (iii) computer simulation of echo proﬁles (of which Fig. 2.3 is an example), and (iv) the cancellation of spurious transient signals in echo studies using a four-step phasing sequence for the two excitation pulses. We begin with a basic derivation of the two-pulse echo, so that the amplitude dependence on pulse rotation angles, as well as the basic phenomenology of the T2 process are illustrated. At the same time the basic principle of spinecho double resonance (SEDOR) can be illustrated. In the ﬁnal subsection we derive the Gaussian echo decay time T2g associated with the indirect nuclear spin-spin couplings ﬁrst investigated in the cuprates by the Slichter group [3] and formulated conveniently in terms of χ (q) by Pennington and Slichter [4]. A.1.1 Basic Derivation of the Two-Pulse Spin Echo. Spin echoes are generally observable with spin systems where the echo decay time is long enough so that two excitation pulses can be applied at some minimal pulse spacing, after which the echo signal can be detected following the “dead time” of the receiver. Another requirement for echo generation which is often overlooked is that the observed nuclei must be subject to a quasi-static broadening eﬀect which is greater than any homogeneous or dynamic broadening. This circumstance can come about through an internal distribution of shifts, HF ﬁelds, EFG values, quasi-static interactions with other spin systems or through the application of an inhomogeneous ﬁeld. If you have a homogeneously broadened NMR line relaxed by ﬂuctuating like-spin couplings or by

R.E. Walstedt: Appendices, STMP 228, 253–261 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 A

254

A Appendices

T1 , you may be able to see the free-induction signal, but the echo will be very elusive. Supposing these conditions are met, let us consider the application of rf pulses to excite an echo. For simplicity, we shall suppose the excitation pulses to be of negligible length. One imagines, then, a very large rotating magnetic ﬁeld H1 (at a suitable frequency) applied for just an instant, during which the magnetization of the nuclei nutates at ω1 = γH1 away from its equilibrium position along the z axis. At time tw1 the magnetization has rotated by θ1 = ω1 tw1 , creating a magnetization component M0 sin θ1 along the x axis. Following the ﬁrst pulse, the spins are allowed to precess freely for a time τ , during which time the transverse magnetization decays quickly to zero. The associated free-induction signal is typically too short to be observed. This decay time is labelled T2∗ , being either the inverse of the width Δ of the distribution P (Δi ) of static frequencies being excited or in a broad line T2∗ ∼ π/ω1 . We consider our typical nuclear spin I i to be subject to a local, static frequency perturbation Δi . We also introduce one source of echo relaxation perturbations, namely the spin-spin coupling term (i) = αij Izi Izj = Ωi Izi , (A.1.1) HII j

where the resulting local frequency perturbation Ωi = j αij mj contributes to the precession frequency between rf pulses. The perturbation Ωi could come from like or unlike spins, and could be ﬂuctuating or static, with results which vary enormously depending on the details. We shall proceed with the calculation assuming the Ωi ’s are static, and then comment on other possible cases. During the interval between the ﬁrst and second pulses, spin I i will precess around the z axis, where in the rotating frame, the transverse component of spin i in the xy-plane precesses through an angle (Δi + Ωi )τ , where Δi and Ωi are as deﬁned above. To capture the eﬀects of these motions we follow the development in the rotating frame1 of the density matrix ρ∗ (t) which obeys the equation of motion [5] i

dρ∗ = [H∗ , ρ∗ ] , dt

(A.1.2)

where starred quantities have been transformed into the rotating frame. For simplicity we drop the star notation, noting that the rest of the calculation will take place in the rotating frame. The initial value of density matrix is ρ0 Ix , where ρ0 ∝ sin θ1 . During the interval τ between pulses and during time interval t − τ following the second pulse, spin I i will precess through the angles (A.1.3) β1i = (Δi + Ωi )τ and β2i = (Δi + Ωi )(t − τ ) , 1

The rotating frame is a reference frame rotating at the frequency of the applied rf pulses.

A.1 Some Basic Properties of Spin Echoes

255

respectively, where at time τ a second pulse of rf ﬁeld H1 is applied, rotating the spins through angle θ2 . The θ2 pulse is known as the “refocussing pulse”. At time t − τ following the latter pulse, the density matrix may be written ρ(t) = exp(iβ2i Izi ) exp(iθ2 Iy ) exp(iβ1i Izi ) Ixi ρ0 exp(−iβ1i Izi ) exp(−iθ2 Iy ) exp(−iβ2i Izi )i ,

(A.1.4)

where the brackets i indicate an average over the entire sample. In (A.1.4) only the exponential operators which survive in the echo amplitude calculation, i.e. in T r(Ix ρ(t)), are kept. At this point we make some remarks about the potential eﬀects of the broadening terms β1,2i in (A.1.4). These terms can always be divided into separate operators exp(iIzi Δi t) exp(iIzi Ωi t), where the eﬀect of the static Δi ’s is particularly simple. If the Ωi terms are static and unaﬀected by the θ2 pulse, then they have no eﬀect and will simply disappear from the calculation. If they are like-spin terms and are aﬀected by the θ2 pulse, then they cause an echo relaxation process. In the next subsection we develop expressions for the θ2 -dependent relaxation time T2g for the Gaussian relaxation from indirect spin-spin coupling in cuprates [4]. If the Ωi terms are from unlike spins, then there is a series of possible eﬀects. If, for example, an rf pulse is applied to the I spins so that their mj values (and thus the Ωi ’s) change, then the echo will undergo a potentially observable eﬀect known as spin echo double resonance (SEDOR). SEDOR has undergone various applications to solid-state science [6, 7], but we shall not discuss this technique further. If the unlike-spin Ωi ’s are ﬂuctuating in time, then there will be an associated echo relaxation process of a character which depends on whether the ﬂuctuations are slow, fast, or intermediate. If the ﬂuctuations are fast or slow, then some estimate of their eﬀects can be obtained with perturbation methods. If they are intermediate in speed, then the eﬀects could be very large and treatment would have to be improvised on a case-by-case basis. In the case where the Ωi ’s are time-dependent between the rf pulses, then it is easy to show that the Ωi τ etc. in (A.1.3) would simply be replaced by τ

Ωi τ →

Ωi (t)dt.

(A.1.5)

0

We now proceed to obtain a general expression for the echo signal from the foregoing expressions. In (A.1.4) only the exponential operators which survive in the echo calculation have been kept. These exponential operators are processed using the relation exp(iφIγ ) Iα exp(−iφIγ ) = Iα cos φ ∓ Iβ sin φ ,

(A.1.6)

where the second term is negative if (α, β, γ) is a positive permutation of (x,y,z) and positive otherwise.

256

A Appendices

Following development of ρ(t) using (A.1.6), we keep only the terms in Ixi , which form the principal component of the echo. The corresponding signal amplitude can then be written E(t) =

1 E0 (1 + cos θ2 )cos(β1i + β2i ) − (1 − cos θ2 )cos(β1i − β2i )i , (A.1.7) 2

is deﬁned below. The echo signal at t = 2τ arises only from the where β1i second term, which becomes ⎛ ⎞ E(t) = (1 − cos θ2 ) P (Δi )cos ⎝Δi (t − 2τ ) + αij [mj τ − mj (t − τ )]⎠ , E0 i j

(A.1.8) ) is the value of mj following the operation eiθ2 Izj e−iθ2 . where mj (deﬁning β1i We shall make use of this in Sect. A.2. The average over the distribution of Δi values gives the time proﬁle of the echo, which has its maximum at t = 2τ . The two terms in the cos argument ( ) in (A.1.8) are very diﬀerent in character. The Δi term vanishes at t = 2τ , but is otherwise large and rapidly varying. The second, relaxation term is a slowly varying perturbation. In a reasonable approximation we evaluate the second term at t = 2τ and separate it from the ﬁrst one and remove it from the sum as a relaxation factor fr (2τ ) = cos[ j αij (mj − mj )]j , where the

j brackets indicate a second, independent averaging process. (A.1.8) is then rewritten as E(t) = C sin θ1 (1 − cos θ2 ) fr (2τ ) P (Δi )cos[Δi (t − 2τ )], (A.1.9) i

where the average over the Δi ’s gives the echo shape function, and where we have inserted sin θ1 to give the full dependence on pulse angles. We now make some observations on the echo expression (A.1.9). First, we recount the area theorem for spin echoes. Although not developed in detail in this derivation (see [2]), an echo excited from a distribution g(ω) of NMR/NQR frequencies is an integral of that distribution over excitation factors, giving an echo proportional to ∞ dω g(ω) sin θ1 (1 − cos θ2 ) cos[(ω − ω0 )(t − 2τ )], (A.1.10) −∞

where the distribution P (Δi ) is eﬀectively replaced by g(ω). If we integrate the area under the echo, i.e. over a range −Δt ≤ t − 2τ ≤ Δt which includes all possible nonzero echo amplitude, this produces delta function in frequency so that 2τ +Δt E(t)dt = 2πC fr (2τ )g(ω0 ) [sin θ1 (1 − cos θ2 ]ω0 , (A.1.11) 2τ −Δt

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling

257

where if the pulse angles are frequency-dependent, they are evaluated at ω0 , which is the frequency of the rf pulses. Thus, the area under the echo is very precisely proportional to g(ω0 ), with a resolution which does not depend on H1 (in principle), but on the the time 2Δt over which the integration can take place. In general the resolution of g(ω0 ) is very good. In practice, the smaller H1 is, the better the resolution which is obtained. A.1.2 Modelling Spin-Echo Decay Secondly, as an example of spin-echo decay, we consider the form which fr (2τ ) from (A.1.9) takes in the limit where the mj ’s are from unlike spins and are ﬂuctuating rapidly. We therefore consider the quantities Ωi (t) to be stochastic variables, where τ ! 2τ Ωi (t)dt − Ωi (t)dt . (A.1.12) fr (2τ ) = cos 0

τ

i

The two integrals over time are equivalent under the average over i, so we expand the cosine, assuming the sine terms to vanish on averaging. Expanding the remaining cosines in power series and keeping just the ﬁrst two terms we ﬁnd τ τ dt dt Ωi (t)Ωi (t )i + · · · . (A.1.13) Fr (2τ ) 1 − 0

0

Taking the indicated average i generates a correlation function which we ∞ write as Ωi2 i C(| t − t |), where 0 C(t)dt = τc τ . The ﬁrst expansion term is therefore linear in τ so that the decay function may be approximated as (A.1.14) fr (2τ ) e−2τ /T2Ω , with 1/T2Ω = Ωi2 τc . The foregoing is an example of exponential spin-echo decay with a rapidly modulated perturbation. Another such eﬀect is echo decay through spin-lattice interactions. This is discussed in some detail in Appendix A.2.1. In the next subsection we give an example of Gaussian spin-echo decay through modulation of like-spin interactions by the refocussing (θ2 ) pulse, which is widely encountered in cuprate NMR studies.

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling The following calculation of spin-echo decay applies to magnetic dipole transitions excited between any pair of HF energy levels for which m = Iz (suitably chosen) is a reasonably good quantum number, i.e. a Δm = ±1 transition. Examples are (i) any high-ﬁeld transition with quadrupolar splittings or (ii) a zero-ﬁeld NQR splitting. For NQR lines with, e.g. I = 3/2, the excitation

258

A Appendices

pulses excite two transitions simultaneously (± 12 ↔ ± 32 ) with their separate signals. We shall be considering the decay of only one of these signals at a time, though the calculation will apply to both. We henceforward consider only the echo amplitude E(2τ ) given by (A.1.8), which can be expanded as a power series in (2τ )2n , where we keep only the τ 2 term: ⎡ ⎤2 τ 2 ⎣ E(2τ ) ≈ E0 (1 − cos θ2 ) 1 − αij (mj − mj )⎦ . (A.2.1) 2 j

i

In squaring the sum j αij (mj − mj ) the cross terms will average to zero. In the diagonal terms the quantity (mj − mj )2 will equal 1 with a probability sin2 (θ2 /2) and will be zero otherwise. (A.2.1) becomes [8] ⎤ ⎡ 2 τ (A.2.2) α2ij ⎦ , E(2τ ) E0 (1 − cos θ2 ) ⎣1 − sin2 (θ2 /2) 2 j where the j indicates a sum only over 63 Cu(2) neighbors which are being ﬂipped by the θ2 pulse. This means, typically, couplings with the same isotope, and mj -values belonging to the resonance transition observed. In high-ﬁeld NMR for I = 3/2, this means half of the neighbor spins. For NQR with I = 3/2, one sums all of the neighbor spins, because they are all part of the observed resonance. The diﬃculty in applying this is, of course, that often the line is broad and the θ2 pulse is not uniform over all of the spins. The factor sin2 (θ2 /2) in such a case is an eﬀective average value. If we suppose that (A.2.2) gives the ﬁrst two expansion terms of a Gaussian decay, then we have for the ﬁnal result for a high-ﬁeld NMR transition for 63 Cu(2), c63 2 1 2 = sin (θ /2) α , (A.2.3) 2 2 T2g 8 j ij where the ﬁnal sum over all neighbor sites is, of course, independent of i. In naturally abundant 63 Cu c63 0.69. A.2.1 Indirect Coupling with a Gaussian Susceptibility The indirect coupling range function used in the text is discussed here for the simple case of a q-independent, isotropic HF tensor and a Gaussian susceptibility χ (q). After deriving the range function from (5.1.7), results for the second moment ( j(=i) a2ij ) obtained in several ways are discussed. The general result for the indirect coupling coeﬃcient of Izi Izj is aα (i, j) =

eiq·(Rj −Ri ) χα (q)Fαα (q)2 , NA gα2 μ2B q

(A.2.4)

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling

259

where the prefactor is suited to a molar susceptibility and an HF tensor in units of s−1 . Here we take Fαα (q) = A0 , and we use the Gaussian susceptibility form employed by Auler et al. [9], which is χα (q) = χAF e−(q−Q)

2 2

ξ /4

.

(A.2.5)

Since χα (q) is symmetric about Q, we move the origin to that point with q = p+(π, π). The imaginary sine term is then seen to vanish by symmetry. For simplicity we drop the prefactor (χAF A20 /NA gα2 μ2B ) and restore it at the end. The sums may then be taken as integrals, giving, π 2 2 2 (−1)(nx +ny ) π dp dpy e−(px +py )ξ /4 cos(nx px + ny py ) . a(i, j) = x 4π 2 −π −π (A.2.6) The cosine factor can be written cos(nx px ) cos(ny py ), since the sine terms vanish. The integrals can now be written g(nx )g(ny ), where 2 2 (−1)n π (−1)n −n2 /ξ2 g(n) = dpe−p ξ /4 cos(np) √ , (A.2.7) e πξ π 0 where the last step approximates the upper limit of the integral as ∞. This is a reasonable approximation, since the exponential factor at p = π is 0.015. We shall check this approximation below, as well. The ﬁnal result for our dimensionless range function is (−1)(nx +ny ) −(n2x +n2y )/ξ2 e . (A.2.8) πξ 2 We now evaluate the second moment sum j(=i) a(i, j)2 in three separate ways, in order to test the approximation in (A.2.7). First, we may do this directly with (A.2.8), giving the expression ⎡ ⎤ 2 2 2 1 a(i, j)2 = 2 4 ⎣ e−2(nx +ny )/ξ − 1⎦ , (A.2.9) π ξ n ,n a(i, j) =

j(=i)

x

y

where the summation is over all integer values of nx , ny which would give an appreciable contribution. In what may seem a crude approximation for ξ 1.3 (see text), we evaluate the sums in (A.2.9) as an integral in a continuum approximation. This is straightforwardly shown to yield the value πξ 2 /2, so that we ﬁnd 2 1 πξ 2 −1 . (A.2.10) a(i, j) = 2 4 π ξ 2 j(=i)

The foregoing result gives the value j(=i) a(i, j)2 = 0.0587 for ξ = 1.3, which is the minimum value we shall use it for. This sum has also been evaluated by computer for the same value of ξ, giving 0.0588 for the result. It seems

260

A Appendices

then that the continuum approximation to the (nx , ny ) sums is accurate to a fraction of a percent. However, the range function itself is an approximate result from (A.2.7). We make a check on the latter result by evaluating the second moment sum using the q-space result (6.1.8), which in the present context becomes 2 −(q2 +p2 )ξ 2 /4 −q2 ξ 2 /4 a(i, j) = e − e . (A.2.11) q

j(=i)

p

q

When the ﬁrst sum is converted to an integral in polar coordinates, the integrand is porportional to exp(−q 2 ξ 2 /2), which, at q = π falls to the value ∼ 2.4 × 10−4 . While this could be accounted for in approximate fashion, we neglect errors of this magnitude for simplicity here. This term then becomes 1/(2πξ 2 ). The second term in (A.2.11) can be cast into a very similar form as that of (A.2.7), where we neglect a correction term of the order of 1.5%. Since this is squared, neglecting these correction means that the second term in (A.2.11) is small by about 3%. The two terms together give j(=i) a(i, j)2 = 1/(2πξ 2 ) - 1/(π 2 ξ 4 ), which is identical to the summing result in (A.2.10). We now see that for ξ = 1.3, this result probably errs on the high side by an amount of order 1%. For larger values of ξ the error will diminish rapidly. Restoring the prefactor and multiplying by the factor c63 /8 gives the physically correct second moment (or (1/T2g )2 ), which is 2 1 πξ c63 χAF A20 1 c63 − 1 . (A.2.12) a(i, j)2 = = T2g 8 8 NA gα2 μ2B ) π 2 ξ 4 2 j(=i)

A.3 Spin Echo Decay via Spin-Lattice Relaxation Spin-lattice relaxation of a spin echo was ﬁrst treated to explain the large disparity between conventional T1 values and the enhanced exponential decay rates 1/T1E of spin echoes for nuclear spins with large I values [10]. The relaxation rate for the (− 12 ↔ 12 ) transition was shown to be 1/T1E = 2 W0 (I + 1 2 2 ) , where 1/T1 = 2 W0 . This result was modiﬁed for the case of an anistropic T1 process by Narath [11], ﬁnding 1 T1Ez

= (Wx + Wy )[I(I + 1) − 1/4] + Wz ,

(A.3.1)

where Wα is the contribution of ﬂuctuations along the α axis to the relaxation rate for a quantization axis perpendicular to that axis. Thus, 1/T1z = Wx +Wy . The latter results have been derived using the “ﬁctitious spin 12 ” technique. They have been derived using other methods as well [3, 12]. Since the Wα ’s are not measured directly, it is also useful to express the result (A.3.1) in terms of the anisotropic T1 values T1x,y,z :

References

1 T1Ez

=

1 1 1 [I(I + 1) − 3/4] + + . T1z 2 T1x 2 T1y

261

(A.3.2)

We also treat the case of arbitrary direction for the quantization axis, represented by the Euler angles (θ, φ). We let that be the z axis with corresponding x axis in the xy plane and mutually perpendicular y axis. The associated rate parameters for the (x , y , z ) axes are Wx = Wx sin2 φ + Wy cos2 φ 2

2

(A.3.3a) 2

2

2

Wy = Wx cos θ cos φ + Wy cos θ sin φ + Wz sin θ Wz = Wx sin2 θ cos2 φ + Wy sin2 θ sin2 φ + Wz cos2 θ ,

(A.3.3b) (A.3.3c)

whereupon 1/T1Ez is given in terms of the Wα ’s by (A.3.1). This result was used to correct the planar 17 O spin echo decay data in [8] for T1 eﬀects.

References 1. E.L. Hahn, Phys. Rev. 80, 580 (1950) 253 2. R.E. Walstedt, “The two-pulse spin echo revisited”, in Pulsed Magnetic Resonance: NMR, ESR and Optics, ed. by D.M.S. Bagguley (Clarendon Press, Oxford, 1992), p. 242 253, 256 3. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 253, 260 4. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 253, 255 5. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 254 6. D. Kaplan and E.L. Hahn, J. Phys. Radium 19, 821 (1958) 255 7. R.E. Walstedt and J.H. Wernick, Phys. Rev. Lett. 20, 856 (1968) 255 8. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995) 258, 261 9. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 259 10. R.E. Walstedt, Phys. Rev. Lett. 19, 146 (1967); 19, 816 (1967) 260 11. A. Narath, Phys. Rev. B13, 3724 (1976) 260 12. T. Imai et al., Phys. Rev. Lett. 71, 1254 (1993) 260

Index

AFM enhancement eﬀects below Tc , 109, 111 AFM ﬂuctuations, 5 antiferromagnetic correlations, 4, 90, 102 ARPES studies of cuprates, 2, 136 ARPES studies of energy gap eﬀects, 136 axial EFG symmetry, 15 axial shift component for 17 O(2,3) in YBCO7, 95 axial shift powder patterns, 23 BCS energy gap anisotropy from coherence peak, 43 BCS energy gap value from T1 in Al metal, 43 BCS theory of T1 for T < Tc , 41 BCS theory of T1 for the d-wave case, 108 characterization of samples, 4, 5 chemical shifts in NMR, 21, 118, 120, 122, 233 χ (q, ω), 5, Sect. 3.5, Chap. 5, 6 χ (q, 0)values derived from T2g measurements, 220 coherence factor: T1 for T < Tc , 40 coherence peak, gap anisitropy eﬀect, 43 core diamagnetic susceptibility for YBCO, 83 core polarization of Y3+ , 78

core–polarization T1 process in d-band metals, 51 core–polarization HF ﬁeld, 44 core–polarization HF mechanism, 46 core–polarization NMR shift, 5, 48, 58 crossover in phase diagram, 70, 146, 243, 246 63,65 Cu, 4 Cu(1,2) site assignment, 75 cuprate phase diagram, 3, 70, 146, 243 d–wave pairing, 6 d-wave conﬁrmation by T2g for T < Tc , 225 d-wave model for T1 at T < Tc , 104, 206 detailed balance in spin–lattice relaxation, 25 Dipolar Contribution to 89 Y HF Coupling, 125, 183 dipolar HF interaction, 33 dipolar NMR shift, 5 discovery of high–Tc , 1 dynamic susceptibility, Sect 3.5, Chap. 5, 6 dynamical structure factor, 101 dynamical susceptibilities for LSCO:x from INS data, 230 dynamical susceptibility, a simpliﬁed model, 127 dynamical susceptibility, exact solution for Heisenberg AFM, 248 dynamical susceptibility, Gaussian model, 180

264

Index

dynamical susceptibility, RPA model, 173 EFG Tensor, 14 exchange enhancement from K(α)– table, 37 Exchange enhancement of 1/T1 – Moriya theory, 36 Fermi surface in cuprates, 2, 136 Ferrell–Anderson theory of spin–orbit scattering below Tc , 39 ﬁeld–dependent T1 eﬀects in type–II superconductors, 61, 111, 200 ﬁrst-order quadrupolar broadening, 15, 94 ﬂuctuation dissipation theorem, 101 ﬂuctuation-dissipation theorem, 5 g–factors for YBCO7, 86 gamma, nuclear gyromagnetic ratio, 21 Ginzburg-Landau parameterκ, 54 Ginzburg-Landau theory, 54 gyromagnetic ratio, nuclear moment, 21 Hamiltonian for NMR/NQR spectra, 14 HF coeﬃcients for YBCO6.63 from scaling of shifts, 123 HF constants for LSCO:0.15 from NMR shift data, 232 HF couplings, 4, 82 HF Hamiltonian–general, 33 HF tensor for 89 Y in YBCO7, 96 HF tensor for 17 O(2,3) in YBCO7, 96 HF tensor, general, for cuprates, 82 HF tensors for YBCO7, 84 hole doping, 3 hole doping in cuprates, 71 Hubbard model calculation of NMR shift below Tc , 205 Hubbard model for T1 at T < Tc , 199 Hubbard model, large U, of spin dynamics, 192 Hubbard model, negative U, 127 Hubbard model, small U, for spin dynamics, 187 indirect spin–spin coupling, 6, 19, 214 indirect spin–spin coupling in LSCO:0.15 from INS data, 239

INS data for χ (q, ω), case of pseudogap, 128 INS data for χ (q, ω) in LSCO:x, 227 INS studies of cuprates, 2, 128, Chap. 6 K–χ analysis, 47 K–χ plot for Pt metal, 48 Knight shift, 32 Knight shift for T < Tc : BCS (Yosida) theory, 38, 108, 206 Korringa calculation of T1 in metals, 34 Korringa product table for metals, 35 Korringa relation, 35, 37 Korringa relation, modiﬁed for multiple HF sources, 127 Korringa relaxation, 33 Kramers–Kronig evaluation of χ (q, 0)for LSCO:0.15, 240 LSCO phase diagram, 2, 46, 70 LSCO structure, 68 LSCO, 63,65 Cu T1 data, 153, 245 LSCO:x, 2 LSCO:x dynamical susceptibility from INS, 227 LSCO:x, 17 O T1 and shift data, 153, 241 LSCO:x, NMR shifts, 152 LSCO:x, NQR spectra, 153 LSCO:x, pseudogap eﬀects, 148, 241 LSCO:x, scaling of susceptibility, 149 Mila–Rice HF tensor, 81 Mott insulator, 1, 69 NMR in d–band metals, 44 NMR probe, 4 NMR shift deﬁned, 22 NMR shift below Tc , Hubbard model calculation, 205 NMR shift correction for superconducting diamagnetism, 105 NMR shift for cuprates at T < Tc , 105 NMR shift in the mixed state of 3d superconductor, 57 NMR shift tensor, 14, 21 NMR shift tensor, scalar approximation, 22 NMR shift tensors for Cu(1) in YBCO7, 84

Index NMR shift tensors for Cu(2) in YBCO7, 84 NMR shift, anisotropic, powder pattern, 23 NMR shift, powder pattern, 23 NMR spectra, 5 NMR spectrum, quadrupolar satellites, 15 NMR studies in the mixed state of type–II superconductors, 55 NQR determination of η, 17 NQR spectrum in zero ﬁeld, 17 17

O(2,3), 5 O doping, 4 17 O EFG tensors for YBCO7, 95 17 O NMR data for YBCO7, 93, 162 17 O relaxation in YBCO7, 92 17 O shift tensors for YBCO7, 75, 95, 164 orbital T1 process in d-band metals, 51 orbital T1 theory by Varma, 195 orbital (Van Vleck) shift and susceptibility – general, 46 orbital HF interaction, 33 orbital NMR shift, 5 orbital shift and T1 process, 44 orbital susceptibilities for YBCO, 83 orbital susceptibility tensors in YBCO7, 85, 86 oriented powder samples for cuprate NMR, 80 orthorhombic phase of LSCO:x, 3, 69 oxygen hole band in YBCO7, 98 oxygen hole bands, 72, 81 17

Pennington Slichter theory of indirect spin–spin coupling, 214 phase diagram for scaling theory of AFM ﬂuctuations, 242 phase diagram of cuprate superconductor, 2, 146, 243 phenomenology of high–Tc , 1 pseudogap eﬀects for YBCO6+x vs. x, 117 pseudogap eﬀects on T1 in underdoped YBCO, 116 pseudogap energy derived from Arrhenius plot, 122, 143

265

pseudogap isotope eﬀect, Y248, 143 pseudogap NMR shift scaling in YBCO6.63, 120 pseudogap temperature, 3 pseudogap, theory by Varma, 146 pseudogaps in cuprates, 115 quadrupolar eﬀects, 4 quadrupolar perturbation, high–ﬁeld limit, 15 quadrupolar powder pattern, 16, 23 quadrupolar powder pattern, second order, 16, 23 quadrupolar tensor, sign of, 15 quantum chemistry of YBCO7, 87 resonant ﬁeld shifts, relation to K, 22 review of bulk properties, 4 RPA calculation of dynamical susceptibility, Monien and Pines, 108 s-contact (Knight) shift, 33, 47 s-contact HF interaction, 33 s-contact NMR shift, 5, 33, 47 saturating comb to measure T1 , 31 scaling theory of χ(q, ω) in quantum critical region, 242 shift vs. susceptibility analysis, 47 simulations of spin–echo decay for LSCO:0.15, 236 speciﬁc heat, pseudogap eﬀects, 134 spin echo spectroscopy, frequency resolution, 19 spin echo, observation of, 20 spin echo, two–pulse, 18, 251 spin Hamiltonian parameters for 63 Cu(2) in YBCO7, 86 spin HF tensor for Cu(2) in YBCO, 89 spin susceptibilities for YBCO, 83 spin susceptibility anisotropy for YBCO7, 86 spin–echo decay, 6, 20, 251, 255 spin–echo decay analysis for LSCO:0.15 from INS data, 236 spin–echo decay by indirect spin–spin coupling, 218, 255 spin–echo decay via T1 , 20, 258 spin–lattice relaxation, deﬁnition, 23

266

Index

spin–orbit NMR shift, 5, 89 spin–orbit scattering eﬀect on susceptibility for T < Tc , 39 spin–spin correlations below Tc , ab plane, 207 spin–spin correlations below Tc , c axis, 208 spin–spin correlations in terms of χ (q, ω), 102 Spin-spin below Tc , Uldry-Meier analysis, 207 spin-spin correlations in YBCO7, 91, 161, 165 Stoner enhancement of susceptibility, 189 structures of compounds with CuO2 , 2, 69 superconducting diamagnetism, 5, 55 susceptibility – uniform, 5, 33, 38, 45 susceptibility analyses for V3 X compounds, 49 susceptibility anisotropy in YBCO7, 87 symmetry factors in d–band T1 processes, 51 T1 at T < Tc , Hubbard model, 199 T1 eigenmodes, 25, 27 T1 ﬁt for T < Tc by Monien and Pines, 110 T1 ﬁtting parameters for T < Tc , Monien and Pines, 110 T1 for 17 O in YBCO7, 97 T1 for d–band metals, 50 T1 formulated in terms of χ (q, ω), 99 T1 in mixed state via spin diﬀusion to normal cores, 62 T1 measurement techniques, 27 T1 measurements for T < Tc : simple metals, 41 T1 model for YBCO using INS data, 179 T1 model for cuprates by Millis, Monien, and Pines, 172 T1 models for cuprates, 159 T1 parameterization by Uldry and Meier, 160 T1 ratios in YBCO7, Mila–Rice interpretation, 90 T1 recovery for (− 21 ↔ 12 ) transition, 28

T1 T1 T1 T1 T1

recovery for NQR, 28 recovery with inversion, 28 recovery with saturation, 28 recovery with spectral diﬀusion, 29 studies in type–II superconductors, 58 T1 with q–dependent structure factors, 101 T1 with Gaussian model compared with UM analysis, 184 T1 , deﬁnition, 23 T1 , magnetic dipolar processes, 23 T1 , quadrupolar processes, 23 T1 : Quadrupolar vs. magnetic dipole, 24 T1 ’s for LSCO:0.15 calculated from INS data, 230 T2 decay for 17 O in LSCO:0.15, 240 T2 for spin echoes, 19, 251, 255 T2 , deﬁnition, 19 T2g , 6, 255 T2g dependence on correlation length, 222 T2g used to calibrate dyanmical susceptibility, 182 T2g values from various systems, 220 T2g variation below Tc , Hubbard model, 224 T2g variation with temperature, 223 T2g , Gaussian model for, 217 t-J model of quasiparticle behavior, 71 tetragonal phase of LSCO:x, 3 transferred HF coupling in cuprates, 81 Type–II superconductivity in d–band metals, 54 Type–II superconductor NMR studies, 53 Wannier wavefunction for Cu(2) – Mila Rice model, 88 89

Y, 4, 5 Y HF coupling from dipolar interaction, 183 89 Y chemical shift by extrapolation, 122 89 Y relaxation in YBCO7, 92 Y248, 2, 74, 92, 118, 160, 175, 181 Y248 analysis by Uldry and Meier, 169 Y248 dynamical crossover T1 T /T2g study, 245 89

Index Y248, NMR shift and T1 , 139 Y248, pseudogap behavior, 138 Y248, pseudogap energy, 141 YBCO structure, 70 YBCO, evaluation of HF coeﬃcients, 83 YBCO, introduction of the Spin Hamiltonian model for 63 Cu(2), 79 YBCO6+x, chemcal shift of 89 Y, 77 YBCO6+x, variation of 89 Y shift with x, 76 YBCO6.63 analysis by Uldry and Meier, 167 YBCO6.63 discussion by Millis, Monien, and Pines, 178 YBCO6.63 pseudogap NMR data, 117 YBCO6.63, 89 Y T1 behavior, 132 YBCO6.63, T1 data, 130 YBCO7, 4

267

YBCO7 T1 modeling by Millis, Monien, and Pines, 175 YBCO7 - early results on 63,65 Cu NMR studies, 73 YBCO7 – 63,65 Cu T1 data, 74 YBCO7 – 63 Cu(2) powder pattern, 76 YBCO7 – early NMR results, 72 YBCO7 – NQR studies, 74, 111 YBCO7 analysis by Uldry and Meier, 163 YBCO7, 63 Cu(2) T1 anisotropy, 79 YBCO7, 63 Cu(2) relaxation models, 79, 159 YBCO7, early results on 89 Y NMR, 73 YBCO7-x, 2 Yosida function calculation for cuprates, 108 Yosida function measurement in Al metal, 40 Zhang–Rice singlet, 70

Starting with Volume 165, Springer Tracts in Modern Physics is part of the [SpringerLink] service. For all customers with standing orders for Springer Tracts in Modern Physics we offer the full text in electronic form via [SpringerLink] free of charge. Please contact your librarian who can receive a password for free access to the full articles by registration at: springerlink.com If you do not have a standing order you can nevertheless browse online through the table of contents of the volumes and the abstracts of each article and perform a full text search. There you will also find more information about the series.

Springer Tracts in Modern Physics Springer Tracts in Modern Physics provides comprehensive and critical reviews of topics of current interest in physics. The following fields are emphasized: elementary particle physics, solid-state physics, complex systems, and fundamental astrophysics. Suitable reviews of other fields can also be accepted. The editors encourage prospective authors to correspond with them in advance of submitting an article. For reviews of topics belonging to the above mentioned fields, they should address the responsible editor, otherwise the managing editor. See also springer.com

Managing Editor Gerhard H¨ohler Institut f¨ur Theoretische Teilchenphysik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 33 75 Fax: +49 (7 21) 37 07 26 Email: [email protected] www-ttp.physik.uni-karlsruhe.de/

Elementary Particle Physics, Editors Johann H. K¨uhn Institut f¨ur Theoretische Teilchenphysik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 33 72 Fax: +49 (7 21) 37 07 26 Email: [email protected] www-ttp.physik.uni-karlsruhe.de/∼jk

Thomas M¨uller Institut f¨ur Experimentelle Kernphysik Fakult¨at f¨ur Physik Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 35 24 Fax: +49 (7 21) 6 07 26 21 Email: [email protected] www-ekp.physik.uni-karlsruhe.de

Fundamental Astrophysics, Editor Joachim Tr¨umper Max-Planck-Institut f¨ur Extraterrestrische Physik Postfach 13 12 85741 Garching, Germany Phone: +49 (89) 30 00 35 59 Fax: +49 (89) 30 00 33 15 Email: [email protected] www.mpe-garching.mpg.de/index.html

Solid-State Physics, Editors Atsushi Fujimori Editor for The Pacific Rim Department of Physics University of Tokyo 7-3-1 Hongo, Bunkyo-ku Tokyo 113-0033, Japan Email: [email protected] http://wyvern.phys.s.u-tokyo.ac.jp/welcome en.html

C. Varma Editor for The Americas Department of Physics University of California Riverside, CA 92521 Phone: +1 (951) 827-5331 Fax: +1 (951) 827-4529 Email: [email protected] www.physics.ucr.edu

Peter W¨olfle Institut f¨ur Theorie der Kondensierten Materie Universit¨at Karlsruhe Postfach 69 80 76128 Karlsruhe, Germany Phone: +49 (7 21) 6 08 35 90 Fax: +49 (7 21) 6 08 77 79 Email: [email protected] www-tkm.physik.uni-karlsruhe.de

Complex Systems, Editor Frank Steiner Institut f¨ur Theoretische Physik Universit¨at Ulm Albert-Einstein-Allee 11 89069 Ulm, Germany Phone: +49 (7 31) 5 02 29 10 Fax: +49 (7 31) 5 02 29 24 Email: [email protected] www.physik.uni-ulm.de/theo/qc/group.html

R.E. Walstedt

The NMR Probe of High-Tc Materials

123

Russell E. Walstedt University of Michigan Department of Physics Ann Arbor, MI 48104, USA [email protected]

R.E. Walstedt, The NMR Probe of High-Tc Materials, STMP 228 (Springer, Berlin Heidelberg 2008), DOI 10.1007/ 978-3-540-75565-4

Library of Congress Control Number: 2007936864 Physics and Astronomy Classification Scheme (PACS): 76.60.- K NMR STUDIES IN GENERAL C UPRATE S UPERCONDUCTORS 74.72.- H ISSN print edition: 0081-3869 ISSN electronic edition: 1615-0430 ISBN 978-3-540-75564-7 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com c Springer-Verlag Berlin Heidelberg 2008 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting: by the authors and Integra using a Springer LATEX macro package Cover design: eStudio Calamar S.L., F. Steinen-Broo, Pau/Girona, Spain Printed on acid-free paper

SPIN: 11935247

543210

To Erwin, Vince, and Hiroshi

Preface

To the old saying that if you want to learn something about a subject, teach a course on it, I would add the much more arduous option of writing a book about it. The upside, of course, is that you may gain a perspective on a longtime favorite subject which can be achieved in no other way. The fact is that the opportunity to write such a book as this is, indeed, a rare opportunity. This is especially so for someone who, by the calendar, is well into retirement years. While high Tc itself is the opportunity of a lifetime for those of us who experienced it, and revisiting the old milestones in writing this monograph was a genuine nostalgia trip, it is also important to reﬂect on the purpose of such a book as this. Now that the great majority of experimental high-Tc studies are ﬁnished, who could be interested in such a book? To give some kind of answer to this, let me pinpoint the 2006 M2 S Conference in Dresden.1 Not only was it at this conference that the idea for this book was hatched, but the conference itself evinced an astonishingly high level of interest in high-Tc issues, especially the theoretical aspects. Since it is now a number of years since a review of high-Tc studies with NMR has appeared, there may be a need on the part of theorists and other interested parties for an organized summary of results and of the ideas which have been advanced to bind them together. The foregoing oﬀers a partial answer to the “Why now?” question, but let me note that excellent answers to that question also emerge from the subject itself. Although many issues were settled as of 10 years ago, new ideas and even new phenomena have appeared since that time. Let me oﬀer two examples. The conﬁrmation by N. Curro and co-workers of a dynamical exponent crossover in the high-temperature phase diagram opens up a new arena of potential experimental activity. D. Pines and co-workers had predicted such an eﬀect and other theorists, including C. Varma, had predicted a phase 1

This was the 8th International Conference on Materials and Mechanisms of Superconductivity and High Temperature Superconductors, Dresden, July 9–14, 2006.

VIII

Preface

boundary in that region. Another interpretive breakthrough is to be credited to A. Uldry and P.F. Meier, who in 2005 created a new, general method for analyzing relaxation (T1 ) data in terms of temperature-dependent spin– spin correlation coeﬃcients for close-neighbor copper sites. Discussed at some length in this volume, this method rests on a very ﬁrm theoretical foundation. It has the great virtue that it separates spin-spin these correlation eﬀects from the temperature dependence of the quasiparticle dynamics, itself, which theoretical modelers have been trying to get at. If this extraordinarily simple method had been “available” 15 years ago, I suggest that our understanding of these issues would be greatly advanced from where it is. As for regrets, they come mainly under the heading of omissions. There are many excellent pieces of work which are not included, simply for want of time and space. The book was conceived of as a monograph and is in no sense an encyclopedia, not even within the narrow purview of high-Tc NMR. As an example, I greatly regret omitting the large and fascinating subject of impurity doping in cuprates, from which we have nonetheless learned a lot. Let me conclude by mentioning just a few of the people who have contributed, directly and indirectly, to the initiation and creation of this book. First let me thank Prof. Hiroshi Yasuoka, for bringing me to Tokai-mura in Japan for a 5-plus year extension of my career in solid-state NMR, and through which I also became involved in the European physics scene. Let me thank Prof. Dr. Frank Steglich for his support during my extensive visits to Dresden in 2006 and 2007. Invaluable support came from the Department of Physics at the University of Michigan in providing work space and the library facilities required for a project such as this. I want especially to thank Prof. Chandra Varma at the University of California at Riverside, for shepherding this book into existence through his role as editor for Springer Verlag and for his reading of much of the manuscript, giving penetrating, enlightening, and invaluable comments on the presentation. I also thank Jinan Yang for help with computer issues and with the preparation of the ﬁgures.

Ann Arbor, MI,

Russell E. Walstedt June 2007

Contents

1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1.1 The Basic Phenomenology of High-Tc Materials . . . . . . . . . . . . . 1 1.2 Carrier Doping and the Master Phase Diagram . . . . . . . . . . . . . . 2 1.3 The NMR Probe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 1.4 Outline of the Remaining Chapters . . . . . . . . . . . . . . . . . . . . . . . . 6 1.4.1 Summary of Chapter 2 – NMR Review . . . . . . . . . . . . . . . 6 1.4.2 Summary of Chapter 3 – Preliminary Cuprate NMR . . . 7 1.4.3 Summary of Chapter 4 – The Pseudogap . . . . . . . . . . . . . 7 1.4.4 Summary of Chapter 5 – T1 Models . . . . . . . . . . . . . . . . . 8 1.4.5 Summary of Chapter 6 – The Dynamical Susceptibility . 9 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10

2

Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Basic NMR Phenomenology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 The Basic Hamiltonian for NMR Spectra . . . . . . . . . . . . . 2.1.2 Observation of NMR/NQR Signals . . . . . . . . . . . . . . . . . . 2.1.3 Deﬁnition and Interpretation of NMR parameters: T2 . . 2.1.4 Deﬁnition and Interpretation of NMR parameters: The shift tensor Kαβ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.5 Deﬁnition and Interpretation of NMR parameters: T1 . . 2.2 NMR Probe of sp-Band Metals and Type I Superconductors . . 2.2.1 NMR Shifts and Relaxation in Simple Pauli Paramagnets 2.2.2 The Moriya Theory of Exchange Enhancement in Simple Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.3 NMR in the Superconducting State of Simple Metals . . 2.3 Static and Dynamic Magnetism in d-band Metals . . . . . . . . . . . . 2.3.1 The d-Electron HF Interactions . . . . . . . . . . . . . . . . . . . . . 2.3.2 Orbital Shift and Susceptibility . . . . . . . . . . . . . . . . . . . . . 2.3.3 Spin-Lattice Relaxation Eﬀects for d-Band Electrons . . . 2.3.4 NMR Studies of 3d Metals as Type-II Superconductors .

13 13 14 17 19 21 23 32 33 36 38 44 45 46 50 53

X

Contents

2.3.5 T1 Phenomenology for Type-II Superconductors . . . . . . . 58 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 63 3

The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO . . . . 68 3.1.1 LSCO: A superconductor with Tc (max) 40 K . . . . . . . 68 3.1.2 The 92 K Superconductor YBa2 Cu3 O7−x (YBCO) . . . . . 70 3.1.3 Physical Models of Itinerant Quasiparticles in Cuprates 71 3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 72 3.2.1 NMR Shift and Relaxation of the 89 Y in YBCO7 . . . . . . 73 3.2.2 Establishing the Site Assignment for the Cu(1) and Cu(2) NQR Spectra . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 75 3.2.3 Variation of the 89 Y shift K89 (x) with x for YBCO6+x . 76 3.2.4 Physical Models for the Relaxation of 63 Cu(2) in YBCO7 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79 3.2.5 Introduction of the Spin Hamiltonian Model for the Cu2+ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79 3.2.6 Experimental Breakthrough: Oriented Powder Samples . 80 3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 81 3.3.1 General Deﬁnition of the HF Tensors . . . . . . . . . . . . . . . . 82 3.3.2 Extracting the Cu(1,2) HF tensors for YBCO7 from Shift and Susceptibility Data Using the Spin Hamiltonian Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 84 3.3.3 Quantum Chemistry of YBCO7 and the Hyperﬁne Tensor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 87 3.3.4 T1 Ratios and Electron Spin Correlation Eﬀects . . . . . . . 90 3.4 Incorporating 17 O and 89 Y data into the Mila-Rice-Shastry Picture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 92 3.4.1 Measurements of T1 for 17 O in YBCO7 . . . . . . . . . . . . . . 97 3.4.2 The One-Band, Two-Band Debate: 89 Y and 17 O(2,3) NMR in YBCO . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 98 3.5 Formulation of T1 in Terms of χ (q, ω) and q -Dependent HF Couplings . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 99 3.5.1 Derivation of Dynamical Susceptibility T1 Equation . . . 99 3.5.2 The Fluctuation-Dissipation Theorem . . . . . . . . . . . . . . . . 101 3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc . . . . . . . . 104 3.6.1 The NMR Shift Behavior for T < Tc . . . . . . . . . . . . . . . . . 105 3.6.2 The Monien-Pines Calculations of NMR Shifts below Tc 107 3.6.3 Calculating the Relaxation Decay Curve . . . . . . . . . . . . . . 108 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112

Contents

XI

4

Pseudogap Eﬀects in Cuprate NMR Studies . . . . . . . . . . . . . . . 115 4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x . . . . . . . . . . . . . . 117 4.1.1 HF Parameters for YBCO6.63 from Scaling of Shift Data . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 120 4.1.2 A Simple Model Theory of Spin Dynamics for YBCO6.63126 4.1.3 INS Data for the Pseudogap of Underdoped YBCO . . . . 128 4.1.4 A Comprehensive T1 Data Set for YBCO6.63 . . . . . . . . . 130 4.2 Pseudogap Phenomenology with Other Probes . . . . . . . . . . . . . . 134 4.2.1 Pseudogap Eﬀects in the Electronic Speciﬁc Heat . . . . . . 134 4.2.2 ARPES Studies of Pseudogapped Cuprates . . . . . . . . . . . 136 4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) . . . . . . . . . . . . . . . . . 138 4.3.1 NMR Shift and Relaxation Behavior in Y248 . . . . . . . . . 139 4.3.2 Measuring the Pseudogap Isotope Eﬀect in Y248 with NMR . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 143 4.3.3 Theory of the Pseudogap by Varma. . . . . . . . . . . . . . . . . . 146 4.3.4 Eﬀect of Zn impurities on the Pseudogap in Y248 . . . . . 147 4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x) . . . . . . . . 148 4.4.1 Spin Susceptibility Scaling for La2−x Srx CuO4 . . . . . . . . . 149 4.4.2 Behavior of the 17 O and 63 Cu NMR Shifts in LSCO:x. . 152 4.4.3 63 Cu NQR spectra and Contrasting T1 Behaviors in LSCO:x. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 153 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 156

5

Relaxation Models for Cuprate NMR . . . . . . . . . . . . . . . . . . . . . . 159 5.1 The Uldry-Meier Parameterization Model . . . . . . . . . . . . . . . . . . . 160 5.1.1 Basic Formulation of the UM Analysis . . . . . . . . . . . . . . . 161 5.1.2 The Uldry-Meier Analysis of YBCO7 . . . . . . . . . . . . . . . . 163 5.1.3 The Uldry-Meier Analysis of YBCO6.63 . . . . . . . . . . . . . . 167 5.1.4 The Uldry-Meier Analysis of YBa2 Cu4 O8 (Y248) . . . . . . 169 5.2 The Millis, Monien, and Pines Model for T1 in Cuprates . . . . . 172 5.3 T1 Model for YBCO Using INS Data for χ (q, ω) . . . . . . . . . . . . 179 5.3.1 The Gaussian Model Susceptibility . . . . . . . . . . . . . . . . . . 180 5.3.2 Comparison with the UM Analysis Results for YBCO7 . 184 5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics . . . . . . . 187 5.4.1 Basic Formulation of the Dynamic Susceptibility . . . . . . 187 5.4.2 Remarks on the Hubbard Model Calculations . . . . . . . . . 189 5.5 The Large-U Hubbard Model of Si, Levin et al . . . . . . . . . . . . . . 192 5.6 Relaxation via Orbital Currents proposed by Varma . . . . . . . . . 195 5.7 Relaxation of Planar 63 Cu and 17 O at T < Tc . . . . . . . . . . . . . . . 199 5.7.1 χ (q , ω) for the Small-U Hubbard Model at T < Tc . . . 201 5.7.2 T1 and Spin-Spin Correlations below Tc : The UM Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 207 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210

XII

Contents

6

Dynamic Susceptibility Studies for the Cuprates . . . . . . . . . . . 213 6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 214 6.1.1 Some General Properties of the Indirect Spin-Spin Coupling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 216 6.1.2 The Gaussian model of Indirect Spin-Spin Coupling in YBCO . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 217 6.1.3 Measuring Indirect Spin-Spin Coupling via Spin-Echo Decay . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 218 6.1.4 Behavior and Interpretation of Indirect Couplings in YBCO and Y248 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 219 6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc . . . . . . . . 224 6.3 Coordinated Interpretation of NMR and INS Data for LSCO . . 227 6.3.1 Review of INS Data for Optimally-Doped LSCO . . . . . . 228 6.3.2 Interpretation of 63 Cu and 17 O T2 Data with INS Data for χ (q) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 236 6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) . . . . . . . . . 242 6.4.1 Phase Diagram and Basic Relationships for T1 , T2g . . . 242 6.4.2 The Dynamical Crossover Study by Curro et al: Y248 . . 245 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 250

A

Appendices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 A.1 Some Basic Properties of Spin Echoes . . . . . . . . . . . . . . . . . . . . . . 253 A.1.1 Basic Derivation of the Two-Pulse Spin Echo. . . . . . . . . . 253 A.1.2 Modelling Spin-Echo Decay . . . . . . . . . . . . . . . . . . . . . . . . . 257 A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling 257 A.2.1 Indirect Coupling with a Gaussian Susceptibility . . . . . . 258 A.3 Spin Echo Decay via Spin-Lattice Relaxation . . . . . . . . . . . . . . . 260 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 261

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 263

1 Introduction

The discovery of high-temperature superconductors among hole-doped CuO2 structures was one of those rare events in the scientiﬁc sphere which launches a whole new world of activity for hundreds of theorists and experimentalists alike. It is now more than twenty years since the New York City APS meeting dubbed the “Woodstock of Physics” witnessed the announcement of the original high-Tc results [1], but the level of activity on this topic remains extraordinarily high. For the nuclear magnetic resonance (NMR) probe, the high-Tc materials have oﬀered a panorama of new phenomenology to be analyzed and categorized in ways which had not previously come into use. It is the purpose of this volume to give a systematic account of many of the phenomena which have come to light in the process. The style of presentation is intended to be partly historical, partly tutorial for the non-specialist, and partly a review. There is by now a very large number of well-established ideas and eﬀects descriptive of the cuprates to be addressed. However, there is also the feeling, even twenty years on, that this monograph oﬀers only a snapshot of a vigorous and ongoing enterprise. We begin by presenting in this introductory chapter a broad perspective on the phenomenology and materials to be addressed, as well as on the NMR probe itself in the context of the cuprates. This is followed by an organizational synposis of the remaining chapters.

1.1 The Basic Phenomenology of High-Tc Materials The concept of a half-ﬁlled “conduction band” which cannot conduct on account of on-site Coulomb repulsion forces was inaugurated in 1949 by N.F. Mott – the “Mott insulator” [2]. Mott, who discussed the case of NiO, commented, “Experiments on the conductivity of cupric salts would be of great interest” [2]. Nearly forty years later a “cupric salt”, with a modest amount of hole-doping in the conduction plane, emerged as a superconductor,

R.E. Walstedt: Introduction, STMP 228, 1–11 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 1

2

1 Introduction

and “high-Tc ” was born. Just how such a system conducts – and superconducts – then became the investigative preoccupation of hundreds, possibly thousands of researchers around the world for many years to follow. The basic process whereby the entire system of localized, S = 12 , Cu2+ moments becomes a set of itinerant quasiparticles with the addition of a far smaller number of mobile hole “carriers” is one of great fascination, upon which even now there seems to be no clear theoretical consensus. As a basic mechanism, however, the Zhang-Rice singlet picture [3] provides at least a conceptual framework. Since the quasiparticles which result are known (through NMR studies) to pair oﬀ at low temperatures into a ground state of magnetically inert Cooper-pair singlets, the resulting scenario of fully itinerant character for the solitary holes on the Cu2+ sites seems at this point incontrovertible. Furthermore, these quasiparticles are known to possess a Fermi surface, with respect to which angle-resolved photoemission studies (ARPES) can be used to measure the superconducting energy gap. However, in many cases, gapping is found to occur in the normal state as well [4, 5, 6], in what is known as the “pseudogap” [7]. Many of the high-Tc systems also exhibit poor, but metallic-like conduction in the normal state, characterized by a non–Fermi– liquid temperature dependence ρ ∝ T instead of the usual T 2 . While the cuprates exhibit certain metallic attributes, they also clearly possess some features characteristic of the undoped insulating host, namely a powerful antiferromagnetic (AFM) exchange interaction between nearestneighbor Cu2+ moments. The eﬀects of these AFM couplings have emerged from virtually all inelastic neutron scattering (INS) studies of the cuprates, and are a major feature of theoretical modelling and experimental ﬁts to nuclear relaxation data as well (see Sect. 1.3).

1.2 Carrier Doping and the Master Phase Diagram There are by now hundreds of host structures known which contain CuO2 quadratic layers that superconduct under suitable doping conditions. A partial list is given in the review by Hazen [8]. In this volume, in order to limit the extent of material to be covered, we focus on the three principal systems La2−x Srx CuO4 (LSCO:x), YBa2 Cu3 O7−x (YBCO7-x), and the related stoichiometric compound YBa2 Cu4 O8 (Y248). These three were chosen, because they emerged early on as systems easy to synthesize and characterize. As a consequence, there is an extensive literature built up around them both in terms of experimental data and, naturally, of theoretical modelling as well. Even with our purview narrowed to these three systems, there are unfortunately many interesting studies which had to be omitted. One of the most important characteristics of the YBCO7-x and LSCO:x are their phase diagrams, plotted with coordinates T vs. δ, where δ represents the doping level of carriers in the CuO2 planes. An early version of the cuprate

1.2 Carrier Doping and the Master Phase Diagram

3

T TS AF

TR

Tc 0

δc

δ L

H

Fig. 1.1. The temperature vs. δ phase diagram of a typical cuprate structure, where δ is the number of hole carriers per formula unit. In the case of La2−x Srx CuO4 , one has δ ∼ x. For very small values of δ there is an antiferromagnetically ordered region. To the right of that is a roughly parabolic region of superconducting behavior which is centered on δ 0.15. See text for additional discussion. Reprinted ﬁgure from T. Tanamoto, H. Kohno, and H. Fukuyama, J. Phys. Soc. Japan 62, 717 (1993). Copyright 1993 Physical Society of Japan

phase diagram is shown in Fig. 1.1, where the superconducting phase lies under a dome extending from δ = 0.05 up to δ ∼ 0.35. At lower δ values there is an AFM phase which as δ → 0 occurs at TN 325 K. The lines extending above and to the left of the superconducting dome represent, in the present instance, maxima in the spin susceptibility and in the nuclear relaxation curves, respectively [9]. In versions of this phase diagram discussed in Chaps. 4 and 6, these lines have other interpretations as well, such as the pseudogap temperature or the crossover between the tetragonal and orthorhombic phases in LSCO, etc. – see Sect. 1.4). There is, in principle, a phase diagram similar to Fig. 1.1 for every cuprate structure. It happens for LSCO:Δ that the hole doping level can be varied across the entire superconducting range by varying δ. In YBCO7-x, on the other hand, the doping is controlled via the oxygen content. At x = 0 (YBCO7) the structure is stoichiometric and the hole-doping level is ∼ 0.33 per Cu ion, which is just slightly above optimal doping [10, 11]. As x is increased, the doping diminishes all the way into the AFM insulating phase. However, the overdoped phase which would correspond to negative values of x simply does not exist. The stoichiometric compound Y248 is structurally similar to YBCO7, but with an extra chain layer. It has a very stable oxygen content up to relatively high temperatures, but its doping level giving Tc 84 K cannot be altered without decomposition. It has been an attractive system for study and will be discussed in Chaps. 4, 5 and 6. Characterization of samples for experimental investigation is a matter of great importance, since a large body of reliable data for mainstream

4

1 Introduction

structures is on hand. Sample characterization includes morphology of the sample material, x-ray crystallography for phase purity, superconducting diamagnetism (Meissner eﬀect) including the value and sharpness of Tc , and magnetic susceptibility for excessive local moment content. The NMR and NQR studies themselves include sample characterization tests, to be mentioned in Sect. 1.3 to follow. For articles discussing structures and a variety of bulk and other measurements, see the reviews edited by D.M. Ginsburg [12].

1.3 The NMR Probe The NMR probe is a local, real–space probe, where the behavior of nuclear spins can be monitored on a site–by–site basis. The magnetic hyperﬁne (HF) interaction of a nucleus couples it to magnetic entities in its immediate environment. This interaction rarely goes beyond nearest-neighbors, though dipolar interactions may have some eﬀects beyond that range. One of the remarkable HF eﬀects in cuprates is the extraordinarily large coupling of 63,65 Cu with neighboring (Cu2+ ) electron spin moments, which is comparable with on–site interactions. There is, however, an intervening O2− ligand, so this is a second-neighbor interaction. Such an eﬀect was unprecedented. The eﬀect of HF couplings is also strongly aﬀected by site symmetry, where strong, but equal couplings to antiferromagnetically correlated neighbor spins may be rendered ineﬀective. Such eﬀects are well known for insulating antiferromagnets (e.g. 19 F in KMnF3 ). The measurements performed and type of data received are also very much conditioned by the properties of the naturally occurring nuclear species in the system investigated. Thus, the 100% abundant, I = 12 , 89 Y in YBCO7, with its nearly isotropic NMR shift, total absence of quadrupole eﬀects, and weak, but adequate relaxation times was the subject of the ﬁrst NMR study on cuprates to be published [13]. The 63,65 Cu isotopes with I = 32 , (nearly) axial site symmetry, and very substantial quadrupolar energies which allow both NMR and NQR to be performed, were quick to follow [14, 15, 16, 17]. Studies of 17 O, which only appeared after an interval of many months, were hampered by the fact that 17 O is present in only trace quantities in natural oxygen. Further, it is too expensive to incorporate into the sample synthesis and has to be diﬀusively exchanged into sample materials at an elevated temperature. Such a process is critically dependent on diﬀusion rates in any given material. In LSCO:x, for example, diﬀusion is fast and single crystals of moderate size are easily doped with 17 O. For YBCO7-x, however, this is only feasible with powders and crystals of the smallest size. With Y248 it is also very diﬃcult, requiring lengthy high-temperature anneals [18]. Nonetheless, 17 O doping eventually became a routine element of technique.

1.3 The NMR Probe

5

A Sampling of NMR Measurements and their Interpretation We give a brief survey of types of NMR observations made and their signiﬁcance for the behavior of cuprate materials. First, the NMR spectrum is fundamental and is a major element of sample characterization. The width and distribution of NMR/NQR resonance lines tells a great deal about the phase purity and microscopic quality of sample material. If there are crystallographically inequivalent sites, they usually have diﬀerent spectra. Quadrupolar frequency shifts and broadening and their ﬁeld/frequency dependence can usually be analyzed to yield values of coeﬃcients from the HF Hamiltonian. These matters are reviewed in some detail in Chap. 2. The NMR shift, which is measured as a frequency shift proportional to the applied ﬁeld, is fundamentally a measure of the various terms in the magnetic polarization of the sample, conveyed to the nuclear spins by HF coupling ﬁelds. The NMR shift is an important source of information on intrinsic susceptibilities. For example, the decay of the spin susceptibility in the superconducting state can usually only be measured via the NMR shift, where direct magnetic measurements would be swamped by the much larger diamagnetic response. There are various contributions to NMR shifts in metals. The s-contact shift, for which we reserve the term “Knight shift” [19], is a mainstay effect in sp-band and d-band metals. In cuprates this term is oddly absent. In its place are the core–polarization shift, orbital shift, dipolar shift, and even “spin-orbit shift”, a second-order eﬀect which arises in the spin Hamiltonian model. There are also very important transferred HF ﬁelds giving rise to NMR shifts, originating in the Mila-Rice [20] and Shastry [21] treatments of cuprate quantum chemistry. NMR shift measurements are a very important tool for determining the HF parameters, since any such determination is independent of model assumptions required for the dynamics. NMR dynamics, as represented by the spin-lattice relaxation time T1 , are a key diagnostic of quasiparticle dynamics in metals and in cuprates in particular. T1 is linked to χ (q, ω) via the ﬂuctuation dissipation theorem [22, 23]. In cuprates, T1 measurements have been interpreted (for the ﬁrst time!) through theoretical modeling of χ (q, ω). What makes this process particularly interesting is the interplay between the strong AFM ﬂuctuation eﬀects, which typically produce an AFM peak near q = (π, π), and the transferred HF couplings at 17 O(2,3) and 89 Y in, e.g. YBCO7-x, which allow their relaxation processes to avoid the AFM peak. Meanwhile, the 63 Cu(2) are quite sensitive to the AFM peak. In eﬀect one has, then, a “q–space spectrometer” for quasiparticle ﬂuctuations. These eﬀects occupy a substantial fraction of the discussion in this volume. T1 measurements are also very sensitive to the diﬀerence between s–wave and d–wave gap characteristics in the superconducting state. Calculations of d–wave T1 characteristics below Tc were among the ﬁrst strong evidences for d–wave singlet character of quasiparticle pairing in cuprates [24, 25].

6

1 Introduction

A second relaxation time, the spin-echo decay time T2g , has taken on a major signiﬁcance in the eﬀort to characterize the dynamic susceptibility of cuprate compounds. This decay time is actually used to measure a static interaction which occurs in cuprates, namely a c-axis indirect spin-spin coupling of the form Hzz = ij= αij Izi Izj , which was ﬁrst identiﬁed by Pennington et al. [26]. How this comes about is discussed in Appendix A.1 and in Chap. 6 of the book. Interpretation of Hzz in terms of χ (q, 0) for q in the vicinity of (π, π) was established by the Pennington–Slichter model calculation [27]. Through measurements of T2g the indirect coupling has become a major element in characterizing the strength of AFM ﬂuctuations in cuprates. In addition, the interpretation of T2g in the superconducting state by Bulut and Scalapino [24] again provided dramatic evidence in favor of d–wave pairing several years before it was widely accepted by the research community. The foregoing is just a sampling of interesting eﬀects which have come to light through NMR studies of cuprate superconductors. We refer the interested reader to sources on the fundamental principles of NMR [28, 29], on NMR studies of conventional metals and superconductors [30, 31, 32], as well as on NMR of high–Tc superconductors [33, 34, 35, 36, 37, 38]. We now give a brief summary of the remaining chapters.

1.4 Outline of the Remaining Chapters This section gives a brief summary of the content of Chaps. 2–6. 1.4.1 Summary of Chapter 2 – NMR Review In Chap. 2 we give a review of the elements of NMR technique and interpretation, where basic deﬁnitions of key NMR parameters are given and some of the pitfalls and complexities associated with powder samples are discussed. The use of spin echoes – the standard tool for conducting NMR measurements – is described, with a detailed derivation including spin echo decay mechanisms presented in Appendix A.1. This leads into a summary of basic relaxation mechanisms for simple metals, including the Moriya theory of electron–electron interaction eﬀects [22] and the BCS-based interpretation of the spin-paramagnetic shift and T1 behaviors in the superconducting state. The Anderson–Farrell resolution of spin-orbit coupling eﬀects for T < Tc is covered in some detail. These eﬀects were struggled over for many years, but almost all problems were ﬁnally resolved. Discussion of the foregoing is extended to d–band metals, including the discovery and establishment of orbital shifts and relaxation eﬀects. The interpretation of NMR spectra and relaxation eﬀects in the mixed state of type-II superconductors is discussed at some length, with data from the literature. Many of the associated problems have cropped up again with the cuprates. The discussion of, e.g. the V3 X’s is oﬀered as a foundation for understanding cuprate mixed-state NMR.

1.4 Outline of the Remaining Chapters

7

1.4.2 Summary of Chapter 3 – Preliminary Cuprate NMR Chapter 3 gives an account of the early stages of high-Tc NMR research. In the ﬁrst two years, almost all studies were done with either random powder samples or microcrystals with very low signal amplitude. There was an intense focus on YBCO7, because of its high Tc (∼ 90 K) and because of its relative ease of preparation. In random powders, 63 Cu(2) NMR spectra (just the − 12 ↔ 1 2 transition) were ∼ 5 kG wide in an 8T laboratory NMR magnet, taking several days of signal averaging to perform a single scan. T1 measurements on the 63,65 Cu were done mainly with NQR, once the frequencies had been extracted from NMR spectra. 63 Cu(2) NMR shifts persisting into the superconducting state were identiﬁed as Van Vleck orbital shifts. The anisotropy and magnitude of these shifts ﬁt well with a simple spin Hamiltonian model of the copper ionic state, which appears to resemble that of a Cu2+ ion in an insulating host for the purpose of analyzing HF eﬀects. This picture has held up even until now. Moreover, the dx2 −y2 ground state orbital dictates that the normally dominant orbital T1 mechanism eﬀectively vanishes in the cuprates. In Sect. 5.6 a proposal for its revival via the marginal Fermi liquid theory is presented [39]. The apparent vanishing of the c–axis spin HF ﬁeld led to the Mila-Rice A proposal: A massive transferred HF coupling from nn Cu2+ ions nearly 4˚ away. This unprecedented HF term made sense of the T1 and NMR shift data for the 63 Cu(2). Their watershed paper, including calculated quantum chemistry, provided a framework for interpretation of cuprate NMR data which has held up ever since [20]. The chapter closes with an account of the ﬁrst interpretation of T1 data in the superconducting state using d–wave pairing with BCS theory, by Monien and Pines [24]. This landmark result gave a clear indication of the correctness of d–wave and the inadmissibility of s–wave, even though it would be ﬁve more years before the correctness of this picture was widely accepted. 1.4.3 Summary of Chapter 4 – The Pseudogap Even before the Mila-Rice resolution of anomalous NMR shift behavior appeared, workers had begun to explore the highly unusual behavior in the underdoped region of the phase diagram in Fig. 1.1. There it was found that low-frequency ﬂuctuations which drive the T1 process, as well as the uniform susceptibility, were beginning to collapse at temperatures far above Tc . It was as though the superconducting energy gap was beginning to develop at some T ∗ well above Tc in anticipation of the actual transition to superconductivity. In the spirit of “spin–charge separation”, an idea that dominated early thinking on cuprate quasiparticle behavior [40], this eﬀect was at ﬁrst dubbed the “spin gap”. There was a tacit assumption that charge states were unaﬀected. Nonetheless, the spin pseudogap was soon recognized as a universal feature of the underdoped phases. Moreover, in a most astonishing bit of prescience,

8

1 Introduction

the appearance of such a precursive energy gap in the cuprates had actually been predicted by Friedel [7], who coined the term “pseudogap”. Pseudogap characteristics via NMR shift and T1 data are documented in detail for several compounds in Chap. 4. Several years after the spin ﬂuctuation properties of pseudogap systems were well established, it came to light through both electronic speciﬁc heat and ARPES measurements that charge properties were also profoundly altered in pseudogap systems. In this chapter we also review these eﬀects brieﬂy. With ARPES one ﬁnds that certain regions of the Fermi Surface, e.g. the quadratic axes, are gapped while while the diagonal regions are not. Since the dynamic susceptibility is a summation over the Fermi surface, this means that the gap reﬂected by χ (q, ω) may vary signiﬁcantly with q. It follows that pseudogap T1 behavior can be quite diﬀerent at the 63,65 Cu site from what it is at the 17 O sites. These diﬀerences are clearly observed in a number of cases discussed. The pseudogap behavior of LSCO:x is particularly interesting. In what was actually the ﬁrst pseudogap behavior to be reported [41], the remarkable scaling of susceptibilies for diﬀerent x values in this system was at ﬁrst interpreted with a model suited to 2D insulating antiferromagnets. This is possible, since the latter systems exhibit a susceptibility temperature maximum which resembles pseudogap behavior. The disparate behaviors of 1/T1 T for the 63,65 Cu and the 17 O also clearly tag this system as having a pseudogap. The low-T χ0 (T ) ∝ T 1/2 behavior of LSCO:x is in accord with the Varma theory of pseudogap behavior [39], as is that of Y248 [42]. 1.4.4 Summary of Chapter 5 – T1 Models From the earliest days of high-Tc NMR one of the main challenges has been to understand the disparate behaviors of T1 at various lattice sites. In addressing this question, there are several important branching points in the ﬂow diagram of deduction so to speak. Magnetic dipole processes are assumed to be predominant. First, then, one must decide whether spin ﬂuctuations alone will suﬃce to explain everything, or whether orbital relaxation, severely inhibited by the dx2 −y2 ground–state orbitals, will play a role as well. Many workers have opted for the spin ﬂuctuation picture, while the existence of a possible orbital mechanism has been pointed out by Varma [39]. A summary of the latter calculation is given in Sect. 5.6. In the purely spin-dynamical picture, one must next decide whether a single dynamical variable per Cu2+ site, namely the itinerant S = 12 hole, is suﬃcient, or do the doped–in hole carriers form a second dynamical entity? The general approach to this question has been to see whether a complete account of the data can be given with one variable per site. Several T1 modeling eﬀorts based on the latter assumption are described in Chap. 5, where it is presumed with Moriya [22] that any successful scenario can be expressed in terms of χ (q, ω). Three of these employ the random–phase approximation in order to incorporate the (mandatory) electron–electron interactions, and

1.4 Outline of the Remaining Chapters

9

one is simply based on the shape and width of the the AFM peak in χ (q, ω) determined by INS studies. Quite recently, however, a novel, but related approach was pioneered by Uldry and Meier [43], in which they attempt to systematize T1 data on several cuprates using electronic spin–spin correlations as parameters which vary with T and in which there is a universal spin ﬂuctuation frequency (correlation time), also a function of T, which applies to all T1 processes. The other central assumption is that the HF Hamiltonian has the Mila–Rice form ⎡ ⎤ (1.4.1) Siα ⎣Aα + B Ijα ⎦ HHF = α

i

j(nn)

for the planar 63,65 Cu nuclei, with similar forms for the ligands. With these ingredients all of the data are ﬁtted in a self-consistent way. The form (1.4.1) and the admissibility of the spin–spin correlations and correlation time as temperature–dependent parameters are the main assumptions here. A theoretical basis for this scheme is derived using χ (q, ω) in Chap. 3. It yields an internally consistent picture, in which the dynamically–derived HF constants basically agree with those derived from the shift. This scheme is useful for evaluating theoretical models as well as for analyzing experimental data. 1.4.5 Summary of Chapter 6 – The Dynamical Susceptibility In this chapter three topics related to modeling and characterization of χ(q, ω) are presented and discussed. First, large indirect spin-spin couplings in cuprates were noted early on and modeled quantitatively by Pennington and Slichter [25]. Further, the strength of indirect spin–spin couplings Hzz noted above can be measured by means of spin-echo decay if the entire nuclear spin transition observed can be inverted by the spin echo refocussing pulse (θ2 π). Measurements of this type have been carried out on a number of systems, yielding a quantitative measure of χ (q, 0) q = (π, π). This has become an important source of input data for the dynamical susceptibility. Another major data source for χ (q, ω) is INS. The compound LSCO:x with x 0.15 became an important test case for χ (q, ω). This system bears the distinction of having been measured with INS in absolute units over most of the ﬁrst Brillouin zone (all known structure), over energies ranging from 1–200 meV, and at temperatures ranging from below Tc to nearly 300 K [44]. The dynamical susceptibility determined in this way was found to be highly incommensurate. These data were used to calculate T1 for 63,65 Cu and for 17 O, with interestingly mixed results. The NMR data behave as though the discommensurations were either much smaller or simply not there at all. The ﬁnal section of Chap. 6 oﬀers a brief review of the behavior of T1 and T2g in the normal state region above and principally on the left side of the superconducting dome in Fig. 1.1. Sokol, Barzykin, and Pines have proposed

10

1 Introduction

a crossover in the value of the dynamical exponent from z = 1 (quantum critical phase) to z = 2 (non-scaling region) [45, 46]. The line dividing these two behaviors is suggested to take place where the correlation length ξ(T ) = 2a (a = lattice constant). This idea has been tested up to 700 K on the cuprate Y248 by Curro et al [47]. A clear transition from z = 1 to 2 was found at T = 500 K, giving support to this scaling theory.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12.

13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29.

J.G. Bednorz, K.A. Mueller, Z. Phys. B64, 189 (1986) 1 N.F. Mott, Proc. Phys. Soc. London Sect. A62, 416 (1949) 1 F.C. Zhang, T.M. Rice, Phys. Rev. B37, 3759 (1988) 2 J.M. Harris, Z.-X. Shen, et al., Phys. Rev. B54, R15665 (1996) 2 A.G. Loeser et al., Science 273, 325 (1996) 2 H. Ding et al., Nature (London) 382, 51 (1996) 2 J. Friedel, Physica C153–155, 1610 (1988) 2, 8 R.M. Hazen, in Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), p. 121 2 T. Tanamoto, H. Kohno, H. Fukuyama, J. Phys. Soc. Japan 62, 717 (1993) 3 T. Graf, G. Triscone, J. Muller, J. Less-Common Met. 159, 349 (1990) 3 M. Horvati´c, T. Auler, C. Berthier, Y. Berthier, et al., Phys. Rev. B47, 3461 (1993) 3 D.M. Ginsberg (ed.), Physical Properties of High Temperature Superconductors I (World Scientiﬁc, Singapore, 1989) and Physical Properties of High Temperature Superconductors II (World Scientiﬁc, Singapore, 1990) 4 J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts, Sol. St. Comm. 63, 847 (1987) 4 D. Brinkmann, L. Pauli, J. Roos, H. Zimmermann, Phys. Lett. A124, 112 (1987) 4 W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 59, 1860 (1987) 4 H. L¨ utgemeier, M.W. Pieper, Sol. St. Comm. 64, 267 (1987) 4 I. Furo, A. J´ anossy, L. Mih´ aly, et al., Phys. Rev. B36, 5690 (1987) 4 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 4 W.D. Knight, Phys. Rev. 76, 1259 (1949); C.H. Townes, C. Herring, W.D. Knight, Phys. Rev. 77, 852 (1950) 5 F. Mila, T.M. Rice, Physica C157, 561 (1989) 5, 7 B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 5 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 5, 6, 8 V. Jaccarino, in Physics of Solids, International School of Physics “Enrico Fermi”, Course XVIII (Acadamic Press, New York, 1966) 5 H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990) 5, 6, 7 N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 5, 9 C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 6 C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 6 A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 6 C.P. Slichter, Principles of Magnetic Resonance, 3rd edn. (Springer-Verlag, New York, 1992) 6

References

11

30. J. Winter, Magnetic Resonance in Metals (Clarendon Press, Oxford, 1971) 6 31. A. Narath, Hyperﬁne Interactions, ed. by A.J. Freeman and R.B. Frankel (Academic Press, New York, 1967), p. 287 6 32. D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, Vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 6 33. C.H. Pennington, C.P. Slichter, In Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsberg (World Scientiﬁc, Singapore, 1990), p. 269 6 34. R.E. Walstedt, W.W. Warren, Jr., Science 248, 1082 (1990) 6 35. C.P. Slichter, in Strongly Correlated Electron Systems, ed. by K.S. Bedell et al., (Addison – Wesley, Reading, MA, 1993), p. 427 6 36. D. Brinkmann, M. Mali, in NMR Basic Principles and Progress, Vol. 31 (Springer Verlag, Berlin, 1994), p. 171 6 37. C. Berthier, M.H. Julien, M. Horvati´c, Y. Berthier, J. Phys. I France 6, 2205 (1996) 6 38. C.P. Slichter, in Handbook of High Temperature Superconductivity, ed J.R Schriﬀer, J.S. Brooks (Springer Science+Business Media, New York, 2007), p. 215 6 39. C.M. Varma: Phys. Rev. Lett. 77, 3431 (1996) 7, 8 40. P.W. Anderson, Science 235, 1196 (1987) 7 41. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 8 42. G.V.M. Williams, et al., Phys. Rev. Lett. 80, 377 (1998) 8 43. A. Uldry, P.F. Meier, Phys. Rev. B72, 094508 (2005) 9 44. G. Aeppli, T.E. Mason, et al., Science 278, 1432 (1997) 9 45. A. Sokol, D. Pines, Phys. Rev. Lett. 71, 2813 (1993) 10 46. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 10 47. N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 10

This page intentionally blank

2 Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors

The ﬁeld of high-Tc NMR developed in a context of many years of NMR studies of conventional superconductors as well as of d-band transition metals, alloys, and intermetallic compounds. It is therefore appropriate to begin this volume with a brief review not only of the NMR probe, itself, but of the general physical phenomena probed by NMR in transition metal systems, in both the normal and superconducting states. The published literature on this subject matter is, of course, vast, and the references cited here will necessarily be rather limited. We begin by citing the standard works on nuclear magnetism by Abragam [1] and Slichter [2], where almost all basic NMR phenomena are derived and discussed. These sources also present an extensive guide to the early literature, which the interested reader will ﬁnd highly informative. For NMR of metallic systems, there are thorough reviews by Narath [3] and Winter [4] and for early NMR studies on superconductivity, there is a detailed and informative review by MacLaughlin [5]. We shall also have recourse to the treatments of superconductivity by Tinkham [6] and Schrieﬀer [7]. Relevant reviews of high-Tc NMR studies will be cited at the beginning of Chap. 3.

2.1 Basic NMR Phenomenology We begin with a brief review of current NMR technique and its capabilities. The basic data one usually hopes to acquire with resonance methods consist of the spectral shape and features, the frequency shift tensor Kαβ , and the relaxation times T1 and T2 . The acquisition and interpretation of these elements of data will be the preoccupation of most of this volume. Here we wish simply to introduce them, and in this Sect. 2.1 the basic measurement and interpretation of these parameters will be reviewed. Some additional discussion of NMR phenomenology is given in the Appendices.

R.E. Walstedt: Introduction to NMR Studies of Metals, Metallic Compounds, and Superconductors, STMP 228, 13–65 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 2

14

2 Introduction to NMR Studies of Metals and Superconductors

2.1.1 The Basic Hamiltonian for NMR Spectra The basic nuclear spin Hamiltonian for spectra is given by (2.1.1), including both the Zeeman term representing the eﬀect of an applied ﬁeld H and a quadrupolar term representing the interaction of the nuclear quadrupole mo∂2V at the nuclear ment with the electrical ﬁeld gradient (EFG) tensor Vuv = ∂u∂v site in question (see [1], Ch. VI). ˆ ·H + ˆ + K) Hspec = −γI · (1

e2 qQ η 2 2 [3I 2 –I(I + 1) + (I+ + I− )], (2.1.1) 4I(2I − 1) z 2

ˆ is the NMR shift tensor and 1 ˆ is the unit tensor. In this equation where K 2 we use conventional notation, where q = | ∂∂ZV2 | = VZZ is the principal component of the EFG tensor, and the EFG asymmetry parameter is deﬁned as η = (VXX -VY Y )/VZZ . The (X, Y, Z) are the principal axes of the tensor, where we deﬁne |VXX | ≤ |VY Y | ≤ |VZZ | and note that LaPlace s equation gives VXX + ˆ q, VY Y + VZZ = 0. It follows that 0 ≤ η ≤ 1. If we permit the parameters K, and η to be distributed, then Hspec will generate the vast majority of NMR spectra found in practice. Although (2.1.1) is frequently quoted, it has the disadvantage that it assumes that the quantization axis is along the principal axis of the EFG tensor. Since one often works with the ﬁeld along some principal axis of the EFG, it is useful to generalize (2.1.1) for an arbitrarily chosen principal axis. In principal axis coordinates, the quadrupolar Hamiltonian becomes [1] eQ Vαα Iα2 . (2.1.2) HQ = 2I(I + 1) α In terms of the Vαα , (2.1.1) becomes in traceless form [2] ˆ ·H + ˆ + ·K) Hspec = −γI · (1

eQ [Vαα (3Iα2 − I(I + 1)) 4I(2I − 1)

1 2 2 + (Vββ − Vγγ )(I+ + I− )] , (2.1.3) 2 where α is the quantization axis and (α, β, γ) are an arbitrary permutation of (X,Y,Z). In this form it is clear that ﬁrst-order splittings will be proportional to | Vαα |, and the second-order splittings will be proportional to (Vββ −Vγγ )2 . While (2.1.1) and (2.1.3) are useful for generating spectra, it should be noted that a number of other terms are necessary for a complete description of NMR phenomena. Some of the omissions are (a) terms to represent ﬁxed internal hyperﬁne (HF) ﬁelds which may occur in ordered magnetic systems, (b) spin and orbital ﬂuctuation terms which drive T1 processes, (c) dipolar and indirect spin-spin coupling terms which generate T2 processes, and (d) radiofrequency (rf ) excitation terms. Such terms will be invoked when the need arises. We make a number of general remarks about the use of (2.1.1) and (2.1.3) to generate and analyze spectra.

2.1 Basic NMR Phenomenology

•

• •

•

•

•

•

15

Experiments are usually carried out in one of two limiting cases, namely, H = 0, so that quadrupolar energies alone determine the spectrum (NQR), e2 qQ and secondly, the high ﬁeld limit γH 4I(2I –1) , wherein the quadrupolar terms may be treated with perturbation theory. For I = 12 the nuclear quadrupole moment Q vanishes identically, according to the Wigner–Eckart theorem (e.g. see [2], Ch.10). For nuclear spin sites with cubic symmetry, one has VXX = VY Y = VZZ = 0, greatly simplifying the spectrum as with I = 12 . For quadrupolar nuclei, the eﬀects of stray EFG’s in nominally cubic structures may still play a role in the spectrum, however. Crystalline disorder caused by impurities, dislocations, etc., often cause a distribution of stray EFG’s to occur at the nuclei of interest. Thus, one often ﬁnds cubic NMR lines with complete ﬁrst-order broadening, so that only the (- 12 ↔ 12 ) transition is easily resolved. Such cases will be discussed as they arise. In the almost universally encountered high-temperature limit deﬁned by γH kB T , Boltzmann factors are always small compared with unity. The sign of qQ in (2.1.1) is immaterial to the spectra and is, in fact, indeterminate. For convenience, we shall always take qQ to be positive. Note also that the term “-I(I+1)” in (2.1.1) has been inserted only to render the quadrupole tensor traceless. It plays no role in the spectral transition frequencies and may be omitted or replaced by some other quantity for calculational convenience. In the most frequently occurring cases of non-cubic site symmetry, i.e. tetragonal or trigonal, the EFG symmetry is termed “axial”, giving VXX = VY Y . Thus, η = 0 and the quadrupolar Hamiltonian is greatly simpliﬁed. We shall focus primarily on this case and comment on how the results are aﬀected if η > 0. In the high-ﬁeld limit with η = 0, we comment brieﬂy on how the EFG term aﬀects the spectrum. If we let the angle between H and the EFG principal axis Z be θ, then the simplest case is when θ = 0. The eigen-energies then have the exact form Em = −γH(1 + K)m + hνQ m2 /2, where νQ = 3e2 qQ 2hI(2I –1) , m is the Iz quantum number, and we have assumed a scalar shift K. In such a case, the energy levels are shifted as shown in Fig. 2.1. In the spectrum shown, the (- 12 ↔ 12 ) transition is not aﬀected by the νQ term, and the (±m ↔ ±(m + 1)) transitions are displaced by ±νQ , ±2νQ , . . ., for m = 12 , 32 , . . ., respectively, as shown in the ﬁgure. The lines displaced by ±nνQ are known as ﬁrst-order satellites. For θ = 0 the eigenfrequencies can often be estimated satisfactorily with second-order perturbation theory (see [1], Ch. VI). The ﬁrst-order resonance frequencies become (1)

νL + ν±n = νL ± nνQ (3cos2 θ − 1)/2,

(2.1.4)

n = 1, 2, . . .. Here, n = 1 corresponds to the (± 12 ↔ ± 23 ) transitions and n > 1 corresponds to transitions with progressively higher values of m.

16

2 Introduction to NMR Studies of Metals and Superconductors Zeeman m = –3/2 m = –1/2 m = 1/2

Zeeman + Quadrupolar

νL

νL + νQ

νL

νL

νL

νL – νQ

m = 3/2 Spectra:

νL

νL – νQ νL νL + νQ

Fig. 2.1. On the left, the nuclear Zeeman term gives uniformly spaced energy levels and a single NMR line. On the right, ﬁrst-order quadrupole splittings produce “ﬁrstorder satellites” from the (±1/2 ↔ ±3/2) transitions. The (−1/2 ↔ 1/2) transition is not aﬀected to ﬁrst order

In the case of powder samples with a uniform distribution of θ over the unit sphere, the ﬁrst-order quadrupole shift stated above gives rise to an intensity distribution over frequencies ranging from νL −nνQ /2 to νL +nνQ if the θ = 0 satellite displacement is nνQ . The normalized distribution function is 1 (2.1.5) ρq (ν) = [6nνQ (ν − νL + nνQ /2)]− 2 ,

•

•

so that the θ = 0 line at frequency nνQ becomes a powder pattern with a square-root singularity at ν = νL − nνQ /2. Here, the Larmor frequency νL = γH(1 + K). We note that m is no longer strictly a good quantum number, so there are second-order frequency shifts as well. Interestingly, the second-order frequency shifts of the satellites at ±nνQ (3cos2 θ − 1) are equal, so that the second-order correction to their pairwise separation 2nνQ (3cos2 θ−1) vanishes. If η > 0, however, the singularities all disappear and the peak at that position becomes progressively broader as η increases. For the often-used (- 12 ↔ 12 ) transition, the frequency to second order is given by 2 νQ 3 (2) ν± 1 = νL − (2.1.6) I(I + 1) − sin2 θ (9 cos2 θ − 1). 2 16νL 4 In the case of a random powder sample, (2.1.4) and (2.1.6) give rise to characteristic powder patterns which are easy to recognize. Such a pattern is shown in Fig. 2.2, where a small amount of Gaussian broadening has been added. In cases where η > 0, these powder patterns are altered signiﬁcantly. Also, if there is shift anisotropy K(θ) with a range comparable to the second-order quadrupole shift of the (- 12 ↔ 12 ) transition, its powder-pattern shape will also be altered signiﬁcantly, whereas the ﬁrstorder peaks will all reﬂect the shift value K(π/2). Further discussion of these eﬀects is given below. When H = 0 we have the case of nuclear quadrupole resonance (NQR). The nuclear spin energies are determined entirely by Q, I, and the local

2.1 Basic NMR Phenomenology

17

Quadrupolar Powder Pattern for (–½ ↔ ½) Transition

–1.5

–1

–0.5

0

0.5

1

1.5

2

2.5

Quadrupole Shift (units of 3νQ2/16νL)

Fig. 2.2. Quadrupolar powder pattern for the (−1/2 ↔ 1/2) transition based on the second-order quadrupolar energy given in 2.1.6 (axial case). Minimal Gaussian broadening has been applied. The coeﬃcient given is for I = 3/2. For arbitrary 2 /64νL half-integral I the coeﬃcient becomes (4I(I + 1) − 3)νQ

EFGs. If νQ (see item 6 above) is large enough, i.e. in the MHz range, then NQR spectroscopy is feasible. Considering the case of η = 0, (2.1.1) then shows that E|m|+1 - E|m| = (2|m| + 1)νQ . Thus, there is a series of I − 12 NQR lines at frequencies νQ , 2νQ , . . .. The m–levels are doubly degenerate, since Em is independent of the sign of m. The two parallel transitions produce identical signals under the usual excitation conditions1 . If η > 0, the levels are still doubly degenerate, but the transition frequencies are now a function of η. If there are two or more NQR frequencies, their ratio can be used to determine η.

2.1.2 Observation of NMR/NQR Signals In the early days of solid-state NMR, it was customary to employ continuous wave methods to observe NMR signals. Techniques such as the marginal oscillator and the popular crossed-coil rf bridge spectrometer manufactured by Varian Associates were used to obtain a wealth of useful NMR data. Compared with pulsed NMR this method has, however, a number of inherent drawbacks. It is not useful for severely broadened lines, it cannot distinguish between static and dynamic line broadening, so it cannot measure T2 , nor a

1

It is possible to separately excite, e.g. the (1/2,3/2) and the (-1/2,-3/2) transitions, using circularly polarized rf pulses (M.J. Weber and E.L. Hahn, Phys. Rev. 120, 365 (1960)). However, for most measurements, there is no advantage in doing so.

18

2 Introduction to NMR Studies of Metals and Superconductors

short value of T1 , to name just a few. Thus, it gradually gave way to pulse methods for solid-state NMR studies2 . The Spin Echo The spin echo[9] is used almost universally for measurement and observation of NMR/NQR signals in solids. Typically, short, medium-power rf pulses applied at the frequency of a |Δm| = 1 transition of the Hamiltonian Hspec are followed by a spin-echo signal as shown in Fig. 2.3. The rf ﬁelds are applied transverse to the axis of spin quantization. The ﬁrst pulse produces a precessing, transverse nuclear magnetization proportional to the instantaneous spin polarization at the time it is applied. The precessing moment following the ﬁrst pulse often decays in a time of the order of the pulse width, as shown in the ﬁgure, and is usually unobservable because of the “dead time” of the receiver. Such a decay time is known as T2∗ 3 . A second rf refocussing pulse at time τ causes the precessing moment to reappear brieﬂy at time 2τ as shown. Using digital electronic methods, such spin echo signals are recorded, noise averaged, and stored for manipulation and analysis. A basic calculation of the spin echo response is presented and discussed in Appendix A.1, including a simple treatment of spin echo decay processes.

Nuclear Spin Echo

–5

–4

–3

–2 –1 0 2ω1 (t – 2τ)/π

1

2

3

Fig. 2.3. A simulated spin echo signal is shown (solid curve), corresponding to the (0.8π/2, π/2) pulse pair (shown) applied to a broad, inhomogeneous distribution of NMR frequencies. The echo is the sum of two contributions which are symmetric and antisymmetric, respectively, (dashed lines) with respect to the center point of the echo. The latter point is at time 2τ + tw2 − tw1 from the leading edge of the ﬁrst pulse, where τ is the time interval between the leading edges of the pulses and tw1,w2 are the respective pulse widths [8] 2

3

There are certain advantages to cw technique, however. If T2 is shorter than a few μs, spin echoes may become unobservable, whereupon cw methods become the only way to observe an NMR signal. T2∗ is often a reﬂection of the inhomogeneous linewidth ΔH, in which case T2∗ ∼ 1/γΔH. If such broadening is severe, then T2∗ will be determined by the length and shape of the exciting rf pulse. In the latter case it is usually unobservable because of ampliﬁer dead time.

2.1 Basic NMR Phenomenology

19

We touch here brieﬂy on an important point regarding spin-echo spectroscopy. This is the frequency resolution of this technique, which is discussed in detail in Appendix A.1. Since the NMR signals are excited using pulse ﬁelds H1 of typically 100 Gauss amplitude, one might suppose that these large ﬁelds would limit the available frequency resolution to ∼ γH1 . However, this is not the case. It is straightforward to demonstrate that the total area under the spin echo waveform is proportional to the line intensity at the frequency of excitation to within a very narrow bandwidth. The resolution obtained in this way is formally independent of the magnitude of the excitation ﬁeld H1 . See Appendix A.1 for details. The question of observability of spin-echo signals is an important one for the NMR spectroscopist. We note here that solid-state NMR signals are typically of the order of microvolts, with expected raw signal-to-noise ratios which are typically of the order of unity or less. Thus, one cannot overemphasize the importance of digital signal averaging methods to the success of modern pulsed NMR technique. The great majority of solid-state NMR studies reported nowadays have used digital signal averaging to improve the signalto-noise ratio. It is also possible to estimate the available NMR signal strength given reasonable estimates of the experimental parameters. A detailed discussion of such matters is beyond the purview of the present volume. 2.1.3 Deﬁnition and Interpretation of NMR parameters: T2 The relaxation time T2 represents a fairly complex realm of phenomenology in NMR. Put most simply, T2 is the transverse decay time for nuclear magnetization. But there are several fundamentally diﬀerent mechanisms for T2 processes as well as two major categories of T2 eﬀects, namely (i) T2 for the free-induction signal excited by a single pulse and (ii) T2 for spin echoes. For both of these, homogeneous broadening refers to the eﬀect of local spin-spin interactions such as dipolar [1], pseudo-dipolar [10], and RKKY [11]. Often, however, NMR lines are statically broadened by disorder and other spurious eﬀects, such that free induction signals are not observable. In contrast, one can nearly always observe the spin echo, which typically does not “see” inhomogeneous broadening. The spin echo is a signal observed when two rf pulses are applied at a time interval τ . At time 2τ from the ﬁrst pulse a signal appears which has typically a much longer decay time than the free induction. For the spin echo, T2 is the decay time constant of the echo amplitude E(2τ ) as the pulse separation τ is increased. A simulated spin echo is shown in Fig. 2.3. A basic discussion of spin echo formation and decay mechanisms is given in Appendix A.1. In high-Tc materials, indirect spin-spin couplings are particularly important. A new and useful formulation of indirect spin-spin couplings in terms of dynamical susceptibilities has been given by Pennington and Slichter[12]. This calculation is discussed in detail in Chap. 6. The

20

2 Introduction to NMR Studies of Metals and Superconductors

measurement of the latter indirect spin-spin couplings via spin-echo decay is analyzed in some detail in Appendix A.1. It is interesting that one can write down a formally exact solution to the spin echo decay problem. The following expression represents the variation of the spin echo amplitude at time 2τ for rf pulses applied at 0 and τ :

∗ ∗ ∗ ∗ E(2τ ) = T r Ix eiHi τ eiθ2 Iy eiHi τ Ix e−iHi τ e−iθ2 Iy e−iHi τ /T r(Ix2 ) , (2.1.7) where the spin system I = i I i is being excited with pulses along the y axis which are assumed for simplicity to be uniform over the entire resonance line. Thus, the initial magnetization lies along the x axis and the refocussing pulse is given a pulse angle θ2 . The interaction Hamiltonian Hi represents all pairwise interaction terms between the spins I i as well as with and among any other nuclear species in the system considered. All such terms have been transformed into a reference frame rotating at the frequency of the applied rf pulses, Hi∗ = exp(iωIz τ )Hi exp(−iωIz τ ), and any non-secular time-dependent terms which result are dropped. Included in Hi is a truncated Zeeman term which might ∗ be written HZ = − i [γH(1 + Ki ) − ω]Iiz . If locally non-uniform, the latter term would have a very important eﬀect on E(2τ ) in that it inhibits ﬂip–ﬂop ﬂuctuation processes among the I i . It is slightly ironic that an inhomogeneous term such as this is frequently necessary for the observation of a spin echo. An expression such as (2.1.7) is not often useful for direct evaluation. However, it can be used to argue the basic features of many special cases of echo decay. We give here a few simple examples. It is the essence of spin echo ∗ mentioned above has no direct eﬀect on formation that a term such as HZ echo amplitude. Any other term in Hi∗ which is static and is unaﬀected by the θ2 pulse will also have no direct eﬀect on echo amplitude. Many spin-spin coupling terms cause ﬂuctuations among the spins I i or among spins which are coupled to the I i . These will cause the echo to decay, and will present many highly complicated sub-cases. A simple example of this behavior is analyzed in Appendix A.1. A case of interest which arises in cuprate NMR is the simple case where all spin ﬂip–ﬂop interactions are blocked by local inhomogeneities. There would be no echo decay process except for the fact that the spins I i are inverted (with a substantial probability) by the θ2 pulse. The typically Gaussian echo decay 2 ] found in this case can then be used to measure the E(2τ ) exp[−(2τ )2 /2T2g indirect spin-spin coupling, as mentioned above. The other important contributor to spin-echo decay is the spin-lattice interaction, which modiﬁes the expression (2.1.7) with a multiplicative factor exp(−2τ /T1E ). The decay constant T1E is a parameter of some complexity and is therefore discussed in detail in Appendix A.2. T1E is only equal to T1 in the case where T1 is isotropic and I = 12 for the nuclei observed, or for I > 12 in the highly unusual case that all |Δm| = 1 transitions are degenerate and are contributing to the echo signal. For a more typical case of half-integral I > 12 , where the (− 12 ↔ 12 ) transition is being observed, then 1/T1E = (I + 12 )2 /T1

2.1 Basic NMR Phenomenology

21

(isotropic T1 ) [13]. It is usually important to account for the eﬀect of T1 in spin echo decay in cuprate NMR studies. Expressions derived for this purpose are given in Appendix A.2. 2.1.4 Deﬁnition and Interpretation of NMR parameters: The shift tensor Kαβ NMR frequency shifts are useful for characterizing a resonance line as well as analyzing diﬀerent components in the magnetic susceptibility of a metallic compound. NMR shifts are useful probes, because they always reﬂect one or more components of magnetic polarization in the system, such as spin or Van Vleck paramagnetism. There can, of course, be magnetic polarization without a palpable NMR frequency shift, but there is no magnetic NMR shift without a source of polarization, i.e. susceptibility, to drive it. There are complications, of course, when there are ﬁxed sources of internal magnetic polarization, such as in the mixed state of a type-II superconductor. Such cases are considered in Sect. 2.3. In general, we have omitted consideration of cases which involve magnetic ordering. Shifts, then, are deﬁned to be linear in the applied magnetic ﬁeld H. Analysis of shifts can be quite complex with random powder samples when the shift is anisotropic, and even more so if they are combined with inherently anisotropic quadrupolar splittings. Such cases occur frequently, and it is important to know how to analyze and characterize them. Deﬁning the NMR Shift In general terms, the NMR shift is a measure of how the magnetic induction B diﬀers at a nuclear site in a metallic specimen from its value in free space when the sample is removed. In practice, shifts are referred to bare values of the nuclear gyromagnetic ratio γ, where γ is the ratio γ=

μ I

(2.1.8)

of the nuclear magnetic moment μ to its angular momentum I. “Bare” values of γ are measured in compounds or other environments which are as magnetically neutral as possible. For nuclei of elements which are highly active magnetically, deﬁning γ can be diﬃcult and somewhat arbitrary. On the other hand, even compounds lacking a form of paramagnetism almost always have so-called chemical shifts, which are typically of the order of tens or hundreds of ppm. Such shifts are orbital in origin and have been discussed in detail in [2], Chap. 4. NMR shifts in metals are typically two orders of magnitude larger than chemical shifts, so that the latter are often ignored. In high-Tc compounds, however, we shall see that, e.g. for 17 O and 89 Y , chemical shifts will play a role in the discussion. In d-band metals, however, the NMR shift is dominated by

22

2 Introduction to NMR Studies of Metals and Superconductors

the spin-paramagnetic and Van Vleck terms mentioned earlier. In Sect. 1.2 we discuss a detailed formulation of these eﬀects as well as methods for analyzing NMR shift data. Here we focus on deﬁning and measuring the shift tensor. Given a suitable reference γ, then, the NMR shift K is deﬁned with respect to a change in the resonant frequency νres = γH(1 + K), or K =

νres − 1. γH

(2.1.9)

Since a lot of NMR spectroscopy is done by scanning the magnetic ﬁeld, it is important to note that the fractional shift in the resonant ﬁeld, which is −K/(1 + K), not only has the opposite sign, but a palpably diﬀerent magnitude than K if the shift is large. The unmistakable hallmark of an NMR frequency shift or of a spectrum of shifts for a powder is that they scale precisely with the applied ﬁeld. If this is not the case, then one is dealing with quadrupole eﬀects or other complications. The NMR Shift: Tensor or Scalar? In practice, most shifts are characterized as scalar parameters. However, formally the NMR frequency shift tensor Kαβ is deﬁned to be the α component of the internal ﬁeld at the nuclear spin divided by the β component of the applied ﬁeld ([1], Ch. VI). In general, then, the induced, internal shift ﬁeld is not parallel to the external ﬁeld. This can be a complication in the interpretation of large shift eﬀects. However, in cases where the shift anisotropy is 1% or less, it is a good approximation to replace the shift tensor with a scalar shift given by K(θ, φ) = KX sin2 θ cos2 φ + KY sin2 θsin2 φ + KZ cos2 θ, where the KX,Y,Z are the principal values of the shift tensor and (θ, φ) give the orientation of the ﬁeld H in the principal axis coordinates. Another approach, which involves no approximation, is to conﬁne shift measurements on oriented powder or single crystal samples to ﬁeld orientations along the principal axes. The (X,Y,Z) axes will generally coincide with crystalline axes of symmetry. In metals with cubic crystal structure or with single crystals, then, shift measurements are usually straightforward. If microscopic disorder is reasonably low, then line-broadening eﬀects will be 0.01% or less and a 1% shift can be reliably measured to good accuracy. If the nuclear site is non-cubic, however, there is the possibility of an anisotropic shift as well as the virtual certainty of quadrupolar shifts and broadening for I > 12 . For such cases it is very helpful to have either single crystals or oriented powders for non-cubic systems4 . Otherwise, data will have to be obtained by analyzing powder patterns, i.e. broadened spectra which result from a sample made up of randomly 4

Oriented powder samples are samples with anisotropic susceptibilities which have been induced to form partially-to-fully ordered dominant magnetic axes in a magnetic ﬁeld. This technique was of great importance for NMR and susceptibility studies of high-Tc materials. See Sect. 3.1 for a more extensive discussion.

2.1 Basic NMR Phenomenology

23

oriented particles. The functional form of the axial shift powder pattern is the same as for the ﬁrst-order quadrupolar satellite pattern (2.1.5), namely, 1

ρK (K) = [6Kax (K − Kiso + Kax /2)]− 2 ,

(2.1.10)

where K is the shift variable, which is distributed over the range Kiso - Kax /2 ≤ K ≤ Kiso + Kax . For a crystal with applied ﬁeld at an angle θ with respect to the axis of symmetry, the shift may be written Kiso + Kax (3cos2 θ − 1)/2, where Kiso and Kax are the isotropic and axial components of shift, respectively. If the three principal shift values are all diﬀerent, then the symmetry is lower than axial and the singularity disappears. The distribution will have edges at the maximum and minimum shift values, with a peak at the intermediate principal shift value. It is possible, although it may be somewhat laborious, to extract anisotropic shift as well as quadrupole frequency parameters from powder patterns. For the (- 12 ↔ 12 ) transition the change of these two eﬀects with ﬁeld are opposite, so that ﬁeld dependence can be employed to determine their separate values. An example of this is shown in Fig. 2.4 axial shift powder patterns. 2.1.5 Deﬁnition and Interpretation of NMR parameters: T1 T1 is the time constant which describes the exchange of nuclear spin energy with the surrounding lattice, hence it is known as the spin-lattice relaxation time. Referring to the energy levels in Fig. 2.1, T1 determines the rates at which nuclei make transitions between these levels. Magnetic T1 processes are generated by ﬂuctuating HF ﬁelds. Each magnetic HF interaction5 has a ﬂuctuation spectrum with an amplitude and an autocorrelation time. The corresponding T1 process is driven by the fourier component of the latter spectrum at NMR/NQR resonance frequency. The magnetic dipole T1 processes are divided broadly into those driven by spin and orbital HF ﬁelds. The formulation of the various relaxation processes for metallic systems including superconductors has been a major work in progress since NMR was ﬁrst discovered. Below we review the interpretation of T1 eﬀects for simple metals and Type I superconductors (Sect. 2.2) and for d-band metals and Type-II superconductors (Sect. 2.3). The interpretation of T1 processes for the cuprate superconductors will be discussed extensively in Chaps. 3–6. Particularly important is the role played by electron-electron interactions in T1 phenomena. Accordingly, we review Moriya’s theory of correlated electron eﬀects in the T1 processes of simple metals in Sect. 2.2. Rather more rare in occurrence are quadrupolar T1 processes generated by ﬂuctuating components of EFG. A general theory of such eﬀects caused by the phonon Raman scattering process was put forward by Van Kranendonk in the early days of NMR [14]. Such processes are extraordinarily weak, however, 5

See Sect. 2.2 for a comprehensive deﬁnition of the magnetic HF interactions.

24

2 Introduction to NMR Studies of Metals and Superconductors 2nd Order Quadrupole + Anisotropic Shift A = 1/2, B = 2

A = 2/3, B = 3/2

A=B=1

A = 2, B = 1/2 –4

–2

0

2

4

Fig. 2.4. Powder patterns are shown for several cases the combined eﬀects of an anisotropic shift and second-order quadrupolar broadening. The total broadening perturbation is A sin2 θ (9 cos2 θ − 1) + B (3cos2 θ − 1). In applied ﬁeld H, A ∝ 1/H and B ∝ H. In reduced units we let B = H, and the frequency displacement is in 2 /16νL (for I = 3/2). The spectra then show a progression of powder units of 3νQ patterns as H is varied from 1/2 up to 2. The dashed vertical lines show the positions of the three edges in the absence of broadening. The prominent upper singularity (see Fig. 2.2) converges with the θ = 0 edge with increasing ﬁeld and disappears above B/A = 8/3. However, there is still a visible maximum for the top example, where B/A = 4. Note that these spectra are actually oriented the way they would appear in a ﬁeld sweep increasing to the right, and, therefore, the anisotropic shift coeﬃcient is negative. With B/A < 0, the patterns would be quite diﬀerent. Studies such as are shown here allow the practitioner to extract values of A and B from experimental data

and have rarely been identiﬁed in metals. Nonetheless quadrupolar relaxation processes for the 63,65 Cu isotopes have occasionally been claimed to exist in solids, using the isotopic ratio of T1 values as a diagnostic.6 When quadrupolar T1 eﬀects occur in metals, it is our conjecture that they are much more likely to be caused by ionic motion (e.g. diﬀusion) than by phonons. The Magnetic Dipole Relaxation Process Nuclear spin transitions generated by the HF interactions in (2.2.1) are known as magnetic dipole transitions (as opposed to electric quadrupolar transitions). Here, we analyze the magnetic dipole T1 process in some detail. We review methods to measure it as well as certain pitfalls to be avoided in conducting 6

The ratio 63 T1 /65 T1 is a good diagnostic for this purpose, since it is (γ65 /γ63 )2 = 1.148 for magnetic relaxation and is (Q65 /Q63 )2 = 0.854 for electric quadrupolar relaxation.

2.1 Basic NMR Phenomenology

25

such measurements. Whether measuring T1 with high-ﬁeld NMR or in zero ﬁeld with NQR, the nuclear spin energy levels Em will be labeled with the Iz quantum number m. To the extent that m is a good quantum number, the transition rate between states m and m may be written | m |I+ |m|2 W = | m|I− |m |2 W = (I − m)(I + m + 1)W δm ,m+1 (2.1.11) If I = 12 , then there is only a single rate W involved. For I > 12 there are I + 12 rate constants and 2I relaxation eigenmodes. The formula (2.1.11) will be correct for the cases (a) when I = 12 , (b) for arbitrary values of I when η = 0 and the ﬁeld is applied along the principal axis of the EFG tensor, and (c) for NQR when η = 0. It is approximately correct for arbitrary η values when νQ γH/2π and for NQR when η is small. In other cases m-state mixing eﬀects become important and it may be necessary to solve the spin Hamiltonian (2.1.1) numerically to obtain accurate matrix elements of I± . In this discussion of T1 analysis, we shall assume (2.1.11) to be valid, and we shall also neglect nuclear quadrupole relaxation eﬀects. They are, as noted above, quite rare in metallic systems. Detailed Balance in T1 Processes T1 in metals is simpliﬁed by the fact that ﬂuctuation spectra for itinerant fermions are constant over the range of typical NMR frequencies. T1 values are therefore found to be independent of the Zeeman splitting and are the same for NMR and NQR measurements alike.7 We shall assume, further, that the lattice constitutes an inﬁnite heat reservoir at equilibrium at temperature T . To illustrate the incorporation of detailed balance into the rate equations, we analyze a two-level system with energies E2 > E1 , deﬁning ΔE = E2 E1 . The populations of these levels are designated p1,2 and will be treated as continuous variables. The rates at which up and down transitions occur are deﬁned to be W21 (up) and W12 (down), respectively. At thermal equilibrium the principle of detailed balance gives W21 = e−βΔE W12 ([2], Ch.5). The rate equations for populations are then dp1,2 = ±[p2 W12 − p1 W21 ] , dt

(2.1.12)

where p1 + p2 = N is the total number of nuclei in the ensemble. When the p1,2 are at equilibrium we have dp1,2 /dt = 0, giving p2 /p1 = W21 /W12 = e−βΔE . Thus, the Boltzmann distribution of spin populations follows from detailed balance. Writing p1,2 = ± 21 (p2 − p1 ) + N/2, the (2.1.12) may be combined to give 7

Note, however, that NMR and NQR reﬂect diﬀerent relaxation modes, as will be seen below. For example, if I = 32 , for NMR 1/T1 = 2W , whereas the single rate measured with NQR is 6W , or one-third the length of the conventionally deﬁned T1 .

26

2 Introduction to NMR Studies of Metals and Superconductors

d(p2 − p1 )/dt = (p2 − p1 )(W12 + W21 ) − N (W12 − W21 ). From this relation we see that the relaxation rate of (p2 − p1 ) is (W12 + W21 ). Since this quantity must be independent of ΔE, we set (W12 + W21 ) = 2W , where W is a rate constant which depends only on T . Detailed balance then leads immediately to W12 =

2W 2W e−βΔE ; W . = 21 (1 + e−βΔE ) (1 + e−βΔE )

Using (2.1.13), (2.1.12) then becomes dp1,2 N e−βE1,2 = −2W p1,2 − −βEi . dt ie

(2.1.13)

(2.1.14)

Even though p1 and p2 appear to act independently, they are not, of course, independent. The general solution to (2.1.14) is seen to be p1,2 (t) = (p1,2 (0) − p01,02 )e−2W t + p01,02 , (2.1.15) where p01,02 = N exp (−βE1,2 )/ i exp (−βEi ) are the equilibrium population values. This result also satisﬁes p1 (t) + p2 (t) = N if p1 (0) + p2 (0) = N , which must be the case. Relaxation Equations for I >

1 2

Generalization of the foregoing result to multi-level nuclear relaxation equations is straightforward. They can always be written in terms of the diﬀerence variables dm = pm – p0m , with p0m = N exp(−βEm )/

exp(−βEm ),

(2.1.16)

m

where m is the quantum number for the energy eigenvalues. We note that the value of p0m does not depend on the choice of the zero-point of energy. In general, then, one can measure T1 by creating a non-equilibrium population distribution, then observing the decay toward equilibrium of the population diﬀerence of some suitable pair of levels using spin-echo excitation. The latter pair must be chosen to have |Δm| = 1 for magnetic excitation, and they must be chosen to reﬂect a non-equilibrium population diﬀerence during the equilibration process. If the initial non-equilibrium condition is created by applying an rf pulse to some pair of levels, note that the recovery can often be observed using spin-echo signals from a diﬀerent pair of levels.8 This degree of experimental freedom is not often used in NMR. It could be used, for example, to avoid multiple echo eﬀects in a T1 measurement when T1 is very short. 8

This requires the ability to be able to apply rf pulses to the sample at two separate frequencies, which can be a very useful adjunct to the usual spectrometer setup.

2.1 Basic NMR Phenomenology

Relaxation Eigenmodes for I >

27

1 2

For multi-level nuclear spin Hamiltonians (I > 12 )9 there is an eigenmode structure to the relaxation equations with multiple relaxation eigenrates. We illustrate this situation with the simple example of I = 32 , for which there are four energy levels as shown in Fig. 2.1. The dynamical equations for the diﬀerences dm are then dd3/2 dt dd1/2 dt dd−1/2 dt dd−3/2 dt

= −3W d3/2 + 3W d1/2

(2.1.17a)

= 3W d3/2 – 7W d1/2

(2.1.17b)

= 4W d1/2 – 7W d−1/2 + 3W d−3/2

(2.1.17c)

= 3W d−1/2 – 3W d−3/2

(2.1.17d)

We seek solutions of the form dm = cm exp(−λW t). Substitution into (2.1.17) then yields the matrix equation ⎧ ⎫ ⎫ ⎡ ⎤ ⎧ 0⎪ λ−3 3 0 0 c3/2 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎨ ⎪ ⎬ ⎬ ⎨ ⎢ 3 λ−7 4 0 c1/2 0 ⎥ ⎢ ⎥ ⎣ 0 0⎪ c 4 λ−7 3 ⎦ ⎪ ⎪ = ⎪ ⎪ ⎪ ⎩ ⎪ ⎭ ⎭ ⎩ −1/2 ⎪ 0 c−3/2 0 0 3 λ−3 This matrix is solved straightforwardly. The characteristic equation is λ4 –20λ3 + 108λ2 –144λ = 0 ,

(2.1.18)

for which the solutions are λ = (0, 2, 6, 12). The corresponding decay rates are 0, 2W = T1−1 , 6W = 3T1−1 , and 12W = 6T1−1. Ignoring the null mode, the corresponding eigenvectors for T1 , T1 /3, and T1 /6 may be written {3, 1, -1, -3}, {-1, 1, 1 ,-1}, and {-1/3, 1, -1, 1/3}, respectively. The solutions to (2.1.17) may be applied to diﬀerent techniques for measuring T1 . We illustrate their use in the simple case of a cubic environment where Em = −γn (1 + K)Hm. Since |Em | kB T , we may write (2.1.16) N p0m ≈ 2I+1 (1 − δm), where δ = γn H(1 + K)β. Then if we apply an rf pulse with pulse angle θ to the spins, the resulting initial condition is pm (0) ≈

N (1 − δ cos θ m). 2I + 1

N As a result, the initial values are dm (0) ≈ 2I+1 (1 − cosθ) m. The dm (0) have the form {3, 1, -1, -3} of the “T1 ” mode, so that the solution can be written 9

This discussion only applies to nuclei with odd half-integer spin quantum numbers. Many nuclei of interest answer to this description, and, in fact, there will be no nuclear spins of interest in this volume which have integer values of I.

28

2 Introduction to NMR Studies of Metals and Superconductors

dm (t) ≈

N mδ (1 − cos θ) e−t/T1 . 2I + 1

If θ = π, then one has a perfect inversion, which gives the largest excursion in signal amplitude. The time variation of the spin echo signal for arbitrary θ is then proportional to pm (t) − pm+1 (t) =

Nδ [1 − (1 − cos θ) e−t/T1 ]. 2I + 1

(2.1.19)

If pm (0) = pm+1 (0) for all applicable m, then we have a condition known as saturation, which also yields a single-exponential recovery ∝ (1−exp(−t/T1 )), regardless of the distribution of the energies Em . Recovery Mode when only the (− 12 ↔ 12 ) Transition is Excited If there are quadrupolar splittings, then a single pulse applied to the (-1/2 ↔ 1/2) transition results in a {dm (0)} vector with the form a0 {0, 1, −1, 0}. Writing the decay mode as a superposition of the foregoing eigenmodes, we have {dm (t)} =

1 a0 [{3, 1, −1, −3} exp−t/T1 +9{−1/3, 1, −1, 1/3} exp−6t/T1 ]. 10

The spin echo signal for the (-1/2 ↔ 1/2) transition will therefore exhibit the well-known decay function E(t) = E0 (0.9 exp−6t/T1 + 0.1 exp−t/T1 ) .

(2.1.20)

Such a precise mathematical form occurs only for excitation of a single pair of levels over a time interval which is short compared with T1 /6. If relaxation begins to take place during the initial excitation phase, then the simple form of the initial condition is lost and the decay will be rather more complicated. In the foregoing example, d3/2 (t) would be proportional to (exp −t/T1 - exp −6t/T1), so that it would deviate very quickly from its initial value of zero. As we noted earlier, the relaxation measurement could be conducted in this fashion, i.e. by monitoring a diﬀerent transition frequency from the one used for the initial excitation. The NQR Case Continuing our discussion of an I = 32 nucleus, we consider ﬁnally the NQR case, where the ± 12 levels and the ± 32 levels are degenerate pairs separated by an energy diﬀerence of hνN QR = hνQ (1 + η 2 /3)1/2 . A single excitation pulse at the NQR frequency then creates an initial condition given by {dm } = a0 {-1, 1, 1, -1}. This eﬀectively 2-level system relaxes entirely via the symmetric mode with a single decay rate 3/T1 . One must be careful to take account of the relaxation mode eﬀects when comparing T1 data obtained with diﬀerent methods.

2.1 Basic NMR Phenomenology

29

We make a few additional remarks about the decay mode eﬀects described above for the I = 32 system. First, there are many nominally cubic systems where the observed signal is dominated by the (-1/2 ↔ 1/2) transition, because transitions to higher m-values are broadened by stray ﬁrstorder quadrupolar splittings. Such splittings are the consequence of impurities and other forms of crystalline disorder. If such broadening is severe, magnetization recovery may take place via (2.1.5) rather than with the expected single-exponential T1 decay. Since there is a dramatic diﬀerence between these two cases, it is very important to be aware of such broadening eﬀects. A second point we wish to emphasize is that the analysis of T1 relaxation curves given here for I = 32 is entirely independent of the nature of the NMR spectrum. The functional behavior depends only on which pair of levels is used to excite a non-equilibrium initial condition, and on the fact that the quantum numbers m = Iz are relatively pure in characterizing the energy eigenstates. If the latter condition is not fulﬁlled, then numerically evaluated eigenfunctions may be needed to generate suﬃciently accurate relaxation curves. Measuring T1 in the Presence of Spectral Diﬀusion We consider brieﬂy some well-known problems encountered in T1 measurements. Two of the most troublesome are the related problems of inhomogeneous broadening and spectral diﬀusion. These problems occur frequently in d-band metals and intermetallic compounds. The key to accurate T1 measurements is the experimenter s ability to create a strongly non-equilibrium population diﬀerence between a pair of nuclear energy levels as an initial condition. The T1 recovery will then be accompanied by a spin-echo signal which undergoes a substantial change in amplitude. In cases of severe inhomogeneous broadening such as that shown in Fig. 2.5, a diﬃculty arises from the fact that a single pulse of rf ﬁeld will only aﬀect a region of width γH1 , where H1 is the amplitude of the rf pulse ﬁeld. The narrow region saturated by a single pulse is shown as a dotted line in Fig. 2.5(a). If the broadening is entirely static, it may be possible to focus the measurement on the polarization behavior at precisely the irradiation frequency, i.e. the center frequency of the population disturbance shown in the ﬁgure. As noted in Sect. 1.2.2, this can be done by carefully integrating the entire area under the spin echo, so that the measured recovery curve will accurately reﬂect what is taking place at ω = ωrf . However, such broadening may actually have a partially dynamical character owing to the presence of spin-spin couplings of the form Hﬀ = BIi± Ij∓

(2.1.21)

between neighboring nuclei. Under circumstances which occur frequently, the Hﬀ interactions lead to ﬂip–ﬂop dynamical processes between neighboring spins, which then leads to a rapid smearing of the band of excited spins

30

2 Introduction to NMR Studies of Metals and Superconductors

Polarization (Arbitrary Units)

1.2

(a)

1 0.8 0.6 0.4 0.2 0

0

200

400

600

Frequency (Arbitrary Units)

Polarization (Arbitrary Units)

1.2

(b)

1 0.8 0.6 0.4 0.2 0

0

200

400

600

Frequency (Arbitrary Units)

Fig. 2.5. (a) The saturation eﬀect of a π/2 pulse applied at frequency ω0 is shown for an eﬀective pulse ﬁeld amplitude of 20 in units of the frequency scale. The polarization curve is also shown at several later times as T1 recovery takes place without spectral diﬀusion. (b) Development with time of the polarization curve is shown at several stages following the same initial saturation pulse as in (a). The curves are a Gaussian model in which there is no T1 recovery eﬀect, thus the total polarization, plus its ﬁrst moment (ω − ω0 )P (ω)dω, are conserved over the time interval shown. Note the spurious “recovery” of the polarization at frequency ω0 as a function of time

over a much wider range of frequencies than those excited directly by the rf pulse(s). This process, known as spectral diﬀusion, is illustrated with dashed lines in Fig. 2.5b. There results what appears to be a rapid recovery of the polarization at the excitation frequency. However, such a recovery has nothing to do with the T1 process, but is easily mistaken for it. Often it is much faster than T1 , and results in the experimenter’s inability to achieve inversion of the

2.1 Basic NMR Phenomenology

31

polarization10 . This highly undesirable eﬀect has been known in adverse cases to render T1 measurements unfeasible. We consider here the circumstances which give rise to spectral diﬀusion eﬀects and oﬀer a few suggestions on how to deal with this problem. The ﬂip– ﬂop process (m, m ) → (m ± 1, m ∓ 1) between (primarily) nearest-neighbor (nn) spins has been recognized since the early days of NMR as essential for spin diﬀusion, as well as for maintaining thermal equilibrium within the nuclear spin system. Spectral diﬀusion is, in fact, a process whereby a disturbance in a narrow frequency range is able to diﬀuse over the entire NMR line so as to create a uniform spin temperature. However, since an energy-conserving ﬂip–ﬂop transition can only take place between neighbors with nominally the same Larmor frequency, i.e. the same shift value, it is interesting to consider how polarization can migrate over large frequency intervals such as depicted in Fig. 2.5b. With coupling energy of the form of (2.1.21), it is plausible that a ﬂip–ﬂop transition could take place between neighboring spins with a Zeeman frequency mismatch of the order of Δω ∼ B and still conserve energy. The diﬀerence in Zeeman energies is taken up by the transverse terms and eventually dissipated by other ﬂip-ﬂop processes. Over a large number of such ﬂuctuations, the narrow polarization disturbance created by an rf pulse could broaden symmetrically over frequencies well beyond the conﬁnes of the initial excitation proﬁle. To have this happen, of course, the inhomogeneous broadening must be local in character and be otherwise conﬁgured to facilitate the process. One method for measuring T1 under these circumstances is to endeavor to saturate the entire line with a string of pulses known as a comb instead of a single pulse. Were this possible, then all polarization variables would relax back to equilibrium with the single time constant T1 . If pulses at a single frequency do not produce the desired saturation eﬀect, then applying frequency modulation to cover the entire resonance line is known to be eﬀective11 . At low temperatures, however, long strings of pulses may produce undesirable heating eﬀects. If T1 is long enough, another more exotic (but widely used) method is to use ﬁeld switching to create a non-equilibrium initial condition for the T1 measurement. The ﬁeld at the sample can be switched mechanically or electronically. The most obdurate cases occur when T1 is too short, even at low temperatures, for ﬁeld switching, and pulse combs are also not feasible. Ones only option may to be hope that spectral diﬀusion will run its course in a time less than T1 , and that the ﬁnal stage of the polarization recovery process can be analyzed to extract the T1 rate. Needless to say, such an approach also has limited applicability. 10

11

Inability to invert polarization can result from fast spectral diﬀusion, but it is also caused by an inhomogeneous rf ﬁeld H1 so that the pulse condition varies over the sample volume. The author is indebted to W.G. Clark for this observation.

32

2 Introduction to NMR Studies of Metals and Superconductors

2.2 NMR Probe of sp-Band Metals and Type I Superconductors In order to put high-Tc materials into context, this section gives as background material a brief summary of the basic static and dynamic magnetism of “simple” metals as sensed by the NMR probe. These systems give a historical perspective of the subject and provide foundation for the treatment of the more complex d-electron metals. In typical good metals we think about electrons as itinerant fermions which occupy Bloch wavefunctions uk (r)eik·r . Such orbitals are often far removed in character from the atomic states they are actually composed of. Calculations of NMR shift, relaxation, and indirect spin-spin couplings in metals were originally formulated in this bandtheoretical language. The s-character of band electrons is always present and often plays a major role. In contrast, high-Tc systems are bad metals, often with just enough mobile carriers to render the d-holes on the Cu2+ sites itinerant. Some properties remain atomic-like in character and can be thought of usefully in terms of localized wavefunctions. Perhaps by accident, there is very little s-character in the wavefunctions of most high-Tc ions, allowing the less familiar p and d orbitals to dominate. In this section we review the energy-band, k-space picture used to describe the static and dynamic magnetism sensed by the NMR probe in both the normal (nonsuperconducting) and superconducting (SC) states. We begin the discussion with the idealized Korringa treatment of NMR shifts and relaxation, then discuss important modiﬁcations of this picture for actual sp-band metals. Historically, the ﬁrst NMR studies of superconductivity were done on this class of materials. We review problems encountered in reconciling both the shift and relaxation behavior with the BCS theory [15] for these systems. It was with the elemental metals Hg, Sn, Pb, and Al that questions such as the role played by spin-orbit coupling in the behavior of the spin susceptibility and corresponding NMR (Knight) shift ﬁrst came to light. They also gave us our ﬁrst clear understanding of the BCS coherence peak in the T1 rate [16]. Since even before the BCS theory of superconductivity[15] was announced, NMR shifts have been employed to investigate the nature of the superconducting state. In the early days the only known metallic NMR shift was the s-contact Knight shift. Moreover, the original BCS ground state was an eigenfunction of Sz , leading to the naive expectation that K(T ) ∝ χspin (T ). The actual reality was rather more complex. This interesting piece of NMR history will be touched upon in Sect. 2.2. Measurement of such eﬀects has become a standard application for NMR studies. Observation of shift behavior is also very important in the study of high-Tc systems and for any of the latter-day unconventional superconductors.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

33

2.2.1 NMR Shifts and Relaxation in Simple Pauli Paramagnets Following on the discovery of the s-contact NMR shift by Knight [17], one of the ﬁrst theoretical milestones for the NMR study of metals was the Korringa relation between the latter shift and the product T1 T , which was also shown to be independent of temperature [18]. These results were expected to apply to cubic sp-band metals, where it is noteworthy that the p-electrons with their far smaller HF couplings have a nearly negligible eﬀect on both the NMR shift and T1 . The surprise of substantial deviations from the Korringa relation for simple systems such as the alkali metals were therefore a stimulus for Moriya’s treatment of electron-electron interactions in these systems. The result was important modiﬁcations to the Korringa relation, which were then veriﬁed experimentally. This was an important step in the treatment and understanding of electron interactions in metals. We review these developments in the following subsections. The Comprehensive HF Coupling Hamiltonian in Solids As a preliminary step we introduce here the comprehensive HF Hamiltonian l s 3r(s · r) 8 πsδ(r) , (2.2.1) + HHF = 2γμB I · 3 − 3 + r r r5 3 where γI is the nuclear moment located at r = 0 and l and s are the orbital and spin angular momentum operators, respectively, of an itinerant fermion located at r (see [1], Ch. VI). (2.2.1) can be written −γI · He , where He is an eﬀective HF-ﬁeld operator which is the ultimate source of all magnetic shift and relaxation eﬀects in the metallic environment. There are three distinct types of interactions, namely the orbital ﬁeld, the dipolar ﬁeld, and the s-contact interaction. Although it took a number of years for them to emerge, calculations for the metallic shifts listed above were all ultimately based on (2.2.1). Evaluating the thermally averaged eﬀects of He in metallic systems is a matter of great subtlety and complexity. In a very real sense, this is the essence of the high-Tc problem for the NMR probe. The Knight Shift: S-contact HF Coupling in an sp-band Metal The so-called s-contact HF ﬁeld and its corresponding NMR shift in copper metal were discovered by W. D. Knight [17]. This shift is simply given by the expectation value of the ﬁnal term of (2.2.1) when spin polarization from an external ﬁeld H is present. There results a temperature-independent NMR shift given by (2.2.2) Ks = αs χsp , 2 where αs = 8π 3 |uk (0)| , indicating an average over the Fermi surface. χsp = 12 (gμB )2 n(EF ) is the spin susceptibility of the sp band, where n(EF ) is the

34

2 Introduction to NMR Studies of Metals and Superconductors

Fermi surface density of states per atom for one direction of spin12 . We also note that the dipolar HF coupling, i.e. the second and third terms of (2.2.1), also yields a palpable NMR shift in many cases. It vanishes at sites having cubic symmetry, and is, in any case, an order of magnitude or so smaller than the contact shift. In high-Tc materials, where contact shifts are often absent, the dipolar terms take on a much greater signiﬁcance than for cubic metals. Interestingly for the case of copper metal, it later developed that some 40% of the orbital character of the Fermi surface is d-like [19]. As a result, a signiﬁcant fraction of the observed Knight shift for copper is attributable to the orbital Van Vleck term discussed in the next subsection [20]. The Korringa Calculation of T1 The idealized viewpoint regarding a simple metal is epitomized by the seminal calculation of NMR shift and relaxation time by Korringa [18]. In this case, noninteracting electrons were assumed, with a density of states at the Fermi surface describable by band theory. HF interactions with the relevant nuclear spins were limited, not unreasonably, to the s-contact interaction (2.2.1), the p-electron dipolar coupling being negligibly weak in comparison. Cubic symmetry allowed quadrupolar eﬀects and p-electron contributions to the NMR shift to be ignored, and any gradient to the density of states deemed too small to alter low–temperature behavior. The shift expression is given above in (2.2.2). Next, we need to develop an expression for T1 at the same level of approximation. We use the basic golden rule expression from time-dependent perturbation theory, where the perturbing interaction is the s-contact term 2 from (2.2.1), Hsc = − 8π 3 γn γe δ(r)I · s. If we consider the elemental transition from state |k ↑ m to state |k ↓ m + 1, where m is the initial nuclear spin quantum number, the rate for such a transition may be written [2] Wk ↓m+1,k↑m =

2π | k ↑ m + 1|Hsc |k ↓ m|2 δ(Ek − Ek ).

(2.2.3)

To complete the calculation this transition rate must be summed over initial electron states |k ↑ which are occupied and ﬁnal states |k ↓ which are unoccupied. The operative term in Hsc is the one ∝ I+ S− , whereupon the squared matrix element becomes 2 4π 2 γn γe |uk (0)uk (0)| (I − m)(I + m + 1). | k ↑ m|Hsc |k ↓ m + 1| = 3 (2.2.4) The principal approximation is to assume that all states in the vicinity of the Fermi surface have approximately the same probability density at the

12

2

In discussions of experimental susceptibilities, it will be more convenient to use molar units, whereupon the shift coeﬃcient αs will be written 8π|uk (0)|2 /3NA , where NA is Avogadro’s number.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

35

nucleus. Thus, we may replace the quantity |uk (0)uk (0)|2 with the squared Fermi surface average |uk (0)|2 2 . Introducing the restricted sums on k and k and noting further that 1/T1 is twice the coeﬃcient of (I − m)(I + m + 1) (see (1.10) 13 ), this gives 1/T1 =

2 (r) 4π 4π γn γe 2 |uk (0)|2 δ(Ek − Ek ). 3

(2.2.5)

k,k

(r) The restricted sums k,k can be replaced with energy integrals where, for example, the sum on k of states with energy E becomes n(E)dE, where n(E) is the density of states, and the occupation restriction is enforced with the Fermi occupation function f (E) = [exp β(E − EF ) + 1]−1 . The summation in (2.2.5) then becomes dE dE n(E)n(E )f (E)(1−f (E ))δ(E−E ) = n(E)2 f (E)(1−f (E)) dE. (2.2.6) The ﬁnal step is to note that the function f (E)(1 − f (E)) is very sharply peaked at EF at the usual experimental temperatures, so that n(E)2 can be replaced with n(EF )2 . Then we note that the area under the peak in f (E)(1 − f (E)) is easily shown to be kB T . The relaxation rate becomes 1/T1 =

4πkB T

2 4π γn γe 2 |uk (0)|2 n(EF )2 . 3

(2.2.7)

This expression may be combined with the result in (2.2.2) to give the Korringa product, which we write as 1 4πkB γn2 = . T1 T Ks2 γe2

(2.2.8)

Equation (2.2.8) suggests that 1/T1 T divided by Ks2 for these kinds of metals should equal an expression made up of physical constants which is independent of the other properties of the metal. As we shall see below, the result of Moriya’s theory is to multiply the right-hand side of (2.2.8) by a constant factor < 1. Setting that aside for the moment, however, let us see how well the Korringa relation is obeyed in simple metals. In Table 2.1 shift and relaxation data from the literature are listed for the alkali metals and the noble metals Cu, Ag, and Au [3]. These elemental metals all have cubic crystal structures, so that dipolar shift eﬀects do not come into play. Using the measured shift values, values of T1 T extracted from (2.2.8) are compared with experimental values. It is seen that the latter values are generally smaller than those obtained from 13

For simplicity, detailed balance considerations are omitted here.

36

2 Introduction to NMR Studies of Metals and Superconductors

Table 2.1. NMR shift and relaxation data are tabulated for alkali metals and for the noble metals, along with values of T1 T derived from (2.2.8). To test the validity of the Korringa relation, a relative Korringa product deﬁned as (T1 T Ks2 )−1 divided by 4πkB γn2 /γe2 is listed in column ﬁve Metal and Isotope 7

Li Na 85 Rb 133 Cs 63 Cu 109 Ag 197 Au 23

Ks (%)

T1 T(expt.) (secK)

0.0263 0.112 0.650 1.47 0.232 0.522 1.4

45.0 4.8 0.81 0.13 0.9 9.0 4.0

± ± ± ± ± ± ±

2 0.1 0.08 0.01 0.2 1.0 0.5

T1 T(Korringa) (secK)

Relative Korr.Prod.

26.0 3.1 0.63 0.069 0.7 4.5 4.5

0.58 0.65 0.78 0.53 0.78 0.50 1.13

(2.2.8). Including p-electron dipolar hyperﬁne ﬁelds in the relaxation calculation would only make this discrepancy larger. Thus, the most serious defect in the Korringa treatment appears to be the neglect of electron-electron exchange enhancement eﬀects, which we shall discuss next. 2.2.2 The Moriya Theory of Exchange Enhancement in Simple Metals There are various corrections one could make to the Korringa treatment of relaxation. The electron-electron interaction potential has the eﬀect of enhancing the spin susceptibility, and thus the NMR shift [21], in close analogy with the enhancement eﬀect of ferromagnetic exchange among localized moments. However, it was pointed out by Moriya [22] that exchange ﬂuctuations would also enhance the T1 process. Moriya’s calculation of this eﬀect in the random phase approximation showed this enhancement eﬀect to be substantial, but not as great as that of the shift and susceptibility. This is consistent with the values shown in Table 2.1, where the experimental Korringa product (Relative Korr. Prod.) is consistently smaller than the result in (2.2.8). Thus, the measured Korringa products can be used with the Moriya theory (see below) to estimate the magnitude of these enhancement eﬀects. We give an outline of the random-phase approximation calculation here, and refer the interested reader to [22] and [3] for a more detailed account. As noted above, the shift has a simple exchange-enhancement factor, Ks = Ks0 /(1 − α) = αs χs0 /(1 − α), where α = ρ0 χs0 , and ρ0 = 2πζ/2 γe2 . Finally, ζ is the q-independent (by assumption) electron-electron interaction potential. The single parameter ζ drives the enhancement of both static and dynamic spin susceptibilities in the random phase approximation picture. For T1 the ﬂuctuation enhancement is q-dependent. In Sect. 3.5 these magnetic properties will be discussed in terms of q and ω–dependent susceptibilities. Here, we simply state the result for a spherical Fermi surface:

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

1 4πkB γn2 = K(α), 2 T1 T Ks γe2

37

(2.2.9)

1 where K(α) = 2(1 − α)2 0 dx x/[1 − αG(x)]2 , and G(x) is the Lindhard function for free electrons given by 12 {1 + [(1 − x2 )/2x]ln|(1 + x)/(1 − x)|}, with x = q/2kF . G(x) is integrated over the range of q values which span the Fermi surface. We see in (2.2.9) that the Korringa product of (2.2.8) is simply multiplied by the quantity K(α). The enhancement factor for Ks is that for q = 0 (G(0) = 1), while that for 1/T1 is for G(q > 0) < 1. Therefore, K(α) declines from 1 to 0 as α varies from 0 to 114 . If other eﬀects which modify the Korringa product are largely absent15 , the experimental value of K(α) can be used to estimate the electron-electron exchange (i.e. the value of α) in sp-band metals. A few examples are given in Table 2.2, where α values in the range of 0.2 ≤ α ≤ 0.4 are seen to be typical. Rather surprisingly, susceptibility enhancement eﬀects are present to the degree of 25% to more than 50% in these nearly free-electron metals. The Korringa product is often used as a diagnostic tool to examine the nature of the T1 process. Table 2.2. A tabulation of enhancement parameters α derived for a selection of s-band metals from experimental data using (2.2.9). For comparison, calculated values given by Pines [21] are listed Elemental Metal 7

Li Na 85 Rb 109 Ag 23

14 15

α from K(α)

α calc. (Pines)

0.36 0.30 0.19 0.43

0.37 0.24 0.15 0.32

A plot showing K(α) vs. α is given in [3]. Experimental values of the Korringa product can deviate sharply from that in (2.2.8) for a number of reasons. We give three examples, First, if the s-character of Fermi surface orbitals is unusually weak, then p-electron contributions which have been neglected here may play a large role. Second, if the degree of s-character is strongly non-uniform over the Fermi surface, then one of the principal assumptions of the calculation breaks down. Third, if there are multiple bands or multiple neighbors (in the case of ligand nuclei), the experimental Korringa product will change drastically. For example, if a ligand nucleus has N independent but equivalent sources of HF ﬁeld and ﬂuctuations, then the shift and relaxation rate will both be N times that from a single source. It follows that the Korringa product will be the value from a single source divided by N. The latter case is encountered frequently for ligand nuclei in intermetallic compounds.

38

2 Introduction to NMR Studies of Metals and Superconductors

2.2.3 NMR in the Superconducting State of Simple Metals We present here a brief account of the superconducting properties of sp– band metals. Historically, several fundamental issues were resolved with these systems following initial uncertainties regarding both theory and experiment. A clear and comprehensive review of early work was given by MacLaughlin [5]. Some elemental metals addressed in the early days were Hg(4.15K), βSn(3.74K), Pb(7.22K), and Al(1.18K), where their respective values of Tc are given in parentheses. They are all Type I superconductors, which means that their coherence lengths ξ(0) are long compared with their London penetration depths λ(0)16 . With the announcement of BCS theory [15], there were a number of interesting issues to investigate. The principal ones for the NMR probe were (a) the expected collapse of the spin susceptibility at T < Tc owing to the SC energy gap for quasiparticle excitations and (b) the existence of a singularity, which becomes the coherence peak, just below Tc in a plot of 1/T1 vs. T . Because of the large superconducting diamagnetism which occurs below Tc , virtually the only means of measuring the relatively tiny Pauli susceptibility term is through the associated Knight shift Ks (2.2.2). We shall discuss the superconducting shift measurements ﬁrst. The Knight shift for T < Tc : Verifying the Yosida function Performing NMR measurements in the SC state of Type I superconductors was a particular experimental challenge, because of the limited magnetic ﬁeld penetration depth λ ∼ 500˚ A for these systems. In order to get a reasonably uniform internal ﬁeld for NMR studies, experiments were performed on ﬁne particles or thin ﬁlms with at least one dimension which was small compared with λ. The resulting samples generally exhibited superconductivity with Tc near the bulk value and NMR lines with relatively little diamagnetic shift or inhomogeneous broadening. Particles with dimension d λ have greatly reduced diamagnetism in the SC state. Other than that, it was generally believed that these samples exhibited bulk NMR properties. However, the peculiar results obtained at ﬁrst for K(T ) vs. T for T < Tc demonstrated that the foregoing statements were not entirely correct. To see this clearly, we must ﬁrst describe the results that were expected from the shift measurements, then what was actually found, and ﬁnally, how to account for the observed data. The BCS theory prescribed an energy gap Δ(T ) above the superconducting ground state for quasi-particle excitations when T < Tc . As Δ(T ) increases below Tc the spin susceptibility χsp (T ) and Ks (T ) = αs χsp (T ) were expected to decline and asymptotically approach 0 as T → 0. The theoretical functional form of χsp (T ) for T < Tc is known as the Yosida function [23]. 16

A brief discussion deﬁning the coherence length and penetration depth parameters is given in Sect. 2.2.4.

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

39

Experimentally, however, large residual T → 0 shift values were reported. For the 199 Hg NMR in SC Hg, for example, Ks (T → 0)/K(T > Tc ) 2/3 was found [24], with similar results for 119 Sn in βSn [25], 207 P b in P b [26], and 27 Al in Al [27]. These results caused great consternation and confusion, and it was a number of years before a satisfactory understanding was reached [28]. Spin–Orbit Scattering: The Ferrell–Anderson Picture In the end, it was realized that the theoretical preparation was incomplete, and further developments with the Al metal samples showed that the earliest results were incorrect. We shall return to the Al story below. The problem with the Yosida/BCS calculation was that it had neglected spin-orbit coupling and its role in generating spin-ﬂip scattering processes. The situation was eventually addressed and for the most part resolved in short papers by Ferrell [29] and Anderson [30], as well as in a longer paper by Abrikosov and Gorkov [31]. We consider brieﬂy the physical picture presented in Anderson s treatment [30]. In the presence of spin-orbit coupling one must bear in mind that Sz for the electrons is no longer a good quantum number, and that the spin-up and spin-down states are mixed into eigenstates which are no longer have any particular average value of spin. However, a very subtle point is this: In clean, bulk regions of the pure metal there is no spin-ﬂip scattering even in the presence of strong spin-orbit coupling. Thus, the spin susceptibility will still vanish as T → 0 in the SC state. However, what modiﬁes this ideal result is a spin-ﬂip scattering lifetime τso which is short enough that the quantity /Δ(0)τso is no longer small. In other words the smearing of the eigenstate energies from τso becomes comparable with the SC energy gap. Spin-ﬂip scattering occurs only where ordinary potential scattering is strong, e.g. near surfaces and near impurities in the bulk. Ironically, then, this eﬀect will be important near surfaces where rf ﬁelds penetrate and NMR signals are excited, but not necessarily in bulk regions which cannot be probed. Anderson treated the spin-orbit scattering problem using his theory of dirty superconductors[32]. His result for the T → 0 susceptibility ratio is an expression which can be integrated numerically, from which the following limiting cases are given [30]: χso (T χso (T χso (T χso (T

1 Tc ) ≈ , Δ(0) /τso > Tc ) 6 Δ(0)τso Δ(0)τso Tc ) ≈1−2 , Δ(0) /τso . > Tc )

(2.2.10a) (2.2.10b)

Equations(2.2.10) show that when τso is long there is only a small residual value of χsp (T Tc ), but when it is short, i.e. strong spin-orbit scattering near surfaces, χsp (T Tc ) is only slightly perturbed from its normal state value. The latter case is often found for heavy metals such as Hg [24] and Pb [26], and was also found for βSn [25, 33]. These authors performed various

40

2 Introduction to NMR Studies of Metals and Superconductors

doping experiments, which were also consistent with (2.2.10). Ferrell obtained a result similar to (2.2.10b) by means of a physical argument [29]. In a metal as light as elemental Al one might expect spin-orbit eﬀects to be very small. Since colloids of Al are diﬃcult to prepare, shift studies were performed on thin ﬁlm samples. The ﬁrst results gave, surprisingly, residual shift values of ∼75% [27]. It appears that orientation of their multi-ﬁlm samples was quite critical, as subsequent work [34] yielded a very small residual shift. Later measurements by Fine, et al., on a single thin-ﬁlm sample [35] gave results in good agreement with the Yosida function [23]. These data are displayed in Fig. 2.6, ﬁnally giving veriﬁcation to the BCS theory-based prediction. T1 Behavior Below Tc : The BCS Coherence Factor The behavior of T1 for an sp-band (Type I) superconductor according to the BCS theory was ﬁrst investigated, theoretically and experimentally, by Hebel and Slichter [16]. We sketch the calculation of T1 in the SC phase following the derivation in [5]. First, recall from Sect. 1.2.1 that the T1 process consists of scattering fermions from an initial state |kσ to a ﬁnal state |k − σ, while the nuclear spin goes from m to m ± 1 so that angular momentum is conserved. This outline is maintained in the SC state, but other circumstances change drastically. For T < Tc there is some fraction of fermions which are paired (|kσ with | − k − σ) into singlet states and do not scatter. The quasiparticles not condensed into the ground state are thermally excited above the energy gap Δ(T ) and are available to scatter as sketched above. The main diﬀerences are that, ﬁrst, there appears in the summation in 2.2.5 a factor C± (k, k) = 1 2 2 [1 ± (Δ /Ek Ek )] known as the coherence factor, and second, the normal state density of states factors in the integrals leading to 2.2.7 are replaced by the BCS density of states nBCS (E) = n(EF )E/(E 2 − Δ2 )1/2 , where Δ ≤ 1.2 27Al

Ks /Ks(T = Tc)

1

in Al

0.8 0.6 0.4 0.2 0

0

0.5

1

1.5

T/ TC

Fig. 2.6. Data for the 27 Al Knight shift in Al metal from [35] are shown, plotted in units of the normal state shift as a function of T /Tc . The solid curve is the Yosida function, i.e. behavior expected on the BCS theory

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

41

E ≤ ∞. The coherence factor arises because of the pairing of electrons in the condensed phase, and is characteristic of many dynamical properties treated with BCS theory [7]. The choice of sign for C± (k, k ) depends on whether the scattering perturbation is invariant under time reversal applied to the fermion bath. If it is, as in the case of phonons (e.g. ultrasonic attenuation) then C− (k, k ) applies. If it is not invariant, such as for electromagnetic absorption and magnetic dipolar nuclear relaxation, then C+ (k, k ) applies. For the superconducting nuclear relaxation rate 1/T1s one ﬁnds, in units of the normal state rate 1/T1n, ∞ 2 dE (EE + Δ2 ) f (E) (1 − f (E )) T1n = , (2.2.11) T1s kB T Δ [(E 2 − Δ2 )(E 2 − Δ2 )]1/2 where E = E ± γn H. Below Tc the excitation probability is the Fermi function f (Eg ) = [exp(βEg )+ 1]−1 of the gapped energy Eg = (E 2 + Δ2 )1/2 . Since the nuclear Zeeman energy γn H is minuscule on the scale of the quasiparticle energy, there is in fact a logarithmic singularity in 2.2.11 for the case of the coherence factor C+ (E, E ). The most satisfactory explanation for how this singularity is “tamed” is by means of anisotropy of the gap energy Δ(T ) [5, 36]17 . The nuclear Zeeman energy will be neglected henceforward. The behavior of T1n /T1s in 2.2.11 may be divided into two regions, kB T Δ(T ) and kB T > Δ(T ). For kB T Δ(T ) the integral is dominated by the peak in nBCS (E) near the gap, which becomes very nearly constant Δ(T ) ≈ Δ(0). In this limit the factor f (E)(1 − f (E)) ≈ exp(−βΔ(0)), so that 1/T1s decays exponentially at low T. In the other limit kB T > Δ(T ) (T near Tc ), the factor f (E)(1 − f (E)) will have nearly its normal-state value, and the singularity in 2.2.11 has the potential to elevate T1n /T1s to values considerably in excess of 1. This is the source of the well-known BCS coherence peak in 1/T1 (T ) at T < Tc . This peak was ﬁrst measured on 27 Al in Al metal and identiﬁed by Hebel and Slichter [16], establishing a major milestone in experimental conﬁrmation of the BCS theory. It is important to note that for measurements such as ultrasonic attenuation the appropriate coherence factor to use is C− (k, k) , whereupon the factor (EE + Δ2 ) in the numerator of (2.2.11) is replaced by (EE − Δ2 ). This eﬀectively cancels the singularity at E Δ. As a result, the ultrasonic attentuation coeﬃcient was expected to fall abruptly below Tc , as had been conﬁrmed experimentally [37]. This striking contrast between results obtained with probes having diﬀerent symmetry properties was an important conﬁrmation of the correctness of the BCS picture. Following the Hebel-Slichter results, Masuda and Redﬁeld [36] reported further T1 measurements on 27 Al in Al metal taken at temperatures ranging 17

This broadening mechanism was suggested in [36], where it was noted that it gave a good account of the variation of T1 below Tc . The uniform energy gap parameter Δ(T ) in BCS theory is, in fact, an approximation, where the actual gap parameter is properly a function of k. See the book by Tinkham [6], Sect. 2–6, for more discussion of this point.

42

2 Introduction to NMR Studies of Metals and Superconductors

from above to well below Tc . Their results (Fig. 2.7) oﬀered a full panorama of the BCS-theoretical behavior, with a coherence peak (in 1/T1 ) rising above the normal state Korringa curve by a factor ∼ 2, then descending into the superconducting state in a clearly exponential fashion. These data were obtained with a ﬁeld-switching technique similar to that used in [16], the main diﬀerence being that pumped 3 He cooling allowed them to extend the measurements to 0.35K, i.e. far below Tc = 1.18K for Al metal. Analyzing T1 Data in the Superconducting State Since the formulation of (2.2.11) has been widely employed to analyze SC-state data on high-Tc materials as well as all manner of unconventional superconductors, we recount here the analytic procedure used to ﬁt the Al data in some detail [5, 36]. These results are referred to in other sections of the book as well. In order to control the singularity in (2.2.11), Hebel and Slichter [16] postulated a broadening of the electronic energy levels. While such a device enabled them to obtain a reasonable result for the coherence peak, it lacked a clear physical basis. Masuda and Redﬁeld, on the other hand, suggested that the

10.0

T1 (SEC)

5.0

THEORY (r = IOεo(O)/εo(T); GAP = 3.2 kTc)

1.0 0.5

PURE 325 MESH POWDER

0.1

1.0

1.5

2.0 Tc / T

2.5

3.0

Fig. 2.7. A semilog plot of T1 data for the superconducting state of Al metal vs. Tc /T (dots) [36]. Also shown is their ﬁt of the data to the BCS theory (solid line), where the coherence peak (i.e. T1 miminum) amplitude was adjusted using a distribution of energy gap values attributed to anisotropy. The low–temperature energy gap value is adjusted to the slope of the data, yielding Δ0 = 3.2 kB Tc in reasonable accord the the BCS weak-coupling value of 3.52 kB Tc . Reprinted ﬁgure from Y. Masuda, A. C. Redﬁeld, Phys. Rev. 125, 159 (1962). Copyright 1962 American Physical Society

2.2 NMR Probe of sp-Band Metals and Type I Superconductors

43

observed peak was conditioned by a mild anisotropy of the gap parameter Δ(T ). This has a clear physical origin in the BCS equations and gives quite a good ﬁt to the data a well. There, the gap parameter is formally a function of k, and the k-independent gap parameter is just a convenient approximation used to solve the equations. Ample theoretical evidence has been reported for gap anisotropy eﬀects from van Hove singularities and other causes [38]. To illustrate the T1 analysis with (2.2.11) we summarize brieﬂy the development in [5] and [36], and refer the reader to these sources for a more detailed discussion. The procedure is to incorportate the gap anisotropy into the BCS density of states factors in (2.2.11) at the point where sums on k and k are converted to energy integrals. We therefore back up a step from (2.2.11) and rewrite it as ∞ T1n 2 = [Ns (E)2 + Ms (E)2 ] f (E) (1 − f (E))dE, (2.2.12) T1s kB T 0 where

a2

E P (a)da , 2 − Δ(T )(1 + a)2 ]1/2 [E a1 a2 Δ(T )(1 + a) P (a)da and Ms (E) = Re . 2 − Δ2 (1 + a)2 ]1/2 [E a1 Ns (E) = Re

(2.2.13a) (2.2.13b)

In (2.2.13) the variation of Δk over the Fermi surface is represented as a distribution P (a) extending over a1 ≤ a ≤ a2 , where Δk ⇒ Δ(T )(1 + a) and a P (a)da = 0 by deﬁnition. As noted in [5], because the averaging over a is followed by integration over E, the precise shape of P (a) is functionally immaterial to the ﬁnal results. In ﬁtting the T1 data of Fig. 2.7, a2 determines the depth of the T1 minimum and Δ(0) ﬁxes the slope of the exponential tail. The ﬁt shown corresponds to 2Δ(0) = (3.2 ± 0.2)kB Tc and a2 1/2 0.05, in reasonable agreement with the BCS weak-coupling theoretical value 2Δ(0) = 3.52kB Tc . Comparable gap values are given by other probes [5]. There has also been extensive experimentation with doping eﬀects on the SC T1 behavior, yielding some interesting eﬀects. For example, it was found that shortening the mean free path l of the quasi-particles led to even larger coherence peaks in the T1 data for Al [39] and In-based [40] dilute alloys. This eﬀect can be rationalized in terms of the theory of “dirty superconductors” [32], where potential scattering caused by impurities can become strong enough to cause eﬀective mixing between Bloch functions on diﬀerent parts of the Fermi surface. The result is a smoothing out of intrinsic gap anisotropy. Data for the Al-based systems was in good agreement with a theory of this eﬀect [41], but for In-based alloys, there was only agreement for l > ξ0 , where ξ0 is the coherence length. It was suggested that gap inhomogeneity might be suppressing the coherence peak in such a case. However, no further resolution of this point has apparently been reported. As we shall see in the next subsection, there are a number of d-electron superconductors where T1 has no coherence peak for reasons which are also not

44

2 Introduction to NMR Studies of Metals and Superconductors

clear. Moreover, among high-Tc systems, suppression of the coherence peak in T1 is universal, as is also the case for many unconventional superconductors. We defer further discussion of this point to subsections below, where fuller descriptions of the systems concerned are presented.

2.3 Static and Dynamic Magnetism in d-band Metals In this subsection we review the additional complexities which arise when a conductive solid has an open d-shell in addition to its sp-band eﬀects. D-electrons in solids are typically more tightly bound to their host ion, interacting more weakly with neighbors. As a result they have narrower, more highly structured energy bands with substantially higher densities of states at their Fermi surfaces. Moreover, they are subject to a crystalline electric ﬁeld (CEF) which results from bonding and proximity to neighboring ions, which breaks the full rotational potential symmetry enjoyed by a free ion. As a result, the d-electron angular momentum “always” has a zero expectation value in the ground state. On the other hand, the greater densities of states of d-bands, when combined with the electron-electron exchange eﬀects [21] which came to light in the Moriya treatment of enhanced NMR shifts and relaxation [22], lead to strongly enhanced susceptibilities and even to permanently magnetized ground states in a number of pure metals (e.g. Fe, Co, and Ni in the 3d series). Moreover, ions with d-electrons as dilute impurities or dopants frequently possess a localized magnetic moment. However, discussion of d-ion systems possessing full atomic magnetism is beyond the scope of this volume. Special Features of NMR in d–Band Metals and Superconductors Keeping superconductivity in mind, we shall restrict our attention to d-electron systems which do not order magnetically. We consider, as an example, the behavior of the V3 X series of compounds, which are superconductors as well. There is a wealth of interesting NMR phenomena which arise in such systems, including: •

•

Prominence of the core-polarization (CP) d-spin HF ﬁeld in studies of d-band magnetism. Since d-electrons have no contact interaction, this isotropic, negative HF coupling, which was identiﬁed by Heine [42] and by Wood and Pratt [43], takes it place. The core polarization plays a major role, since dipolar interactions are often smaller and are cancelled by cubic symmetry. The greatly enhanced importance of orbital eﬀects, both the static (Van Vleck) shift and susceptibility and the robust orbital T1 mechanism. The d-band orbital susceptibility was ﬁrst formulated by Kubo and Obata [44]. Its contribution to the NMR shift was identiﬁed by Clogston et al., [45] in connection with the V3 X compounds, where it had important consequences for the interpretation of superconducting shift data.

2.3 Static and Dynamic Magnetism in d-band Metals

•

•

45

The latter authors [46] also pioneered the use of the K−χ plot as a means of analyzing NMR shifts and their corresponding susceptibility components in d-band metals. This technique continues to be used very widely and has led to great insight into the magnetic infrastructure of metals and intermetallic compounds. We present their method below. When d-electron metals are superconductive, they are nearly always TypeII superconductors. Thus, NMR studies are very often conducted in the mixed state, i.e. in the presence of a large magnetic ﬁeld and a vortex lattice. The ﬁeld penetrates throughout the sample, dividing itself into as many ﬂux bundles as possible, which occurs when each vortex contains just one ﬂuxon. We shall review results on NMR shifts, lineshapes, and on T1 studies as well. These eﬀects are directly relevant to superconductive highTc NMR studies, since they are often conducted under the same conditions.

2.3.1 The d-Electron HF Interactions In general there are two types of d-electron HF interactions, namely spin and orbital, the latter arising from the ﬁrst term in (2.2.1), and the former from the second two terms. In d-band metals there are also multiple bands with their own Fermi surface density of states and corresponding HF interaction terms. These terms will make additional contributions to the NMR shift and relaxation rates, rendering the task of analyzing experimental data for these parameters a bit more complex. By and large, however, d-electron bands are somewhat more “lively” than their rather prosaic s and p counterparts, and tend to dominate the nuclear spin properties. In high-Tc materials, depending on your point of view, there is scant evidence for actual sp-bands per se, so the d-electron HF eﬀects are, by any measure, the dominant ones. Anisotropic d-Spin Susceptibility and HF Tensor If we allow the d-spin HF coupling to be anisotropic, we then take Hds =

Adξ Iξ Sξ with χdξ =

ξ=x,y,z

NA gξ μB Sξ . H

(2.3.1)

The d-spin shift coeﬃcient is then deﬁned as αdξ =

Kdξ Adξ = . χdξ NA γgξ μB

(2.3.2)

For ordinary 3d metals we shall take gξ ∼ 2, whereupon αd becomes isotropic. However, these deﬁnitions will carry over into the cuprate discussion in Chap. 3, where for the cuprates there is evidence for substantial g-shifts. We also note here that the HF coeﬃcient can be quoted as simply Adξ in ergs, as Adξ / in units of s−1 , as 10−3 Adξ /γ in kG/spin, as 10−3 Adξ /γgξ in units of kG/μB , or as Adξ /1.60218 × 10−12 in eV. Although it may be somewhat

46

2 Introduction to NMR Studies of Metals and Superconductors

confusing, one ﬁnds all of these units in use in the high–Tc literature. The d-spin HF ﬁeld is also known as the core-polarization HF ﬁeld (hence Ad → Acp ), which we now discuss. Core-Polarization Hyperﬁne Coupling: The Mechanism Since d-electron wavefunctions vanish at the site of the nucleus, they possess no direct contact HF ﬁeld from the ﬁnal term in (2.2.1). However, they do activate the contact HF term indirectly in such a way as to generate an eﬀectively isotropic HF coupling with the nuclear spins. This mechanism came to light with the work of Heine [42] and of Wood and Pratt [43]. Detailed calculations have been given by Freeman and Watson [47]. The mechanism of the core polarization HF ﬁeld is a simple consequence of the Pauli exclusion principle, and works as follows. In d-electron atoms there are two or more ﬁlled s-shells which are magnetically inert. Nonetheless, these ﬁlled s-shells undergo repulsive coulombic interactions with the Fermi-surface d-electrons which, generally speaking, lie outside of them, i.e. at larger distances from the nucleus. Thus, coulomb repulsion drives the s-shell electron orbitals closer to the nucleus. This repulsive eﬀect is, however, dependent on spin. Consider the majority d-spin moment to point up. The up-moment s-shell electrons are then known to avoid close proximity with the up-moment d-electrons in a Pauli-exclusion eﬀect known as the Fermi hole. The down-moment s-electrons have no such eﬀect. With the same wavefunction, then, the down-moment s-electrons will have a higher coulomb repulsion energy. For that reason, the down-moment s-shell orbitals will tend to “shrink” toward smaller radii relative to the upmoment s-shell orbitals, creating a net down moment of s-electron density at the nucleus, i.e. a net negative contact HF interaction. The diﬀerential orbital distortion eﬀect is small, but the core s-shell HF couplings are enormous, so that there is a substantial net HF coupling. For 3d-electrons the resulting Hf ﬁeld is ∼ −125kG/μB , increasing gradually across the 3d series. For the 4d and 5d shells the eﬀect is generally larger [47]. As an example, we note that the 5μB S-state moment of Mn2+ in MnF2 generates a HF ﬁeld −127kOe/μB at the 55 Mn nucleus. This compound has purely 3d-spin magnetism. 2.3.2 Orbital Shift and Susceptibility The orbital term in (2.2.1) comes into play for both the NMR shift and T1 . The orbital shift is driven by the Van Vleck orbital susceptibility, which was ﬁrst formulated for band electrons by Kubo and Obata [44]. The susceptibility was formulated in a tight-binding approximation, yielding the following expression for the α-axis susceptibility, dk f (Enk ) − f (En k )

nk|lα |n k n k|lα |nk , χorb = NA Ωμ2B (2π)3 En k − Enk nn (2.3.3)

2.3 Static and Dynamic Magnetism in d-band Metals

47

where NA is Avogadro’s number, Ω is the atomic volume, and the summing indices n and n represent the ﬁve d-orbital subbands as well as the spin quantum number. The quantity f (Enk = [exp(β(Enk − EF )) + 1]−1 is the Fermi occupation function. χorb is written here as a molar susceptibility. Clogston et al., [48] have derived a companion expression to (2.3.3), which gives the induced orbital hyperﬁne ﬁeld at the nucleus when the eﬀects of the spin-orbit coupling and certain other terms in the general expression, deemed to be small, are neglected. The simpliﬁed expression is dk f (Enk ) − f (En k ) 2

nk|2lα /r3 |n k n k|H lα |nk, Horb = ΩμB (2π)3 En k − Enk nn (2.3.4) where the ﬁeld H is taken to be directed along the α axis. If we make the assumption that the radial functions of all the d-orbitals in the band are approximately the same, then we may extract 1/r3 from the latter expression, ﬁnding (2.3.5) Korb = [2 1/r3 /NA ] χorb , where the quantity in brackets is identiﬁed as the orbital shift coeﬃcient αorb . When using calculated ionic values for 1/r3 [47], the foregoing authors suggest that a correction factor ξ = 1/r3 metal / 1/r3 ion 0.75 be invoked for realistic estimates of the metallic shift coeﬃcient αorb . Analysis of NMR Shift and Susceptibility for d-Band Metals: The (K, χ) plot With the foregoing additions to our list, we are now in a position to formulate a complete model of the shift and susceptibility of a d-band metal. The following model would apply to a pure metal from the 3d, 4d, or 5d transition series, but is also intended to represent a binary or ternary intermetallic compound a long as its Fermi surface can be modeled with two bands, an sp-band which belongs mostly to the transition metal atoms and a d-band which belongs exclusively to the transition metal atoms. The p–orbitals on the ligands are assumed to be strongly mixed into the d–band, while the s–orbitals are not, i.e. are presumably nearly ﬁlled [46]. We then write for the susceptibility, χtot = χdia + χs + χd (T ) + χorb ,

(2.3.6)

where χs and χd (T ) are the spin-paramagnetic terms, χorb is the d-electron orbital term given by (2.3.3), and χdia is the core diamagnetic term. Among these, χs is quite small, though its associated Knight shift may not be, so that any Landau diamagnetism is very small, indeed. Neither the latter nor χdia has any appreciable NMR shift eﬀect[48]. Molar susceptibilities are used throughout this volume18 18

From the standpoint of the microscopic physics of solids, we regard the susceptibilities per atom χat (or per formula unit χf u ) as fundamental, representing the

48

2 Introduction to NMR Studies of Metals and Superconductors

The NMR shift for the nucleus of a transition-metal ion, then, has three signiﬁcant terms [48], K(T ) = Ks + Kd (T ) + Korb = αs χs + αd χd (T ) + αorb χorb ,

(2.3.7)

in conventional notation for the shift coeﬃcients. Typically, the only temperature dependence originates in χd (T ). Therefore an experimental plot of K(T ) vs. χtot (T ) with T as the implicit variable should yield a straight line of slope αd . An experimental K vs. χ plot is just the beginning of a full (K, χ) analysis of the various terms in (2.3.6) and (2.3.7). Such an analysis for the case of Pt metal was presented in [48], with the plotted result shown here in Fig. 2.8. We give a brief account of the analytic procedure. First, any K − χ analysis must begin at the origin, and several parameters need to be estimated in order to proceed. We refer the reader to the original paper for full details. The ﬁrst step is to plot χdia −28 × 10−6 emu/mole

(3) (2)

1

(1) –40

0

40

120 160 200 χ (10–6 emu/mole)

–1

K(%) –2 –3

Range of experimental data:

Fig. 2.8. A K-χ plot is shown for 195 P t in Pt metal. Plotting of successive contributions to (K,χ) carries one from the origin to point 1 (χdia ), then from point 1 to point 2 (Ks , χs ), and ﬁnally from point 2 with an estimated slope αorb . The intersection at point 3 with the line through the experimental data completes the partition of the susceptibility. A detailed discussion of the analysis is given in the text. Reprinted ﬁgure from A. M. Clogston, V. Jaccarino, Y. Yafet: Phys. Rev. 134, A650 (1964). Copyright 1964 American Physical Society magnetic polarization which occupies one Wigner-Seitz (or unit) cell. Their companion molar susceptibilities are χM = NA χat and χM f u = NA χf u . If Ω is the atomic (or Ωc the unit cell) volume, then the dimensionless volume susceptibility fundamental to electromagnetic theory is χV = χat /Ω (χf u /Ωc ), and the gram susceptibility is χgm = χat /Ωρ, where ρ is the volume density. It is clear that the actual dimensions of χM are cm3 and of the α shift coeﬃcients are cm−3 , although these are usually cited as emu/mole and (emu/mole)−1 .

2.3 Static and Dynamic Magnetism in d-band Metals

49

at K = 0 (point 1), since there is no appreciable diamagnetic shift [48]. This value of χdia may be taken from the literature [49]. From point 1 we construct a line of slope αs to extend over the interval Δχ = χs . For this step, αs was obtained from HF structure parameters derived from optical data, yielding αs 2.12 × 103 (emu/mole)−1 . χs is estimated using a free-electron model, where the number ns,d of (s, d) electrons satisﬁes ns + nd = 10. With a parabolic model for the 5d-band a value of ns = 10 − nd = 0.2 was obtained, giving χs 4.8 × 10−6 (emu/mole). The s-band line in Fig. 2.8 then extends from point 1 to point 2. Next, we construct a line from point 2 with a slope equal to the estimated value of αorb = 2 1/r3 /NA . The ionic value of 1/r3 has been estimated to be 9.5a.u. from HF spectroscopic data, leading to the value αorb 264(emu/mole)−1, including a relativistic correction [48]. Drawing a line with slope αorb from point 2, the intersection of that line with the line through the data (point 3) then partitions the remaining susceptibility into orbital and d-spin contributions as shown. In the case of Pt metal, χtot is dominated by χd (T ), and χorb is a relatively small fraction ( 15%) of χtot . In cases where χorb is a signﬁcant fraction of the total, its temperature dependence may be a big enough eﬀect so that a simple (K, χ) plot is no longer reliable [48]. Nonetheless, the (K, χ) method has been widely used to analyze NMR shift data with experimental susceptibilities. For example, it was used to determine that substantial χorb terms were present in the V3 X’s and in V metal [45]. We reproduce in Table 2.3 the table of results from [45]. In this table, values of χorb from (K, χ) analyses are subtracted from experimental susceptibilities to estimate χd , which is given as χexpt - χorb . The latter values are then to be compared with d-spin susceptibilities estimated 2 from the speciﬁc heat coeﬃcient γ, where χsp.ht. = 3μ2B γ/π 2 kB . A simple theory gives electron-phonon enhancement of γ by a factor [1 + N (0)V]. V is the BCS electron-phonon interaction parameter. Since χd is not so enhanced Table 2.3. Table of susceptibility components and BCS parameters for V3 X compounds and V metal. The estimates for χorb were determined using (K, χ) plot analyses. The values of χd = χexpt - χorb so deduced are checked using density-of-states estimates from speciﬁc heat data as corrected for electron-phonon enhancement by means of BCS theory. See text for detailed explanation. All susceptibilities are in units of 10−4 emu/mole R ≡ χd (0) /χd (Tc )

χexpt

χorb

χsp.ht.

χexpt − N (0)V χorb (Sp.Ht.)

N (0)V (BCS)

V3 Ga

0 ≤ R ≤ 0.25

17.9

5.2–7.5

14.0

0.35

V3 Si

0 ≤ R ≤ 0.25

15.7

5.2–7.5

10.7

12.7– 10.4 10.5– 8.2 0.971

V

3.08

2.11

1.22

0.13– 0.39 0.09– 0.35

0.35 0.244

50

2 Introduction to NMR Studies of Metals and Superconductors

[50], one may estimate VN (0) χsp.ht. /χd − 1. In the last two columns of Table 2.3, values of N (0)V deduced in that way are compared with those derived from Tc using the BCS formula N (0)V = [ln(0.855 θD /Tc)]−1 . Considering the diﬃculty of estimating the relevant parameters, this analysis gives a nicely consistent picture in which it is established that (a) χd at T Tc is a small fraction of its normal-state value, and (b), values of χd consistent with electron-phonon enhancement of γ are obtained. Note that χs 0.3 (units of Table 2.3) has been ignored and is essentially negligible. 2.3.3 Spin-Lattice Relaxation Eﬀects for d-Band Electrons An open d-band brings added richness - and complications - to the T1 process as well, contributing a total of three additional terms to the T1 rate. These are the d-spin core polarization (CP), the d-spin dipolar, and the d-orbital terms. The d-orbital relaxation process was ﬁrst discussed by Obata [51]; we shall spell out the results of that calculation below. The general treatment of the CP relaxation process, on the other hand, is an enterprise of great complexity. Under a set of straightforward restrictions, Yafet and Jaccarino have presented a very clear discussion of this problem [52], which has been useful under a variety of circumstances. Here we discuss brieﬂy the approximations employed and give the results. The stated approximations are as follows: • • • • • • •

Spin-orbit coupling is disregarded. The unperturbed states (i.e. without HF terms) are taken to be HartreeFock solutions of the simpliﬁed Hamiltonian. Exchange intergrals responsible for the CP eﬀect are treated in ﬁrst order. Exchange eﬀects between conduction band orbitals are neglected. Conduction band states are self-consistent Bloch states, which are admixtures of s, p, and d orbitals. The conduction band d-states are treated in a tight-binding approximation. Finally, consideration is limited to the case of a cubic metal. As a result, the cross terms between sp and d-orbital matrix elements can be shown to vanish. The resulting expressions for the shift and relaxation rate are: K=

4π (γe )2 [ φ2s (0)(1 − Fd ) − |φcp (0)|2 Fd ]n(EF ) 3

(2.3.8)

and 1 = T1 T

4πkB

4π 3

γn γe 2

2

[ φ2s (0)(1 − Fd )2

+|φcp (0)|4 Fd2 ( 13 f 2 + 12 (1 − f )2 )]n(EF )2 ,

(2.3.9)

2.3 Static and Dynamic Magnetism in d-band Metals

51

where Fd is the fraction of d-character of all the states at the Fermi surface, and n(EF ) is the total density of states (of all “bands”) at the Fermi surface. Thus, even if there is appreciable s-d mixing in the Bloch functions the contributions to shift and relaxation will occur separately as shown. CP terms are only kept for the d-orbitals, even though they may occur in the calculation for the s and p orbitals. The reason for this is that the contact terms dominate the sp regions of the Fermi surface, and any CP terms are neglected for those states as small corrections. The parameter f gives the relative weight of Γ5 character for d-orbitals at the Fermi surface, while 1 − f gives the proportion of Γ3 character19 . It is seen that the sp-contact and d-CP portions of the formulas for K and 1/T1 T obey separate Korringa-like relations (see 2.2.8), where the Korringa relation for the CP terms has a reduction factor q(f ) = 13 f 2 + 12 (1 − f )2 , i.e.

2

4πkB γn2 2 Kcp q(f ), γe2 (2.3.10) where the second equality shows the modiﬁed Korringa relation. q(f ) is essentially a degeneracy factor, having a value 1/2 for the two Γ5 orbitals (f = 1), 1/3 for the three Γ3 orbitals (f = 0), and 1/5 when all ﬁve d-orbitals are equally weighted (f = 0.6). Thus the ﬁve d-orbitals contribute independently to 1/T1CP , very much like the ﬂuctuations of separate magnetically-active neighbors contribute to the T1 process of a ligand nucleus. The diﬃculty in utilizing (2.3.10 is that the parameter f for d-band metals is generally unknown. The orbital T1 process was ﬁrst discussed in detail by Obata [51], treating both orbital and dipolar relaxation rates in the same calculation. As with the CP calculation above, spin-orbit coupling is neglected, the d-orbitals are treated in a tight-binding approximation, and the system considered is a cubic metal. There are no cross terms between orbital and spin-scattering relaxation processes. It was noted in [52] that the dipolar process has interference with the contact and CP processes, but if the states at the Fermi surface can be separated into a d-band and an sp-band, then the interference terms vanish. For a cubic metal, both the orbital and dipolar relaxation rates are isotropic, but both depend on the symmetry parameter f , according to 1 4πkB 1 , [γn Horb ]2 nd (EF )2 p(f ), [d(f )], (2.3.11) = T1orb T T1dip T 4πkB = T1cp T 1

4π γn γe 2 |φcp (0)|2 3

nd (EF )2 q(f ) =

5 1 2 [ 3 f + 25 (1 − f )]. where Horb = 2μB 1/r3 , p(f ) = 23 f [2 − 53 f ], and d(f ) = 49 Comparison of the dependences of q(f ), p(f ) and d(f ) on f is shown in Fig. 2.9. The orbital relaxation rate (p(f )) is seen to vary from zero, when the Γ5 orbitals alone are occupied at the Fermi surface, to a maximum when all 19

In the present notation of d-functions in the cubic space group, Γ3 refers to the d functions dxy , dyz , and dzx , while Γ5 refers to dx2 −y 2 and d3z 2 −r2 .

52

2 Introduction to NMR Studies of Metals and Superconductors 0.5 0.45 q

0.4 q, p, and d

0.35 0.3 0.25 0.2

p

0.15 0.1

d

0.05 0 0

0.2

0.4

0.6

0.8

1

f

Fig. 2.9. The symmetry factors q(f ), p(f ), and d(f ) pertaining to CP, orbital, and dipolar relaxation rates discussed in the text [52], respectively, are plotted as a function of the fraction f of Γ5 character in the relevant d-band orbitals at the Fermi surface. The point f = 0.6 represents equal weight of all ﬁve d-orbitals and is the maximum and minimum point of p(f ) and q(f ), respectively. In many cases the dipolar rate is negligible, as it is only ∼ 9% of the average value of the closely related orbital rate. Reprinted ﬁgure from Y. Yafet, V. Jaccarino: Phys. Rev. 133, A1630 (1964). Copyright 1964 American Physical Society

ﬁve orbitals are equally occupied, since the orbital matrix elements between the two symmetries are the largest ones. The dipolar relaxation rate (d(f )) varies only slightly across the full range of f , but it is only about 10% of the average value of p(f ). Thus, the dipolar relaxation is only signiﬁcant when p(f ) is near zero. The complete list of magnetic relaxation processes for d-band metals is then (2.3.12) 1/T1 = 1/T1s + 1/T1cp + 1/T1orb + 1/T1dip . We illustrate the analysis of experimental T1 rates into these diﬀerent contributions with calculations given in [52] for d-band metals V and Nb. In stating these results we deﬁne Hs = (8/3)πμB φ2s (0) and Hcp = (8/3)πμB |φcp (0)|2 , whereupon (2.3.9) becomes 1 4πkB = [γn Hs,cp ]2 n2s,d [1, q(f )] T1s,cp T

(2.3.13)

for the s-band and CP contributions. The parameters Hs,cp are the HF ﬁelds per unit of spin from these sources. The T1 contributions from the three main sources have been estimated [52] for V and N b metals as listed in Table 2.4. For this purpose, Hs has been estimated using data from the literature [52], and Hcp and Horb have been derived from Hartree-Fock calculations given by Freeman and Watson [53]. The total densities of states for these elements are taken from speciﬁc heat measurements, where the s-band components are

2.3 Static and Dynamic Magnetism in d-band Metals

53

Table 2.4. Table of HF parameters and speciﬁc heat densities of states leading to estimates of (T1 T )−1 for elemental V and N b using the formulas given in the text. The total relaxation rates are stated for f = 0.6, but would not change signiﬁcantly for other values of f . The theoretical estimate undoubtedly exceeds the experimental numbers because of the electron-phonon enhancement of the speciﬁc heat density of states, which does not aﬀect nuclear relaxation rates. See text for data sources and additional discussion. HF ﬁelds are given in units of 106 Oe, densities of states in states/eV-atom, and relaxation rates in (sK)−1 Hs

Hcp

Horb ns (EF ) nd (EF ) Rs

V 1.12 -0.117 0.19 0.12 Nb 2.48 -0.21 0.285 0.14

1.84 1.66

Rcp R1orb (T1calc kT )−1 (T1exp T )−1

0.642 1.65 4.35 3.76 3.74 6.9

2.86 7.55

1.27 2.8

estimated assuming for simplicity one s-electron per atom. The quantities Rs , Rcp , Rorb are deﬁned to be the expressions given above for 1/T1 T from these sources without the symmetry factors [1, q(f ), p(f )]. The experimental values of (T1exp T )−1 are data reported by Butterworth [54]. This table illustrates the importance of the CP and orbital relaxation mechanisms in d-band metals. For the lighter metals, where the s-band contribution is smaller, these d-electron terms may even be the dominant ones. On the other hand, we see that the speciﬁc heat density of states clearly overestimates the relaxation rates, pointing to a substantial electron-phonon enhancement eﬀect for V and Nb metals (which are also superconductors). In [5] a quantitative discussion of the latter eﬀect is given, ﬁnding reasonable agreement between the nuclear relaxation data and estimates from other measurements, somewhat like the comparisons in Table 2.3. As the details go beyond the intended scope of this discussion, the reader is referred to [5] and references therein for details. This completes our discussion of normal-state NMR shift and relaxation eﬀects in transition metals. The mechanisms in (2.3.2) and (2.3.12) are the foundation of eﬀects to be found in high-Tc materials, though the details remain to be worked out. We next consider the eﬀects of Type II superconductivity in the d-band metals. 2.3.4 NMR Studies of 3d Metals as Type-II Superconductors The type-II superconductivity of d-band metals and intermetallic compounds presents a rather diﬀerent set of problems from those of the type-I systems discussed in Sect. 1.2.2. First, type-II systems exhibit great complexity of behavior in a magnetic ﬁeld, showing three phases as a function of the magnitude of the applied ﬁeld for T < Tc and exhibiting two critical ﬁelds, Hc1 and Hc2 . Below Hc1 there is the typical Meissner exclusion of all magnetic ﬂux except for the usual penetration depth λ. Between Hc1 and Hc2 there is a state of essentially complete, but inhomogeneous ﬁeld penetration in the form of superconducting current vortices

54

2 Introduction to NMR Studies of Metals and Superconductors

which allow a single ﬂuxon of ﬁeld to exist in a region of normal (i.e. nonsuperconducting) metal with a diameter ∼ ξ0 , the Pippard coherence length. Of course, the magnetic ﬁeld of a ﬂuxon penetrates the surrounding material to a depth of ∼ λ. Each ﬂuxon comprises one ﬂux quantum Φ0 = hc/2e = 2.07 × 10−7 G cm2 . Because of the accommodation of type-II superconductivity to applied ﬁelds through the penetration of vortices, the superconducting state can persist up to ﬁelds much higher than the thermodynamic critical ﬁeld Hc . One can make a rough estimate of Hc2 using a picture of vortices with normal cores of approximate radius ξ0 . In the mixed state with ﬁeld H (T Tc ) the density of vortices is H/Φ0 . The fraction of normal sample material is then ∼ πξ02 H/Φ0 . Setting this expression equal to 1 gives an estimate Hc2 ∼ Φ0 /πξ02 . This is only slightly larger than the expression deduced from Ginzburg-Landau (GL) theory, Φ0 . (2.3.14) Hc2 = 2πξ02 As was ﬁrst demonstrated by Abrikosov√[55], the normal-superconducting boundary wall has positive energy for λ < 2ξ. On the other hand, if the GL √ parameter κ = λ/ξ > 2, then the boundary wall has negative energy, so that the system will lower its free energy by making the boundary area as large a possible. Thus, the ﬁeld arranges iself into individual ﬂuxons, each surrounded by a normal-superconducting wall. Abrikosov predicted the existence of such a mixed state, in which the vortices arrange themselves (in reasonably clean material) into an ordered lattice [55]. The lowest energy state of such a lattice was shown to be minimized by a triangular arrangement of vortices by Kleiner et al., [56]. Below, we describe NMR spectra which are consistent with this theoretical conclusion. It is interesting to look at simple expressions for ξ and λ to see why there is a general tendency for d-electron superconductors to exhibit type-II superconductivity. The expressions m c2 vF , (2.3.15) and ξ0 = a λ0 = 2 4πns e kB Tc where a is a constant of order unity, come from the London equations and from Pippard’s uncertainty principle argument, respectively. Since d-bands tend to have large eﬀective masses and high-Tc materials in particular have low carrier densities ns , we expect λ0 values to be larger than for sp-band superconductors. Furthermore, small values of EF (and thus of vF ) as well as higher √ values of Tc will make for short ξ0 ’s. Thus, it is generally expected that λ > 2ξ0 . As an example, we mention V3 Si, a superconductor at ∼ 17K which we shall discuss further below. Here, we only note that Greytak and A and a related estimate of Wernick [57] reported a measurement of λ0 = 1500˚ ξ0 = 25˚ A. Thus, κ 60 and from (2.3.14) we estimate Hc2 530 kG. A second estimate can be made from the thermodynamic critical ﬁeld Hc = 6370 G [58]

2.3 Static and Dynamic Magnetism in d-band Metals

55

and the measured value of λ0 using (4–62) from [6], Hc2 = 4πλ20 /Φ0 . This yields Hc2 = 550kG, which is in surprisingly good accord with the previous number. In any case, V3 Si is a very “hard” superconductor, indeed. Internal Field Distributions in the Mixed State from NMR Studies NMR studies of type-II superconductors are typically done in the mixed state, i.e. for Hc1 < H < Hc2 . There is substantial NMR line broadening from spatially-dependent shielding supercurrents in the mixed state. We shall ﬁrst review studies conducted to map the distribution of such currents, after which we will look at shift and relaxation studies. A number of internal ﬁeld studies have been reported for V and Nb metals [59, 60, 61]. We review brieﬂy the results given by Redﬁeld [60], who conducted the following ﬁeld-switching NMR experiment on 51 V in V metal. The sample was polarized in 10 kG, after which the ﬁeld was switched to a value below Hc2 ∼ 3, 000 G for a time of 0.1s, during which an rf ﬁeld was applied transverse to the steady ﬁeld. The ﬁeld was then switched back to 10 kG where the nuclear polarization was recorded. By scanning the frequency of the rf, the spectrum of internal ﬁelds could be mapped out. Results from this study are shown in Fig. 2.10a for two ﬁeld values. These data have been ﬁtted to calculated internal ﬁeld distributions based on the GL equations in the Abrikosov limit, assuming both square and triangular lattices [60]. The raw calculated distributions are shown in Fig. 2.10b. Fits are carried out by convoluting the latter distributions with a Gaussian of adjustable width, then adjusting the width and total area for best ﬁt. The triangular lattice unit cell is shown as an inset to Fig. 2.10b, where the points V, C, and S are seen to correspond to the maximum ﬁeld, minimum ﬁeld, and the singularity in the distribution, respectively. The singularity appears much closer to C for triangular lattice than for the square lattice. Results for the lower ﬁeld value ( 0.73Hc2 ) are seen to be in good accord with the triangular lattice. The higher ﬁeld value is rather closer to Hc2 , where a kind of gapless superconducting state sets in and there are many corrections to the simple ﬁeld-distribution calculation. Thus, it is not surprising that the simple triangular lattice calculation is no longer accurate [60]. Studies of eﬀects near Hc2 are reviewed in [5]. We shall, however, restrict our attention here to the region Hc1 H Hc2 . It is interesting to compare the ﬁeld distribution results from [60] with theoretical predictions. For example, the results from Kleiner, et al., [56] predict that HV − HS = 1.35 (H − B). From [60] we ﬁnd for the conditions of Fig. 2.10 the experimental value HV − HS = 285 G, while 1.35 (H − B) under the same conditions 165 G, a considerable underestimate. On the other hand, 1.35 (H − B) according to the Abrikosov solution [5, 55] equals 1.35 (Hc2 − H)/βa (2κ2 − 1), which we ﬁnd to be 520 G, which is a considerable overestimate. For this purpose we take βa = 1.16 for the triangular

56

2 Introduction to NMR Studies of Metals and Superconductors

(a)

RELATIVE ABSORPTION

(a) B = 0.73 HC2

LOCAL FIELD

(b) B = 0.88 HC2

LOCAL FIELD

RELATIVE ABSORPTION

TRIANGULAR LATTICE UNIT CELL

(b)

SQUARE LATTICE

V S V

C S

S V

S B

B

C

V FREQUENCY OR LOCAL FIELD H

Fig. 2.10. (a) Distributions of diamagnetic shielding ﬁelds measured using rf saturation of the 51 V NMR in superconducting V metal, and (b) simulations of internal ﬁeld distributions under similar circumstances for both square and triangular vortex lattices. In (a) results are given for T 1.4 K and for ﬁelds of 0.73 Hc2 and 0.88 Hc2 as shown, where Hc2 = 2720 G. For (b) the ﬁeld simulations were done on the basis of solutions of the Ginzburg-Landau equations in the Abrikosov limit. The inset shows the triangular lattice unit cell, with points there and on the distribution labelled V, S, and C corresponding to a vortex (V), a saddle point (S) showing a divergence, and the minimum ﬁeld (C). Reprinted ﬁgure from A. G. Redﬁeld: Phys. Rev. 162, 367 (1967). Copyright 1967 American Physical Society

lattice from [56] and employ (2.3.14) to obtain ξ0 = [Φ0 /2πHc2 ]1/2 = 348˚ A. The estimate λ = 400˚ A [62] then leads to κ = 1.15. Substantial corrections to these simple theoretical results have been given by Eilenberger [63].

2.3 Static and Dynamic Magnetism in d-band Metals

57

The NMR Shift in Type-II Superconductors In the foregoing study of elemental vanadium, the precision with which the vortex lattice could be characterized was not great enough to resolve changes in the d-spin shift Kd (T ) below Tc [60]. However, in a truly hard type-II system where κ 1, it is possible to resolve small shift changes at ﬁeld values such that Hc1 H Hc2 . The reason for this is that the NMR lineshape is then strongly dominated by the singularity from the saddle regions S (Fig. 2.10b), which is therefore shifted only slightly away from the applied ﬁeld. Moreover, the NMR linewidth from diamagnetic shielding is typically only modestly greater than one might ﬁnd in the normal state. We illustrate these points with data and discussion of the closely related cases of V3 Si and V3 Ga, where V3 Si was touted earlier as a truly hard superconductor. Interestingly, somewhat before the nature of the the type-II diamagnetic shielding was investigated in detail in the 1960’s, The NMR shifts in these compounds of both 51 V and 71 Ga were reported by Clogston et al., [45]. We reproduce their (K, χ) plot in Fig. 2.11. The interesting point here is that all NMR shift values here are consistent with the interpretation that, at T = 1.8 K, the corresponding d-band susceptibility is diminished to ∼ 25% of its value at 20 K. Further, its low temperature value is smaller than that at room temperature. Since these NMR shifts were measured in the mixed state at a ﬁeld of 14 kOe, where they found “negligible diamagnetic rf susceptibility” [45], one can only conclude that spurious frequency shift eﬀects from the diamagnetic shielding are negligibly small in comparison. Note that the total range of 51 V shift values in Fig. 2.10 is only ∼ 0.1%. It is interesting to consider the nature of the internal ﬁeld distribution in A and 1500˚ A, respecV3 Si given the values of its parameters ξ0 and λ0 (25˚ tively) stated above. First, the second moment of this distribution has been calculated by Pincus et al., [58], yielding the expression

ΔH 2 1/2 av

Φ0 4π 3/2 λ2

(2.3.16)

under conditions where not only Hc1 H Hc2 holds, but also λ/d 1, where d is the separation of vortices in the√mixed state. At H = 14 kOe (i.e. A for the triangular for the data of Fig. 2.11), we ﬁnd d = [2Φ0 / 3H]1/2 = 413˚ 1/2 lattice, giving λ/d = 3.6. For these conditions (2.3.16) gives ΔH 2 av = 41 Oe for a square lattice. This may be a slight overestimate, but is of the right order, since the measured peak-to-peak derivative linewidth is 39 ± 5 Oe [58]. It is interesting to note in this case, where κ 1, the Abrikosov relation [5, 55] yields HV − HS = 86 G, barely twice the second moment estimate. We therefore ﬁnd for the hard type-II superconductors that it is quite feasible to measure shift values with weak temperature dependences in the mixed state of superconductivity. This is a very important result for high-Tc NMR studies.

58

2 Introduction to NMR Studies of Metals and Superconductors

2.3.5 T1 Phenomenology for Type-II Superconductors In this ﬁnal subsection of Chap. 2 we review T1 behavior at T < Tc for typeII d-band superconductors. Because of the complications which attend the measurement and interpretation of T1 in the mixed state of these systems, our discussion of this topic will be limited to a few simple cases. A clear and thorough discussion of these eﬀects, in terms of both theory and experiment, is given in [5]. The hallmarks of type-I system T1 behavior are the coherence peak (in T1−1 ) just below Tc and the exponential decay T1−1 ∝ exp(−Δ0 /kB T )

1.0 V51

0.8

1.8° B

295°

0.6

KNIGHT SHIFT IN PERCENT

1.8°

295° V3Si

0.4

V3Ga x x

20° 20°

0.2 0 1.8°

–0.2

295° –0.4

V3Ga

Ga71 –0.6

–0.8 1.0

20°

0

2

4

6

8

10

12

SUSCEPTIBILITY (EMU/MOLE)

14

16 18 ×10–4

Fig. 2.11. Measured Knight shifts are plotted vs. molar susceptibilities for 51 V in both V3 Si and V3 Ga and for 71 Ga in V3 Ga [45]. For the 51 V shifts a (K, χ) construction is shown, including the s-band contribution (point A) and the orbital contribution (points A-B), which intersects with lines through the data points. For the 71 Ga the results clearly show a transferred shift which is driven by the temperaturedependent d-band susceptibility. In both cases the location of the shift values measured at 1.8 K are shown, indicating that the negative CP shift is diminished to ∼ 75% of its value at 20 K, and that the values of |Kd (T )| in both cases are smaller than the values found at room temperature. Reprinted ﬁgure from A. M. Clogston, A. C. Gossard, V. Jaccarino, Y. Yafet: Phys. Rev. Lett. 9, 262 (1962). Copyright 1962 American Physical Society

2.3 Static and Dynamic Magnetism in d-band Metals

59

for T Tc . For type-II systems these behaviors carry over in a modiﬁed way or not at all. The diﬀerences found between type-I and type-II behavior appear to be caused by the ﬁeld penetration in the mixed state and the consequent spatial inhomogeneities. The Coherence Peak Region, T ≤ Tc (H) Caroli et al., have shown that in the vicinity of a vortex core the excited state energies are diminished to ΔE ∼ Δ20 /EF Δ0 [64]. Thus, for points near the (H, T ) phase boundary, i.e. for H near Hc2 (T ), there is a gapless region which has received a detailed theoretical examination [65, 66, 67]. The ﬂuctuation (i.e. T1 ) properties in this region are diﬀerent from a type-I system and appear to depend on whether the carriers have a long mean-free path l ξ0 (“clean”) or whether it is short l < ξ0 (“dirty”). In the simpler dirty limit case the electronic properties are local in character, and Cyrot [68] has derived the relation ec T1n =1+ (Hc2 − H) g(t), T1s σkB Tc

(2.3.17)

where t = T /Tc , σ is the normal state conductivity and Hc2 = Hc2 (T ). This relation is only valid for (Hc2 − H) Hc2 , so that it only gives the slope −1 T1n d(T1s )/dH near Hc2 . The function g(t) > 0 for t > 0.6, while g(t) < 0 below that point. One must be very careful in using (2.3.17) to interpret actual data, since T1 is usually measured by scanning temperature rather than ﬁeld. Masuda and Okubo have obtained T1 data on 51 V in V3 Sn, a superconductor with Tc 3.6 K (their sample) and Hc2 (0) = 16 kG [69, 70]. Their data are shown for three values of applied ﬁeld in Fig. 2.12. These authors used (2.3.17) to show that d(T1n /T1s )/dT ∝ g(t) (T ≤ Tc (H)),

(2.3.18)

as well, and have evaluated the constant of proportionality. We note that for H = (4470, 8940, 13410) G, Tc (H) = (3.2, 2.6, 1.8) K and thus t(Hc2 ) = (0.89, 0.72, 0.50) for the three data curves in Fig. 2.12. Thus, the slopes of the data plots at T ≤ Tc are nicely consistent with these parameters, since d(T1n /T1s )/dT is positive for the ﬁrst two, then turns negative for the third, where t(Hc2 ) falls below 0.6. It seems, then, that measurements at low (or zero) ﬁeld on V3 Sn yield a conventional BCS coherence peak, but that it is gradually quenched out by ﬂuxoids at higher ﬁeld values. We mention three other cases of type-II T1 studies at T ≤ Tc . Each is somewhat anomalous in its own way. The ﬁrst is the case of elemental V metal [71], where no convincing coherence peak was observed. The authors considered a number of possible explanations, ﬁnally suggesting that the T1 peak may be suppressed by trapped ﬂux. However, sometime after these results were published, a theory of T1 in the clean limit emerged [65], and this interpretation was applied to the case of vanadium by Pesch [67]. The result

60

2 Introduction to NMR Studies of Metals and Superconductors

was a good ﬁt to the data for both samples [71], with no sign of a coherence peak. It seems, then, that coherence peaks will appear at low ﬁelds in the dirty limit, but not in clean samples. No coherence peaks were observed in any of the V3 X compounds, where X = Ga, Si, Ge, and Pt, in the study conducted by Silbernagel et al., [72, 73]. The ostensible reason for this is disorder caused by the “Martensitic” structural transformation which was reported at temperatures just above Tc in these compounds [74, 75]. The authors oﬀer no further discussion of the point [73]. The third and most anomalous case to be reported was that of niobium [76]. The relaxation of 93 N b nuclear spins was studied in the SC state at ﬁeld values varying from 2.40 kG up to 6.80 kG corresponding to Tc values which vary from 6.8 K down to 3.0 K. Using (2.3.14), Hc2 corresponds to A, so that the given mean-free path l 140˚ A is on the borderline ξ0 ∼ 200˚ between the clean and dirty cases. In any case, the T1 data were found to ﬁt the gapless theory [66, 67] for the higher ﬁeld values. For the lower two ﬁeld values, however, the T1 data were found to execute a deep minimum just below Tc (H), contrary to the gapless theoretical ﬁts. Such behavior is clearly reminiscent of the V3 Sn data in Fig. 2.12, and one might inquire as to whether the calculation of d(T1n /T1s )/dT given in [70] based on (2.3.17) could be applied in this case. The authors did such a calculation and found that the coeﬃcient of g(t) for Nb is smaller by a factor 150–200, so that 2000 GAP = 3.5 kTc(O)

1000

T1

2.6 °K 3.2 °K 3.6 °K

T1T = 0.42 sec °K

msec

15 MHz 1.8 °K

100

50 0.5

1

2 Tc(O)/T

(13410G)

10 MHz

(8940G)

5 MHz

(4470G)

3

Fig. 2.12. A semilog plot of data for T1 of 51 V in V3 Sn vs. Tc (0)/T in the superconducting state for three values of applied ﬁeld [69]. The data shown exhibit coherence peaks for 1341 G and 8940 G, but not for 13410 G. All three plots show deviations from the exponential BCS behavior at the lowest temperatures, an eﬀect attributable to spin diﬀusion to the normal cores. See text for discussion. Reprinted ﬁgure from N. Okuda, Y. Masuda: Phys. Rev. Lett. 20, 1475 (1968). Copyright 1968 American Physical Society

2.3 Static and Dynamic Magnetism in d-band Metals

61

similar behavior cannot be expected on that basis. There seems to be no straightforward explanation for this anomalous result. Type-II T1 Behavior for T Tc −1 For values of T well below Tc , an exponential decay T1s ∝ exp(−Δ0 /kB T ) has generally been found to appear. However, as this intrinsic BCS rate weakens, another contribution attributable to the ﬂuxoids is often seen. Since the energy gap near the ﬂuxoids is very small [64], T1s for a region of area ∼ ξ02 is essentially that of the normal state. When the BCS T1 process in the bulk of the SC material becomes very slow, then a process whereby the nuclear polarization diﬀuses to the normal cores becomes predominant. This process was found to be present in three of the four examples given above [69, 71, 72] but was studied most systematically in the case of V3 Si [72]. 51 V T1s data for V3 Si [72] are plotted semilogarithmically in Fig. 2.13 as a function of Tc /T , where Tc = 15.35 K. Results are given for four

1000

BCS

T1 (BCS Theory) Experimental Data H0 = 4.45 kG

100 T1 seconds 10

H0 = 8.95 kG H0 = 13.4 kG H0 = 17.8 kG

Values of T1 Extrapolated to H0 = 0

1.0

N

T1 (Korringa Theory) 51

V3 Si T1 vs T1 / T T = 4.2 °K – 1.4 °K Tc = 15.35 °K

0.1

0.01

2

4

6

8

10

12

14

Tc / T

Fig. 2.13. A semilog plot of data for T1 of 51 V in V3 Si vs. Tc /T in the superconducting state for four values of applied ﬁeld as shown [72]. The data shown exhibit no coherence peaks, but follow exponential BCS-theory behavior up to Tc /T ∼ 4. Beyond that point the mechanism of spin diﬀusion to the normal ﬂuxoid cores takes over, giving a relaxation rate which is proportional to the applied ﬁeld (i.e., to the ﬂuxoid density), as expected. See text for further discussion. Reprinted ﬁgure from B. G. Silbernagel, M. Weger, J. H. Wernick: Phys. Rev. Lett. 17, 384, (1966). Copyright 1966 American Physical Society

62

2 Introduction to NMR Studies of Metals and Superconductors

diﬀerent ﬁeld values at temperatures in the SC state which extend down below Tc /10. At higher temperatures the data points asymptotically approach the dashed line which represents BCS behavior, i.e. T1s ∝ exp Δ0 /kB T , where Δ0 = 1.76 kB Tc . T1s veers away from the BCS curve at Tc /T ≥ 4, then ranges up to values more than three orders of magnitude longer than its value at Tc . The ﬂattening of these curves is suggested to be caused by spin diﬀusion to the normal cores, which then becomes the only eﬀective T1 mechanism at the lowest temperatures. If the spin diﬀusion time, estimated below, is not an impediment, then at the lowest temperature we should have pξ 2 H T1n = 0 . T1s Φ0

(2.3.19)

where p is a numerical factor of order unity. Equation (2.3.19) simply states that the normal T1 should be diluted by the ratio of pξ02 to the area per ﬂuxoid Φ0 /H. First, we note that 1/T1s should be linear in H, as is clearly the case in A for V3 Si given above, we ﬁnd p = 1.9, Fig. 2.13. With the estimate ξ0 25˚ so that the eﬀective area of normal-state relaxation is a circle of radius slightly smaller than ξ0 for each ﬂuxoid. The corresponding spin diﬀusion times for the results in Fig. 2.13 can be estimated with tdiﬀ ∼

d2 , 4Dsp

(2.3.20)

where d is the distance between ﬂuxoids and Dsp is the spin diﬀusion constant. √ Taking d = [2Φ0 / 3H]1/2 and Dsp ∼ 10−12 cm2 s [77], we ﬁnd tdiﬀ ∼ 13s at H = 4450 G. This is an order of magnitude less than T1 itself, lending credence to the use of (2.3.19). While the foregoing scenario gives an appealingly straightforward interpretation of the V3 Si data for T1s , there did arise in the literature a rather knotty problem in connection with this interpretation. Genack and Redﬁeld suggested some time later [78] that the spin diﬀusion relaxation mechanism in type-II superconductors would not work, because it did not conserve energy. We give the essence of their argument here, then cite further work which provided something of an antidote to this objection. If spin diﬀusion takes place along a ﬁeld gradient, then the simple ﬂip–ﬂop events between neighboring nuclei no longer conserve energy. The diﬀerence in Zeeman (ﬁeld) energies has to be taken up by the spin-spin (usually dipolar) interactions. Viewing this process thermodynamically, the dipolar reservoir then quickly becomes overheated and must, itself, relax to the lattice. The total relaxation process by spin diﬀusion is thus formulated as a dual process, with Zeeman (magnetization) and dipolar energies both diﬀusing to the normal cores in the mixed superconducting state. These processes were analyzed in [78] and found to be too slow to provide the observed T1 processes in V metal [71]. It was concluded that these clearly observed diﬀusion-like T1 processes must originate in some other way [78].

References

63

The problem is, of course, that no other ideas to explain type-II relaxation have been forthcoming. However, more recently, this problem has been revisited in terms of basically the same ideas, but using more sophisticated mathematical methods (see [79] and references cited therein). These authors have analyzed in detail the relaxation curves of 51 V in V metal at T Tc taken from [71] in terms of spatially varying Zeeman and dipolar spin temperatures. They ﬁnd a good ﬁt to the vanadium data, where the dipolar relaxation time constants are relatively short, thus not obstructing the longer diﬀusion-mediated Zeeman T1 ’s. It seems, then, that the phenomenology of (2.3.19) is basically correct, so that low-temperature type-II T1 behavior is clearly understood. This is very important for the interpretation of T1 data for high-Tc systems as well. However, as we shall see, the fundamental behavior of T1 in high-Tc compounds involves SC gap symmetries which usually have line nodes, giving power-law behavior at low temperatures [80]. Thus, the issues regarding T1 data analysis diﬀer somewhat from those of d-band SC metals discussed here. Nonetheless, the spin-diﬀusion-to-normal-cores T1 mechanism in the mixed state has been found to play a signiﬁcant role in the phenomenology of cuprate superconducting T1 eﬀects. The understanding of this eﬀect gained with ordinary 3d metals will be an important resource in the chapters to follow.

References 1. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 13, 14, 15, 19, 22, 33 2. C.P. Slichter, Principles of Magnetic Resonance, 3rd edn. (Springer-Verlag, New York, 1992) 13, 14, 15, 21, 25, 34 3. A. Narath, Hyperﬁne Interactions, ed. by A.J. Freeman and R.B. Frankel (Academic Press, New York, 1967), p.287 13, 35, 36, 37 4. J. Winter, Magnetic Resonance in Metals, (Clarendon Press, Oxford, 1971) 13 5. D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 13, 38, 40, 41, 42, 43, 53, 55, 57, 58 6. M. Tinkham, Introduction to Superconductivity, (McGraw-Hill, New York, 1975) 13, 41, 55 7. J.R. Schrieﬀer, Theory of Superconductivity, (Westview Press, Boulder, 1999) 13, 41 8. R.E. Walstedt, “The two-pulse spin echo revisited”, in Pulsed Magnetic Resonance: NMR, ESR and Optics, ed. by D. M.S. Bagguley (Clarendon Press, Oxford, 1992), p. 242 18 9. E.L. Hahn, Phys. Rev. 80, 580 (1950) 18 10. N. Bloembergen, T.J. Rowland, Phys. Rev. 97, 1679 (1955) 19 11. M.A. Ruderman, C. Kittel, Phys. Rev. 96, 99 (1954); T. Kasuya, Prog. Theoret. Phys. 16; K. Yosida, Phys. Rev. 106, 893 (1957) 19 12. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 19 13. R.E. Walstedt, Phys. Rev. Lett. 19, 146 (1967); 19, 816 (1967) 21

64 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54.

2 Introduction to NMR Studies of Metals and Superconductors J. Van Kranendonk, Physica 20, 781 (1954) 23 J. Bardeen, L.N. Cooper, J.R. Schrieﬀer, Phys. Rev. 108, 1175 (1957) 32, 38 L.C. Hebel, C.P. Slichter, Phys. Rev. 113, 1504 (1957) 32, 40, 41, 42 W.D. Knight, Phys. Rev. 76, 1259 (1949); C.H. Townes, C. Herring, W.D. Knight, Phys. Rev. 77, 852 (1950) 33 J. Korringa, Physica 16, 601 (1950) 33, 34 D.L. Randles, Proc. Roy. Soc. London, Ser. A331, 85 (1972) 34 R.E. Walstedt, Y. Yafet, A.I.P. Conference Proceedings 24, 522 (1974) 34 D. Pines, in Solid State Physics, vol. I, ed. by F. Seitz, D. Turnbull (Academic Press, New York, 1954), p. 1 36, 37, 44 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 36, 44 K. Yosida, Phys. Rev. 110, 769 (1958) 38, 40 F. Reif, Phys. Rev. 102, 1417 (1956); 106, 208 (1957) 39 G.M. Androes, W.D. Knight, Phys. Rev. 121, 779 (1961) 39 W.A. Hines, W.D. Knight, Phys. Rev. Lett. 18, 341 (1967); Phys. Rev. B4, 893 (1971) 39 R.H. Hammond, G.M. Kelly, Rev. Mod. Phys. 36, 185 (1964) 39, 40 See Ref.5 for a more detailed account of these developments 39 R.A. Ferrell, Phys. Rev. Lett. 3, 262 (1959) 39, 40 P.W. Anderson, Phys. Ref. Lett. 3, 325 (1959) 39 A.A. Abrikosov, L.P. Gorkov, Zh. Eksp. Teor. Fiz. 42, 1088 (1962); [Sov. Phys.–JETP 15, 752 (1962)] 39 P.W. Anderson, J. Phys. Chem. Solids 11, 26 (1959) 39, 43 F. Wright, W.A. Hines, W.D. Knight, Phys. Rev. Lett. 18, 115 (1967) 39 R.H. Hammond, G.M. Kelly, Phys. Rev. Lett. 18, 156 (1967) 40 H.L. Fine, M. Lipsicas, M. Strongin, Phys. Lett. 29A, 366 (1969) 40 Y. Masuda, A.C. Redﬁeld, Phys. Rev. 125, 159 (1962) 41, 42, 43 H. B ommel, Phys. Rev. 96, 220 (1954) 41 C.R. Leavens, J.P. Carbotte, Solid State Commun. 9, 75 (1971); Ann. Phys. (N.Y.) 70, 338 (1972) 43 Y. Masuda, Phys. Rev. 126, 1271 (1962) 43 J.D. Williamson, D.A. MacLaughlin, Phys. Rev. B8, 125 (1973) 43 J.R. Clem, Phys. Rev. 148, 392 (1966) 43 V. Heine, Phys. Rev. 107, 1002 (1957) 44, 46 J.H. Wood, G.W. Pratt Jr., Phys. Rev. 107, 995 (1957) 44, 46 R. Kubo, Y. Obata, J. Phys. Soc. Japan 11, 547 (1956) 44, 46 A.M. Clogston, A.C. Gossard, V. Jaccarino, Y. Yafet, Phys. Rev. Lett. 9, 262 (1962) 44, 49, 57, 58 A.M. Clogston, V. Jaccarino, Phys. Rev. 121, 1357 (1961) 45, 47 R.E. Watson, A.J. Freeman, Hyperﬁne Interactions, ed. by A. J. Freeman, R.B. Frankel (Academic Press, New York, 1967), p. 53 46, 47 A.M. Clogston, V. Jaccarino, Y. Yafet, Phys. Rev. 134, A650 (1964) 47, 48, 49 F.E. Hoare, J.C. Matthews, Proc. Roy. Soc. (London) A212,137 (1952); D.W. Budworth et al., ibid. A257, 250 (1960) 49 L.P. Kadanoﬀ, Phys. Rev. 132, 2073 (1963) 50 Y. Obata, J. Phys. Soc. Japan 18,1020 (1963) 50, 51 Y. Yafet, V. Jaccarino, Phys. Rev. 133, A1630 (1964) 50, 51, 52 R.E. Watson, A.J. Freeman: Phys. Rev. 123, 2027 (1961) 52 J. Butterworth, Phys. Rev. Lett. 5, 305 (1960); J. Butterworth, Proc. Phy. Soc. London 85, 735 (1965) 53

References

65

55. A.A. Abrikosov, Zh. Eksperim. i Teor. Fiz. 32,1442 (1957) [English transl.: Soviet Phys.- JETP 5, 1174 (1957) 54, 55, 57 56. W.H. Kleiner, L.M. Roth, S.H. Autler, Phys. Rev. 133, A1226 (1964) 54, 55, 56 57. T.J. Greytak, J.H. Wernick, J. Phys. Chem. Solids 25, 535 (1964) 54 58. P. Pincus, A.C. Gossard, V. Jaccarino, J.H. Wernick, Phys. Lett. 13, 21 (1964) 54, 57 59. J.-M. Delrieu, J.-M. Winter, Solid State Commun. 4, 545 (1966) 55 60. A.G. Redﬁeld, Phys. Rev. 162, 367 (1967) 55, 57 61. D. Rossier, D.E. MacLaughlin, Phys. Kondens. Mater. 11, 66 (1970) 55 62. P.R. Radebaugh, P. Keesom, Phys. Rev. 149, 209 (1966); 149, 217 (1966) 56 63. G. Eilenberger, Phys. Rev. 153 584 (1967) 56 64. C. Caroli, P.G. deGennes, J. Matricon, Phys. Lett. 9, 307 (1964) 59, 61 65. U. Brandt, W. Pesch, L. Tewordt, Z. Physik 201, 209 (1967) 59 66. U. Brandt, Phys. Letters 27A, 645 (1968) 59, 60 67. W. Pesch, Phys. Letters 28A, 71 (1968) 59, 60 68. M. Cyrot, J. Phys. (Paris) 27, 283 (1966) 59 69. N. Okuda, Y. Masuda, Phys. Rev. Lett. 20, 1475 (1968) 59, 60, 61 70. Y. Masuda, N. Okuda, J. Phys. Soc. Japan 26, 309 (1969) 59, 60 71. W. Fite, A.G. Redﬁeld, Phys. Rev. 162, 358 (1967) 59, 60, 61, 62, 63 72. B.G. Silbernagel, M. Weger, J.H. Wernick, Phys. Rev. Lett. 17, 384, (1966) 60, 61 73. B.G. Silbernagel, M. Weger, W.G. Clark, J.H. Wernick, Phys. Rev. 153, 535 (1967) 60 74. B.W. Batterman, C.S. Barrett, Phys. Rev. Lett. 13, 390 (1964) 60 75. A.C. Gossard, Phys. Rev. 149, 246 (1966) 60 76. D. Rossier, D.E. MacLaughlin, Phys. Rev. Lett. 22, 1300 (1969) 60 77. A.G. Redﬁeld, W.N. Yu Phys. Rev. 169, 443 (1968); 177, 1018 (1969) 62 78. A.Z. Genack, A.G. Redﬁeld, Phys. Rev. Lett. 31, 1204 (1973) 62 79. G.B. Furman, S.D. Goren, Phys. Rev. B68, 064402 (2003) 63 80. H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990); N. Bulut, D. Scalapino, Phys. Rev. B45, 2371 (1992) 63

This page intentionally blank

3 The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR

The purpose of this chapter is twofold. First, it is partly historical, to recount the somewhat uncertain beginnings and explain how ideas developed the way they did, and secondly, to review the early milestones which laid the foundations for the many years of study which were to follow. These agendas will unfold simultaneously in an essentially chronological recounting of the important ﬁrst steps in constructing the ediﬁce of high-Tc NMR phenomenology which exists today. Although the cuprates form a large family of compounds1 , in recounting the major accomplishments in the ﬁeld of NMR studies, one’s attention is drawn to three compounds, namely La2−x Srx CuO4 (LSCO:x), YBa2 Cu3 O7−x (YBCO7-x), and YBa2 Cu4 O8 (Y248). These three have played a major role, both in terms of experimental results and theoretical interpretation. There are other interesting compounds with higher Tc ’s (e.g. Tl2 Ba2 CaCu2 O8 ) and with quantum chemistry just as clean (Hg2 Ba2 Cu2 O4 ). It seems that it was just an historical accident that the three listed above became prominent. Accordingly, they will become our main focus. In Sect. 3.1 we review the structures, phase diagram, and some of the early theoretical models regarding transport and quasiparticle dynamics. Of course with a research topic as completely new and unfamilair as the cuprates, one spends a great deal of time and eﬀort at the outset simply establishing the basic experimental features of the system under investigation. Some of this activity is reviewed in Sect. 3.2, where we shall see that the anomalous nature of the spin dynamics (i.e. T1 ) emerged from the earliest papers to appear. A major milestone in understanding all HF eﬀects in the cuprates came with the Mila-Rice-Shastry picture of predominant transferred HF couplings with their quantum-chemical foundations [2, 3]. This work, presented and discussed in Sect. 3.3 for 63,65 Cu, established a model HF Hamiltonian for the principal nuclei which has been an important touchstone ever since. The 1

See, for example, the wide variety of cuprate structures reviewed by Hazen [1].

R.E. Walstedt: The Superconducting Cuprates: Preliminary Steps in their Investigation via NMR, STMP 228, 67–114 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 3

68

3 Preliminary Steps in Cuprate NMR

application of this picture to the NMR studies of planar 17 O and the 89 Y in the YBCO structure is the subject of Sect. 3.4. The relationship between nuclear spin-lattice relaxation (T1 ) and the dynamical susceptibility χ(q, ω) via the ﬂuctuation-dissipation theorem has been well known for many years [4]. With the cuprates, however, this quantity quickly became the basis for the expression of static and dynamic NMR, for inelastic neutron scattering (INS) results, as well as for theoretical modeling. In Sect. 3.5 we review the derivation of the basic results and give standard expressions for T1 at various nuclear sites in cuprates for reference throughout the book. Finally, in Sect. 3.6 the early and highly signiﬁcant d-wave interpretation of T1 in the superconducting state by Monien and Pines [5] is reviewed in some detail. This was based on an RPA model of the dynamical susceptibility which formed a basis for future modeling of normal-state dynamics as well [6, 7]. As we shall see throughout the volume, fundamentally d-wave behaviors for T1 and for the transverse decay constant T2g were ﬁrmly established several years in advance of the Josephson junction phase-boundary results which ﬁnally turned the tide on the d-wave vs. s-wave question.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO The ﬁrst high-Tc materials to be announced [8] left some degree of uncertainty about the actual crystal structures of the superconducting phases. In the weeks that followed, among the ﬁrst structural reﬁnements to be announced were those of La2−x Srx CuO4 (LSCO) [9] and Y Ba2 Cu3 O7−δ (YBCO) [10]. For that reason as well as the fact of their ease of synthesis into high-quality specimens and of subsequent characterization, these two compounds and closely related materials have been a strong focus of NMR/NQR studies from the inception down to the present era. In this section we present a brief discussion of the structures, doping, and quasiparticle dynamics in these typical cuprates. Discussions of NMR studies on the LSCO family of compounds will be given in Chaps. 4 and 6. 3.1.1 LSCO: A superconductor with Tc (max) 40 K LSCO has the K2 N iF4 crystal structure shown in Fig. 3.1(a) [11]. The key structural element in all of the cuprate superconductors is the CuO2 quadratic array (Cu-O1 in Fig. 3.1(a)), which has been identiﬁed as the region where the hole current is carried in these systems. Note that the O1 ions also form a ◦ quadratic √ array rotated 45 from that of the Cu, and having a lattice constant of a/ 2. Cu ions in adjacent planes are staggered, so that AFM couplings between layers are exremely weak. The physics of these structures is strongly two dimensional.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO

69

(a)

(b)

Cu (2) Y

O (2)

O (3)

c

Ba O (4) O (1) Cu (1)

b

La, Sr O2 O1 Cu

a

Fig. 3.1. (a) The (K2 NiF4 ) structure of La2−x Srx CuO4 , showing the locus of the CuO2 conducting plane. The Sr2+ dopant ions go substitutionally into the La3+ sites, leading to a set of mobile holes which run on the square lattice of planar O2− ions [11]. The structure shown has tetragonal symmetry. However, below a few hundred K an orthorhombic distortion sets in, where the CuO6 octahedra tilt through small angles in the [110] planes. Reprinted ﬁgure from J.D. Jorgensen, H.-B. Sch¨ uttler, et al., Phys. Rev. Lett. 58, 1024, (1987). Copyright 1987 American Physical Society. (b) The YBa2 Cu3 O7−x structure is shown with the chain layers (Cu(1)) on the top and bottom and a pair of Cu(2)O(2,3)2 layers in the middle [12]. Note that there is no bonding between adjacent Cu(2) layers except via rather inert Y3+ ion cores. The O1 sites are shown ﬁlled, forming chains along the b axis. The structural symmetry is orthorhombic. Reprinted ﬁgure from J.D. Jorgensen, B.W. Veal, W.K. Kwok, et al., Phys. Rev. B36, 5731 (1987). Copyright 1987 American Physical Society

The physics of transport is dramatically diﬀerent in the cuprates from what it is in an ordinary d-band metal. For LSCO we consider ﬁrst the case of x = 0, i.e. La2 CuO4 . With the expected valence (La3+ , Cu2+ , and O2− ), the conduction plane consists of Cu2+ ions, i.e. with a single hole in the d shell (dx2 −y2 ) plus O2− closed-shell ion cores. The 3d holes are strongly hybridized with the O2− 2p orbitals, such that over 30% of the localized d-hole density resides on the planar oxygens [13, 14]. In the conventional picture of weaklyinteracting fermions, this would simply be a half-ﬁlled band like an alkali metal. On the contrary, however, the hopping process which might lead to hole conduction is strongly inhibited by coulomb repulsion (U ∼ 10 eV ) on the Cu+2 ion complexes in what is known as a “Mott insulator” [15]. Instead, immobile S = 1/2 local moments on the Cu+2 ions condense to an insulating, antiferromagnetic ground state with TN 325 K. In order to generate conductivity in the CuO2 planes, it is necessary to dope additional holes into the system. This may be done by replacing some of the La+3 ions with Sr+2 ions

70

3 Preliminary Steps in Cuprate NMR

as in LSCO. For each such subsititution a hole must appear in or near the CuO2 plane. Above a small threshold concentration these holes become mobile. In the Zhang-Rice singlet picture, they combine with Cu2+ holes to form a singlet quasiparticle. After considerable investigation and debate, such singlets have ﬁnally been concluded to have negligible HF interactions on their own. It has been suggested that they serve the function of rendering the Cu2+ holes itinerant [16]. The LSCO Phase Diagram The phase diagram of Fig. 1.1 illustrates the resulting behavior as a function of the hole-doping parameter δ ∼ x. First, the antiferromagnetism collapses very quickly with hole doping. At x ∼ 0.02 there is an insulator-to-metal transition, though conductivity is still rather poor. In this region, spin-glassbehavior is thought to occur. At x 0.05 the superconducting phase appears, although the normal-state conductivity is still that of a very bad metal. With an optimum concentration of x = 0.15, Tc then peaks at ∼ 40 K. Beyond that point is the overdoped region, where the system becomes more and more like a normal metal. Tc then declines to zero at x ∼ 0.35. The pattern seen with LSCO is repeated with essentially every cuprate superconductor, except that in many cases it is not possible to vary the carrier content all the way from the antiferromagnetic phase through superconductivity and into the overdoped phase. The line in Fig. 1.1 running from the top of the superconducting dome upward to the left (“S”) is the locus of maxima in the spin susceptibility, and also an approximate boundary between the tetragonal (above) and orthorhombic (below) phases in LSCO. However, there is a “crossover” line in approximately that position in various theories of magnetic behavior [17, 18], for which there is growing experimental evidence in other cuprate compounds. In the Barzykin-Pines model this is a boundary between mean-ﬁeld behavior for the dynamical exponent (z = 2) on the high-temperature side and quantum-critical (z = 1) behavior on the low-temperature side. NMR evidence supporting this picture will be presented and discussed in Chap. 6. 3.1.2 The 92 K Superconductor YBa2 Cu3 O7−x (YBCO) Many cuprates have multiple CuO2 planes neighboring each other with a single layer of cations between them. Y Ba2 Cu3 O7−x (YBCO7-x) has two such neighboring planes separated by a single layer of Y 3+ ions, as shown in Fig. 3.1(b) [12]. This structure also features a “chain” layer, known as the Cu(1) sites, which is a quadratic array of copper ions, but where half of the ligand O2− ions seen in the Cu(2) layers are absent, leaving 1D Cu-O chains running along the b axis of the crystal. The chain sites are a complication in understanding the behavior of YBCO, because as we shall see below, the Cu(1) and Cu(2) sites behave rather diﬀerently.

3.1 Cuprate Structures and Doping Eﬀects: LSCO and YBCO

71

On the other hand, regarding the level of mobile carriers, the YBCO7-x system is self-doping. The minimum doping level is eﬀectively zero when x = 1, giving six oxygens per formula unit. With the expected valencies (Y3+ , Ba2+ , Cu(1)+ , Cu(2)2+ , and O2− ), YBa2 Cu3 O6 is in a vacuum state for conductivity similar to La2 CuO4 . In this structure there are no oxygens at all in the Cu(1) planes, and their corresponding valence state is Cu1+ . The maximum doping occurs when x = 0, whereupon the Cu(1) chains are fully oxygenated, and one has an average valence of 2.33 per Cu ion. This is considered to be slightly overdoped, where the maximum Tc 92 K occurs for x 0.1. It is noteworthy, however, that YBCO7 is stoichiometric and therefore has minimal disorder, i.e. far less disorder than optimally doped LSCO. 3.1.3 Physical Models of Itinerant Quasiparticles in Cuprates At optimum doping levels, then, the cuprate conduction planes then appear to contain a small concentration of mobile holes moving in a sea of S = 1/2, exchange-coupled local moments. Because of the coulomb repulsion, these holes are thought to be restricted to the oxygen sites. The description of this mixture as a superconducting quantum ﬂuid is therefore dramatically diﬀerent from a simple 3d-band of partially-occupied Bloch functions. It has posed a stiﬀ theoretical challenge from the beginning, and even now there is not a clear consensus about it. One thing we understand is that it is not a set of exchange-coupled local moments simply coexisting with a hole band of itinerant fermions. For example, at T Tc all spin magnetism decays to a small fraction of its normal-state level, as we know from NMR shift and relaxation measurements (Sect. 3.2.5). Upon a (low, but) suﬃcient level of doping, then, all Cu2+ holes become eﬀectively itinerant and part of a superconducting quantum ﬂuid at T < Tc . The t-J Model How this takes place has been the topic of many theoretical papers. We mention here the “t-J” model [19, 20], which is an approximation to the one-band Hubbard model. A number of theory papers have shown that the t-J model Hamiltonian (here simplﬁed) Ht−J = J Si · Sj + t [c∗i cj + ci c∗j ] (3.1.1) i,j(nn)

i,j(nn)

results in a band of itinerant quasiparticles of width ∼ J ∼ 0.15 eV [21]. Zhang-Rice Singlets A detailed model for the structure of the quasiparticles themselves, known as the “Zhang-Rice singlet model”, appeared very early on and is still considered an interesting conceptual picture [16]. In this model the mobile holes form

72

3 Preliminary Steps in Cuprate NMR

a singlet complex with neighboring Cu2+ “localized” holes, rendering them itinerant. In spite of their small numbers, the mobile holes are said to render all of the Cu2+ moments eﬀectively itinerant and part of a quantum liquid which condenses into a superconducting spin-paired ground state. That this actually occurs is concluded from decay of the Cu(2) Knight shift and relaxation rate, and thus the spin paramagnetism of YBCO7, to a value small compared with its normal-state value for T Tc (see Sect.3.2). The “Oxygen Hole Band” Issue Contrary to the Zhang-Rice singlet picture, many early papers considered that the doped holes in cuprates would result in a separate hole band residing on the oxygen lattice with its own independent HF eﬀects. This idea was often advanced when it seemed that the ﬂuctuating S = 12 moments which occupy the Cu2+ sites would not give an adequate explanation of NMR shift and relaxation eﬀects at all sites studied. Often the papers concerned made important contributions in spite of maintaining this point of view. Eventually, as will become clear in Chap. 4 and 5, it was realized that there was simply no need for oxygen hole bands with independent HF eﬀects and no evidence for them either. This issue will be mentioned as appropriate in reviewing the relevant literature.

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO It was, of course, realized immediately that NMR studies of the 63,65 Cu, 17 O, and in the case of YBCO, 89 Y nuclear spins could yield a great deal of detailed information about static and dynamic fermion behavior in these systems. Perhaps because of its very high Tc value, there was an intense focus on YBCO at the outset, which was facilitated by the ease with which samples could be synthesized. Accordingly, there were a great many NMR papers on YBCO, mainly fully doped (YbCO7) during the ﬁrst year or two. Our focus in this section will be these early studies of YBCO and the issues they raised. LSCO eventually received its share of attention, and will be addressed both in the next chapter and in Chap. 6. In this section we examine the developments which took place during 1987-88 following the discovery of high-Tc superconductors. It was a time of intensive activity, but at the same time, sample preparation was still in a rather primitive state. There was a deﬁnite focus on YBCO7, the 90 − 92 K superconductor, because of its spectacularly high Tc value and because it is a stoichiometric compound. Even so, almost all of the samples studied during this period were either random powders or milligram-scale crystals which gave narrow resonance lines, but very small signals. The random powders gave (− 12 ↔ 12 ) transition spectra ∼ 5T wide in a typical laboratory (7–8 T) ﬁeld,

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO

73

and it took a great deal of noise averaging to obtain a single spectrum. Only with NQR was it possible to do a T1 measurement. Even so, many basic issues concerning the NMR/NQR study of the cuprates were addressed during this time period, and impressive progress was made toward their resolution. At the end of the two-year period we are focusing on, there were two events which marked the beginning of a more settled period, namely the appearance of the Mila-Rice-Shastry papers to clarify the quantum chemistry and transferred HF interaction picture [2, 3], and secondly, the advent of the oriented powder sample preparation method, which dramatically improved the prospects for precise determination of nearly all experimental NMR parameters. The Mila-Rice-Shastry picture for HF couplings in YBCO is presented in Sect. 3.3. 3.2.1 NMR Shift and Relaxation of the

89

Y in YBCO7

Not surprisingly, the ﬁrst papers on cuprate nuclear spin dynamics to appear featured studies of 89 Y T1 behavior in both the normal and superconducting states [22, 23]. The 89 Y nuclei have very small, I = 1/2 nuclear spin moments, but are 100% abundant. They are very weakly hybridized with the Cu(2) 3d moments, giving them a long T1 , but a relatively isotropic NMR shift, so that they are easy to study in a random powder sample. The quick appearance of these 89 Y studies was a harbinger of a great many fruitful 89 Y NMR studies to follow. The T1 data from [22], shown in Fig. 3.2, immediately revealed two striking behaviors. First, T1 follows a Korringa-like, inverse–T law in the normal state, giving actually a misleading impression of the behavior at its neighboring Cu(2) site to be unveiled soon after. The normal-state data of [23] were in agreement with this ﬁnding, and both papers found a normal-state shift K 0.02% as well. As for T1 , there is no hint of any coherence peak below Tc ; moreover, the decline of 1/T1 below Tc is remarkably abrupt. It behaves in a roughly exponential fashion when plotted vs. T /Tc , and has a slope much larger that the expected asymptotic BCS slope (plotted). If the BCS curve reﬂects a gap 2ΔBCS 3.5 kB Tc , the 89 Y T1 curve shows a gap value 2ΔY 11.2 kB Tc . While such a characterization is somewhat superﬁcial at this stage, it shows at least that the superconducting T1 behavior is dramatically diﬀerent from that of any ordinary d-band metal. (See Sect. 3.6 for further elucidation of T1 behavior below Tc .) NMR/NQR Studies of and T1 (T)

63,65

Cu(1, 2): The Quadrupolar Tensor

Next, many papers appeared in which the four-line NQR spectrum (or part thereof) was reported (63,65 Cu(1) and 63,65 Cu(2)) in YBCO7 [23, 24, 25, 26]. Of course, for the I = 3/2, 63,65 Cu nuclei the value of η cannot be derived from NQR frequencies alone. The full quadrupolar frequency tensor has been

74

3 Preliminary Steps in Cuprate NMR

Spin–lattice Relaxation Rate (s–1)

10–1 YBa2Cu3O9 – δ

Korringa 10–2 89Y

fo = 12.2 MHz BCS

0

1 Tc / T

2

Fig. 3.2. 1/T1 of 89 Y in Y Ba2 Cu3 O9−δ is plotted vs. Tc /T in a semilog plot, where δ 2.1 [22]. In the normal state the data are within error limits of a Korringa curve (solid line, 1/T1 ∝ T ). Below Tc the measured relaxation rate drops much faster than the BCS energy gap would allow (dashed curve - BCS). See text for discussion. Figure reprinted from J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts: Sol. St. Comm. 63, 847 (1987). Copyright 1987 Elsevier Ltd.

deduced from NMR studies of small single crystals of YBCO7-x, with x 0 [27, 28], yielding essentially equivalent results. After some reﬁnement, these tensors may be given (in MHz) as ναα = (-19.03(7), 19.17(7), -0.16(3)) for Cu(1) and (15.94(5), 15.56(5), -31.50(5)) for Cu(2) at 100 K [29], where the numbers in parentheses are the uncertainties in the last digit quoted. This quadrupolar tensor has been analyzed by Frank Adrian [30]. NQR Studies of Cu(1,2) T1 in YBCO7 NQR was used to measure T1 for both the 63 Cu(1) and 63 Cu(2) lines at 22 M Hz and 31.5 M Hz, respectively, giving the ﬁrst glimpse of T1 behavior for the copper sites in the cuprates [24, 23]. The T1 data from [24] are displayed in Fig. 3.3, where markedly diﬀerent behavior is seen to occur for the two copper sites, both above and below Tc . In the normal state, the Cu(1) site T1 behavior is rather Korringa-like, similar to the 89 Y , whereas the Cu(2) site 1/T1 behaves initially like a+bT , but then ﬂattens oﬀ near room temperature. The normal state data from [23] behave in a similar fashion to that in Fig. 3.3, except that T1 values appear to be about 15% longer than from [24]. The value quoted in [31] is also slightly longer, but well within error limits of the data in Fig. 3.3. The reader may note that diﬀerent references cited here give T1 values which are deﬁned variously, none of which agree with the discussion

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 30

(T1T)–1 (sK)–1

12.0

RELAXATION RATE (103 s–1)

75

10.0 8.0

20 10 0 60

6.0

80

100

120

140 160

TEMPERATURE (K)

4.0 2.0 0

0

100 200 TEMPERATURE (K)

300

Fig. 3.3. The 63 Cu relaxation rate 1/T1 is shown plotted vs. T for Cu(1) and Cu(2) in a YBCO7 sample (Tc 92 K) [24]. The NQR rate is shown, which is 3 times the formally deﬁned rate 1/T1 . Reprinted ﬁgure from W.W. Warren, Jr., R.E. Walstedt et al: Phys. Rev. Lett. 59, 1860 (1987). Copyright 1987 American Physical Society

of T1 in Sect. 1.1.5. Recall that the NQR value of relaxation time measured for I = 3/2 is 1/3 of the formally deﬁned T1 (see Sect. 1.1.5). Finally, regarding the data shown in Fig. 3.3, we shall not consider the temperature dependence of T1 in depth until Chap. 5. We comment brieﬂy on the general features of these data. Below Tc the Cu(2) relaxation rate declines very steeply, rather like the 89 Y data in Fig. 3.2. The data from [23] for T < Tc are also similar, the main diﬀerence being that the Cu(2) curve is extended to somewhat lower temperatures, where it is found to level oﬀ markedly. Such behavior is very likely sample dependent. Fitting the Cu(2) rate below Tc (Fig. 3.3) to a BCSstyle exponential decay, a reasonable ﬁt gives 2ΔY 8.3 kB Tc with Tc = 92 K [24]. This is a qualitatively similar result to the slope found above for the 89 Y , but since the latter studies were done in a ﬁeld of 50 kG and the present data were taken in zero ﬁeld, a quantitative comparison may not be warranted. As we shall see in Sect. 3.6, this low-temperature behavior is characteristic of d-wave pairing. 3.2.2 Establishing the Site Assignment for the Cu(1) and Cu(2) NQR Spectra Following the publication of [24] (and [32]) there was a brief period of controversy, caused by the fact that the identiﬁcation of the NQR frequencies with the Cu(1) and Cu(2) sites in these papers was reversed from the correct assignment stated above. The T1 results are valid when attributed to the correct sites, but a large portion of the discussion, based on the incorrect identiﬁcation, would need to be revised [24, 32]. Since a number of discussion points have also been rendered moot by later insights and improved understanding,

76

3 Preliminary Steps in Cuprate NMR

we shall attempt no such revision here. The incorrect assignment was made on the basis of (i) similarity of normal-state T1 curves between the 63 Cu(1) (Fig. 3.3) and the 89 Y (Fig. 3.2) and (ii) on the relative intensities of the 21 M Hz and 31.5 M Hz NQR lines in [24] as well as in other papers [25, 26]. These intensities were essentially reversed from the 2:1 ratio expected from the Cu(2):Cu(1) site count, showing the general unreliability of NQR intensities recorded at diﬀerent frequencies. Following these papers, other papers appeared whose main purpose was to document the correct site assignment. References [27, 28] argued the correct assignment on the basis of data for the EFG tensor. After all, the Cu(2) site has very nearly axial symmetry, while Cu(1) does not, features which are expressed very strikingly in the EFG tensor. Meanwhile, [33] argued the case on the basis of 63 Cu relaxation studies conducted on a sample of GdBa2 Cu3 O7 . The Gd3+ ions each possess a localized moment of nearly 7μB , which ﬂuctuates as a consequence of exchange couplings with the other Gd3+ moments. The nearby Cu(2) nuclei are strongly relaxed by ﬂuctuating dipolar ﬁelds from these moments, whereas, the Cu(1) are largely unaﬀected. These observations conﬁrm the correct assignment. The (− 12 , 12 ) Quadrupolar Powder Pattern for Cu(2) in YBCO7 The authors of [24, 32] also conducted NMR intensity studies for the purpose of site veriﬁcation, partitioning the (-1/2,1/2) NMR line intensity for YBCO7 into Cu(2) and Cu(1) contributions [34] (see also [27]). The intensity of the NMR spectrum was calibrated by comparison with spectra from a known quantity of Cu2 O, yielding an absolute intensity of 2.7 ± 0.3 Copper ions per unit cell of the YBCO7. The Cu(2):Cu(1) intensity ratio was found to be 2 within experimental error. A by-product of the latter exercise was a very precise ﬁt to the η = 0, second-order quadrupolar powder pattern for the (-1/2,1/2) (central) transition at T = 105 K [34], using the same procedures which gave sample powder patterns in Figs. 2.2 and 2.4. This ﬁt is shown in Fig. 3.4, both as spin echo intensity data recorded at pulse separation τ = 20 μs and as the extrapolated, τ = 0 curve with its ﬁt to a quadrupolar powder pattern form (see Fig. 2.2) with Gaussian broadening shown as a dashed line. The residual area above the dashed line ﬁt curve is identiﬁed as the Cu(1) site intensity. See [34] for a detailed discussion. Shift values for the Cu(2) are also deduced from this ﬁt (see below). 3.2.3 Variation of the

89

Y shift K89 (x) with x for YBCO6+x

A study of the doping dependence of the 89 Y NMR shift K89 (x) in YBCO6+x by Alloul and coworkers [35] uncovered some very interesting behavior regarding the Pauli paramagnetism of this system. For x ≥ 0.4 they found an essentially linear increase K89 (x) ∝ (x − 0.4), below which K89 levelled oﬀ to a value which remained constant throughout the insulating phase. It was

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO 5

SPIN ECHO AMPLITUDE (ARBITRARY UNITS)

4

77

63Cu:YBa Cu O 2 3 7

(a)

3 2 τ = 20μsec 1

0 (b)

4

2 τ=0 0 70

72

74

76

78

Ho(kG)

Fig. 3.4. NMR ﬁeld-sweep spectrum of 63 Cu in YBCO7 at T = 105 K and an NMR frequency of 84.07 M Hz. Part (a) is uncorrected data taken with a spin-echo pulse separation of 20 (μs). In part (b) the signal has been extrapolated back to τ = 0 using measured values of T2 at various points in the spectrum. The outer singularity peaks are characteristic of an η = 0 (-1/2,1/2) quadrupolar powder pattern. Such a powder pattern has been ﬁtted to these peaks (dashed line), and serves to distinguish the Cu(2)-site intensity from that of the Cu(1) sites, which lies above the dashed line. There is a spurious peak to the left of center thought to be caused by accidental powder orientation in this otherwise random sample. The calculated Cu(1) intensity with this scheme is 54% of that assigned to the Cu(2) sites. Reprinted ﬁgure from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B38, 9299 (1988). Copyright 1988 American Physical Society

concluded that the latter value of shift K89 2.25 × 10−5 relative to the shift of YCl3 is actually the zero of K89 in this system. The discrepancy with the YCl3 was attributed to a diﬀerence in the chemical shifts of the two systems. However, similar results by Balakrishnan et al. [36] included a study of chemical shifts suggesting that the actual chemical shift in YBCO6+x at low values of x is somewhere above 200 ppm relative to YCl3 , contrary to the foregoing

78

3 Preliminary Steps in Cuprate NMR

conclusion. Eventually, the latter value gained acceptance as the correct zero for the 89 Y spin paramagnetic shift in YBCO. The behavior of K89 (x) with doping is shown in Fig. 3.5. The change in K89 above x = 0.4 is seen to be negative and is attributed to the core polarization of the Y3+ 4d orbitals hybridized into the conduction band in the CuO2 planes of YBCO6+x. The Pauli paramagnetism varies in a similar fashion to K89 , so that in a plot of K89 (x) vs. χm (x) the behavior for x > 0.4 is linear with a slope dK89 /dχm = -4.6 (emu/mole)−1. This is much smaller than would correspond to the full core polarization HF ﬁeld, showing that the 4d admixture is very slight. The authors comment that this behavior seems contrary to the proposed separation of spin and charge behavior of the RVB model [19, 20].

89Y

8

NMR

YBa2Cu2O6 + x

Bo = 7.5 Tesla T = 293 K 6

–105 ΔK

4

2 AF 89YCl

0

–2

3

K=0

0

0.2

0.4

0.6

0.8

1

X 89

Fig. 3.5. The room temperature Y NMR shift in YBa2 Cu3 O6+x is plotted for a series of x value ranging from nearly zero to one. The is interpreted (see text) to mean that the Pauli paramagnetism vanishes below X = 0.4 and the shift value below that point is simply the diﬀerence in chemical shifts between YBCO6 and YCl3 . Figure reprinted from H. Alloul, P. Mendels, et al., Phys. Rev. Lett. 61, 746 (1988). Copyright 1988 American Physical Society

3.2 Early NMR/NQR Studies: The Early Predominance of YBCO

3.2.4 Physical Models for the Relaxation of

63

79

Cu(2) in YBCO7

One of the major challenges to the NMR community and to the theorists as well has been the interpretation of the copper-site T1 data, which is to say the magnitude of T1 , its anisotropy, and its temperature dependence. We discuss the temperature dependence of T1 (for all sites) in Chap. 5, and as of this writing, it is still an unsettled issue. The magnitude and anisotropy of T1 , however, came to light early and were the main inﬂuences which brought about the Mila-Rice discussion and formulation of the problem. We review here two background developments which highlighted the situation, namely the model treatments of T1 in experimental papers by Walstedt et al. [37] and by Pennington et al. [29]. Reference [37] reported the ﬁrst data on the anisotropy of the 63 Cu(2) T1 , ﬁnding T1c /T1ab 3.5.This was done with a random powder sample, using NQR (θ = 0), and the up-ﬁeld and down-ﬁeld singularities of the (-1/2,1/2) powder pattern (θ 43◦ and θ = 90◦ , respectively). The data were not ﬁrstrate, but the result for T1c /T1ab held up in later studies with oriented powders [38]. The paper goes on to discuss the feasibility of explaining the foregoing T1 data using the typical formulation of spin-lattice relaxation in 3d metals given by Yafet and Jaccarino [39] and discussed in detail in Sect. 2.3. The hyperﬁne constants are well-known for the Cu2+ , and the density of states is derived from the susceptibility, where the orbital component is estimated and subtracted oﬀ. The result is, if anything, an overestimate for n(EF ). The normally dominant orbital relaxation mechanism is vitiated in YBCO by the nearly pure dx2 −y2 ground state, which has negligible matrix elements for the orbital HF process. As a result, the estimated relaxation rate with this scheme falls far short of the magnitude of the observed rates, and the peak anisotropy available falls well short of the measured ratio. The standard dband relaxation model was concluded to be incapable of accounting for the cuprate T1 data. 3.2.5 Introduction of the Spin Hamiltonian Model for the Cu2+ A diﬀerent tack was taken by Pennington, Durand, et al. [29]. The Cu(2) relaxation tensor was measured using NMR on single crystal samples, ﬁnding similar numbers, but an anisotropy of 4.2, rather larger than the 3.5 reported in [37]. This discrepancy is most likely a diﬀerence in samples. In any case it has never been resolved. For the analysis of T1 these authors adopt a model of ﬂuctuating Cu2+ local moments, adopting a spin Hamiltonian form for the spin HF tensor [40] and simply deducing the anisotropy of the spin HF ﬁeld from the corresponding anisotropy of T1 for Cu(2) given above. Simultaneously, however, Takigawa, Hammel et al. announced their result that the c axis NMR shift changed very little below Tc , while other components underwent substantial changes [33, 41]. They concluded that the spin paramagnetism declined eﬀectively to zero for T Tc . It followed that the net c axis

80

3 Preliminary Steps in Cuprate NMR

spin HF component for Cu(2) is nearly zero! From this observation sprang the Mila-Rice model for Cu(1,2) HF couplings, presented in Sect. 3.3. Both papers introduced a local moment-based calculation of the orbital susceptibilities on the Cu2+ sites, which, along with the spin and orbital HF tensors, constitutes the spin Hamiltonian picture for the detailed physics of the Cu2+ ions [42]. We shall discuss this point of view in detail in Sect. 3.3. In the meantime, it is interesting to consider the vanishing of the cuprate spin susceptibility χs (T ) at temperatures T Tc , postulated above, in the context of all of the diﬃculties over this point which occurred vis-a-vis the simpler superconductors discussed in Sect. 2.2.2. We recall that vanishing of χs (T ) required that the inverse lifetime from spin-orbit scattering must be small compared with the energy gap [43] (see (2.2.8)). That this must be so for YBCO7 results from that combined facts that (i) Cu is a very light element with relatively small spin-orbit coupling and (ii) energy gaps in the cuprates are roughly an order of magnitude larger than those found for sp-band superconductors. It is reasonable to suppose, then, that /Δ(0)τso 1 (1.2.8a), even in the mixed state, from which it follows that χs (T Tc )/χs (T > Tc ) 1. 3.2.6 Experimental Breakthrough: Oriented Powder Samples Late in 1987 a paper appeared which reported the technique of creating powdered samples of YBCO in which each crystallite is oriented with its c axis parallel to an applied magnetic ﬁeld [44]. This scheme relies upon the anisotropy of the (orbital) susceptiblity to provide the torque necessary to align each particle with the ﬁeld. The other necessary condition has to do with the morphology of the polycrystalline material to be oriented. It is assumed that upon reducing sample material synthesized in polycrystalline form to ﬁne powder, each particle of such a powder will be a single crystal, and thus, free to orient with its c axis along the applied ﬁeld. Any particle consisting of two or more crystallites will not align properly. The success of this technique is therefore dependent on the particular cuprate under study. YBCO is generally a good candidate for this eﬀect, where one can generally expect the Cu(2) (- 12 , 12 ) NMR line to assume a width of 100 Oe or less [38]. Following the original announcement, many NMR studies have appeared using oriented samples [28, 38]. Powder orientation results in an emormous improvement in the NMR signal strength, where signals requiring accumulation of ∼ 105 echo traces for adequate noise resolution [32] become visible on a single oscilloscope trace. The Cu(1) NMR signal is also greatly improved, where the quadrupole splitting along the c axis corresponds to an extraordinarily small component of the quadrupolar tensor, resulting in a weakly split line [38]. The real signiﬁcance of this method is that one can now measure the anisotropy of T1 with a conveniently large signal [38], although remarkably good results were obtained with milligram-scale single crystals [29]. To measure oriented samples in a transverse ﬁeld, one customarily sets the oriented particles in epoxy. Field oriented samples yield a 2D powder

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

pattern in a transverse ﬁeld, which is also important for studies of the and 89 Y NMR parameters.

81 17

O

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates The Mila-Rice-Shastry model [2, 3] for HF coupling with itinerant Cu2+ holes in a superconducting cuprate clariﬁed a number of murky points regarding NMR shift and T1 behavior. Important features were (i) transferred HF couplings, (ii) the ability to account for observed behavior with a single “band” of excitations, and (iii) the quantum chemistry framework for the HF Hamiltonian which emerged. Looking back, this was an important turning point in our understanding of HF interactions and of their dynamics. Previous workers had tried to formulate the NMR shift and relaxation in terms of Cu2+ local moment dynamics driving purely on-site HF couplings, but found peculiar results when trying to ﬁt the extraordinarily large T1 anisotropy at the Cu(2) site [29]. The demise of the local HF coupling picture was sealed by the observation that the Cu(2) c–axis shift term attributable to 3d-spin moments was vanishingly small [33, 41], while, in contrast, c–axis HF ﬂuctuations dominated the T1 process [29, 37, 38]. It was clear that there were two or more independent contributions to the c–axis HF coupling which vanished when superimposed to form the net shift, but produced ﬂuctuations which did not cancel and were in fact very large. The Cu(2)-Cu(2) Transferred HF Coupling The resolution of the vanishing c-axis spin shift question was concluded to be a highly unusual transferred HF coupling between a Cu-site nuclear spin and the four nn Cu spin moments, which is a great deal larger that previously identiﬁed interactions of this sort [45]. The putative isotropic transferred nn coupling may be written HTr = B I · Si , (3.3.1) i(nn)

where the sum is over the four nearest-neighbor Cu(2) sites to the site in question. Nonetheless, it was argued that the only alternative to this was HF coupling with mobile holes on the planar oxygen lattice. Any such hole state would need to hybridize with the Cu(2) 4s state, in order to explain the large, isotropic HF coupling. Suitable oxygen hole states for this purpose were argued to be energetically unfavorable [2]. It was also argued by Mila and Rice that doped holes would be in singlet states which have negligible HF coupling with nuclear moments [46]. Whether this is correct or not is unresolved. To

82

3 Preliminary Steps in Cuprate NMR

our knowledge, however, no unidentiﬁed HF eﬀect, static or dynamic, has ever been reported to contradict this conclusion. The result is a quantum ﬂuid of Cu2+ holes which is expected to be the sole source of HF eﬀects in the normal state and to form spin pairs in the superconducting ground state. Hybridization with the O2− neighbors has been proposed as the source of spin HF eﬀects for the 17 O(2,3) sites by Shastry [3], and hybridization with the Y3+ 4d orbitals has been demonstrated by Alloul et al. [35]. That this is a correct picture is evidenced by the vanishing of 1/T1 at T Tc for the 63,65 Cu, 17 O, and 89 Y NMR lines for which data have been reported, as well as of the spin-paramagnetic NMR shifts. 3.3.1 General Deﬁnition of the HF Tensors Before entering into the details of extracting the HF tensors from shift and susceptibility data, we set down a general framework for the structure of all HF couplings to be discussed from this point forward. The YBCO HF tensor components are deﬁned by ⎧ ⎫ ⎪ (1) ⎪ ⎪ ⎪ (1) (1) ⎪ ⎪ Aα Siα + B Iiα ⎪ Sjα ⎪ HHF = ⎪ ⎪ ⎩ ⎭ i,α j(nn) ⎧ ⎫ ⎪ (2) ⎪ ⎪ ⎪ ⎪A(2) ⎪ + Iiα ⎪ Siα + B (2) Sjα ⎪ ⎪ ⎪ α ⎩ ⎭ i,α

+

i,α

17

Iiα

j(nn)

j(nn)

Cα Sjα +

i,α

89

Iiα

Dα Sjα .

(3.3.2)

j(nn)

The four terms in (3.3.2) refer, respectively, to nuclei on the Cu(1), Cu(2), O(2,3), and Y sites. In the ﬁrst two terms the nn couplings B (1,2) are in(1,2) troduced as deﬁned in the foregoing paragraph. The coeﬃcients Aα are composites of the on-site Cu(1,2) HF couplings which are derived from the spin Hamiltonian model below. For the O(2,3) and Y, the sums on j cover two and eight nn Cu(2) sites, respectively. Omitted are oxygen sites O(1) and O(4) for the sake of simplicity. Their shift and relaxation behavior have been recorded, but are not essential to our understanding of the CuO2 planes where (1) the superconductivity resides. The 63,65 Cu(1,2) nuclear spins are labelled I i (2) 17 17 and I i in an obvious notation. The O(2,3) spins are labelled I i and the 89 Y spins are labelled 89 I i . Note that all HF eﬀects are assumed to be driven by the Cu2+ spin operators S j , which are rendered itinerant by the hole doping as in the Zhang-Rice model [16]. Our viewpoint regarding hole doping is that there are no HF effects which stem directly from the doped holes [46]. Such eﬀects have been discussed extensively in the literature, and we shall review these discussions where appropriate. It is not felt, however, that convincing evidence for oxygen hole-band HF eﬀects has ever been developed for the cuprates.

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

83

Evaluation of the HF Coeﬃcients (1)

(2)

The clearest and simplest way to evaluate HF coeﬃcients (e.g. Aα , Aα , Cα , and Dα in (3.3.2)) is by means of analysis of the NMR shifts and the measured susceptibility. In the case of YBCO7-x which we are concerned with here, there is the complication of partitioning the measured susceptibility between the Cu(1,2) sites and neighbors, principally because modeling the behavior of the Cu(1) sites involves a certian amount of guesswork. The spinHamiltonian model is used to estimate the orbital terms. In the end, MR simply partitioned χs (T ) equally between the three copper sites. Eﬀorts in the literature to improve on this have only been partially successful [47]. To proceed, then, we ﬁrst estimate the orbital (Van Vleck) susceptibilities and NMR shifts by means of the spin Hamiltonian model [42]. The core diamagnetic term can be estimated from tables. Subtracting these terms from the measured total then yields the spin susceptibility χs (T ). Provisions to be described below will be made for its anisotropy, which for the Cu(2) sites will be ∝ gα2 , α = ab, c, according to the spin Hamiltonian. HF tensor components will then be derived We take the 17 O(2,3) as17follows. sites as a typical example, where HHF17 = i Iiα Cα j Sjα is the O(2,3) nuclear spin Hamiltonian term from (3.3.2). Taking the expectation value of this term in the presence of a ﬁeld H along the ξ axis and equating this result to a nuclear shift Zeeman term −γ17 H i Iiξ Kξ , we ﬁnd Kξ (T ) =

2Cξ χsξ (T ) = α17ξ χsξ (T ), γ17 gξ μB NA

(3.3.3)

where α17ξ is the shift coeﬃcient and χsξ (T ) = −gξ μB NA Sjξ /H is the molar susceptibility ( Sjξ < 0 is independent of j) of a Cu(2) site. In practice the shift coeﬃcient is determined experimentally by dividing a measured spin-paramagnetic shift by a “best estimate” of the corresponding molar susceptibility. The tensor Cβ has the units of energy, so what we will tabulate is the quantity Cξ = NA μB α17ξ /2 = Cξ /γ17 gξ ,

(3.3.4)

in units of “kOe/μB ”, since this is the HF ﬁeld which would be found if there were a magnetization of one μB on each Cu(2) site. It is divided by 2, because each O(2,3) has two Cu(2) neighbors. Appropriate deﬁnitions of the HF constant for each case discussed will be given as they come up. We ﬁnally want to emphasize one point, which is that the scale of the HF constants will depend on the value of the χs (T ) tensor adopted. It is given in Table 3.4, and corresponds to T = 100K. No other standard will be used for HF coeﬃcients for YBCO7-x, including for the deoxygenated phases. As we shall see, the shift values for YBCO7 are fairly well established, and if more accurate values for the χsξ (100K) are determined, it is a simple matter to scale all of the HF coeﬃcients uniformly. We proceed, then, with the determination of the HF coeﬃcients.

84

3 Preliminary Steps in Cuprate NMR

3.3.2 Extracting the Cu(1,2) HF tensors for YBCO7 from Shift and Susceptibility Data Using the Spin Hamiltonian Model As a preamble to their quantum chemical calculation of hybridized wavefunctions for the Cu(1,2) sites, Mila and Rice [2] analyzed the measured shifts and susceptibility for YBCO7 with the aid of a spin Hamiltonian model, yielding both spin and orbital HF tensors for the Cu(1,2) sites, as well as crystal-ﬁeld splittings for the Cu(2) site. Although the spin Hamiltonian model is most appropriate for insulators, it appears to provide an accurate description of HF eﬀects in the narrow-bandwidth doped cuprate superconductors. Since late 1988 when this was ﬁrst proposed, a good deal of additional data for all the experimental quantities has been reported. Although the original data used served a very important purpose, newer data were published with smaller error bars, and we believe that they lead to a picture with better internal consistency. Accordingly, we discuss here the original K and χ analysis, but re-work the numbers at the same time. The changes are small, but appear to be signiﬁcant. The Spin and Orbital NMR Shift Tensors for Cu(1) in YBCO7 (1,2)

(1,2)

(1,2)

We shall use the notation Kt (a, b, c) = Korb (a, b, c) + Ks (a, b, c) to represent the total, orbital, and spin shifts along the a, b, c axes for Cu(1,2). In Table 3.1 we list the original Cu(1)-site shifts [33, 41] and other data which were published a bit later. The total shift values listed were measured at T = 100 K, and the orbital shifts, which are assumed to be temperature (1,2) independent, were measured at 4.2 K, where it is assumed that Ks (a, b, c) = 0. The spin components listed then correspond to 100 K. Note that the diﬀerences between these two sets of data are not large, but are outside of the stated error bars in a number of cases. Spin and Orbital NMR Shift Tensors for Cu(2) in YBCO7 For the Cu(2) NMR shift data in Table 3.2 there are additional data sources listed, and we also include susceptibility data. Since it is not feasible to resolve Table 3.1. Table comparing Cu(1)-site shift values from the original Mila-Rice data [33, 41] and other data which appeared later. The data from [48] are used in the analysis discussed in the text. The spin components are obtained by subtraction: Ks = Kt - Korb . Shift values are in (%). The numbers in parentheses are uncertainties in the last digit quoted (1)

(1)

(1)

(1)

(1)

(1)

(1)

(1)

(1)

Source Kt (a) Kt (b) Kt (c) Korb (a) Korb (b) Korb (c) Ks (a) Ks (b) Ks (c) [33, 41] 1.34(2) 0.61(2) 0.60(8) 1.18(2) 0.43(2) 0.31(8) 0.16(2) 0.18(2) 0.29 (8) [29] 1.38(7) 0.55(7) 0.60(4) [48] 1.32(2) 0.56(2) 0.59(1) 1.08(4) 0.27(4) 0.25(1) 0.25(4) 0.29(4) 0.33(1)

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

85

Table 3.2. Table comparing Cu(2)-site shift values for YBCO7 from the original Mila-Rice data [33, 41] with other sets of data which have subsequently been reported. Data from the bottom line are employed for the analysis discussed here [48]. No distinction is made between the a and b planar axes. The susceptibility components given for [34] are derived by the procedure stated in the text. We note that the spin components are obtained by subtraction: Ks = Kt - Korb . Shift values are in (%) and susceptibilities in units of (10−6 emu/mole f.u.). The numbers in parentheses are uncertainties in the last digit quoted (2)

(2)

(2)

(2)

(2)

(2)

Source Kt (ab) Kt (c) Korb (ab) Korb (c) Ks (ab) Ks (c) χt (ab) χt (c) [33, 41] 0.61(2) [29] 0.59(4) [34] 0.55(5) [50] [48] 0.58(2)

1.27(8) 0.24(2) 1.267(1) 1.30(3) 0.25(2) 1.27(1) 0.28(1)

1.35(8) 0.37(2)

−0.08(8) 250

339

224(10) 361(10) 1.28(2) 1.28(2) 0.30(1)

−0.01(1)

a and b axis data for the Cu(2) shift, nor for the susceptibility, the in-plane data are labelled “ab”. Again, the original Mila-Rice data are given on the top line, and other sources of data are listed below. There is reasonably good consistency between the last two sources listed. We shall use the bottom line numbers for analysis here. The susceptibility components attributed to [34] were obtained in the following way. The actual data in [34] are measurements on a random powder sample. The 100K susceptibility from these data (2.70×10−4(emu/molef.u.)) has been partitioned between χt (c) and χt (ab) assuming the ratio χt (c)/χt (ab) = 1.61, as reported in [49]. This is, to our knowledge, the largest anisotropy ratio which has been reported for an oriented powder sample, and therefore corresponds to an unusually high degree of crystalline alignment. The resulting values for χt (ab) and χt (c) are given in the table and are used in the analysis discussed in the text. Determination of the Orbital Susceptibility Tensors Our next step is to use the Cu(1,2) shift tensors from the bottom lines of Tables 3.1 and 3.2 to determine the orbital susceptibilities, using the relation χorb (a, b, c) = Korb (a, b, c)/αorb ,

(3.3.5)

where αorb = 2 r−3 /NA . Equation (3.3.5) may be employed for either Cu site. We take r−3 = 6.3 a.u. from [2], yielding αorb = 141 (emu/mole)−1. The resulting orbital susceptibility values for the Cu(1,2) sites are listed in Table 3.3. Note that the a and b axis values are identical for Cu(2). Also tabulated are susceptibility values labelled “s+orb”, which are obtained with the following equation: tot tot χtot s+orb = χs + χorb = χt − χdia

(3.3.6)

86

3 Preliminary Steps in Cuprate NMR

Table 3.3. Table listing orbital susceptibility components derived from the orbital shifts from the bottom lines of Tables 3.1 and 3.2 using (3.3.5). Also, total susceptibilities from second line of Table 3.2 are listed here after correction for atomic core diamagnetism (see text). Susceptibilities are given in units of (10−6 emu/mole) for individual sites and (10−6 emu/molef.u.) for χtot s+orb (1)

(1)

(1)

(2)

(2)

76.5

19.1

17.7

19.8

90.7

tot χorb (a) χorb (b) χorb (c) χorb (ab) χorb (c) χtot s+orb (ab) χs+orb (c)

399

536

where χt is the experimental value, and where we use the (isotropic) χdia = −1.75 × 10−6 (emu/mole) from [2]. The measured susceptibilities cannot distinguish between the a and b axes. Determination of the Spin Hamiltonian Parameters Using the spin Hamiltonian expressions [42] χorb (c) = 0.70 (8μ2B /Δ0 ) and χorb (ab) = 0.70 (2μ2B /Δ1 ), we may now use the numbers in Table 3.3 to estimate the crystal ﬁeld energies Δ0,1 . The numerical factors 0.70 in these formulas are reduction factors based on measurements [13] and calculations [14] of covalency in the CuO2 planes. (2) Inserting the values of χorb (ab, c) from Table 3.3 then leads to Δ0 = 2.00 eV and Δ1 = 2.29 eV, in accord with calculations by McMahan et al. [51] which suggest that the Δ0,1 lie in the vicinity of 2.0 eV and diﬀer by ∼ 10%. We can now evaluate the g-factor expressions g⊥ = 2 − 2λ/Δ1 and g = 2 − 8λ/Δ0 , where λ is the spin-orbit coupling parameter. The free ion value of λ −830 cm−1 ([42], Table 7.6). Mila and Rice adopted the value λ = −710 cm−1 = −0.088 eV . We suggest that a slightly greater reduction factor is appropriate here, such as the value 0.75 given by Owen and Thornley for N i2+ in MgO [52]. This yields λ = −0.077 eV , which we employ henceforward. With this value we ﬁnd g⊥ = 2.067 ; g = 2.308.

(3.3.7)

The expected value for the anisotropy As of the spin susceptibility, is As = 2 = 1.247. We note that g-factor anisotropies in metals are χs /χs⊥ = g 2 /g⊥ not unusual, as may be seen in data reported for Cu and other noble metals [53]. Our next task is to partition the measured susceptibility between the Cu(1) and Cu(2) sites. Where Mila and Rice assumed the same isotropic spin susceptibilities for Cu(1) and Cu(2), we shall use the same axial susceptibility tensors for both sites. As discussed in [2] this is an oversimpliﬁed viewpoint for the Cu(1) site, for which the error incurred is hopefully not too large. We equate the “s+orb” values in Table 3.3 to expressions using the same axial spin susceptibility tensor components for the Cu(1) site (a axis) and the

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

87

Cu(2) sites (c axis). For this purpose we introduce the variable χs⊥ for a singlesite transverse component and χs = A χs⊥ for the longitudinal component, where A and χs⊥ are to be determined. This leads to the following equations for A and χs⊥ : (2)

(1)

χtot s+orb (c) = 2 χorb (c) + χorb (c) + (2A + 1) χs⊥ (3.3.8a) (2)

(1)

(1)

2 χtot s+orb (ab) = 4 χorb (ab) + χorb (a) + χorb (b) + (A + 5) χs⊥ . (3.3.8b) Inserting the numbers from Table 3.3 we solve (3.3.8), ﬁnding A = 1.166 and χs⊥ = 1.01 × 10−4 (emu/mole). This ”experimental” value for A is somewhat smaller than the spin Hamiltonian g-factor-based estimate of 1.247 calculated in the previous paragraph. The spin susceptibility tensor components deduced here are then 1.01 and 1.18×10−4(emu/mole) for χs⊥ and χs , respectively, as compared with the isotropic Mila-Rice value of 1.08×10−4(emu/mole). It is interesting to inquire what the possible source might be for the foregoing discrepancy in values for A. First, it seems likely that the correct value would agree with the spin Hamiltonian model, since other aspects of the model are quite successful. Next, it seems unlikely that approximate treatment of the Cu(1) site behavior is the source of the discrepancy. For example, assuming the Cu(1) site susceptibility to be isotropic would only increase the deduced anistropy for the Cu(2) site by ∼ 1%. On the other hand, the deduced anistropy A is quite sensitive to the experimental anisotropy value, which was taken to be χt (c)/χt (ab) = 1.61 [49] in the foregoing analysis. If this were increased by less than 4% to 1.67, (3.3.8) would yield the the spin Hamiltonian value χs /χs⊥ = 1.247. This result suggests that the correct value for the susceptibility anisotropy may be a few percent larger than the largest value which has been reported. 3.3.3 Quantum Chemistry of YBCO7 and the Hyperﬁne Tensor While it is to be expected that there is strong covalency between the Cu2+ moments and the oxygen ligands in the cuprate conducting planes, it seems quite surprising that there is a substantial admixture of the 4s wavefunctions of the nearest-neighbor Cu2+ ions, as posited in (3.3.1). Yet this is precisely what the quantum-chemical calculations show [2, 54]. We outline the calculation here and refer the reader to the original papers for the details. The tight-binding quantum-chemical calculations for Cu(2) are based on the diagram shown in Fig. 3.6, where the relevant orbitals are shown at each ionic site. The dx2 −y2 orbital is shown at the central (planar) Cu2+ ion, the pσ orbitals on the oxygen ligands, and the 4s orbitals on the four nn Cu2+ ions. With the sign conventions given in the ﬁgure, the p and s-orbital admixtures which couple to the central dx2 −y2 orbital are p = (p1x − p2y − p3x + p4y )/2 and s = (s1 − s2 + s3 − s4 )/2. The energies are as follows: The 3d-orbital energy is taken as the origin, d = 0. The ligand on-site energies are taken to be p = 4 eV and s ∼ −6 eV . The hopping energies shown in Fig. 3.6 are t1

88

3 Preliminary Steps in Cuprate NMR + s 2

×

+ p2y t8 s3

+ ×

t1

–

dx2 – y2 +

–

p3x

–

+

+

+ –

p1x –

–

+

+ ×

s1

t3 p4y

+ × s4

Fig. 3.6. A schematic representation of the dx2 −y 2 orbital at a Cu(2) site and the pσ orbitals of the O2− ligands, as well as the 4s orbitals on the four nn Cu(2) sites, which are admixed to form the total wavefunction of the Cu(2) 3d-holes for the Mila-Rice quantum chemistry calculation (see text). The tα ’s show hopping matrix elements, and the signs give phase conventions for admixed orbitals. Figure reprinted from F. Mila, T.M. Rice, Physica C157, 561 (1989). Copyright 1989 Physica C

= 0.33 eV, t3 = 1.38 eV, and t8 = 3.9 eV. The Hamiltonian is then solved in conjunction with the somewhat more complex Cu(1)-site Hamiltonian. The Wannier Wavefunction for Cu(2) The Cu(2) tight-binding (Wannier) wavefunction is written |ψ(2) = αd |dx2 −y2 + αp |p + αs |s ,

(3.3.9)

where the solution presented gives αd = 0.9, αp = -0.34, and αs = -0.26. In addition there is a coupling via the oxygen ligand to the nearest Cu(1) site and to the 4s state on that site. This coupling has some eﬀect on the Cu(2) shift, but an essentially negligible eﬀect on the Cu(2) T1 . For simplicity we shall omit these terms. The transferred isotropic HF coupling (3.3.1) from the nn Cu(2) sites may be estimated as follows. The 4s contact HF coupling from EPR data for atomic Cu [55] is 16π |ψ4s (0)|2 = 0.45 × 1027 cm−3 . 3

(3.3.10)

Referring to (1.2.2) and (1.2.7), the corresponding 4s contact HF coupling is 2,080 kOe/μB . The total transferred coupling is then estimated to be α2s ×2080 = 141 kOe/μB , as compared with ∼ 160 kOe/μB required to give the nearly vanishing c axis spin-paramagnetic shift. Mila and Rice note that the value stated is for atomic Cu, whereas Cu2+ will have an enhanced value of |ψ4s (0)|2 because of the ionic plus charge. There seems little doubt that the nn 4s admixture eﬀect is the correct answer to the c axis HF anomaly.

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

89

The Composite Cu(2) Spin Hyperﬁne Tensor Let us now state the remainder of the HF coupling terms for Cu(2) and then formulate the Mila–Rice T1 relaxation tensor. The full HF tensor may be written [42], (2) HHF = A(2) I · Si , (3.3.11) α Iα S0α + B(2) α

with

i(nn)

(2)

(2) (2) A(2) α = Acp + Adip,α + Aso,α ,

(3.3.12)

where the three terms shown are the isotropic core polarization term, the dipolar term, and the spin-orbit term, and where α = (ab, c) for the axially symmetric Cu(2) site. The spin-orbit terms, being a second-order perturbation eﬀect to higher crystal ﬁeld states driven by the spin-orbit coupling, are a special feature of the spin Hamiltonian picture. They are actually an orbital ﬁeld admixed into the spin HF terms. The core-polarization term is sometimes given as proportional to r−3 , which is a holdover from EPR studies where the origin of this term had not been identiﬁed2 . Here we shall simply appeal to systematic studies, which give Acp /2γn −127 kOe/μB . The dipolar and spin-orbit terms may be written (in energy units) 2 Adip,ab = 2γn μB r−3 , 7 4 Adip,c = −2γn μB r−3 , 7 11λ −3 , Aso,ab = 2γn μB r − 7Δ1 6λ 8λ . − Aso,c = 2γn μB r−3 − 7Δ1 Δ0

(3.3.13a) (3.3.13b) (3.3.13c) (3.3.13d)

We use the same parameters used earlier to evaluate the Van Vleck orbital susceptibilities and in (3.3.7) for the anisotropic g-factor to calculate the spin HF tensor. These are λ = −0.077 eV , Δ0 = 2.00 eV , Δ1 = 2.29 eV , and r−3 = 6.3 a.u. The resulting values for the Cu(2) spin HF tensor (3.3.11) are listed in Table 3.4 in units of kOe/μB (see Sect. 2.3.1). We also employ a reduction factor of 0.70 derived from determinations of covalency [13, 14] for these parameters, as well as the core polarization HF ﬁeld, in the second line of Table 3.4. The value of B (2) shown is adjusted to give minimum error for (2) (2) the Cu(2) spin-paramagnetic shift values Ks (ab) and Ks (c) (bottom line (2) (2) of Table 3.2). The estimated values KsE (ab) and KsE (c), given by 2

The work of Heine [56] later revealed that it had no connection with r −3 .

90

3 Preliminary Steps in Cuprate NMR

Table 3.4. Listing of values of spin HF tensor components for the Cu(2) sites, as derived in the foregoing paragraph. On the second line the free-ion component values have been corrected with a reduction factor 0.70 to account for covalency as mentioned above. A value of B (2) is stated (see (3.3.11)) which minimizes the errors in the spin-paramagnetic shift components given in the bottom line of Table 3.2. This value of B (2) is in reasonable accord with the estimate derived from quantum chemistry [2]. The spin susceptibility tensor associated with each Cu(1,2) site deduced earlier is shown, along with the Cu(2) site spin-paramagnetic shift tensor corresponding to the HF parameters given. Finally, the composite on-site HF tensor components given by (3.3.12) are listed. All HF tensor components are in units of kOe/μB , with susceptibilities in 10−6 (emu/mole) (2)

Acp

(2)

(2)

(2)

(2)

(2)

(3.3.13) −127 113 Corr. −89 79

−225 21 −158 15

131 92

55 38

(2) KsE (ab, c) (2)

(2)

(2)

(2)

Adip,ab Adip,c Aso,ab Aso,c B (2) χs⊥ χs KsE (ab) KsE (c) Aab Ac

(2)

(2)

=

101 118 0.28%

(2)

Aab,c NA μB

−0.01% 5

−155

χs⊥, ,

(3.3.14)

(2)

where Aξ = Acp + Adip,ξ + Aso,ξ + 4B (2) , are also listed in the table. A good ﬁt is seen to be achieved. To the far right are listed the components (2) of the composite on-site HF tensor Aα deﬁned by (3.3.12). 3.3.4 T1 Ratios and Electron Spin Correlation Eﬀects Mila and Rice introduced the concept of electronic spin-spin correlation factors in their T1 calculation, but did not use them in their discussion of T1 anisotropy. Subsequent discussions of the T1 problem in cuprates have made extensive use of this idea. Here, we ﬁnd it necessary to consider the eﬀect of spin-spin correlations to obtain agreement with experimental data. All HF constants are given in (kG/μB ). The primed notation for this option introduced with (3.3.4) is suppressed in this subsection for simplicity. Using expressions similar to MR, we now present results for the Cu(2) 2 (ab, c)χs (ω0 ), where the relaxation tensor. The 1/T1ab,c have the form HHF squared HF ﬁeld parameters are (2) 2

(2)

2 (c) = 2 [Aab +4 B (2) 2 +8 Aab B (2) K01 +4 B (2) 2 (2 K12 +K13 )] (3.3.15) HHF

and (2) 2

2 HHF (ab) = [Aab

(2)

2 (2) + A(2) + 8 B (2) 2 + 8 (Aab + A(2) K01 c c )B

+8 B (2) 2 (2 K12 + K13 )],

(3.3.16)

where Kij = · S j is the normalized spin-spin correlation between sites labeled i and j (see Fig. 3.6). The quantity χs (ω0 ) has the dimensions of a correlation time, but also has in it the density of states and temperature factors 4 3 S i

3.3 The Mila-Rice-Shastry Model: A Universal HF Tensor for the Cuprates

91

that arise out of some speciﬁc model of quasiparticle dynamics appropriate to the cuprates. If the system were a Fermi liquid one would have χs (ω0 ) ∝ T . Without such modeling this theory cannot give absolute values for T1 , but it can predict the anisotropy of T1 at the Cu(2) site using the HF tensor data from Table 3.4. Having minimized the error in the spin paramagnetic shift tensor to estimate the value of B (2) given in the table, we insert the parameter values into the ratio of (3.3.16) to (3.3.15) to determine the expression, T1c [1 − 1.69 K01 + 0.38 (2 K12 + K13 ] = 2.64 . T1ab [1 + 0.29 K01 + 0.99 (2 K12 + K13 )]

(3.3.17)

Equation (3.3.17) is to be compared with experimental data giving values of T1c /T1ab of ∼ 4.5 [29], ∼ 3.6 [38], or the later value ∼ 3.4 [57]. 3 In any case, it is clear that the spin-spin correlation factors in (3.3.17) are going to have to play a role in order to achieve quantitative consistency with experiment. Regarding (3.3.17), since K01 is a nearest-neighbor correlation it must be negative, while K12 and K13 are correlations between neighbors on the same “sublattice”, so to speak, so they will be positive and undoubtedly smaller in magnitude that K01 . Thus, K01 will have a clear eﬀect of increasing the ratio if its value is negative and appreciable. For example, if we neglect the K12,13 terms for the moment, then a value of K01 = -0.07 would yield a T1 ratio of 4. With only a modest amount of correlation we can obtain a realistic value for T1c /T1ab . Temperature-Dependent Spin-Spin Correlations It is not clear from the Mila-Rice presentation, either, whether they intended the correlations to be used as temperature-dependent parameters or not, but a number of subsequent developments have employed them in just that role. For example, temperature-varying correlations give a straightforward explanation for the variation found for the T1 anisotropy in YBCO7 between 100 K and 300 K [38]. These data are shown in Fig. 3.7, where it is seen that T1c /T1ab diminishes by barely 10% over that temperature interval, and is only barely outside of the error bars. Nonetheless, the trend persists over a series of data points and is clearly established.4 As we shall see in Chap. 5, extensive use has been made of the Kij ’s as temperature-dependent parameters to describe the behavior of T1 . In the Uldry-Meier T1 analysis, for example, the temperature dependence of all T1 ’s is described in terms of the spin-spin correlations and an eﬀective correlation time [58]. The theoretical basis for this approach is derived in Sect. 3.5. 3

4

The diﬀerence between these two measurements is outside of error estimates, and can only be attributed to a diﬀerence in samples. The lower numbers agree with earlier measurements made on a random powder [37]. It would have been desirable to have this eﬀect conﬁrmed by another experimental group. To our knowledge, no such conﬁrmation has been reported.

92

3 Preliminary Steps in Cuprate NMR 5

1.4

1.2 (θ = π/2)

4

3 0.8 (θ = 0) 0.6

2 63Cu

T1–1 (msec–1)

T1–1 (msec–1)

1.0

(2) 0.4

ν = 85 MHz 1

0.2

0

0

100

200 T (K)

300

Fig. 3.7. 1/T1ab (θ = π/2) and 1/T1c (θ = 0) are plotted vs. temperature over the range 90 K ≤ T ≤ 300 K for Cu(2) sites in an oriented powder sample of fully oxygenated YBCO7 [38]. The data are scaled so that T1 values for the two orientations coincide at T = 100 K, so as to highlight the decrease of the T1c /T1ab ratio over range of T measured. Reprinted ﬁgure from R.E. Walstedt, W.W. Warren, Jr., et al: Phys. Rev. B40, 2572 (1989). Copyright 1989 American Physical Society

Meanwhile, we also recall that the ﬁrst Mila-Rice paper [2] made no attempt to apply their model to the interpretation of the peculiar temperature dependence of the T1 data. Indeed, theories addressing the behavior of T1 (T ) were fairly quick to follow, but are still under discussion, as will be seen in Chap. 5.

3.4 Incorporating 17 O and 89 Y data into the Mila-Rice-Shastry Picture Following the Mila-Rice (MR) paper there were many new developments, some going beyond the scope of the present chapter. There were new data on 17 O NMR in YBCO, as well as a great deal of discussion regarding the question of a two-ﬂuid picture of quasiparticle dynamics, i.e. whether there is evidence for a separate hole band on the oxygen sites. There were also eﬀorts to treat

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

93

the temperature dependence of the copper T1 , along with discussion of just how the Cu(1) chain sites in YBCO diﬀer from the Cu(2). In the midst of these many challenging questions and almost immediately following Mila and Rice, reports on the peculiar behavior of the oxygen-deﬁcient phases made a sudden appearance. These eﬀects, known collectively as the pseudogap and their interesting history in the high-Tc ﬁeld are the subject of Chap. 4. We consider here the ﬁrst reports on the behavior of the planar 17 O NMR, as well as the closely related 89 Y. Detailed theories which address the contrasting behavior of 63,65 Cu, 17 O, and 89 Y in YBCO are presented in Chap. 5. Following the discussion of the 17 O data for YBCO7, we consider again the possible occurrence of oxygen hole bands along with the Cu2+ -related (ZhangRice) quasiparticles in the total picture of fermion dynamics. 17

O(2,3) NMR Data and Interpretation for YBCO7

By the middle of 1989, 17 O NMR studies on YBCO7 had been reported by several groups [59, 60, 61, 62]. Here we shall review and discuss the results reported by Takigawa, Hammel et al. [59, 60] in some detail. A comparable set of results was reported by Horvati´c et al. [61], covering a wider range of temperatures. The high temperature results for the quadrupolar and shift tensors for the O(2,3) sites from the latter study were found to agree within error bars with those from [59], and the quadrupolar data from [62] are also in accord. The HF tensor is analyzed below and compared with the MR model calculation. There is some disagreement in detail, but this, we suggest, may arise from inaccuracies in the MR quantum chemistry results. 17 O spectra were taken on oriented powder samples of YBCO7 [59], for which 17 O-enriched oxygen gas was used to exchange 17 O into the sample material at a temperature of 900◦ C. The resulting (nearly) complete NMR spectrum for all of the oxygen sites is shown in Fig. 3.8 for the case of ﬁeld oriented along the c axis. The identiﬁcation of all the peaks in this spectrum is a real tour-de-force of NMR shift and quadrupole splitting analysis. Although the c axis is expected to be one of the principal axes of the EFG tensors for each oxygen site, the EFG tensors are decidedly non–axial in character. The peaks have been ﬁtted using the I = 52 second-order perturbation formulas [59] 1 1 2 − ↔ (3.4.1a) : Δν = ν0 Kz + (νx − νy )2 /ν0 , 2 2 9 5 1 3 (3.4.1b) ± ↔± : Δν = ν0 Kz ± νz + (νx − νy )2 /ν0 , 2 2 36 5 1 3 (3.4.1c) ± ↔± : Δν = ν0 Kz ± 2νz − (νx − νy )2 /ν0 , 2 2 9 where ν0 = γn Hres and Δν = νres - ν0 . The NMR frequency is νres , and Hres is the value of the ﬁeld at the peak in question. The quantities νx,y,z are quadrupole frequency parameters deﬁned as να = 3eQ 20 Vαα . Equation (3.4.1a)

94

3 Preliminary Steps in Cuprate NMR

SPIN ECHO INTENSITY

A0, A1, A2 : O (1) B0 – B4 B1´ – B´4 : O (2), O (3)

νres / γ

N

C0, C1, C2 : O (4) B0 B´3

B3

B2

B1

B4

B´1

C1

B´2

B´4

C2 A2

C0

A1 A0 × 7.2 84

× 7.2 85

× 4.5

×1

× 2.6

86

× 5.1 87

× 7.2 88

MAGNETIC FIELD (kOe)

Fig. 3.8. 17 O NMR spectrum taken at 49.8 MHz on an oriented powder sample of YBCO7 with enriched 17 O content [59]. The ﬁeld was oriented along the c axis. Sample temperature was 160 K. For 17 O γn /2π was taken to be 0.577186 kHz/Oe. The sites were identiﬁed as labelled, with the (Bn , Bn ) pairs of lines very close together for the O(2,3) sites. See text for discussion of the quadrupolar and shift tensors for the O(2,3) sites. Reprinted ﬁgure from M. Takigawa, P.C. Hammel, et al: Phys. Rev. Lett. 63, 1865 (1989). Copyright 1989 American Physical Society

will be recognized as (2.1.3) written out with Vαα parameters. Note that no relative size or sign relationship is implied here among the νx,y,z , except, of course, that α να = 0. The parameters are adjusted for each site so as to give a best ﬁt to the spectrum shown, as well as spectra taken with H ⊥ the c axis, an exercise of considerable complexity. For the case of the O(2,3) sites, it was not clear from the data alone whether the principal axis of the EFG was along the c axis or along the bond axis. To decide this, trial calculations of the EFG tensor were made assuming a point-charge contribution multiplied by a Sternheimer factor (1 − γ∞ ) [63], where γ∞ was taken to be 9, plus an on-site p-electron contribution of 3 ( 20 )( 45 e2 |Q| r−3 , where r−3 was taken to be 3.63 a.u. [59]. On this basis, the only reasonable outcome was obtained assuming the principal axis is the bond axis, giving an estimated result (0.97, −0.42, −0.55) MHz as compared with (0.976, −0.598, −0.378) MHz shown in Table 3.5. Note that the transverse axis values are reversed between modeling and experiment, so that the ﬁt is close, but not exact. The principal EFG values for all sites lie along the bond axes. Our interest in the shift data shown in the table is in comparing them with the results calculated by MR, and ultimately to see whether the 17 O data are compatible with a single-ﬂuid description of the distribution of electronic

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

95

(i.e. hole) spin density. Shift values are given for all sites at two temperatures, 160 K and 30 K. In the latter case, we suppose that the spin susceptibility is essentially zero (see e.g. shift measurements for T < Tc in [41, 48]), so that these residual values may be regarded as orbital shifts. This surmise is veriﬁed by a detailed plot of Kc (T ) vs. T by Horvati´c et al., (see Fig. 4 in [61]). Subtracting the 30 K shift values from the 160 K ones, we ﬁnd estimates of the spin paramagnetic shift components, listed under “Ks (160 K)”. The latter values form a tensor for each site, which has been divided into an isotropic component Kiso = (K + 2K⊥ )/3 and an anisotropic (axial) component with Kax = (K − K⊥ )/3. The latter parameters are tabulated in the ﬁnal two columns. It is seen for the O(2,3) that there is a fairly large isotropic component as expected, with quite a sizeable axial shift Kax = 0.03% as well. It seems that the main hybridization is into the 2pσ orbitals as expected. On the other hand, the MR quantum chemistry calculation predicted a rather smaller value for Kax than what was found. We analyze this point by noting that the axial shift coeﬃcient for a pσ orbital occupied with a fraction f of the S = 12 moment is given by αax = 25 f r−3 /NA . According to the MR quantum chemistry (Sect. 3.3), f = α2p /2 = 0.058. Using the value

r−3 = 3.63 a.u. [59], we ﬁnd ασ = 0.94(emu/mole)−1. With a transverse susceptibility component of 1.01 × 10−4 (emu/mole Cu(2)) (Table 3.4), we ﬁnd Kax (MR) 0.0095%. This is approximately 1/3 the experimental value in Table 3.5. So although the experimental value has a large error bar, it is certainly much larger than the MR calculated value. Is this evidence for an oxygen hole band? We think not, but unfortunately, there is no trend with doping or even temperature dependence to check such a hypothesis. However, there is another experimental number which comes to mind here, namely the determination of the covalency of La2 CuO4 at high Table 3.5. Experimental quadrupolar tensors and shift data from spectra such as Fig. 3.8 are shown at two temperatures in the left-hand columns, followed by deduced spin components, which are then broken down into isotropic and axial parts [59]. The 30 K values are taken to be of purely orbital origin. Site and orientation labels are shown at the far left. Frequencies are given in MHz and shifts in % Site

Axis να

Kα (160 K) Kα (30 K) Ks (160 K) Ks (iso) Ks (ax)

O(1)

⊥ c -0.484 ⊥ c 1.629 c -1.145

0.23 0.22 0.24

... 0.13(1) 0.13(3)

... 0.09(1) 0.11(3)

0.10(1) 0.01(1)

O(2,3) ⊥ c (0.986,0.966) 0.31 ⊥ c -0.598 0.17 c (-0.389,-0.369) 0.18

0.05(1) 0.01(1) 0.02(3)

0.26(1) 0.16(1) 0.16(1)

0.19(1) 0.03(1)

-0.01(1) 0.04(1) 0.03(1)

-0.01(1) -0.01(1) 0.05(1)

0.01(1) 0.02(1)

O(4)

⊥ c -0.375 ⊥ c -0.721 c 1.096

-0.02 0.03 0.08

96

3 Preliminary Steps in Cuprate NMR

temperatures using 17 O NMR shift measurements [13]. The total fraction of spin density residing on the O(2,3) with the MR result (foregoing paragraph) is 2f = 11.6%. The comparable experimental result for La2 CuO4 is 31% [13]. Scaling the foregoing estimate by the ratio of these numbers, one ﬁnds a result nearly a factor of 3 larger and in much better agreement with the O(2,3) axial shift in Table 3.5. The La2 CuO4 measurement is also in good agreement with, but actually slightly less than theoretical values given by H¨ usser, et al. [14]. We suggest that the value for La2 CuO4 should not be very diﬀerent from that for YBCO7. Thus, it is possible that the expected number for the 2pσ spin density is quite a bit larger than the MR value, and that the reported 17 O(2, 3) shift values in [59] are consistent with a one-band picture. HF Tensors for

17

O(2,3) and

89

Y in YBCO7

In Table 3.6 we collect data for the 17 O(2,3) and 89 Y NMR shift tensors and list the corresponding HF tensors deﬁned in (3.3.2) and (3.3.4). For the 17 O(2,3) case we take NMR shift data from Table 3.5. For the 89 Y case the data are taken from Alloul et al. [64], which reports the highest numbers available for an oriented powder sample5 . The HF tensors are then obtained with (3.3.4) using the spin susceptibilities in Table 3.4. The HF constants for the various sites in and near the CuO2 in Tables 3.4 and 3.6 are expected to hold for reduced oxygen phases of YBCO7-x as well. A very important test of this idea occurs in Chap. 4, where these values are compared with precisely determined relative values for the YBCO6.63 phase. Table 3.6. Spin components of NMR shift are tabulated for the 17 O(2,3) and 89 Y, 17 Ksα and 89 Ksα , respectively, for YBCO7 at T = 100 K. See text for the source of these data. The corresponding HF tensors obtained with (3.3.4) are also listed, along with the susceptibility tensor from Table 3.4. Note that for the 89 Y case the denominator in (3.3.4) is “8” rather than “2”. Cα and Dα are given in kOe/μB and χsα in 10−4 (emu/mole) Axis a b c

5

17

Kα (%)

0.26(1) 0.16(1) 0.16(1)

89

Kα (ppm) Cα

247 247 315

Dα

χsα (100 K)

72(3) 1.71(9) 1.01 44(2) 1.71(9) 1.01 38(2) 1.86(9) 1.18

We take larger numbers for the 89 Y NMR shift at 100 K to be a sign of full oxygenation. Moreover, the plot reported for 89 Kα (T ) vs. T [64] shows a gradual increase from 300 K down to a maximum at T ∼ 120 K. This is a characteristic of a fully oxygenated sample as well [47], rather than declining curves which then give smaller values of 89 Kα at T = 100 K [65].

3.4 Incorporating

17

O and

89

Y data into the Mila-Rice-Shastry Picture

3.4.1 Measurements of T1 for

17

97

O in YBCO7

The foregoing authors also reported T1 measurements for various oxygen sites in YBCO7 [60]. As found earlier for the 89 Y [22, 23], the 17 O(2,3) relaxation in the normal state is very Korringa-like, with T1 T 2.7 sK. The authors chose to give a qualitative discussion of this result, along with their 63 Cu(2) data, in terms of the Korringa relation (1.2.8). Following that, however, they discuss the T1 results in terms of the dynamic susceptibility χ (q, ω), which became the method of choice for analyzing relaxation data. In the following sect. (3.5) we present for reference purposes a derivation of the relaxation rates for 89 Y, 17 O(2,3), and 63 Cu(2) in YBCO in terms of χ (q, ω). We shall use formulas given there for our present discussion of data from [60]. First, let us consider the simple Korringa relation (2.2.8) in relation to the current problem. One could hardly expect it to apply in any strict fashion to YBCO, owing to unknown particle dynamics, q-dependent HF coupling tensors, etc. Nonetheless, it does serve a sort of qualitative purpose in comparing the behavior of diﬀerent nuclear sites. The 89 Y and 17 O(2,3) T1 processes are at least Korringa-like in their temperature dependence, though this may be somewhat illusory because of spin-spin correlation effects. Nonetheless, if you take the isotropic shift value from Table 3.5, you ﬁnd for 17 O(2,3) 4πkB γn2 1 1.4 × . (3.4.2) Ks (iso)2 T1 T γe2 To compare the latter result with the Cu(2) site they used T1ab , because it relates to the largest on-site HF term Ac = -221 kOe/μB . Since Aab is very small, however, they divided the expression (3.4.2) by two,6 ﬁnding a multiplier of 11 for the Cu(2) Korringa product. So there is a very clear enhancement of the Cu(2) relaxation, with almost none for the O(2,3). If we look at the q-dependent expressions for 1/T1 in Sect. 3.5, the Cu(2) expression for the ﬁeld ⊥ c axis, it is essentially independent of q, whereas for both the 89 Y and 17 O(2,3) cases, the integrand vanishes at QAF = (π/a, π/a). If χ (q, ω) has an AFM enhancement peak, the Cu(2) rate will receive full enhancement, but the 89 Y and 17 O(2,3) will have little or none. This is the explanation oﬀered in [60] for the discrepancy in Korringa ratios which they ﬁnd, but has been put forward by many other observers as well [66]. It was also generally thought to be related to the peculiar temperature dependence of the Cu(2) relaxation rate while the 89 Y and 17 O(2,3) rates were Korringalike. Reference [60] also presented data on relaxation rates for T < Tc for YBCO7, but discussion of those results will be combined with consideration of the Cu(2) data in Sect. 3.6. 6

Thus, only one axis is eﬀectively contributing to the T1 rate.

98

3 Preliminary Steps in Cuprate NMR

3.4.2 The One-Band, Two-Band Debate: in YBCO

89

Y and

17

O(2,3) NMR

The MR model theory purported to explain the Cu(1,2) NMR (in YBCO7) behavior at 100 K with a single spin ﬂuid, where all HF couplings were assumed to originate with the S = 1/2 coupled moments on the Cu2+ sites. At the same time or slightly later, other interpretive papers appeared as well as experimental papers with more data on the 89 Y and 17 O NMR shift and relaxation properties. In this subsection we consider arguments presented on the question of one quantum ﬂuid vs. two separate ﬂuids needed to account for the T1 data. Monien, Pines, and Slichter [67] presented an analysis similar to MR, including the transferred HF term for the Cu(2) sites, but also considering a possible “oxygen hole band” characterized by susceptibility χh as well as a Cu(2) HF coupling Ah . In similar fashion to Sect. 3.3, they concluded that the one-ﬂuid model could not explain the data unless there were spin-spin correlations. However, they also pointed out the possibility that the (χh , Ah ) oxygen band, if present, could be the explanation. The question was how to decide whether the hole band was necessary. A substantive discussion of this point was given by Mila and Rice themselves in a follow-up paper [46]. We shall brieﬂy recap their main points here. First, they note that while one could consider the possibility of a hole band on the O(2,3) sites, the Zhang-Rice singlet picture essentially rules this out, since the singlets are magnetically inert 7 . Thus, one would expect that HF parameters should not depend on the doping level. In this connection they noted that in the large 89 Y study by Alloul et al. [65], the slope of K vs. χ plots is invariant from full doping all the way down into the insulating regime. Thus, the 89 Y HF coupling is independent of doping, consistent with the Zhang-Rice singlet picture. Next, they consider what one would expect if there actually were a hole band. On the basis of quantum chemistry, MR argue that such a hole band would have a much stronger HF coupling with the 89 Y nuclei than the Cu2+ moments have. The reasoning is as follows. First, the Cu2+ are too far from the 89 Y for direct coupling, and for the (strongly) hybridized 2pσ orbitals on the O(2,3), the MR Wannier wavefunction (3.3.9) has the wrong symmetry to couple to the Y s or d orbitals. The answer, they suggest, is a possible double hybridization path through 2pπ orbitals to the Y 4d. This is, of course, very weak, and they argue that any hole band which occupies either the 2pσ or 2pπ orbitals will have hybridization at least 5 times larger. Because of this, the 89 Y HF parameter in such a case would vary sharply with hole concentration. Since it does not, they conclude that an oxygen hole band is essentially ruled out. 7

There were, however, two-band models proposed at the time, such as that given by Emery and Reiter [68].

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

99

There was further discussion of oxygen bands in a few additional papers [48, 5], but no really cogent evidence conﬁrming their existence. In Chap. 5 a discussion is presented of several models for calculation and interpretation of T1 data for various nuclear species in the YBCO family of compounds. With the development of various theoretical models and schemes for interpretation of relaxation eﬀects, there seemed less and less motivation to include oxygen hole bands. There was no evidence to support their suggested existence once it was realized that q–dependence susceptibilities and HF couplings could account for the observed behavior. There, however, we shall also reconsider the possibility of an orbital relaxation term (see Sect. 5.6).

3.5 Formulation of T1 in Terms of χ(q, ω) and q-Dependent HF Couplings Even though transferred HF couplings quite obviously underlie the shift and relaxation eﬀects of the 89 Y nuclei in YBCO [22, 23, 35, 36], their presence – and the concomitant eﬀects of antiferromagnetic (AFM) spin-spin correlations – were brought to our attention by the MR [2] analysis. However, the spin-spin correlation picture was not destined to become the language of choice for this problem, but rather that of the well-known dynamical susceptibility χ(q, ω) [69, 70]. While these pictures are, as will be seen below, completely equivalent, the q–space methodology is perhaps a bit more convenient, as well as tying in directly with INS measurements. While the potential of this approach to distinguish the behavior of 63,65 Cu, 17 O, and 89 Y in YBCO was noted early on [34], its dramatic consequence of cancelling AFM ﬂuctuations at the planar oxygen was ﬁrst articulated by the analysis of Shastry [3]. Subsequently, it has been widely invoked for discussion of T1 eﬀects [6, 7, 46, 60, 66, 71]. 3.5.1 Derivation of Dynamical Susceptibility T1 Equation The formula for T1 in terms of χ (q, ω) and q-dependent HF couplings is widely quoted. For reference, we give here a simple derivation of this result, starting from the master equation for the interaction representation density matrix for nuclear spins ρ∗ (t) [72], ∞ dρ∗ =− dτ [H1∗ (t), [H1∗ (t − τ ), ρ∗ (t)]], (3.5.1) dt 0 where H1 is the spin-lattice interaction being treated here as a perturbation, and the overline represents an average over t which is long compared with the correlation time scale of τ , but short compared with the time for the nuclear spin polarization to change. The star indicates operators which have been transformed into the interaction representation as in O∗ (t) = exp(i(F + H0 )t)O exp(−i(F + H0 )t), where H0 is the unperturbed nuclear

100

3 Preliminary Steps in Cuprate NMR

spin Hamiltonian, and F is the Hamiltonian for the rest of the dynamical variables in the system. Here, for simplicity we take H0 to be a Zeeman term with a ﬁeld H applied along the cartesian axis labelled α, H0 = −ω0 Iαi , (3.5.2) i

where ω0 = γn H. The densitymatrix for spin-lattice relaxation in such a case is simply ρ∗ (t) = ρ(t) = a(t) i Iαi , where a(t) is a variable which represents the changing nuclear magnetization during a T1 experiment. We illustate the q-dependent HF coupling eﬀects with H1 for the Cu(2) sites, Ijβ Aα Sjβ + B Skβ , (3.5.3) H1 = j,β

k=nn

where the B term is an isotropic coupling between I j and the four nn spins Sk to the j site. It will simplify the procedure if we neglect the imaginary part of the time factors exp(±iω0 t) which occur for each of the operators Ijβ in the interaction representation, and simply represent them as a factor cosω0 τ times the correlation functions. The correlation functions are assumed to be even in the variable τ , and the sinω0 τ terms will always vanish in the applications considered here. A second simpliﬁcation occurs if we operate on both sides of (3.5.1) with T r(Iiα ...). Since the spin correlation functions are even functions of τ so that Sjβ (t)Skβ (t + τ ) = Sjβ (t + τ )Skβ (t), we may write (3.5.1), in part, as (N)

a−1

da =− dt i

∞ 0

dτ cosω0 τ [Ax Six (t) + B

Skx (t)][Ax Six (t + τ ) + B

k=nn

Skx (t + τ )], (3.5.4)

k=nn

where we are displaying only the x axis ﬂuctuation term as an example. The next step is to Fourier transform the spin operators with Siβ (t) =

(N )

eiq·ri Sq (t) , β = x, y, z,

(3.5.5)

q

(N ) where the summations are normalized so that q exp[iq · (r − r i )] = δr,ri , etc. In (3.5.5) Sq (t) is deﬁned to be an isotropic, q-dependent spin ﬂuctuation operator. Using (3.5.5) in both factors in (3.5.4) and noting that (N ) exp[i(q + q ) · ri ] = δq,−q , (3.5.4) becomes i a

−1 da

dt

= −

(N ) q

2

Ax (q)

∞

dτ Sq (t)S−q (t + τ )cosω0 τ, 0

(3.5.6)

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

101

where Ax (q) = [Ax + 2B(cos(qx a) + cos(qy a)]. In (3.5.6) the Ax (q) are in circular frequency units per unit of spin. We now proceed to replace the time average with an ensemble average ∞ ∞ dτ Sq (t)S−q (t + τ ) cos ω0 τ = dτ Sq (0)Sq (τ )Ens cos ω0 τ = S(q, ω0 ), 0

0

(3.5.7) where we have also assumed that Sq (t) has inversion symmetry. The quantity on the far right of (3.5.7) is known as the dynamical structure factor. 3.5.2 The Fluctuation-Dissipation Theorem The dynamical structure factor may be related to χ(q, ω0 ) using the ﬂuctuationdissipation theorem [4], which says (eω0 β − 1) S(q, ω0 ), (3.5.8) eω0 β where β = 1/kB T and we note that ω0 β 1. The subscript “s” is a reminder that the spin-only susceptibility deﬁned by (3.5.8) has a dimension of inverse energy. Inserting this into (3.5.6) and combining terms for x and y-axis ﬂuctuations yields for −a−1 da/dt, Im [χs (q, ω0 )] = χs (q, ω0 ) =

(N ) γ 2 kB T 1 = Aξ (q)2 χξ (q, ω0 )/(gξ2 ω0 ). T1α μ2B q

(3.5.9)

ξ

The latter expression for 1/T1α uses Aξ (q) in Gauss per unit of spin (see Sect. 2.3.1) and a conventional susceptibility per formula unit of CuO2 . The sum on ξ is over the two directions normal to α. Next, we introduce a convenient simpliﬁcation. One could use (3.5.9) by absorbing the g-factor denominator into the HF coeﬃcients and work with the primed coeﬃcients via (3.3.4). Following Auler et al., [73], we ﬁnd it more convenient to deﬁne an isotropic susceptibility via χiso (q, ω) = 4 χξ (q, ω)/gξ2 , whereupon (3.5.9) becomes (N ) γ 2 kB T 1 = Aξ (q)2 χiso (q, ω0 )/ω0 . T1α 4 μ2B q

(3.5.10)

ξ

In this way only the natural anisotropy of the HF couplings from (3.3.2) comes into the T1 formula. We now present expressions for 1/T1 for the various nuclear species in YBCO, using the HF tensors developed in the text. For the c axis relaxation of Cu(2), Aξ = Aab , for both terms, so (3.5.9) becomes (N ) 1 γ 2 kB T = [Aab + 2B (cos qx a + cos qy a)]2 χiso (q, ω0 )/ω0 , T1c Cu(2) 2 μ2B q (3.5.11)

102

3 Preliminary Steps in Cuprate NMR

where the susceptibility is per CuO2 . For the ﬁeld in the ab plane, we have 1 T1ab

= Cu(2)

(N ) 1 γ 2 kB T + [Ac + 2B (cos qx a + cos qy a)]2 2T1c Cu(2) 4 μ2B q χiso (q, ω0 )/ω0 .

(3.5.12)

However, for the Cu(2) HF couplings given in Table 3.4, Ac is the dominant term, so that for 1/T1ab the contribution of 1/2T1c is essentially negligible. Unless the correlations are known to be large, a good estimate can be obtained by dropping the “B” term as well, so that the HF coupling becomes essentially independent of q. For the planar oxygen sites and the yttrium sites in YBCO the HF couplings are dominated by hybridization eﬀects with the 2s [3] and 4d [35] holes, giving HF coupling terms AO,ξ (q) = 2Cξ cos qx a/2 and AY,ξ (q) = 8Dξ cos qx a/2 cos qy a/2, (3.5.13) respectively, where it is noted that the HF coupling for the Y3+ is thought to be dominated by the 4d core-polarization HF ﬁeld [35]. The corresponding expression for the 17 O relaxation rate is, e.g., (N ) 1 γ 2 kB T 2 = [C (1 + cos qy a) + Cy2 (1 + cos qx a)]χiso (q, ω0 )/ω0 , T1c O 2 μ2B q x (3.5.14) where T1 along other axes is analogous to the case for Cu(2). For the case of 89 Y, we give here an expression in which interplanar correlations are neglected. Thus, (N ) 1 4γ 2 kB T 2 = [Dx + Dy2 ](1 + cosqx a)(1 + cosqy a)χiso (q, ω0 )/ω0 . T1c Y μ2B q (3.5.15) Kij and Xat Expressed in Terms of χ (q, ω) Dynamical AFM spin-spin correlation eﬀects in these relaxation processes are embodied in the factors such as (1 + cos qx,y a), the mean value of which will approach zero in the event of strong correlations. Such correlation factors were introduced by Mila and Rice [2], where in Sect. 3.3 they took the form Kij = 4 Siα Sjα . It is useful to introduce an equivalent deﬁnition of the Kij in terms of χ (q, ω). For example, the sum on q in (3.5.14) can be put into the form (N ) [ ] = [Cx2 + Cy2 ][1 + K01 ]Xat , (3.5.16) q

3.5 Formulation of T1 in Terms of χ (q, ω) and q-Dependent HF Couplings

103

where Xat =

(N ) χ (q, ω0 ) is

ω0

q

and K01 =

(N ) 1 χ (q, ω0 ) cos kx,y a is . Xat q ω0

(3.5.17)

The quantity Xat (T ) is a fundamental dynamical index for χis (q, ω) at low frequencies. It contains the basic correlation time for the spin ﬂuctuations. Furthermore, the quantity (kB T )/μ2B )Xat ∼ kB T N (0)2 gives the correlation time along with the statistical weight of the T1 process, where N (0) is the density of states/atom at the Fermi surface for one direction of spin in an energy band environment. The other factor (1 + K01 (T )) gives the temperature variation of T1 arising from dynamical correlations for the case of transferred HF interactions. Equation (3.5.16) therefore eﬀects a separation of these two fundamental – and physically very diﬀerent – factors in the temperature dependence of T1 . To complete the picture of spin–spin correlations used for the YBCO family of compounds, we have, in analogy with (3.5.17), K12

(N ) 1 χ (q, ω0 ) = cos kx a cos ky a iso and Xat q ω0

K13 =

(N ) 1 χ (q, ω0 ) cos 2kx,y a iso . Xat q ω0

(3.5.18)

We may now introduce these forms into the T1 expressions (3.5.11)– (3.5.15). As an example we consider the expression (3.5.11), where the HF coeﬃcient factor [ ]2 may be expanded as A2α + 4B 2 + 2B 2 (cos 2qx a + cos 2qy a) + 8B 2 cos qx a cos qy a (3.5.19) + 4Aα B (cos qx a + cosqy a). Using the deﬁnitions (3.5.17) and (3.5.18), the expression for 1/T1 becomes 2 γ63 kB T 1 = Xat {A2ab + 4B 2 [1 + 2 K12 + K13 ] + 8Aab BK01 }, (3.5.20) T1c Cu(2) 2 μ2B where we recognize the same expression for the HF constants and correlation functions as in (3.3.14) and (3.3.15). Expressions such as (3.5.20) give a more direct idea of the dependence of T1 on the spin-spin correlations than expressions given earlier in terms of χ (q, ω). The corresponding equations for 17 O(2,3) and 89 Y are γ 2 kB T 1 = 17 2 Xat [Cx2 + Cy2 ][1 + K01 ], (3.5.21) T1z O 2 μB

104

and

3 Preliminary Steps in Cuprate NMR

2 1 kB T 4 γ89 = Xat [Dx2 + Dy2 ][1 + 2K01 + K12 ], T1z Y μ2B

(3.5.22)

for any permutation of axes (x,y,z). Equations (3.5.20), (3.5.21), and (3.5.22) are quite general and are useful for discussing cases where Xat (T ) and the Kij (T )’s are both changing substantially with temperature. The formulation of T1 in terms of Xat and the Kij ’s described here is the theoretical basis for the comprehensive T1 data interpretation scheme pioneered by Uldry and Meier [58], which is discussed in Chap. 5.

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc Following Mila and Rice, a number of relaxation model calculations were developed which made use of the random phase approximation (RPA) to include the eﬀects of electron–electron interactions. Several of these model calculations are reviewed in Chap. 5, as well as a proposed orbital relaxation term for the 63 Cu(2) based on the marginal Fermi liquid hypothesis [74]. Among the RPA schemes which appeared early on was an interacting Fermi liquid theory with strong AFM exchange couplings put forward by Monien and Pines (MP) [5], where they used the RPA to construct a model for χ (q, ω) with an adjustable enhancement level in the vicinity of QAF . An important innovation in this work was the introduction of an energy gap with d-wave symmetry for T1 and NMR shift calculations for T < Tc . Even though there were theoretical developments from very early on suggesting the suitability of d-wave superconductivity for the cuprates [75, 76, 77], up to this point no one had tried to interpret NMR data with the d-wave picture. In spite of the apparent success of this interpretation as seen in [5], widespread acceptance of d-wave symmetry did not occur until the dramatic conﬁrmation of d-wave superconductivity in the cuprates by means of phase jumps at Josephson junction boundaries, which was still several years away [78, 79]. The NMR modeling described here followed closely upon a successful application of d-wave theory to Raman scattering experiments [80]. The RPA theory of [5] was applied to giving a realistic account of the shift and of T1 vs. T at the Cu sites in YBCO7 for T < Tc . This ﬁrst NMR test of dwave calculations was an important step along the path of eventual adoption of the singlet d-wave interpretation of cuprate superconductivity. By this point in time, there was ample T1 data below Tc on which to apply calculations such as this. As we shall see, however, both the theoretical details and some of the data were destined to undergo revision in later years. Nonetheless, these preliminary exercises in understanding the cuprate NMR data were both very encouraging and highly suggestive.

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

105

3.6.1 The NMR Shift Behavior for T < Tc To discuss the Cu(1,2) NMR shift below Tc , we must ﬁrst address the experimental situation. We therefore digress brieﬂy here to discuss the NMR shift measurements conducted by Takigawa et al., [81] and by Barrett et al., [48]. Both papers appear to be very careful pieces of work. The biggest problem involved in such measurements is accounting for the diamagnetic shift of the internal ﬁeld in the superconducting vortex state. This was dealt with in sharply contrasting ways in the two papers cited, leading, unfortunately, to slightly diﬀerent results. Here we suggest a compromise interpretation. Correcting for Diamagnetism via Magnetization In [81] the internal ﬁeld was corrected for using an eﬀective demagnetizing factor, which is applied to the measured magnetization of the oriented powder sample. The demagnetizing factor was determined with a careful calibration procedure, which is too lengthy to discuss here. However, the risk with such a procedure lies perhaps not in the demagnetizing factors, but in using magnetization measurements on a powder sample set in epoxy. There is a risk of non-intrinsic Curie-Weiss-like anomalies aﬀecting such a procedure. Indeed, the c-axis shift for Cu(2) has an upturn below ∼ 50K which we suggest may be spurious. This is shown in Fig. 3.9(a) where the Cu(2)site shift results are plotted with corrections. Interestingly, no such feature is found for the ab-plane result. This same kind of anisotropic Curie-Weiss background eﬀect was also reported later in an attempt to determine the intrinsic normal-state susceptibility of YBCO [50]. In the present case we note that the shift corrections become nearly 0.25% as T → 0. The size and temperature dependence of this eﬀect does not seem compatible with superconducting diamagnetism. Calibration of Internal Field with the

89

Y Shift

On the other hand, in [48] the 89 Y NMR line was used as a reference for the internal ﬁeld at low temperatures, which is a very sound method in principle, as long as the 89 Y NMR shift is reliably known. If, for example, the resonance frequencies ν63 and ν89 were measured in the same ﬁeld, then we have ⎧ ⎫ ν γ ⎩ 63 89 ⎪ ⎭ + KY − 1. (3.6.1) KCu = ⎪ ν89 γ63 In practice, KY −0.03% at T = 100 K, and it was assumed [48] that KY ∝ Ys (T ), Ys (T ) being the Yosida function [82] for s-wave gap symmetry. Since one may be looking here for a d-wave Yosida function eﬀect, the foregoing assumption may cause a problem, but in fact the diﬀerence is small enough to be within the error bars. The Cu(2) shift results are shown in Fig. 3.9(b) and (c). It is noteworthy that the maximum c-axis internal ﬁeld correction (for Ks (c)) is ∼ 0.05% or only ∼ 20% of that found at low T in Fig. 3.9(a).

106

3 Preliminary Steps in Cuprate NMR

Although the latter correction cannot be arbitrarily curtailed, it seems likely that it is primarily responsible for the discrepancy between the c-axis results. The ab-plane results are also slightly outside error bars [0.37(2)% for [81] and 0.30(2)% for [48]]. However, this diﬀerence is as much a result of disparate normal-state shifts as it is of low-T corrections, which are similar. We suggest the following composite picture based on the combined results of [81] and [48]. The c-axis result of [48] is to be accepted as is, which says that Ks (c) is negligibly small on the scale of Ks (ab). The axial and isotropic shifts thus behave in a very similar fashion, since they both reﬂect the behavior of Ks (ab). Thus, we suggest that the contrasting behaviors of Kax (T ) and Kiso (T ) highlighted in [81] may have been generated, in part, by subtracting and adding the strongly corrected c-axis shift, respectively. It is suggested that the sharp contrast which results is unreliable. On the other hand, the corrected Kab (T ) curve in Fig. 3.9(a) shows a very interesting linear-T behavior below 50 K which is clearly not a result of the correction process. This may therefore be a sign of d-wave symmetry behavior, as reﬂected in the MP interpretation below. The behavior of Kax (T ) in Fig. 3.9(b) and (c) is also compatible with d-wave, as we shall see below. Both of these papers considered the isotropic 1.5 χs(T)/χs(100)

1.0 →

1.0 Cu(2)

(a)

0.8

(b)

0.6 0.4 0.2 0.0

→

H⊥ cˆ

0.5

1.0

Ks Korb

0

0

100 T(K)

(c)

0.8

200

χs(T)/χs(100)

KNIGHT SHIFT (%)

H cˆ

0.6 0.4 0.2 0.0

–0.2

0.2 0.4 0.6 0.8 1.0 1.2 1.4 T/ Tc

Fig. 3.9. (a) Corrected and uncorrected NMR shift data for Cu(2) in YBCO7 from [81] are shown plotted as a function of temperature for ﬁeld parallel (top) and perpendicular (bottom) to the c axis. The correction scheme is described in the text. Figure reprinted from M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989). Copyright 1989 American Physical Society. In (b) and (c), Cu(2) NMR shift data for YBCO7, i.e. Ks (c) - Ks (ab) normalized to 1 at 100 K, are plotted vs. T /Tc [48]. Yosida function ﬁts to the data are shown using s-wave symmetry (b) and d-wave (d’-wave) symmetries (c) from Fig. 3.10(a) as a solid (dashed) line. Fit parameters are shown in Table 3.7 and discussed in the text. Figure reprinted from S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990). copyright 1990 American Physical Society

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

107

component of shift as heavily contaminated with “oxygen hole band” eﬀects. Following MR and MR2 [2, 46], we maintain their occurrence to be unlikely. 3.6.2 The Monien-Pines Calculations of NMR Shifts below Tc MP began by applying diﬀerent pairing symmetries to the interpretation of NMR shift variation below Tc . For comparison purposes they applied the pairing symmetries shown in Fig. 3.10(a). The pure s-wave and d-wave are ﬂat and ∝ cos φ, respectively, where φ is the azimuthal angle for the cylindrical 2D Fermi surface for the CuO2 planes. They argue in detail that triplet pairing states are inappropriate for this case [5]. Then, still concerned about the possibility of an oxygen hole band, following [81] they consider only the axial component of the shift, which they suggest would reﬂect only the spin paramagnetism of the Cu(2)2+ sites 8 The data which were ﬁtted are shown in Fig. 3.10(b) [81] and in Fig. 3.9(b) and (c). 1.2

(a)

s

1.0

Data of Takigawa et al.[4] d state d´ state

1.0 s´

0.8

0.8 0.6

s

Kax(2)

Δ /Δ max

d´

0.6 d

0.4

0.4 0.2 0.2 0

(a) 0

0

π/4 φ

(b)

π/2

–0.2

0

0.2

0.4

0.6 T / Tc

0.8

1.0

1.2

Fig. 3.10. (a) Gap energy variation for several choices of gap symmetry from [5] shown as a function of azimuthal angle φ over one quadrant. (b) Plot of Ks (ax) from [81] as a function of T /Tc (dots) for temperatures in the superconducting state. The solid and dashed lines are calculated ﬁts for gap functions labelled “d” and “d ” in the (a) portion [5], as described in the text. Noteworthy is the d-wave-like linear T behavior at the lowest temperatures. Figure reprinted from H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990). Copyright 1990 American Physical Society 8

The essential assumption here is that any oxygen hole-band NMR shift would be isotropic.

108

3 Preliminary Steps in Cuprate NMR

Calculating the Yosida Function To compare with NMR shift data, the Yosida function Y(T) is calculated using the weak-coupling BCS formula for an anisotropic, singlet superconductor, ∞ ⎧ ⎫ ∂f ⎪ ⎩− ⎭ N (E), (3.6.2) Y (T ) = dE ⎪ ∂E −∞ where N (E) is the density of states, and f is the Fermi distribution function. The behavior of Y (T ) for an s-state gap is Ys (T ) ∝ exp(−Δmin /kB T ) for T Tc , Δmin being the minimum gap energy as T → 0. In contrast, for the case of a d-state gap N (E) ∝ E for E Δ(0), leading to a linear variation of Yd (T ) with T for T Tc . MP used the maximum gap value Δ(0)/kB Tc and the speciﬁc heat jump at Tc ⎫ ⎧ ⎪ ∂Δ2 ⎪ ⎪ ΔC/C ∝ ⎪ (3.6.3) ⎭ ⎩ ∂T Tc as parameters for calculating Yd (T ), which is plotted in Fig. 3.10(b). The dwave result is seen to be in good agreement with the Cu(2)-site Kax data from [81]. Values of the parameters for the cases of (i) weak-coupling BCS theory and (ii), (3.6.2) ﬁtted to the NMR shift data in Fig. 3.10(b) and in Fig. 3.9(b) and (c), are given in Table 3.7. Strong coupling eﬀects are seen to be appreciable, but also, the d-wave calculation is quite successful in reproducing the linear temperature behavior of the shift data. 3.6.3 Calculating the Relaxation Decay Curve By ﬁtting the relaxation, the viability of using d-wave gap symmetry to interpret NMR data was tested BCS theory of T1 for the d-wave case. We begin Table 3.7. Table of ﬁtting parameters Δ0 /kB Tc and ΔC/C from [5] for the NMR shift data in Fig. 3.10(b) [81] (top part) and for the data in Fig. 3.9(b) and (c) (bottom). The values of these parameters for weak-coupling BCS theory are shown on the left-hand side for comparison. The pairing states shown in Fig. 3.10(a) were used for these calculations Data Plot

Weak Coupling Weak Coupling Optimal Fit Optimal Fit ΔC/C Δ0 /kB Tc ΔC/C Pairing State Δ0 /kB Tc

Fig. 3.10(b) d Fig. 3.10(b) d

2.13 1.93

0.95 1.17

2.44 1.74

1.97 2.36

Fig. Fig. Fig. Fig.

1.76 2.10 2.13 1.93

1.43 1.27 0.95 1.17

1.90 2.16 14.7 3.13

2.77 2.49 1.76 2.14

3.9(b) 3.9(b) 3.9(c) 3.9(c)

s s d d

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc

109

with a brief synopsis of the calculation of T1 [5]. In the presence of an AFM interaction Jef f (q, T ) the RPA expression for the dynamic susceptibility becomes χ0 (q, ω) , (3.6.4) χ(q, ω, T ) = 1 − N (0)Jef f (q, T )χ0 (q, ω) where χ0 (q, ω) is the ”bare spin-spin correlation function” [5]. For a T1 calculation such as (3.5.9) from the previous subsection, one only needs the imaginary or dissipative part χ (q, ω). Monien and Pines make the following approximations to treat T1 behavior below Tc . Assuming AFM enhancement eﬀects are large (such as for Cu(2) in YBCO), the enhancement denominator in (3.6.4) is ﬁrst replaced by its average, temperature-dependent value at QAF , so that (3.6.4) becomes

where

1 1 1 = , T1 (T1 )f ree [1 − λ(T )]2

(3.6.5)

λ(T ) = N (0)Jef f (QAF , T )χ0 (QAF , T ).

(3.6.6)

It was then further assumed that the real part of the dynamic susceptibility at QAF , χ0 (QAF , T ), scales with temperature like the noninteracting uniform susceptibility χ0 (q = 0, T ). T1 (3.6.5) can then be expressed in terms of the Yosida function (see Sect. 1.2.2)

as

Y (T ) = χ0 (q = 0, T )/χ0 (q = 0, Tc)

(3.6.7)

1 1 1 = , T1 (T1 )BCS [1 − λ(Tc )Y (T )]2

(3.6.8)

where 1/(T1 )BCS may be calculated for any pairing symmetry desired in the absence of quasiparticle interactions. In this simple approximation the falloﬀ of 1/T1 below Tc will be enhanced by the decline of the enhancement factor, which in turn falls oﬀ according to how the Yosida function diminishes below Tc . For other than s-wave gap symmetries, we may write the BCS relaxation expression (cf. Sect. 1.2.2) ∞ ⎧ ⎫ 1 ∂f ⎪ 2 ⎩− ⎭ [N (E) + M 2 (E)], ∝ dE ⎪ (3.6.9) (T1 T )BCS ∂E −∞ where N (E) and M (E), which account for the BCS coherence factor, are deﬁned by [83] N (E) =

⎧ ⎪ ⎪ Re ⎪ ⎩

⎫ ⎪ E ⎪ ⎪ ⎭ (E 2 − Δ2k )1/2

and M (E) = FS

⎧ ⎪ ⎪ Re ⎪ ⎩

⎫ ⎪ Δk ⎪ ⎪ . ⎭ (E 2 − Δ2k )1/2 FS (3.6.10)

110

3 Preliminary Steps in Cuprate NMR

The latter deﬁnitions allow for the possibility of a complex gap function. Combining (3.6.8) with (3.6.10) yields an expression for the relaxation rate which will decline below Tc , both because of the growth of the superconducting energy gap and because of the decline of the enhancement factor owing to the decrease in Y (T ). Because of the d-wave gap function described above, the linear-E density of states will lead to asymptotic 1/T1 ∝ T 3 behavior for T Tc . Application of MP T1 Calculations to Cu(2) Data for YBCO7 MP illustrated the above formalism by using it to ﬁt the NQR T1 data on Cu(2) in YBCO7 by Imai et al., [84]. The ﬁtting function is shown as a solid line in Fig. 3.11(a), and is seen to give an excellent representation of the data over two full orders of magnitude of the decline of 1/T1 below Tc . We make a number of remarks regarding this T1 ﬁt. First, for the d-wave gap function (see Fig. 3.10(a)), there is no vestige of the coherence peak, unlike what is found for the s-wave cases [5]. Moreover, the very steep decline found just below Tc can be achieved in two diﬀerent ways. This is illustrated by the ﬁt parameters shown in Table 3.8. The actual curve plotted in Fig. 3.11 does not allow the enhancement factor to change below Tc , for reasons to be discussed presently. As a consequence, a very large gap parameter of 5.12kB Tc is needed to cause the steep fall-oﬀ near Tc . However, MP have calculated another ﬁt curve for the data shown, corresponding to the second row of parameters in the table, which is almost indistinguishable from the ﬁrst ([5], Fig. 3(d)). In the latter case the enhancement parameter λ 0.5 (see ([5])) contributes to the decline of 1/T1 , but the gap parameter Δ0 /kB Tc = 2.44 is only half as great as for the calculation shown. This may be a more physically reasonable scenario. The corresponding (second row) parameters from Table 3.8 is in fact the same set used to ﬁt the shift data in Fig. 3.9(c). Referring to Fig. 3.11(b), the solid dots plot the same data as in the (a) panel. There we compare the decline of 1/T1 with a line of slope ∝ T 3 in the middle region and a linear T curve at the lowest temperatures. The ∝ T 3 behavior is expected at low T as mentioned earlier, because of the 63

Table 3.8. Table of ﬁtting parameters for the T1 data of Fig. 3.11(a) using a d-wave gap function [5]. The top line shows parameter values for a ﬁt assuming a constant enhancement below Tc . In this case the eﬀective value of λ is zero. The second line shows an essentially equivalent ﬁt in which λ is allowed to decay below Tc according to the d-wave Yosida function. The remaining parameters are those used to ﬁt the NMR shift data, as shown in Fig. 3.9(c) Weak Coupling Weak Coupling Optimal Fit Optimal Fit ΔC/C Δ0 /kB Tc ΔC/C λ(Tc ) Δ0 /kB Tc 2.13 2.13

0.95 0.95

5.12 2.44

1.89 1.97

0.0 0.5

3.6 A d-Wave Model for the NMR Shift and T1 at T < Tc 10

10

(a) YBCO7

(b) YBCO7 1

1/ T1 (ms–1)

1

1/ T1 (ms–1)

111

0.1

0.01

0.1

∝T3

NMR 0.01 0.001

0.001 0.0001 0.1

MP Fit

NQR 0.0001

1 T/ Tc

10

0.00001

∝T 1

10

100

1000

T(K)

Fig. 3.11. (a) NQR T1 data for Cu(2) in YBCO [84] is plotted vs. T /Tc for temperatures above and below Tc . The MP theoretical ﬁt described in the text is shown as a solid line. Figure reprinted from H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990). copyright 1990 American Physical Society (b) The same data as in part (a) are plotted as dots on a scale of absolute temperature. Also plotted for comparison are a set of NMR data (open squares) for the same nominal compound taken in a ﬁeld of 7.4 T [60]. For the NQR data the regions of data which vary as T 3 and as T are indicated with straight lines (see text for discussion). Figure reprinted from P.C. Hammel, M. Takigawa et al., Phys. Rev. Lett. 63. 1992 (1989). Copyright 1989 American Physical Society

linear-E character of N (E) which results from the d-wave gap having a line of nodes. Further, the suggested crossover to linear T behavior often results from disorder in the sample causing quasiparticle states to occur in the gap region. The progression of T 3 → T behavior has been found to occur below Tc in many non-cuprate unconventional superconductors. A few cases we could mention are 115 In in CeIrIn5 [85], 69 Ga in PuCoGa5 [86], 69 Ga in PuRhGa5 [87], and 23 Na in Na0.35 CoO2 ·yH2 O [88]. Does AFM Enhancement Decay Below Tc ? Next, we discuss the diﬀerence between the NMR and NQR data shown in Fig. 3.11(b). Along with the NMR data shown, Hammel et al., also reported a T1 curve for the (planar) O(2,3) sites over the same temperature range. Their NMR data for the Cu(2) and the O(2,3) created something of a sensation when the variation below Tc turned out to be precisely the same for these two nuclei over two decades. In terms of the MP theory outlined above the implication is that even though the Cu(2) undergoes substantial enhancement in the normal state, any such enhancement becomes temperature independent below Tc . This was taken to be a constraint on the theory, and is the reason

112

3 Preliminary Steps in Cuprate NMR

why MP calculated the solid curve ﬁt in Fig. 3.11(a) without allowing the enhancement to vary with temperature. However, the contrast between the NQR and NMR measurements suggests very strongly that there is an additional T1 mechanism operating in a high magnetic ﬁeld. Detailed studies which came later showed this to be the case, namely relaxation to the normal cores in the vortex state just as occurred in V3 Si (see Fig. 2.13). For that reason, the Cu(2) and O(2,3) relaxation curves in [60] are not really intrinsic superconducting behavior. Later studies, as we shall see in Chap. 5, show that the AFM enhancement in the SC state really does decay away to zero at low temperatures. Therefore, for the data of Fig. 3.11(a), the ﬁt calculated including enhancement decay is probably the more realistic one. In sum, we ﬁnd that the d-wave description of the YBCO7 NMR eﬀects for T < Tc according to the MP model theory was successful in an essentially quantitative way. Fitted parameter values suggest that strong-coupling eﬀects are quite important. It remained to be seen whether this kind of RPA model for the dynamic susceptibility could be applied to interpret the disparate temperature dependences which occur in the normal state. This is the theme of a series of theory papers which came soon after MP and which are expounded in some detail in Chap. 5. We shall see that the latter papers uphold the continued success of the single quantum ﬂuid picture of these systems which was initiated by the calculations of Mila and Rice. Meanwhile, the pseudo-gap eﬀect for low-doping materials came to light, and as we shall see in the next chapter, this eﬀect became a major sub-theme of cuprate physics.

References 1. R.M. Hazen, in Physical Properties of High Temperature Superconductors, Vol. II, ed. by D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), p. 121 67 2. F. Mila, T.M. Rice, Physica C157, 561 (1989) 67, 73, 81, 84, 85, 86, 87, 90, 92, 99, 102, 107 3. B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 67, 73, 81, 82, 99, 102 4. T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 68, 101 5. H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990) 68, 99, 104, 107, 108, 109, 110 6. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 68, 99 7. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 68, 99 8. J.G. Bednorz, K.A. Mueller, Z. Phys. B64, 189 (1986) 68 9. R.J. Cava, R.B. Van Dover, B. Batlogg, E.A. Rietman, Phys. Rev. Lett. 58, 408 (1987) 68 10. M.K. Wu, J.R. Ashburn, et al., Phys. Rev. Lett. 58, 908 (1987) 68 11. J.D. Jorgensen et al., Phys. Rev. Lett. 58, 1024 (1987) 68, 69 12. J.D. Jorgensen et al., Phys. Rev. B36, 5731 (1987) 69, 70 13. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B64, 014404 (2001) 69, 86, 89, 96 14. P. H¨ usser, H.U. Suter, E.P. Stoll, P.F. Meier, Phys. Rev. B61, 1567 (2000) 69, 86, 89, 96 15. N.F. Mott, Proc. Phys. Soc. London Sect. A 62, 416 (1949) 69 16. F.C. Zhang and T.M. Rice, Phys. Rev. B37, 3759 (1988) 70, 71, 82 17. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 70

References

113

18. C.M. Varma, Phys. Rev. Lett. 77, 3431 (1996) 70 19. P.W. Anderson, Science 235, 1196 (1987) 71, 78 20. P.W. Anderson, in Frontiers and Borderlines in Many-Particle Physics, ed. by R.A. Broglia, J.R. Schrieﬀer, International School of Physics “Enrico Fermi,” Course CIV (North-Holland, Amsterdam, 1988) 71, 78 21. S. Trugman, Phys. Rev. B37, 1597 (1988); B.J. Shraiman, E.D. Siggia, Phys. Rev. Lett. 60, 740 (1988); S. Sachdev, Phys. Rev. B39, 12232 (1989); C.K. Lane, P.A. Lee, N. Read, Phys. Rev. B39, 6880, (1989) 71 22. J.T. Markert, T.W. Noh, S.E. Russek, R.M. Cotts, Sol. St. Comm. 63, 847 (1987) 73, 74, 97, 99 23. D. Brinkmann, L. Pauli, J. Roos, H. Zimmermann, Phys. Lett. A 124, 112 (1987) 73, 74, 75, 97, 99 24. W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 59, 1860 (1987) 73, 74, 75, 76 25. H. L¨ utgemeier, M.W. Pieper, Sol. St. Comm. 64, 267 (1987) 73, 76 26. I. Furo, A. J´ anossy, L. Mih´ aly et al., Phys. Rev. B36, 5690 (1987) 73, 76 27. C.H. Pennington, D.J. Durand et al., Phys. Rev. B37, 7944 (1988) 74, 76 28. T. Shimizu, H. Yasuoka, T. Imai et al., J. Phys. Soc. Japan 57, 2494 (1988) 74, 76, 80 29. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 74, 79, 80, 81, 84 30. F. Adrian, Phys. Rev. B38, 2426 (1988) 74 31. C.H. Pennington, D.J. Durand, C.P. Slichter et al., Phys. Rev. B39, 2902 (1989) 74 32. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B36, 5727 (1987) 75, 76, 80 33. M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B38, 2832 (1988) 76, 79, 81, 84, 85 34. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B38, 9299 (1988) 76, 85, 99 35. H. Alloul, P. Mendels, et al., Phys. Rev. Lett. 61, 746 (1988) 76, 82, 99, 102 36. G. Balakrishnan, R. Dupree et al., J. Phys. C: Solid State Phys. 21 L847 (1988) 77, 99 37. R.E. Walstedt, W.W. Warren, Jr., R. Tycko et al., Phys. Rev. B38, 9303 (1988) 79, 81, 91 38. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 79, 80, 81, 91, 92 39. Y. Yafet, V. Jaccarino, Phys. Rev. 133, A1630 (1964) 79 40. B. Bleaney, K.D. Bowers, M.H.L. Pryce, Proc. R. Soc. London A228, 166 (1955) 79 41. M. Takigawa, P.C. Hammel et al., Phys. Rev. B39, 300 (1989) 79, 81, 84, 85, 95 42. A. Abragam and B. Bleaney, Electron Paramagnetic Resonance of Transition Ions, (Clarendon Press, Oxford, 1970), p. 455 80, 83, 86, 89 43. P.W. Anderson, Phys. Ref. Lett. 3, 325 (1959) 80 44. D.E. Farrell et al., Phys. Rev. B36, 4025 (1987) 80 45. R.E. Watson, A.J. Freeman, Hyperﬁne Interactions, ed A.J. Freeman, R.B. Frankel (Academic Press, New York, 1967), p. 53 81 46. F. Mila and T.M. Rice, Phys. Rev. B40, 11382 (1989) 81, 82, 98, 99, 107 47. R.E. Walstedt et al., Phys. Rev. B45, 8074 (1992) 83, 96 48. S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 84, 85, 95, 99, 105, 106 49. W.C. Lee, D.C. Johnston, Phys. Rev. B41, 1904 (1990) 85, 87 50. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990) 85, 105 51. A.K. McMahan, R.M. Martin, and S. Satpathy, Phys. Rev. B38, 6650 (1988) 86 52. J. Owen, J.H.M. Thornley, Rep. Prog. Phys. 29, 675 (1966) 86

114 53. 54. 55. 56. 57. 58. 59. 60. 61. 62. 63. 64. 65. 66. 67. 68. 69. 70. 71. 72. 73. 74. 75. 76. 77. 78. 79. 80. 81. 82. 83.

84. 85. 86. 87. 88.

3 Preliminary Steps in Cuprate NMR D.L. Randles, Proc. Roy. Soc. London, Ser. A331, 85 (1972) 86 F. Mila, Phys. Rev. B38, 11358 (1988) 87 T. Moriya, J. Phys. Soc. Japan 19, 681 (1964) 88 V. Heine, Phys. Rev. 107, 1002 (1957) 89 J.A. Martindale, S.E. Barrett et al., Phys. Rev. Lett. 68, 702 (1992) 91 A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 91, 104 M. Takigawa, P.C. Hammel, et al., Phys. Rev. Lett. 63, 1865 (1989) 93, 94, 95, 96 P.C. Hammel, M. Takigawa et al., Phys. Rev. Lett. 63. 1992 (1989) 93, 97, 99, 111, 112 M. Horvati´c, Y. Berthier, et al., Physica C159, 689 (1989) 93, 95 C. Coretsopoulos et al., Phys. Rev. B39, 781 (1989) 93 R. Sternheimer, Phys. Rev. 84, 244 (1951); 86, 316 (1952); 95, 736 (1954) 94 H. Alloul, A. Mahajan, H. Casalta, O. Klein, Phys. Rev. Lett. 70, 1171 (1993) 96 H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989) 96, 98 N. Bulut, D.W. Hone et al., Phys. Rev. B41, 1797 (1990); Phys. Rev. Lett. 64, 2723 (1990) 97, 99 H. Monien, D. Pines, C.P. Slichter, Phys. Rev. B41, 11120 (1990) 98 V.J. Emery, G. Reiter, Phys. Rev. B38, 4547 (1988) 98 T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 99 V. Jaccarino, in Physics of Solids, International School of Physics ”Enrico Fermi”, Course XVIII (Academic, New York, 1967) 99 H. Monien, D. Pines, Phys. Rev. B41, 6297 (1990); N. Bulut, D. Scalapino, Phys. Rev. B45, 2371 (1992) 99 A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 99 T. Auler, M. Horvatic et al., Physica C313, 255 (1999) 101 C.M. Varma, P. Littlewood et al., Phys. Rev. Lett. 63, 1996 (1989) 104 C. Gros, R. Joynt, T.M. Rice, Z. Phys. B68, 425 (1987) 104 F.C. Zhang, C. Gros, T.M. Rice, H. Shiba, Supercond. Sci. Technol. 1, 36 (1988) 104 G. Kotliar, J. Liu, Phys. Rev. B38, 5142 (1988) 104 J. Kirtley, C.C. Tsuei, et al., Nature (London) 373, 225 (1995) 104 D.H. Wollman, D.J. van Harlingen, et al., Phys. Rev. Lett. 74, 797 (1995) 104 H. Monien, A. Zawadowski, Phys. Rev. Lett. 63, 911 (1989) 104 M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 105, 106, 107, 108 K. Yosida, Phys. Rev. 110, 769 (1958) 105 D.E. MacLaughlin, “Magnetic Resonance in the Superconducting State”, in Solid State Physics, Vol. 31, ed. by H. Ehrenreich, F. Seitz, D. Turnbull (Academic Press, New York, 1976), p. 1 109 T. Imai, T. Shimizu, H. Yasuoka, J. Phys. Soc. Jpn. 57, 2280 (1988) 110, 111 G.-q. Zheng, et al., Phys. Rev. Lett. 86, 4664 (2001) 111 N.J. Curro, et al., Nature 434, 622 (2005) 111 H. Sakai, Y. Tokunaga, et al., J. Phys. Soc. Japan 74, 1710 (2005) 111 T. Fujimoto, G.-q. Zheng, et al., Phys. Ref. Lett. 92, 047004 (2004) 111

4 Pseudogap Eﬀects in Cuprate NMR Studies

Up to this point the discussion has focused on fully oxygenated YBCO7 and nearby compositions, for which Tc is very near its peak value 92 K for this compound. In 1989, detailed studies began to appear for underdoped YBCO7x, x ∼ 0.4, as well as for La2−x Srx CuO4 over its entire range of superconducting behavior 0.05 ≤ x ≤ 0.35. These phases brought new and surprising eﬀects to light, detailed theories for which are only recently beginning to appear. The principal new eﬀect was a gapped appearance to the NMR shifts, susceptibility, and low-energy excitations via 1/T1 T . These eﬀects were at ﬁrst attributed to pairing correlations forming at temperatures well above Tc , since there appeared to be no clear distinction between the pseudogaps and superconducting gaps. In the prevailing notion of “spin-charge separation” these eﬀects were initially called “spin gaps” in the mistaken belief that they only aﬀected spin–magnetic properties. Eventually, energy gaps were observed with a wide variety of probes (e.g. ARPES), uncovering a major element in the phenomenology of cuprate superconductivity. In this chapter we recount the beginnings as well as the current status of the pseudogap eﬀect. In the pre-pseudogap days, the behavior of YBCO7 did not appear to be aﬀected by pseudogap eﬀects. With its relatively ﬂat susceptibility and Korringa-like relaxation for the 89 Y and 17 O, the NMR properties seemed to resemble a normal Fermi liquid. However, in retrospect, such a simple picture was illusory. A cuprate with no trace of a pseudogap is clearly a very special case, and the vast majority of other phases which came to light were dominated by pseudogap behavior. Typically, as the doping level decreases from the optimum Tc value, (i) the susceptibility develops a gapped appearance, beginning at progressively higher temperatures, (ii) the temperature variation of 1/T1 T for 89 Y and 17 O develops a similar shape, while that for 63,65 Cu(2) remains non-monotonic with a peak at a lower temperature, and (iii) instead of a sharp break downward in the NMR shift and 1/T1T below Tc , these quantities execute smooth, declining curves through Tc without any noticeable discontinuity in slope. Among conventional superconductors, behavior such as this is unknown.

R.E. Walstedt: Pseudogap Eﬀects in Cuprate NMR Studies, STMP 228, 115–157 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 4

116

4 Pseudogap Eﬀects in Cuprate NMR Studies

Δν (MHz)

We illustrate these eﬀects with data from two early NMR papers on the pseudogap [1, 2]. Similar results for the Cu(2) were given by Horvati´c et al. [3] and Yasuoka et al. [4]. Warren et al. presented NQR curves for 1/T1 T vs. T for 63 Cu(2) and similar NMR measurements for 89 Y in the Tc 64 K phase of YBCO7-x, 0.3 ≤ x ≤ 0.51 . These are shown in Fig. 4.1

(a)

30

0.4 0

1 / T1 T (s K)–1

60

80

100

TEMP (K)

20

10

63Cu

0 0

100

200

300

T(K) 0

1 / T1 T (10+4 s K)–1

(b) 2

1 89Y

0

0

100 200 TEMPERATURE (K)

300

Fig. 4.1. (a) 1/T1 T is plotted vs. T over the interval 40K ≤ T ≤ 300K for two NQR peaks associated with 63 Cu(2) sites in YBCO6.64 (Tc 64K) [1]. For comparison, the dashed line shows the behavior recorded earlier for the YBCO7 phase (Tc 90K). The inset shows the shift in the resonance frequency of the NQR coil which occurs as the sample goes superconducting at T 64K. (b) 1/T1 T is plotted vs. T for 89 Y NMR in the same sample used as in (a). These data show a sharp deviation from YBCO7-phase Korringa behavior, which is characteristic of the pseudogap. Figure reprinted from W.W. Warren, Jr., R.E. Walstedt, et al., Phys. Rev. Lett. 62, 1193 (1989). Copyright 1989 American Physical Society 1

Although a continuum of Tc values has been reported for YBCO7-x, the 60 K phase is the most homogeneous underdoped phase, since dTc /dx is quite small in that region.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

117

where the low-frequency excitation spectrum ( q A2q χ (q, ω)/ω) is seen to decline at low temperatures as though an energy gap had set in below T ∼ 300 K. At Tc 64 K there is no break or other feature in the Cu(2) T1 data (Fig. 4.1(a)), in complete contrast with the sharp drop which takes place for the YBCO7 phase (see Fig. 3.11). Nonetheless, monitoring the rf coil susceptibility (Fig. 4.1(a), inset) gives good evidence that the sample material undergoes a transition to bulk superconductivity at that temperature. This behavior will be conﬁrmed below for this as well as other cuprates. A second body of both NMR shift and relaxation data for 89 Y in YBCO6+x is shown in Fig. 4.2, where curves with very similar shapes for both parameters are presented [2]. There, a progressive gapping eﬀect is seen to advance steadily from x ∼ 1.0 to the non-superconducting phase at x ∼ 0.4. Although these results were ﬁrst interpreted on a Fermi-liquid model, that interpretation was later revised [5]. In retrospect, the results concerned appear to establish another important pseudogap result contrary to the usual Korringa behavior. The relaxation rate product 1/T1 T is very nearly proportional to Ks (T ) and therefore to the spin susceptibility χs (T ). In Sect. 4.1 we will discuss the physical meaning of this along with a theoretical model which yields this result. Reference was made [2] to the theoretical prediction by Friedel [6] that precursive pairing eﬀects in 2D superconductors might give rise to a “pseudogap” well above Tc in the excitation spectrum. As we shall see in Sect. 4.2, the pseudogap also turned up fairly quickly in charge-related eﬀects such as speciﬁc heat and ARPES data. We mention one ﬁnal result which appeared around the same time as the foregoing eﬀects were reported, namely the susceptibility scaling eﬀect for underdoped LSCO which was reported by D.C. Johnston [7]. It was found that χs (T ) for a series of underdoped samples of La2−x Srx CuO4 not only exhibited a gap-like feature, but were found to scale rather precisely with a reduced temperature variable T /T ∗ . Although this eﬀect was interpreted at the time in terms of a theoretical model for insulating antiferromagnets and was not linked for some time with the pseudogap eﬀect, it seems clear in retrospect that it was, in fact, closely related to the eﬀects presented above for YBCO7-x. Later in this chapter we shall also discuss pseudogap eﬀects in the high-Tc systems LSCO and Y248.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x Since spin pseudogap eﬀects in the NMR data ﬁrst came to light in studies of YBCO7-x with some depletion of the oxygen content (and thus of hole doping), it was for this system that the most precise and comprehensive bodies of data were ﬁrst developed. In this section we present and discuss a set of results on both the NMR shifts and relaxation rates for 89 Y, 17 O(2,3), and

118

4 Pseudogap Eﬀects in Cuprate NMR Studies

63

Cu(2) for a representative composition YBCO6.63 [8, 9, 10]. This compound is a well-characterized example of a high-Tc pseudogap system. –ΔK (ppm) 50

x = 1.0

1–ε

0.85 0.75 0.63 0.53

0

0.48 0.35 0.41

–50

(a) 89Y

–100

104 (T1T)–1 (sec °K)–1

2

ν0 = 15.64 MHz

Y Ba2 Cu3 O6 + x 200 T (°K)

100 3

89Y

NMR

300

NMR

(b)

ν = 15.64 MHz x=1 1–ε 0.85

0.75 0.63 0.53 0.48

1

0.41

Y Ba2 Cu3 O6 + x 0

100

200 T (°K)

300

Fig. 4.2. (a) The negative of the 89 Y NMR shift ΔK is plotted as a function of temperature for a series of compositions YBCO6+x, for 0.4 ≤ x ≤ 1.0 [2]. ΔK is measured relative to the 89 Y gyromagnetic ratio found with a solution of YCl3 . In Sect. 4.1 the chemical shift is determined to be 89 Korb,α 160 ppm, where α = ab,c. (b) Plots of 1/T1 T vs. T for the same series of compositions used in (a) [2]. In both cases the data show the progressive development of a pseudogap eﬀect in which they exhibit a maximum at progressively higher T for increasing dilution of hole carriers. These data can also be plotted to show the relation 1/T1 T ∝ (89 Korb,α − ΔKα (T )) characteristic of the pseudogap region. Figure reprinted from H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989). Copyright 1989 American Physical Society

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

(a)

(b)

Fig. 4.3. Continued

119

120

4 Pseudogap Eﬀects in Cuprate NMR Studies

4.1.1 HF Parameters for YBCO6.63 from Scaling of Shift Data We ﬁrst discuss NMR shift and susceptibility data for YBCO6.63. In Fig. 4.3(a) NMR shift data for 63 Cu(2) in an oriented powder specimen are plotted for ﬁeld orientation both parallel to and perpendicular to the c axis [1]. The c axis data show only a slight increase below Tc , so that 63 Korb,c = 1.28(1)% and 63 Ks,c = –0.01(1)% (near 300K). This result for 63 Korb,c is indistinguishable from that for YBCO7.0 [11]. The zero–temperature intercept for 63 Kab (T ) is 63 Korb,ab = 0.25(2)%, which is also unchanged from YBCO7 [11]. The downward–curving spin paramagnetism is the essence of spin pseudogap behavior. In Fig. 4.3(b) are plotted 17 O NMR shift values (17 K , 17 K⊥ , 17 Kc ) as functions of temperature for the three principal axes of the O(2,3) sites [9]. The quadrupole tensor has also been evaluated and is virtually indistinguishable from what was determined for YBCO7 (see Fig. 3.8 and discussion). The shift 17 K (T ) corresponding to the Cu(2)-Cu(2) bond axis is seen to be more than half again as large as the transverse components. The latter (17 K⊥ (T ) and 17 Kc (T )) have slightly diﬀerent chemical (i.e. orbital) shifts, but their temperature variation is essentially indistinguishable. The 17 O(2,3) shift can therefore be characterized by axial and isotropic components deﬁned by 17 Kax = (17 K - 17 K⊥ )/3 and 17 Kiso = (17 K + 17 K⊥ + 17 Kc )/3. As with YBCO7 (Sect. 3.4) there is a dominant isotropic HF eﬀect from 3d-2s hybridization [12] and a lesser axial shift term corresponding to dipolar coupling from the 3d-2pσ hybridization, although the latter admixture is much greater than the former. The 17 O NMR shifts for 17 K and 17 K⊥ , plus that for 63 Cu(2) [9] have been scaled to coincide with 17 Kc (T ), the most accurate data set, between Tc and 300K, and are plotted with separate vertical axes in Fig. 4.4. All shifts are seen to follow a common temperature variation very closely, i.e. that of the spin susceptibility. From the scaling ﬁts the following relations are obtained: Fig. 4.3. (a) The NMR shift for 63 Cu(2) in an oriented-powder sample of YBCO6.64 [8] is plotted vs. temperature for ﬁeld orientation parallel and perpendicular to the c axis. The upper solid line is a representation of data for YBCO7, while the lower one is a guide to the eye. As with YBCO7 it is assumed that the orbital shifts are independent of temperature and that the spin susceptibility goes to zero at T Tc . The breakdown of both shifts into spin and orbital components is given in the text. Figure reprinted from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990). copyright 1990 American Physical Society (b) Data for the 17 O(2,3) NMR shift is plotted as a function of temperature up to 300K for an oriented powder sample with ﬁeld oriented along three mutually perpendicular axes, where the axis for 17 K is the Cu(2)-Cu(2) bond axis [9]. The solid line is the variation of 17 Kc (T ) for YBCO7 [11]. Analysis of these results is given in the text. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). copyright 1991 American Physical Society

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x 17

121

Kax (T ) = 0.1886 ×17 Kc (T ) + 0.0151%,

(4.1.1a)

Kiso (T ) = 1.057 × Kc (T ) + 0.039%, 63 Kab (T ) = 1.522 ×17 Kc (T ) + 0.32%.

(4.1.1b) (4.1.1c)

17

17

This result gives additional strong evidence for a one-component quasiparticle state, since multiple bands would have to have susceptibilities with precisely matching spin-gapped temperature variation to produce this result. Such an eﬀect seems quite implausible. 0.2

0.25

10

0.05

0.6

0.2

χ

0.4

(%)

(%) 17K C

0.15

1 0

17K ax

(%) 17K iso

0.5

63K ab

(%)

0.04

6 5

10 15 20 25

1000/T(K) 0.1 17

0.03

17

Tc

0.1

17K iso 63 Kab

y = 0.37

0.05

Kc Kax

4

2

χspin [10–5 emu/mol Cu (2)]

0.15

8

ΔGap = 104K

0.02 0.05 0

100

200

0 300

T (K)

Fig. 4.4. (a) Data for 63 Kab (T ) for the Cu(2) sites [9] (similar to Fig. 4.3(a)) as well as for 17 K (T ) and 17 K⊥ (T ) have been scaled to 17 Kc (T ) and are plotted with the latter data as a function of temperature. The T → 0 (orbital shift) limits of these shifts plots have been determined as discussed in the text, leading to an estimate for the zero of the spin components of the shifts and of the spin susceptibility. Scales for the various shift components are shown on the left. The scale for χs (T ) has been estimated from the knowledge of HF constants (see text) and is shown on the right side of the plot. The solid line represents the estimate of χs (T ) so determined. The inset shows an Arrhenius plot of ln(χs (T )) vs. 1000/T(K). The linear behavior suggests an energy-gap nature for χs (T ), where ΔGap 104K. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). copyright 1991 American Physical Society

The scaled curves in Fig. 4.4 come apart a bit below Tc , an eﬀect which is attributed to varying levels of diamagnetic shielding for the diﬀerent cases. However, because 17 K and 17 K⊥ are both measured with ﬁeld ⊥ c axis, there is no diamagnetic correction to 17 Kax . Directly from extrapolating the

122

4 Pseudogap Eﬀects in Cuprate NMR Studies

curves in Fig. 4.3(b) to T = 0, then, one ﬁnds 17 Kax (0) = 0.013(2)%. One can then use the (4.1.1) to obtain the other orbital (i.e. zero temperature) shift values. One ﬁnds 17 Kc (0) = -0.014(7)%, 17 Kiso (0) = 0.024(11)%, and 63 Kab (0) = 0.30(2)%. These values are virtually unchanged from 17 O orbital shifts determined earlier for YBCO7 (See Table 3.2). Using the relation χs (T ) = 63 Kab (T )/fCu (Aab + 4B), where Aab + 4B 198 kOe/μB [13], and the estimate fCu 0.7 for the fraction of χs which resides on the Cu(2) site, the scale shown for χspin (T ) in Fig. 4.4 has been determined. The parameters derived from a Mila-Rice ﬁt to the data in Sect. 3.2 (see Table 3.4) would give a slightly larger value for (Aab + 4B). Other ﬁts to the shift and relaxation data in Chap. 5 will also give slightly diﬀerent values for the scale of χs (T ). We only note that this scaling factor is not critical at this point. It will be discussed further in Chap. 5. Regardless of the scale of χs (T ), we may examine the question of its gapped nature by plotting the data of Fig. 4.4 in an Arrhenius plot, i.e. as χs (T ) = χ0 exp(−ΔGap /T ). Such a plot is shown in the inset to Fig. 4.4,2 where it is found to yield a very accurate representation of the data, with ΔGap 104K. Such a result was implied by the ﬁtting procedure of Uldry and Meier [14], to be discussed in Chap. 5. To our knowledge, this representation has not been predicted by any model calculation up to now and has not been emphasized in the literature. This result will be compared with INS data on a similar sample below. The 89 Y NMR shift and relaxation data which came two years later [10] completed the NMR data picture for YBCO6.63. The corresponding shift data for both YBCO6.63 and YBCO7 cases were plotted vs. T as in Fig. 4.5(a), where the “6.63” data are seen to exhibit a very similar temperature dependence as the scale plot Fig. 4.4. This idea is tested in Fig. 4.5(b) where the latter data for both ﬁeld orientations are plotted vs. 17 Kc (T ) data from Fig. 4.3. The resulting curves are straight lines within narrow error limits, and the extrapolation to 17 Kc (0) = -0.014(7)% then gives the chemical shifts 89 Korb,c = 160(15) and 89 Korb,ab = 152(10) ppm. Thus, the 89 Y shift data also follow the curve in Fig. 4.4 to high precision. Scaling of HF Coeﬃcients to Match YBCO7. We therefore have a complete characterization of NMR shifts for all signiﬁcant sites and ﬁeld orientations in YBCO6.63 in terms of a single universal curve [9]. The resulting shift values at T = 300K are listed in Table 4.1 (“300K Values”). Also listed there is the estimated Cu(2) susceptibility tensor at 300K from [9]. We suggest, however, that the latter values are very approximate and that better values for both the susceptibility tensor and the HF coeﬃcients can be assigned by scaling the HF tensor components so that they match the 2

Please note that this inset was not part of the original ﬁgure in [9], but was added later.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

123

200

–89

K (ppm)

(a) 100

O7

Kc Kab

0 O6.63 Kc Kab

–100 0

100

200 T (K)

300

100 (b)

0

89

Kc

89

Kab

–89

K (ppm)

50

–50

–100

0

0.05

0.1 17

0.15

Kc (%)

Fig. 4.5. (a) The negative of the 89 Y NMR shift in YBCO6.63 is plotted as a function of temperature for applied ﬁeld both parallel and perpendicular to the c axis of an oriented powder sample [10], which is actually the same sample used in the foregoing Cu(2) and O(2,3) NMR studies [9]. For comparison, previous data on YBCO7 [10] are also shown. (b) The YBCO6.63 shift data from part (a) are plotted vs. the oxygen shift data 17 Kc (T ) from [9]. Extrapolation of these curves to 17 Kc (0) yields the chemical shift values for 89 Y given in the text. These linear ﬁts also demonstrate that all NMR shifts in YBCO6.63 follow the same temperature dependence, namely that of χs (T ). Figure reprinted from M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993). Copyright 1993 American Physical Society

YBCO7 values from Tables 3.4 and 3.6 as closely as possible. For convenience, the latter set of values (“YBCO7 (Ai )”) is listed in Table 4.1. A “trial” set of HF coeﬃcients can be deﬁned from the data in Table 4.1 using the relation from (3.3.4) Ai = NA μB Ki /zi χsi ,

(4.1.2)

where Ki are the “300K” values from the table, zi are the numbers of Cu(2) neighbors, and χsi is the appropriate susceptibility estimate from the same

124

4 Pseudogap Eﬀects in Cuprate NMR Studies

Table 4.1. The NMR shift tensors for 17 O(2,3) and 89 Y in YBCO6.63 at 300 K [9, 10] are listed in the top line, then the corresponding HF coeﬃcients are stated for YBCO7 from Tables 3.4 and 3.6, below which the scaled coeﬃcient values for YBCO6.63 derived from the stated shift values are listed for comparison. The scaling procedure is described in the text, wherein the weighted sum of fractional errors deﬁned by (4.1.3) is minimized. Weighting factors wi are designed to give each species the statistical weight it has in the unit cell. NMR shift values are given in %, the spin HF coeﬃcients in kOe/μB , and susceptibilities in 10−6 emu/Cu(2) Shift Comp.

63

Ks,ab

17

300K Values 0.218 (2) Aab

Spin HF Coef. YBCO7 (Ai ) 155 YBCO6.63 152 Ri 1.370 4 wi

Ks,a

17

Ks,b

17

Ks,c

89

Ks,ab

89

Ks,c χs⊥ (300 K) χs (300 K)

0.205 0.124 0.143 0.0173 0.0255 Ca

Cb

Cc

72 44 38 71.4 43.2 40.0 1.386 1.372 1.470 8/3 8/3 8/3

Dab

Dc

1.71 1.51 1.231 1

1.86 1.87 1.338 1

58

72

80

100

line of the table. The Ai are multiplied by a scaler S, which is then adjusted to minimize a weighted total fractional squared error deﬁned by ERR =

wi [SAi − Ai ]2 = wi [1 − SRi ]2 , 2 A i i i

(4.1.3)

where the YBCO7 coeﬃcients are labelled Ai , and Ri = Ai /Ai . This procedure will also yield a new estimate of the susceptibility tensor, from (4.1.2), of χsi /S. The ratios Ri are listed in Table 4.1, and are seen to be grouped closely around a value 1.36. It is easy to show that the errors are minimized when wi Ri (4.1.4) S = i 2 = 0.723. i wi Ri The optimally scaled coeﬃcients obtained are stated in Table 4.1 (“YBCO6.63”). Correspondence with the YBCO7 values is seen to be quite satisfactory. The resulting (scaled) susceptibility components are also given. They are somewhat larger than the values from Fig. 4.4, but are ∼ 80% of the corresponding values in Table 3.4, in reasonable agreement with the relative values shown by experimental data given by Takigawa et al. in [9]. One important consequence of this ﬁtting procedure is that the reduction factor 0.70 used to estimate the HF coeﬃcients in Table 3.4 is corroborated by the YBCO6.63 shift scaling (Fig. 4.4) results. These results strongly suggest (2) that the composite Cu(2) shift coeﬃcient, for which we ﬁnd the value Aab 155kOe/μB (Table 4.1), must, in fact, be rather smaller than the value 198kOe/μB given by Monien et al. [13].

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

125

Next, we consider the anisotropy of the 17 O(2,3) and 89 Y HF coeﬃcients and Dα , respectively. Not surprisingly, the Cα have a strong axial component along the Cu(2)-Cu(2) bond axis owing to the 2pσ hybridization. The observed c/a axis anisotropy is, however, mainly a g-factor eﬀect. The constants Cα to be used in the main Hamiltonian (3.3.4) are proportional to gα Cα , which diﬀers by only a few percent between the b and c axes. This is within the expected errors. The Dα values, however, display a clear anisotropy if we consider the quantities g Dc vs. g⊥ Dab , where the former is ∼ 30% larger. The origin of this eﬀect is not clear, but the Y 3+ HF response is clearly more than simply the isotropic core polarization HF ﬁeld, as noted in [9]. Cα

Dipolar Contribution to

89

Y HF Coupling.

One candidate eﬀect for the Dα anistropy is direct dipolar coupling from the Cu2+ moments, which has been considered by Takigawa et al. [10]. Since the 89 Y HF couplings are rather small for YBCO, one must considerthe possibility that the dipolar interaction between any Cu2+ moment − α gα μB Sα u ˆα , where u ˆα is a cartesian unit vector, and a 89 Y nuclear spin moment 89 I, 89 ( I · r) g S r γ89 μB α α α (89) α Hdip = − (4.1.5) gα Sα 89 Iα − 3 2 r3 r α is a signiﬁcant HF energy. The importance of this is that (4.1.5) does not have the simple diagonal form of (3.3.2), thereby changing the nature of the dynamical calculations if it is an important eﬀect. To consider the direct dipolar HF coupling with the 89 Y, we note that owing to hybridization, the Cu2+ moment at the origin (Fig. 2.1(b)) actually consists of a fraction 1 − 4δ on the Cu(2) site and fractions δ located on the four nn O(2,3) sites. At the hybridization level δ 0.08, the two O(2,3) sites nearest the 89 Y are quite signiﬁcant, since they are rather closer to the Y 3+ than the Cu(2). We ignore the two more distant O(2,3) sites in this estimate. The positions of various ions in the crystal (Fig. 3.1) are such that the Cu(2)O(2,3) horizontal distance is d = 1.95 ˚ A, and the vertical distances between 89 Y and Cu(2) and O(2,3) are Δc1 = 1.65 ˚ A and Δc2 = 1.42 ˚ A, respectively. Using (4.1.5) we then ﬁnd for the total contribution to the HF coeﬃcients ⎧ ⎫ ⎧ ⎫ 1 − 4δ ⎪ d2 ⎪ δ ⎪ d2 ⎪ ⎪ ⎪ ⎪ ⎪ − 3 + − 3 = −8μB ΔDdip,ab ⎩1 ⎭ ⎩2 3 2 3 2 ⎭ (4.1.6a) rCu rCu rO rO ⎧ ⎫ ⎧ ⎫ 1 − 4δ ⎪ Δc12 ⎪ 2δ ⎪ Δc22 ⎪ ⎪ ⎪ ⎪ ⎪ 1 − 3 + 1 − 3 = −8μB ΔDdip,c ⎩ ⎭ 3 2 3 ⎩ 2 ⎭ ,(4.1.6b) rCu rCu rO rO ˆ + kΔc1 ˆ ˆ where rCu = ˆid + jd and rO = ˆid + kΔc2. Inserting the foregoing numbers into these equations, we ﬁnd ΔDdip,ab = 0.14 kOe/μB and ΔDdip,c = -0.28 kOe/μB . These are of the order of 20-30% of Dα and so they are quite appreciable as suggested in [9]. However, since they have the opposite sign of

126

4 Pseudogap Eﬀects in Cuprate NMR Studies

the observed anisotropy, it is clear that there is another source of anisotropy which is twice as large.3 The other noteworthy point is that there are a number of dipolar terms which are eﬀective for the T1 process but which have an angular dependence which does not vanish at the “magic angle” and therefore may be considerably larger than the shift coeﬃcients estimated above. Thus, one may not ﬁnd that T1 for 89 Y exhibits the expected anisotropy from the measured Dα coeﬃcients. The dipolar eﬀects for the 89 Y were also discussed in detail by Auler et al. [15]. We shall address this matter further in the next subsection. 4.1.2 A Simple Model Theory of Spin Dynamics for YBCO6.63 The Spin-Hamiltonian formulation of HF coupling at the Cu2+ sites combined with the Mila-Rice-Shastry [12, 16] picture of transferred HF couplings from the Cu2+ moments to the Y and O(2,3) sites provides a deﬁnite basis for discussing electron spin-based static and dynamic NMR properties. In the last subsection we saw that one ﬁnds a consistent picture of HF couplings from NMR shift data, which apply to both YBCO7 and YBCO6.63. The coupling constants we refer to here are found in Tables 3.4, 3.6, 4.1. They were used in the Mila-Rice discussion of T1 in Chap. 3. Meanwhile, here we consider the relaxation properties of YBCO6.63, where spin-spin correlations will be used to discuss comparative temperature variations of T1 in terms of dynamical spin ﬂuctuations. As was noted in Sect. 3.3.3, dynamical spin correlations are the apparent cause of the T-varying 63 Cu(2) T1 anisotropy for YBCO7 [17]. Although a comparable data set is not available for YBCO6.63, we shall ﬁnd application in this case for similar formulations of the 89 Y and 17 O(2,3) relaxation properties as well as the 63 Cu(2). Let us anticipate some of the themes as well as stumbling blocks which arise in the course of trying to account for the relaxation behavior of the YBCO6.63 (60 K) phase. First, we note the pervasive characteristic temperature variation 1/T1 T ∝ Ks (T ), which arose in an empirical way, but then found a measure of theoretical justiﬁcation [18]. Secondly, the case of 89 Y has two special problems, which have been discussed by Takigawa et al. [10]: (i) The direct dipolar interaction is large enough to make an important contribution to the overall HF coupling, as we saw in the previous subsection. Thus, the HF coupling Hamiltonian does not have the simple form of (3.3.2). This complicates the relaxation calculations. (ii) The 89 Y relaxation is driven by Cu2+ spin moments in neighboring CuO2 planes (see Fig. 3.1), so the question of interplanar spin correlations is an important one for T1 . As there is neutron-scattering evidence for such correlations [19], the 89 Y T1 phenomena are more complex on that account. 3

A simple sign check is the following: For the c–axis case, ΔDdip,c has the same sign as for the limit Δc1, 2 → 0. In the latter case, ”up” moments on the Cu(2) or O(2,3) sites would clearly give ”down” (i.e. negative) HF ﬁelds at the 89 Y sites, in accord with the calculated result.

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

127

T1 Enhancement and a Model Susceptibility for Underdoped Cuprates. It was ﬁrst noted empirically that the quantity (T1 T Ks (T ))−1 is approximately constant for 89 Y and 17 O(2,3) in both the YBCO7 and YBCO6.63 phases [8]. Moreover, the same quantity for the 63 Cu(2) no longer exhibits a peak around 150 K, but executes a roughly power-law rise as T approaches Tc in the normal state. These behaviors are shown in Fig. 4.6 using data from various sources (see ﬁgure caption). Interestingly, the 63 Cu(2) data for YBCO7 show a similar temperature characteristic. The 89 Y and 17 O(2,3) shown indicate very little change with T , i.e. 1/T1T ∝ χs (T ). Later, more complete data, however, deviated from this simple picture. The data plotted in Fig. 4.6 are scaled as [T1 (Korr.)/T1 (T )][Ks (300K)/ Ks (T )], where T1 (Korr.) = Ns γe2 /(4πkB T γn2 Ks2 ), (4.1.7) which is the usual Korringa expression with a factor Ns to account for multiple sources of HF ﬂuctuations. Here, Ns = 4, 2, and 8 for Cu(2), O(2,3) and Y, respectively. Note that Ns = 4 for the c-axis Cu(2) T1 process, which is dominated by the four nn couplings. The shift has also been normalized arbitrarily to its room-temperature value, so that the absolute values plotted are only a relative indication of ﬂuctuation enhancement levels. Clearly, for Cu(2) the YBCO6.63 case is smartly enhanced over the YBCO7, and both of these by a considerable margin over the ligands. These eﬀects are attributed to AFM ﬂuctuations, which barely touch the ligands, but strongly enhance the Cu(2) relaxation and increase quickly with carrier dilution. The proportionality between 1/T1 T and Ks (T ) is suggested by the model form [8, 22] πχ0 ω χ (q, ω) = G(q) (4.1.8) Γ for the low-frequency dynamics (ω Γ ) of the quasiparticles, where χ0 is interpreted as an estimate of the static susceptibility, and the factor G(q) embodies any q-dependent enhancement eﬀects which occur. Since 1/T1 T ∝ G(q), this form suggests that 1/T1 T ∝ χ0 . To use this form even when χ0 q has the gapped temperature characteristic of an underdoped cuprate is to go beyond the usual mean-ﬁeld theory interpretation of (4.1.8). Nonetheless, this procedure has been adopted in order to treat T1 phenomena in spin-gapped superconductors [23]. However, not long after the latter work appeared, a theoretical model was developed which actually exhibited such behavior. This was the “attractive” (i.e. negative-U) Hubbard model of Randini and Trivedi, which was studied using QMC techniques [18]. The authors only studied local, q-independent HF couplings, and emphasized that this was not a suitable model for cuprate physics in other ways. Nonetheless, their results for the gapped behavior of both susceptibility and 1/T1 T , shown in Fig. 4.7, give a remarkably realistic version of the eﬀects seen in Fig. 4.6 for, e.g. the 89 Y and 17 O(2,3) sites.

4 Pseudogap Eﬀects in Cuprate NMR Studies (T1T)–1 (sK)–1

128

100

8

6

4

KORRINGA RATIOS

0

50

T (K)

300

10 5

1 50

70

90

200

300

T (K)

Fig. 4.6. The quantity [T1 (Korr.)/T1 ][Ks (300 K)/Ks (T )] is plotted vs. T in a log-log plot over the range 50 K ≤ T ≤ 300 K for a series of cases as follows: Open and closed circles are for 63 Cu(2) in YBCO6.63 [8] and YBCO7 [17], respectively. Closed squares are 89 Y data from Alloul et al. [2] using, however, an independently determined value for the 89 Y chemical shift [8]. (A similar value was reported later by Alloul et al. [5].) The open squares are data for YBCO7 from [20] using the same chemical shift. Finally, the open triangles represent 17 O(2,3) data on YBCO7 from [21]. See text for a deﬁnition of T1 (Korr.) Figure reprinted from R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990). Copyright 1990 American Physical Society

To account for the Cu(2) data would require inclusion of q-dependent enhancement eﬀects in the negative-U Hubbard model, which has not, to our knowledge, been done. In any case, the results of Fig. 4.7 oﬀer some support for the phenomenological treatment based on (4.1.8) with χ0 = χs (T ). 4.1.3 INS Data for the Pseudogap of Underdoped YBCO Before we attempt to interpret T1 data for YBCO6.63 it is also important to discuss some neutron-scattering studies which are related to the low-frequency dynamical behavior. Several groups have reported spin correlations as well as AFM ﬂuctuation peaks in χ (q, ω) for this compound [19, 24, 25]. INS data for a YBCO6.6 sample with Tc = 53 K are shown in Fig. 4.8 [19]. At ω = 15 meV, q-scans through the AFM point [h(1 + δ), h(1 - δ), -1.8], for two values of δ and h = 0.5, record the ﬂat-topped AF peaks in χ (q, ω) at T = 10 K shown in Fig. 4.8(a) and (b) [19]. This appears to be a superposition

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

129

0.1

[ T1T ] –1

0.075

0.05

(n) = 0.5

0.025

U=4 U=8

0

0

0.05

0.1

0.15

χs Fig. 4.7. The variation of 1/T1 T vs. χs , with T as an implicit parameter, for the attractive-U Hubbard model calculations of [18]. Over the lower 40% of the variation of 1/T1 T , this quantity shows a very clear linearity with the spin susceptibility, with a constant of proportonality which is essentially independent of the value of U . Figure reprinted from M. Randeria, N. Trivedi, A. Moreo, R.T. Scalettar, Phys. Rev. Lett. 69, 2001 (1992). Copyright 1992 American Physical Society

of incommensurate peaks, but in any case it is a sign of strong in-plane AFM correlations. The authors suggest that this is strong enough to account for any observed enhancement of the Cu(2) relaxation. The temperature dependence of the integrated area under the AFM peak in χ (q, ω) (q ∼ QAF ) shows an energy-gap behavior with a gap value given as 9 meV 104 K [19]. This is the same gap energy as was derived from the static susceptibility data with an Arrhenius plot (Fig. 4.4, inset) for YBCO6.63. It seems that χs (T ) (i.e. q = 0) and χ (q, ω), q ∼ QAF (for YBCO6.60) exhibit the same gap energy. Such a result is implied by the dynamic susceptibility model (4.1.8) and is therefore supportive of such a model. Finally, a very substantial neutron intensity modulation has been observed in scanning q along the c axis. The scan of (0.5,0.5,l) for −3.5 ≤ l ≤ 3.5 is shown in Fig. 4.8(c), where a modulation amplitude approaching 50% is seen to occur at T = 100 K. Since the in-plane correlation length is only a few lattice spaces at most, the c-axis modulation reﬂects a larger exchange coupling between layers than one can easily account for. As was emphasized in [10], such an intensity modulation implies relatively strong interplanar spin correlations which cannot be ignored when we estimate the 89 Y relaxation rate. However, it is possible that the c-axis correlation eﬀect could diminish rapidly with increased doping level, and thus be smaller for YBCO6.63. Such a measurement needs to be compared with NMR data on the same sample material.

130

4 Pseudogap Eﬀects in Cuprate NMR Studies 150

(a)

δ=0

50 Intensity (counts / 16 min)

Intensity (counts / 7 min)

100

0 (b)

δ = 0.066 100 50 0 0.2

0.3

0.4

0.5

0.6

0.7

0.8

150

100

50 (c) 0 –4

–2

0

2

4

Fig. 4.8. (a) Neutron scattering intensity is shown for two scans in the vicinity of the AFM point along the diagonal (see text for details). These steep-sided peaks show signs of an incommensurability. They have been ﬁtted with a pair of Gaussians as shown. (b) A scan along (0.5,0.5,l) is recorded for an energy transfer of 9 meV at T = 100 K on a crystal of YBCO7-x, with x = 0.55 and Tc 45 K. The solid line is a resolution-corrected calculation of the inelastic structure factor from [19]. The variation of modulation amplitude with x is not known. Figure reprinted from J.M. Tranquada, et al., Phys. Rev. B46, 5561 (1992). Copyright 1992 American Physical Society

4.1.4 A Comprehensive T1 Data Set for YBCO6.63 We now consider the relaxation data for 63 Cu(2), 17 O(2,3), and 89 Y corresponding to the NMR shift and spin susceptibility results of Figs. 4.4 and 4.5. In Fig. 4.9 are displayed the high-quality T1 data for 63 Cu(2) and 17 O(2,3) in YBCO7 (“y = 0”) and YBCO6.63 (“y = 0.37”) from Takigawa et al. [9]. The Tc points indicated refer to YBCO6.63, where Tc 64 K. For the case of YBCO7 (open circles) the data for both 17 O(2,3) and 63 Cu(2) show very similar sharp declines at Tc 92 K. For YBCO6.63 (closed circles), however, the overall curves are very diﬀerent, and neither data plot shows any visible feature at Tc (indicated by arrows), where both curves are smooth and continuous. As shown in the inset to Fig. 4.1(a), however, the resistive superconducting transition remains as sharp as ever. As with χs (T ) (Fig. 4.4), then, the low-frequency spin dynamics show only a smooth decline in the vicinity of Tc . This behavior shows that the pseudogap merges smoothly into the superconducting gap which presumably forms below Tc . Considering the 63 Cu(2) T1 data in Fig. 4.9(b), a plot of these data similar to Fig. 4.6 yields essentially the same result4 . However, in spite of the 4

As an example we consider the value of [T1 (Korr.)/T1 ][Ks (T )/Ks (300)] at T = 100 K. Using (4.1.7) with Ns = 4, we take 1/T1 630 s−1 from Fig. 4.9(b),

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x 0.4

131

y = 0.37 6

y=0

TC

(63T1T)–1 (s–1K–1)

(17T1T)–1 (s–1K–1)

0.3

y = 0.37

0.2

0.1

0

2

(a)

TC 0

y=0 4

100

200 T (K)

(b) 300

0

0

100

200

300

T (K)

Fig. 4.9. (a) Data for 1/T1 T for 17 O(2,3) in both YBCO7 (“y = 0”, open circles) and YBCO6.63 (“y = 0.37”, closed circles) are plotted from 300 K down to well below Tc [9]. (b) With the same notation and symbols as in (a) the corresponding data for 63 Cu(2) are shown. Figure reprinted from M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991). Copyright 1991 American Physical Society

large numbers one sees in Fig. 4.6, the actual enhancement of 1/T1 T for Cu(2) is a relatively small number. From (3.3.14) one sees that 1/T1c ∝ χs (T )[1+0.29K01 +0.99(2K12 +K13 )]. The Kij ’s presumably have small values above 300 K, and as T → Tc could approach −1 for K01 and +1 for K12 and K13 . Thus, the AFM exchange enhancement factor [ ] varies from unity to a maximum [ ] 3.68. Examination of the data plot in Fig. 4.9(b) shows that it changes substantially between 100 K and 300 K, but stays well within those limits. Considering T1 data for 17 O(2,3) in Fig. 4.9(a), we see that it very closely resembles the susceptibility curve in Fig. 4.4. A plot of (T1 T Kc (T )) vs. T using data from the latter ﬁgures yields a curve varying by only a few percent between 100 K and 300 K [9]. The simple model form (4.1.8) for χ (q, ω) now 17 O(2,3) is leads us, however, into some diﬃculty. The correlation factor for simply [1 + K01 ], where the remainder of the expression ∝ q χ (q, ω)/ω, has been shown by neutron studies to vary with temperature in the same energygapped fashion as χs (T ). Thus, (T1 T Ks (T ))−1 constant for the 17 O(2,3) means [1 + K01 ] constant, which is not consistent with the “substantial” change in the correlations required by the 63 Cu(2) above. We shall now see that the 89 Y data lead to further diﬃculties with the model susceptibility (4.1.8). Ks (100 K) 0.11%, and [Ks (T )/Ks (300)] 0.5. Inserting these parameter values, one ﬁnds [T1 (Korr.)/T1 ][Ks (100)/Ks (300)] 39, which lies among the closed circle points in Fig. 4.6.

132

4 Pseudogap Eﬀects in Cuprate NMR Studies

The Problem of

89

Y T1 Behavior in YBCO6.63.

In Fig. 4.6 89 Y T1 data are plotted so as to test the pseudogap scaling with χs (T ). The result is a very ﬂat curve, based on data from [2]. However, there are two more recent sets of T1 measurements, by Takigawa et al. [10] and by Alloul et al. [5], neither of which agree with the previous conclusion. Data plots from [10] are shown in Fig. 4.10. In Fig. 4.10(a) are plotted 1/T1T for 89 Y in YBCO6.63 with both ﬁeld orientations as a companion to the NMR shift measurements in Fig. 4.5 on the same sample, as well as the 17 O(2,3) relaxation data from Fig. 4.9 for comparison. It is clear that 1/T1 T for the oxygen declines rather less at low temperatures than either 89 Y measurement. This point is illustrated further in Fig. 4.10(b), where 17 T1c /89 T1c is plotted for 100 K ≤ T ≤ 300 K. At 100 K this ratio is seen to have increased by more than 20% over its value at 300 K. Similar data are given in [5] for both Ks (T ) and 1/T1T for 89 Y in YBCO6.64. Although the latter data have somewhat larger error bars, they are consistent with the data shown in Fig. 4.10. Since these more recent data are much more complete than those shown in Fig. 4.6, we conclude that (T1 T Ks (T ))−1 for 89 Y is not constant in this composition, in contrast with the 17 O(2,3) data in Fig. 4.9. We discuss the data in Fig. 4.10 further by means of the general T1 formulas (3.5.22) and (3.5.21). Taking the ratio of these equations, we ﬁnd 89

T1ab 17 T 1c

=

2 [1 + K01 ] [Ca2 + Cb2 ] γ17 2 2 + D 2 ] [1 + 2K IC ] γ89 [Dab 01 + K12 + K c

(4.1.9)

where we have added an interplanar correlation coeﬃcient KIC to take account roughly of that possibility for the 89 Y. In the high temperature limit where 2 2 2 [Ca2 + Cb2 ]/γ89 [Dab + Dc2 ]. Kij 1, one would expect 89 T1ab /17 T1c → γ17 Inserting parameter values from Table 4.1, we ﬁnd a limiting ratio of 2360, as compared with the experimental ratio of 1305 at T = 300 K (Fig. 4.10) [10]. It seems, then, that the estimated rate 1/89 T1 is too small by as much as a factor ∼ 2 when analyzed on the same basis as the 17 O(2,3). On the other hand, this analysis has some positive points. First, the anisotropy of 89 T1 according to the model (3.5.22) is given by 89 T1c /89 T1ab = 2 2 [Dab + Dc2 ]/[2Dab ] 1.17 by the data in Table 4.1. With modest error bars on that value, the data in Fig. 4.10 are in reasonable agreement with the latter estimate for both YBCO7 and YBCO6.63 and at all temperatures shown. Furthermore, when correlations become important at low temperatures, one would certainly expect that [1 + 2K01 + K12 + KIC ] < [1 + K01 ].

(4.1.10)

One would therefore expect 89 T1α /17 T1α to increase at low T, as it does in Fig. 4.10(b). If we examine the eﬀects of dipolar terms, in the case of negligible correlations they add less than 10% to the estimated rates. The case of dipolar

4.1 The Pseudogap in Oxygen–Deﬁcient YBCO7-x

89W (sec–1K–1)

x10–4 O7

2

89W ab 89W c 17W c

0.4

0.2

1 89

O6.63

(a) 0

100

0

200

Wab

–1 –1 c (sec K )

0.6

17W

3

133

89

Wc 17W c 300

0

T(K)

R = 17Wc / 89Wc

2000

1800

1600

O6.63 O7

1400 (b) 1200

0

100

200

300

T(K)

Fig. 4.10. (a) Data for 1/T1 T for 89 Y (89 Wab,c ) in both YBCO7 (O7 ) and YBCO6.63 (O6.63 ) and for both “ab” and “c” axis ﬁeld orientations are plotted from 100 K to above 300 K [10]. For comparison, 1/T1 T for 17 O(2,3) (17 Wc ), measured on the same samples, is also plotted. (b) With the same notation as in (a) the ratios R = 17 Wc /89 Wc are plotted for both compositions and the same temperature range. Figures reprinted from M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993). Copyright 1993 American Physical Society

terms in the presence of intraplanar and interplanar correlations has been discussed in detail by Takigawa et al. [10]. While they could become signiﬁcant in such a case, they have the opposite anistropy to the Dα ’s, which is a serious drawback. One cannot see how a calculation based entirely on the model Hamiltonian (3.3.2) can heal the disparity in the estimated T1 for 89 Y. Additional calculations with the full dipolar Hamiltonian have been performed by Auler et al. [15], where a substantial dipolar contribution to the 89 Y relaxation was estimated. These results are discussed in Sect. 5.3. Another possible answer for the 89 Y T1 problem is that there may be enough Y(3d)-hole character hybridized into the Cu2+ spin states to generate

134

4 Pseudogap Eﬀects in Cuprate NMR Studies

a signiﬁcant orbital T1 eﬀect. After all, the measured Dα coeﬃcients in Table 4.1 are undoubtedly the result of such an hybridization, which has its main eﬀect through the core-polarization term. The orbital HF eﬀects are typically of the same order, but are probably more nearly isotropic. Since there is no Fermi-surface orbital shift eﬀect related to the orbital T1 term, the latter would just appear as a “background” relaxation eﬀect unrelated to the spin HF eﬀects. There could also be a small Van Vleck orbital NMR shift as part of the positive, temperature-independent chemical shifts recorded for the 89 Y. We turn now to pseudogap phenomenology as seen with other probes.

4.2 Pseudogap Phenomenology with Other Probes In this section we address brieﬂy several topics relating to pseudogap eﬀects in the cuprates, but not directly related to NMR. Thus, we are discussing “background material”, the point of which is to give a deeper context in which to present and discuss the NMR results. It is essential to point out that pseudogap eﬀects have been observed and studied in great detail with several other techniques. In particular, it is interesting to note that the presence of the pseudogap is felt in both spin and charge-based properties. One example is the in-plane conductivity σab (T ) of underdoped YBCO at 250 cm−1 , which according to Rotter et al. [26] exhibits a gap-like feature at low temperatures very similar to 1/T1 T for 89 Y and 17 O(2,3) for that case (see Figs. 4.1(b) and 4.9(a)). A clearly presented review of pseudogap eﬀects has been given by Randeria [27]. 4.2.1 Pseudogap Eﬀects in the Electronic Speciﬁc Heat We oﬀer brief descriptions of experimental results which detect and elucidate the pseudogap eﬀect in cuprates, the ﬁrst of which is the electronic speciﬁc heat. By using a very precise diﬀerential technique, J.W. Loram and co-workers have produced an extraordinarily clear and detailed picture of the behavior of low-energy electronic states in the cuprates [28, 29, 30]. We review here a selection of their results on YBCO7-δ. A sampling of speciﬁc heat results is shown in Fig. 4.11(a) and (b). In (a) one sees that, ﬁrst, the peak in γ el (T) (≡ Cp (T )/T ) at Tc gradually vanishes as δ is increased from 0, and simultaneously a pseudogap maximum appears at temperatures T Tc , causing γ el to decline as it approaches Tc from above. The peak at Tc makes a rather weak reappearance at Tc ∼ 60 K, then declines further as superconductivity fades away at larger δ values. T In Fig. 4.11(c) the entropy S el = 0 γ el (T )dT is plotted as S el /T vs. T. Such a plot closely resembles γ el (T ). The superconducting gap feature is very pronounced for δ 1, persisting up to δ ∼ 0.20. Then entropy loss at T > Tc becomes a major feature, namely the pseudogap, as δ increases, while

4.2 Pseudogap Phenomenology with Other Probes

135

7

δ

6

0.08

0.03

(a)

5 0.13

4 3

0.20

γel (mJ / g-at K2)

2

0.24 0.27

1 0

(b)

0.20 2

0.24 0.43 0.52 0.57

0.27 1

0.62 0

0

50

100

150

0.71

0.84

200

250

T(K) 2

δ 0.03 0.08 0.13 0.20 0.24 0.27 0.33 0.43 0.52 0.57

Sel / T (mJ / g-at K2)

1.5

1

0.62 0.71 0.84

(c) 0.03 0.13 0.20 0.43 0.52 0.57

0.5

0.62 0.71 0.84

0

0

50

100

150 T(K)

200

250

300

Fig. 4.11. (a) and (b) Data for the electronic speciﬁc heat coeﬃcient γ el of YBCO7δ, obtained via diﬀerential measurements with YBCO6.0, are plotted for diﬀerent doping levels δ as a function of temperature up to 250 K [30]. In (b) there is clear

136

4 Pseudogap Eﬀects in Cuprate NMR Studies

the decline in S el /T begins at ever higher temperatures. Note, however, that a vestige of the superconducting gap feature beginning at T ∼ Tc remains in place until superconductivity disappears altogether. These eﬀects on γ el and S el (T) seem to be entirely consistent with what one would expect based on the spin susceptibility and low-energy spin excitations reﬂected in the 1/T1 T results given in Sect. 4.1. Loram et al. present a companion set of spin susceptibility curves [30] to conﬁrm this point. There is a clear conclusion here of non-separation of spin and charge behavior, contrary to some of the early models of high-Tc properties [31, 32]. 4.2.2 ARPES Studies of Pseudogapped Cuprates Angle-resolved photoemission studies (ARPES) on cuprates exhibiting pseudogap eﬀects have also given a great deal of insight into the microscopic physics of cuprate superconductors as well as the pseudogap phenomena per se. Since this method oﬀers good resolution of energies as well as of k values, one is able to study both gap energies and their anisotropy over the Fermi surface. Extensive investigations of the cuprate properties have been conducted. We shall brieﬂy review studies of pseudogap eﬀects in the Bi2212 family of superconductors by Harris, Shen et al. [33, 34, 35]. What ARPES reveals is not only that gaps appear anisotropically around the Fermi surface, but also that quasiparticle peaks in the normal state are greatly diminished. They appear mainly at temperatures below Tc . Gap energies are measured, then, as the distance between EF and the “leading edge midpoint” of the photoemission intensity. The pseudogap is found to behave in similar fashion to a d-wave superconducting gap, namely to be at its maximum along the cut from (π, 0) to (π, π) and to vanish along the diagonal cut (0, 0) to (π, π). With that in mind, we examine the temperature dependence of experimental gap data, which oﬀers some insight into the relation between the pseudogap behavior and that of the superconducting gap which sets in below Tc . Harris et al. reported a study of Bi2 Sr2 Ca1−x Dyx Cu2 O8+δ untwinned thinﬁlm crystals with variable doping controlled by the parameters x and δ [33]. Fig. 4.11. (Continued) evidence for a pseudogap creating broad maxima in γ el at progressively higher temperatures with increasing carrier dilution. (c) The quantity S el /T, where S el is the electronic entropy calculated from the data in (a) and (b), is plotted as a function of temperature up to 300 K. The superconducting gaps occurring at Tc as well as the pseudogap eﬀects in these data are discussed in the text. Figure reprinted from W.Y. Liang, J.W. Loram, Physica C 263, 277 (1996). Copyright 1996 Physica C

4.2 Pseudogap Phenomenology with Other Probes

137

Their gap energy data scans extend over 1/8 of the (2D) Fermi surface.5 Two separate doping levels yielded a sample with a “strong” pseudogap eﬀect (Tc = 42 K) and a second one with a much “weaker” pseudogap (Tc = 78 K), where “strong” and “weak” are to be deﬁned presently. In Fig. 4.12(a) and (b) experimental gap energies are shown along an arc of the Fermi surface which extends from the diagonal (0.4, 0.4)π) where the abscissa is zero to (1, 0.2)π, where it is nearly one. The abscissa is deﬁned as 0.5|cos kx a-cos ky a|, which would yield a linear variation of gap energy with a d-wave (dx2 −y2 ) superconducting gap. For the data in Fig. 4.12(a), the superconducting state data (closed circles) show a nearly linear variation of gap energy along this path. In a conventional superconductor there would be no gap energy above Tc ; thus, the curve would remain ﬂat. However, this Tc = 78 K sample has a “weak” pseudogap, such that substantial gap energies occur

30

25 leading edge midpoint (meV)

10%Dy-BSCCO Tc = 46 K

10%Dy-BSCCO Tc = 78 K

20

13K

13K

100K

75K

150K

150K

15

(a)

(b) 10

5 0 0

0.2 0.4 0.6 0.8

1 0

0.2 0.4 0.6 0.8

1

0.5Icoskxa – coskyal

Fig. 4.12. ARPES measurements of gap energies, taken as decribed in the text on untwinned thin ﬁlm crystals of Bi2 Sr2 Ca1−x Dyx Cu2 O8+δ . In (a), gap variation results are shown along the Fermi surface at three temperatures for a “strong” pseudogap composition, and in (b) gap energies are shown at three temperatures for a “weak” pseudogap system, as described and discussed in the text. Figure reprinted from J.M. Harris, Z.-X. Shen, et al, Phys. Rev. B54, R15665 (1996). Copyright 1996 American Physical Society

5

The region of k-space considered is triangular, extending from (0,0) to (π,0), then to (π, π) and back to (0,0). The Fermi surface is an arc extending from ∼(0.4,0.4)π on the diagonal around to the point ∼(1,0.2)π on the (0,π) - (π, π) axis.

138

4 Pseudogap Eﬀects in Cuprate NMR Studies

at 100 K and 150 K, but which behave only qualitatively like the superconducting gap. On the other hand, the Tc = 46 K sample exhibits a “strong” pseudogap, which means that the gap energy proﬁle shown is the same both above and below Tc , exhibiting a ﬂat region near the null (abscissa = 0) and rising to a maximum which is the same near the point (1,0.2)π both above and below Tc . At 150 K the gap energy shows a small decline. Thus, with a “strong” pseudogap, the gap energy proﬁle in k–space is very nearly the same above and below Tc . For either a weak or strong pseudogap, the gap energy behaves in k–space in a very similar fashion to a superconducting gap, giving the impression that these eﬀects are related. At what temperature, then, does the energy gap ﬁnally collapse in an underdoped sample? An experimental answer to this question was given in [33], where measured gap energies at the maximum point were plotted vs. temperature up to T = 250 K on a sample with Tc = 85 K. Over this range of T the pseudogap declines completely to zero, beginning somewhere below Tc . The anisotropic gap behavior found in this system and presumably occurring widely in the cuprates would have interesting consequences for the behavior of χ (q, ω) and therefore for T1 measurements of pseudogap systems. Although to our knowledge no such calculation has been reported, it seems very likely that the observed anisotropy of gap eﬀects over k space would result in some distribution of gapping eﬀects in q space as well. Speculating about the consequences of this, it seems likely that nuclei such as 89 Y and 17 O(2,3) in YBCO, which depend for relaxation on q values over the entire zone except near the (0,π) axes would therefore always be subject to pseudogap eﬀects. On the other hand, the pseudogap anisotropy may allow situations where the ﬂuctuations peak strongly at (π, π) and are driven by k vectors on or near the diagonals. Such behavior could tend to dominate the planar 63 Cu T1 process, which would not then be strongly aﬀected by the pseudogap behavior. Such a case is found for La2−x Srx CuO4 , as will be discussed in Sect. 4.4.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) Another pseudogap system which has been studied intensively is Y248, a superconductor which is unique among the cuprates in having a ﬁxed, stoichiometric carrier doping level, which pegs it as slightly underdoped. It appears to have a pseudogap not unlike that of YBCO6.63 presented in Sect. 4.1. The structure of Y248 is closely related to YBCO7, except that there are two oxygenated chain layers between the pairs of CuO2 planes instead of one. Cu(1) sites in the chain layers are staggered along the b (chain) axis, so that the b-axis oxygen sites O(4) for one chain are apical oxygens for Cu(1) sites in the neighboring chain. Thus, planar arrays separated by a double chain layer

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

139

˚ high [36]. This structure of are also staggered, making the unit cell ∼ 27A chains is unusually stable, as the chain oxygens remain bound in the crystal up to temperatures beyond 700 K. Thus, Y248 is a nearly ideal cuprate on which to conduct high-temperature studies. The equilibrium stoichiometric structure of Y248 also yields unusually narrow NMR lines, oﬀering the possibility of high-precision NMR studies. We shall see some examples of this in Sect. 4.3.2. It is very diﬃcult to measure the ratio of mobile holes which occupy the Cu(1) and Cu(2) regions of the Y248 structure. It is, however, useful to estimate the doping level with the simple valence method. Assigning the usual valences, there is a single mobile hole per formula unit of YBa2 Cu4 O8 , which gives 0.25 carrier holes per Cu ion. With YBCO6.63, by comparison, the situation is more complicated in that 63% of the chain sites are oxygenated Cu2+ and 37% are two-fold coordinated Cu+ ions. On that basis one calculates 0.24 mobile holes per Cu2+ ion, giving very nearly equal doping for these two systems. There are marked diﬀerences in Tc , however, which is ∼ 81 K for the “best” samples of Y248, but only 60-65 K for YBCO6.63. As we shall see, there are other important diﬀerences as well. 4.3.1 NMR Shift and Relaxation Behavior in Y248 It is both interesting and informative to compare the pseudogap character of Y248 with that of YBCO6.63 and other systems. Owing to the simple and seemingly immutable character of this compound, a large responsibility seems to have been placed upon it and a great deal expected of it. Here we examine the general behavior of the pseudogap eﬀect as reﬂected in NMR shift (i.e. susceptibility) and relaxation data. Our point of reference will be the simple behavior found for YBCO6.63 as reﬂected by the data in Figs. 4.4 and 4.9. As concerns the immutability issue, we shall consider the reproducibility of experimental measurements in data from several research groups. Let us ﬁrst look at the overall relaxation behavior in Fig. 4.13. The log scales give a broad overview of the Cu(1,2) sites both above and below Tc [37]. The Cu(1) relaxation rate crosses through Tc looking Korringa-like, much as it did in YBCO7. For the Cu(2) there is a near discontinuity of slope at Tc which is much more pronounced than in the YBCO6.63 data of Fig. 4.9. Below Tc there is a steep drop into a very brief T 3 region, which then ﬂattens into a presumably disorder-related (i.e. states in the gap) Korringa runout below ∼ 20 K. Above Tc there is a near-Korringa stretch which ﬂattens into a very gradual increase above ∼ 200 K. Similar data have been given by Zimmerman et al. [38]. Apart from the pseudogap onset point around ∼ 200 K, the normal state behavior is quite featureless. Nonetheless, it is useful to have data extending as high as 700 K. For another view of 63 Cu(2) data for Y248 see the presentation by Yasuoka [39]. In Fig. 4.14 similar data for 63 Cu(2) are plotted as 1/T1 T vs. T [40]. These data were also taken with NQR, but on a diﬀerent sample, and are

140

4 Pseudogap Eﬀects in Cuprate NMR Studies

Spin-lattice relaxation rate 1 / T1(sec–1)

10000 YBa2Cu4O8 Cu(1) site Cu(2) site

1000

Tc

100

10

1

.1

1

10 100 Temperature (K)

1000

Fig. 4.13. NQR results for 1/T1 vs. T are shown for the 63 Cu(1) and 63 Cu(2) sites in Y248 and for temperatures ranging from 4.2 K up to 700 K [37]. The log-log plot emphasizes major features in the data. See text for detailed discussion. Figure reprinted from T. Machi, I. Tomeno, et al, Physica C173, 32 (1991). Copyright 1991 Physica C

in good agreement with Fig. 4.13. In Fig. 4.14, data for the 17 O(2,3) are compared with those for 63 Cu(2) up to 250 K. The 17 O(2,3) data also show a very deﬁnite kink at Tc , below which they fall well below the corresponding curve for YBCO6.63. Recall that the latter 17 O(2,3) T1 data in Fig. 4.9(a) show no feature whatever at Tc . The pseudogap eﬀect in Y248 is therefore somewhat like the Tc = 78 K BSCCO sample in Fig. 4.12(b) for which the superconducting gap has its own distinct character, while YBCO6.63 is like the Tc = 46 K (a) sample in that same ﬁgure, where the SC gap is completely merged into the pseudogap. In contrast with T1 data, neither the Cu(2) NMR shift [37] nor that of the 17 O(2,3) shown any abrupt change at Tc . The latter shift data 17 Ki,c (T ), i = 2 and 3, are shown in Fig. 4.15 where, unlike the case of YBCO6.63, they are resolved and separately measurable. The latter data presumably oﬀer a reasonable measure of the pseudogap, but unfortunately these data have a very large, negative intercept at T = 0, and no value of the zero shift has been given for either site. We shall make some guesses about the T = 0 shifts and diamagnetic corrections in our analysis below. Another peculiar feature of the latter 17 O(2,3) NMR shift data is the fact that these two sites have distinct and well-resolved T = 0 shift values, but as

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248) Cu(2)

0.25

141

7

0.20

5

0.15

4 O(2,3) 3

0.10

2 0.05

1

Tc = 81K 0.00

0

50

100

(83T1T)–1 (sec–1 K–1)

(17T1T)–1 (sec–1 K–1)

6

150

200

250

0 300

Temperature (K)

Fig. 4.14. Relaxation data for both 63 Cu(2) and 17 O(2,3) in Y248 are plotted as 1/T1 T vs. T , showing detailed behavior near Tc . Like the 63 Cu(2) plot in Fig. 4.13, the planar 17 O show a visible break in slope at Tc . Figure reprinted from I. Tomeno, T. Machi, et al., Phys. Rev. B49, 15327 (1994). Copyright 1994 American Physical Society

the temperature rises above Tc the two lines gradually merge together. This could be entirely coincidental, resulting from slightly diﬀerent HF coeﬃcients. Alternatively, there could be chemical migration of O2− ions in the CuO2 −1 planes at a rate τcm which increases with temperature and eventually becomes fast enough (4.3.1) γ17 HΔK2,3 τcm 1 , so that the two NMR lines merge into one. The latter possibility seems a bit remarkable, but would avoid an even more remarkable coincidence with the HF coeﬃcients. It would be easy to test the chemical migration hypothesis with selective saturation techniques. As far as we know this has not been done. We now inquire as to whether the Y248 NMR shift data can provide a simple measure of the pseudogap energy, as they did for YBCO6.63 (see the inset to Fig. 4.4). Accordingly, several NMR shift data sets are plotted as ln(K(T)) vs. 1000/T in Fig. 4.16 for temperatures down to Tc . The linear slope of such a plot gives one measure of the pseudogap energy. The data shown here have been scaled up and down for display purposes. At the top we see data set (i), 17 Kc,ab (T ) and 65 Kab (T ) (triangles, diamonds and circles) from Bankay et al. [41]. The straight line drawn through these points deﬁnes a gap energy TG 84 K, which is ∼ 20% smaller than that of YBCO6.63. The open and ﬁlled squares are both plots of the data for 17 O(3) from Fig. 4.15, with two diﬀerent assumptions regarding 17 K3,c (0). In (ii) 17 K3,c (0) is assumed to be -0.04%, with a diamagnetic correction of -0.005%, while in (iii) it is assumed to be -0.02% with a diamagnetic correction of -0.025%. Both assumptions

142

4 Pseudogap Eﬀects in Cuprate NMR Studies 0.15 YBa2Cu4O8

17K

i,c (%)

0.10

0.05

17K

0.00 Tc = 81K –0.05

0

50

100 150 200 Temperature (K)

2,c

17K

3,c

250

300

Fig. 4.15. 17 O(2,3) NMR shift data for Y248 are plotted vs. T for temperatures up to 300 K [37]. Note that the O(2) and O(3) NMR lines are resolved below T ∼ 150 K, but merge above that point. See text for discussion and possible interpretation. Figure reprinted from T. Machi, I. Tomeno, et al, Physica C173, 32 (1991). Copyright 1991 Physica C

lead to a reasonable straight line, with TG 96 K and 106 K for (ii) and (iii), respectively. Option (ii) probably makes better physical sense and gives a gap energy closer to that of data set (i). Our main conclusion from plots (i)-(iii) is that Y248 NMR shifts show Arrhenius-type behavior with pseudogap energies 10-20% smaller than YBCO6.63. Data plot (iv) in Fig. 4.16 shows the 89 Y NMR shift data by Williams et al. [42], which the authors presented in a proposed test of the pseudogap isotope eﬀect. The undiﬀerentiated data points shown are for both 16 O and 18 O-doped samples, which gave indistinguishable behavior over the range of temperatures (131 K - 370 K) shown. The data are very precisely measured as one can see from the small scatter of the points, but the most striking thing is, ﬁrst, how diﬀerently these 89 Y data points behave compared with the other two data sets, and secondly, that they do not appear to correspond to a welldeﬁned gap energy in this kind of plot. Noting that in a stoichiometric sample of Y248 with low disorder one would expect NMR shifts of the 89 Y, 17 O(2,3), and 63,65 Cu(2) to follow a common temperature dependence as they did in YBCO6.63 (Fig. 4.4), the results shown suggest that the sample material used for data set (iv) is somewhat diﬀerent from that used for data sets (i)-(iii). In the following subsection we review eﬀorts which have been reported to measure the pseudogap isotope eﬀect in Y248.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

143

1

YBa2Cu4O8 (Scaled)

(i)

(ii)

17K, 63K, 89K

(iii) (iv)

0.1 0

2

4 1000/T

6 (10–3

8

10

12

K–1)

Fig. 4.16. An Arrhenius plot of several sets of NMR shift data for Y248 is presented to make estimates of the pseudogap energy for the density of states. The data are scaled to arbitrary positions along the vertical axis for display purposes. The data shown are, set (i): 17 Kab (T ) (triangles), 17 Kc (T ) (diamonds), 65 Kab (T ) (circles) from [41]; set (ii) and (iii) (same data, see text) 17 Kc (T ) (open and closed squares) from [40]; and set (iv) 89 Kc (T ) (dots) from [42]. The lines drawn are approximate ﬁts to the data for the purpose of extracting pseudogap energies from the slopes

4.3.2 Measuring the Pseudogap Isotope Eﬀect in Y248 with NMR The 89 Y data set (iv) in Fig. 4.16 were reported as part of an eﬀort to evaluate the isotope eﬀect, if any, on the pseudogap and on Tc in Y248 [42]. The samples employed for that purpose were annealed with 16 O and and with 18 O, respectively, and were found to have Tc (16 O) - Tc (18 O) 0.65 K, in reasonable agreement with previous work [43]. The shift data, as noted in the previous subsection, show no isotope eﬀect to the unaided eye for T > 130 K, while undergoing a pseudogap-related decrease of ∼ 40% from their peak values at 370 K. It is interesting at this point to inquire as to how large a change in the NMR shift curve is expected if the isotope eﬀect on the pseudogap temperature Tg is the same as that on Tc . First, let us deﬁne αc,g = dln(Tg,c )/dln(M ), where M is the oxygen atomic weight. Note that if αc = αg , then ΔTg /Tg = ΔTc /Tc . We shall now use this in a very simple way to estimate the change which might be expected in the 89 Y NMR shift curve. If we consider the gap function K(T) = K0 exp(−Tg /T ) (or any function purely of Tg /T ), then the temperature interval ΔT between equal values of shift for the two curves is |ΔT /T | = |ΔTg /Tg |. The ﬁts to shift data in Fig. 4.16 gave Tg ∼ 90 K; at T = 130 K, then, we expect curves

144

4 Pseudogap Eﬀects in Cuprate NMR Studies

shifted by ΔT ∼ 1.1 K.6 At the lower end of the data curve the slope is ∼ 1 ppm/K, leading one to expect deviations with the foregoing temperature shift of ∼ 1 ppm. As the inset shows, there are deviations of that order, but the ﬂuctuations are large. To resolve such an eﬀect would require a very precise ﬁtting curve and a large number of data points. In the light of the analysis given below for a diﬀerent experimental eﬀort to achieve the same end, we suggest that the 89 Y NMR shift data given were excellent, but the foregoing analysis in the present case does not quite rule out the possibility of a pseudogap isotope eﬀect. A second eﬀort to measure the pseudogap isotope eﬀect was made via NQR studies of the 63 Cu(2) relaxation curve for Y124, with the basic data plot of 1/T1T vs. T shown in Fig. 4.18(b) [44]. The data shown are for two samples, one with 16 O and one with ∼ 90%18 O, as in the previous case. The peaks in the two curves are seen to occur at T ∼ 150 K, where there is a razorthin margin between the curves ﬁtted to the two sets of data. The measured diﬀerence in Tc values ∼ 0.47 K for the 16 O and 18 O samples is slightly smaller than in the previous case. The key to analyzing the isotope eﬀect here is to ﬁnd a precise functional ﬁt to the data curves. For this purpose the authors have used Δ C 1 2 = 1 − tanh , (4.3.2) 63 T T Ta 2kB T 1 where the factor T −a , a ∼ 1, ﬁts the Curie-like decline of 1/T1 T at high temperatures, and Δ = kB T ∗ acts as the spin pseudogap energy - see discussion below. The data are a good ﬁt to (4.3.2), but the deviations were not quite random. The authors have therefore tinkered with the temperature scale a bit [44] and thus achieved the high-quality ﬁt to the data shown in Fig. 4.18. This ﬁt gives a shift in T ∗ for the two samples tested of 0.96 K. It is interesting that this temperature shift is less than was predicted for the 89 Y NMR shift curves in Fig. 4.17, but was resolved using a precisely ﬁtting function and a large number of data points. The pseudogap energy value turned out to be T ∗ = 246.9 K for the 1/T1 T curves [44]. This is more than twice the values found with the Arrhenius plots in Fig. 4.16. Further, although (4.3.2) is just a ﬁtting function, T ∗ really serves as an energy gap, since the asymptotic form of (4.3.2) is 1/T1 T ∝ T −a exp(−T ∗ /T ) for T ∗ /T 1. Note, however, that the NMR shifts represent the residual density of states, whereas T ∗ may represent the DOS squared. The appropriate comparison would then be between T ∗ /2 and Tg ∼ 90 K from the NMR shift results. This point of view does not appear, however, to be supported by pseudogap theory [45] (see the following subsection). It seems, then, at least for the dynamics that there is a pseudogap isotope eﬀect which is similar to that of Tc . As far as we are aware, there is no 6

This estimate is somewhat smaller than that of the authors [42], which is not stated explicitly.

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

145

( Y(18O)–89Y(16O)) (ppm)

40 20 0 –20

– 89

–89Y

NMR Shift (ppm)

60

–40 150

1.0 0.5 0.0 –0.5

200 300 Temperature (K)

200 250 300 Temperature (K)

350

Fig. 4.17. 89 Y NMR shift data measured on two samples of Y124, one with nearly 100% 16 O (+ symbols) and the other with 94% 18 O (circles) [42]. The diﬀerence between these data plots is clearly smaller than the plotting symbols. Inset: Plot of the diﬀerences along with calculated diﬀerence curves. See text for discussion. Figure reprinted from G.V.M. Williams, et al., Phys. Rev. Lett. 80, 377 (1998). Copyright 1998 American Physical Society

(T1T)–1 (s–1T–1)

20

18 21

16 20

14

12

19 100

100

140

180

300

200 T(K)

Fig. 4.18. T1 data are plotted as 1/T1 T vs. T for two samples of Y124, one with 16 O and the other with ∼ 88% 18 O [44]. Using the functional ﬁt shown (see text) the diﬀerence in these two relaxation curves near their peak at T ∼ 150 K is analyzed to ﬁnd a diﬀerence in the pseudogaps roughly equal to that found for Tc . See text for detailed discussion. Inset: Detailed view of the peak vicinity. Figure reprinted from F. Raﬀa, T. Ohno, et al., Phys. Rev. Lett. 81, 5192 (1998). Copyright 1998 American Physical Society

146

4 Pseudogap Eﬀects in Cuprate NMR Studies

theoretical prediction available for the variation of the pseudogap with the atomic weight of the oxygen. 4.3.3 Theory of the Pseudogap by Varma. The only successful theory of the pseudogap which we are aware of is that by Varma [45]. Varma has constructed a theory of cuprate superconductivity and ancillary properties, based on the existence of a quantum critical point (QCP) at the center of the superconducting dome of the phase diagram shown in Fig. 4.19, where the abscissa is the doping level or carrier concentration in the CuO2 planes. Region I is the marginal Fermi liquid regime proposed and expounded in [46]. The pseudogap eﬀects occur in Region II below the line Tp (x) [45]. In Region II there is a broken symmetry based on time-reversal violating (TRV) states in which ﬂuctuating currents ﬂow in the CuO2 plane. The existence of such currents has been veriﬁed experimentally via neutronscattering experiments [47]. The aforesaid theory also predicts anisotropic gapping in k-space near the chemical potential in Region II of the phase diagram, as was depicted by the gapping curves in Sect. 4.2.2. Corresponding calculations of the density of states in the pseudogap regime have been presented for comparison with experimental data on Y248. In Fig. 4.20 the 89 Y NMR shift data from [42] (see

T Pseudogapped metal

Tp

II

Crossover

Marginal Fermi liquid

I

III Fermi liquid

AFM

x (doping) QCP Superconductivity

Fig. 4.19. Phase diagram of doped cuprates showing the putative quantum critical point at the center of the superconducting dome [45]. From normal metal behavior at high doping levels (III), there is a crossover to the marginal Fermi liquid behavior in (I) followed by pseudogap behavior below the line Tp (x) emanating from the QCP. The calculations presented in [45] are for Region II. Figure reprinted from C.M. Varma, Phys. Rev. B73, 155113 (2006). Copyright 2006 American Physical Society

4.3 Pseudogap Behavior of YBa2 Cu4 O8 (Y248)

147

T/TG 60

0.4

0.6

0.8

1.0

89Y

NMR Shift (ppm)

40 20 0

89Y in YBa2Cu4O8

–20 –40 100

200

300

400

T(k)

Fig. 4.20. The 89 Y NMR shift data from Y248 (see Fig. 4.17) is shown here ﬁtted by the pseudogap theory given by Varma [45] (solid line), yielding an excellent ﬁt

Fig. 4.17) are compared with a calculated pseudogapped density of states from [45], where an excellent correspondence is seen to occur. It would, of course, be most interesting if more detailed calculations of, e.g. χ (q, ω) would be forthcoming, for comparison with the q-dependent relaxation eﬀects in these systems. 4.3.4 Eﬀect of Zn impurities on the Pseudogap in Y248 From early on it has been known that Zn impurities – thought to substitute for the Cu(2) – cause a dramatic reduction of Tc in high-Tc cuprates [48]. Even though Zn2+ is a nonmagnetic ion core, its presence in the CuO2 plane (as well as Li+ ) is thought to cause potential scattering which destroys d-wave pairs, and it also causes the occurrence of a small localized magnetic moment in the same vicinity [49]. The latter is a very interesting eﬀect in its own right, even exhibiting a Kondo eﬀect [50, 51]. The strategy of Zn-doping to eliminate the eﬀect of the SC transition on the pseudogap was adopted by Zheng et al. [52]. However, instead of the collapse of AFM spin ﬂuctuations as found with YBCO7-x, the Zn-doped Y248 undergoes an enhancement of 1/T1 for 63,65 Cu similar to the ”CurieWeiss” behavior of T1 T in LSCO:x [53], as shown in Fig. 4.21. With 2% Zn substitution, the peak value of 1/T1 T is almost three times the peak value of that quantity in the undoped case. Meanwhile, the NMR shift proﬁle remains spin-gapped with eﬀectively no change [52], in spite of a reduction of Tc by a factor ∼ 3. The latter result suggests that the SC transition was already having very little eﬀect on the shift proﬁle in the undoped case.

148

4 Pseudogap Eﬀects in Cuprate NMR Studies

1/ T1T (sec–1K–1)

20 YBa2(Cu1–xZnx)4O8 : X=0 : X = 0.01 : X = 0.02 10

0

200 100 Temperature (K)

300

Fig. 4.21. A plot of data for 1/T1 T for 63 Cu(2) in Y248 made with samples which are undoped (open circles) and doped with 1% Zn (closed circles) and 2% Zn (closed diamonds), showing suppression of Tc from 74 K to 53 K and ∼ 27 K, respectively, combined with large progressive increases in the value of 1/T1 T at T = Tc [52]. The corresponding change in the NMR shift curve is slight and barely resolvable. Figure reprinted from G.–Q. Zheng, T. Odaguchi, T. Mito, Y. Kitaoka et al: J. Phys. Soc. Japan 62, 2591 (1993). Copyright 1993 Physical Society of Japan

The Zn impurities, while suppressing Tc , have the very speciﬁc eﬀect of un-gapping the Fermi surface regions which contribute to χ (q, ω) near q = (π, π), or so it would appear. In connection with these remarkable data, the results of two additional relaxation measurements would be of great interest. First, a comparative plot of T2g for the 63 Cu(2) over the same temperature range would give a direct measure of the doping eﬀect on χ (Q) (see Sect. 6.1). Second, the T1 behavior of either 89 Y or of 17 O(2,3) would test the eﬀect of Zn doping on low–frequency ﬂuctuations away from Q as a corroboration of the unchanged NMR shift results. In other words, these measurements would further test the scenario where the Zn doping eﬀect appears to be conﬁned to the region of the AFM peak.

4.4 “Pseudogap-like” Eﬀects in La2−xSrxCuO4 (LSCO:x) Apart from introducing the LSCO structure in Sect. 3.1, there has been up to this point no discussion of LSCO. In spite of its rather low Tc relative to other cuprates, LSCO played a major role in high-Tc physics research. This was because, (i) it was one of the ﬁrst cuprate structures identiﬁed [54], (ii) it has a very interesting and accessible phase diagram similar to Fig. 1.1, and (iii) it is relatively easy to make large, homogeneous single crystals of LSCO:x. For the latter reason a great many neutron scattering measurements have been conducted on this system, making its dynamic susceptibility perhaps the best

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

149

characterized of all of the cuprates. This will be discussed extensively, along with NMR measurements, in Chap. 6. From the standpoint of NMR technique, LSCO is a far simpler system to work with than YBCO. First, there are only one Cu2+ site and two O2− sites, making spectra and relaxation studies generally easier to interpret. For the purposes of conducting 17 O NMR studies in crystals, LSCO is also a favorable case, because it has very high oxygen mobility at relatively modest temperatures. Thus, it is easy to exchange 17 O into a crystal and homogenize it with simple annealing procedures. The foregoing circumstances notwithstanding, we shall see that the pseudogap eﬀect in LSCO is not quite the same as in the other cuprates. One rarely even ﬁnds the word pseudogap applied to LSCO, so we refer here instead to “pseudogap-like” eﬀects. While the NMR shift and susceptibility behavior is pseudogap-like (with important diﬀerences), the relaxation behavior of the 63 Cu is quite diﬀerent from that of YBCO6.63. On the other hand, the planar 17 O shift and relaxation appear to follow the spin susceptibility rather like the 17 O(2,3) data for YBCO6.63 in Fig. 4.9(a), making the overall picture pseudogap-like except for the 63 Cu T1 results. We now present a detailed account of these points. 4.4.1 Spin Susceptibility Scaling for La2−x Srx CuO4 . Around the time that the ﬁrst studies of underdoped YBCO7-x appeared, it was revealed by D.C. Johnston that the susceptibility of LSCO:x obeys a simple scaling law over essentially the entire range of superconducting compositions [7], χ(x, T ) = χ0 (x) + χs,max (x) Fs (T /Tmax (x)) + C(x)/T ,

(4.4.1)

where χ0 (x) is a temperature-independent background susceptibility, χs,max is the maximum spin susceptibility for composition x, which occurs at Tmax (x), and Fs (T /Tmax(x)) is a scaling function valid for 0.05 ≤ x ≤ 0.30 [7]. C(x) is a spurious Curie term which occurs at higher doping levels [55]. By deﬁnition, Fs (1) = 1. The term χ0 (x) represents Van Vleck orbital and diamagnetic contributions (see Sect. 2.3.2). The function Fs (T /Tmax (x)) is such that χ(x, T ) is qualitatively similar to the YBCO6.63 result in Fig. 4.4. To illustrate the behavior of χ(x, T ) for LSCO:x we display the somewhat more complete data set reported later by Nakano et al. [55] in Fig. 4.22 for 0.08 ≤ x ≤ 0.26, all superconducting samples. While the latter data extend up to ∼ 550 K, data from another study extending up to ∼ 1000 K show that χ(x, T ) for x ≤ 0.09 had no (accessible) maximum value, but all data plots for x > 0.09 exhibited a maximum at some temperature [56]. This CurieWeiss-like rise in susceptibilities at low temperatures for the higher doping levels is one factor which sets LSCO:x apart from the pseudogap behavior of other cuprates.

150

4 Pseudogap Eﬀects in Cuprate NMR Studies X = .26 La2–xSrxCuO4 χ (10–7 emu/g)

4

.22 .20 .18

2

.14 .10 .08

0

200

400

600

T(K)

Fig. 4.22. Susceptibility data for La2−x Srx CuO4 are plotted as a function of temperature for a series of random powder samples with 0.08 ≤ x ≤ 0.26 [55]. These data are found to scale as described in the text and in Fig. 4.23. Figure reprinted from T. Nakano et al., Phys. Rev. B49, 16000 (1994). Copyright 1994 American Physical Society

Nonetheless, there is a clear gap feature in χ(x, T ), which may be seen in Fig. 4.23, where χs (T )/χs,max = (χ(x, T ) − χ0 )/χs,max vs. T /Tmax is plotted [55]. The data for the eleven compounds shown follow this scaling curve to a remarkable degree. It seems highly plausible that this behavior is related to the pseudogap eﬀect identiﬁed in both YBCO6.63 and Y1248. This scaling of data may not reﬂect a simple energy gap parameter as in Fig. 4.4. The limiting, lowT behavior χs (T ) ∝ T β , β ∼ 0.5, is actually one of the predictions of Varma’s theory of the pseudogap [45], which was ﬁtted to the data in Fig. 4.20. It is interesting to examine the behavior of the other parameters in the ﬁt to (4.4.1). The values obtained for Tmax (x), χ0 (x), and C(x) are displayed as a function of x in Fig. 4.24(a). It is seen that there is a peculiar sort of transition point between data ﬁts for 0.10 ≤ x < 0.20 (Region I) and 0.20 ≤ x ≤ 0.28 (Region II). In Region I, Tmax declines in a roughly linear fashion7 from Tmax ∼ 700 K for x = 0.10 down to Tmax ∼ 100 K at x = 0.20. In region II, Tmax ∼ 100 K. In Region I, χ0 rises from a slightly negative value at x = 0.10 to χ0 ∼ 1.8×10−7 emu/g at x = 0.20 and remains constant above that point. Finally, C(x) = 0 in Region I, rising rapidly in Region II to where it becomes a major feature of the susceptibility data. Although there is no result given which identiﬁes χ0 (x) as the residual susceptibility at T Tc , we regard χs (T ) as the spin susceptibility. The magnetic behavior then distinguishes Regions I and II very clearly as “underdoped” and “overdoped”, respectively. In a more speculative vein, one could term these subcritical and supercritical relative to a putative quantum critical point at x 0.20. 7

There were no ﬁts to data below x = 0.10.

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

151

2 1

χs(T)/χs max

s s χ (T)/χ max

La2–xSrxCuO4

0

1

1

T/Tmax

X = 0.10 0.11 0.16 0.18 0.115 0.22 0.125 0.24 0.14 0.26 0.15 Universal Curve F

0

2 T/Tmax

5

4

Fig. 4.23. The data from Fig. 4.22 are plotted as χs (T )/χs,max vs. T /Tmax as deﬁned in (4.4.1). The resulting scaling curve deﬁnes the function Fs (T /Tmax (x)) from the latter equation as well, identiﬁed as “Universal Curve F” [55]. The inset shows that compared with previous scaling curves (e.g. [7]) represented by the dashed line, the present data decline more sharply as T → 0. As noted in the text, the theory by Varma [45] predicts χs (T ) ∝ T 1/2 near T = 0, very near to what is observed 800

(a) 400

1

χo (10–7emu/g)

Tmax(K)

2

0

C(10–7emu K/g)

0 60 La2–xSrxCuO4 40

(b)

20

0

0.1

0.2

0.3

X

Fig. 4.24. (a) The ﬁtting parameters Tmax (x) and χ0 (x), and (b) C(x) from (4.4.1) are plotted as a function of x for the series of ﬁts shown in Fig. 4.23 [55]. The behavior of these parameters clearly divides this doping range into regions I and II, where x 0.20 is the boundary line. See text for more discussion

152

4 Pseudogap Eﬀects in Cuprate NMR Studies

4.4.2 Behavior of the

17

O and

63

Cu NMR Shifts in LSCO:x.

Scaled 17 O NMR shift values are plotted as a function of temperature in Fig. 4.25 for x = 0.15 and 0.24 [55]. The shift data used for these plots are from Ishida et al. for x = 0.15 [57] and from Zheng et al. for x = 0.24 [58]. The lines drawn represent susceptibility data from [55], but the shift scales have been omitted from the ﬁgure. We note that the original data reﬂects c-axis shift coeﬃcients 50 − 60 kOe/μB , which is somewhat larger than the values of Cα for YBCO6.63 in Table 4.1. In both cases, the scaled 17 O shift values are a good quantitative match to the susceptibility data. Data for the 63 Cu c-axis NMR shifts in LSCO:x (not shown) have been found to have the following features [59]. With ﬁeld along the c axis, compositions in the superconducting range show a very nearly constant shift Kc 1.22% independent of temperature. For ﬁelds in the ab plane, shift data appear to follow the same trends as the susceptibility data in Fig. 4.22. Although to our knowledge they have not been scaled with susceptibility data as in Fig. 4.25, a simple estimate of ΔKab /Δχ gives a value Aab 149 kOe/μB , within 2-3% or so of the values given (Table4.1) for the composite 63 Cu(2) shift coeﬃcients in YBCO. For the Cu2+ at least, the Mila-Rice HF Hamiltonian from Sect. 3.3.3 appears to have near universal validity in the cuprates. The static spin-paramagnetic eﬀects for LSCO:x therefore behave in an internally consistent fashion, exhibiting a gap-like decline at low temperatures which becomes more pronounced at lower doping levels. The gapping feature is, however, superimposed on a Curie-Weiss-like increase at low temperatures which is often found in itinerant antiferromagnets. There is also a weak maximum in the susceptibility of the Cu(2) sites in YBCO7. Since the overdoped region is inaccessible for YBCO, one cannot say whether or not Curie-Weiss

La2–xSrxCuO4

χ (10–7 emu/g)

2

Tc 1

Tc x = 0.15 (K. Ishida et al.) x = 0.24 (G. –Q. Zheng et al.)

0

200 T(K)

400

Fig. 4.25. The 17 O NMR shifts measured for La2−x Srx CuO4 with x = 0.15 [57] and 0.24 [58] are ﬁtted to susceptibility curves such as those shown in Fig. 4.22 and plotted vs. temperature [55]. The scale of shift values is such that Cc = 50-60 kOe/μB

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

153

behavior is found there. Be that as it may, we shall now see that the Cu-site T1 behavior is distinctly diﬀerent for these two systems. 4.4.3

63

Cu NQR spectra and Contrasting T1 Behaviors in LSCO:x.

Whereas oxygen-deﬁcient YBCO7-x shows line-broadening caused by crystalline disorder, LSCO:x has nearly resolved 63 Cu NQR and NMR “impurity” lines attributable to sites neighboring the Sr2+ dopant ions. NQR spectra are shown in Fig. 4.26 for three Sr2+ doping levels [60]. The spectra have been analyzed into pairs of 63,65 Cu NQR lines representing sites neighboring the impurities and “bulk” Cu2+ sites away from the Sr2+ sites. Since the charge environment near a dopant site is quite diﬀerent from that of a bulk site, it is not surprising to ﬁnd a diﬀerent EFG at such sites. For a sample with x = 0.30 there is a very high probability that a Cu2+ site will have a Sr2+ neighbor, and the corresponding impurity line is now larger than the bulk line (see Fig. 4.26). Perhaps it is because of this high level of impurity-induced disorder in LSCO:x that Tc peaks at ∼1/2 the peak value for YBCO7-x. T1 Results for

63

Cu.

As noted earlier, the peak Tc value in LSCO:x also occurs in samples (x 0.15) with quite a pronounced pseudogap feature in the susceptibility. However, the T1 curve for 63 Cu in such a sample is shown in Fig. 4.27 is not unlike what is found for YBCO7, although the relaxation rate is nearly three times as great. There is a ﬂatter-than-linear characteristic in the normal state and a pronounced T 3 region in the superconducting state just below a region which is somewhat steeper than that. These measurements have been taken both on the bulk and impurity-neighbor NQR lines, with very similar results for both sites [60]. There is little indication of the spin-gapped nature of the susceptibility data in the behavior of T1 for this composition. Apart from the fact that the LSCO relaxation is ∼ 3 times faster, the results in Fig. 4.27 bear a strong resemblence to the YBCO7 results in Fig. 3.11. T1 and NMR Shift Results for

17

O.

The dynamic susceptibility χ (q, ω) for underdoped LSCO:x near q ∼ QAF = (π/a, π/a) is therefore not aﬀected by the static, uniform pseudogap eﬀect noted earlier. For the behavior of low-frequency excitations over the rest of the zone we look at T1 behavior of the planar 17 O nuclear spins. A plot of 1/T1 T for the planar 17 O in LSCO:0.15 is shown in Fig. 4.28, along with NMR shift data on the same system [61]. The 17 O data stand in sharp contrast with the 63 Cu results, where they are seen to follow the shift data, 1/T1 T ∝ Ks (T ). This is similar behavior to the 17 O(2,3) data for YBCO6.63 in Fig. 4.9(a), and therefore a “classic” pseudogap result. The 17 O data suggest that gapped excitations similar to those at q ∼ 0 occupy the bulk of the Brillouin zone, and only those near QAF are immune to the gapping eﬀect. The latter excitations

154

4 Pseudogap Eﬀects in Cuprate NMR Studies A

La2–xSrxCuO4

SPIN-ECHO INTENSITY (arbitrary units)

B x = 0.15

x = 0.20

x = 0.30

30

35 40 FREQUENCY (MHZ)

45

Fig. 4.26. NQR spectra for 63,65 Cu in LSCO:x are shown for three typical values of x. the spectra have been analyzed into a pair of “A” lines , which represent bulk material away from the doping centers, and a pair of “B” lines representing sites which have at least one Sr2+ neighbor. For each case there are two lines representing the two isotopes with their roughly 7:3 (63:65) abundance ratio. For x = 0.30 the B lines have well over half of the intensity. The dashed lines shown are Gaussian components in the spectrum which sum up to the solid lines drawn, giving a reasonable facsimile of the experimental spectra. Figure reprinted from K. Yoshimura, T. Imai, et al., J. Phys. Soc. Japan 58, 3057 (1989). Copyright 1989 Physical Society of Japan

must be very strong, however, as they dominate the ultra-fast relaxation of the 63 Cu. The LSCO:x system therefore exhibits a mixture of pseudogap and nonpseudogap-like features. However, it seems quite clear that the pseudogap eﬀect is present and well-deﬁned for LSCO:x, for both static, q = 0 behavior, as well as for low-frequency quasiparticle excitations over the bulk of the Brillouin zone. However, the Fermi surface, which is known to be diﬀerent from that of YBCO7, could very well be situated so that the dynamic susceptibility near (π, π) samples only the non-gapped regions (see discussion of this point in Sect. 4.2). Moreover, the AFM peak for LSCO:x=0.15 must be so large that it completely dominates the 63,65 Cu relaxation rate. The planar oxygen then evidently have a dramatically diﬀerent relaxation character.

4.4 “Pseudogap-like” Eﬀects in La2−x Srx CuO4 (LSCO:x)

155

104 Tc = 38 k

1/T1 (sec–1)

103

102

10

~T3

La1.85Sr0.15CuO4 1

1

102

10

103

T (K)

Fig. 4.27. Data are plotted for 1/T1 as a function of temperature for both the A (open circles) and B (closed circles) sites identiﬁed in Fig. 4.26 in a sample with x = 0.15. The two data sets, where comparable, are quite similar in character. The A-site measurements show a typical ﬂat region in the normal state, with a steep drop below Tc , then a T 3 region [60]. Very little evidence is seen of the pseudogap feature found in the susceptibility for this composition

0.20 2.5 0.15

2.0 1.5 La1.85Sr0.15CuO4

1.0

0.05

0.5 0.0

0.10

Ks17p(%)

(17T1pT)–1 (10–1sec–1K–1)

3.0

(17T1pT)–1

Ks

17p

0.00 0

50

100

150

200

250 300

Temperature(K)

Fig. 4.28. 1/T1 T data for the planar 17 O in the LSCO 0.15 system are plotted (solid circles, left axis) in comparison with scaled data on the same sample for Ks (T ) (open triangles, right axis), showing that these two quantities are proportional over the range 100 K ≤ T ≤ 200 K [61]. Note the sharp contrast in behavior between the 63 Cu relaxation, represented by the dotted line, and the planar 17 O in this system. Figure reprinted from R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994). Copyright 1994 American Physical Society

156

4 Pseudogap Eﬀects in Cuprate NMR Studies

There will be further discussion of relaxation eﬀects in LSCO:x in Chap. 6, where there is extensive discussion of INS results on this compound as well as of T2g data in connection with the quantum critical scaling model of Pines and co-workers.

References

1. W.W. Warren, Jr., R.E. Walstedt et al., Phys. Rev. Lett. 62, 1193 (1989) 116, 120 2. H. Alloul, T. Ohno, P. Mendels, Phys. Rev. Lett. 63, 1700 (1989) 116, 117, 118, 128, 132 3. M. Horvati´c, P. S´egransan, C. Berthier, Y. Berthier et al., Phys. Rev. B39, 7332 (1989) 116 4. H. Yasuoka, T. Imai, T. Shimizu, In Strong Correlations and Superconductivity, ed H. Fukuyama, S. Maekawa, A.P. Malozemoﬀ (Springer-Verlag, Berlin, 1989) See also H. Yasuoka, S. Kambe, et al., Physica B199&200, 278 (1994) 116 5. H. Alloul, A. Mahajan, H. Casalta, O. Klein, Phys. Rev. Lett. 70, 1171 (1993) 117, 128, 132 6. J. Friedel, Physica C153-155, 1610 (1988) 117 7. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 117, 149, 151 8. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B41, 9574 (1990) 118, 120, 127, 128 9. M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991) 118, 120, 121, 122, 12 10. M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993) 118, 122, 123, 124, 11. S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 120 12. B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 120, 126 13. H. Monien, D. Pines, M. Takigawa, Phys. Rev. B43, 258 (1991) 122, 124 14. A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 122 15. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 126, 133 16. F. Mila, T.M. Rice, Physica C157, 561 (1989) 126 17. R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 126, 128 18. M. Randeria, N. Trivedi, A. Moreo, R.T. Scalettar, Phys. Rev. Lett. 69, 2001 (1992) 126, 127, 129 19. J.M. Tranquada et al., Phys. Rev. B46, 5561 (1992) 126, 128, 129, 130 20. G. Balakrishnan, R. Dupree et al., J. Phys. C: Solid State Phys. 21 L847 (1988) 128 21. M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 128 22. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 127 23. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 127 24. P.M. Gehring, J.M. Tranquada, et al., Phys. Rev. B44, 2811 (1991) 128 25. J. Rossat-Mignod, et al., Physica B169, 58 (1991) 128 26. L.D. Rotter et al., Phys. Rev. Lett. 67, 2741 (1991) 134 27. M. Randeria, Precursor Pairing Correlations and Pseudogaps, [Varenna Lectures 1997]; cond-mat/9710223 134 28. J.W. Loram et al., Phys. Rev. Lett. 71, 1740 (1993) 134 29. J.W. Loram et al., Physica C 135-140 134 (1994) 134 30. W.Y. Liang, J.W. Loram, Physica C 263, 277 (1996) 134, 135, 136 31. P.W. Anderson, Science 235, 1196 (1987) 136 32. N. Nagaosa, P.A. Lee, Phys. Rev. B45, 966 (1992) 136

References 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60. 61.

157

J.M. Harris, Z.-X. Shen et al., Phys. Rev. B54, R15665 (1996) 136 A.G. Loeser et al., Science 273, 325 (1996) 136 H. Ding et al., Nature (London) 382, 51 (1996) 136 R.M. Hazen, in Physical Properties of High Temperature Superconductors, ed D.M. Ginsburg (World Scientiﬁc, Singapore, 1990), Vol. II, p.121 139 T. Machi, I. Tomeno, et al., Physica C173, 32 (1991) 139, 140, 142 H. Zimmerman, et al., Physica C159, 681 (1989) 139 H. Yasuoka, Hyperf. Int. 105, 27 (1997) 139 I. Tomeno, T. Machi et al., Phys. Rev. B49, 15327 (1994) 139, 143 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 141, 143 G.V. M. Williams et al., Phys. Rev. Lett. 80, 377 (1998) 142, 143, 144, 145, 146 J.P. Franck, in Physical Properties of High Temperature Superconductors, ed D.M. Ginsburg (World Scientiﬁc, Singapore, 1994), Vol. IV, p.189 143 F. Raﬀa, T. Ohno et al., Phys. Rev. Lett. 81, 5192 (1998) 144, 145 C.M. Varma, Phys. Rev. B73, 155113 (2006) 144, 146, 147, 150, 151 C.M. Varma, P. Littlewood et al., Phys. Rev. Lett. 63, 1996 (1989) 146 B. Fauqu´e et al., Phys. Rev. Lett. 97, 197001 (2006) 146 G. Xiao, M.Z. Cieplak et al., J. Phys. Soc. Japan 62, 2591 (1993) 147 A.V. Mahajan, H. Alloul, G. Collin, J.F. Marucco, Phys. Rev. Lett. 72, 3100 (1994) 147 J. Bobroﬀ, W.H. MacFarlane, H. Alloul, P. Mendels et al., Phys. Rev. Lett. 83, 4381 (1999) 147 W.H. MacFarlane, J. Bobroﬀ, H. Alloul, P. Mendels, N. Blanchard, Phys. Rev. Lett. 85, 1108 (2000) 147 G.–Q. Zheng, T. Odaguchi, T. Mito, Y. Kitaoka et al., J. Phys. Soc. Japan 62, 2591 (1993) 147, 148 S. Ohsugi, Y. Kitaoka, K. Ishida, G.-q. Zheng, K. Asayama, J. Phys. Soc. Japan 63,700 (1994) 147 R.J. Cava, R.B. Van Dover, B. Batlogg, E.A. Rietman, Phys. Rev. Lett. 58, 408 (1987) 148 T. Nakano et al., Phys. Rev. B49, 16000 (1994) 149, 150, 151, 152 R. Yoshizaki et al., Physica C 166, 417 (1990) 149 K. Ishida et al., J. Phys. Soc. Japan 60, 3516 (1991) 152 G.-q. Zheng, et al., Phys. Rev. Lett. 86, 4664 (2001) 152 S. Ohsugi, Y. Kitaoka, K. Ishida, G.-Q. Zheng, K. Asayama, J. Phys. Soc. Japan 63, 700 (1994) 152 K. Yoshimura, T. Imai et al., J. Phys. Soc. Japan 58, 3057 (1989) 153, 155 R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 153, 155

This page intentionally blank

5 Relaxation Models for Cuprate NMR

From the very beginning of cuprate NMR studies, it was clear that understanding the relaxation properties for all sites with nuclear spin species would be a major challenge for theorists and experimentalists alike. In Chap. 3 the Mila-Rice-Shastry model [1, 2] was presented, including the quantum-chemical basis for transferred HF couplings and the spin Hamiltonian treatment of local spin and orbital HF eﬀects at the Cu2+ sites. With the latter formulation a complete characterization of the NMR shift tensors for YBCO7 and YBCO6.63 has been carried out in Chaps. 3 and 4. Then, using general expressions for 1/T1 , Mila and Rice discussed T1 anisotropy for 63 Cu(2) in YBCO7 (Sect. 3.3.4). A simpliﬁed model given in Sect. 4.1.2 oﬀered an interpretation of T1 anisotropies and spin correlation eﬀects for the 89 Y and 17 O(2,3) sites. These developments set the stage for the most serious challenge, which is the locally-varying, overall temperature dependences of the T1 processes in these compounds. Such a panorama of complex relaxation behavior had never been encountered before the cuprates were discovered. A variety of models treating the relaxation processes have been put forward in the literature. Here, we will review the results of several of these models in an eﬀort to gauge the present status of our understanding of these matters. There have been phenomenological models put forward by Monien and Pines [3] and Millis, Monien, and Pines [4, 5], where the AFM ﬂuctuations are taken into account by means of an RPA treatment of the AFM exchange interactions. Moreover, it is assumed and is consistent with experiment that the Cu2+ spin variables are itinerant and undergo pairing in the superconducting state. Similar modeling along these lines has also been put forward by Horvati´c et al. [6]. These models were presented early on and gave a reasonable account of the data which were available at the time. In particular, they met the challenge of explaining the behavior of all measured relaxation processes with a single dynamical variable per Cu site, and did so using only HF couplings generated by the Cu2+ spin moments, in a picture consistent with the Mila-Rice model [1] of on-site spin–Hamiltonian and transferred HF couplings of the general

R.E. Walstedt: Relaxation Models for Cuprate NMR, STMP 228, 159–211 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 5

160

5 Relaxation Models for Cuprate NMR

form α Aα Sα Iα . A possible deviation from this form may occur in the case of 89 Y in YBCO compounds, where the transferred coupling is very weak and the dipolar interactions, which do not have the latter form, come into play. A slightly diﬀerent approach to modeling the dynamical susceptibility has been pursued by Auler et al., [7], where the basic form of the dynamic susceptibility was taken directly from INS data. This scenario had the unusual feature that the range of spin-spin correlations was ﬁxed, although their strength certainly increased as temperature was lowered. These authors also made the unusual step of using spin-echo decay time (T2g ) measurements to determine the strength of the AFM susceptibility peak. In reviewing the results of their an analysis, we shall ﬁnd that a satisfactory account of the data can be achieved in this fashion. Beyond phenomenology, there have also been ﬁrst-principles model calculations by Bulut and Scalapino [8] and by Si, Levin, and co-workers [9]. The latter are, of course, more diﬃcult to formulate and execute, but these have yielded impressive insights. Finally, there has been a proposal by Varma which departs from the usual spin HF-only picture wherein an intersite orbital matrix element is suggested to make an important contribution to the Cu(2)-site relaxation process [10]. The essence of these various results will be summarized below. This chapter will begin, however, with a discussion of the characterization of the cuprate relaxation properties developed quite recently by Uldry and Meier [11] (UM). This is a scheme of a fairly general nature for characterizing the spin dynamics and spin-spin correlations which determine the relaxation behavior in the CuO2 planes. It serves as a useful framework for evaluating almost any experimental data or theoretical model.

5.1 The Uldry-Meier Parameterization Model The Uldry-Meier (UM) approach to the analysis of cuprate relaxation data relies only on a general formulation of spin-ﬂuctuation T1 processes, which is characterized by just three elements, (i) the HF constants, (ii) real-space, dynamical spin-spin correlation coeﬃcients, and (iii) an eﬀective correlation time parameter in which the temperature variation of the spin dynamics is also implicit in a very general way. The HF parameters used are those derived from the Mila-Rice-Shastry model (3.3.2) for each site in and near the CuO2 planes.1 The spin-spin correlations and correlation time which characterize the relaxation processes are assumed to apply to all nuclear species considered, e.g. the 63 Cu(2), 17 O(2,3), and the 89 Y in YBCO7 and YBCO6.63, etc. The spin-spin correlations are allowed to be anisotropic, but the correlation time variable is assumed to be isotropic and common to all spin ﬂuctuation processes. After describing the UM analysis, the broader signiﬁcance of this methodology will be discussed at the end of this section. 1

The Cu(1) sites and environs in YBCO are set aside as a separate problem.

5.1 The Uldry-Meier Parameterization Model

161

5.1.1 Basic Formulation of the UM Analysis In the ﬁrst step, UM deﬁne single-axis T1 components 1 = Uβ + Uγ , T1α

(5.1.1)

where the subscripts are a permutation of the axes (a,b,c). Thus, Uα is an axis-speciﬁc ﬂuctuation term given by Uα =

1 α [Aiα Ajα Kij ]τeﬀ , 4 i,j

(5.1.2)

where Aiα is the HF coeﬃcient for the ith neighbor spin S iα (see (3.3.2)), and α the Kij are now deﬁned as α = 4 Siα Sjα , Kij

(5.1.3)

where the index α allows the spin-spin correlations to be anisotropic. The α α α α α ’s which will occur in the analysis are Kii = 1 and K01 , K12 , and K13 , only Kij where the subscripts refer to the sites in Fig. 3.6. These correlation factors, originally introduced by Mila and Rice [1] were deﬁned and discussed in Sect. 3.3 and 3.5. In particular, they are easily expressed in terms of χ (q, ω) (see (3.5.17) and (3.5.18)). The parameter τeﬀ plays the role of a correlation time in (5.1.2), but also contains the eﬀects of quasiparticle dynamics in the calculation. At low temperatures, for example, τeﬀ ∝ T . In (3.5.17) a similar quantity Xat was introduced, where we can make the identiﬁcation τeﬀ = (kB T /)Xat . In ﬁtting (5.1.2) to the experimental data, the principal assumption is the form of the HF coupling Hamiltonian (3.3.2), where it should be noted that deviations from this form (e.g. dipolar coupling) are not unusual. In Sect. 3.5 the Kij ’s were also formulated in terms of χ (q, ω), giving a ﬁrm theoretical foundation for (5.1.2) in terms of spin-ﬂuctuation relaxation processes. The determination of T1 for any nuclear spin site given χ (q, ω) and a set of HF tensors is clear enough in terms of the foregoing deﬁnitions. However, the innovative task performed by Uldry and Meier was to devise a scheme to extract the HF constants, τeﬀ , and the Kij ’s, including temperature dependences, from a comprehensive body of relaxation data for a cuprate compound. We review their method here, using the example of YBCO7. In order to fully characterize the relaxation process of a given nuclear site, it is necessary to have T1 data from all three axes, since from (5.1.1) we have Uα = 12 [1/T1β + 1/T1γ - 1/T1α ]. It simpliﬁes, of course, if there is ab plane symmetry. Thus, it is necessary to have a full data set for all nuclear sites of interest in order to apply this scheme of analysis to any given cuprate. In Fig. 5.1(a)–(c), a 100 K - 300 K data set is shown for 63 Cu(2) [12, 13], 17 O(2,3) [14], and 89 Y[15] in YBCO7, plotted as 1/T1 T vs. T . Using (5.1.1), the corresponding (interpolated) plots for 63 Uα , 17 Uα , and 89 Uα are shown

162

5 Relaxation Models for Cuprate NMR 50

4000

(a) 63Cu(2) Uα [S–1]

3000

30 20

(d) 63Cu(2) 2000

63

(63T1αT)–1[S–1K–1]

40

1000 10 0

0

200

400

0 100

600

150

250

300

250

300

Uα [S–1]

60

0.3 0.2

40

17

17 –1 –1 –1 ( T1αT) [S K ]

300

(e) 17O(2,3)

0.4

(b) 17O(2,3)

0.1

0

200

400

600

20

0 100

800

150

Temperature[K]

200 Temperature[K]

0.05

2.5

0.04 Uα [S–1]

3

2

89

(89T1αT)–1[10–4 S–1K–1]

250

80

0.5

0

200 Temperature[K]

Temperature[K]

1.5

(f) 89Y

0.03 0.02

(c) 89Y 0.01

1 0 0

200

400 Temperature[K]

600

800

0 100

150

200 Temperature[K]

Fig. 5.1. (a)–(c) Relaxation data for YBCO7 plotted as circles, upward triangles, and diamonds from [12] (63 T1c ), [13] (63 T1ab ), [14] (17 T1α ), and [15] (89 T1γ ) are plotted as 1/T1 T vs. T . Solid lines drawn are ﬁtted curves derived from the UM model calculations (see text). The downward triangles are supplemental data included to illustrate high-T behavior for the 17 O(2,3) [16] and the 89 Y [17], as discussed in the text. (d)–(f) Interpolated values of k Uα (T) derived from the data shown and described in (a)–(c), with which the actual ﬁtting process was conducted. The solid lines drawn are guides for the eye. The straight line drawn in panel (d) shows 1/63 T1 vs. T for Cu metal for comparison. Reprinted ﬁgures from A. Uldry and P. F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

5.1 The Uldry-Meier Parameterization Model

163

in Fig. 5.1(d)–(f). It is remarkable how similar the latter curves look when plotted as 1/T1 rather than as 1/T1T . The next step was to make a simplifying approximation regarding the Kij ’s. Since the three √ described above correspond to spin sites separated α by distances a/2, a/ 2, and a, respectively, UM have assumed that K12 = √ α α α 2 2 (K01 ) , and K13 = (K01 ) , which is equivalent to the assumption of the form α Kij = exp(−2rij /aλα ). At each temperature, then, the ﬁt procedure only has α to determine the two values λab,c , rather than six Kij ’s. If this approach should prove unsatisfactory it could easily be modiﬁed. It is also convenient to deﬁne, along with the k Uα ’s, a parallel set of coeﬃcients k Vα , given by k Uα = k Vα τeﬀ . Then from (3.5.20), (3.5.21), and (3.5.22) we have 1 2 α α [A + 4B 2 + 8 Aα BK01 (T ) + 8B 2 K12 (T ) 4 α α (T )] +4B 2 K13 1 17 α Vα (T ) = Cα2 [1 + K01 (T )] 2 89 2 α α Vα (T ) = 2 Dα [1 + 2 K01 (T ) + K12 (T )], 63

Vα (T ) =

(5.1.4a) (5.1.4b) (5.1.4c)

where superscripts are used to label the isotope concerned. Since the HF coeﬃcients used here relate directly to (3.3.2), their anisotropies as well as those of the λα ’s should stem directly from the data in a natural way. 5.1.2 The Uldry-Meier Analysis of YBCO7 The following procedure was used to apply the foregoing analytical scheme to the data in Fig. 5.1(d)–(f). Deﬁning the six ratios, 63

r1 =

Uc

17 U

c

63

; r2 =

Uab ; 17 U a

63

r3 =

Uab ; 17 U b

17

r4 =

Ub

17 U

c

89

; r5 =

Uc

89 U

ab

17

; r6 =

Ua , 89 U c

(5.1.5) the HF constants in (5.1.4) and the λα ’s are then determined by minimizing the quantity np nr 1 [riexp (Tj ) − rimod (Tj )]2 χ2 = , (5.1.6) nr i j riexp (Tj )2 where nr and np are the numbers of ratios (= 6) and the numbers of points (= 10), respectively, and where the rimod for the “model” are actually calculated from (5.1.4) in terms of the HF constants and the λα ’s. Note that the ri ’s do not involve the quantity τeﬀ . The HF parameters so obtained are listed in Table 5.1, where for comparison a “standard” set of parameter values from UM are given, as well as the YBCO parameters derived from NMR shift data in Chaps. 3 and 4. We consider these comparisons in detail below. A plot of τeﬀ vs. T is then determined for each parameter Uα via (5.1.2). The λα ’s and the results for τeﬀ so determined are displayed in Fig. 5.2(a) and

164

5 Relaxation Models for Cuprate NMR

Table 5.1. HF coeﬃcients deﬁned in (3.3.4) and derived from the UM ﬁt procedure with the T = 100 K relaxation data shown in Fig. 5.1, as described in the text, are listed and compared with data presented by Nandor et al., [17] as well as with data derived from NMR shift measurements as described and presented in Tables 3.4 and 3.6. HF coeﬃcient values are given in units of 10−6 eV . See text for discussion of these results HF Constant UM Fit Nandor Shift Coef.

63

Ac

−1.68 −1.6 −1.67

63

Aab

0.168 0.29 0.05

B 0.438 0.4 0.409

17

Ca

0.259 0.25 0.355

17

Cb

0.173 0.13 0.217

17

Cc

−89 Dab

−89 Dc

0.196 0.156 0.209

0.00280 0.0048 0.00286

0.00349 0.0048 0.00369

(b), respectively. The correlation lengths, which are of the order of the lattice constant, are seen to execute a smooth progression toward longer values as T decreases, a process which accelerates below 150 K. They also ﬁnd consistent anisotropy of ∼ 20%, the stronger c-axis correlations suggesting the possibility of a corresponding exchange anisotropy between neighboring Cu2+ spins. Although the ﬁtting scheme with the ratios ri promotes consistency among τeﬀ values it is nonetheless remarkable how nicely they each describe a very similar arc with temperature. As we shall see below, some of the most subtle physics of the cuprate spin ﬂuctuations is embodied in the behavior of τeﬀ , where even at this point a great deal remains to be understood. The HF coeﬃcients from the ﬁt are compared with values from other sources in Table 5.1. The HF constants labelled “Nandor” [17] are actually mostly derived from Barzykin and Pines [18], and are seen to be in rough accord with the ﬁt. The “Shift Coef.” values shown have been converted from the primed coeﬃcients in Tables 3.4 and 3.6 using (3.3.4) so that g-factor anisotropy (3.3.7) comes into play. The value of B given, for example, comes from c-axis shift measurements. The value of 63 Aab = 0.05×10−6eV is obtained by subtraction of large values and is correspondingly unreliable. The agreement of the 63 Ac and of the 89 Dα tensors is very good, indeed. The ﬁtted values of the 17 Cα are 10–20% below those derived from the NMR shifts. This is an interesting point, because the “T1 problem” for the 89 Y discussed in Sect. 4.1.2 has been managed in the UM ﬁt process not by enhancing the 89 Dα tensor coeﬃcients, but by reducing the 17 Cα ones. Either way, there will be a discrepancy between shift coeﬃcients and those derived from relaxation. We continue to believe that there is an additional 89 Y relaxation process (orbital or dipolar), which is beyond the eﬀects of the MR Hamiltonian (2.3.2). In spite of this eﬀect, there is quite a good correspondence between HF constants derived from the UM ﬁt and those from NMR shifts. It is also noteworthy that the ﬁtting procedure based on 5.1.5 is independent of scale. That is, all HF constants (e.g. the k Vα ’s in (5.1.4)) can be multiplied by a uniform scale factor and the results will not be aﬀected. Thus,

5.1 The Uldry-Meier Parameterization Model

165

any set of results for the HF constants needs to be keyed to some particularly reliable value. In Table 5.1 the results are, in eﬀect, keyed to 63 Vc . The UM ﬁtting procedure leads to temperature dependences for the correlation lengths λα shown in Fig. 5.2(a) and to seven estimates (from the k Vα ’s in (5.1.4)) for the correlation time curve τeﬀ (T ), which are summarized in a plot in Fig. 5.2(b). In the latter case the extrema of the bundle of seven curves are shown as dashed lines, where the circles are the average values. The dotted line is a functional ﬁt described below. Considering the 89 Y relaxation rate

λ[a]

(a)

λ[a]

1.2

1

100

1

300 T[K]

0.8

0.6 100

150

200

250

300

Temperature[K]

(b)

τeff[10–15 s]

1.5

1

0.5

0

0

100

200

300

400

500

600

Temperature[K]

Fig. 5.2. (a) Correlation lengths λab (circles) and λc (triangles) derived from the UM ﬁt to YBCO7 are plotted vs. T over the range of the ﬁt. Inset: Low and high-T asymptotic behavior used to extrapolate the λα ’s is shown with dotted lines. (b) The average (circles) and extremal (dashed lines) values for the seven sets of τeﬀ parameters obtained from the T1 data ﬁt for YBCO7 are plotted vs. T . The dotted line is a ﬁt to these data which is extrapolated down to T = 0 and upward to T = 600 K. This ﬁt and its interpretation are described in the text. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

166

5 Relaxation Models for Cuprate NMR

anomaly noted above and in Sect. 4.1.2, the degree of consistency among τeﬀ values is surprisingly good. Extrapolation of the Fits to Higher Temperatures In Fig. 5.1(a)–(c) we see that the ﬁts are generally very good over the ﬁtting temperature range. However, UM went on to extrapolate their ﬁts to higher temperatures with a ﬁtting function ansatz as follows. The general behavior of τeﬀ (T ) in Fig. 5.2(b) is one of downward curvature, but linear in T at the lowT end. The latter feature is expected in metallic hosts, but the curving over is much greater than could be attributed to loss of Fermi-statistical degeneracy. They propose a ﬁtting function wherein a Fermi-statistical term τ1 = aT is combined in an inverse fashion with a constant term τ2 which dominates at high temperatures. Thus [11], 1 1 1 1 1 + , = + = τeﬀ τ1 τ2 aT τ2

(5.1.7)

where a = 7 × 10−18 s/K and τ2 = 3 × 10−15 s. The line representing this function is plotted in Fig. 5.2(b) as a dotted line up to 600 K. In Sect. 5.4 and 5.5 we shall look for the possible origin of this ﬂattening eﬀect in the Hubbard models. However, it does not appear to have been successfully identiﬁed yet. The physics of the ansatz (5.1.7) is a bit unfamiliar, because normally when two rates combine inversely, it is the “faster” of the two which dominates. Here, however, at high temperatures when the Korringa T1 is very short, it is undercut by a weaker relaxation process. As for the form of τ1 , Pines and Slichter [19] suggest a picture where τ1 = τc T /TF is made up of a correlation time factor τc ∼ /EF representing the dwell time of a carrier in the unit cell, and T /TF represents a Fermi-statistical scattering probability factor. Thus, a = /kB TF2 , from which UM estimated TF ∼ 1000 K. Meanwhile, τ2 appears to represent the behavior of the gas of quasiparticles when the degeneracy is completely lifted. This extrapolation of the curve for τeﬀ (T) is also used to extrapolate the ﬁt curves in Fig. 5.1(a)–(c). It is interesting to compare these extrapolations with high-temperature data by Nandor et al., [17] for 17 O(2,3) and for 89 Y, shown in panels (b) and (c) as downward triangles. The data for 17 O(2,3) fall somewhat below the ﬁtted data, but show a temperature dependence which is in general accord with the extrapolated model prediction. For the 89 Y, however, contrary to the model the data are ﬂat if not slightly rising with temperature. This behavior is consistent with the ﬁnding in Sect. 4.1.2 that there is an additional relaxation term for the 89 Y beyond what is derived from (2.3.2). A possible orbital term was mentioned in Sect. 4.1.2. There are also dipolar terms which do not follow the spin-spin correlations [15]. The dipolar terms have also been calculated by Auler et al., [7] and are discussed further in Sect. 5.3.

5.1 The Uldry-Meier Parameterization Model

167

The Spin Correlations and the “Basic” Relaxation Mechanism The ﬁt to YBCO7 data illustrates rather dramatically the role played by antiferromagnetic (AFM) spin-spin correlations in the relaxation processes of all nuclei. It is interesting in this connection to examine the behavior of the k Vα (T ). According to the deﬁnitions (5.1.4), the k Vα (T ) can vary from a hightemperature limit where Kij → 0, to a fully correlated limit at low T where (in principle) K01 → −1 and K12 , K13 → 1. The T → ∞ limits for the k Vα (T ) are deﬁned to be k Vα0 , and are given by 63

Vα0 =

1 2 (A + 4B 2 ) 4 α 1 17 0 Vα = Cα2 2 89 0 Vα = 2 Dα2 .

(5.1.8a) (5.1.8b) (5.1.8c)

The “basic” relaxation mechanism is what it would be in the absence of AFM correlations and is given by 1/k T1α = k Vα0 τeﬀ . Thus, apart from a scale factor, it is the same for all nuclei in the system. The AFM correlation factors are the only thing which distinguishes the behavior of diﬀerent nuclei. Fig. 5.3(a)–(c) illustrate this point by plotting the k Vα (T ) vs. T for the YBCO7 ﬁt. (Fig. 5.3(d)–(f) plot the same quantities for YBCO6.63 - see discussion below.) The high-temperature (Kij = 0) limits are shown as solid bars on the right, and the low-temperature limits by solid bars on the left side of the ﬁgures. The T → 0 behaviors are estimated by extrapolating the correlation lengths in Fig. 5.2(a) by means of the dotted lines shown in the inset. The behavior seen in these plots shows (i) that the correlation causes the relaxation rates of the 63 Cu(2) to increase and those of the 17 O(2,3) and the 89 Y to decrease, and (ii) that the behavior of all three nuclear species is changed by similar amounts as a result of the correlations. In this picture it is something of an accident that the 17 O(2,3) and the 89 Y relaxation processes appear to be Korringa-like in the normal state. According to Fig. 5.3(a)-(c) the AFM correlations make sharp increases in the superconducting state. It must be emphasized that this is an extrapolation of normal-state behavior and is entirely hypothetical. As we shall see in Sect. 5.7, the actual behavior below Tc is quite diﬀerent from what is shown here. 5.1.3 The Uldry-Meier Analysis of YBCO6.63 A very similar analysis to that described above was carried out by UM for YBCO6.63. The quality of the input data was perhaps not quite as good, and there were no data at all for 63 T1ab . The analysis was simpliﬁed a bit by adopting the HF tensor values shown in Table 5.1 for the YBCO6.63 analysis (recall that the values derived from NMR shifts in Chap. 4 were found to be nearly the same). The ﬁtted curves (not shown) were only slightly less good, where, not surprisingly, the 89 Y ﬁts were noticeably worse than the others.

168

5 Relaxation Models for Cuprate NMR 5000

7000

Cu(2)

4000

YBCO7

4000 3000

(d) 63Cu(2) 3000

YBCO6.63 2000

63

Vα [1015s–2] 63

5000

Vα [1015s–2]

(a)

6000

63

2000

1000 1000 0 0

100

200

300

400

500

0

600

100

Temperature [K]

200

300

Temperature [K] 60

80

(e) 17O(2,3) Vα [1015s–2]

(b) 17O(2,3)

17

40

17

Vα [1015s–2]

60

20

YBCO6.63

40

20

YBCO7 0 0

100

200

300

400

500

100

600

Temperature [K]

(f) 89Y

(c) 89Y Vα [1015s–2]

0.05 0.04 0.03

89

Vα [1015s–2]

300

0.03

0.06

89

200 Temperature [K]

0.02

0.02

0.01

YBCO7

YBCO6.63

0.01 0

0 0

100

200

300

400

Temperature [K]

500

600

100

200

300

Temperature [K]

Fig. 5.3. (a)–(c) Curves are plotted representing 63 Vα (T ), 17 Vα (T ), and 89 Vα (T ) for the ﬁt to YBCO7 in (a), (b), and (c), respectively. The solid bars on the right represent the values of k Vα0 corresponding to zero spin correlations, and the bars on the left represent maximum correlations as explained in the text. The data plotted are seen to run between these two limits. The zero-temperature points for these curves were obtained by extrapolating the variation of the λα ’s near 100 K to zero temperature. Such an extrapolation is entirely hypothetical. (d)–(f) Curves are plotted representing 63 Vα (T ), 17 Vα (T ), and 89 Vα (T ) for the ﬁt to YBCO6.63 in (d), (e), and (f), respectively. These results are similar to those on the left, but AFM correlations show a wider range and reversed curvature as compared with YBCO7. Reprinted ﬁgures from A. Uldry and P. F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

5.1 The Uldry-Meier Parameterization Model

169

The results for k Vα (T ) curves are shown in Fig. 5.3(d)–(f), where they are seen to be quite diﬀerent from those for YBCO7. The correlation lengths for YBCO6.63 were longer than for YBCO7, reaching ∼ 2.5 a or so. As a result the range and magnitude of the correlation factors driving the k Vα (T ) curves are considerably greater than for YBCO7. Another interesting feature is that the curvature of the k Vα (T ) curves is in all cases the opposite in these two systems. There was also slightly more scatter in the τeﬀ (T ) curves for YBCO6.63, shown in Fig. 5.4(a), where they execute a considerably greater range than for YBCO7 (Fig. 5.2(b)). This, of course, results from the gapped nature of the static and dynamical properties of YBCO6.63. The average curve for τeﬀ (circles) was again ﬁtted with the ansatz (5.1.7), except that a gap feature is introduced into the density of states with τ1 (T ) = a T exp(−Tg /T ).

(5.1.9)

With that modiﬁcation, (5.1.7) was ﬁtted to the data in Fig. 5.4(a) and is shown as a dotted line extending from 0 K to 600 K. The ﬁtting parameters are listed below in Table 5.2, where a and τ2 are seen to be quite similar to those for YBCO7. The gap energy Tg = 94 K is very close to that (104 K) derived from the susceptibility in Fig. 4.4, rather than being twice that value as we found for Y248 in Sect. 4.3. The slightly lower value for a suggests a somewhat lower degeneracy temperature for YBCO6.63 as shown in the table. 5.1.4 The Uldry-Meier Analysis of YBa2 Cu4 O8 (Y248) The foregoing analytical scheme was also applied, in a somewhat restricted fashion, to the case of Y248, analyzing the same body of NQR data for 63 Cu(2) as were discussed in Sect. 4.3. The method was restricted owing to a total lack of T1 data for other sites and orientations. As a consequence, the 63 Vab (T ) curve for YBCO7 (see Fig. 5.3(a)) was adopted for the Y248 calculation, where 1 = 2 63 Vab τeﬀ . (5.1.10) 63 T 1c This is a fairly “neutral” assumption, since the temperature proﬁle of 63 Vab (T ) is seen to be very ﬂat for both YBCO7 and YBCO6.63 in Fig. 5.3, but particularly in the former case. In any case, the ﬁt to the data for 1/63 T1c T , shown in Fig. 5.5(a) and (b), is seen to be excellent, and furthermore, extends up beyond 700 K. Note that the 100 K – 350 K data set from Raﬀa et al., [20] (crosses) has been augmented with high-temperature data from Curro et al., [21] (triangles pointing right) and from Tomeno et al., [22] (triangles pointing down). Although the proﬁle of τeﬀ (T ) may be slightly diﬀerent from what one would ﬁnd with a full-blown analysis such as that for YBCO7, it behaves in a very interesting fashion as shown in Fig. 5.4(b). Here there is only one

170

5 Relaxation Models for Cuprate NMR 2

τeff[10–15 s]

1.5

1 (a) YBCO6.63 0.5

0

0

100

200

300

400

500

600

500

600

Temperature[K] 2

τeff[10–15 s]

1.5 (b) Y248 1

63Cu(2)

0.5

0

0

100

200

300

400

Temperature[K]

Fig. 5.4. (a) The data for τeﬀ (T ) derived from the ﬁt to several relaxation curves from YBCO6.63, as described in Sect. 5.1.3. The circles plot the average values of τeﬀ , and the dashed lines show the most extreme values. The dotted line is a ﬁt of (5.1.7) and (5.1.9) to the average values, extrapolated to 0 K and 600 K. (b)Values for τeﬀ (T ) derived from the ﬁt to the relaxation curve for 63 Cu(2) in Y248, shown in Fig. 5.5, as described in Sect. 5.1.4. The dotted line is a ﬁt of (5.1.7) and (5.1.9) to the data (circles), extrapolated to 0 K and 600 K. Parameters from the ﬁts shown are presented in Table 5.2 and discussed in the text. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

data set from the ﬁt (circles), which has very little scatter. The dotted line is a ﬁtting of the ansatz (5.1.7) with the gap modiﬁcation (5.1.9) used for YBCO6.63. The parameters from this ﬁt are given in Table 5.2, where they may be compared with those for YCBO7 and YBCO6.63. The parameters in Table 5.2 show an interesting progression for the three YBCO-related systems. Although the forms of τeﬀ (T ) in (5.1.7) and (5.1.9) are really just educated guesses, they match the temperature dependence from

5.1 The Uldry-Meier Parameterization Model

171

Table 5.2. Parameters from ﬁts to the ansatz (5.1.7) for YBCO7 and with the gap modiﬁcation (5.1.9) for YBCO6.63 and Y248 are listed, showing a, τ2 , and the gap, crossover, and Fermi temperatures derived from their respective (average) data curves for τeﬀ (T ). The crossover temperature is where τ1 = τ2 , and the estimated Fermi temperature is obtained from TF ∼ (/kB a)1/2 . These results are discussed in the text System

a (s/K)

YBCO7 YBCO6.63 Y248

7 × 10−18 10 × 10−18 44 × 10−18

τ2 (s) 3.0 × 10−15 2.9 × 10−15 1.9 × 10−15

Tg (K) 0 97 195

Tcr (K) 420 375 154

TF (K) 1,050 880 420

the ﬁts better than one might have expected, giving very convincing extrapolations to higher and lower temperatures. After modest changes between YBCO7 and YBCO6.63, with the appearance of a ∼ 100 K gap in the √ latter case, the jump to Y248 shows a doubling of the density of states (∝ a) and a corresponding reduction by half of the estimated degeneracy temperature, as well as a doubling of the gap energy, which now exceeds the cross-over temperature. A somewhat diﬀerent view of the dynamic magnetism of Y248 via dynamical scaling theory is presented in Sect. 6.4. The Wider Role of the Uldry-Meier Model Analysis The UM analysis has oﬀered a highly revealing and greatly unifying look into the microscopic phenomena associated with the cuprate T1 processes. From this perspective, the diﬀerence between diﬀerent sites and nuclear species essentially ceases to be an issue. This analysis is in no sense a theory, though it incorporates a widely accepted and time-tested formulation of the T1 process, and it puts the Mila-Rice HF Hamiltonian to a severe test, which it mostly passes in good order. Note that this Hamiltonian is essentially unique to cuprates among metallic environments. It is worth emphasizing that the UM picture is also implicit in the general χ (q, ω) formulation of the T1 process, as demonstrated in Sect. 3.5. Perhaps the most signiﬁcant advantage of the UM analysis is that it partitions the T1 problem into three independent phenomenological pieces. These are (i) HF constants, which are essentially inert, (ii) AFM correlation factors, which are much larger and universally more important than hitherto realized, and (iii) a comprehensive ﬂuctuation rate, which embodies all of the lowfrequency spin ﬂuctuation physics of the cuprates, including, but not limited to, Fermi liquid, spin pseudogap, and exchange-coupled local moments. The ability to separate elements (ii) and (iii) in either an experimental or theoretical evaluation is a considerable simpliﬁcation and an enormous advantage over previous practice. We emphasize that this analysis oﬀers a useful way to evaluate model theories of χ (q, ω). One can simply evaluate (ii) and (iii)

172

5 Relaxation Models for Cuprate NMR

7

(63T1cT)–1

(a) 6

5

4 50

100

150

200

250

300

350

400

Temperature[K] 7 6 (b)

(63T1cT)–1

5 4 3 2 1 0 200

400

600

800

Temperature[K]

Fig. 5.5. (a) 63 Cu(2) NQR data from [20] for Y248 (crosses) are plotted as 1/T1 T vs. T . The solid line shows the Uldry-Meier ﬁt to these data described in Sect. 5.1.4. (b) The ﬁt curve shown in part (a) is extended to above 700 K. Also shown there are high-temperature data by Curro et al., [21] (triangles pointing right) and by Tomeno et al., [22] (triangles pointing down). The data and the ﬁt are seen to be extremely precise. Reprinted ﬁgures from A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005). Copyright 2005 American Physical Society

as deﬁned above and judge these components separately on their own merits. This procedure oﬀers a new perspective on theory building for the cuprates and quite possibly for other materials as well.

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates This straightforward phenomenological model [4, 5] served the important role of discussing and testing certain key ideas in the early days when both NMR

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates

173

shift and relaxation data were still unfolding. This model emerged at a time when there was still a great deal of uncertainty about what the ultimate theoretical basis for cuprate T1 processes was going to be. Of the several lines of theoretical approach to cuprate spin dynamics which we discuss in this chapter, the conceptually simple MMP model is a good place to begin. One of the main objectives of MMP was to show that the relaxation of 63 Cu(2), 17 O(2,3), and 89 Y can all be accounted for with a single dynamical variable associated with each Cu2+ site. In ths matter they largely succeeded, although as noted in Sects. 4.3 and 5.1 there are other apparent contributions to the 89 Y relaxation process. However, there is no evidence for another set of dynamical variables besides the Cu2+ spin moments. In addition to the foregoing, these two papers [4, 5] give an in-depth discussion of the physics issues surrounding the NMR T1 problem in cuprates. Although the actual model they expound is a phenomenological treatment of the Mila-Rice Hamiltonian [1], they present a derivation [5] showing that such treatment is equivalent to a tight-binding, band-theory model of an interacting Fermi liquid. The MMP model is based on a mean-ﬁeld treatment of AFM exchange interaction eﬀects in a system of itinerant quasiparticles, i.e. a metal, which would be a simple Fermi liquid without the exchange interactions. We begin by reviewing their derivation of the mean-ﬁeld dynamic susceptibility, in the course of which the relevant parameters are introduced and discussed. The following is just a brief summary. We refer the interested reader to the original papers for greater detail [4, 5] dynamical susceptibility, RPA model. The mean-ﬁeld complex susceptibility χ(q, ω) = χ (q, ω) + i χ (q, ω) of an interaction spin system is given by χ(q, ω) =

χ(q, ω) , 1 − Jq χ(q, ω)

(5.2.1)

where χ(q) is the noninteracting susceptibility, and Jq is the interaction potential. Since NMR frequencies are generally much smaller than the electronic frequencies in such a system, we are concerned here with the region near ω → 0. In this limit it is assumed that ω ω χ (q, ω)|ω→0 → π χ (q, ω = 0) ≡ π χq , (5.2.2) Γq Γq where Γq is a characteristic energy for spin ﬂuctuations at wave vector q. Correspondingly, in the same limit (5.2.1) gives χ (q, ω) −→ π

ω 1 χ , Γq (1 − Gq )2 + (πω/Γq )2 G2q

(5.2.3)

where Jq χq ≡ Gq . As we are treating AFM ﬂuctuations which appear to be diverging as the system is approaching a Ne´el point, Gq is assumed to be peaked at the AFM point Q = (π/a, π/a), at which point it has a value of

174

5 Relaxation Models for Cuprate NMR

slightly less than 1. For (5.2.3) we expand Gq about the AFM point: Gq ≈ GQ - q 2 β02 , where q is measured from Q. The correlation length is deﬁned by GQ = 1 - ξ02 /ξ 2 . Setting Gq = 1 in the second term of the denominator of (5.2.3), we obtain πχ0 πχ (ξ/ξ0 )4 (ξ/ξ0 )4 χ (q, ω) = . 2 2 2 2 4 ω Γ (1 + q ξ ) + (πω/Γ ) (ξ/ξ0 ) Γ (1 + q 2 ξ 2 )2

(5.2.4)

Because of the peaked nature of this function, the q-dependence of the parameters χq and Γ q has been dropped. They argue further that when q is far away from Q, χ (q, ω) should be comparable with the uncorrelated value, so a q-independent term of that magnitude is added in, giving χ (q, ω) πχ (ξ/a)4 = , (5.2.5) 1 + β ω (1 + q 2 ξ 2 )2 Γ ω→0 where β = (a/ξ0 )4 (χ/χ0 )(Γ/Γ ), χ0 is the uniform susceptibility, and Γ is the spin ﬂuctuation frequency of the noninteracting system. Equation (5.2.5) may then be used to model quasiparticle dynamics for cuprate systems not too far from an AFM instability, i.e. when ξ/a 1. From (5.2.4) we also see that the eﬀective spin ﬂuctuation frequency is ωSF ∼

Γ ξ02 , ξ2

(5.2.6)

which can be greatly diminished if ξ ξ0 . The q-dependent HF coupling Hamiltonian terms are denoted k Fα (q) here (3.5.6) for nuclear spin species k and axis α. Thus, the relaxation rate k Wα ≡ 1/k T1α is given by [5] kB T k k 2 k 2 χ (q, ω) Wα = Fβ (q) + Fγ (q) , (5.2.7) 4μ2B q ω ω→0 where (α, β, γ) is any permutation of the (a,b,c) axes. In (5.2.7) the k Fα (q) have the dimension of s (cf. (3.5.10)), where g-factor anisotropy is not included. For YBCO the k Fα (q) are Fα (q) =63 Aα − 2B(cos qx a + cos qy a), 17 Fα (q) = 2 Cα cos2 ( qx,y a/2) ,

(5.2.8a) (5.2.8b)

Fα (q) = 8Dα cos(qx a/2) cos(qy a/2) cos(qz a/2)

(5.2.8c)

63

89

(see (3.5.10) - (3.5.14)). The ﬁtting procedure, which is described brieﬂy below, thus consists of estimating the HF constants (A, B, C, D’s) from NMR shift and susceptibility data, and then adjusting the parameters Γ , β0 , and ξ from (5.2.5) to match the calculated rates k Wα (T ) as well as possible with experimental data.

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates

175

The MMP Fitting Process for YBCO7 Here we summarize the issues regarding this ﬁtting procedure as well as a brief description of the procedure itself. We ﬁrst note that the squared Lorentzian form for χ (q, ω) in (5.2.5) is valid when ξ/a 1, whereas the deduced YBCO7 values of ξ/a are of order unity. For this reason, MM also discussed the case of a Gaussian form for the peak at Q [5]. The latter is more nearly consistent with peaks in χ (q, ω) which have been reported from neutron scattering studies [23]. The latter results also showed some sign of incommensurability, which is also a major eﬀect in LSCO. The question is whether the incommensurability observed by neutron scattering at energies of more than 1 meV is still present at NMR frequencies, which are roughly four orders of magnitude smaller. In Chap. 6 it will be shown that incommensurability in χ (q, ω) is incompatible with NMR data on LSCO. We assume this is also true here and adopt with MM [5] a picture with commensurate AFM ﬂuctuations. The HF parameters used by MM are compared with those from the UM ﬁt as well as those from NMR shift values in Chap. 3 (see Table 5.1) in Table 5.3. In MM the HF values are given in units of μ2B /χ0 . Here we convert them to units of 10−6 eV . Since the susceptibility is assumed to be isotropic, we have used the powder average susceptibility per Cu(2) ion from Table 3.4 for this purpose. It was also assumed that Ac + 4B = 0, essentially consistent with earlier practice. The other MM values show some small diﬀerences with the other values listed. The ratio Ca to Cc is ∼ 1.5, in rough agreement with the others. However, the ratio Ca /D 69 is rather smaller than the “Shift Coef.” value 113, so that the “problem” with the T1 of 89 Y (see Sect. 4.1.2) will not arise here. We ﬁrmly believe this problem to exist. In the MM ﬁt there was no value available for Aab , so this was left as a parameter to be “ﬁtted”. From the Cu(2) T1 anisotropy 63 Wab /63 Wc it was decided that 0.1 ≤ Aab /4B ≤ 0.2, which is not unreasonable. This estimation is compared with other values in Table 5.3. The susceptibility parameters β and ξ from (5.2.5) – and their temperature dependences – were to be extracted Table 5.3. The HF parameters for YBCO7 and YBCO6.63 used by MM [5] are compared with values from the UM ﬁt and those derived from NMR shift coeﬃcients in Chap. 3 (both given in Table 5.1). The coeﬃcients in MM were given in units of μ2B /χ0 , which have been converted to eV using the powder average susceptibility based on values given in Table 2.4, where χ0 is interpreted to be the value for a single Cu(2) site. The values for Ca and Cc have been reversed, since the larger value corresponds to the Cu-O-Cu (a) axis and the smaller one to the c axis. Parameters are given in units of 10−6 eV Source

Aab + 4B

Aab /4B

Ca

Cc

D

MM [5] UM Fit Shift Coef.

1.45 1.92 1.69

0.1-0.2 0.096 0.03

0.33 0.259 0.355

0.22 0.196 0.209

0.0048 0.00303 0.00314

176

5 Relaxation Models for Cuprate NMR

from the data ﬁts. This was not a simple matter, since these parameters have qualitatively similar eﬀects on the results. There were two main questions to be decided: (i) Can the relaxation of all three nuclei be quantitatively accounted for with (5.2.5) and (5.2.8); and (ii) does a picture of AFM correlations emerge here, where ξ(T ) increases when T descends toward Tc ? The ﬁrst answer is deﬁnitely “yes”, but the second one is a bit more murky. It depended on the relative behavior of 17 Wα (T ) and 89 Wα (T ), for which the available data for the input parameters were not particularly accurate. Calculated ratios of these relaxation rates from MM are shown in Fig. 5.6 for the cases of Gaussian and Lorentzian models for χ (q, ω) and several sets of parameters. The calculations are based on the assumption that 63 Wc /17 Wc = 19 at 100 K and 63 Wc /17 Wc = 10 at 300 K, these values being taken from experiment. Shown is the variation of 17 Wc (T )/89 Wc (T ) between 100 K and 300 K for several sets of parameters, which are shown in Table 5.4. There are two assumed cases here: (i) β is constant and ξ varies with temperature, and (ii) ξ is constant and β varies with temperature. The experimental ratio is around 1,300 and is very nearly ﬂat. These circumstances favor the Gaussian form for χ and the assumption of a constant β with temperature-varying ξ, and thus the solid line in Fig. 5.6(b), case (B). Thus, it was concluded that the constant β picture was more the satisfactory, because if β varies, while ξ is constant, then Γ must have a compensating temperature dependence to keep the pre-factor in (5.2.5) approximately constant. This may be diﬃcult to account for. MM also concluded that ξ/a 1.0–1.5 for the Gaussian case and 1.5–2.0 for the Lorentzian case, while β ∼ 15 or greater. It is interesting to view the results of the MMP analysis in the context of the results of the UM analysis of Sect. 5.1. The parameter values obtained in these cases are similar with some important diﬀerences. The MMP scheme assumed HF parameters derived from NMR shift measurements which are at Table 5.4. Parameter values for the calculated curves in Fig. 5.6 are listed for the three cases plotted for a Lorentzian susceptibility peak (a) and for a Gaussian peak (b). Two curves are plotted for each case, both with the same parameters at T = 100 K and at 300 K with a constant value of β with ξ varied (ﬁrst values listed) and with both ξ and β varied (values in parentheses). The constant β curves are solid lines and those for varying β are dashed lines Case

T(K)

ξ (Lor.)

β (Lor.)

ξ (Gauss.)

β (Gauss.)

A A B B C C

100 300 100 300 100 300

1.9 1.3(1.9) 2.4 1.7(2.4) 3.7 2.5(3.7)

30 30(16) 10 10(3.4) 3.0 3.0(1.1)

1.4 1.1(1.4) 2.0 1.4(2.0) 3.3 2.2(3.3)

30 30(11) 10 10(4) 3.0 3.0(1.2)

5.2 The Millis, Monien, and Pines Model for T1 in Cuprates (a) YBa2Cu3O7 α = 0.2 Lorentzian χ”

(A) 1500

c/

89W c

177

17W

(B) (C)

1000

100

200

300

T(K)

17W / 89W c c

(b) YBa2Cu3O7 α = 0.2 Gaussian χ” 1500

(A)

(B) (C) 1000

100

200 T(K)

300

Fig. 5.6. Plots of the ratio 17 Wc (T )/89 Wc (T ) vs. T for 100 K ≤ T ≤ 300 K calculated with the model susceptibility shown in (5.2.5) (Lorentzian case) in panel (a) and a Gaussian version in panel (b). The Gaussian is written as β exp(−q 2 ξ 2 ) and is centered at Q. The calculations are based on the ratios 63 Wc /17 Wc = 19 at 100 K and 10 at 300 K. Since the variation of 17 Wc (T )/89 Wc (T ) is roughly linear, straight lines are drawn between values calculated for the two extremal temperatures. Calculations are carried out for constant β and T-varying ξ (solid lines) and for constant ξ with β varying (dashed lines). The parameter sets used are listed in Table 5.4. The same parameters are used at 100 K, but then diﬀerent ones for 300 K. These calculated results are simply connected with a straight line. Reprinted ﬁgures from A. J. Millis and H. Monien, Phys. Rev. B45, 3059 (2005). Copyright 1992 American Physical Society

least a rough facsimile of those obtained in Chap. 3 and of those obtained from the UM ﬁt (Table 5.3). The coherence lengths appear to be similar, though it is not clear whether ξ from MMP can be directly compared with the λα ’s in Fig. 5.2(a). The trend with temperature is, of course, the same. trouble spot in this comparison is the variation of the integrated area One q χ (q, ω)/ω with temperature. For the UM picture, this simply goes as τeﬀ /T , while in the MMP case (i.e. from (5.2.5)) this area is very nearly equal to

178

5 Relaxation Models for Cuprate NMR

q

χ (q, ω)/ω

πχ [1 + βξ 2 ]. Γ

(5.2.9)

If the prefactor is independent of T as one might suppose for YBCO7, then the known behavior of τeﬀ (T ) from the UM ﬁts tells us that βξ 2 from the MMP model should be roughly constant. Thus, if ξ varies appreciably with T , β should vary inversely and twice as fast. This does not square well with the MM result. On the positive side of things, one could say that the results of the UM analysis would be an excellent starting point for someone setting out to model the mean-ﬁeld dynamic susceptibility as MMP did. As regards the possibility of accounting for cuprate T1 behavior with an RPA type of model where the q-dependence of χ (q, ω) (and thus ξ) has no temperature dependence, the UM analysis also gives a deﬁnite negation of any such possibility. Millis and Monien: Discussion of YBCO6.63 and of Neutron Scattering Characterization of χ (q, ω) MM analyze YBCO6.63 in a fashion similar to YBCO7. They note that rather larger values of 63 Wc /17 Wc indicate stronger AFM correlations in YBCO6.63, in accord with the UM result. As a result, they note that the constant-ξ option implies a somewhat larger increase in the ratio 17 Wc /89 Wc at lower temperatures, inconsistent with preliminary data available at the time. However, the subsequent T1 results of Takigawa et al., [15] showed an increase in the latter ratio of ∼ 20% below 300 K, which therefore cannot quite rule out the constant-ξ hypothesis. Again, the UM analysis of YBCO6.63, showing longer and more temperature-dependent correlation lengths in YBCO6.63, would preclude a ﬁxed-ξ scenario. One slightly troubling point about the MM discussion of YBCO6.63 is the assumption without justiﬁcation that χ0 in (5.2.5) be simply replaced by the gapped χ(T ) shown in Fig. 4.4 (or its equivalent). Some kind of assumption along these lines is evidently necessary for this model, but then leads to diﬃculties in accounting for 89 Wα (T ) and 17 Wα (T ), as was noted in Sect. 4.1.2. This played, unfortunately, into the weakness of employing the MMP model to deduce the temperature dependences of both ξ and β from NMR data alone. MM oﬀer a deep and useful discussion [5] of the behavior of χ (q, ω) at higher frequencies, with an eye to gleaning further insight about its characteristics from inelastic neutron scattering (INS) data. Again, speciﬁcally, would it be possible to determine the behavior of ξ(T ) from the width of the peak at Q? They note, with a detailed model example, that there is a tendency at typical INS frequencies for the measured peak width to appear independent of temperature while ξ is undergoing a signiﬁcant variation with T1 and that measurements must be conducted at very low energies to avoid this. There appears to be relatively little useful data from INS on the T-dependence of AFM peak widths in cuprates or on pseudogap eﬀects on χ (q, ω), the main exception to this being LSCO. If we take the INS results

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

179

of Tranquada et al. [23] as an example, the desired eﬀects are often masked by incommensurability. However, unknown at the time of MMP and MM, penetrating insights about pseudogap behavior in cuprates would come not from INS, but from ARPES (see a brief review of this in Sect. 4.2). This point will be considered further in Chap. 6, where extensive INS studies of LSCO will be discussed.

5.3 T1 Model for YBCO Using INS Data for χ(q, ω) In the ﬁrst two subsections of this chapter we saw how both UM and MMP interpreted cuprate relaxation data in terms of AFM ﬂuctuations with a temperature-dependent correlation length. In the present subsection we review a ﬁt procedure performed by the Berthier group, wherein T1 data from a YBCO6.9 sample are interpreted in terms of an AFM ﬂuctuation peak characterized by INS measurements [7]. INS data are quoted which show the AFM peak to have a constant width, i.e. the ﬂuctuations are interpreted to have a temperature-independent correlation length.2 Here we review the data and analysis for this interesting case, which also includes extracting dynamic susceptibility parameters from data for T2g , the Gaussian spin-echo decay from indirect spin-spin couplings (see Chap. 6). We compare this case with the UM ﬁts in Sect. 5.1 in some detail. In the end, it is found that they are strikingly similar, and that the contrast between them reﬂects a diﬀerence in samples rather than one of methods. When large single crystals of YBCO7 became available, extensive neutron scattering measurements were reported, e.g. by Regnault et al., [24], RossatMignod et al., [25], and by Tranquada, Sternleib et al., [23, 26]. NMR measurements on 63 Cu(2) and 89 Y in single crystals so characterized have been reported by Auler et al., [7], where they noted that the AFM peaks from INS data on their sample and related samples are well-ﬁtted by a Gaussian, with a peak width which is essentially independent of temperature. The sample of YBCO6.9 in question gave some indication of disorder in spite of being nearly fully oxygenated. This was attributed to the presence of Sr2+ as a dilute substitutional impurity for Ba2+ , leading to fairly broad NMR lines with ﬁeld ⊥ c axis [27]. However, the NMR measurements were conducted normally. The other apparent consequence of this was that the sample exhibited a somewhat pseudogapped character compared with other YBCO samples with Tc = 90 ± 1 K. The pseudogap eﬀect is noticeable in relaxation curves for 63 Cu(2) shown in Fig. 5.7, where the data are seen to roll oﬀ below T ∼ 125 K for both ﬁeld orientations. Furthermore, there is no visible break in the relaxation curve at Tc , which is a characteristic of pseudogapped material. On the other hand, the 2

The MMP picture did not rule this possibility out, but in the absence of reliable INS data favored the scenario with temperature-variable correlation lengths [5].

180

5 Relaxation Models for Cuprate NMR

20 H0 // ab 15 10

H0 // c

63(T

1

T)–1 (s–1 K–1)

25

NQR 5 0

100

200

300

T (K)

Fig. 5.7. Relaxation rate 1/T1 T for 63 Cu(2) in YBCO6.9 [7], showing typical anisotropy for YBCO7, but pseudogap-like rolling oﬀ of the data below 120-130 K. Note that there is no break or other feature in the data at Tc ∼ 90 K. Reprinted ﬁgure from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

ratio T1c /T1ab 3.7 at T ∼ 100 K and declines slightly at higher temperatures, which is typical behavior for YBCO7. This YBCO sample is therefore rather unique in having pseudogap features with Tc ∼ 90 K. Both NMR shift and relaxation data for the 89 Y nuclei are shown in Fig. 5.8. The NMR shift is seen to roll oﬀ at lower temperatures, much like one of the slightly deoxygenated samples in Fig. 4.2. Correspondingly, 1/T1 T in Fig. 5.8(b) is also seen to decline at lower temperatures, though not quite so much as for YBCO6.6 (see, e.g. Fig. 4.1(b)). Again, like the 63 Cu(2), the general character is that of a pseudogapped system. 5.3.1 The Gaussian Model Susceptibility The authors introduce their Gaussian susceptibility model as follows [7]. Beginning with the standard form (cf. (4.2.2)) χ (q, ω) χ (q, 0) = , (5.3.1) ω Γq ω→0 it is supposed that on account of AFM exchange forces χ (q, 0) is peaked at q ∼ Q, and the spin ﬂuctuation frequency Γq has a minimum at the same point. Further, it is assumed that χ (q) = χAF (Q) f (q − Q) and Γq−1 = −1 f (q − Q) have the same functional form in the vicinity of Q, which is ΓAF taken to be a Gaussian f (Δq) = exp(− | Δq |2 ξ 2 /4).

(5.3.2)

The value ξ = 1.3a is taken from INS measurements on the same sample material [7]. Then, if we put the origin in q-space at Q, we may write f (Δq)

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

181

–150 (a) (ppm)

–100

89K

–50 H0 // ab

0

H0 // c (b)

2

1

89(T

1T)

–1

(104 S–1 K–1)

50

0 50

100

150

200

250

300

T (K)

Fig. 5.8. (a) NMR shift data for 89 Y in YBCO6.9 from [7] for ﬁeld oriented both and ⊥ c axis. 89 Kα (T ) shows pseudogap-like decline below T ∼ 200 K. (b) Data for the 89 Y relaxation rate 1/T1 T for the same sample and conditions as in part (a) Reprinted ﬁgure from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

= exp[−0.4225 (qa)2]. As in the MMP model, a noninteracting, q-independent term χ0 /Γ0 is added to give the relations χ (q, ω) χ0 χ (Q) exp[−0.845 (qa)2] = + AF (5.3.3a) ω Γ0 ΓAF (Q) ω→0 χ (q) = χ0 + χAF (Q) exp[−0.4225 (qa)2] .

(5.3.3b)

The parameters in this model ((5.3.2) and (5.3.3)) were then extracted from experimental data. We give here just a brief summary of the procedure. χ0 (T ) was deﬁned to be the uniform susceptibility, the temperaturedependence of which is derived from NMR shift data in Fig. 5.8(a), where the orbital shift value 89 Kc,orb = 160 ppm is taken from [15]. The scale factor for χ0 (T ) was obtained by comparing shift coeﬃcients for 89 Y and 17 O with values from the literature [7]. The resulting curve of χ0 (T ) vs. T is shown in Fig. 5.9(a). In that same ﬁgure is shown the curve for χAF (T ). This was extracted from data for 63 T2g (T ), which is shown in Fig. 5.9(b), using the relations ⎡ 2 ⎤ 1 c63 ⎣ z (5.3.4) = (aind (q))2 − azind (q) ⎦ 63 T 2 8 2g q q

182

5 Relaxation Models for Cuprate NMR

with azind (q) =

γ63 χ (q) [Ac + 4B cos qx a]2 . gc2 μ2B

(5.3.5)

These formulas are derived and discussed in Chap. 6. Here, we simply note that the T2g data of Fig. 5.9(b) were analyzed with the foregoing equations to obtain the plot of χAF (T ) shown in Fig. 5.9(a).

χ′ (10–4 emu / mol Cu(2))

1,5 10

χ′AF (QAF)

1,0

(a) 5

0

χ0

100

150

0,5

250

200

0,0

T (K)

8 (T2g)–1 (ms–1)

4

10 Δ ν1/2

63

63(T

12

(b)

–1 2g)

(ms–1)

12

8

0 50

100

0

100

150

T = 120 K 200 300 1/τ (kHz)

200 T (K)

400

250

300

Fig. 5.9. (a) The susceptibilities χ0 and χAF are plotted as a function of temperature. χ0 is the uniform susceptibility, with temperature dependence and amplitude scale derived principally from 89 Y NMR shift measurements as discussed in the text. χAF is the amplitude of the AFM ﬂuctuation peak at Q. Its value as a function of temperature was derived from measurements of T2g for the 63 Cu(2) NMR line. Equations (5.3.4) and (5.3.5) were used to interpret T2g data shown in part (b) of this ﬁgure. See text and Chap. 6 for more details [7]. (b) Data for T2g on 63 Cu(2) taken in the present study [7]. These data were interpreted to yield the values of χAF shown in part (a) of this ﬁgure. See text and Chap. 6 for more details of interpretation. The inset shows how data vary with the bandwidth of the refocussing π-pulse of the echo sequence, where a large bandwidth is essential to obtain accurate data Reprinted ﬁgures from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

183

The ﬁnal step, which is to evaluate the spin ﬂuctuation parameters Γ0 and ΓAF as functions of temperature, requires a bit more explanation. Auler et al., [7] note that the dipolar interaction makes an appreciable contribution to 1/89 T1 , which is not taken account of by the “D” terms of the HF tensor (3.3.2). This point has been noted by Takigawa et al., [15] and was discussed brieﬂy in Sect. 4.1.2. Auler et al., provide a separate calculation to estimate the extra dipolar relaxation terms, which behave a bit like the 63 Cu(2) terms in that they do not cancel at q = Q. In evaluating Γ0 and ΓAF as functions of temperature, these authors present several “options” regarding the dipolar terms. We ﬁrst describe their procedure for obtaining the Γ ’s and then describe the options. The values of Γ0 and ΓAF are obtained by ﬁtting the 63 Cu(2) and 89 Y T1 data with the model susceptibility (5.3.3) with (5.3.2), using (3.5.11)-(3.5.14), i.e. the standard Mila-Rice HF Hamiltonian. As an example, these authors note that if the AFM susceptibility peak were narrow enough it would not make a signiﬁcant contribution to 1/89 T1 T , which would then be given by [7] 1 89 T

1T

=

2 2γ89 kB Dab gab μB Γ0 (T )

89

Kab (T ) ,

(5.3.6)

so that Γ0 (T ) could be extracted directly from the data for 89 Kab (T ) and T1 (T ). In practice, (5.3.6) is not a good approximation, but serves to illustrate the method. In general, one has to use the data mentioned plus 63 T1 (T ) to evaluate both Γ0 and ΓAF simultaneously. For this purpose they have used values of the 63 Cu(2) and 89 Y HF tensors, in units of 10−6 eV , as follows: Ac = -1.56 (-1.64), Aab = 0.35 (0.16); B = 0.39 (0.41); Dab = -0.0035 (-0.0028); and Dc = -0.0043 (-0.0035), where the values in parentheses are the ﬁtted values from the UM analysis in Table 4.1 for comparison. Apart from Aab , which is small and diﬃcult to evaluate, these are all quite reasonable. The values derived for Γ0 and ΓAF are plotted in Fig. 5.10(a) and (b), respectively. The down triangles are obtained ignoring the dipolar terms altogether, while the open circles correspond to taking the dipolar terms fully into account. For the up triangles the value of Aab was also increased by 25%. Our main concern here will be the open circles, which correspond to apportioning a sizeable fraction of the 89 Y relaxation to dipolar terms. Since the susceptibility model has an AFM peak with a temperatureindependent width, the temperature dependence of the T1 data has to be accounted for by assigning the temperature variation (of 1/T1 T ) to the susceptibilities χ0 and χAF and to the spin-ﬂuctuation parameters Γ0 and ΓAF . The value of Γ0 is seen to approximately double from 250 K down to 100 K and ΓAF to change by less than that. It is, of course, very diﬃcult to know whether this is a reasonable scenario from the standpoint of microscopic physics, but it describes the data well enough. What is interesting is to compare this outcome with the results of the UM analysis, for which a temperature-dependent correlation length ξ(T ) was employed (Sect. 5.1). 89

184

5 Relaxation Models for Cuprate NMR 400

Γ0 (meV)

(a) 200

0 (b)

ΓAF (meV)

40

20 T* 0

100

150

200

250

T (K)

Fig. 5.10. (a) Values of the spin-ﬂuctuation frequency Γ0 deduced from ﬁtting the relaxation data for both 63 Cu(2) and 89 Y to the form for χ (q, ω) (5.3.3) discussed in the text. Results from the oversimpliﬁed approximation in (5.3.6) are shown as solid squares. Open circles show values obtained when the dipolar terms for the 89 Y relaxation are taken into account, and down triangles show values obtained when they are not. The up triangles result when the dipolar terms are kept, and the value of Aab is increased by 25 % over that given in the text. See text for discussion. (b) Values of ΓAF (see (5.3.3)) obtained in same way as in (a), with symbols indicating the same cases listed there. Reprinted ﬁgures from T. Auler, M. Horvatic et al, Physica C 313, 255 (1999). Copyright 1999 Physica C

5.3.2 Comparison with the UM Analysis Results for YBCO7 To eﬀect a comparison with the UM analysis, we use (3.5.17) and (3.5.18) to calculate τeﬀ and the Kij ’s, since χ (q, ω) is fully speciﬁed by (5.3.3) and (5.3.2) with the parameter values in Fig. 5.9(a) and Fig. 5.10(a) and (b) (circles). For these evaluations we use the other parameter values from [7], which were stated above. We ﬁrst note the contrast in parameterization of the Kij ’s between UM and the present work. We adopt a general form (5.3.7) Kij = K0 g(rij /λ) , where K0 and λ are both possible functions of temperature. In the UM analysis, K0 was taken to be unity and g(rij ) = exp(−2 rij /aλ), with all temperature dependence in the correlation length λ. For the Gaussian χ (q, ω) model of Auler et al., [7], however, the width parameter ξ is ﬁxed. The temperature variation has to reside in K0 (T ). Thus, it is possible to have temperature

5.3 T1 Model for YBCO Using INS Data for χ (q, ω)

185

varying correlations even when there is a ﬁxed correlation length. Calculations of the Kij ’s (see below) reveal that K01 (T ) reaches a value of –0.47 at 100 K and is about half that value at 250 K. These are typical numbers from the UM analysis. For comparison purposes the quantities τeﬀ (T) and the 63 Vα ’s have been evaluated using the model susceptibility parameters given by the analysis of Auler et al., described above. First, we evaluate τeﬀ (T) using (3.5.17) and (5.3.3), ﬁnding kB T χ0 χ τeﬀ (T ) = 2 + 0.0936 AF , (5.3.8) 4μB NA Γ0 ΓAF where the prefactor has been adjusted for susceptibilities in (emu/mole). Using the parameters from Fig. 5.9(a) and 5.10(a) and (b) (circles), we ﬁnd the values plotted in Fig. 5.11(a) vs. T (open squares). For comparison, The curves of τeﬀ (T) for YBCO7 (open circles) and YBCO6.63 (closed circles) from the UM analyses (Fig. 5.2(b) and 5.4(a), respectively) are plotted. Recalling that the YBCO6.63 curve was “gapped”, we see that there is a remarkably close correspondence in absolute magnitudes for τeﬀ and that the values from the present study are deﬁnitely “gapped” as well. As we noted earlier, the NMR shift and relaxation curves showed deﬁnite signs of a spin pseudogap. Corresponding to the foregoing expression for τeﬀ , we ﬁnd for the Kij ’s, Kij =

0.0936 χAF Γ0 [−0.745; 0.555; 0.309] , χ0 ΓAF + 0.0936χAF Γ0

(5.3.9)

where the numbers in the brackets represent K01 , K12 , and K13 , respectively. To plot 63 Vc and 63 Vab , this expression was used with interpolated data from Fig. 5.9(a) and 5.10(a) and (b) to calculate the 63 Vα ’s shown in Fig. 5.11(b) (ﬁlled squares for 63 Vc and ﬁlled diamonds for 63 Vab ). For comparison the same quantities for YBCO7 from the UM analysis (Fig. 5.3(a)) are plotted as solid lines. Again, considering that these materials are quite diﬀerent in detail, the correspondence is remarkably close. Notice that the three Kij ’s are in a constant ratio of -0.745:0.555:0.309 at all temperatures, but their coeﬃcient changes by about a factor two over 100 K≤ T ≤ 250 K. It seems, then, that there may be a variety of parameterizations which will give the same form for τeﬀ (T) and k Vα (T ), which is all that is needed to ﬁt the relaxation data. If follows that it will be very diﬃcult to work backward from such data to try to determine the details of some particular parameterization, as was the case with MMP. In ﬁrst-principles model theories such as those in the next two subsections, however, we suggest that it would be very useful and informative to calculate both τeﬀ and the Kij ’s as diagnostics.

186

5 Relaxation Models for Cuprate NMR 1.4 (a)

1.2

τeff (10–15 S)

1 0.8 0.6 0.4 0.2 0

0

50

100

150

200

250

300

200

250

300

T(K) 4.5 4

(b)

63Vα(1015s–2)

3.5 3 2.5 2 1.5 1 0.5 0

0

50

100

150 T(K)

Fig. 5.11. (a) Data for τeﬀ (T) have been calculated using (5.3.8) with interpolated data from Fig. 5.9(a) and 5.10(a) and (b) (open squares). These are compared with plots of τeﬀ (T) for YBCO7 (open circles) and for YBCO6.63 (dots), which have been calculated using (4.1.17) and (4.1.19) with parameter values form Table 4.2. Comparison shows a marked similarity with a clearly gapped character for the present YBCO6.9 sample. The main diﬀerence between the present case and the UM YBCO7 ﬁt is the marked pseudogap character of the results. (b) Plots of 63 Vc (ﬁlled squares) and 63 Vab (ﬁlled diamonds) for the same series of temperatures shown for τeﬀ in part (a). These quantities have been calculated with the HF parameter values from [7] given in the text using (5.3.9). Shown for comparison are the same quantities from the YBCO7 ﬁt by UM (Fig. 5.3(a)) (solid lines), where the discrepancy in both cases is a scale factor of order unity

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

187

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics Extensive model calculations of NMR shift and relaxation behavior have been performed by Bulut et al. [8], using the 2D Hubbard model to represent a cuprate-like system with enhanced magnetic ﬂuctuations near the AFM wavevector Q. These calculations with the Hubbard model bear some similarity to the mean-ﬁeld phenomenological model of MMP, the diﬀerence being that one is actually doing a ﬁrst-principles calculation of quasiparticle dynamics using a simpliﬁed Hamiltonian and approximate methods. The up side of this is that the results of such calculations have been adapted to realistic cuprate (i.e. Mila-Rice-Shastry) HF couplings and form factors to obtain shift and relaxation behavior which is not unlike typical experimental data. If there is a down side, it is that the 2D Hubbard model, as solved in this way, presents some rather quirky behavior with certain parameters which have no clear relation to microscopic physics. There is also some “implausible ﬁne tuning” of parameters to obtain desired behavior. The authors argue that this is simply a necessary aspect of using such a Hubbard model. In this section we present a brief summary of Hubbard model behavior and some calculated results for the NMR shift and relaxation of 63 Cu(2) and 17 O(2,3) sites of YBCO7. Behavior at T < Tc has also been treated in detail with these methods. The latter results will be presented in Sects. 5.7 and 6.2, along with other model results for the superconducting state. 5.4.1 Basic Formulation of the Dynamic Susceptibility The following is a summary and discussion of results for the square-lattice Hubbard model of a doped system with metallic behavior. For derivations the reader is referred to the original papers [8] and references therein. The basic Hamiltonian is + H = −t [c+ ni↑ ni↓ , (5.4.1) iσ cjσ + cjσ ciσ ] + U ijα

i

consisting of nearest-neighbor hopping terms and on-site coulomb repulsion, where U is actually a renormalized interaction parameter. The basic (U = 0) band proﬁle has width W = 8t with a logarithmic singularity at the center. The band ﬁlling is 0 ≤ n ≤ 2 particles per site. Near half ﬁlling there are commensurate and incommensurate spin-density wave phases, which must be avoided. For the assumed ratio U/W = 0.25, the critical value is nc = 0.865, above which there is an “unphysical phase transition” for the Hubbard model where U χ(q ∗ , 0) = 1. The amount by which n falls below nc determines the temperature T ∗ at which the amplitude of AFM ﬂuctuations saturates on lowering the temperature. Thus, n is only qualitatively related to the doping level parameter of the cuprate being modeled.

188

5 Relaxation Models for Cuprate NMR

The basic solutions to the Hubbard model (5.4.1) are as follows: The band energy is E(k) = −2t (cos kx a + cos ky a) and the single-particle density of states is 1 N (E) = K[(1 − (E/4)2 )1/2 ], (5.4.2) 2π 2 where K[ ] is the complete elliptic integral. The U = 0 (noninteracting) susceptibility is then given by χ0 (q, ω) =

f (Ep+q ) − f (Ep ) 1 , N p ω − (Ep+q − Ep ) + i0+

(5.4.3)

where f (Ep ) = 1/[exp(β(Ep − μ)) + 1] is the Fermi occupation function and μ is the chemical potential. For the interacting system the authors use the RPA to approximate χ(q, ω), giving χ0 (q, ω) , (5.4.4) χ(q, ω) = 1 − U χ0 (q, ω) closely analogous to (4.2.1). However, while (4.2.1) gave a peak near Q which dominated the behavior of interest or could be modeled with something else, here it was pointed out that the RPA approximation (5.4.4) does not accurately render the detailed dependences of K(T ) and 1/T1 on U and on the band ﬁlling n [8]. The best one can hope for is to choose U and n appropriately to extract the essential features of large-q spin ﬂuctuations. If we choose a band ﬁlling n near to but less than nc , then AFM ﬂuctuations will grow with declining temperature down to some point T ∗ where their amplitude saturates. T ∗ is controlled by the value of n. By choosing U/W = 0.25 and n = nc , the authors presented results for a case with large AFM enhancement eﬀects and a peak in χ (q, ω) near (but not precisely at) Q. The calculated NMR properties then give for the shift at low temperatures K=

N (μ) 2γe , A(0) γn 1 − U N (μ)

(5.4.5)

for a HF interaction parameter A(q), and for the relaxation rate 1 χ (q, ω0 ) kB T = A(q)2 , T1 N q ω0

(5.4.6)

where A(q) has the dimensions of frequency and χ (q, ω) of inverse energy (see (3.5.8)), and where the actual form of A(q) varies from site to site as usual. With the RPA susceptibility (5.4.4), (5.4.6) can be rewritten ! 1 |A(p − p )|2 kB T = , (5.4.7) T1 N [1 − U χ0 (p − p )]2 where the brackets indicate that p and p are to be summed over the Fermi surface.

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

189

The foregoing formalism has been used to calculate approximations to the NMR shift and relaxation behavior for 63 Cu(2), 17 O(2,3), and 89 Y in YBCO7. For this purpose calculations on the simple square-lattice Hubbard model have been generalized to include the eﬀects of Cu-O hybridization in a Hubbard model of CuO2 [8]. With a 3-center unit cell, the CuO2 lattice is modeled using “partial susceptibilities”, with coulomb repulsion only on the Cu site [8]. T1 calculations were presented with and without this modiﬁcation and, remarkably, the diﬀerences in T1 behavior were found to be fairly subtle. Here we present some of the results for each model. The NMR shifts at all sites undergo some Stoner enhancement according to (5.4.5), with very little temperature dependence. In Figs. 5.12 and 5.13, some of the T1 results are displayed, to be compared with experimental data for YBCO7. The bandwidth W is set at 1.2 eV, with U/W = 0.70, and n = 0.865, very near to the critical value. The ﬁeld is placed along the c axis. An on-site HF coupling form has been used for both the Cu(2) and O(2,3) for the ﬁrst two results shown. In Fig. 5.12(a), the relaxation curves for Cu(2) and O(2,3) are compared, where each is plotted as a fraction of its value at T /W = 0.025, which is approximately room temperature. The Cu(2) relaxation rate is seen to level oﬀ completely by room temperature, with rather more downward curvature than exhibited by the data (see Fig. 3.7), while the O(2,3) data also exhibit a slight downward curvature which is not unlike the experimental data (Fig. 4.9(a)). It seems that this extreme rollover of the Cu(2) relaxation is necessary in order to achieve the desired level of enhancement. The enhancement is shown for both Cu(2) and O(2,3) in Fig. 5.12(b), where the Korringa products (T1 T K 2 )−1 are plotted vs. T as fractions of the noninteracting values (T1 T K 2 )−1 = [(4π/kB )(γn /γe )2 ]. This gives an 0 enhancement of 4 for the Cu(2) and slightly greater than 1 for the O(2,3). The authors quote experimental values of 5.5 for Cu(2) and 1.4 for O(2,3) [12], in reasonable accord with their calculations. The Cu(2) enhancement, however, has declined to near the noninteracting value by just above room temperature, which is rather unlike the experimental results. Finally, we show in Fig. 5.13 a comparison of Hubbard model calculations with experimental data for 63 Cu(2) and 17 O(2,3) in YBCO7. For these calculations, the simple Hubbard model results were used [8] with realistic MilaRice-Shastry HF coupling form factors (i.e. | Aab /Ac | = 0.21 and | B/Ac | = 0.22), where we note that Aab is a bit larger here than usual estimates. In this case the Hubbard model parameters were also slightly diﬀerent from the foregoing, with U/W = 0.25 and n = 0.86 slightly below the critical value. Taken with the others, these calculations show that a fair range of T1 behaviors can be obtained with this model. 5.4.2 Remarks on the Hubbard Model Calculations One must, of course, evaluate the merits of this model in terms of the time frame of its development, in which case it was obviously highly successful. This

190

5 Relaxation Models for Cuprate NMR 1.2

1.0

ε / W = 0.7

(a)

U/W = 0.7 nh = 1.165

0.8 T1–1 T1–1(0.025)

0.6

0.4 Cu U = 0 Cu RPA O RPA

0.2

0.0 0.000

0.005

0.010

0.015

0.020

0.025

T/ W 10

ε / W = 0.7 U/W = 0.7 nh = 1.165

(b)

8 Cu O

6 (T1TK2)–1 (T1TK2)0–1 4

2

0 0.000

0.005

0.010

0.015

0.020

0.025

T/ W

Fig. 5.12. (a) Relaxation rates 1/T1 calculated for the Cu(2) and O(2,3) sites in YBCO7 and scaled to their values at T /W = 0.025 (approx. 300 K) are plotted vs. T /W . Calculations are made with the CuO2 model described in the text and references, using on-site HF couplings. The U = 0 (dashed) curves are also shown for reference. Conditions shown are E = 0, U/W = 0.7, and nh = 2 − n = 1.165, where E is the energy of the O(2pσ) orbitals where Ed = 0, and nh is somewhat above the critical value nh = 1.135. (b) The Korringa ratios for both Cu(2) and O(2,3) are plotted as a function of T /W in units of their noninteracting fermion values (4π/kB )(γn /γe )2 . The low-T enhancement ∼ 4 for the Cu(2) has decayed most of the way to its noninteracting, high-T limit by 300 K. Reprinted ﬁgure from N. Bulut, D. W. Hone, D. J. Scalapino, and N. E. Bickers, Phys. Rev. B41, 1797 (1990). Copyright 1990 American Physical Society

5.4 A Small-U Hubbard Model of Cuprate Spin Dynamics

O Cu O Exp. Cu Exp.

1.5

60 1.0 40

(T1 –1)c (msec–1)

(T1 –1)0 (sec–1)

80

191

0.5 20

0

0

100

200

0.0 300

T (K) Fig. 5.13. Small-U Hubbard model calculations, similar to those for Fig. 5.12, have been applied to ﬁtting T1 data, where the Mila-Rice HF tensor given in the text has been used. Calculated T1 curves have been ﬁtted to 63 Cu(2) (+) and 17 O(2,3) (•) data curves from [12] and [28], respectively. The conditions are slightly diﬀerent from Fig. 5.12, with U/W = 0.25 and n = 0.86. Reprinted ﬁgure from N. Bulut, D. W. Hone, D. J. Scalapino, and N. E. Bickers, Phys. Rev. Lett. 64, 2723 (1990). Copyright 1990 American Physical Society

is a ﬁrst-principles model for the spin dynamics of superconducting cuprates which gives a remarkable facsimile of experimental behavior with a single dynamical variable. The model was also an important test for the use of suitable form factors to shield the O(2,3) sites from enhanced AFM ﬂuctuations while the Cu(2) sites are very directly aﬀected by them. That said, the authors note that this model probably cannot be made to give a truly quantitative account of the NMR data in the normal state. The physics of the high-temperature region is quite diﬀerent from an actual cuprate, which typically approaches the degeneracy temperature not far above room temperature. The Hubbard model spin dynamics will clearly be Korringa-like up to any experimentally attainable temperature, while it seems that the cuprates are making a transition to insulator-like dynamics at high temperatures. The latter result is illustrated by the behavior of τeﬀ (T) for several systems in Sect. 5.1. In spite of the apparent drawbacks, however, the authors went on to treat relaxation in the superconducting state with the Hubbard model, yielding very interesting results. The latter results are discussed in Sects. 5.7 and 6.2.

192

5 Relaxation Models for Cuprate NMR

5.5 The Large-U Hubbard Model of Si, Levin et al An RPA model of cuprate quasiparticle dynamics, which is of the same class of models as the MMP mean-ﬁeld model [4, 5] and the small-U Hubbard model of Bulut et al., [8], has been developed and discussed extensively by Si, Levin, and co-workers [9, 29, 30, 31]. This is a 3-band Hubbard model with U essentially inﬁnite, wherein the nearest-neighbor AFM exchange from combined O2− –mediated superexchange plus RKKY sources is incorporated using the RPA approximation. Thus, it is similar to the foregoing models, except that the authors report that they have microscopically derived the Lindhard (noninteracting) susceptibility. As we shall see, this is not only a ﬁrst-principles calculation, but one with entirely realistic physical parameters. Here we will comment very brieﬂy on their results, and discuss a comparison with INS data and with T1 curves for 63 Cu and 17 O nuclei in the CuO2 planes. We suggest below that further calculations with this theory would be very interesting. The interesting diﬀerence between this model and those mentioned in previous subsections is that on a decrease in doping level, the system nears a localization transition rather than a magnetic (AFM) one. Moreover, owing to strong coulomb correlation eﬀects, the renormalized antibonding band narrows as the insulating limit is approached. Thus, the principal bandwidth parameter tpd → tpd (1 − nd )1/2 , where Mott localization occurs as the electron concentration nd → 1. The latter eﬀect, then, lowers the coherence temperature at which Fermi liquid behavior gives way to temperature-independent relaxation. In cases under consideration, this has been estimated to occur at a few hundred Kelvin [9, 29, 30]. Evidence for such eﬀects is clearly present in the Uldry-Meier analysis of cuprate T1 data in Sect. 5.1. For example, in Table 4.2 the eﬀective degeneracy temperature for YBa2 Cu4 O8 (Y248) is seen to be as low as 420 K. It would be very interesting if the large-U, tight-binding, Hubbard model calculation could account for this eﬀect. Extensive calculations of dynamical susceptibilities have been made with the method described [31]. These results may then be compared with INS data and with T1 data for both the 63 Cu and 17 O nuclei in the CuO2 plane. Plots of the structure factor S(q, ω) (i.e. χ (q, ω)) for two diﬀerent scans in q − space (see ﬁgure caption) are shown in Fig. 5.14(a) for YBCO7 and (b) for YBCO6.7.3 These results were calculated with the expression χrr (q, ω) = χ0rr (q, ω) +

χ0rd (q, ω)[−JH (q]χ0dr (q, ω) , 1 + JH (q)χ0dd (q, ω)

(5.5.1)

where the χrr ’s are “partial susceptibilities” [32], with r = p or d, χ0rr (q, ω) is the microscopically-derived Lindhard function [32], and JH (q) is the composite Cu-Cu exchange coupling, which is modeled here with 3

Similar results were also presented for LSCO. These are invoked in a discussion of that system in Chap. 6.

5.5 The Large-U Hubbard Model of Si, Levin et al

193

Q = (q,q)

0.2 0

T = II mev

q (r..u.) 0.3

0.5

0.7

S(Q,w) [arb. units]

T = 1 mev

0

0.2 S(Q*,w)

YBo2Cu3O7

Q = (q,q)

0.2

Q* = (1,qy) 2

T = 1 mev

Q* = (1,qy) 2

0.2 (a) 0 0.1

0.3

q Q = (q,q)

1

0.5 0.7 qy (r..u.)

0.9

T = II mev

q (r..u.) 0.3

0.5

Q* = (1,qy) 2

0.7 T = 1 mev

qy 0

Q* = (1,qy) 2

1

T = II mev

T = 1 mev

0

1

qy

0

Q = (q,q)

1

0 S(Q,w)

S(Q,w) [arb. units]

0.4

0 0.1

T = II mev

(b) 0.3 0.5 0.7 qy (r..u.)

0.9

Fig. 5.14. (a) Cross sections of S(q, ω) for YBCO7 are shown for ω = 15 meV, ﬁrst along the diagonal at T = 1 meV and 11 meV, and then along the qy axis for q = ( 12 , qy ) for the same two temperatures. (b) Cross sections of S(q, ω) for YBCO6.7 are shown for the identical set of conditions as in part (a). See the original papers for details of these calculations. Reprinted ﬁgures from Q. Si, Y. Zha, K. Levin, and J. P. Lu, Phys. Rev. B47, 9055 (1993). Copyright 1993 American Physical Society

JH (q) = J0 [cos qx a + cos qy a].

(5.5.2)

There is a critical value J0 = Jc , above which χrr (q, ω) is unstable. For YBCO7, J0 was taken to be 0.5Jc and for YBCO6.7 J0 = 0.7Jc , while the doping for these two was x = 0.18 and 0.36, respectively. For other details we refer the reader to [31] and [32]. Referring to the theoretical scan results in Fig. 5.14, plots of χ (q, ω) are shown for T ∼ 12 K and T ∼ 120 K. The AFM peak is commensurate and noticeably narrower for YBCO6.7, as expected. Although the authors emphasize the constancy of these results with temperature [31], the peaks in all cases seem somewhat lower and wider at 120 K, this eﬀect being incrementally greater for YBCO6.7. One can only imagine that at 300 K the peaks would be even wider, giving a palpable temperature dependence to the correlation lengths. Comparing these results with the INS data for reduced oxygen YBCO given by Tranquada et al., in Fig. 4.8 [23], there is some diﬀerence in peak shape, with the INS scan distinctly narrower. On the other hand, the INS crystal had a nominally lower doping level at x = 0.6 with Tc 50 K. The frequency of the measurement was ω ∼ 15 meV, while that of the calculation is 10 meV. All in all, one would say that the correspondence is satisfactory. The authors also use their results for χ (q, ω) to simulate relaxation rate curves for 63 Cu and 17 O as a function of temperature, using the same HF

194

5 Relaxation Models for Cuprate NMR

tensors as those employed by Bulut et al., in [8]. The results are shown for both compositions in Fig. 5.15 as temperature plots up to 360 K [31]. We make the following remarks about the nature and signiﬁcance of these results. •

•

•

•

Comparing these plots with experimental data (see Fig. 4.9), certain trends are seen to be qualitatively correct. The deviation from Korringa behavior is greater for the 63 Cu than for the 17 O, and greater for the YBCO6.7 than for the YBCO7. The amplitude trends are dramatically diﬀerent from the experimental data, where for 63 Cu, the experimental curves are intertwined so that YBCO6.7 rises above YBCO7 at T ∼ 150 K, but falls below YBCO7 at room temperature. For 17 O the curves are reversed, where experimentally (Fig. 4.9(a)), 1/T1 T for YBCO7 is relatively ﬂat and lying above the curve for YBCO6.7, which descends to a small fraction of its room temperature value at T = Tc ∼ 60–65 K. The latter circumstances arise, in part, because YBCO6.7 exhibits a spin pseudogap eﬀect in which the susceptibility, as well as 1/T1 T for the 17 O, decline at low temperatures ∝ exp(−Δ/kB T ), where Δ/kB = 104 K (see Sect. 4.1.2). The Hubbard model discussed here [31, 32] does not have this feature, so that comparison with YBCO6.7 data, especially at low temperatures, is not meaningful. A model of low-frequency spin ﬂuctuations for the case of a pseudogap has been given by Varma [33]. The authors have some concern that the 17 O results are not as Korringalike as the experimental data for YBCO7 and/or are not compatible with their calculation for 63 Cu. The straightforward answer to this is found in the Uldry-Meier analysis of T1 data, presented in Sect. 5.1. This type 3.5

3.5

(a)

2.5 2.0 1.5 YBa2Cu3O7

1.0 0.5 0

(b)

3.0 YBa2Cu3O6.7

(1/ T)0 [arb. units]

(1/T1)Cu [arb. units]

3.0

YBa2Cu3O6.7

2.5 2.0 1.5 1.0

YBa2Cu3O7

0.5 0

60

120 180 240 300 360 T(K)

0

0

60

120 180 240 300 360 T(K)

Fig. 5.15. (a) Relaxation rates 1/T1 for 63 Cu, calculated for both YBCO7 and YBCO6.7 using the results for χ (q, ω) shown in Fig. 5.14 and the HF tensor given by Bulut et al., [8], are plotted as a function of temperature [31]. (b) Similar calculated results are plotted vs. T for the case of planar 17 O, using the same methods. Reprinted ﬁgures from Q. Si, Y. Zha, K. Levin, and J. P. Lu, Phys. Rev. B47, 9055 (1993). Copyright 1993 American Physical Society

5.6 Relaxation via Orbital Currents proposed by Varma

•

•

•

195

of analysis was not, of course, available in the early 1990’s when the Hubbard-model calculations were being developed. The main signiﬁcance of the UM analysis is that it separates the dynamical from the quasiparticle spin-spin correlations (Kij from (2.5.17)–(2.5.18)) dynamical function (2.5.17) Xat (T ) = q [χ (q, ω)/ω]ω→0 . (The UM analysis uses the related parameter τeﬀ (T ) = (kB T /)Xat (T ).) Given a theory for χ (q, ω), then Kij and τeﬀ are straightforward quantities to evaluate. In the latter formulation, the 63 Cu and 17 O curves contain the same dynamical information, but very diﬀerent correlation eﬀects. The latter may be seen in Fig. 5.3(a) and (b). The experimental dynamical function for YBCO7 is shown in Fig. 5.2(b). Si et al., attributed the strong curvature of the 63 Cu 1/T1 curve to a coherence temperature [29]. This may be something of a misapprehension, since the curve is strongly aﬀected by T-dependent spin-spin correlations. The true picture of dynamical behavior with temperature would be given by τeﬀ vs. T . It would be most interesting to see whether this theory would provide an explanation for the ﬂattening oﬀ of dynamical ﬂuctuations at high temperatures, since at the present time there is no theory for this available. The large-U RPA model seems especially suited to this, because the band-narrowing eﬀect with hole dilution [9] is similar to what is observed in practice (see Table 4.2). We further suggest that the reason for the strong deviation from Korringalike behavior for the 17 O in Fig. 5.15(b) is that the corresponding peak in Fig. 5.14 has much wider wings than the INS-measured peak in Fig. 4.8. This situation is a bit like the Lorentzian vs. Gaussian models by MM [5], where the Gaussian model with steeper sides gives far less contribution to the 17 O(2,3) relaxation rate. The downward curvature of the plot of 1/T1 for the 17 O is probably mainly due to the dynamical correlation factor, leaving the impression that τeﬀ (T) may be nearly linear in T . Nonetheless, an actual evaluation of τeﬀ for diﬀerent carrier levels would answer a very interesting question about the large-U Hubbard model, namely whether it can account for the high-temperature transition in the dynamics seen in the experimental data, such as Fig. 5.2(b) and Fig. 5.4(b).

5.6 Relaxation via Orbital Currents proposed by Varma Up to this point only spin-paramagnetic T1 processes have been considered for the doped cuprate superconductors. However, in 1989 a somewhat radical idea was proposed for these systems, namely that for a certain class of charge excitations the polarizability has a term which obeys [34] " −N (0)(ω/T ) f or | ω |< T ImP˜ (q, ω) ∼ , (5.6.1) −N (0) sgn(ω) f or | ω |> T

196

5 Relaxation Models for Cuprate NMR

where N(0) is the one-particle density of states. Applying this marginal Fermi liquid (MFL) ansatz to magnetic processes at NMR frequencies ω0 kB T /, we have 2 N (0)ω0 χmf l (q, ω) = , (5.6.2) kB T where we have added the factor 2 /kB to make clear that this is dimensionally a correlation time. To apply this ansatz to an HF perturbation process, we suppose that there is a quasiparticle interaction term γn Hmf l I ·f (q) with a (dimensionless) q-dependence factor f (q). Then, by the usual argument ((3.5.8)–(3.5.9) this generates a temperature-independent T1 process 2 χmf l (q, ω0 ) 4γn2 Hmf 1 l kB T 2 = f⊥ (q)2 = 4γn2 Hmf f⊥ (q)2 , l N (0) T1 ω 0 q q

(5.6.3) where the second step used (5.6.2), and N (0) ∼ /EF is a correlation time. Such processes in metals would be very strong. It has already been noted that such a dynamic would not apply to spin ﬂuctuation processes in cuprates. However, it was subsequently proposed by Varma [10] that the MFL scenario could be applied to magnetic ﬂuctuations which result from circulating orbital currents, yielding a T1 process for the Cu(2) sites. Here we review the arguments leading to an estimate given for 63 T1orb [10]. The proposed T1 mechanism would operate via the orbital HF interaction (see (2.2.1)) Horb = I · M orb = iI · L/r3 = iI·r × ∇/r3 ,

(5.6.4)

where the local angular momentum operator L is associated with the Cu(2) site. Horb could then act to scatter quasiparticles from k + q/2 to k − q/2, where the squared matrix element for the relaxation process would be summed over k and q. However, since the occupied 3d wavefunction in the cuprates is thought to be purely dx2 −y2 , the orbital HF matrix element ∗ (r)

k + q/2 | M orb | k − q/2 = e−iq·r Uk+q/2

L Uk−q/2 (r), r3

(5.6.5)

(exp[i(k + q/2) · r]Uk+q/2 (r) is a typical Bloch function) will have no intrasite contribution ∼ forb γn μB r−3 , where forb is the orbital symmetry factor (see Fig. 2.9) and r−3 ∼ 6 a.u. for 3d electrons. Thus, for a dx2 −y2 ground state forb = 0. It is for this reason that the conventional orbital T1 mechanism, which is often predominant in d-band metals, is absent in the cuprates. The leading contribution to (5.6.5) will come from cross terms between the Cu(2) site and its oxygen neighbors. To show how this develops, the behavior of k + q/2 | Morb | k − q/2 was examined [10] for k ∼ 0 and small values of q. In this limit, Uk+q/2 (r) ∼ U0 (r) can be written 1 Ai,α (0) φ(r − Ri,α ) , U0 (r) = √ N i,α

(5.6.6)

5.6 Relaxation via Orbital Currents proposed by Varma

197

where α is summed over the three sites in the CuO2 unit cell, and i is summed over cells. The local wavefunctions are φ(r − Ri,α ) ∼ dx2 −y2 in a Cu(2) site and ∼ pσ = px,y on the oxygen neighbors. The phase factors Ai,α (0) = ±1 must be adjusted appropriately (see [10], Fig. 1). The principal HF ﬂuctuations from orbital currents will be along the c axis, which we label z. Since Lz φd (r) ∼ dxy for φdx2 −y2 at the origin, one must ﬁnd dxy -like symmetry on the oxygen neighbors. For small q the relevant term (5.6.5) becomes Lz q · rφp (r − Rn ) 3 φd (r), (5.6.7)

k + q/2 | Morb | k − q/2 i r n where n is summed over the neighbors. One can then choose the term from rφp (r − Rn ) which has xy symmetry to obtain a non-zero matrix element. There will evidently be a non-zero contribution from larger values of q as well. On the other hand it is argued that there is no corresponding non-zero Cu-O term if the origin is placed on the oxygen site. This is fairly obvious, because at r ∼ ˆix, Lz px ∼ py , and xpy is orthogonal to dx2 −y2 . So the orbital currents can produce a z-axis T1 ﬂuctuation, and possibly through the apical oxygens some smaller in-plane ﬂuctuations at the Cu(2) site, but not at the O(2,3) sites. To estimate the strength of the corresponding T1 process, we can write the orbital dynamical structure factor, in analogy with (3.5.4)–(3.5.7), as 1 T1orb

=

2 2 μB 2kB T γ63

Morb (q)Morb (−q)ω0 ω0 2 q

=

kB T ω0

63

A2orb

(qa)2 χmf l (q, ω0 ) ,

(5.6.8)

q

where 63 Aorb is γ63 μB / times the intersite matrix element from the righthand side of (5.6.7). To obtain the ﬁnal expression for T1orb the MFL ansatz correlation time (5.6.2) is modiﬁed by replacing the eﬀective quasiparticle scattering rate kB T / in the denominator by kB T / + 1/τ0 , where 1/τ0 is a disorder-generated scattering rate of the order of tens of degrees [10]. With this change, (5.6.8) then gives 1 kB T = 63 A2orb N (0) . T1orb kB T + /τ0

(5.6.9)

In applying this to cuprate relaxation data, we note that for T > 100 K (5.6.9) assumes a nearly constant value 1/T1orb 63 Aorb N (0). The HF parameter 63 Aorb is very diﬃcult to estimate from (5.6.7). The main contribution will come from the overlap region between the Cu(2) and O(2,3) sites, and is probably 1–2 orders of magnitude smaller than the 3d on-site orbital HF ﬁeld (see Sect. 3.2.3 and Table 3.4) Horb = 2μB r−3 3d ∼ 125 kOe/μB . From the UM analysis of Sect. 5.1 (Table 5.2) we estimate N (0) ∼ /kB TF

198

5 Relaxation Models for Cuprate NMR

8 × 10−15 s for YBCO7. In this case, taking an optimal symmetry factor forb = 0.6, we ﬁnd for the maximal, on-site orbital relaxation rate 1 2 2 = forb γ63 Horb N (0) = 3.8 × 103 s−1 . (5.6.10) T1orb opt This is ∼ 3 times the measured relaxation rate for YBCO7 at T = 100 K. The rate in (5.6.9) is estimated to be a few percent of (5.6.10) at most. Interestingly, the combination of (5.6.9) and spin-paramagnetic processes which vary as 1/T1 ∝ T have been shown to give a good account of 63 Cu(2) relaxation data for both YBCO7 and optimally-doped LSCO. These results are shown in Fig. 5.16, where they are compared with data from [13] and [35]. For the calculated curves in this ﬁgure 1/τ0 is taken to be 25 K and 100 K for YBCO7 and LSCO, respectively. The quantity 63 A2orb N (0) is taken to be ∼ 3 × 103 s−1 , which is very near the estimated upper limit for an orbital contribution. A ﬁnal point has to do with how the orbital relaxation would ﬁt into the scheme of T1 analysis described in earlier subsections of this chapter. Since the UM analysis in Sect. 5.1, for example, is internally consistent and is consistent with the Mila-Rice, spin Hamiltonian parameters derived from shift measurements in Chaps. 3 and 4, a contribution from 1/T1orb at the 10% 5

–1) –1 (msec CuT1,⊥

4

3

2 –1 (YBa Cu O CuT1,⊥ 2 3 6,9)

1

0

–1 CuT1,NQR (La1.85Sr0.15CuO4)

0

100

200 300 Temperature (K)

400

Fig. 5.16. Orbital relaxation rates estimated with (5.6.9) are compared with experimental data for YBCO7 [13] and optimally-doped LSCO [35] as shown. For the plotted curves 63 A2orb N (0) is taken to be 3200 s−1 and 2800 s−1 , and 1/τ0 is taken to be 25 K and 100 K for YBCO7 and LSCO, respectively. See text for discussion of these calculations. Reprinted ﬁgure from C. Varma, Phys. Rev. Lett. 77, 3431 (1996). Copyright 1996 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

199

level would pose no problem. To accommodate a larger contribution than that would pose something of a challenge to the internal consistency of our current thinking on T1 in the cuprates. The presence of orbital current ﬂuctuations in cuprates has now been veriﬁed by neutron scattering studies [36], so there is no doubt about their existence. Further, they appear to be closely associated with the pseudogap eﬀect. Whether these ﬂuctuations are observable via NMR (other than the well-known NMR pseudogap eﬀects reviewed in Chap. 4) remains to be established. An important theoretical step toward further elucidation would be a serious eﬀort to evaluate the intersite orbital matrix element in (5.6.7).

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

In Sect. 3.6 we saw how a straightforward adaptation of the RPA susceptibility model to the BCS formulation of nuclear relaxation by Monien and Pines [3] gave a good account of the NQR T1 (T ) for 63 Cu(2) at T < Tc (YBCO7). Following that pioneering work there were important developments on the experimental side. As shown in Fig. 3.11(b), there had been a serious discrepancy between high-ﬁeld NMR T1 data below Tc and that obtained with NQR. One suspected that, as was found for the V3 X compounds in Sect. 2.3.5 (see Fig. 2.13), relaxation by spin diﬀusion to the normal cores becomes appreciable in high ﬁelds. Thus, the precise scaling between T1 curves for 63 Cu(2) and 17 O(2,3) observed by Hammel et al., is strongly dependent on the applied ﬁeld [12]. In an eﬀort to determine the intrinsic relaxation times for 63 Cu(2), a careful study of the ﬁeld dependence of T1 below Tc in YBCO7 using oriented powder samples was conducted by Martindale et al., [37]. The results are as follows: For ﬁeld (i.e. quantization axis) along the c axis, T1 was measured in 8.31 T, 4.14 T, and 0 T (NQR). For ﬁeld ⊥ c axis, T1 was measured in 8.31 and 0.45 T. Measurements were conducted at a series of temperatures 20 K≤ T ≤ 100 K, with the results plotted semilogarithmically in Fig. 5.17(a). For H0 c axis, the variation of T1 with ﬁeld is substantial, where at 20 K and 8 T ﬁeld increases the relaxation rate by a factor ∼ 5. The ﬁeld dependence with the ﬁeld in the ab plane is measureable, but much smaller.4 In the remainder of the discussion, then, NQR data or data taken in very low applied ﬁeld will be preferred. In Fig. 5.17(b) 1/63 T1ab T , scaled to its value at Tc , is plotted semilogarithmically vs. T . It is seen to behave very nearly as 1 e−b(1−T /Tc ) , (5.7.1) 63 T 1ab T 4

The authors refer to the conclusion by Redﬁeld and Genack [38] that relaxation by diﬀusion to the normal cores in the vortex state is not physically viable. Further analysis of this problem by Furman and Goren seems to have restored the validity of such a T1 process [39]. Expermental evidence for it is, of course, very strong.

200

5 Relaxation Models for Cuprate NMR 101

(a)

63W 1

(ms–1)

100

H0 = 0.45T

10–1

H0 = 8.31T H0 = 0T

10–2

H0 = 8.31T H0 = 4.14T

10–3

0

20

40

60 80 100 Temperature (K)

120

140

100

63W

10–1 T / Tc

1a /

63W

1a(Tc)

(b)

H0 = 0.45T

10–2

H0 = 8.31T 10–3 0.0

0.2

0.4

0.6

0.8

1.0

T / Tc

Fig. 5.17. 63 Cu(2) relaxation data from the work of Martindale et al., [37]. (a) Semilog plot of 1/T1 for 63 Cu(2) (63 W1 ) vs. T in the range 0≤ T ≤ 100 K for YBCO7. Data are presented for diﬀerent values of applied ﬁeld, including NQR data for zero ﬁeld. The open symbols show data with ﬁeld (i.e., quantization axis) along the c axis, while ﬁlled symbols are for ﬁeld ⊥ the c axis. (b) Semilog plot of 1/T1ab T for 63 Cu(2) (63 W1a /T ), normalized to its value at Tc , as a function of T ≤ Tc . This plot illustrates the exponential behavior, as well as the weak ﬁeld dependence of 1/T1ab T below Tc . Reprinted ﬁgures from J.A. Martindale, S.E. Barrett, C.A. Klug, K.E. O’Hara, S.M. DeSoto, C.P. Slichter, T.A. Friedmann, and D.M. Ginsburg, Phys. Rev. Lett. 68, 702 (1992). Copyright 1993 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

201

with b ∼ 6. The c axis data exhibits similar behavior, except that it begins a bit more slowly and the coeﬃcient b is slightly larger. Over a decline in −1 63 −1 relaxation rates of a factor ∼ 300, the ratio 63 T1ab / T1c behaves as shown in Fig. 5.19(a). To discuss the curves and data presented there, however, we must ﬁrst review the calculations reported by Bulut and Scalapino [40, 41]. 5.7.1 χ (q , ω) for the Small-U Hubbard Model at T < Tc The calculations by Bulut et al., [8] of T1 behavior in the normal state based on χ(q, ω) =

χ0 (q, ω) , [1 − U χ0 (q, ω)]

(5.7.2)

where U is the coulomb repulsion renormalized due to particle-particle correlations, is discussed at some length in Sect. 5.4. This theory was ﬁtted to relaxation data by choosing U = 2t and band occupation number n = 0.86. Their treatment of the superconducting state with these same parameter values [40, 41] is discussed in this subsection. To model the dynamic susceptibility for T < Tc , these authors used the RPA form (5.7.2) with the “irreducible BCS susceptibility” given by [41] χ0 (q, ω) = f (Ep+q ) − f (Ep ) 1 1 Ep+q Ep + Δp+q Δp 1+ N p 2 Ep+q Ep ω − (Ep+q − Ep ) + iΓ 1 Ep Ep+q Ep + Δp+q Δp 1 − f (Ep+q ) − f (Ep ) Ep+q + 1− + − 4 Ep+q Ep Ep+q Ep ω + (Ep+q + Ep ) + iΓ Ep Ep+q Ep + Δp+q Δp 1 − f (Ep+q ) − f (Ep ) 1 Ep+q − − − 1+ 4 Ep+q Ep Ep+q Ep ω − (Ep+q + Ep ) + iΓ (5.7.3) In (5.7.3) the dispersion relation is Ep = (Ep2 +Δ2p )1/2 and Ep = −2t (cos pxa + cos py a) −μ, where μ is the chemical potential and Δp is the gap function. For Δp we will consider here the case of a d-wave form Δp (T ) = [Δ0 (T )/2](cos pxa − cos py a),

(5.7.4)

where a BCS temperature dependence is adopted for Δ0 (T ). There is a ﬁnite broadening parameter Γ (T ) to be speciﬁed below. Finally, the superconducting transition temperature was taken to be Tc = 0.1 t, where at T = Tc the 63 Cu(2) relaxation rate has approximately the correct value and degree of AF enhancement to correspond to YBCO7 at 100 K. In [41] this formalism was used to treat and discuss both s-wave and d-wave gap symmetries with diﬀerent choices of parameter values. Since this work was completed several years before d-wave symmetry was conﬁrmed for the

202

5 Relaxation Models for Cuprate NMR

cuprates through the observation of phase jumps at the boundaries of Josephson junctions [42, 43], at that time there were still many proponents of s-wave pairing. We shall not dwell on the s-wave case here, but will point out how convincingly the relaxation behavior argues in favor of d-wave pairing in this theory. The early work of Monien and Pines [3] discussed in Sect. 3.6 also weighed heavily on the side of d-wave. We ﬁrst look at the behavior of T1 as treated with this formalism [41]. The usual expression (4.2.7) kB T 1 2 χ (q, ω0 ) = | A(q) | (5.7.5) T1 4 q ω ω→0

is employed with with the Mila-Rice-Shastry HF tensors (4.2.8). To see how this model distinguishes s-wave and d-wave behavior, it is useful to consider how the quantity [χ (q, ω)/ω]ω→0 χ (q, ω) = 0 (5.7.6) ω [1 − U χ0 (q)]2 ω→0 behaves with temperature in diﬀerent regions of q-space. For the s-wave case, χ0 (q, 0) declines for all q values below Tc , so that the enhancement factor [1 − χ(q, 0)]−2 will decline for all HF tensors [41]. In contrast, for the d-wave case, χ0 (q, 0) is only suppressed for | q |≤ 1/ξsc , where ξsc is the superconducting correlation length. The region around Q = (π, π) is not suppressed because of the nodes in the gap. Thus, AFM ﬂuctuations persist into the SC state for the d-wave case. The other factor present in (5.7.6) is χ (q, ω) D0 (q) = 0 . (5.7.7) ω ω→0 Fig. 5.18(a) is a plot of how D0 (q) varies with temperature for a very small value of q, and in part (b) it is shown how it varies for q near to Q. In the s-wave case the two are very nearly the same, but for d-wave they are quite diﬀerent. This sets up a diagnostic where if we look at the ratio of T1 values for sites which depend very diﬀerently on q, there will be a large expected diﬀerence between predicted behavior for s-wave and d-wave. Comparison of RPA Calculations with T1 Data The authors have calculated and discussed T1 behavior for a number of cases of parameter values with both s-wave and d-wave gap symmetry. The contrast between these two symmetries is best displayed by taking the ratio of T1 values for cases which have diﬀerent degrees of dependence on ﬂuctuations near Q, as shown in Fig. 5.18. As was clearly illustrated by Takigawa et al., [44], T1ab for 63 Cu(2) is most strongly dependent on AFM ﬂuctuations, with a lesser

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

203

dependence for T1c , and very nearly zero dependence for the oxygen 17 O(2,3) relaxation T1O (for any axis). To illustrate the foregoing eﬀect, calculations and experimental data were presented for T1c /T1ab (63 Cu(2) in YBCO7) [40], which we reproduce in Fig. 5.19(a). Over a range of ∼ 3 orders of magnitude in relaxation rates, the variation of T1c /T1ab is relatively slight, but has a deﬁnite signature. The data shown are the low-ﬁeld measurements of Martindale et al., [37] (squares) reviewed above, and similar low-ﬁeld measurements of T1ab combined with low-ﬁeld NMR measurements (ﬁlled circles) and NQR (H = 0) measurements (open circles) of T1c [44], which give equivalent results. The theory curves plotted for s-wave (2Δ0 /kB Tc = 4 (dotted line) and 8 (dashed line)) are seen to drop slightly, then remain ﬂat, since there is no real distinction between the D0 (q) curves (Fig. 5.18). For the d-wave case (solid curve), however, the drop and then rise reﬂect clearly the diﬀerence in behavior of the respective D0 (q) curves in Fig. 5.18(a) and (b). The observed ratio in Fig. 5.19(a) is a very clear sign in favor of d-wave gap behavior, which appeared several years before d-wave symmetry was widely accepted for the cuprates. The ratio T1O for 17 O(2,3) to T1c in Fig. 5.19(b) is also clearly supportive of d-wave symmetry. The message here is somewhat muted, owing to the fact that no low-ﬁeld 17 O(2,3) T1 data were available at the time, so the entire data base for the latter plot is 7–8 T NMR data [12]. The latter circumstance would only aﬀect behavior at the low-temperature end, however, so the comparison with theory is for the most part justiﬁed. 1

1.5 s – wave d – wave

0.8

(b) D0(q)

(a)

1 D0 (q)

s – wave d – wave

q = (0.05π, 0) 0.5

0.6 q = (π, 0.9π) 0.4 0.2

0

0

0.2

0.4 0.6 T/ TC

0.8

1

0

0

0.2

0.3

0.6

0.8

1

T/ TC

Fig. 5.18. (a) The quantity D0 (q), deﬁned in (5.7.7), characterizes the variation in intensity of low-energy ﬂuctuations over the Brillouin zone. In part (a) this quantity is plotted vs. T /Tc at q = (0.05π, 0) for s-wave and d-wave gaps as shown. Here and in part (b), 2Δ0 = 3.52 kB Tc , and broadening Γ = 0.3Tc has been used to control the coherence factor singularity. (b) The quantity D0 (q) is plotted for the same parameters as in part (a), except that q = (π, 0.9π). A sharp contrast between s-wave and d-wave behavior is seen to occur. Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. B45, 2371 (1992). Copyright 1992 American Physical Society

204

5 Relaxation Models for Cuprate NMR 6 5

T1c / T1ab

4 3 2

(a)

1 0

0

0.2

0.4

0.6

0.8

1

0.6

0.8

1

T/ TC 0.4 0.2

T10 / T1c

1 0.8 0.6 0.4

(b) 0.2 0

0

0.2

0.4 T/ TC

Fig. 5.19. (a) For 63 Cu(2) in YBCO7, a plot of the ratio T1c /T1ab vs. T /Tc for temperatures in the superconducting state. The square symbols represent low-ﬁeld data from Fig. 5.17 [37]. The circles are data from Takigawa et al., [44], where the open circles represent T1c data taken using NQR (H = 0) and the closed circles represent data taken in a c-axis ﬁeld of 0.44 T. The data for T1ab were taken in a transverse ﬁeld of 0.44 T. See the text for an explanatory note on these measurements. The solid line is the calculated curve for a d-wave gap as described in the text, using 2Δ0 /kB Tc = 8. The other lines represent calculations with an s-wave gap assuming 2Δ0 /kB Tc = 4 (dotted) and 8 (dashed), respectively. (b) The ratio of the 17 O(2,3) relaxation time T1O and T1c (for 63 Cu(2)) is plotted vs. T /Tc as in (a), but with plotted data scaled to their value at Tc . The data are from Hammel et al., [12] and were measured in ﬁelds of 7–8 T. The calculated curves correspond to the same set of cases as in (a). Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. Lett. 68, 706 (1992). Copyright 1992 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

205

It is interesting to note that a simple modiﬁcation of the analysis would make the displayed eﬀect in Fig. 5.19(a) somewhat more dramatic. This is suggested by the method of T1 measurement employed by Takigawa et al., [44], in which they write 1 1 = Jab + Jc ; = 2 Jab , T1ab T1c

(5.7.8)

where the Jα ’s are terms corresponding to HF ﬂuctuations along the α axis.5 With ﬁeld applied ⊥ to the NQR principal axis to measure T1ab , a complex set of terms occurs in the relaxation process. Thus, Jc (T ) and Jab (T ) are actually measured separately. Compared with T1c /T1ab , a plot of Jab /Jc [44] would show a more striking contrast between s-wave and d-wave. Finally, it is interesting to simply compare an RPA calculation of T1c (T ) for T < Tc [41] with NQR data attributed to Takigawa, Smith, and Hults [44]. These results are shown in Fig. 5.20(a), where the experimental points are open circles and the calculation is shown as a solid line. The data points are seen to drop very steeply below Tc , then approach a T 3 behavior (dashed line), as expected for a d-wave gap. The RPA calculation gives a very good account of this behavior [41].

RPA Theory for the NMR Shift below Tc Bulut and Scalapino also calculated the NMR shift behavior with their model [40, 41], which is simply given by Ks (T ) ∝ χ(q → 0, 0) =

χ0 (q → 0, 0) . 1 − U χ0 (q → 0, 0)

(5.7.9)

There is also a temperature-independent Van Vleck shift term, which renders the zero of Ks (T ) a bit uncertain. This has been subtracted oﬀ in the data plot of Fig. 5.20(b). The data shown are for 63 Cu(2) by Barrett et al., [16] (crosses) and 17 O(2,3) by Takigawa et al., [45, 46] (circles). All data are scaled to their total estimated excursion between Tc and 0 K. Theoretical curves are shown for U = 2t and several values of the d-wave gap parameter 2Δ0 /kB Tc . As the authors note [41], the lowest-temperature value is very important here. If the curves had been least-squares ﬁtted to the two sets of data, it appears that the dashed curve (2Δ0 /kB Tc = 6) would have been an excellent ﬁt. The distinction between Ks (T ) for s-wave and that for d-wave is that for d-wave the curve approaches T = 0 with a ﬁnite slope, but with zero slope for s-wave [41]. The data are certainly consistent with a ﬁnite slope, although 5

This is the same procedure as that used in the UM analysis of Sect. 5.1., where the Uα ’s deﬁned there are the same as the present Jα ’s.

206

5 Relaxation Models for Cuprate NMR

log10[T1–1(T)/ T1–1(Tc)]

0

(a) –1

–2

–3 –0.8

–0.6

–0.4 –0.2 log10(T/ Tc)

0

0.2

1.2 2Δ0 = 3.52KTc

1

2Δ0 = 5.0KTc 2Δ0 = 6.0KTc 2Δ0 = 3.52KTc

Ks(T)/Ks(Tc)

0.8 0.6

(b) 0.4 0.2 O(2,3) 0 –0.2

Cu(2) 0

0.2

0.4

0.6 T/ Tc

0.8

1

1.2

Fig. 5.20. (a) The c-axis relaxation rate T1c for 63 Cu(2), scaled to its value at Tc , is plotted logarithmically vs. T /Tc . The data are attributed to Takigawa, Smith, and Hults [44]. The relaxation rate drops sharply below Tc , then falls very nearly as T 3 (dashed line). The solid curve shows the RPA theory calculation for the d-wave case with U = 2t and 2Δ0 /kB Tc = 8. (b) The behavior of the NMR shift Ks (T ), scaled to its value at Tc , is plotted for 0≤ T /Tc ≤ 1. The crosses with error bars are 63 Cu(2) data from Barrett et al., [16], and the open circles are 17 O(2,3) data from Takigawa et al., [45, 46]. The lines plotted are calculations for a d-wave gap with U = 2t and various values of Δ0 as shown. Reprinted ﬁgures from N. Bulut and D. J. Scalapino, Phys. Rev. B45, 2371 (1992). Copyright 1992 American Physical Society

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

207

the scatter is large enough so that s-wave is not ruled out. All in all, the shift results are a nice complement to the T1 data. The two together make a very strong case for d-wave symmetry. 5.7.2 T1 and Spin-Spin Correlations below Tc : The UM Analysis In this ﬁnal subsection we consider the behavior of T1 below Tc from another standpoint, one which does not employ any particular microscopic model of the spin dynamics, but relies only on the general formulation of the T1 process involving χ (q, ω) and the Mila-Rice HF Hamiltonian (3.3.2) (see Sect. 3.5.3). This, of course, is the basic premise of the Uldry-Meier analysis of cuprate T1 data presented in Sect. 5.1. These authors and co-workers have also employed this approach to discuss the behavior of spin-spin correlations above and below Tc and have come to two remarkable conclusions [47]. First, they ﬁnd that inplane spin-spin correlations vanish as T → 0 in a fashion roughly symmetrical to how they vanish at high temperatures. Secondly, they give evidence that it is only the in-plane correlations which vanish, while the c-axis correlations remain basically unchanged below Tc . To review the UM formulation, relaxation of the k th nuclear spin species quantized along the α axis is written (see Sect. 5.1) 1 kT

1α (T )

= [k Vβ (T ) + k Vγ (T )] τeﬀ (T ) ,

(5.7.10)

where (α, β, γ) are a permutation of the axes (a,b,c) and k Vα (T ) is expressed in α terms of the HF constants and the correlation functions Kij (T ). For example, 17 for O(2,3) one has 17

Vα (T ) =

1 2 α C [1 + K01 (T )] , 22 α

(5.7.11)

α where we emphasize that the Kij were allowed to be anisotropic. For YBCO7 c ab it was found, for example, that the Kij were ∼ 20% larger than the Kij (see Fig. 5.2(a)).

Behavior of ab Plane Correlations In this same notation we also have (5.1.4) 63

Vα (T ) =

1 α α α [A2 + 4 B 2 + 8 Aα BK01 (T ) + 8 B 2 K12 (T ) + 4 B 2 K13 (T )] . 42 α (5.7.12)

Thus, 17

T1c = 63 T 1c

2 2 2 63 Vab (T ) =⇒ Aab + 4 B K →0 ij 2 17 V (T ) + 17 V (T ) Ca2 + Cb a b

(5.7.13)

is purely a function of in-plane correlations, approaching the value on the right as they vanish.

208

5 Relaxation Models for Cuprate NMR

Several sets of low-ﬁeld data for 17 T1c /63 T1c are plotted in Fig. 5.21(a) as a function of T /Tc for 0 ≤ T /Tc ≤ 4.5 for YBCO7 [17, 48, 49, 50] (see ﬁgure caption for details) and for Y248 [51]. Since the only temperature dependence for this ratio comes from the Kij (T )’s, what the ﬁgure shows is that correlations are small at the highest temperature, grow as T is reduced until they ab (Tc ) ∼ -0.4, and then decline again toward zero at low reach a peak value K01 temperatures. The dashed line in this plot shows the value of 17 T1c /63 T1c for ab Kij = 0 (5.7.13), evaluated with numbers from the UM ﬁt to YBCO7 data (Table 5.1). This line is seen to be in very good agreement with the high and low-temperature limiting values of the experimental T1 ratio. The shaded triangles in Fig. 5.21(a) show the same plot for Y248, taken from the results of Bankay et al., [51]. There we see that the correlation eﬀects are more than twice as great as in YBCO7 and do not seem to be very much aﬀected by the spin pseudogap, which has quite a powerful eﬀect on τeﬀ for ab this compound. It follows that the Kij (T )’s are not much aﬀected. Behavior of c-axis Correlations ab The foregoing results show that the ab-plane correlations Kij (T ) are strongly peaked at Tc in these systems and vanish at low temperatures T Tc . However, if one looks at the ratio T1c /T1ab for 63 Cu(2), the value of T1ab is strongly dominated by c-axis ﬂuctuations, for which 63 Vα (T ) is markedly dependent c on Kij (T ). What Uldry et al., found is that 63 Vα (T ) behaves as though the c Kij (T ) do not change appreciably below Tc [47]. Data for T1c /T1ab vs. T /Tc are plotted in Fig. 5.21(b), showing the variation of this ratio for both YBCO7 and Y248 [51]. Both sets of data were measured in low magnetic ﬁelds. In the normal state T1c /T1ab is fairly ﬂat for both of these compounds, with a value ∼ 3.7 for YBCO7 and ∼ 3.3 for Y248. Below Tc the data decline slightly, then rise to new maximum values, Y248 slightly higher than YBCO7. To discuss these data we use 63 Vc (T ) 1 T1c = 1 + 63 . (5.7.14) T1ab 2 Vab (T )

Data for T2G , to be deﬁned and discussed in Chap. 6, suggest that c-axis correlations do not change much below Tc [47]. If that were true, then the T1 ratio in (5.7.14) will have the value 12 [1 + 63 Vc (Tc )/63 Vab (Tc )] at Tc and the value 12 [1 + 63 Vc (0)/63 Vab (Tc )] at T = 0. For YBCO7, these values are obtained from the ﬁts and parameter plots from the original UM paper [11] (see Table 5.1 and Fig. 5.3). The resulting ratio values are plotted in Fig. 5.21(b) (open circles), where they are seen to be in good agreement with the YBCO7 data. To evaluate T1c /T1ab for Y248 one needs a special procedure, because the magnitude of the correlations at Tc is not known from experimental data. The asymptotic, high-temperature value of T1c /T1ab 3.3 for 63 Cu(2) was obtained from the measurements of Bankay et al., [52]. However, it seems

5.7 Relaxation of Planar

63

Cu and

17

O at T < Tc

209

70

R63c /17c = 63T1c–1/ 17T1c–1

60

(a)

50 40 30 20 10 0

0

2 T/ Tc

1

4

3

R63ab/63ac = 63T1ab–1/ 63T1c–1

7

(b)

6 5 4 3 2 1 0

0

0.2

0.4

0.6

0.8

1

1.2

T/ Tc

Fig. 5.21. (a) The ratio of 17 O(2,3) to 63 Cu(2) T1c values is plotted vs. T /Tc for YBCO (squares and circles) and for Y248 (shaded triangles). For YBCO7 the open circles are high-ﬁeld data from Yoshinari et al., [48], and ﬁlled circles are lowﬁeld data from Martindale et al., [49]. The ﬁlled squares denote data points where 63 Cu(2) data from Barrett et al., [50] are combined with 17 O(2,3) data from Nandor et al., [17]. The Y248 data are high-ﬁeld 17 O(2,3) data combined with NQR data for 63 Cu(2), both from Bankay et al., [52]. The dashed line is the model prediction ab = 0). (b) The ratio T1c /T1ab for for vanishing transverse AFM correlations (K01 63 Cu(2) is plotted vs. T /Tc for YBCO7 (ﬁlled circles) and for Y248 (ﬁlled triangles). The YBCO7 data are low-ﬁeld data from Takigawa et al., [44] and the Y248 data are low-ﬁeld data from Bankay et al., [52]. The dotted and dashed lines are normal state ratios from the same sources for YBCO7 and Y248, respectively. The open symbols are corresponding predictions from UM model calculations at Tc and at 0 K, which are obtained as described in the text. Reprinted ﬁgures from A. Uldry, M. Mali, J. Roos, and P. F. Meier, J. Phys. Condens. Matter 17, L499 (2005). Copyright 2005 I.O.P

210

5 Relaxation Models for Cuprate NMR

α unlikely that this corresponds to Kij ∼ 0. From ﬁt results for YBCO7 [11], if α α Kij = 0, one has T1c /T1ab 2.75. For Y248, then, the values of K01 were estimated from the ﬁt values for YBCO6.63, arguing that these two compounds ab (Tc ) -0.53 and have similar carrier densities and pseudogaps. Taking K01 c K01 (Tc ) -0.61 from data ﬁts for YBCO6.63 [11], they obtained T1c T1c 3.00; 5.78 . (5.7.15) T1ab T =Tc T1ab T =0

These approximate values are plotted in Fig. 5.21(b) as open triangles, and are seen to correspond well with the data [47]. The point here is, of course, that these results give good evidence that the c-axis correlations do not decay at low temperatures. If the c-axis correlations decay to zero as T → 0, then according to (5.7.14) T1c /T1ab → 2.75 in Fig. 5.21(b) for both compounds. This value is below the dashed and dotted lines and is not in good accord with the data. Comparing this discussion with the analysis given by Bulut and Scalapino in Sect. 5.7.1, their Hubbard model gives a functional form for χ (q, ω) at low frequencies at T < Tc which they have used in eﬀect to evaluate the α (T ) (see (3.5.17) and (3.5.18)), and thus the behavior of T1c /T1ab vs. T , Kij etc. The major diﬀerence with the present analysis by Uldry et al., [47] is that χ (q, ω) for the Hubbard model is isotropic and would not predict the anisotropic correlation eﬀects seen here. Further, the Hubbard model with d-wave symmetry does not inhibit AFM correlations in the superconducting state. As we have seen from the analysis of this subsection, only the c-axis correlations survive below Tc , with in-plane correlations declining to zero as T → 0. Thus, with the simple analytic method pioneered by Uldry and Meier, important eﬀects have been uncovered which might never have seen the light of day through the usual process of theoretical modeling.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12.

F. Mila, T.M. Rice, Physica C157, 561 (1989) 159, 161, 173 B.S. Shastry, Phys. Rev. Lett. 63, 1288 (1989) 159 H. Monien, D. Pines, Phys. Rev. B 41, 6297 (1990) 159, 199, 202 A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 159, 172, 173, 192 A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 159, 172, 173, 174, 175, 178, 179, 192, 1 M. Horvati´c, C. Berthier, Y. Berthier, et al., Phys. Rev. B48, 13848 (1993) 159 T. Auler, M. Horvatic, et al., Physica C 313, 255 (1999) 160, 166, 179, 180, 181, 182, 183, 18 N. Bulut, D.W. Hone, et al., Phys. Rev. B41, 1797 (1990); Phys. Rev. Lett. 64, 2723 (1990) 160, 187, 188, 189, 192, 194, 201 J.P. Lu, Q. Si, J.H. Kim, K. Levin, Phys. Rev. Lett. 65, 2466 (1990) 160, 192, 195 C.M. Varma, Phys. Rev. Lett. 77, 3431 (1996) 160, 196, 197 A. Uldry and P.F. Meier, Phys. Rev. B72, 094508 (2005) 160, 166, 208, 210 P.C. Hammel, M. Takigawa, et al., Phys. Rev. Lett. 63. 1992 (1989) 161, 162, 189, 191, 199

References 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52.

211

R.E. Walstedt, W.W. Warren, Jr., et al., Phys. Rev. B40, 2572 (1989) 161, 162, 198 J.A. Martindale, P.C. Hammel, et al., Phys. Rev. B57, 11769 (1998) 161, 162 M. Takigawa, W.L. Hults, J.L. Smith, Phys. Rev. Lett. 71, 2650 (1993) 161, 162, 166, 178, S.E. Barrett, D.J. Durand, et al., Phys. Rev. B41, 6283 (1990) 162, 205, 206 V. Nandor, et al., Phys. Rev. B60, 6907 (1999) 162, 164, 166, 208, 209 V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 164 D. Pines, C.P. Slichter, Phys. Rev. 100, 1014 (1955) 166 F. Raﬀa, T. Ohno, et al., Phys. Rev. Lett. 81, 5192 (1998) 169, 172 N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 169, 172 I. Tomeno, T. Machi, et al., Phys. Rev. B49, 15327 (1994) 169, 172 J.M. Tranquada, et al., Phys. Rev. B46, 5561 (1992) 175, 179, 193 L.P. Regnault, et al., Physica C 235-240, 59 (1994); Physica B 213-214, 48 (1995) 179 J. Rossat-Mignod, et al., Physica B 192, 109 (1993) 179 B.J. Sternleib, et al., Phys. Rev. B47, 5320 (1993); Phys. Rev. B50, 12915 (1994) 179 M. Horvati´c, C. Berthier, Y. Berthier, et al., Phys. Rev. B48, 13848 (1993) 179 M. Takigawa, P.C. Hammel, et al., Physica (Amsterdam) 162-164C, 853 (1989) 191 Q. Si, J.H. Kim, J.P. Lu, K. Levin, Phys. Rev. B42, 1033 (1990) 192, 195 Q. Si, K. Levin, Phys. Rev. B44, 4727 (1991) 192 Q. Si, Y. Zha, K. Levin, J.P. Lu, Phys. Rev. B47, 9055 (1993) 192, 193, 194 Q. Si, J.P. Lu, K. Levin, Phys. Rev. B45, 4930 (1992) 192, 193, 194 C.M. Varma, Phys. Rev. B73, 155113 (2006) 194 C.M. Varma, P. Littlewood, et al., Phys. Rev. Lett. 63, 1996 (1989) 195 R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 198 B. Fauqu´e, et al., Phys. Rev. Lett. 97, 197001 (2006) 199 J.A. Martindale, et al., Phys. Rev. Lett. 68, 702 (1992) 199, 200, 203, 204 A.Z. Genack, A.G. Redﬁeld, Phys. Rev. Lett. 31, 1204 (1973) 199 G.B. Furman, S.D. Goren, Phys. Rev. B68, 064402 (2003) 199 N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 68, 706 (1992) 201, 203, 205 N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 201, 202, 205 J. Kirtley, C.C. Tsuei, et al., Nature (London) 373, 225 (1995) 202 D.H. Wollman, D.J. van Harlingen, et al., Phys. Rev. Lett. 74, 797 (1995) 202 M. Takigawa, J.L. Smith, W.L. Hults, Phys. Rev. B44, 7764 (1991) 202, 203, 204, 205, 206, M. Takigawa, P.C. Hammel, R.H. Heﬀner, Z. Fisk, Phys. Rev. B39, 7371 (1989) 205, 206 M. Takigawa, P.C. Hammel, et al., Physica (Amsterdam) 162-164C, 853 (1989) 205, 206 A. Uldry, M. Mali, J. Roos, P.F. Meier, J. Phys. Condens. Matter 17, L499 (2005) 207, 208, 210 K. Yoshimura, T. Imai, et al., J. Phys. Soc. Japan 58, 3057 (1989) 208, 209 J.A. Martindale, S.E. Barrett, et al., Phys. Rev. B47, R9155 (1993) 208, 209 S.E. Barrett, J.A. Martindale, et al., Phys. Rev. Lett. 66, 108 (1991) 208, 209 M. Bankay, M. Mali, J. Roos, D. Brinkmann, Phys. Rev. B50, 6416 (1994) 208 M. Bankay, M. Mali, et al., Phys. Rev. B46, R11228 (1992) 208, 209

This page intentionally blank

6 Dynamic Susceptibility Studies for the Cuprates

In Chap. 3 and 5 we saw how the dynamic susceptibility has come to play a pivotal role in interpreting cuprate spin-lattice relaxation data and rationalizing the sharp contrasts in T1 behavior among sites in and near the CuO2 planes. The principal driving force in all of the magnetic phenomenology of the cuprates is clearly the AFM ﬂuctuation peak at or near Q = (π, π), which occurs in varying degrees of dominance depending in an inverse fashion on the degree of carrier doping. This scenario appears to be a unique property of doped Mott insulators. A second consequence of strong AFM ﬂuctuation eﬀects is the indirect spin-spin coupling between neighboring nuclear spins which is thereby induced. This eﬀect was recognized early on by Pennington et al., [1], shortly after which the Pennington-Slichter (PS) theory of indirect spin-spin coupling appeared, formulating this eﬀect in terms of the static, q-dependent susceptibility χ (q, 0). Equally important was the recognition that these couplings were responsible for a Gaussian spin-echo decay (T2g ) process which, with due care, could be measured experimentally [2]. In the ﬁrst section of this chapter we review the PS formulation and survey a range of experimental cuprate results and interpretations. The importance of indirect spin-spin couplings for cuprate magnetism research is that T2g (T ) oﬀers a second method of characterizing χ(q, ω). T2g has been shown (and we document in Sect. 6.1) to be a fairly direct measure of the key parameter χ (Q). It soon became de rigueur to measure T2g as well as the NMR shift and T1 in a cuprate NMR study. In this chapter we illustrate why this is the case. The connection between χ (q, ω) and χ (q, 0) is the rather tenuous one through the Kramers-Kronig (KK) relation. It is, of course, not tenuous in principle, but diﬃcult to implement experimentally, because it requires the entire frequency spectrum of χ (q, ω). In theoretical modeling, T2g through the KK relation becomes a constraint on model parameters. For example, Bulut and Scalapino have extended their calculations of dynamical properties using a small-U Hubbard model to the case of indirect spin-spin coupling (T2g )

R.E. Walstedt: Dynamic Susceptibility Studies for the Cuprates, STMP 228, 213–251 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 6

214

6 Dynamic Susceptibility Studies for the Cuprates

in the superconducting state. When compared with the data of Ohsugi et al., [3], the result was a dramatic conﬁrmation of d-wave gap structure below Tc for Y248. We review these developments at the end of Sect. 6.1. For a purely experimental implementation of the KK relation we turn to the case of optimally doped LSCO:x, x ∼ 0.15. For this system there has been an INS characterization of χ (q, ω) for eﬀectively all q values (in the ﬁrst BZ) and for all frequencies for which there is a substantial contribution. Moreover, the latter characterization is in absolute units, leading to a direct comparison between INS and T1 data with no adjustable parameters. The story of this ﬁrst-ever quantitative juxtaposition of quantitative INS and NMR data is recounted in detail in Sect. 6.2. A closely-related T2 study for both 63,65 Cu and 17 O is included as well, where a successful implementation of the KK integral has been reported. The points where INS and NMR data are clearly incompatible is also an interesting part of the story. An interesting interconnection between T1 , T2g , and the dynamic susceptibility components has been created by the dynamic scaling theories of Pines and co-workers. This topic is addressed in Sect. 6.4, where in the limit of long AFM correlation lengths ξ the two parameters ξ(T ) and the spin ﬂuctuation frequency ωsf (T ) appear to control the dynamical properties accessible to the NMR probe. In this context a high-temperature investigation of 63 Cu(2) static and dynamic NMR/NQR properties of YBa2 Cu4 O8 (Y248) by Curro et al., [4] has given evidence for a sharply-deﬁned crossover temperature (∼ 500 K) for the dynamical exponent (z = 1→2) in this system. These interesting developments are reviewed in detail, as well as suggestions for extension to other systems.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter Indirect couplings between nuclear spins are very strong in the cuprates [1]. As was ﬁrst demonstrated by Pennington and Slichter [2], these can be formulated in terms of the real part of the dynamic susceptibility χ (q, 0). χ (q, 0) can, in turn, be expressed in terms of χ (q, ω), so the estimation of χ (q, ω) (ω = 0) through measurements of the spin-echo T2 make the indirect couplings a powerful element in the NMR methodology for solids. In this section we give the derivation of the Pennington-Slichter result, which is straightforward, after which various applications of this result will be presented throughout the chapter. There are indirect couplings between any pair of neighboring nuclei in (or near) the CuO2 plane. We shall begin with the pertinent example of interactions among the 63,65 Cu nuclear spins. Although T1 can be formulated in terms of χ (q, ω) having the dimension of inverse energy (see discussion in Sect. 3.5), here we will use susceptibilities per mole, since χ (q, ω) becomes the measurable uniform, static susceptibility at ω = 0. We calculate the indirect coupling

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

215

of a 63 Cu with surrounding 63,65 Cu spins, an eﬀect which is mediated via the bath of ﬂuctuating electronic spins S i . It is driven by the HF coupling tensor HHF =

⎡ ⎣Aα Iiα Siα + B

α,i

⎤ Iiα Sjα ⎦ ,

(6.1.1)

j(nn)

where j(nn) is taken over the four nearest-neighbor spins to the site i. Through this HF Hamiltonian a spin polarization is created in the local environment by a nuclear spin I i located at Ri . The HF energy (6.1.1) can be written as an eﬀective ﬁeld Hiα (R) which this nucleus exerts on spin moments −gα μB Sα (R) in the vicinity. The ﬁeld is given by Hiα (R) =

Iiα Fαα (R, Ri ), with Fαα (R, Ri ) = [Aα δR,Ri + B δR,Rj ] . gα μB j(nn)

(6.1.2) The eﬀect of Hiα (R) on the surrounding medium can be calculated in terms of χ (q, 0), which we denote χα (q). The ω = 0 component is used, because in a metallic environment nuclear spin motion is very slow on the time scale of electronic spin ﬂuctuations. However, the ﬁeld driving χα (q) is the q–component of Hiα (R). One may write the Fourier transform Hiα (q) = k exp(−iq · Rk )Hiα (Rk ) in the form Iiα −iq·Ri e Fαα (q), with Fαα (q) = [Aα + 2B (cos qx + cos qy )]. gα μB (6.1.3) Hiα (q) then induces a q-component of spin moment Hiα (q) =

Sα (q) = −

1 Hiα (q)χα (q) , NA gα μB

(6.1.4)

where we divide χ (q) by Avogadro’s number for an atomic susceptibility. The inverse Fourier transform of Sα (q) gives the resulting spin polarization in the vicinity of Ri , i.e. Sα (R) =

q

eiq·R Sα (q) = −

Iiα iq·(R−Ri ) e χα (q)Fαα (q) , (6.1.5) NA gα2 μ2B q

where q is a normalized sum over the Brillouin zone. The interaction energy with a second nucleus I j may now be obtained by inserting (6.1.5) into (6.1.1), where we use the notation of (6.1.2) to ﬁnd aα (i, j)Iiα Ijα = Ijα Sα (Rk )Fαα (Rk , Rj ) . (6.1.6) α

α

Rk

216

6 Dynamic Susceptibility Studies for the Cuprates

Substituting from (6.1.5) then gives the general result [5] 1 eiq·(Rj −Ri ) χα (q)Fαα (q)2 . NA gα2 μ2B q

aα (i, j) =

(6.1.7)

Under suitable conditions the spin-spin interactions in (6.1.6) and (6.1.7) can be measured via the spin-echo decay time (T2 ) process, to be discussed in Sect. 6.1.3. The parameter controlling this process is the second moment contribution of the interaction (6.1.7). A useful relation for calculating the second moment of the line as well as the Gaussian decay time T2g of the spin echo may be derived using (6.1.7). This result, given independently by Takigawa [6] and by Thelen and Pines [7], is ⎡ 2 ⎤ 1 ⎣ [χα (q)Fαα (q)2 ]2 − aα (i, j)2 = χα (q)Fαα (q)2 ⎦ . 2 μ2 )2 (N g A α B q q j (6.1.8) 6.1.1 Some General Properties of the Indirect Spin-Spin Coupling We adopt a notation where q is dimensionless and Ri = (nxi , nyi ) in units of a, where nxi,yi are integers. We shift the origin of the q sum to Q, i.e. q = p + π π (π, π). Then χα (p) is a symmetric function, where p → (1/2π)2 dpx dpy , π

π

and Fαα (p) = [Aα − 2B(cos px + cos py )]. The exponential factor in (6.1.7) reduces to cos (nx px ) cos (ny py ), since the sine terms cancel by symmetry, where nx = nxj - nxi , etc. Thus, (6.1.7) becomes aα (i, j) =

(−1)(nx +ny ) NA gα2 μ2B

where Gα (nx , ny ) =

1 π2

n x +2

Cα (nx , ny )Gα (nx , ny ) ,

(6.1.9)

nx =nx −2 ny =ny −2

π

dpx 0

ny +2

π

dpy χα (p) cos(nx px ) cos(ny py ),

(6.1.10)

0

and where the Cα (nx , ny ) are functions of Aα and B. Some general properties of aα (i, j) are as follows: • • •

Terms in χ (q, 0) which are independent of q give no contribution to aα (i, j). The essential range function of a(i,j) is the Fourier transform of the peak function χα (q). A sign reversal on moving between nn sites results from the the AFM nature of the ﬂuctuations.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

• •

217

The range function depends only on the magnitudes of the nx,y and is invariant on exchange of nx and ny . Therefore aα (i, j) is symmetric about the x and y axes, and also about the x = ±y axes.

6.1.2 The Gaussian model of Indirect Spin-Spin Coupling in YBCO In the MM follow-up to MMP [8], a Gaussian model was suggested for χ (q, ω). Citing this example, Imai et al., [9] made use of this model in their interpretation of data for T1 and T2g (see below for deﬁnition of T2g ). More recently, Auler et al., [10] employed this model for similar purposes, citing INS studies which showed a Gaussian-like shape with a width essentially independent of temperature. Their interpretation of T1 data on this basis was presented and discussed in Sect. 5.3. INS data provide an important characterization of χ (q, ω), which is then used to interpret NMR data. An important question regarding INS data is to what extent they are dependent on the frequency scale. Does a peak in χ (q, ω) at or near Q with a certain measured width at ω = 10 meV have the same shape and width at an NMR frequency four orders of magnitude lower? With the limitations of current spectroscopic techniques one cannot answer this question experimentally. Many discussions of NMR T1 interpretation tacitly assume that the INS results will still be valid at NMR frequencies. We address this question in various contexts throughout this chapter. For the purposes of the present discussion we adopt the Gaussian shape and width for the AFM peak given by Auler et al.,: χα (q) =

gα2 −(qx2 +qy2 )ξ2 /4 χ e , 4 AF

(6.1.11)

with ξ 1.3, where we place the origin at Q = (π, π) and we denote χ (Q) = χAF . Inserting this into (6.1.10), a simpliﬁcation occurs, where we can write Gα (nx , ny ) = (gα2 /4)χAF g(nx )g(ny ), with g(n) =

1 π

0

π

2 2

dpe−p

ξ /4

2 2 1 cos(np) ≈ √ e−n /ξ . πξ

(6.1.12)

In (6.1.12) the result on the far right is obtained by extending the upper integration limit to ∞. Since exp(−π 2 ξ 2 /4) 0.015, we suggest that this is a reasonable approximation. Inserting this expression for Gα (nx , ny ) into (6.1.9), we ﬁnd, with nx = nxj - nxi , etc.,

218

6 Dynamic Susceptibility Studies for the Cuprates

aα (i, j) = (−1)(nx +ny )

2 2 2 χAF e−(nx +ny )/ξ {A2α + 4B 2 πNA ξ 2 gα2 μ2B 2

− 4Aα B e−1/ξ [cosh(2nx /ξ 2 ) + cosh(2ny /ξ 2 )] 2

+ 8B 2 e−2/ξ cosh(2nx /ξ 2 ) cosh(2ny /ξ 2 ) 2

+ 2B 2 e−4/ξ [cosh(4nx /ξ 2 ) + cosh(4ny /ξ 2 )]} .

(6.1.13)

Equation (6.1.13) is used below to calculate indirect coupling energies for YBCO6.9 and to discuss results which have appeared in the literature. Before that, however, we make a brief digression to introduce spin echo decay measurements. 6.1.3 Measuring Indirect Spin-Spin Coupling via Spin-Echo Decay Under suitably restrictive assumptions, it is possible to get good estimates of the indirect spin-spin coupling (6.1.7) by measuring spin-echo decay times. We give here a brief review of some of the essential points of spin-echo decay, followed by a discussion of results from the literature in the next subsection. We consider spin-echo decay for the speciﬁc problem of 63,65 Cu(2) NMR in the CuO2 planes of a cuprate superconductor. If the 63,65 Cu isotopes are labelled A and B, where the A spins are under observation, then the nuclear spin-spin coupling has the general form AA AB BB + HII + HII . HII = HII

(6.1.14)

For cases of orthorhombic symmetry or higher, the latter terms can be written AA A A A A A A AB A A αij Izi HII = Izj + βij Ixi Ixj + γij Iyi Iyj , and HII = αij Izi Izj , i>j

i>j

(6.1.15) AB the x and y terms where we have taken z to be the quantization axis. For HII have been omitted, because they are non-secular and have no measurable AA are secular, i.e. physically eﬀects. Whether or not the x and y terms for HII viable, is a matter of some discussion. In cases where there is no detuning of neighboring A spins, i.e., where locally, the Zeeman splitting γA (1 + K)H as well as quadrupolar splittings are homogeneous, then the x and y terms are technically viable. However, if the zz coeﬃcient αij is much larger than βij and γij (a realistic case as we shall see below), then “ﬂip-ﬂop” processes such as | mA , mB → | mA + 1, mB − 1 may become severely inhibited and the transverse terms become de facto nonsecular. Below, a simple test is suggested to determine the eﬀectiveness of the dynamical terms. For the moment we shall assume the ﬂip-ﬂop terms to be inoperative. This is a simple limiting case for which the spin-echo decay process has been calculated in Appendix A.1. Approximating the decay function with a Gaussian 2 ), then the echo decay time constant is found to be exp(−(2τ )2 /2T2g

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

⎤1/2 ⎡ c 1 63 = sin(θ2 /2) ⎣ α2 ⎦ , T2g 8 j ij

219

(6.1.16)

where c63 0.69, and the sum is over all neighbors. The dependence on refocussing pulse angle θ2 suggests an interesting test for the spin dynamics of the sample. If the spins are completely static on the time scale of the echo sequence, then T2g should become correspondingly long when θ2 is small. If T2g does not change a great deal over a range of values for θ2 , it probably means that there is an appreciable degree of ﬂip-ﬂop motion taking place among the spins. 2 In applying (6.1.16) to actual measurements of j αij , it is clearly necessary to be able to ﬂip over nearly all of the spins with the θ2 pulse. This is an important constraint on experimental technique. For cuprates this means that one will probably have to employ only the (−1/2 ↔ 1/2) transition, and possibly work at low ﬁelds in addition in order to narrow the line. 6.1.4 Behavior and Interpretation of Indirect Couplings in YBCO and Y248 There have been a number of measurements of T2g for both YBCO and Y248 in the literature, with much discussion of its behavior as compared with T1 . Since they are both driven, at least in part, by AFM ﬂuctuations, these relaxation times are reﬂections of the same underlying quasiparticle physics. Thus, the advent of T2 g as an additional characterization of cuprate hole dynamics was a most welcome development. Results Given by Pennington and Slichter In their original paper formulating the indirect couplings, expounded in the previous subsection, PS [2] presented calculations of coupling coeﬃcients aα (i, j) as well as of T2g for fully oxygenated YBCO7. They calculated their range function using the MMP Lorentzian form (ξ/ξ0 )2 ) χ (q) = χ0 1 + (6.1.17) 1 + (q − Q)2 ξ 2 centered on Q. The ξ 2 factor gives only a rough normalization for χ (q), since q χ (q) depends on ln(ξ). The resulting relaxation time is found to vary 1/T2g ∝ ξ [2]. The parameters and assumptions for various calculations of T2g discussed here are shown in Table 6.1. Adopting the MMP estimate [11] ξ = 2.5 a, the half-width of the AFM peak in the PS calculations with (6.1.17) is 0.4. Also from (6.1.17), χ (Q) = 1.66 × 10−3 emu/mol Cu(2). With values of Ac and B as shown in Table 5.1, PS ﬁnd a value of 1/T2g which is just slightly smaller than their experimental number, which clearly validates their formulation of the indirect spin-spin coupling.

220

6 Dynamic Susceptibility Studies for the Cuprates

Table 6.1. Models, data, and results for c-axis indirect coupling values of 1/T2g are presented from various sources for diﬀerent doping levels in YBCO. The ﬁrst line gives the original results of Pennington and Slichter with a Lorentzian model. HF parameters vary only slightly between calculated results given. Experimental data in the ﬁnal column corresponds generally to 100 K. Under “Source”, Imai and Auler are ﬁrst authors, as are Bulut and Itoh. The Takigawa reference is [6]. For Imai et al., and Auler et al.,, the estimated values of 1/T2g have been made using (6.1.13) and direct summation to give j ac (i, j)2 . For the Takigawa estimate, which was made with a Lorentzian model, the PS result is simply scaled to the larger value of χ (Q) shown. The units of parameters given are as follows: Ac and B (10−6 eV ); χ (Q) (10−3 emu/mol); 1/T2g (ms−1 ). These results are discussed extensively in the text System

Source

χ (q) Form

H.W.(a−1 ) Ac

B

χ (Q) (1/T2g )est (1/T2g )exp

YBCO7 YBCO7 YBCO7 YBCO6.9 YBCO6.9 YBCO6.63

PS[2] Bulut/Itoh Itoh(c63 = 1) Imai[9] Auler[10] Takigawa

Lorentzian Hubbard RPA Hubbard RPA Gaussian Gaussian Lorentzian

0.40 0.5 0.5 0.37 1.28 0.40

0.38 0.38 0.38 0.45 0.39 0.38

1.66 1.23 1.23 3.28 1.41 6.14

-1.53 -1.53 -1.53 -1.77 -1.56 -1.53

5.26 9.0 10.8 9.2 7.5 19.5

7.7 11.1 12.9 9.6 11.5 18.4

Eﬀects of Transverse Coupling and of Dipolar Fields Before proceeding with discussion of experimental data, we note in passing that transverse and dipolar coupling contributions to Hzz are much smaller and can be ignored for most purposes. The dipolar coupling coeﬃcient for 2 3 quantization axis ⊥ CuO2 plane is simply αdip c (i, j) = γ /Rij , which has −1 63 the value 908 s for nn Cu(2). The corresponding second moment value is less than 6% of the estimated indirect coupling value calculated above. Moreover, it has a constant positive sign for all in-plane neighbors, so that its eﬀects tend to cancel when combined with the staggered indirect coupling. We shall ignore the dipolar terms from this point forward. The transverse indirect coupling terms are also much smaller than the c-axis contribution, giving a second moment only 15% of the latter eﬀect using Aab ∼ 0.31 in the units of Table 6.1, with B having the same value as for the c-axis terms. As far as we are aware, no eﬀort has been made to measure the transverse terms, and we shall not discuss them further. Comparison of the PS Results with Other Models and Data Throughout the derivation of indirect spin-spin coupling given above [2], it is assumed that the resulting spin-echo decay process will be Gaussian in form or nearly so. Itoh et al. have tested this hypothesis for the case of NQR studies of 63 Cu(2) in Y248 [12]. Their results are plotted in Fig. 6.1(a) and (b) for several temperatures. After corrections for T1 eﬀects (see Appendix A.3), it is seen that these decay curves exhibit nearly perfect Gaussian character over two orders of magnitude. Some discussion of the origin of such Gaussian behavior, which is very widespread in T2g studies, is presented in Sect. 6.3.

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter 1.0

221

(b)

(a)

E(2τ)/E(0)

280K 0.1 4.2K 0.01 100K 0.001 0

242 (2τ)2/102μsec2

484 0

98

196

(2τ)2/102μsec2

Fig. 6.1. (a) and (b) Spin echo decay curves, corrected for T1 eﬀects, are plotted semilogarithmically vs. (2τ )2 , showing nearly perfect Gaussian behavior over two orders of magnitude of decay at several temperatures. These are data for 63 Cu(2) in YBa2 Cu4 08 . Reprinted ﬁgures from Y. Itoh, H. Yasuoka, et al.,, J. Phys. Soc. Japan 61, 1287 (1992). Copyright 1992 Physical Society of Japan

In the second line of Table 6.1 we list the calculated result of Bulut and Scalapino (BS) based on their small-U Hubbard model calculations [13] along with experimental numbers from Itoh, Yasuoka et al., [12]. BS calculated the indirect coupling using the same model and parameters they had applied to the T1 problem [14, 15], ﬁnding good agreement with experimental data with an AFM peak width ∼ 25% greater than that used by PS. Itoh et al., also tested the proportionality of 63 Cu(2) second moment to the concentration of 63 Cu by measuring a sample which contained 100% 63 Cu. The result, shown on the third line of Table 6.1, is within experimental error of the expected increase 1/T2g ∝ (c63 )1/2 . The BS calculated result scaled in this fashion is shown for comparison. Itoh et al. [12] also measured the behavior of T2g in the superconducting state of Y248. The latter results and the BS model calculations for this case are discussed in the next subsection. We make further comparisons with the results in Table 6.1 with calculations using (6.1.13) based on the parameters provided by Auler et al., [10]. Results obtained with a Gaussian peak for χ (q) and other parameters from Auler et al., [10] are listed in line ﬁve of the table. The INS-derived peak width is more than three times that used by PS. The value of (1/T2g )est is substantially larger than the PS value with a slightly smaller value for χ (Q). Although this is a satisfactory result, it is puzzling that it does not give the rather larger relaxation rate which they quote, and from which the value given for χ (Q) was supposedly derived [10]. The origin of this discrepancy is not understood. In line four of Table 6.1 are listed the results of a similar calculation based on (6.1.13) as well as the HF coupling, χ (Q), and peak width parameters given by Imai et al., [9], on which the calculation is based. The estimated value of 1/T2g is in good agreement with the experimental value given. A result

222

6 Dynamic Susceptibility Studies for the Cuprates

reported by Takigawa [6] is given in the bottom line of the table. Parameter values were stated in [6] for the Lorentzian model with a range of peak widths. Choosing the peak width used by PS for the same model with the same HF parameter values, we simply scale the PS result to the larger value of χ (Q) given in [6] to yield the value of (1/T2g )est stated in the table, which is in good agreement with the experimental value given for YBCO6.63. The greatly enhanced AFM ﬂuctuations in YBCO6.63 are clearly reﬂected in a shorter decay time T2g . Before continuing to discuss the signiﬁcance of these results, we address the question of how the results for 1/T2g scale with the correlation length. Scaling of T2g with χ (q) Parameters There appears to be an interesting diﬀerence between Lorentzian and Gaussian models of χ (q) which has to do with their dependence on the correlation length parameter ξ. For the Gaussian model as prescribed by Auler et al., [10], we ﬁnd that the second moment ∝ j α(i, j)2 varies roughly as ξ −1 . From (6.1.16) it follows that T2g ∼ ξ 1/2 . In contrast, PS note that T2g ∝ ξ −1 for their Lorentzian model. However, the latter model (see (6.1.17)) included a prefactor ∝ ξ 2 multiplying a peak function of unit amplitude, whereas the Gaussian has none. The ξ 2 prefactor by itself accounts for the stated variation of T2g with ξ. Without the prefactor eﬀect, then, the PS result is that T2g is essentially independent of ξ. We next consider whether it is possible to account for the foregoing behaviors using the expression (6.1.8) for the second moment. While under some circumstances it may be possible to deduce how j α2ij scales with ξ using (6.1.8), there is no simple answer to this question in general for two reasons. First, if Fαα (q) contains transferred HF couplings, the cosine factors do not scale in any way. Second, in the case of a Lorentzian form for χ (q), simple the sum q χ (q) does not converge at the boundaries, so that the integration limits become ξ–dependent. This problem is particularly severe for small values of ξ. Nonetheless we shall consider what sort of results (6.1.8) gives for q-independent HF couplings. Such a calculation is presented in Appendix A.2 for the case of a Gaussian susceptibility, with the result 1 2 2 αij = 1− 2 . (6.1.18) 2πξ 2 πξ j Thus, as ξ declines, the leading term gives T2g ∝ ξ. However, at small values of ξ the correction term in the brackets becomes increasingly important. For ξ ∼ 1.3, the correction term increases T2g by ∼ 25%. We suggest that the q-dependent HF couplings also contribute to the behavior mentioned above for YBCO, where T2g ∝ ξ 1/2 . For the Lorentzian case, with χ (q) = χ (Q)/(1+q 2 ξ 2 ), the leading term in (6.1.8) gives T2g ∝ ξ as with the Gaussian case. However, the second term gives

6.1 The Indirect Spin-Spin Coupling Theory of Pennington and Slichter

223

a somewhat larger correction than in (6.1.18), so that j α2ij levels oﬀ and may even diminish at low values of ξ. It is plausible that over a modest range of ξ values j α2ij may be rather ﬂat, leading to the ξ-independent behavior noted, in eﬀect, by PS. Therefore, it appears that the contrast between Gaussian and Lorentzian susceptibilities may be accounted for in this simple fashion. A second and equally important conclusion which we draw from this discussion is that the results for T2g do not depend strongly on ξ or on the choice of Gaussian or Lorentzian for the shape of the AFM peak in χ (q). For this reason it will also be diﬃcult to extract information from T2g data on either of these points. At the same time, the results in Table 6.1 show that T2g can be analyzed to yield semi-quantitative results for χ (Q), even if the width and detailed character of the associated AFM peak are not well established. Comparing the Temperature Variation of T2g with that of T1 The relatively weak dependence of T2g on the width of the AFM peak in χ (q) leads to an interesting contrast between echo decay times and T1 processes. While 1/T1T is given by sums of χ (q, ω) over all of q-space, 1/T2g is very nearly proportional to χ (Q), i.e. to the staggered susceptibility. T1 is, of course, also sensitive to the staggered susceptibility, since it measures the area under the AFM peak in χ (q, ω) at Q. But T1 for 63 Cu(2) has major contributions from the rest of the Brillouin zone as well, much of which collapses in the presence of a pseudogap. We see the result of this in Fig. 6.2 from Takigawa [6]. The curve for 1/T2g indicates that the staggered susceptibility is rising fairly rapidly in a Curie-Weiss-like fashion. T1 for the 63 Cu(2) rises below 300 K at a similar rate. When the spin pseudogap sets in around 200 K, however, 1/T1T goes over a maximum and then begins a steep descent which indicates collapsing behavior for χ (q, ω) over much of the BZ. The fact that 1/T2g is immune to the pseudogap decline suggests that χ (Q) is made up from parts of the Fermi surface which are not gapped. A related result is presented in the next subsection, where 1/T2 for Y248 does not decay in the superconducting state, presumably because contributions to χ (Q) are not aﬀected by the superconducting gap either. Curie-Weiss behavior for 1/T2g is also found in YBCO7 [9, 10], though with rather smaller increases between 300 K and Tc . It would be, of course, most enlightening to be able to compare such results with INS data on the same systems, including temperature dependences. While the INS characterizations are not easy to perform, the cuprates provide an ideal test bed for comparison of results for the dynamic susceptibilities. We shall see this in more detail in Sect. 6.3 with the system LSCO. Takigawa also made an eﬀort to apply the scaling theory of Sokol and Pines [16] to the susceptibility behavior of YBCO6.63 [6]. The scaling eﬀect may be seen in Fig. 6.2, where just at the upper end of the temperature range the ratio T1 T /T2g approaches a constant value. Eﬀects such as this have become a major branch of the study of cuprate magnetism and will be reviewed at some length in Sect. 6.4.

224

6 Dynamic Susceptibility Studies for the Cuprates

6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc Bulut and Scalapino (BS) used their small-U Hubbard model of spin dynamics to treat both T1 (Sect. 5.7) and T2g in the superconducting state [13]. In the latter case they found a major distinction between the cases of s-wave and d-wave pairing. We ﬁrst describe their calculation, and then review the experimental T2g data of Itoh, Yasuoka et al., [12] on YBa2 Cu4 O8 (Y248) which has been compared with the BS theory. Model Calculations of Bulut and Scalapino: T2g in the Normal State The BS calculations of T2g used much the same parameter values as employed in related work on T1 (see Sect. 5.4) [14, 15], where they used the RPA formula χ (q) =

χ0 (q) 1 − U χ0 (q)

(6.2.1)

for the real part of the dynamic susceptibility χ (q) at ω = 0. They give for the noninteracting susceptibility χ0 (q → 0) = 0.214 t−1, where t is the hopping integral giving band energies Eq = −2t[cos qx + cos qy ] − μ. The chemical potential was set so that the band occupation n = 0.86, very near the critical value for instability (see [15] and Sect. 5.4). The enhanced curve of χ (q) from the BS model is shown in Fig. 6.3(a) for the path in q-space shown in the inset. We determine the molar value of χ (Q) 20 8

6

10

4 –1/T2G

5

1/T1 T(s–1K–1)

1/T2G (ms–1)

15

2

–1/T1T

0

0 0

100

200

300

T(K)

Fig. 6.2. Measured values of 1/T2g and 1/T1 T for 63 Cu(2) in YBCO6.63 are plotted vs. temperature. The data have been scaled to coincide near room temperature, where they show similar behavior. Reprinted ﬁgure from M. Takigawa, , Phys. Rev. B49, 4158 (1994). Copyright 1994 American Physical Society

6.2 The Bulut-Scalapino Calculation of 1/T2g for T < Tc

225

as follows. From discussion of NMR shift calculations in [15] the q = 0 Stoner enhancement is given as 1.75. Equating their c-axis susceptibility result to χc = 1.18 × 10−4 emu/mol Cu(2) from Table 2.4, we ﬁnd χ0 (0) = 6.74 × 10−5 emu/mol Cu(2). Relative to that value, the peak value in Fig. 6.3(a) is enhanced by a factor ∼ (3.8/0.214), giving the estimate χ (Q) 1.23 × 10−3 emu/mole Cu(2). The latter value is within ∼ 15% of the result obtained by taking t = 0.1 eV [15]. The AFM peak half-width of ∼ 0.5 (Table 6.1) is also taken from Fig. 6.3. The latter results apply in the vicinity of 100 K. BS also calculated the temperature variation of 1/T2g , both in the normal state up to 300 K and below Tc down to essentially zero temperature. Their results as given are shown as the dashed line in Fig. 6.3(b), where they are seen to fall just below the YBCO7 data from Itoh et al., [12] (ﬁlled circles). The open circles in the same ﬁgure are a plot of measured values of 1/T2g for 63 Cu(2) in Y248 also taken from [12]. The latter data have been compared with the BS calculations (solid lines) from [13], which have been scaled to coincide with the experimental data in the region around 100 K1 . The result is a dramatic comparison of T2g data with the s and d-wave BS model calculation [13]. The Superconducting State: A Dramatic Success for d-Wave The normal-state calculation gives a reasonable account of the Y248 data for 1/T2g in Fig. 6.3. In the superconducting state, these data, combined with the BS calculations, give a very dramatic conﬁrmation of d-wave pairing symmetry. The eﬀect of superconducting pairing on the susceptibility curve is shown in Fig. 6.3(a) where calculated susceptibility curves at T = 0.8Tc are shown for both s-wave (dashed line) and d-wave (dotted line). The contrast between these two is attributed by BS to nodes in the d-wave energy gap which simply allow contributions to χ (Q) to persist into the superconducting state. This is very likely related to the continued c-axis spin correlations below Tc which were demonstrated by Uldry et al., [17], as was discussed in Sect. 5.7. It may also be related to the fact that χ (Q) is immune to the pseudogap in the normal state, exhibiting Curie-Weiss behavior down to Tc . Thus, the pseudogap and the superconducting gap have similar character in this respect. 1

Since the Y248 data were obtained using NQR, the original (dotted) curve was √ ﬁrst rescaled by 2 to reﬂect the enhanced NQR relaxation rate (see Appendix A.2.1 for a discussion of this eﬀect). Following that, rescaling with the Stoner factor has been done using (6.2.1) as follows. It is presumed that the temperature dependence of χ (Q) is driven by that of χ0 (Q). From [13] it was determined that the enhancement at the peak of the curve in Fig. 6.3(a) is 5.4 at T = 100 K. Using that fact and (6.2.1) to recover χ0 (Q) as a function of T, the dotted curve with an adjusted value of U was plotted as the solid curve in Fig. 6.3(b). For the region below Tc , the original curves from [13] were simply rescaled to meet the normal-state curve at T = 82 K.

226

6 Dynamic Susceptibility Studies for the Cuprates 6

(a)

5

(π,π)

4

χ(q)

q 3 (π,0)

(0,0) 2 1 0 (0,0)

(π,0)

(π,π)

(0,0)

q

25

D

(b) Y248

1/T2G ms–1

20

15

10

S YBCO7

5

0

0

100

200

300

T(K)

Fig. 6.3. (a) The enhanced susceptibility χ (q) obtained with (6.2.1) [13] is plotted for the path in q-space shown in the inset. The solid curve shows behavior at T ∼ 100 K, while the dashed and dotted curves show behavior for s-wave and d-wave pairing, respectively, at T = 0.8 Tc . See text and part (b) of this ﬁgure for discussion of this eﬀect. (b) NMR measurements of 1/T2g for YBCO7 (dots) and NQR measurements for Y248 (open circles) by Itoh et al., [12] are plotted vs. temperature. The dotted line shows the normal-state calculations of Bulut and Scalapino [13] for 63 Cu(2) NMR in YBCO7. The solid curves are determined as follows. For the nor√ mal state the dotted line is scaled by 2 for the NQR case, then the enhancement is re-calculated using (6.2.1) to match the experimental curve near 100 K. For T < Tc the curves from [13] are simply scaled to meet the normal-state curve at Tc = 82 K. See text for additional discussion

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

227

The present results along with the dramatic T1 eﬀects discussed in Sect. 5.7 consitituted a very strong case for d-wave pairing several years before it was widely accepted by the high-Tc community. To summarize, we have seen in this section and the last that the formulation of indirect spin-spin coupling in terms of χ (q) by Pennington and Slichter opened up a very important new avenue of approach for the characterization of the AFM enhancement peaks as well as of χ (Q).

6.3 Coordinated Interpretation of NMR and INS Data for LSCO In Sect. 4.4 we discussed data for the NMR shift, uniform susceptibility, and spin-lattice relaxation time T1 for 63 Cu in LSCO:x, for x ranging over the superconducting region, 0.06 ≤ x ≤ 0.25. This system was seen to exhibit a peculiar sort of pseudogap eﬀect, which strongly aﬀects the susceptibility even at the peak of the Tc curve, but allows the 63 Cu T1 curves to follow a Curie-Weiss-like behavior down to temperatures very close to Tc . Here, we look at another aspect of the LSCO system which came about, because this system emerged as being unique among the cuprates in havineg received a very thorough characterization of χ (q, ω) by means of INS. The detailed geometry of the four mildly incommensurate peaks near (π, π) has been scanned in great detail over a wide range of frequencies. As a consequence, LSCO became a classic “test bed” for the theoretical relationship between NMR and χ (q, ω). We ﬁrst review the theoretical basis for such an investigation. The ﬂuctuation-dissipation theorem relation between spin-ﬂuctuationgenerated T1 processes in a metallic environment and the dissipative term χ (q, ω) of the dynamical susceptibility, as recounted in Sect. 3.5, had been known for many decades [18] before it was tested using experimental INS data for χ (q, ω). The latter test was conducted via T1 measurements for 63 Cu and 17 O (both planar and apical) in LSCO:0.15 [19] and was based on the INS data of Cheong et al., [20] and Mason et al., [21]. Such an enterprise – to correlate two pieces of experimental data using an “exact” theoretical relationship2 – may not seem well motivated at the outset. However, this relationship had not been tested experimentally before. Furthermore, it led to the uncovering of some interesting limitations, among which is the clash between INS and NMR data for the case of planar 17 O [19], which we review below. In this section we review the circumstances of the latter test, which call into question the usual assumption that INS results may safely be extrapolated to NMR frequencies, which are lower by a factor ∼ 104 . Additional INS data which have appeared since that time may throw some new light on the 2

This relationship is very nearly exact under the assumption that spin hyperﬁne processes are predominant. However, it has not yet been determined how important the orbital relaxation rates are for the cuprates (see Sect. 5.6).

228

6 Dynamic Susceptibility Studies for the Cuprates

situation, as well. We shall also review indirect spin-spin coupling measurements for LSCO:0.15, interpreted with values of χ (q) which were calculated from the measurements of χ (q, ω) using the Kramers-Kronig relation [22] 2 ∞ χ (q) = dωχ (q, ω)/ω . (6.3.1) π 0 From (6.3.1) one sees that such a procedure requires data for χ (q, ω) over a wide range of frequencies. Since that time, such high-frequency data have actually appeared in the literature [23]. The latter data will be taken into account in reviewing this calculation. For the T2 processes we come to a similar conclusion as with T1 , namely there is a successful account of the 63 Cu data with (or without) discommensurations, but not for the planar 17 O (see Sect. 6.3.2). 6.3.1 Review of INS Data for Optimally-Doped LSCO We ﬁrst set the stage with a brief review of relevant INS data for LSCO:x, with x ∼ 0.15. It seems that of all the cuprate compounds, LSCO alone was available in large, uniform crystals with homogeneous oxygen content. Conveniently enough, χ (q, ω) is a quantity which can be measured directly by means of INS. The principal diﬃculty is that INS measurements can only be made at frequencies several orders of magnitude higher than those at which NMR data are recorded. We examine the available INS data with that problem in mind. INS data for χ (q, ω) at energies of a few mV are shown in Fig. 6.4. In part (a) we see data for scans through two of the four incommensurate peaks located at (π, π) ± δ(0, π) and (π, π) ± δ(π, 0), where δ = 0.245 for La1.86 Sr0.14 CuO4 [21]. The peaks are seen to be well resolved, with relatively little diﬀerence between behavior near Tc = 35 K and that at 4.6 K. There is, however, an increase in intensity at the point between the peaks at higher energy. That trend is also visible in the lower-energy scans from Thurston et al., [24] in part (b) of Fig 6.4, where at ω = 1.5 meV the peaks are completely resolved, while) at 4.0 meV there is already some ﬁlling in of the space between peaks. The incommensurability varies with composition, δ 2x [20], but it shows no measureable variation with energy at the lowest energies scanned [24]. From available INS results for LSCO, then, it does not appear that discommensurations will vanish at lower (i.e. at NMR) frequencies, although the point remains at issue. At higher frequencies, however, early work showed the discommensurations fading into a single broad peak by ω = 15 meV [20]. That this trend would continue to higher energies was veriﬁed by studies to above 200 meV carried out at ISIS [23]. In that study, results for LSCO:x, x = 0.14, were compared with the undoped antiferromagnet La2 CuO4 , both qscans and energy spectra. For LSCO:0.14, discommensurations are not visible

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

229

ζ 1.1 1.2

–10

150

(a)

counts (11 min)

90 70 90 70 Background

50 T = 35 K T = 4.6 K

120 80 60 60

40

20

40

Q = ζ(π,π) + δ/√2(–π,π)

0.6

0.8

1.0 ζ

1.2

75

1.4

ω = 3.0mev T = 35K

0 150 ω = 3.0mev T = 10K 75

50

50

25

25

150

ω = 1.5mev T = 35K

0 200 ω = 1.5mev T = 10K 150

100

100

50

50

0

counts (11 min)

100

40

80

0 200

6.1 mev

counts (11 min)

140

35K

150 ω = 2.0mev T = 35K 120

40

0 100

110

ω = 4.0mev

counts (11 min)

Intensity (Counts/6 minutes)

130

60

(b)

counts (11 min)

0

T = 35 K T = 4.6 K

ΔI (Counts)

9 mev

counts (11 min)

80 10

0 0.6 0.8 1.0 1.2 1.4 0.6 0.8 1.0 1.2 1.4 q1/π q1/π

Fig. 6.4. (a) INS q-scans along the path shown at the bottom of the ﬁgure are plotted for T ∼ Tc and for T Tc for the two scattering energies shown [21]. These data show the well-resolved incommensurate peaks and a relatively small diﬀerence in scattering intensity for the two temperatures. The inset shows the diﬀerence in intensity measured for the two temperatures at 9 meV. Note the small, but deﬁnite increase in intensity between the peaks between 6 meV and 9 meV. Reprinted ﬁgure from T. E. Mason, G. Aeppli, H. Mook, Phys. Rev. Lett. 68, 1414 (1992). Copyright 1992 American Physical Society. (b) INS data at energies ω ≤ 4.0 meV, showing very well-resolved incommensurate peaks with no measurable variation of the discommensuration δ with ω. These authors ﬁnd δ = 0.22 for La1.85 Sr0.15 CuO4 . They also ﬁnd relatively small variation of intensity with temperature below Tc . Reprinted ﬁgure from T. R. Thurston, P. M. Gehring, G. Shirane, et al.,, Phys. Rev. B46, 9128 (1992). Copyright 1992 American Physical Society

in the lowest energy scans (25-50 meV) reported [23], nor any above that. The resolution in q-space may be somewhat marginal for this purpose, although the AFM (Bragg?) peak at 295 K for La2 CuO4 showed a width Δq ∼ 0.25 r.l.u. We display three composite data plots from Hayden et al., [23], namely ∞ the equal-time spin correlation function S(q) = −∞ dω χ (q, ω), the zero∞ frequency susceptibility χ (q) = (2/π) 0 dωχ (q, ω) /ω, and the local sus ceptibility χ (ω) = q χ (q, ω). These quantities have been computed from the results of the spallation–source study [23]. The local susceptibilities are shown in Fig. 6.5(a) and (b), where it is noteworthy that the results are plot-

230

6 Dynamic Susceptibility Studies for the Cuprates

ted in absolute units, and where in (b), reactor-based results are included below ∼ 25 meV . Below we shall compare these data with the absolute susceptibility results which were used to calculate T1 in [19]. The results in Fig. 6.5(a) and (b) show that the eﬀect of doping is to concentrate χ (q, ω) at energies below 50 meV (as compared with La2 CuO4 ), and that the peak seen at 22 meV is a “new energy scale” for this superconductor [23]. This energy is also a rough upper limit for the appearance of discommensurations. The solid line plotted in panel (b) is Γω , (6.3.2) χ = (Γ 2 + ω 2 ) with Γ = 22 ± 5 meV . The equal-time correlation function S(q) and the zero-frequency susceptibility χ (q) obtained with (6.3.1) in [23] are shown in Fig. 6.5 for the undoped ((c) and (d)) and the doped ((e) and (f)) cases, respectively. Owing to the near-constant width of χ (q, ω) in q-space for LSCO:0.14 [23], there is very little diﬀerence between S(q) and χ (q). The associated energy integrals have been carried out for ω ranging from 15 to 150 meV. The central peak in Fig. 6.5(e) and (f) has an HWHM of κ = 0.26(5) ˚ A−1 , which is just slightly larger than the incommensurate splitting. (See below for deﬁnition of κ.) Since the Kramers-Kronig integral favors low energies, one wonders whether there would be visible incommensurate peaks in χ (q) if the reactor-based intensity (e.g. that which gives the open circles in Fig. 6.5(b)) were included in the calculation of χ (q). As noted below, such a contribution might be appreciable for indirect spin-spin coupling with the planar 17 O. The Calibrated Susceptibility for T1 Calculations in LSCO In order to discuss T1 behavior in LSCO we need two main ingredients. The ﬁrst is a calibrated susceptiblity function χ (q, ω) for vanishing ω, with detailed q-dependence, and the second is a measured HF tensor or a near approximation thereto. We begin with the calibrated susceptibility, which was used earlier in [19], but originated with the measurements of Mason et al., [21]. The absolute calibration to these was presented in [25], but had also been used, it seems, in the paper by Hayden et al., [23]. We shall recount here the calibration used in [19]. Some careful checking ﬁnds that the latter result leads to a value for the initial slope of χ (ω) in Fig. 6.5(b) within 10% or less of the plotted value. The low-energy INS data for χ (q, ω), part of which is displayed in Fig. 6.4(a), may be represented in the normal state by the function χ (q, ω) K0 A2 θ[Γc − Γn (q)] = , (6.3.3) ω Γn (q)2 ω→0 where Γn (q) = A2 [κ2 + R(q)], with R(q) =

1 8π 2 a2L δ 2

{[(qx − qy )2 − π 2 δ 2 ]2 − [(qx + qy )2 − π 2 δ 2 ]2 } .

(6.3.4)

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

231

(a) La2CuO4(T = 295K)

4 3

χ′(ω)(μ2B eV–1 tu–1)

2 1 0 4

(b) La186Sr0.14CuO4(T = 17K)

3

Risa ISIS

2 1

S(Q)(μ2Btu–1)

0

0

50

100 hω

150

200

250

(meV)

3

(e)

15–150 meV

2

(c) 1

2

χ′(Q)(μBeV–1tu–1)

0 40 30

(d)

(f)

20 10 0 0

0.5

1 1.5 h (r.l.u)

0

0.5

1 1.5 h (r.l.u)

2

Fig. 6.5. (a) and (b) The local susceptibilities χ (ω) for La2 CuO4 (295 K) and LSCO:0.14 (17 K), derived from the data presented in [23], are plotted as a function of energy ω. As compared with La2 CuO4 , the eﬀect of doping is seen to concentrate the amplitude at low energies, giving a peak at ∼ 22 meV . Below that point are plotted data from earlier reactor-based studies [21], which serve to determine the initial slope used for T1 calculations. (c) and (e) are the equal-time spin correlation functions S(q) deﬁned in the text, for La2 CuO4 and LSCO:0.14, respectively. (d) and (f) are zero-frequency susceptibilities χ (q) obtained with (6.3.1) in a similar fashion. For LSCO:0.14 ((e) and (f)) these quantities are nearly indistinguishable, since the width of χ (q, ω) shows very little dependence on energy [23]. In (c)–(f) the rise in intensity to the right is caused by phonons, where the suggested behavior of the quasiparticle properties is indicated by dashed lines. Although the spallation source resolution width is not as good as in reactor-based studies, it is clearly well below the peak widths found for LSCO:0.14 in (e) and (f). Reprinted ﬁgures from S. M. Hayden, G. Aeppli, H. Mook, et al.,, Phys. Rev. Lett. 76, 1344 (1996). Copyright 1993 American Physical Society

232

6 Dynamic Susceptibility Studies for the Cuprates

Here aL = 3.8˚ A is the CuO2 lattice constant and δ = 0.245 is the discommensuration [21]. The other quantities in (6.3.3) are • •

• •

The constant A2 = 3.858 eV ˚ A2 comes from a form used to ﬁt INS data at ﬁnite values of ω [21]. The peak width parameter κ = [(0.034)2 + 31.35(kB T )2 ]1/2 ˚ A−1 is also from an expression used to ﬁt data over a range of ω values, but is stated here for ω = 0. In this expression kB T is to be entered in units of eV. We note that this representation of κ has been updated [25] from what was used in [19]. The two expressions give very similar values for temperatures of 100 K or less. The calibration obtained using acoustic phonons [25] gives K0 A2 2.5μ2B . The function θ[p] = 1 if p > 0 and 0 otherwise. In (6.3.3) Γc is taken to be an estimated maximum magnon energy ∼ 0.3 eV .

The foregoing function describes χ (q, ω) in q-space as having four incommensurate peaks located at (π, π)± (0, π)δ and (π, π)± (π, 0)δ. These peaks have calibrated widths given by κ. As stated, the function has units of μ2B /eV 2 per formula unit. This is the initial slope of χ (q, ω), determined by INS data at energies of just a few meV. From the standpoint of INS methodology, it is supposed that this function would apply in the energy range in which it was determined and to all energies below that as well. As we shall see below, however, there is a problem with this interpretation in connection with the T1 data for the planar 17 O, which will be discussed in Sect. 6.3. We note here that there is also a second problem with using INS measurements as a calibration of χ (q, ω) for NMR frequencies. This has to do with the behavior in the superconducting state. We know from T1 measurements for 63 Cu in LSCO (as well as those for other superconductors at T < Tc ) that the eﬀective value of χ (q, ω) declines typically by a large factor. For LSCO 1/T1 drops by a factor ∼ 100 at a temperature of 4.2 K relative to its value in the normal state [3]. The INS data for χ (q, ω) as given by Thurston et al.,, for example, shows no decline whatever below Tc , particularly at the lowest energies tested ω ∼ 1.5 meV. As the latter authors have commented [24], this is a situation for which ”further theory is required”. It seems, then, that we do not always understand when the INS results will apply at NMR frequencies and when they do not. NMR Shift and Susceptibility Analysis for LSCO Below, we apply the calibrated expression (6.3.3) for χ (q, ω) to T1 data for Cu and planar 17 O in LSCO. For this purpose, The numbers are similar to those for YBCO given in Chap. 3, but need, of course, to be established independently. Working from the 63 Cu shift results of Ohsugi et al. [3], it is ﬁrst noted that Kc (T ) is constant at ∼ 1.20% well into the superconducting state. Similar to YBCO, then, we have Ac + 4B 0. Next, Kcvv is slightly smaller than that ( 1.28%) for YBCO. Thus, the crystal-ﬁeld energies for 63

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

233

Table 6.2. Compilation of parameters related to the analysis of 63 Cu and planar 17 O NMR shifts and susceptibilities for LSCO:0.15 at T = 300 K. These quantities are deﬁned and discussed in the text. The units are as follows: NMR shifts: %; susceptibilities: 10−6 emu/mol; HF constants: kOe/spin. The HF constants are deﬁned by (3.3.2). They will have their proper energy units when multiplied by 103 γ17,63 gab gc

vv s vv Kab Kcvv Kab χvv χsab χsc B Aab Ac ab χc

Ka17 Kb17 Kc17 Ca Cb Cc

2.06 2.27 0.27 1.20 0.41 19.1 85.1 145 177 76 19 -304 0.274 0.162 0.214 108 64 77

LSCO are a bit higher and the g-factors slightly smaller as well. Estimated values are given in Table 6.2. From the Kαvv tensor we use the eﬀective orbital HF shift coeﬃcient αorb = 141 (emu/mol)−1 given with (2.3.5) for YBCO. This leads to the Van Vleck susceptibility components given in Table 6.2. The Van Vleck susceptibility tensor is combined with the estimate χdia −99 × 10−6 emu/mol [26, 27] to extract the spin susceptibility tensor from χexpt = χsα + χvv α α + χdia .

(6.3.5)

The powder average susceptiblity was found to be 98 × 10−6 emu/mol (300 K) [19], a value within 5% of those given by Ishida et al., [28] and Johnston [29]. Since χsα ∝ gα2 [18], we deﬁne a quantity χs0 with the relation χsα = (gα2 /4)χs0 . This leads to the expression for the powder average spin susceptibility 13 (χsc + 2 χsab ) = 1.137 χs0 using g-values from the table. With (6.3.5) and the numbers given, we ﬁnd χs0 = 137.1 × 10−6 emu/mol. The values for χsα in Table 6.2 follow immediately. These are essentially the susceptibility results given in [19]. Note that the spin susceptibilities are substantially larger than those found for YBCO7 (Table 3.4). We now can extract the 63 Cu spin HF constants for LSCO:0.15. The shift s s coeﬃcient for Kab 0.41% (300 K) [3] is Kab /χsab = 28.3 (emu/mol)−1 . Using (2.3.4) this gives Aab + 4B = γ63 325 kOe/spin. From studies of undoped La2 CuO4 [30] we take the result Aab − 4B = −286 kG/spin. Combining the latter two relations leads to Aab and B as given in Table 6.2, as well as the estimate Ac = −4B = −304 kG/spin. All results are summarized in Table 6.2. We believe that these slightly smaller numbers than used in [31] give a more realistic outcome. The corresponding values Cα for the planar 17 O were derived from roomtemperature NMR shift measurements and reported in [19]. The shift meaorb surements, which have been corrected for orbital background shifts Ka,b,c = (0.046,0.008,-0.027) (in %, from Takigawa et al., [32]), and their corresponding HF constant values are listed in Table 6.2. Evaluation of T1 for

63

Cu and

17

O from INS Data

With HF couplings from Table 6.2, we can now evaluate T1 for 63 Cu and 17 O in LSCO:0.15 using the INS susceptibility data embodied in (6.3.3). Relaxation rates were calculated for 63 Cu with (3.5.11) and for 17 O with (3.5.14) [19].

234

6 Dynamic Susceptibility Studies for the Cuprates 40

8

(63T1NQRT)–1

6

30

4

20

2

10

(63T1NQRT)–1 sec–1 K–1)

(17T1pT)–1 (10–3 sec–1 K–1)

(a)

(17T1pT)–1 0

0

50

100 200 150 Temperature(K)

250

300

0

3.0 0.20

0.15

2.0 1.5

0.10

1.0

Ks17p(%)

(17T1pT)–1 (10–1 sec–1 K–1)

(b) 2.5

0.05 0.5

(17T

–1 1pT)

Δ

K317p 0.00

0.0 0

50

100 150 200 Temperature(K)

250

300

Fig. 6.6. (a) Data for 1/T1 T are plotted vs. T for 63 Cu (ﬁlled squares, +’s: righthand scale) and for apical 17 O (dots: left-hand scale) in LSCO:0.15 [19]. The data plotted as +’s are from Imai et al. [33]. The dotted curve is a plot of the calculated rate based on INS data given with (6.3.3) and HF constants from [19]. See text for discussion of expected behavior with HF constants from Table 6.2. (b) 1/T1 T data (dots) are plotted vs. T for planar 17 O in LSCO:0.15 [19]. Also plotted are s (open triangles), which have been scaled data points for the c-axis NMR shift K17p to coincide with the relaxation data (right- hand scale). The calculated behavior for 1/T1 T based on INS data given with (6.3.3) and HF constants from Table 6.2 is shown as a dotted line. See text for discussion of these results. Reprinted ﬁgures from R. E. Walstedt, B. S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994). Copyright 1994 American Physical Society

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

235

Experimental data plotted as 1/T1 T for both 63 Cu and the apical 17 O in LSCO:0.15 are shown in Fig. 6.6(a). 63 Cu NQR data are plotted as ﬁlled squares, while some earlier data from Imai et al., [33] are plotted as “+” symbols. These data sets are in very good accord where they overlap. In addition, data for the apical 17 O scaled to coincide with the 63 Cu data between 100 K and 200 K are shown as dots with error bars. Since the apical 17 O is relaxed purely by local HF contact with one Cu-site spin, it is expected to behave roughly like the 63,65 Cu. Owing to a very weak HF coupling, the latter data (i.e. 17 T1 ) are in the seconds range at 50 K, while the corresponding numbers for 63 Cu are in the sub-millisecond region. The apical oxygen appears to be diverging at the lowest temperatures a bit faster than the 63 Cu, but they otherwise show a very similar temperature dependence. The calculated values of 1/T1 T for the 63 Cu based on INS data for χ (q, ω) are shown as a dotted line cutting through the data plot at a rather steep angle [19]. With very limited parameter adjustability, the agreement between INS data and the 63 Cu relaxation rate is quite satisfactory. However, our current estimate of the HF parameters, i.e. B in particular in Table 6.2, is somewhat smaller than that used in [19]. The latter values would therefore lead to estimates of 1/T1 T ∼ 30% smaller than those plotted in the ﬁgure. We suggest that this would give a somewhat more realistic result, although it would clearly show that some other mechanism – presumably from a “background” contribution to χ (q, ω), which cannot be see with INS – becomes important at higher temperatures. In Fig. 6.6(b) are plotted 1/T1 T data for the planar 17 O (dots: lefthand scale) scaled with three NMR shift data points (open triangles: righthand scale). Thus, 1/T1 T follows the susceptibility curve as was found for YBCO6.63 (Figs. 4.4 and 4.9), in behavior which is typical of a spin pseudogap. On the other hand, the calculated 1/T1 T curve based on INS data and (3.5.14), shown as a dotted line, has the correct magnitude, but varies with temperature in a fashion which is totally incompatible with the NMR data. The magnitude of the INS-based estimates of 1/T1 T is generally correct for both nuclear spin species, verifying in part the extrapolated use of INS data at such low frequencies. What appears to be the case for the planar 17 O , however, is that the discommensurations do not appear to hold up at the very low NMR frequencies3 . With the same parameters for χ (q, ω), except that δ ∼ 0, the planar 17 O curve would drop by more than an order of magnitude. It follows, then, that the 17 O relaxation process is completely dominated by 3

The decay of the discommensurations at low frequencies implies, of course, that there is another energy scale in the problem where this happens. We must point out that there is no other evidence for such an eﬀect. Moreover, such a crossover to commensurate ﬂuctuations has been suggested to imply an instability in the system as well (C. Varma, private communication). We only wish to emphasize that the discommensurations observed in INS studies lead to predicted NMR eﬀects which are not found.

236

6 Dynamic Susceptibility Studies for the Cuprates

a broad background term in χ (q, ω) which covers most of the BZ and which has the pseudogap (NMR shift–like) temperature dependence. In [19] it was suggested that a two-band model of quasiparticle dynamics may be the answer to the 17 O T1 problem. However, in view of all of the negative discussion of that option in earlier chapters, such a possibility seems to be quite out of the question at this point. On the other hand, just how the discommensurations disappear and below what energy scale this happens are just as much a mystery now as they were in 1994. To this we must add the discrepancy which occurs in the superconducting state, where INS shows only a modest decline in the vicinity of Q = (π, π) [21, 24]. Before concluding from this discrepancy with NMR data that there is some problem in principle here, however, one must verify that this is not a sample-dependent eﬀect.4 6.3.2 Interpretation of for χ (q)

63

Cu and

17

O T2 Data with INS Data

In Sect. 6.1 the interpretation of spin-echo decay (T2g ) measurements with the purely static indirect coupling term Hzz (see Appendix A.1) was discussed in some detail. This technique has been applied widely to cuprate NMR/NQR measurements. Here we consider the case of LSCO:0.15, for which we shall use the INS-derived calibration of χ (q, ω), along with the Kramers-Kronig relation (6.3.1), to obtain quantitative estimates of χ (q). The latter data, combined with HF constants from Table 6.2, are used for the indirect coupling calculation. Spin echo decay in LSCO:0.15 presents a number of complications which did not occur in the “static” cases discussed in Sect. 6.1. The eﬀects of T1 ﬂuctuations, both direct and indirect (i.e., of neighbors), are quite important. Moreover, there is strong evidence that like-spin 63,65 Cu neighbors in the m = ± 21 states are ﬂuctuating among themselves on the time scale of T2 , changing the nature of the problem in a fundamental way. The planar 17 O also present a diﬀerent and unique situation, in that T2 is dominated by the 63,65 Cu-17 O indirect spin-spin coupling term, which is time-modulated by the 63,65 Cu T1 processes. The 17 O-17 O coupling term is reckoned to be negligibly small. The somewhat diﬀerent methodology needed to treat these cases was reported in [31]. The techniques used there will be reviewed brieﬂy here in the course of discussing the T2 data for LSCO:0.15 and its interpretation. 63,65

Cu T2 Data and Simulations of Nuclear Spin Fluctuations

Spin-echo decay measurements for 63,65 Cu were carried out on a partially oriented powder sample of LSCO:0.15 containing ∼ 30% 17 O [31] at T 100 K. The measurements were made on the (− 12 ↔ 12 ) transition in a ﬁeld of 7 T. Decay curves were measured for 63 Cu with several levels of refocussing 4

The author thanks T. E. Mason for an informative discussion of this point.

6.3 Coordinated Interpretation of NMR and INS Data for LSCO 100

237

100 63

Cu: Cu:

Cu: Δ + O

65

63 65

(a)

10–1

Echo Decay (Arb. units)

Echo Decay (Arb. units)

Cu: ×

(b) 10–1 100 63

Cu: Cu:

65

(c)

10–2 0.0

10–1 0.5 1.0 (2τ)2(μ sec2)

1.5 ×104

0.0

0.5

1.0

(2τ)2(μ sec2)

1.5

×104

Fig. 6.7. (a) Spin echo decay curves for 63,65 Cu taken on the (− 21 ↔ 12 ) transition in a ﬁeld of 7 T at a temperature of 100 K. Data for diﬀerent refocussing pulses have been displaced vertically for clarity. Conditions are as follows: Full power, θ2 π (63 Cu: Δ). Power down 10 db, θ2 3π/4 (63 Cu: +). Power down 10 db, θ2 π/4 (63 Cu: ◦). Full power, θ2 π (65 Cu: ×). The curvature is thought to be caused by a distribution of indirect coupling strengths. The bottom curve is a composite of all the data. The solid line is the estimated Gaussian decay with T2g = 75.6 μs. These data have all been corrected for direct T1 eﬀects as described in the text. (b) and (c) Simulated decay curves obtained with random-number selection techniques as described in [31]. Small dots and triangles show static decay curves for 63 Cu and 65 Cu, respectively, where the decay is caused by a single π pulse. The solid lines show pure Gaussian decay. For (b) the large triangles and dots show how the decay curves are modiﬁed if random transitions simulating T1 relaxation eﬀects are included. For (c) the large triangles and dots show results for when both T1 ﬂuctuations and ﬂipﬂop transitions between the ± 21 levels for 63,65 Cu are included as described in the text. Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

pulse as well as for 65 Cu with θ2 π. The echo decay data obtained are shown in Fig. 6.7(a) [31]. The decay data shown have been corrected for direct T1 relaxation eﬀects using results from Appendix A.3. The essence of the procedure is as follows. Direct T1 relaxation eﬀects result in a factor exp(−2τ /T1E ) multiplying the spin echo decay function. The value of T1E depends on the T1 process of the nuclei observed, i.e. on its anistropy and on the transition being excited. Deﬁning Wα to be the contribution to 1/T1 from ﬂuctuations along the α axis,

238

6 Dynamic Susceptibility Studies for the Cuprates

then the relaxation rate with ﬁeld along the z axis becomes 1/T1z = Wx + Wy . For arbitrary half-integral spin the (− 12 ↔ 12 ) transition echo decay rate for isotropic spin-lattice relaxation is 1/T1E = (I + 12 )2 /T1 . For the anisotropic case this becomes 1 T1Ez

=

[I(I + 1) − 3/4] 1 1 + + , T1z 2T1x 2T1y

(6.3.6)

in terms of T1 values measured along the three axes. For axial symmetry with I = 32 this becomes 1/T1Ez = 3/T1z + 1/T1xy in an obvious notation. With known values of T1α for LSCO:0.15, this formula gives T1Ec = 90μs for 63 Cu and 80 μs for 65 Cu. The corresponding correction factors have been applied to the echo decay data in Fig. 6.7(a). The decay curves in Fig. 6.7(a) have been shifted vertically for clarity. At the bottom of the ﬁgure is a composite plot of all four curves, which shows that they are very nearly indistinguishable. This is a remarkable result in the sense that the decay is independent of θ2 and is also the same for both isotopes, whose γ values diﬀer by ∼ 7%. The ﬁrst eﬀect shows that there is considerable amount of “ﬂip-ﬂop” motion taking place, and the second can be rationalized by means of the latter eﬀect combined with the eﬀect of T1 ﬂuctuations [31]. We give here a brief account of these mechanisms, which were presented in detail in [31]. In order to take account of the foregoing eﬀects in a calculation of spin echo decay, the decay process has been simulated with a model where the spin in question is coupled to neighbor spins with a set of randomly chosen coeﬃcients. The coeﬃcients are scaled to give a second moment adjusted at ﬁrst to produce the observed value of 1/T2g (line drawn in Fig. 6.7(a)) in a static decay process for 63 Cu. In a statistical simulation of such a static echo decay this yields the small dots in Fig. 6.7(b) for 63 Cu and small triangles for 65 Cu. Straight lines representing precise Gaussian decay functions are drawn for comparison. Note that the 65 Cu spin echo decays much more slowly than the 63 Cu. This is because the 31% abundant 65 Cu has only half as many “like-spin” neighbors with which to relax the echo [31]. The next step is to introduce the “indirect T1 eﬀects” by allowing the neighbor spins to execute random transitions between m levels at the correct rate dictated by magnetic dipole coupling T1 processes. The result of this is shown as large dots (63 Cu) and large triangles (65 Cu) in Fig. 6.7(b). The decay constant 1/T2g for 63 Cu is increased by ∼ 15% by the T1 ﬂuctuations, but for 65 Cu the increase is nearly three times as much. This is because the number of neighbor spins relaxing the 65 Cu is increased by about a factor of six, whereas the increase for 63 Cu is much smaller. Now the 63 Cu are relaxing ∼ 10% faster than the 65 Cu. The ﬁnal step is to initiate ﬂip-ﬂop transitions between the ± 12 levels of both isotopes. That these are actually taking place is evidenced by the absence of change in the decay curve with θ2 in Fig. 6.7(a). Since the (± 12 ↔ ± 32 ) transitions undergo severe ﬁrst-order quadrupolar broadening, ﬂip-ﬂop transitions

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

239

are only allowed for the ± 12 levels. Estimates from the indirect interaction calculations suggest that ﬂip-ﬂops are present on a time scale of about 50 μs. Introducing these into the simulation then gives the decay curves shown in Fig. 6.7(c) (large dots and triangles). The 65 Cu decay time increases slightly, but the 63 Cu increases by more than 10%, so that the two now very nearly coincide. Evidently, the ﬂip-ﬂops give a slightly greater “narrowing” eﬀect for like spins than for unlike spins. In any case, now the decay times are nearly the same for both isotopes, as was observed. Quite coincidentally, they are both now equal to the initially estimated static decay time for 63 Cu within just a small error. We do not believe that there is any simple way to obtain this result except by simulation [31]. Indirect Coupling Calculations for

63

Cu

Having determined a reasonable experimental estimate of 1/T2g for the 63 Cu in LSCO:0.15, we could now compare that number with calculations based on an evaluation of aα (i, j) with (6.1.7), the HF parameters from Table 6.2, and χ (q) calculated with INS data for χ (q, ω) using the Kramers-Kronig relation (6.3.1). This kind of calculation was reported in [31], using the form (6.3.3) for χ (q, ω) at all energies. Below, we display the latter results and then make a critical commentary on how this evaluation should be modiﬁed in the light of more recent INS data, particularly the high-energy spallation source results [23].

χ0′ (ω,T)/hω (103μB2 /eV2)

2.0 × 104

|αij|(sec–1)

1.5

1.0

ωpeak 5

0

ωco

0

20 40 hω (meV)

0.5

0.0

0

2

4

6

8

10

rij /aL

Fig. 6.8. The calculated range function αij for the “zz” indirect coupling terms among the 63,65 Cu is shown as ﬁlled circles vs. rij . Only coeﬃcients greater than 2% of the nn value are included in the plot. The inset shows the coeﬃcient from (6.3.7) which occurs in the KK integral, adjusted to yield the measured value of T2 . Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

240

6 Dynamic Susceptibility Studies for the Cuprates

In [31] the same basic expression (6.1.9) was used for the coeﬃcients, where the Kramers-Kronig integral of the expression χ (q, ω) =

χ0 (ω, T )κ4 (ω, T ) , [κ2 (ω, T ) + R(q)]2

(6.3.7)

in the same notation as (6.3.3), is used for χα (q). In this expression, one has A−1 and ET = κ2 (ω, T ) = κ20 + a2L [(kB T /ET )2 + (ω/Eω )2 ], with κ0 = 0.034 ˚ Eω = 47 meV [25]. For the low-frequency region (ω < 20 meV ), the function χ (ω, T ) can be represented as linear in ω and declining with temperature as 1/T 2 [25]. It was found that the KK integral up to 20 meV was insuﬃcient to account for 1/T2g , so the integral was extended, with χ (ω, T ) = constant, up to a cutoﬀ for an evaluation at T = 100 K. Adjusting the cutoﬀ to obtain the experimental value of 1/T2g , it was found to be ωco 50 meV. The range function αij for the 63 Cu coupling (Hzz ) calculated as described is displayed in Fig. 6.8(a), where the KK integrand χ (ω, T )/ω is shown in the inset. Since there are usually four neighbors at each value of rij , this ﬁgure shows that the indirect coupling second moment is dominated by 15–20 neighbor nuclei. It is interesting to consider what modiﬁcation would be made to this analysis in the light of high-frequency χ (q, ω) data [23] (Fig. 6.5), which were not available at the time [31] was submitted. There are two main diﬀerences if one envisions using the data of Fig. 6.5. First, to the extent that discommensurations survived in χ (q), they would no doubt be greatly diminished in importance with data from Fig. 6.5, which would be represented by a single peak with amplitude varying as Γ ω/(Γ 2 + ω 2 ) with Γ = 22 ± 5 meV . This is probably of little signiﬁcance for the 63,65 Cu, but it will ﬁgure in our discussion of 17 O below. Second, the Lorentzian gives a broader “spectrum” of contributions, extending out to 150 meV and beyond. Interestingly, if one performs the KK integral for these two cases, the results agree within a few percent. Thus, the new data [23] corroborate the earlier result for 63,65 Cu[31]. T2 Decay of the Planar

17

O at 100 K

The planar 17 O spin-echo decay data at 100 K are displayed in Fig. 6.9. This decay curve cannot be characterized in a simple way, a circumstance resulting, we believe, from the nature of the sample. Whereas only a modest percentage of ﬁeld-oriented sample material contributed to the Cu NMR signals, the 17 O second-order quadrupolar shifts are negligibly small. As a result, essentially all of the poorly-aligned sample material contributes to the planar 17 O line. We therefore treat the system as a random powder. Furthermore, quite unexpectedly, the dipolar spin-spin coupling alone accounts for the decay curve in Fig. 6.9. Its peculiar character, with a long tail of low amplitude, is caused by the “magic angle” region of phase space where 3 cos2 θ − 1 ∼ 0. The corresponding subset of nuclei relax very slowly.

6.3 Coordinated Interpretation of NMR and INS Data for LSCO

241

100

SPIN ECHO AMPLITUDE (Arb. Units)

17 17O: 0:

10–1

10–2 0

1

2

3

4

5

6

(2τ)2(msec2)

Fig. 6.9. Experimental data for the 17 O spin echo decay at 100 K (ﬁlled circles) are plotted vs. (2τ )2 . The ﬁeld is oriented along the c axis. A simulated decay curve calculated with the combined eﬀects of dipolar and indirect coupling calculated as for the 63,65 Cu is shown as “×” symbols. A simulated decay curve with purely dipolar couplings modulated by T1 processes alone is plotted with ﬁlled triangles connected by a solid line. The same calculation with both T1 modulation and dynamic ﬂip-ﬂop transitions between the ± 12 levels of the 63,65 Cu neighbors, shown as ﬁlled squares connected by a solid line, is seen to be in good accord with the data [31]. Reprinted ﬁgures from R. E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995). Copyright 1995 American Physical Society

There is, however, more to the story than just those simple points. On evaluating the indirect coupling terms for the planar 17 O, it was found that the 17 O–17 O terms were small, but that there was a sizeable 63,65 Cu –17 O term, which gives an unlike spin indirect second moment Δω 2 IAB = 1.5 × 107 s−2 6 −2 [31], larger than the corresponding dipolar term Δω 2 dip AB = 6.25 × 10 s 63,65 (98% of which is contributed by the two nn Cu spins). This unlike-spin second moment is expected to dominate the 17 O spin-echo decay, because of its time-modulation by the 63,65 Cu T1 processes. Thus, for a crystal of unique orientation one has 1/T2O = Δω 2 AB T1Cu . The calculation of the powder-average decay curve, including indirect couplings evaluated as for the 63,65 Cu case above, leads to the decay curve plotted with “×” symbols in Fig. 6.8(b). This is widely at variance with the

242

6 Dynamic Susceptibility Studies for the Cuprates

experimental data. The diﬃculty, we surmise, is again related to the assumed discommensurations at NMR frequencies. If δ → 0 in R(q) (6.3.4), the indirect coupling drops by a large factor and its contribution to Δω 2 AB becomes negligibly small. This inconsistency with discommensurations is on the same scale as the estimate of T1 in Fig. 6.6(b). It again suggests that the discommensurations in the INS data ((6.3.3) and (6.3.4)) are not “seen” at NMR frequencies. There is yet another small surprise in the interpretation of Fig. 6.9. If one takes the dipolar second moment in the foregoing formula, i.e. 1/T2O =

Δω 2 dip AB T1Cu , averaged over all orientations, one ﬁnds the curve plotted with small triangles in Fig. 6.8(b), not quite in quantitative agreeement with the data. The ﬁnal curve, plotted with ﬁlled squares, is only obtained when one includes the 50 μs–rate ﬂip-ﬂops between the ± 12 levels. These, we recall, were important in interpreting the 63,65 Cu T2 decay curves as well. In the end, however, the most astonishing result is the total abnegation of indirect spin-spin coupling for the planar oxygen nuclei.

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) A large body of work has grown up around the discussion of scaling theories in the normal state of YBCO, Y248, and LSCO by Pines and co-workers [16, 34] and Moriya et al., [35]. We oﬀer here a brief summary of NMR/NQR results and interpretation in terms of the theories mentioned. Although a great deal has been done, there seem to be important questions which remain unresolved as well. The details of these theoretical models go beyond the scope of this book, so we shall focus here on predicted behavior and experimental tests thereof. In the interest of presenting a compact account of this subject, many interesting experimental details have been omitted. The interested reader is referred to the literature cited for a more detailed account of these matters. 6.4.1 Phase Diagram and Basic Relationships for T1 , T2g To facilitate discussion we display the basic phase diagram presented by Barzykin and Pines (BP) [34] in Fig. 6.10, which refers speciﬁcally to YBCOy (see also the paper by Sokol and Pines (SP) [16]). For the superconducting phases (6.45≤ y ≤7.0) the important regions are labelled “quantum critical” (QC), “quantum disordered” (QD), and “no scaling”, which was formerly termed the “overdamped” (OD) region [16]. These terms refer, of course, to the behavior of the AFM ﬂuctuations in the system, which are generally assumed to control the static and dynamic magnetic properties. One of the key parameters is a temperature-varying correlation length ξ, which is dimensionless in units of the lattice constant a. In the QC region, ξ 1 but grows shorter with increasing temperature, until at ξ ∼ 2 there is a crossover labelled Tcr to the OD region, in which ξ is of the order of 1 or less. At higher

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

243

temperatures and doping levels the AFM ﬂuctuations cease to be a controlling factor and the system reverts to a normal Fermi liquid. The temperature T∗ which marks the boundary between QC and QD will be deﬁned below. It is useful to note that the phase boundary in Fig. 6.10 is similar to the phase boundary between regions I and II of the phase diagram proposed by Varma (see Fig. 4.19). The implied physical signiﬁcance of these phase boundaries may also be quite diﬀerent in detail [36]. In Fig. 6.10, Tcr has also been identiﬁed with a maximum in the uniform susceptibility by BP, and data points shown in Fig. 6.10 for Tcr have derived from NMR shift data. Large error bars reﬂect the ﬂatness of such maxima. Below, we review an eﬀort to locate Tcr more precisely with NQR studies of T1 and T2 of 63 Cu(2) in Y248. From the behavior of 89 Y NMR shift data, Han et al., [37] have determined that the equivalent oxygen level of Y248 in the YBCOy family is at YBCO6.8. On that basis, BP suggest that Tcr for Y248 should occur at ∼ 500 K. Although drawn for YBCO, the phase diagram structure shown in Fig. 6.10 is presumed to apply to all cuprates. The superconducting region lies within the QD region. A system doped to the right of the Tcr line has no pseudogap and lies in the OD region at all temperatures. If there are AFM ﬂuctuations in the OD region, they are assumed to obey mean-ﬁeld behavior [35] as opposed to QC behavior. We now deﬁne the behavior of χ(q, ω) according to the BP model [16, 34]. 1400 1200

Temperature (K)

1000

No scaling

800 RC(z = 1)

600

QC(z = 1)

400 Neel

200

Tcr

T QD

0 6

6.2

6.4 6.6 6.8 oxygen content, y

7

Fig. 6.10. Phase diagram from Barzykin and Pines [34] for magnetic scaling behavior in the YBCO family of cuprates. In the superconducting phases there are three regions identiﬁed, the quantum critical (QC: z=1), the quantum disordered (QD: z=1), and the “no scaling” (or overdamped OD: z=2). Deﬁnition and measurement of the phase boundaries is discussed in the text. Reprinted ﬁgure from V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995). Copyright 1995 American Physical Society

244

6 Dynamic Susceptibility Studies for the Cuprates

To consider the SP-BP model, AFM correlations are characterized by the correlation length ξ and the low-frequency ﬂuctuation energy scale ωsf , both of which may vary with temperature. These energy and length scales are related by the dynamical exponent z, thus ωsf ∼ ξ z . In this connection it is also useful to employ the MMP model susceptibility [4, 11, 16] χ(q, ω)MMP =

ξ 2 χ0 1 + q 2 ξ 2 − iω/ωsf

(6.4.1)

as was employed by PS in their indirect coupling calculation [2]. Then, taking the simpliﬁed forms χ (q, ω) 1 1 ∼ d2 q , ∼ d2 q χ (q, 0)2 , (6.4.2) T1 T ω T2g ω→0 one ﬁnds the relations

T 1 1 ∼ , ∼ ξ. T1 ωsf T2g

(6.4.3)

Without paying much attention to the approximations involved, we apply (6.4.3) to diﬀerent parts of the phase diagram. In the overdamped, z = 2 −1 2 region, we have ωsf ∼ ξ 2 , leading to T1 T /T2g ∼ constant, which was the scaling prediction of Moriya et al., [38]. On this basis it was suggested that 2 is approximately constant for YBCO7 [6, 16] (however, see further T1 T /T2g discussion of this point below). At high temperatures BP suggest ωsf ∼ T , so that T1 ∼ constant and T2g ∼ T 1/2 , which is at least a semiquantitative description of the data of Imai et al., [9]. The point here is that across the Tcr line in Fig. 6.10 the behavior is expected to be qualitatively diﬀerent. Moreover, the approximations for (6.4.2) −1 ∼ ξ and one and (6.4.3) are better in that ξ 1. Thus, with z = 1, ωsf expects that T2g /T1 T ∼ constant. Again, at high T , ωsf ∼ T , so with (6.4.3) on again expects T1 ∼ constant[34]. An interesting example of the latter behavior is seen in the LSCO data of Ohsugi et al., [3] shown in Fig. 6.11. The behavior of T1 T vs. T is such that the curve is linear at high temperatures for all compositions of LSCO:x up to x = 0.24. Lest one suppose that x = 0.24 is “overdoped” (or OD), however, it is noteworthy that at low temperatures 1/T1 T for LSCO:0.24 is more than twice as great as for YBCO7 [3]. What is quite remarkable, however, is that for x = 0.075 the linear behavior of T1 T in Fig. 6.11 extrapolates nearly to the origin; T1 is almost perfectly constant from ∼ 75 K up to 300 K. The latter ﬁgure also illustrates the QC-QD boundary T∗ , which is the point at which the data for T1 T break away from the linear high-T behavior. T∗ is seen to range from ∼ 50 K to ∼ 100 K over the range of compositions tested. We note in passing that the behavior of T1 T in Fig. 6.11 suggests that the 63,65 Cu relaxation process over this range of temperature and concentrations is dominated by a single mechanism, namely the contribution of the AFM

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω) La2–xSrxCuO4

63Cu

NQR x= 0.24 0.20 0.15 0.13 0.10 0.075

100

T1T (10–3 secK)

245

50

Tc –100

0

100 T (K)

200

300

400

Fig. 6.11. Plot of T1 T data vs. T for compositions of LSCO:x, with x ranging over the supeconducting phase [3]. These data exhibit the high-temperature limiting behavior of the SP model [16], where T1 T goes asymptotically as ωsf ∼ T . Reprinted ﬁgure from S. Ohsugi, Y. Kitaoka, K. Ishida, G-q. Zheng, and K. Asayama, J. Phys. Soc. Japan 63, 700 (1994). Copyright 1994 Physical Society of Japan

peak(s) in the vicinity of (π, π). That viewpoint, however, is not quite consistent with the behavior seen in Fig. 6.6(a), where it appears from the INS data employed there that by room temperature the relaxation will be dominated by a “background” term not resolvable with INS. This discrepancy remains to be analyzed and understood. n , n = 1 or As for the behavior of T2g in LSCO, the variation of T1 T /T2g 2, was examined in some detail in a study where the indirect T1 corrections to spin echo decay discussed in Sect. 6.3 were carefully evaluated [39]. It was found for LSCO:0.15 that T1 T /T2g is constant well within the errors and 2 T1 T /T2g was not, clearly placing this system in the QC category. Interestingly, a similar evaluation for YBCO7 found that QC behavior for this system was favored as well [39], contrary to the conclusion mentioned earlier [16]. In much of the literature, the indirect T1 corrections to T2g have not been taken account of. Note, however, the work of Keren et al., [40]. 6.4.2 The Dynamical Crossover Study by Curro et al: Y248 A very interesting piece of experimental work regarding the z = 1 to z = 2 crossover is that of Curro et al., [4], who performed a temperature scan of the dynamics on the system Y248. To our knowledge, no other such test of the

246

6 Dynamic Susceptibility Studies for the Cuprates

Tcr boundary has been reported. Y248 is an excellent system for such a test, because it is stable (i.e. does not lose oxygen) for temperatures well beyond 700 K. This study reported T1 and T2g data up to the latter temperature. In order to perform such a study it was necessary to use a random powder sample, since no known epoxy resin would be stable at such high temperatures. Thus, T1 and T2g were measured using NQR and the NMR shift was measured using the powder-pattern NMR spectrum. Stray magnetic ﬁelds had to be shielded out of the sample space to a fraction of a Gauss, because they disturb the NQR spin echo decay function. Finally, the authors examined and corrected for the indirect T1 modiﬁcations of T2g described in Sect. 6.3 for LSCO [31]. One stimulus for the Y248 study discussed here was the conjecture by Barzykin and Pines [34] that the Y248 system would exhibit a crossover transition at T ∼ 500 K. The 63 Cu(2) T1 data from Y248 exhibited a curve of T1 T vs. T very similar to one of the lightly-doped compounds in Fig. 6.11 with T∗ ∼ 200 K, but showed no feature at 500 K [4]. The T2g data, on the other hand, showed a deﬁnite kink near 500 K, as may be seen in Fig. 6.12. Also shown in that ﬁgure are data (open circles) from a previous study by Corey et al., [41] which are in excellent accord, but extend only to ∼ 450 K. In Fig. 6.13 T1 and T2g data for 63 Cu(2) are combined to make plots of both 2 (lower panel), using the data described. T1 T /T2g (upper panel) and T1 T /T2g

160 140

NQR T2G (μS)

120 100 80

500K

60 40 20 0 0

200

400

600

800

Temperature (K) Fig. 6.12. Plot of measured T2g for 63 Cu(2), taken on the NQR line of Y248. Data from the study of the dynamical crossover in Y248 by Curro et al. [4] are shown as solid circles. The open circles are from a previous study by Corey et al., [41]. Note the abrupt change of slope at 500 K. Reprinted ﬁgure from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

247

5000 (a) T1T/ T2G (K)

4000 3000 2000 500K

1000

(a)

0 0

200

400 600 Temperature (K)

800

80

T1T/ T2G2 (Kμs–1)

(b) 60

500K

40

20 (b) 0 0

200

400 600 Temperature (K)

800

Fig. 6.13. Data for T1 and T2g for 63 Cu(2) in Y248, plotted as T1 T /T2g vs. T (a) 2 vs. T (b) (closed circles). The (a) panel shows the scaling (QC: z=1) and as T1 T /T2g regime extending from T∗ ∼ 200 K to Tcr 500 K. The (b) panel shows the onset of the non-scaling (OD: z=2) regime at 500 K. The earlier data of Corey et al., [41] are shown as open circles. Reprinted ﬁgures from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

The upper panel data show that once past T∗ ∼ 200 K, T1 T /T2g remains very nearly constant up to the crossover Tcr 500 K, as expected for QC behavior. Above that point it veers upward very slightly. In the lower panel, the ratio 2 T1 T /T2g is plotted with the same data. Up to 500 K the latter ratio is seen to execute a downward path, levelling oﬀ at 500 K just where the putative entry into the OD phase should occur. This seems about as clear-cut a crossover as one could expect. Moreover, these data show that the transition from QC to OD behavior is relatively sharp. The foregoing identiﬁcation of the crossover was also corroborated by NMR shift data, which indicate (Fig. 6.14) a ﬂat maximum in the uniform susceptibility in the vicinity of 500 K. These data do not locate the crossover as

248

6 Dynamic Susceptibility Studies for the Cuprates

precisely as the dynamical plots, but they are consistent with the results in Fig. 6.13. The authors have also developed a procedure to observe the crossover directly in terms of ξ(T ). Using, ﬁrst, (6.4.3) with the coeﬃcient adjusted to give the BP predicted value 2.0˚ A at the crossover, they ﬁnd the bottom curve in Fig. 6.15 (triangles). Secondly, they have adopted the exact solution for the susceptibility of a Heisenberg AFM given by Sokol, Singh, and Elstner (SSE) [42] to give a second estimate of the ξ(T ) curve, where the latter workers also suggested that this would be a reasonable approximation to the behavior of lightly-doped cuprates at high temperatures [4]. The latter susceptibility is given by χ0 (T )[1 + θ(T )] , (6.4.4) χ(q, ω, T )SSE = 1 + θ(T )γ(q) + iΓq ω where γ(q) = 12 [cos qx + cos qy ], θ(T ) = 4ξ 2 (T )/[1 + 4ξ 2(T )], and Γq is a ﬂuctuation rate which is not required for χ (q, 0) (and thus T2g ). In using (6.4.4) to interpret the T2g data, the value of χ0 (T ) was taken from the NMR shift measurements, the known HF constants were used, and the second moment was calculated using the full expression (6.1.8). The only unknown parameter ξ(T ) is then extracted from the T2g data in Fig. 6.12. These values are plotted in Fig. 6.15 as open circles. According to this determination, ξ = 1.4 at the crossover temperature, somewhat less than the BP estimate. If the de-

0.25

63KS

⊥ (%)

0.20

0.15

0.10

0.05

0.00 0

100

200

300

400

500

600

700

800

Temperature (K) Fig. 6.14. The 63 Cu(2) NMR shift is plotted vs. temperature, showing the maximum of the uniform susceptibility at Tcr ∼ 500 K, in agreement with the plot of T2g (Fig. 6.12. Reprinted ﬁgure from N. Curro, T. Imai, C.P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

6.4 The Sokol-Barzykin-Pines Scaling Theory of χ(q, ω)

249

termination using (6.4.3) is adjusted to give ξ = 1.4 at 500 K, then the curve with ﬁlled squares results, which is remarkably similar to the exact solution by SSE. In all three of the plotted curves for ξ(T ) vs. T there is a deﬁnite point very near to 500 K which one would naturally associate with a transition from one type of behavior to another, even if there had been no theoretical prediction of such a point. With the SSE susceptibility (6.4.4), however, there is a remarkably large change in the slope of the curve at Tcr , giving very dramatic evidence of the dynamical crossover. In conclusion, it seems that the QC, z = 1 behavior for AFM ﬂuctuations is clearly established for Y248 as well as for LSCO [39]. For Y248, the present work ﬁnds a clear-cut crossover transition at T 500 K. In the case of LSCO there is evidence for a crossover curve from susceptibility [43, 44] as well as Hall eﬀect data [34, 45]. It appears quite possible that a crossover curve for n plots as was done with Y248. LSCO could also be established using T1 T /T2g Measurements would probably have to be done with single-crystal samples and conducted in an oxygen atmosphere in order to maintain sample integrity at

0.9 0.8 0.7

(ξ /a)–1

0.6 0.5 0.4 0.3 0.2 0.1 0

200

400

600

800

Temperature (K) Fig. 6.15. Values of correlation length ξ(T ) derived from the data for T2g in Fig. 6.12 as follows: Triangles are from (6.4.3) with coeﬃcient adjusted to give ξ = 2.0 at T = 500 K. Open circles are from the SSE exact solution ([42]), where χ0 (T ) is derived from the shift data in Fig. 6.14. Closed squares are from (6.4.3) with the coeﬃcient adjusted to give ξ = 1.4 at T = 500 K. See text for interpretation of this result. Reprinted ﬁgure from N. Curro, T. Imai, C. P. Slichter, and B. Dabrowski, Phys. Rev. B56, 877 (1997). Copyright 1997 American Physical Society

250

6 Dynamic Susceptibility Studies for the Cuprates

elevated temperatures (e.g. see [46]). It would be interesting and important to investigate the sharpness of the crossover transition in this fashion, since the present work has shown that this could be a very interesting issue [4].

References

1. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 213, 214 2. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 213, 214, 219, 220, 244 3. S. Ohsugi, Y. Kitaoka, K. Ishida, G-q. Zheng, K. Asayama, J. Phys. Soc. Japan 63,700 (1994) 214, 232, 233, 244, 245 4. N. Curro, T. Imai, C.P. Slichter, B. Dabrowski, Phys. Rev. B56, 877 (1997) 214, 244, 245, 2 5. D. Pines, C.P. Slichter, Phys. Rev. 100, 1014 (1955) 216 6. M. Takigawa, Phys. Rev. B49, 4158 (1994) 216, 220, 222, 223, 244 7. D. Thelen, D. Pines, Phys. Rev. B49, 3528 (1994) 216 8. A.J. Millis, H. Monien, Phys. Rev. B45, 3059 (1992) 217 9. T. Imai, C.P. Slichter, et al., Phys. Rev. B47, 9158 (1993) 217, 220, 221, 223, 244 10. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 217, 220, 221, 222, 223 11. A.J. Millis, H. Monien, D. Pines, Phys. Rev. B42, 167 (1990) 219, 244 12. Y. Itoh, H. Yasuoka, et al., J. Phys. Soc. Japan 61, 1287 (1992) 220, 221, 224, 225, 226 13. N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 67, 2898 (1991) 221, 224, 225, 226 14. N. Bulut, D.J. Scalapino, Phys. Rev. Lett. 68, 706 (1992) 221, 224 15. N. Bulut, D.J. Scalapino, Phys. Rev. B45, 2371 (1992) 221, 224, 225 16. A. Sokol, D. Pines, Phys. Rev. Lett. 71, 2813 (1993) 223, 242, 243, 244, 245 17. A. Uldry, M. Mali, J. Roos, P.F. Meier, J. Phys. Condens. Matter 17, L499 (2005) 225 18. T. Moriya, J. Phys. Soc. Japan 18, 516 (1963) 227, 233 19. R.E. Walstedt, B.S. Shastry, S.-W. Cheong, Phys. Rev. Lett. 72, 3610 (1994) 227, 230, 232, 20. S-W. Cheong, G. Aeppli, T.E. Mason et al., Phys. Rev. Lett. 67, 1791 (1991) 227, 228 21. T.E. Mason, G. Aeppli, H. Mook, Phys. Rev. Lett. 68, 1414 (1992) 227, 228, 229, 230, 231, 22. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 228 23. S.M. Hayden, G. Aeppli, H. Mook et al., Phys. Rev. Lett. 76, 1344 (1996) 228, 229, 230, 23 24. T.R. Thurston, P.M. Gehring, G. Shirane et al., Phys. Rev. B46, 9128 (1992) 228, 232, 236 25. G. Aeppli, T.E. Mason et al., Science 278, 1432 (1997) 230, 232, 240 26. K. Ishida et al., J. Phys. Soc. Japan 60, 2351 (1991) 233 27. B. Batlogg, in Physics of High-Temperature Superconductors, ed S. Maekawa and M. Sato, Springer Series in Solid-State Sciences, Vol. 106 (Springer-Verlag, Berlin, 1992), p. 219 233 28. K. Ishida et al., J. Phys. Soc. Japan 60, 3516 (1991) 233 29. D.C. Johnston, J. Magn. Magn. Mater. 100, 219 (1991) 233 30. T. Imai, C.P. Slichter, et al., Phys. Rev. Lett. 70, 1002 (1993) 233 31. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995) 233, 236, 237, 238, 239, 240, 241 32. M. Takigawa, A.P. Reyes, P.C. Hammel, Phys. Rev. B43, 247 (1991) 233 33. T. Imai et al., J. Phys. Soc. Japan 59, 3846 (1990) 234, 235 34. V. Barzykin, D. Pines, Phys. Rev. B52, 13585 (1995) 242, 243, 244, 246, 249 35. T. Moriya, Prog. Theor. Phys. 28, 371 (1962) 242, 243 36. C.M. Varma, Phys. Rev. B73, 155113 (2006) 243 37. Z.P. Han, R. Dupree et al., Phys. Rev. Lett. 69, 1256 (1992) 243

References

251

38. T. Moriya, Y. Takahashi, K. Ueda, Phys. Rev. Lett. 59, 2905 (1990) 244 39. R.E. Walstedt, S-W. Cheong, Phys. Rev. B53, R6030 (1996) 245, 249 40. A. Keren, H. Alloul, P. Mendels, Y. Yoshinara, Phys. Rev. Lett. 78, 3547 (1997) 245 41. R.L. Corey, N. Curro, et al., Phys. Rev. B53, 5907 (1996) 246, 247 42. A. Sokol, R.P. Singh, N. Elstner, Phys. Rev. Lett. 46, 4416 (1990) 248, 249 43. D.C. Johnston, Phys. Rev. Lett. 62, 957 (1989) 249 44. T. Nakano et al., Phys. Rev. B49, 16000 (1994) 249 45. H.Y. Hwang, B. Batlogg, H. Takagi et al., Phys. Rev. Lett. 72, 2636 (1994) 249 46. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B64, 014404 (2001) 250

A Appendices

A.1 Some Basic Properties of Spin Echoes We give in this appendix a brief discussion of the behavior of two-pulse spin echoes. For the original derivations of spin echo phenomena see the paper by Hahn [1]. A shorter exposition by this author discussed some special topics having to do with echo studies in solids [2]. A brief list is (i) echo behavior with phase variation between the pulses, (ii) the “area theorem” (see also below), (iii) computer simulation of echo proﬁles (of which Fig. 2.3 is an example), and (iv) the cancellation of spurious transient signals in echo studies using a four-step phasing sequence for the two excitation pulses. We begin with a basic derivation of the two-pulse echo, so that the amplitude dependence on pulse rotation angles, as well as the basic phenomenology of the T2 process are illustrated. At the same time the basic principle of spinecho double resonance (SEDOR) can be illustrated. In the ﬁnal subsection we derive the Gaussian echo decay time T2g associated with the indirect nuclear spin-spin couplings ﬁrst investigated in the cuprates by the Slichter group [3] and formulated conveniently in terms of χ (q) by Pennington and Slichter [4]. A.1.1 Basic Derivation of the Two-Pulse Spin Echo. Spin echoes are generally observable with spin systems where the echo decay time is long enough so that two excitation pulses can be applied at some minimal pulse spacing, after which the echo signal can be detected following the “dead time” of the receiver. Another requirement for echo generation which is often overlooked is that the observed nuclei must be subject to a quasi-static broadening eﬀect which is greater than any homogeneous or dynamic broadening. This circumstance can come about through an internal distribution of shifts, HF ﬁelds, EFG values, quasi-static interactions with other spin systems or through the application of an inhomogeneous ﬁeld. If you have a homogeneously broadened NMR line relaxed by ﬂuctuating like-spin couplings or by

R.E. Walstedt: Appendices, STMP 228, 253–261 (2008) c Springer-Verlag Berlin Heidelberg 2008 DOI 10.1007/978-3-540-75565-4 A

254

A Appendices

T1 , you may be able to see the free-induction signal, but the echo will be very elusive. Supposing these conditions are met, let us consider the application of rf pulses to excite an echo. For simplicity, we shall suppose the excitation pulses to be of negligible length. One imagines, then, a very large rotating magnetic ﬁeld H1 (at a suitable frequency) applied for just an instant, during which the magnetization of the nuclei nutates at ω1 = γH1 away from its equilibrium position along the z axis. At time tw1 the magnetization has rotated by θ1 = ω1 tw1 , creating a magnetization component M0 sin θ1 along the x axis. Following the ﬁrst pulse, the spins are allowed to precess freely for a time τ , during which time the transverse magnetization decays quickly to zero. The associated free-induction signal is typically too short to be observed. This decay time is labelled T2∗ , being either the inverse of the width Δ of the distribution P (Δi ) of static frequencies being excited or in a broad line T2∗ ∼ π/ω1 . We consider our typical nuclear spin I i to be subject to a local, static frequency perturbation Δi . We also introduce one source of echo relaxation perturbations, namely the spin-spin coupling term (i) = αij Izi Izj = Ωi Izi , (A.1.1) HII j

where the resulting local frequency perturbation Ωi = j αij mj contributes to the precession frequency between rf pulses. The perturbation Ωi could come from like or unlike spins, and could be ﬂuctuating or static, with results which vary enormously depending on the details. We shall proceed with the calculation assuming the Ωi ’s are static, and then comment on other possible cases. During the interval between the ﬁrst and second pulses, spin I i will precess around the z axis, where in the rotating frame, the transverse component of spin i in the xy-plane precesses through an angle (Δi + Ωi )τ , where Δi and Ωi are as deﬁned above. To capture the eﬀects of these motions we follow the development in the rotating frame1 of the density matrix ρ∗ (t) which obeys the equation of motion [5] i

dρ∗ = [H∗ , ρ∗ ] , dt

(A.1.2)

where starred quantities have been transformed into the rotating frame. For simplicity we drop the star notation, noting that the rest of the calculation will take place in the rotating frame. The initial value of density matrix is ρ0 Ix , where ρ0 ∝ sin θ1 . During the interval τ between pulses and during time interval t − τ following the second pulse, spin I i will precess through the angles (A.1.3) β1i = (Δi + Ωi )τ and β2i = (Δi + Ωi )(t − τ ) , 1

The rotating frame is a reference frame rotating at the frequency of the applied rf pulses.

A.1 Some Basic Properties of Spin Echoes

255

respectively, where at time τ a second pulse of rf ﬁeld H1 is applied, rotating the spins through angle θ2 . The θ2 pulse is known as the “refocussing pulse”. At time t − τ following the latter pulse, the density matrix may be written ρ(t) = exp(iβ2i Izi ) exp(iθ2 Iy ) exp(iβ1i Izi ) Ixi ρ0 exp(−iβ1i Izi ) exp(−iθ2 Iy ) exp(−iβ2i Izi )i ,

(A.1.4)

where the brackets i indicate an average over the entire sample. In (A.1.4) only the exponential operators which survive in the echo amplitude calculation, i.e. in T r(Ix ρ(t)), are kept. At this point we make some remarks about the potential eﬀects of the broadening terms β1,2i in (A.1.4). These terms can always be divided into separate operators exp(iIzi Δi t) exp(iIzi Ωi t), where the eﬀect of the static Δi ’s is particularly simple. If the Ωi terms are static and unaﬀected by the θ2 pulse, then they have no eﬀect and will simply disappear from the calculation. If they are like-spin terms and are aﬀected by the θ2 pulse, then they cause an echo relaxation process. In the next subsection we develop expressions for the θ2 -dependent relaxation time T2g for the Gaussian relaxation from indirect spin-spin coupling in cuprates [4]. If the Ωi terms are from unlike spins, then there is a series of possible eﬀects. If, for example, an rf pulse is applied to the I spins so that their mj values (and thus the Ωi ’s) change, then the echo will undergo a potentially observable eﬀect known as spin echo double resonance (SEDOR). SEDOR has undergone various applications to solid-state science [6, 7], but we shall not discuss this technique further. If the unlike-spin Ωi ’s are ﬂuctuating in time, then there will be an associated echo relaxation process of a character which depends on whether the ﬂuctuations are slow, fast, or intermediate. If the ﬂuctuations are fast or slow, then some estimate of their eﬀects can be obtained with perturbation methods. If they are intermediate in speed, then the eﬀects could be very large and treatment would have to be improvised on a case-by-case basis. In the case where the Ωi ’s are time-dependent between the rf pulses, then it is easy to show that the Ωi τ etc. in (A.1.3) would simply be replaced by τ

Ωi τ →

Ωi (t)dt.

(A.1.5)

0

We now proceed to obtain a general expression for the echo signal from the foregoing expressions. In (A.1.4) only the exponential operators which survive in the echo calculation have been kept. These exponential operators are processed using the relation exp(iφIγ ) Iα exp(−iφIγ ) = Iα cos φ ∓ Iβ sin φ ,

(A.1.6)

where the second term is negative if (α, β, γ) is a positive permutation of (x,y,z) and positive otherwise.

256

A Appendices

Following development of ρ(t) using (A.1.6), we keep only the terms in Ixi , which form the principal component of the echo. The corresponding signal amplitude can then be written E(t) =

1 E0 (1 + cos θ2 )cos(β1i + β2i ) − (1 − cos θ2 )cos(β1i − β2i )i , (A.1.7) 2

is deﬁned below. The echo signal at t = 2τ arises only from the where β1i second term, which becomes ⎛ ⎞ E(t) = (1 − cos θ2 ) P (Δi )cos ⎝Δi (t − 2τ ) + αij [mj τ − mj (t − τ )]⎠ , E0 i j

(A.1.8) ) is the value of mj following the operation eiθ2 Izj e−iθ2 . where mj (deﬁning β1i We shall make use of this in Sect. A.2. The average over the distribution of Δi values gives the time proﬁle of the echo, which has its maximum at t = 2τ . The two terms in the cos argument ( ) in (A.1.8) are very diﬀerent in character. The Δi term vanishes at t = 2τ , but is otherwise large and rapidly varying. The second, relaxation term is a slowly varying perturbation. In a reasonable approximation we evaluate the second term at t = 2τ and separate it from the ﬁrst one and remove it from the sum as a relaxation factor fr (2τ ) = cos[ j αij (mj − mj )]j , where the

j brackets indicate a second, independent averaging process. (A.1.8) is then rewritten as E(t) = C sin θ1 (1 − cos θ2 ) fr (2τ ) P (Δi )cos[Δi (t − 2τ )], (A.1.9) i

where the average over the Δi ’s gives the echo shape function, and where we have inserted sin θ1 to give the full dependence on pulse angles. We now make some observations on the echo expression (A.1.9). First, we recount the area theorem for spin echoes. Although not developed in detail in this derivation (see [2]), an echo excited from a distribution g(ω) of NMR/NQR frequencies is an integral of that distribution over excitation factors, giving an echo proportional to ∞ dω g(ω) sin θ1 (1 − cos θ2 ) cos[(ω − ω0 )(t − 2τ )], (A.1.10) −∞

where the distribution P (Δi ) is eﬀectively replaced by g(ω). If we integrate the area under the echo, i.e. over a range −Δt ≤ t − 2τ ≤ Δt which includes all possible nonzero echo amplitude, this produces delta function in frequency so that 2τ +Δt E(t)dt = 2πC fr (2τ )g(ω0 ) [sin θ1 (1 − cos θ2 ]ω0 , (A.1.11) 2τ −Δt

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling

257

where if the pulse angles are frequency-dependent, they are evaluated at ω0 , which is the frequency of the rf pulses. Thus, the area under the echo is very precisely proportional to g(ω0 ), with a resolution which does not depend on H1 (in principle), but on the the time 2Δt over which the integration can take place. In general the resolution of g(ω0 ) is very good. In practice, the smaller H1 is, the better the resolution which is obtained. A.1.2 Modelling Spin-Echo Decay Secondly, as an example of spin-echo decay, we consider the form which fr (2τ ) from (A.1.9) takes in the limit where the mj ’s are from unlike spins and are ﬂuctuating rapidly. We therefore consider the quantities Ωi (t) to be stochastic variables, where τ ! 2τ Ωi (t)dt − Ωi (t)dt . (A.1.12) fr (2τ ) = cos 0

τ

i

The two integrals over time are equivalent under the average over i, so we expand the cosine, assuming the sine terms to vanish on averaging. Expanding the remaining cosines in power series and keeping just the ﬁrst two terms we ﬁnd τ τ dt dt Ωi (t)Ωi (t )i + · · · . (A.1.13) Fr (2τ ) 1 − 0

0

Taking the indicated average i generates a correlation function which we ∞ write as Ωi2 i C(| t − t |), where 0 C(t)dt = τc τ . The ﬁrst expansion term is therefore linear in τ so that the decay function may be approximated as (A.1.14) fr (2τ ) e−2τ /T2Ω , with 1/T2Ω = Ωi2 τc . The foregoing is an example of exponential spin-echo decay with a rapidly modulated perturbation. Another such eﬀect is echo decay through spin-lattice interactions. This is discussed in some detail in Appendix A.2.1. In the next subsection we give an example of Gaussian spin-echo decay through modulation of like-spin interactions by the refocussing (θ2 ) pulse, which is widely encountered in cuprate NMR studies.

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling The following calculation of spin-echo decay applies to magnetic dipole transitions excited between any pair of HF energy levels for which m = Iz (suitably chosen) is a reasonably good quantum number, i.e. a Δm = ±1 transition. Examples are (i) any high-ﬁeld transition with quadrupolar splittings or (ii) a zero-ﬁeld NQR splitting. For NQR lines with, e.g. I = 3/2, the excitation

258

A Appendices

pulses excite two transitions simultaneously (± 12 ↔ ± 32 ) with their separate signals. We shall be considering the decay of only one of these signals at a time, though the calculation will apply to both. We henceforward consider only the echo amplitude E(2τ ) given by (A.1.8), which can be expanded as a power series in (2τ )2n , where we keep only the τ 2 term: ⎡ ⎤2 τ 2 ⎣ E(2τ ) ≈ E0 (1 − cos θ2 ) 1 − αij (mj − mj )⎦ . (A.2.1) 2 j

i

In squaring the sum j αij (mj − mj ) the cross terms will average to zero. In the diagonal terms the quantity (mj − mj )2 will equal 1 with a probability sin2 (θ2 /2) and will be zero otherwise. (A.2.1) becomes [8] ⎤ ⎡ 2 τ (A.2.2) α2ij ⎦ , E(2τ ) E0 (1 − cos θ2 ) ⎣1 − sin2 (θ2 /2) 2 j where the j indicates a sum only over 63 Cu(2) neighbors which are being ﬂipped by the θ2 pulse. This means, typically, couplings with the same isotope, and mj -values belonging to the resonance transition observed. In high-ﬁeld NMR for I = 3/2, this means half of the neighbor spins. For NQR with I = 3/2, one sums all of the neighbor spins, because they are all part of the observed resonance. The diﬃculty in applying this is, of course, that often the line is broad and the θ2 pulse is not uniform over all of the spins. The factor sin2 (θ2 /2) in such a case is an eﬀective average value. If we suppose that (A.2.2) gives the ﬁrst two expansion terms of a Gaussian decay, then we have for the ﬁnal result for a high-ﬁeld NMR transition for 63 Cu(2), c63 2 1 2 = sin (θ /2) α , (A.2.3) 2 2 T2g 8 j ij where the ﬁnal sum over all neighbor sites is, of course, independent of i. In naturally abundant 63 Cu c63 0.69. A.2.1 Indirect Coupling with a Gaussian Susceptibility The indirect coupling range function used in the text is discussed here for the simple case of a q-independent, isotropic HF tensor and a Gaussian susceptibility χ (q). After deriving the range function from (5.1.7), results for the second moment ( j(=i) a2ij ) obtained in several ways are discussed. The general result for the indirect coupling coeﬃcient of Izi Izj is aα (i, j) =

eiq·(Rj −Ri ) χα (q)Fαα (q)2 , NA gα2 μ2B q

(A.2.4)

A.2 The Gaussian Decay Time T2g for Indirect Spin-Spin Coupling

259

where the prefactor is suited to a molar susceptibility and an HF tensor in units of s−1 . Here we take Fαα (q) = A0 , and we use the Gaussian susceptibility form employed by Auler et al. [9], which is χα (q) = χAF e−(q−Q)

2 2

ξ /4

.

(A.2.5)

Since χα (q) is symmetric about Q, we move the origin to that point with q = p+(π, π). The imaginary sine term is then seen to vanish by symmetry. For simplicity we drop the prefactor (χAF A20 /NA gα2 μ2B ) and restore it at the end. The sums may then be taken as integrals, giving, π 2 2 2 (−1)(nx +ny ) π dp dpy e−(px +py )ξ /4 cos(nx px + ny py ) . a(i, j) = x 4π 2 −π −π (A.2.6) The cosine factor can be written cos(nx px ) cos(ny py ), since the sine terms vanish. The integrals can now be written g(nx )g(ny ), where 2 2 (−1)n π (−1)n −n2 /ξ2 g(n) = dpe−p ξ /4 cos(np) √ , (A.2.7) e πξ π 0 where the last step approximates the upper limit of the integral as ∞. This is a reasonable approximation, since the exponential factor at p = π is 0.015. We shall check this approximation below, as well. The ﬁnal result for our dimensionless range function is (−1)(nx +ny ) −(n2x +n2y )/ξ2 e . (A.2.8) πξ 2 We now evaluate the second moment sum j(=i) a(i, j)2 in three separate ways, in order to test the approximation in (A.2.7). First, we may do this directly with (A.2.8), giving the expression ⎡ ⎤ 2 2 2 1 a(i, j)2 = 2 4 ⎣ e−2(nx +ny )/ξ − 1⎦ , (A.2.9) π ξ n ,n a(i, j) =

j(=i)

x

y

where the summation is over all integer values of nx , ny which would give an appreciable contribution. In what may seem a crude approximation for ξ 1.3 (see text), we evaluate the sums in (A.2.9) as an integral in a continuum approximation. This is straightforwardly shown to yield the value πξ 2 /2, so that we ﬁnd 2 1 πξ 2 −1 . (A.2.10) a(i, j) = 2 4 π ξ 2 j(=i)

The foregoing result gives the value j(=i) a(i, j)2 = 0.0587 for ξ = 1.3, which is the minimum value we shall use it for. This sum has also been evaluated by computer for the same value of ξ, giving 0.0588 for the result. It seems

260

A Appendices

then that the continuum approximation to the (nx , ny ) sums is accurate to a fraction of a percent. However, the range function itself is an approximate result from (A.2.7). We make a check on the latter result by evaluating the second moment sum using the q-space result (6.1.8), which in the present context becomes 2 −(q2 +p2 )ξ 2 /4 −q2 ξ 2 /4 a(i, j) = e − e . (A.2.11) q

j(=i)

p

q

When the ﬁrst sum is converted to an integral in polar coordinates, the integrand is porportional to exp(−q 2 ξ 2 /2), which, at q = π falls to the value ∼ 2.4 × 10−4 . While this could be accounted for in approximate fashion, we neglect errors of this magnitude for simplicity here. This term then becomes 1/(2πξ 2 ). The second term in (A.2.11) can be cast into a very similar form as that of (A.2.7), where we neglect a correction term of the order of 1.5%. Since this is squared, neglecting these correction means that the second term in (A.2.11) is small by about 3%. The two terms together give j(=i) a(i, j)2 = 1/(2πξ 2 ) - 1/(π 2 ξ 4 ), which is identical to the summing result in (A.2.10). We now see that for ξ = 1.3, this result probably errs on the high side by an amount of order 1%. For larger values of ξ the error will diminish rapidly. Restoring the prefactor and multiplying by the factor c63 /8 gives the physically correct second moment (or (1/T2g )2 ), which is 2 1 πξ c63 χAF A20 1 c63 − 1 . (A.2.12) a(i, j)2 = = T2g 8 8 NA gα2 μ2B ) π 2 ξ 4 2 j(=i)

A.3 Spin Echo Decay via Spin-Lattice Relaxation Spin-lattice relaxation of a spin echo was ﬁrst treated to explain the large disparity between conventional T1 values and the enhanced exponential decay rates 1/T1E of spin echoes for nuclear spins with large I values [10]. The relaxation rate for the (− 12 ↔ 12 ) transition was shown to be 1/T1E = 2 W0 (I + 1 2 2 ) , where 1/T1 = 2 W0 . This result was modiﬁed for the case of an anistropic T1 process by Narath [11], ﬁnding 1 T1Ez

= (Wx + Wy )[I(I + 1) − 1/4] + Wz ,

(A.3.1)

where Wα is the contribution of ﬂuctuations along the α axis to the relaxation rate for a quantization axis perpendicular to that axis. Thus, 1/T1z = Wx +Wy . The latter results have been derived using the “ﬁctitious spin 12 ” technique. They have been derived using other methods as well [3, 12]. Since the Wα ’s are not measured directly, it is also useful to express the result (A.3.1) in terms of the anisotropic T1 values T1x,y,z :

References

1 T1Ez

=

1 1 1 [I(I + 1) − 3/4] + + . T1z 2 T1x 2 T1y

261

(A.3.2)

We also treat the case of arbitrary direction for the quantization axis, represented by the Euler angles (θ, φ). We let that be the z axis with corresponding x axis in the xy plane and mutually perpendicular y axis. The associated rate parameters for the (x , y , z ) axes are Wx = Wx sin2 φ + Wy cos2 φ 2

2

(A.3.3a) 2

2

2

Wy = Wx cos θ cos φ + Wy cos θ sin φ + Wz sin θ Wz = Wx sin2 θ cos2 φ + Wy sin2 θ sin2 φ + Wz cos2 θ ,

(A.3.3b) (A.3.3c)

whereupon 1/T1Ez is given in terms of the Wα ’s by (A.3.1). This result was used to correct the planar 17 O spin echo decay data in [8] for T1 eﬀects.

References 1. E.L. Hahn, Phys. Rev. 80, 580 (1950) 253 2. R.E. Walstedt, “The two-pulse spin echo revisited”, in Pulsed Magnetic Resonance: NMR, ESR and Optics, ed. by D.M.S. Bagguley (Clarendon Press, Oxford, 1992), p. 242 253, 256 3. C.H. Pennington, D.J. Durand, C.P. Slichter, Phys. Rev. B39, 274 (1989) 253, 260 4. C.H. Pennington, C.P. Slichter, Phys. Rev. Lett. 66, 381 (1991) 253, 255 5. A. Abragam, Principles of Nuclear Magnetism (Oxford University Press, New York, 1983) 254 6. D. Kaplan and E.L. Hahn, J. Phys. Radium 19, 821 (1958) 255 7. R.E. Walstedt and J.H. Wernick, Phys. Rev. Lett. 20, 856 (1968) 255 8. R.E. Walstedt, S.-W. Cheong, Phys. Rev. B51, 3163 (1995) 258, 261 9. T. Auler, M. Horvatic et al., Physica C 313, 255 (1999) 259 10. R.E. Walstedt, Phys. Rev. Lett. 19, 146 (1967); 19, 816 (1967) 260 11. A. Narath, Phys. Rev. B13, 3724 (1976) 260 12. T. Imai et al., Phys. Rev. Lett. 71, 1254 (1993) 260

Index

AFM enhancement eﬀects below Tc , 109, 111 AFM ﬂuctuations, 5 antiferromagnetic correlations, 4, 90, 102 ARPES studies of cuprates, 2, 136 ARPES studies of energy gap eﬀects, 136 axial EFG symmetry, 15 axial shift component for 17 O(2,3) in YBCO7, 95 axial shift powder patterns, 23 BCS energy gap anisotropy from coherence peak, 43 BCS energy gap value from T1 in Al metal, 43 BCS theory of T1 for T < Tc , 41 BCS theory of T1 for the d-wave case, 108 characterization of samples, 4, 5 chemical shifts in NMR, 21, 118, 120, 122, 233 χ (q, ω), 5, Sect. 3.5, Chap. 5, 6 χ (q, 0)values derived from T2g measurements, 220 coherence factor: T1 for T < Tc , 40 coherence peak, gap anisitropy eﬀect, 43 core diamagnetic susceptibility for YBCO, 83 core polarization of Y3+ , 78

core–polarization T1 process in d-band metals, 51 core–polarization HF ﬁeld, 44 core–polarization HF mechanism, 46 core–polarization NMR shift, 5, 48, 58 crossover in phase diagram, 70, 146, 243, 246 63,65 Cu, 4 Cu(1,2) site assignment, 75 cuprate phase diagram, 3, 70, 146, 243 d–wave pairing, 6 d-wave conﬁrmation by T2g for T < Tc , 225 d-wave model for T1 at T < Tc , 104, 206 detailed balance in spin–lattice relaxation, 25 Dipolar Contribution to 89 Y HF Coupling, 125, 183 dipolar HF interaction, 33 dipolar NMR shift, 5 discovery of high–Tc , 1 dynamic susceptibility, Sect 3.5, Chap. 5, 6 dynamical structure factor, 101 dynamical susceptibilities for LSCO:x from INS data, 230 dynamical susceptibility, a simpliﬁed model, 127 dynamical susceptibility, exact solution for Heisenberg AFM, 248 dynamical susceptibility, Gaussian model, 180

264

Index

dynamical susceptibility, RPA model, 173 EFG Tensor, 14 exchange enhancement from K(α)– table, 37 Exchange enhancement of 1/T1 – Moriya theory, 36 Fermi surface in cuprates, 2, 136 Ferrell–Anderson theory of spin–orbit scattering below Tc , 39 ﬁeld–dependent T1 eﬀects in type–II superconductors, 61, 111, 200 ﬁrst-order quadrupolar broadening, 15, 94 ﬂuctuation dissipation theorem, 101 ﬂuctuation-dissipation theorem, 5 g–factors for YBCO7, 86 gamma, nuclear gyromagnetic ratio, 21 Ginzburg-Landau parameterκ, 54 Ginzburg-Landau theory, 54 gyromagnetic ratio, nuclear moment, 21 Hamiltonian for NMR/NQR spectra, 14 HF coeﬃcients for YBCO6.63 from scaling of shifts, 123 HF constants for LSCO:0.15 from NMR shift data, 232 HF couplings, 4, 82 HF Hamiltonian–general, 33 HF tensor for 89 Y in YBCO7, 96 HF tensor for 17 O(2,3) in YBCO7, 96 HF tensor, general, for cuprates, 82 HF tensors for YBCO7, 84 hole doping, 3 hole doping in cuprates, 71 Hubbard model calculation of NMR shift below Tc , 205 Hubbard model for T1 at T < Tc , 199 Hubbard model, large U, of spin dynamics, 192 Hubbard model, negative U, 127 Hubbard model, small U, for spin dynamics, 187 indirect spin–spin coupling, 6, 19, 214 indirect spin–spin coupling in LSCO:0.15 from INS data, 239

INS data for χ (q, ω), case of pseudogap, 128 INS data for χ (q, ω) in LSCO:x, 227 INS studies of cuprates, 2, 128, Chap. 6 K–χ analysis, 47 K–χ plot for Pt metal, 48 Knight shift, 32 Knight shift for T < Tc : BCS (Yosida) theory, 38, 108, 206 Korringa calculation of T1 in metals, 34 Korringa product table for metals, 35 Korringa relation, 35, 37 Korringa relation, modiﬁed for multiple HF sources, 127 Korringa relaxation, 33 Kramers–Kronig evaluation of χ (q, 0)for LSCO:0.15, 240 LSCO phase diagram, 2, 46, 70 LSCO structure, 68 LSCO, 63,65 Cu T1 data, 153, 245 LSCO:x, 2 LSCO:x dynamical susceptibility from INS, 227 LSCO:x, 17 O T1 and shift data, 153, 241 LSCO:x, NMR shifts, 152 LSCO:x, NQR spectra, 153 LSCO:x, pseudogap eﬀects, 148, 241 LSCO:x, scaling of susceptibility, 149 Mila–Rice HF tensor, 81 Mott insulator, 1, 69 NMR in d–band metals, 44 NMR probe, 4 NMR shift deﬁned, 22 NMR shift below Tc , Hubbard model calculation, 205 NMR shift correction for superconducting diamagnetism, 105 NMR shift for cuprates at T < Tc , 105 NMR shift in the mixed state of 3d superconductor, 57 NMR shift tensor, 14, 21 NMR shift tensor, scalar approximation, 22 NMR shift tensors for Cu(1) in YBCO7, 84

Index NMR shift tensors for Cu(2) in YBCO7, 84 NMR shift, anisotropic, powder pattern, 23 NMR shift, powder pattern, 23 NMR spectra, 5 NMR spectrum, quadrupolar satellites, 15 NMR studies in the mixed state of type–II superconductors, 55 NQR determination of η, 17 NQR spectrum in zero ﬁeld, 17 17

O(2,3), 5 O doping, 4 17 O EFG tensors for YBCO7, 95 17 O NMR data for YBCO7, 93, 162 17 O relaxation in YBCO7, 92 17 O shift tensors for YBCO7, 75, 95, 164 orbital T1 process in d-band metals, 51 orbital T1 theory by Varma, 195 orbital (Van Vleck) shift and susceptibility – general, 46 orbital HF interaction, 33 orbital NMR shift, 5 orbital shift and T1 process, 44 orbital susceptibilities for YBCO, 83 orbital susceptibility tensors in YBCO7, 85, 86 oriented powder samples for cuprate NMR, 80 orthorhombic phase of LSCO:x, 3, 69 oxygen hole band in YBCO7, 98 oxygen hole bands, 72, 81 17

Pennington Slichter theory of indirect spin–spin coupling, 214 phase diagram for scaling theory of AFM ﬂuctuations, 242 phase diagram of cuprate superconductor, 2, 146, 243 phenomenology of high–Tc , 1 pseudogap eﬀects for YBCO6+x vs. x, 117 pseudogap eﬀects on T1 in underdoped YBCO, 116 pseudogap energy derived from Arrhenius plot, 122, 143

265

pseudogap isotope eﬀect, Y248, 143 pseudogap NMR shift scaling in YBCO6.63, 120 pseudogap temperature, 3 pseudogap, theory by Varma, 146 pseudogaps in cuprates, 115 quadrupolar eﬀects, 4 quadrupolar perturbation, high–ﬁeld limit, 15 quadrupolar powder pattern, 16, 23 quadrupolar powder pattern, second order, 16, 23 quadrupolar tensor, sign of, 15 quantum chemistry of YBCO7, 87 resonant ﬁeld shifts, relation to K, 22 review of bulk properties, 4 RPA calculation of dynamical susceptibility, Monien and Pines, 108 s-contact (Knight) shift, 33, 47 s-contact HF interaction, 33 s-contact NMR shift, 5, 33, 47 saturating comb to measure T1 , 31 scaling theory of χ(q, ω) in quantum critical region, 242 shift vs. susceptibility analysis, 47 simulations of spin–echo decay for LSCO:0.15, 236 speciﬁc heat, pseudogap eﬀects, 134 spin echo spectroscopy, frequency resolution, 19 spin echo, observation of, 20 spin echo, two–pulse, 18, 251 spin Hamiltonian parameters for 63 Cu(2) in YBCO7, 86 spin HF tensor for Cu(2) in YBCO, 89 spin susceptibilities for YBCO, 83 spin susceptibility anisotropy for YBCO7, 86 spin–echo decay, 6, 20, 251, 255 spin–echo decay analysis for LSCO:0.15 from INS data, 236 spin–echo decay by indirect spin–spin coupling, 218, 255 spin–echo decay via T1 , 20, 258 spin–lattice relaxation, deﬁnition, 23

266

Index

spin–orbit NMR shift, 5, 89 spin–orbit scattering eﬀect on susceptibility for T < Tc , 39 spin–spin correlations below Tc , ab plane, 207 spin–spin correlations below Tc , c axis, 208 spin–spin correlations in terms of χ (q, ω), 102 Spin-spin below Tc , Uldry-Meier analysis, 207 spin-spin correlations in YBCO7, 91, 161, 165 Stoner enhancement of susceptibility, 189 structures of compounds with CuO2 , 2, 69 superconducting diamagnetism, 5, 55 susceptibility – uniform, 5, 33, 38, 45 susceptibility analyses for V3 X compounds, 49 susceptibility anisotropy in YBCO7, 87 symmetry factors in d–band T1 processes, 51 T1 at T < Tc , Hubbard model, 199 T1 eigenmodes, 25, 27 T1 ﬁt for T < Tc by Monien and Pines, 110 T1 ﬁtting parameters for T < Tc , Monien and Pines, 110 T1 for 17 O in YBCO7, 97 T1 for d–band metals, 50 T1 formulated in terms of χ (q, ω), 99 T1 in mixed state via spin diﬀusion to normal cores, 62 T1 measurement techniques, 27 T1 measurements for T < Tc : simple metals, 41 T1 model for YBCO using INS data, 179 T1 model for cuprates by Millis, Monien, and Pines, 172 T1 models for cuprates, 159 T1 parameterization by Uldry and Meier, 160 T1 ratios in YBCO7, Mila–Rice interpretation, 90 T1 recovery for (− 21 ↔ 12 ) transition, 28

T1 T1 T1 T1 T1

recovery for NQR, 28 recovery with inversion, 28 recovery with saturation, 28 recovery with spectral diﬀusion, 29 studies in type–II superconductors, 58 T1 with q–dependent structure factors, 101 T1 with Gaussian model compared with UM analysis, 184 T1 , deﬁnition, 23 T1 , magnetic dipolar processes, 23 T1 , quadrupolar processes, 23 T1 : Quadrupolar vs. magnetic dipole, 24 T1 ’s for LSCO:0.15 calculated from INS data, 230 T2 decay for 17 O in LSCO:0.15, 240 T2 for spin echoes, 19, 251, 255 T2 , deﬁnition, 19 T2g , 6, 255 T2g dependence on correlation length, 222 T2g used to calibrate dyanmical susceptibility, 182 T2g values from various systems, 220 T2g variation below Tc , Hubbard model, 224 T2g variation with temperature, 223 T2g , Gaussian model for, 217 t-J model of quasiparticle behavior, 71 tetragonal phase of LSCO:x, 3 transferred HF coupling in cuprates, 81 Type–II superconductivity in d–band metals, 54 Type–II superconductor NMR studies, 53 Wannier wavefunction for Cu(2) – Mila Rice model, 88 89

Y, 4, 5 Y HF coupling from dipolar interaction, 183 89 Y chemical shift by extrapolation, 122 89 Y relaxation in YBCO7, 92 Y248, 2, 74, 92, 118, 160, 175, 181 Y248 analysis by Uldry and Meier, 169 Y248 dynamical crossover T1 T /T2g study, 245 89

Index Y248, NMR shift and T1 , 139 Y248, pseudogap behavior, 138 Y248, pseudogap energy, 141 YBCO structure, 70 YBCO, evaluation of HF coeﬃcients, 83 YBCO, introduction of the Spin Hamiltonian model for 63 Cu(2), 79 YBCO6+x, chemcal shift of 89 Y, 77 YBCO6+x, variation of 89 Y shift with x, 76 YBCO6.63 analysis by Uldry and Meier, 167 YBCO6.63 discussion by Millis, Monien, and Pines, 178 YBCO6.63 pseudogap NMR data, 117 YBCO6.63, 89 Y T1 behavior, 132 YBCO6.63, T1 data, 130 YBCO7, 4

267

YBCO7 T1 modeling by Millis, Monien, and Pines, 175 YBCO7 - early results on 63,65 Cu NMR studies, 73 YBCO7 – 63,65 Cu T1 data, 74 YBCO7 – 63 Cu(2) powder pattern, 76 YBCO7 – early NMR results, 72 YBCO7 – NQR studies, 74, 111 YBCO7 analysis by Uldry and Meier, 163 YBCO7, 63 Cu(2) T1 anisotropy, 79 YBCO7, 63 Cu(2) relaxation models, 79, 159 YBCO7, early results on 89 Y NMR, 73 YBCO7-x, 2 Yosida function calculation for cuprates, 108 Yosida function measurement in Al metal, 40 Zhang–Rice singlet, 70

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close